Fundamentals of Crystallography C. GIACOVAZZO, H. L. MONACO, D. VITERBO F. SCORDARI, G. GILLI, G. ZANOTTI, M. CATTl Edited by
C. GIACOVAZZO Dipartimento Geomineralogico, University of Bari, ltaly and lstituto di Ricerca per lo Sviluppo delle Metodologie Cristallografiche, CNR, Bari, ltaly
INTERNATIONAL UNION OF CRYSTALLOGRAPHY OXFORD UNIVERSITY PRESS
OXFORD UNIVERSITY PRESS
Great Clarendon Street, Oxford 0x2 6 D P Oxford University Press is a department of the University of Oxford. It furthers the University's objective of excellence in research, scholarship, and education by publishing worldwide in Oxford New Yorlz Athens Auclzland Bangkok Bogota Buenos Aires Calcutta Cape Town Chennai Dares Salaam Delhi Florence Hong Kong Istanbul Karachi KualaLumpur Madrid Melbourne MexicoCity Mumbai Nairobi Paris S%oPaulo Shanghai Singapore Taipei Tokyo Toronto Warsaw with associated companies in Berlin Ibadan Oxford is a registered trade mark of Oxford University Press in the UK and in certain other countries Published in the United States by Oxford University Press Inc., New York O C. Giacovazzo, H. L. Monaco, D. Viterbo, F. Scordari, G. Gilli, G. Zanotti, M. Catti, 1992 The moral rights of the author have been asserted Database right Oxford University Press (maker) Parts of this work first appeared as Introduzione alla cristallografia moderna by M. Bolognesi, A. Coda, C. Giacovazzo, G. Gilli, F. Scordari, and D. Viterbo, edited by C. Giacovazzo, and published by Edizioni Fratelli Laterza, O 1985 First published by Oxford University Press 1992 Reprinted 1994,1995,1998,2000 All rights resewed. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press, or as expressly permitted by law, or under terms agreed with the appropriate reprographics rights organization. Enquiries concerning reproduction outside the scope of the above should be sent to the Rights Department, Oxford University Press, at the address above You must not circulate this book in any other binding or cover and you must impose this same condition on any acquirer A catalogue record for this book is available from the British Library Library of Congress Cataloging in Publication Data Fundamentals of crystallography/C. Giacovazzo . . . [et al.]; edited by C. Giacovazzo. (International Union of Crystallography texts on crystallography; 2). Includes bibliographical references. 1. Crystallography. I. Giacovazzo, Carmelo. 11. Series. QD905.2.F86 1992 548dc2O 9127271 ISBN 0 19 855578 4 (Pblz.) Printed in Great Britain on acidfree paper by The Bath Press, Bath
Preface
Crystallography, the science concerned with the study of crystals, is a very old subject. However, only in this century has it developed into a modern science, after the discovery of Xrays and their diffraction by crystals. In recent years crystallography as assumed an increasingly important role in the modern sciences because o its interdisciplinary nature, which has acted as a bridge between, and often as a stimulus for, various rapidly evolving disciplines. Indeed, Chemistry, Physics, Earth Sciences, Biology, Mathematics, and Materials Science have all provided stimuli to the development of new crystallographic interests and techniques. In turn, crystallography has significantly contributed to the advancement of these sciences. Thus, while on the one hand crystallography has been enriched, on the other hand writing a textbook describing all of its aspects has been made more difficult. Recently, the demand for a compact book that gives a comprehensive account of the modern crystallographic subjects has increased. This volume should therefore be a useful and handy textbook for university courses that cover crystallography, fully or only partially. It should also be useful at the more advanced level required for doctorate studies as well as for experienced researchers. It was with these ideas in mind that I first set out to coordinate the in 1985, of a textbook in Italian (Introduzione alla cristallograjia moderna, Edizioni Fratelli Laterza, Bari) of which Fundamentals of crystallography is not only an English translation, but a completely revised and updated version with a new chapter on crystal physics. It was clear to me that (a) the book had to be written by several authors in order to take advantage of their specific expertise; (b) the different chapters had to be carefully harmonized in order to conform them to a unified plan. It seems to me that these two requirements are even more valid today and their achievement is entirely due to the creative cooperation of the coauthors of this book. Two of the coauthors of the Italian textbook, M. Bolognesi and A. Coda, were unable to carry out the translation and revision of their chapters. I wish to express my thanks for their valuable contribution to the previous edition. In this book their topics are treated by G. Zanotti and H. L. Monaco. An additional chapter on crystal physics has been written by M. Catti. I thank the three new authors for entering our team and all the authors for their enthusiastic participation in this project.
f
Bari, Italy August 1991
C.G.
Acknowledgements
We have the pleasant task of expressing our gratitude to Dr C. K. Prout and to Dr D. J. Watkin for encouraging us to write this book and for their useful advice. We have also to thank many friends and colleagues who have commented on the manuscript or given technical support. The cover picture was kindly provided by Professor A. Zecchina and Dr S. Bordiga, who used the ChemX software of Chemical Design Ltd, Oxford, UK. Thanks are also due from C. Giacovazzo to Mr D. Trione for his accurate and rapid typing of the manuscript, to Mr G. Pellegrino for his aid with the drawings and to Ms C. Chiarella for her technical support; from H. L. Monaco to Mr M. Tognolin for the figures, to Mr R. Pavan for the photographs, and to Mrs A. Migliazza for typing the manuscript; from F. Scordari to Professor F. Liebau for the critical reading of the silicate section and for helpful suggestions, Mr Trione is also acknowledged for the typing of the manuscript; from G. Gilli to Professor V. Bertolasi, Dr V. Ferretti, and Dr P. Gilli for their help in the critical reading of the manuscript; from M. Catti to Mr M. Bandera for his aid with the drawings.
Contents
List of contributors 1
...
1.D The spacegroup rotation matrices 1.E Symmetry groups l . F Symmetry generalization
Xlll
Symmetry in crystals
Carmelo Giacovazzo The crystalline state and isometric operations Symmetry elements Axes of rotational symmetry Axes of rototranslation or screw axes Axes of inversion Axes of rotoreflection Reflection planes with translational component (glide planes) Lattices The rational properties of lattices Crystallographic directions Crystallographic planes Symmetry restrictions due to the lattice periodicity and vice versa Point groups and symmetry classes Point groups in one and two dimensions The Laue classes The seven crystal systems The Bravais lattices Plane lattices Space lattices The space groups The plane and line groups On the matrix representation of symmetry operators Appendices: 1.A The isometric transformations l . B Some combinations of movements 1.C WignerSeitz cells
References
Crystallographic computing
Carmelo Giacovazzo Introduction The metric matrix The reciprocal lattice Basic transformations Transformation from triclinic to orthonormal axes Rotations in Cartesian systems Some simple crystallographic calculations Torsion angles Best plane through a set of points Best line through a set of points Principal axes of a quadratic form Metric considerations on the lattices Niggli reduced cell Sublattices and superlattices Coincidencesite lattices Twins Calculation of the structure factor Calculation of the electron density function The method of least squares Linear least squares Reliability of the parameter estimates Linear least squares with constraints Nonlinear (unconstrained) least squares
viii
I
Contents
Leastsquares refinement of crystal structures Practical considerations on crystallographic least squares Constraints and restraints in crystallographic least squares Alternatives to the method of least squares Rietveld refinement The basis of the technique Some practical aspects of Rietveld refinement Analysis of thermal motion The effect of thermal motion on bond lengths and angles About the accuracy of the calculated parameters Appendices: 2.A Some metric relations between direct and reciprocal lattices 2.B Some geometrical calculations concerning directions and planes 2. C Some transformation matrices 2.D Reciprocity of F and I lattices 2.E Transformations of crystallographic quantities in rectilinear spaces 2.F Derivation of the normal equations 2.G Derivation of the variancecovariance matrix M, 2.H Derivation of the unbiased estimate of Mx 2.1 The FFT algorithm and its crystallographic applications 2.5 Examples of twin laws References
3
The diffraction of Xrays by crystals
Carmelo Giacovazzo
Introduction Thomson scattering Compton scattering Interference of scattered waves Scattering by atomic electrons Scattering by atoms The temperature factor Scattering by a molecule or by a unit cell Diffraction by a crystal Bragg's law The reflection and the limiting spheres Symmetry in reciprocal space Friedel law Effects of symmetry operators in the reciprocal space Determination of the Laue class Determination of reflections with restricted phase values Systematic absences Unequivocal determination of the space group Diffraction intensities Anomalous dispersion The Fourier synthesis and the phase problem Modulated crystal structures Appendices: 3.A Mathematical background 3.B Scattering and related topics 3.C Scattering of Xrays by gases, liquids, and amorphous solids 3.D About electron density mapping 3 .E Modulated structures and quasicrystals References 4
Experimental methods in Xray crystallography
Hugo L. Monaco Xray sources Conventional generators Synchrotron radiation
Contents
Monochromatization, collimation, and focusing of Xrays Data collection techniques for single crystals The Weissenberg camera The precession camera The rotation (oscillation) method in macromolecular crystallography Densitometry The singlecrystal diffractometer Area detectors Data collection techniques for polycrystalline materials Xray diffraction of polycrystalline materials Cameras used for polycrystalline materials Diffractometers used for polycrystalline materials Uses of powder diffraction Data reduction Lorentz correction Polarization correction Absorption corrections Radiation damage corrections Relative scaling Appendices: 4.A Determination of the number of molecules in the unit cell of a crystal References 5
Solution and refinement of crystal structures
Davide Viterbo Introduction Statistical analysis of structure factor amplitudes The Patterson function and its use The heavy atom method Advanced Patterson methods Direct methods Introduction Structure invariants and semiinvariants Probability methods Fixing the origin and the enantiomorph
Phase determination procedures Completing and refining the structure Difference Fourier method Leastsquares method Absolute configuration Appendices: 5.A Structure factor probability distributions 5.B Patterson vector methods 5.C Two examples of deriving phase information from positivity 5.D Probability formulae for triplet invariants 5 . E Pseudotranslational symmetry 5.F Magic integers 5.G New multisolution techniques 5.H Procedures for completing a partial model References 6
Ionic crystals
Fernando Scordari The structure of the atom Atoms with a single electron Atoms with more than one electron Interactions between ions Notes on chemical bonds Ionic crystals Lattice energy: the contributions of attractive and repulsive terms Lattice energy: CFSE contribution Applications of lattice energy calculations Ionic radius Maximum filling principle Coordination polyhedra Radius ratio rule Applications of the concept of ionic radius
I
ix
x
1
Contents
Closest packings Pauling's rules Pauling's first rule Pauling's second rule Pauling's third rule Pauling's fourth rule Pauling's fifth rule Ideal and defect structures MX structures MX, and M2X structures MX3 and M,X, structures A,B,X, structures On the classification of silicates Liebau's crystallochemical classification Structural formulae Relationship between classification parameters and properties of the cations Appendices: 6.A Application of the concept of the packing coefficient (c,) 6.B Structural inferences from crystallochemical parameters References 7
Molecules and molecular crystals
Ring conformations Ring conformation and group theory Computation of puckering coordinates Molecular geometry and the chemical bond An overview of bond theories The VSEPR theory Valence bond (VB) theory Hybridization. The machinery Molecular mechanics Molecular hermeneutics: the interpretation of molecular structures Correlative methods in structural analysis Some threecentrefourelectron linear systems Nucleophilic addition to organometallic compounds Nucleophilic addition to the carbonyl group A case of conformational rearrangement Resonance assisted hydrogen bonding (RAHB) References 465
Gastone Gilli Chemistry and Xray crystallography Crystal and molecular structure The growth of structural information The nature of molecular crystals Generalities A more detailed analysis of intermolecular forces Thermodynamics of molecular crystals Free and lattice energy of a crystal from atomatom potentials Polymorphism and the prediction of crystal structures Effect of crystal forces on molecular geometry Elements of classical stereochemistry Structure: constitution, configuration, and conformation Isomerism
8
465
486
Protein crystallography
Giuseppe Zanotti Introduction Protein crystals Principles of protein crystallization The solvent content of protein crystals Preparation of isomorphous heavyatom derivatives How isomorphous are isomorphous derivatives? The solution of the phase problem The isomorphous replacement method Anomalous scattering: a complementary (or alternative) approach to the solution of the phase problem The use of anomalous scattering in the determination of the absolute configuration of the macromolecule The treatment of errors
Contents
The refinement of heavyatom parameters Picking up minor heavyatom sites: the differenceFourier synthesis A third approach to the solution of the phase ambiguity: realspace filtering Rotation and translation functions and the molecular replacement method Direct methods and the maximumentropy principle in macromolecular crystallography The interpretation of electron density maps and the refinement of the model The interpretation of electron density maps Interactive computer graphics and model building The refinement of the structure Protein structure General aspects Levels of organization of proteins: secondary structure Polypeptide chain description Higher levels of organization: tertiary and quaternary structure, domains, and subunits Groups other than amino acids Thermal parameters and disordered structures Solvent structure The influence of crystal packing Protein classification Appendices: 8.A Some formulae for isomorphous replacement and anomalous dispersion 8.B Translation functions 8.C Macromolecular leastsquares refinement and the conjugategradient algorithm 8.D Conventions and symbols for amino acids and peptides
References and further reading
, 9
Physical properties of crystals Michele Catti
Introduction Crystal anisotropy and tensors Tensorial quantities Symmetry of tensorial properties Overview of physical properties Electrical properties of crystals Pyroelectricity Dielectric impermeability and optical properties Elastic properties of crystals Crystal strain Inner deformation Stress tensor Elasticity tensor Examples and applications Piezoelectricity Symmetry properties of the piezoelectric tensor Crystal defects Experimental methods Planar defects Line defects: dislocations The Burgers circuit Xray topography of dislocations Energy of a dislocation Motion and interaction of dislocations Partial dislocations Smallangle grain boundaries Point defects Thermal distribution of defects Diffusion Ionic conductivity Appendix: 9.A Properties of secondrank tensors Further reading Index
1
xi
Nec possunt oculi naturam noscere rerum: proinde animi vitium hoc oculis adfingere noli. Lucretius, De Rerum Natura, IV, 3867.
Contributors
Carmelo Giacovazzo, Dipartimento Geomineralogico, Universith di Bari, Campus Universitario, 70124 Bari, Italy; Istituto di Ricerca per lo Sviluppo delle Metodologie Cristallografiche, CNR, 70124 Bari, Italy. Hugo L. Monaco, Dipartimento di Genetica e Microbiologia, Sezione di Biologia Molecolare e Biofisica, Universith di Pavia, Via Abbiategrosso 207 27100, Pavia, Italy. Davide Viterbo, Dipartimento di Chimica, Inorganica, Chimica Fisica e Chimica dei Materiali, Universith di Torino, Via P. Giuria 7, 10125 Torino, Italy. Fernando Scordari, Dipartimento Geomineralogico, Universith di Bari, Campus Universitario, 70124 Bari, Italy. Gastone Gilli, Dipartimento di Chimica and Centro di Strutturistica Diffrattometrica, Universith di Ferrara, Via L. Borsari 46, 44100 Ferrara, Italy. Giuseppe Zanotti, Dipartimento di Chimica Organica, Universith di Padova, Via Marzolo 1, 35126 Padova, Italy. Michele Catti, Dipartimento di Chimica Fisica ed Elettrochimica, Universith di Milano, Via Golgi 19, 20133 Milano, Italy.
Symmetry in crystals CARMELO G I A C O V A Z Z O
The crystalline state and isometric operations Matter is usually classified into three states: gaseous, liquid, and solid. Gases are composed of almost isolated particles, except for occasional collisions; they tend to occupy all the available volume, which is subject to variation following changes in pressure. In liquids the attraction between nearestneighbour particles is high enough to keep the particles almost in contact. As a consequence liquids can only be slightly compressed. The thermal motion has sufficient energy to move the molecules away from the attractive field of their neighbours; the particles are not linked together permanently, thus allowing liquids to flow. If we reduce the thermal motion of a liquid, the links between molecules will become more stable. The molecules will then cluster together to form what is macroscopically observed as a rigid body. They can assume a random disposition, but an ordered pattern is more likely because it corresponds to a lower energy state. This ordered disposition of molecules is called the crystalline state. As a consequence of our increased understanding of the structure of matter, it has become more convenient to classify matter into the three states: gaseous, liquid, and crystalline. Can we then conclude that all solid materials are crystalline? For instance, can common glass and calcite (calcium carbonate present in nature) both be considered as crystalline? Even though both materials have high hardness and are transparent to light, glass, but not calcite, breaks in a completely irregular way. This is due to the fact that glass is formed by long, randomly disposed macromolecules of silicon dioxide. When it is formed from the molten state (glass does not possess a definite melting point, but becomes progressively less fluid) the thermal energy which remains as the material is cooled does not allow the polymers to assume a regular pattern. This disordered disposition, characteristic of the liquid state, is therefore retained when the cooling is completed. Usually glasses are referred to as overcooled liquids, while nonfluid materials with a very high degree of disorder are known as amorphous solids. A distinctive property of the crystalline state is a regular repetition in the threedimensional space of an object (as postulated as early as the end of the eighteenth century by R. J. Haiiy), made of molecules or groups of molecules, extending over a distance corresponding to thousands of molecular dimensions. However, a crystal necessarily has a number of defects at nonzero temperature and/or may contain impurities without losing its order. Furthermore: 1. Some crystals do not show threedimensional periodicity because the
2
1
Carmelo Giacovazzo basic crystal periodicity is modulated by periodic distortions incommensurated with the basic periods (i.e. in incommensurately modulated structures, IMS). It has, however, been shown (p. 171 and Appendix 3.E) that IMSs are periodic in a suitable (3 + d)dimensional space. 2. Some polymers only show a bidimensional order and most fibrous materials are ordered only along the fiber axis.
3. Some organic crystals, when conveniently heated, assume a state intermediate between solid and liquid, which is called the mesomorphic or liquid crystal state. These examples indicate that periodicity can be observed to a lesser or greater extent in crystals, depending on their nature and on the thermodynamic conditions of their formation. It is therefore useful to introduce the concept of a real crystal to stress the differences from an ideal crystal with perfect periodicity. Although nonideality may sometimes be a problem, more often it is the cause of favourable properties which are widely used in materials science and in solid state physics. In this chapter the symmetry rules determining the formation of an ideal crystalline state are considered (the reader will find a deeper account in some papers devoted to the subject, or some exhaustive or in the theoretical sections of the International Tables for Cryst~llography).[~~ In order to understand the periodic and ordered nature of crystals it is necessary to know the operations by which the repetition of the basic molecular motif is obtained. An important step is achieved by answering the following question: given two identical objects, placed in random positions and orientations, which operations should be performed to superpose one object onto the other? The well known coexistence of enantiomeric molecules demands a second question: given two enantiomorphous (the term enantiomeric will only be used for molecules) objects, which are the operations required to superpose the two objects? An exhaustive answer to the two questions is given by the theory of isometric transformations, the basic concepts of which are described in Appendix 1.A, while here only its most useful results will be considered. Two objects are said to be congruent if to each point of one object corresponds a point of the other and if the distance between two points of one object is equal to the distance between the corresponding points of the other. As a consequence, the corresponding angles will also be equal in absolute value. In mathematics such a correspondence is called isometric. The congruence may either be direct or opposite, according to whether the corresponding angles have the same or opposite signs. If the congruence is direct, one object can be brought to coincide with the other by a convenient movement during which it behaves as a rigid body. The movement may be: (1) a translation, when all points of the object undergo an equal displacement in the same direction; (2) a rotation around an axis; all points on the axis will not change their position;
Symmetry in crystals
(3) a rototranslation or screw movement, which may be considered as the combination (product) of a rotation around the axis and a translation along the axial direction (the order of the two operations may be exchanged). If the congruence is opposite, then one object will be said to be enantiomorphous with respect to the other. The two objects may be brought to coincidence by the following operations: (1) a symmetry operation with respect to a point, known as inversion; (2) a symmetry operation with respect to a plane, known as reflection; (3) the product of a rotation around an axis by an inversion with respect to a point on the axis; the operation is called rotoinversion; (4) the product of a reflection by a translation parallel to the reflection plane; the plane is then called a glide plane.
(5) the product of a rotation by a reflection with respect to a plane perpendicular to the axis; the operation is called rotoreflection.
Symmetry elements Suppose that the isometric operations described in the preceding section, not only bring to coincidence a couple of congruent objects, but act on the entire space. If all the properties of the space remain unchanged after a given operation has been carried out, the operation will be a symmetry operation. Symmetry elements are points, axes, or planes with respect to . which symmetry operations are performed. In the following these elements will be considered in more detail, while the description of translation operators will be treated in subsequent sections.
Axes of rotational symmetry If all the properties of the space remain unchanged after a rotation of 2nIn around an axis, this will be called a symmetry axis of order n ; its written symbol is n. We will be mainly interested (cf. p. 9) in the axes 1, 2, 3, 4, 6. Axis 1 is trivial, since, after a rotation of 360" around whatever direction the space properties will always remain the same. The graphic symbols for the 2, 3, 4, 6 axes (called two, three, four, sixfold axes) are shown in Table 1.1. In the first column of Fig. 1.1 their effects on the space are illustrated. In keeping with international notation, an object is represented by a circle, with a + or  sign next to it indicating whether it is above or below the page plane. There is no graphic symbol for the 1 axis. Note that a 4 axis is at the same time a 2 axis, and a 6 axis is at the same time a 2 and a 3 axis.
(
3
4
1
Carmelo Giacovazzo Table 1.1. Graphical symbols for symmetry elements: (a) axes normal to the pfane of projection; (b) axes 2 and 2, ,parallel to the plane of projection; (c) axes parallel or inclined to the plane of projection; (d) symmetry pfanes normar to the plane of projection; (e) symmetry planes parallel to the plane of projection
Fig. 1.1. Arrangements of symmetryequivalent objects as an effect of rotation, inversion, and screw axes.
Symmetry in crystals
Axes of rototranslation or screw axes A rototranslational symmetry axis will have an order n and a translational component t, if all the properties of the space remain unchanged after a 2nln rotation around the axis and the translation by t along the axis. On p. 10 we will see that in crystals only screw axes of order 1, 2, 3, 4, 6 can exist with appropriate translational components.
Axes of inversion An inversion axis of order n is present when all the properties of the space remain unchanged after performing the product of a 2nln rotation around the axis by an inversion with respect to a point located on the same axis. The written symbol is fi (read 'minus n' or 'bar n'). As we shall see on p. 9 we will be mainly interested in 1, 2, 3, 4, 6 axes, and their graphic symbols are given in Table 1.1, while their effects on the space are represented in the second column of Fig. 1.1. According to international notation, if an object is represented by a circle, its enantiomorph is depicted by a circle with a comma inside. When the two enantiomorphous objects fall one on top of the other in the projection plane of the picture, they are represented by a single circle divided into two halves, one of which contains a comma. To each half the appropriate + or  sign is assigned. We may note that: (1) the direction of the i axis is irrelevant, since the operation coincides with an inversion with respect to a point; (2) the 2 axis is equivalent to a reflection plane perpendicular to it; the properties of the halfspace on one side of the plane are identical to those of the other halfspace after the reflection operation. The written symbol of this plane is m; (3) the 3 axis is equivalent to the product of a threefold rotation by an inversion: i.e. 3 = 31; (4) the
4 axis is also a 2 axis;
(5) the 6 axis is equivalent to the product of a threefold rotation by a reflection with respect to a plane normal to it; this will be indicated by 6 = 3/m.
Axes of rotoreflection A rotoreflection axis of order n is present when all the properties of the space do not change after performing the product of a 2nln rotation around an axis by a reflection with respect to a plane normal to it. The written symbol of this axis is fi. The effects on the space of the 1, 2, 3, 4, 6 axes coincide with those caused by an inversion axis (generally of a different order). In particular: i = m, 2 = 1, 3 = 6, 4 = 4, 6 = 3. From now on we will no longer consider the ii axes but their equivalent inversion axes.
1
5
6
1
Carmelo Giacovazzo
Reflection planes with translational component (glide planes) A glide plane operator is present if the properties of the halfspace on one side of the plane are identical to those of the other halfspace after the product of a reflection with respect to the plane by a translation parallel to the plane. On p. 11 we shall see which are the glide planes found in crystals. Symmetry operations relating objects referred by direct congruence are called proper (we will also refer to proper symmetry axes) while those relating objects referred by opposite congruence are called improper (we will also refer to improper axes).
Lattices
/Cl
/Cl
/Cl
,,Cl
/Cl
,,Cl
o H , H? ?H ? H ? H? H? /C1
/Cl
/Cl
/Cl
H
H
H
H
&C1
7 1
,Cl
H /Cl
~ i ~ (a). R~~~~~~~~~ of a graphical motif as an example of a twodimensional crystal; (b) corresponding lattice with some examples Of primitive cells; (c) corresponding lattice with some examples of multiple cells.
Translational periodicity in crystals can be conveniently studied by considering the geometry of the repetion rather than the properties of the motif which is repeated. If the motif is periodically repeated at intervals a, b, and c along three noncoplanar directions, the repetition geometry can be fully described by a periodic sequence of points, separated by intervals a, b, c along the same three directions. This collection of points will be called a lattice. We will speak of line, plane, and space lattices, depending on whether the periodicity is observed in one direction, in a plane, or in a threedimensional space. An example is illustrated in Fig. 1.2(a), where HOCl is a geometrical motif repeated at intervals a and b. If we replace the molecule with a point positioned at its centre of gravity, we obtain the lattice of Fig. 1.2(b). Note that, if instead of placing the lattice point at the centre of gravity, we locate it on the oxygen atom or on any other point of the motif, the lattice does not change. Therefore the position of the lattice with respect to the motif is completely arbitrary. If any lattice point is chosen as the origin of the lattice, the position of any other point in Fig. 1.2(b) is uniquely defined by the vector where u and v are positive or negative integers. The vectors a and b define a parallelogram which is called the unit cell: a and b are the basis vectors of the cell. The choice of the vectors a and b is rather arbitrary. In Fig. 1.2(b) four possible choices are shown; they are all characterized by the property that each lattice point satisfies relation (1.1) with integer u and v. Nevertheless we are allowed to choose different types of unit cells, such as those shown in Fig. 1.2(c), having double or triple area with respect to those selected in Fig. 1.2(b). In this case each lattice point will still satisfy (1.1) but u and v are no longer restricted to integer values. For instance, the point P is related to the origin 0 and to the basis vectors a' and b' through ( 4 v) = (112, 112). The different types of unit cells are better characterized by determining the number of lattice points belonging to them, taking into account that the points on sides and on corners are only partially shared by the given cell. The cells shown in Fig. 1.2(b) contain only one lattice point, since the four points at the corners of each cell belong to it for only 114. These cells are called primitive. The cells in Fig. 1.2(c) contain either two or three
Symmetry in crystals
points and are called multiple or centred cells. Several kinds of multiple cells are possible: i.e. double cells, triple cells, etc., depending on whether they contain two, three, etc. lattice points. The above considerations can be easily extended to linear and space lattices. For the latter in particular, given an origin 0 and three basis vectors a , b, and c, each node is uniquely defined by the vector = ua
+ ub + W C .
II
(1.2)
The three basis vectors define a parallelepiped, called again a unit cell. The directions specified by the vectors a , b, and c are the X , Y, Z crystallographic axes, respectively, while the angles between them are indicated by a, 0, and y, with a opposing a , opposing b, and y opposing c (cf. Fig. 1.3). The volume of the unit cell is given by
a Fig.
Notation for a unit cell.
where the symbol '.' indicates the scalar product and the symbol ' A ' the vector product. The orientation of the three crystallographic axes is usually chosen in such a way that an observer located along the positive direction of c sees a moving towards b by an anticlockwise rotation. The faces of the unit cell facing a , b, and c are indicated by A, B, C, respectively. If the chosen cell is primitive, then the values of u, u, w in (1.2) are bound to be integer for all the lattice points. If the cell is multiple then u, u, w will have rational values. To characterize the cell we must recall that a lattice point at vertex belongs to it only for 1/8th, a point on a edge for 114, and one on a face for 112.
The rational properties of lattices Since a lattice point can always be characterized by rational numbers, the lattice properties related to them are called rational. Directions defined by two lattice points will be called rational directions, and planes defined by three lattice points rational planes. Directions and planes of this type are also called crystallographic directions and planes.
Crystallographic directions Since crystals are anisotropic, it is necessary to specify in a simple way directions (or planes) in which specific physical properties are observed. Two lattice points define a lattice row. In a lattice there are an infinite number of parallel rows (see Fig. 1.4): they are identical under lattice translation and in particular they have the same translation period. A lattice row defines a crystallographic direction. Suppose we have chosen a primitive unit cell. The two lattice vectors Q , and Q,,,,, ,, ,, with u, u, w, and n integer, define two different lattice points, but only one direction. This property may be used to characterize a direction in a unique way. For instance, the direction associated with the vector Q9,,,, can be uniquely defined by the vector Q,,,,,with no common factor among the indices. This direction will be indicated by the symbol [3 1 21, to be read as 'three, one, two' and not 'three hundred and twelve'.
Fig. 1.4. Lattice rows and planes.
1
7
8
1
Carmelo Giacovazzo
When the cell is not primitive u, v, w, and n will be rational numbers. Thus Q112,312,113 and Q512,1512,5,3 define the same direction. The indices of the former may therefore be factorized to obtain a common denominator = Q3,6,6,,6 + and no common factor among the numerators: Q, [3 9 21 to be read 'three', nine, minus two'.
,,,,
Crystallographic planes Three lattice points define a crystallographic plane. Suppose it intersects the three crystallographic axes X , Y , and Z at the three lattice points ( p , 0, 0 ) ) (0, q, 0 ) and (0, 0 , r ) with integer p, q, r (see Fig. 1.5). Suppose that m is the least common multiple of p, q , r. Then the equation of the plane is
x'lpa
+ y'lqb + z'lrc = 1.
If we introduce the fractional coordinates x = x ' l a , y = y ' l b , z = z l / c , the equation of the plane becomes
xlp
+ y l q + z l r = 1.
(1.3)
Multiplying both sides by m we obtain
hx + ky
+ lz = m
(1.4)
Fig. 1.5. Some lattice planes of the set (236).
where h , k , and 1 are suitable integers, the largest common integer factor of which will be 1. We can therefore construct a family of planes parallel to the plane (1.4), by varying m over all integer numbers from m to +m. These will also be crystallographic planes since each of them is bound to pass through at least three lattice points. The rational properties of all points being the same, there will be a plane of the family passing through each lattice point. For the same reason each lattice plane is identical to any other within the family through a lattice translation. Let us now show that (1.4) represents a plane at a distance from the origin m times the distance of the plane
The intercepts of the plane (1.5) on X, Y , Z will be l l h , l l k and 111 respectively and those of (1.4) m l h , m l k , m l l . It is then clear that the distance of plane (1.4) from the origin is m times that of plane (1.5). The first plane of the family intersecting the axes X , Y , and Z at three lattice points is that characterized by a m value equal to the least common mutiple of h , k , I. We can therefore conclude that eqn (1.4) defines, as m is varied, a family of identical and equally spaced crystallographic planes. The three indices h , k , and 1 define the family and are its Miller indices. To indicate that a family of lattice planes is defined by a sequence of three integers, these are included within braces: ( h k I ) . A simple interpretation of the three indices h, k , and I can be deduced from (1.4) and (1.5). In fact they
Symmetry in crystals
indicate that the planes of the family divide a in h parts, b in k parts, and c in 1 parts. Crystallographic planes parallel to one of the three axes X, Y, or Z are defined by indices of type (Okl), (hol), or (hkO) respectively. Planes parallel to faces A, B, and C of the unit cell are of type (hOO), (OkO), and (001) respectively. Some examples of crystallographic planes are illustrated in Fig. 1.6. As a numerical example let us consider the plane
0
k.
(110)
1
9
(010)
(zio)
which can be written as
Fig. 1.6. Miller indices for some crystallographic planes parallel to Z ( Z i s supposed to be normal to the page).
The first plane of the family with integer intersections on the three axes will be the 30th (30 being the least common multiple of 10, 15, and 6) and all the planes of the family can be obtained from the equation lox + 15y 62 = m, by varying m over all integers from m to +m. We observe that if we divide p, q, and r in eqn (1.6) by their common integer factor we obtain x/3 y/2 z/5 = 1, from which
+
+
+
Planes (1.7) and (1.8) belong to the same family. We conclude that a family of crystallographic planes is always uniquely defined by three indices h, k, and 1 having the largest common integer factor equal to unity.
Symmetry restrictions due to the lattice periodicity and vice versa Suppose that the disposition of the molecules in a crystal is compatible with an n axis. As a consequence the disposition of lattice points must also be compatible with the same axis. Without losing generality, we will assume that n passes through the origin 0 of the lattice. Since each lattice point has identical rational properties, there will be an n axis passing through each and every lattice point, parallel to that passing through the origin. In particular each symmetry axis will lie along a row and will be perpendicular to a crystallographic plane. Let T be the period vector of a row passing through 0 and normal to n. We will then have lattice points (see Fig. 1.7(a)) at T, T, T', and T". The vector T'  T" must also be a lattice vector and, being parallel to T, we will have T'  T" = mT where m is an integer value: in a scalar form 2 cos (2nIn) = m
(m integer).
(1.9)
Equation (1.9) is only verified for n = 1, 2, 3, 4, 6. It is noteworthy that a 5 axis is not allowed, this being the reason why it is impossible to pave a room only with pentagonal tiles (see Fig. 1.7(b). A unit cell, and therefore a lattice, compatible with an n axis will also be 3, 3, 4, 6 will also be compatible with an ii axis and vice versa. Thus axes I, allowed.
(b) Fig. 1.7.(a) Lattice points in a plane normal to the symmetry axis n passing through 0.(b) Regular pentagons cannot fill planar space.
10
1
Carmelo Giacovazzo
Let us now consider the restrictions imposed by the periodic nature of crystals on the translational components t of a screw axis. Suppose that this lies along a row with period vector T. Its rotational component must correspond to n = 1, 2, 3, 4, 6. If we apply the translational component n times the resulting displacement will be nt. In order to maintain the periodicity of the crystal we must have nt = p T , with integer p , or For instance, for a screw axis of order 4 the allowed translational components will be (0/4)T, (1/4)T, (2/4)T, (3/4)T, (4/4)T, (5/4)T, . . .; of these only the first four will be distinct. It follows that: (1) in (1.10) p can be restricted within 0 s p < n ; (2) the nfold axis may be thought as a special screw with t = 0. The nature of a screw axis is completely defined by the symbol n,. The graphic symbols are shown in Table 1.1: the effects of screw axes on the surrounding space are represented in Fig. 1.8. Note that: If we draw a helicoidal trajectory joining the centres of all the objects related by a 3, and by a 32 axis, we will obtain, in the first case a righthanded helix and in the second a lefthanded one (the two helices are enantiomorphous). The same applies to the pairs 4, and 4,, 61 and 6,, and 6, and 6,. Fig. 1.8. Screw axes: arrangement of symmetryequivalent objects.
4, is also a 2 axis, 6, is also a 2 and a 32, 64 is also a 2 and a 3,, and 63 is also a 3 and a 2,.
Symmetry in crystals We will now consider the restrictions imposed by the periodicity on the translation component t of a glide plane. If we apply this operation twice, the resulting movement must correspond to a translation equal to pT, where p may be any integer and T any lattice vector on the crystallographic plane on which the glide lies. Therefore 2t = p T , i.e. t = ( p / 2 ) T .As p varies over all integer values, the following translations are obtained OT, (1/2)T, (2/2)T, (3/2)T,. . . of which only the first two are distinct. For p = 0 the glide plane reduces to a mirror m. We will indicate by a, b, c axial glides with translational components equal to a / 2 , b / 2 , c / 2 respectively, by n the diagonal glides with translational components ( a b ) / 2 or ( a + c ) / 2 or ( b c ) / 2 or ( a + b + c ) / 2 . In a nonprimitive cell the condition 2t = p T still holds, but now T is a lattice vector with rational components indicated by the symbol d. The graphic symbols for glide planes are given in Table 1.1.
+
+
Point groups a n d s y m m e t r y classes In crystals more symmetry axes, both proper and improper, with or without translational components, may coexist. We will consider here only those combinations of operators which do not imply translations, i.e. the combinations of proper and improper axes intersecting in a point. These are called point groups, since the operators form a mathematical group and leave one point fixed. The set of crystals having the same point group is called crystal class and its symbol is that of the point group. Often point group and crystal class are used as synonyms, even if that is not correct in principle. The total number of crystallographic point groups (for threedimensional crystals) is 32, and they were first listed by Hessel in 1830. The simplest combinations of symmetry operators are those characterized by the presence of only one axis, which can be a proper axis or an inversion one. Also, a proper and an inversion axis may be simultaneously present. The 13 independent combinations of this type are described in Table 1.2. When along the same axis a proper axis and an inversion axis are simultaneously present, the symbol n/ri is used. Classes coinciding with other classes already quoted in the table are enclosed in brackets. The problem of the coexistence of more than one axis all passing by a common point was first solved by Euler and is illustrated, with a different approach, in Appendix 1.B. Here we only give the essential results. Let us suppose that there are two proper axes I , and l2 intersecting in 0 (see Fig. 1.9). The I , axis will repeat in Q an object originally in P, while 1, will Table 1.2. Singleaxis crystallographic point groups Proper axis
Improper axis
Proper and improper axis
1 2 3 4 6
1
(i[i = i)
5

= m
3
4
212= 2jm (3[3 = 3) 414 = 4/m 616 = 6/m
31
6 = 3/m
+
5
+
3
= 13
I
11
12
t.'
( Carmelo Giacovazzo 11
Table 1.3. For each combination of symmetry axes the minimum angles between axes are given. For each angle the types of symmetry axes are quoted in parentheses
.
'.
P
0
0 Fig. 1.9. Arrangement of equivalent objects around two intersecting symmetry axes.
Combination of symmetry axes
cu (ded
B (ded
Y (ded
2 3 4 6 2 4
90 90 90 90 54 35
90 (2 2) 90 (2 3) 90 (2 4) 90 (2 6) 54 44'08" (2 3) 45 (2 4)
90 60 45 30 70 54
2 2 2 2 3 3
2 2 2 2 3 2
(22) (2 3) (2 4) (2 6) 44'08" (2 3) 15'52" (2 3)
(22) (2 2) (2 2) (2 2) 31 '44" (3 3) 44'08" (4 3)
repeat in R the object in Q. P and Q are therefore directly congruent and this implies the existence of another proper operator which repeats the object in P directly in R. The only allowed combinations are n22, 233, 432, 532 which in crystals reduce to 222, 322, 422, 622, 233, 432. For these combinations the smallest angles between the axes are listed in Table 1.3, while their disposition in the space is shown in Fig. 1.10. Note that the combination 233 is also consistent with a tetrahedral symmetry and 432 with a cubic and octahedral symmetry. Suppose now that in Fig. 1.9 1, is a proper axis while 1, is an inversion one. Then the objects in P and in Q will be directly congruent, while the object in R is enantiomorphic with respect to them. Therefore the third operator relating R to P will be an inversion axis. We may conclude that if one of the three symmetry operators is an inversion axis also another must be an inversion one. In Table 1.4 are listed all the point groups characterized by combinations of type PPP, PII, IPI, IIP (P=proper, I = improper), while in Table 1.5 the classes with axes at the same time proper and improper are given. In the two tables the combinations coinciding with previously considered ones are closed within brackets. The
Fig. 1.10. Arrangement of proper symmetry axes for six point groups.
Symmetry in crystals Table 1.4. Crystallographic point groups with more than one axis PPP
PI1
I P I
IIP
(43
2
432 
rnlm
Table 1.5. Crystallographic point groups with more than one axis, each axis being proper and improper simultaneously
results so far described can be easily derived by recalling that: If two of the three axes are symmetry equivalent, they can not be one proper and one improper; for example, the threefold axes in 233 are symmetry referred by twofold axes, while binary axes in 422 differing by 45" are not symmetry equivalent. If an evenorder axis and a ? axis (or an m plane) coexist, there will also be an m plane (or a ? axis) normal to the axis and passing through the intersection point. Conversely, if m and ? coexist, there will also be a 2 axis passing through ? and normal to m. In Tables 1.2, 1.4, and 1.5 the symbol of each point group does not reveal all the symmetry elements present: for instance, the complete list of symmetry elements in the class 2/m33 is 2/m 2/m 2/m?3333. On the other hand, the symbol 2/m% is too extensive, since only two symmetry operators are independent. In Table 1.6 are listed the conventional symbols used for the 32 symmetry classes. It may be noted that crystals with inversion symmetry operators have an equal number of 'left' and 'right' moieties; these parts, when considered separately, are one the enantiomorph of the other. The conclusions reached so far do not exclude the possibility of crystallizing molecules with a molecular symmetry different from that of the 32 point groups (for instance with a 5 axis). In any case the symmetry of the crystal will belong to one of them. To help the reader, some molecules and their point symmetry are shown in Fig. 1.11. It is very important to understand how the symmetry of the physical properties of a crystal relates to its point group (this subject is more extensively described in Chapter 9). Of basic relevance to this is a postulate
1
13
E E E E E E E E E Ekkbmm .2E341mmo E E
E E E E E EEE E EkEnmm .  2 E 9 3 ~ ~ m wE E
Symmetry in crystals
1
15
2. The variation of the refractive index of the crystal with the vibration direction of a planepolarized light wave is represented by the optical indicatrix (see p. 607). This is in general a threeaxis ellipsoid: thus the lowest symmetry of the property 'refraction' is 2/m 2lm 2/m, the point group of the ellipsoid. In crystal classes belonging to tetragonal, trigonal, or hexagonal systems (see Table 1.6) the shape of the indicatrix is a rotational ellipsoid (the axis is parallel to the main symmetry axis), and in symmetry classes belonging to the cubic system the shape of the indicatrix is a sphere. For example, in the case of tourmaline, with point group 3m, the ellipsoid is a revolution around the threefold axis, showing a symmetry higher than that of the point group. We shall now see how it is possible to guess about the point group of a crystal through some of its physical properties: 1. The morphology of a crystal tends to conform to its point group symmetry. From a morphological point of view, a crystal is a solid body bounded by plane natural surfaces, the faces. The set of symmetryequivalent faces constitutes a form: the form is open if it does not enclose space, otherwise it is closed. A crystal form is named according to the number of its faces and to their nature. Thus a pedion is a single face, a pinacoid is a pair of parallel faces, a sphenoid is a pair of faces related by a diad axis, a prism a set of equivalent faces parallel to a common axis, a pyramid is a set of planes with equal angles of inclination to a common axis, etc. The morphology of different samples of the same compound can show different types of face, with different extensions, and different numbers of edges, the external form depending not only on the structure but also on the chemical and physical properties of the environment. For instance, galena crystals (PbS, point group m3m) tend to assume a cubic, cubeoctahedral, or octahedral habit (Fig. 1.12(a)). Sodium chloride grows as cubic crystals from neutral aqueous solution and as octahedral from active solutions (in the latter case cations and anions play a different energetic role). But at the same temperature crystals will all have constant dihedral angles between corresponding faces (J. B. L. Rome' de l'Ile, 17361790). This property, the observation of which dates back to N. Steno (1669) and D. Guglielmini (1688), can be explained easily, following R. J. Haiiy (17431822), by considering that faces coincide with lattice planes and edges with lattice rows. Accordingly, Miller indices can be used as form symbols, enclosed in braces: {hkl). The indices of welldeveloped faces on natural crystals tend to have small values of h, k, 1, (integers greater than six are rarely involved). Such faces correspond to lattice planes with a high density of lattice points per unit area, or equivalently, with large intercepts alh, blk, cll on the reference axes (Bravais' law). An important extension of this law is obtained if space group symmetry (see p. 22) is taken into account: screw axes and glide planes normal to a given crystal face reduce its importance (DonnayHarker principle). The origin within the crystal is usually chosen so that faces (hkl) and (hit) are parallel faces an opposite sides of the crystal. In Fig. 1.13 some idealized crystal forms are shown. The orientation of the faces is more important than their extension. The orientations can be represented by the set of unit vectors normal to them. This set will tend to assume the pointgroup symmetry of the given crystal
(b) Fig. 1.12. (a) Crystals showing cubic or cubeoctahedral or octahedral habitus, (b) crystal with a sixfold symmetry axis.
16
1
Carmelo Giacovazzo independently of the morphological aspect of the samples. Thus, each sample of Fig. 1.12(a) shows an m3m symmetry, and the sample in Fig. 1.12(b) shows a sixfold symmetry if the normals to the faces are considered instead of their extensions. The morphological analysis of a crystalline sample may be used to get some, although not conclusive, indication, of its pointgroup symmetry.
Fig. 1.13. Some simple crystal forms: (a) cinnabar, HgS, class 32; (b) arsenopyritf, FeAsS, class mmm; (c) ilmenite, FeTiO,, class 3; (d) gypsum, CaSO,, class 2/m.
2. Electrical charges of opposite signsmay appear at the two hands of a polar axis of a crystal subject to compression, because of the piezoelectric effect (see p. 619). A polar axis is a rational direction which is not symmetry equivalent to its opposite direction. It then follows that a polar direction can only exist in the 21 noncentrosymmetric point groups (the only exception is the 432 class, where piezoelectricity can not occur). In these groups not all directions are polar: in particular a direction normal to an evenorder axis or to a mirror plane will never be polar. For instance, in quartz crystals (SOz, class 32), charges of opposite sign may appear at the opposite hands of the twofold axes, but not at those of the threefold axis.
3. A point group is said to be polar if a polar direction, with no other symmetry equivalent directions, is allowed. Along this direction a permanent electric dipole may be measured, which varies with temperature (pyroelectric effect, see p. 606). The ten polar classes are: 1, 2, m, mm2, 4, 4mm, 6, 6mm, 3, 3m. Piezo and pyroelectricity tests are often used to exclude the presence of an inversion centre. Nevertheless when these effects are not detectable, no definitive conclusion may be drawn. 4. Ferroelectric crystals show a permanent dipole moment which can be changed by application of an electric field. Thus they can only belong to one of the ten polar classes.
5. The symmetry of a crystal containing only one enantiomer of an optically active molecule must belong to one of the 11 point groups which do not contain inversion axes. 6. Because of nonlinear optical susceptibility, light waves passing through noncentrosymmetric crystals induce additional waves of frequency twice the incident frequency. This phenomenon is described by a thirdrank tensor, as the piezoelectric tensor (see p. 608): it occurs in all noncentrosymmetric groups except 432, and is very efficientL7]for testing the absence of an inversion centre.
7. Etch figures produced on the crystal faces by chemical attack reveal the face symmetry (one of the following 10 twodimensional point groups).
Point groups in one and two dimensions The derivation of the crystallographic point groups in a twodimensional space is much easier than in three dimensions. In fact the reflection with respect to a plane is substituted by a reflection with respect to a line (the same letter m will also indicate this operation); and ii axes are not used. The total number of point groups in the plane is 10, and these are indicated by the symbols: 1, 2, 3, 4, 6, m, 2mm, 3m, 4mm, 6mm. The number of crystallographic point groups in one dimension is 2: they are 1 and m = (I).
Symmetry in crystals
The Laue classes In agreement with Neumann's principle, physical experiments do not normally reveal the true symmetry of the crystal: some of them, for example diffraction, show the symmetry one would obtain by adding an inversion centre to the symmetry elements actually present. In particular this happens when the measured quantities do not depend on the atomic positions, but rather on the interatomic vectors, which indeed form a centrosymmetric set. Point groups differing only by the presence of an inversion centre will not be differentiated by these experiments. When these groups are collected in classes they form the 11 Laue classes listed in Table 1.6.
The seven crystal systems If the crystal periodicity is only compatible with rotation or inversion axes of order 1, 2, 3, 4, 6, the presence of one of these axes will impose some restrictions on the geometry of the lattice. It is therefore convenient to group together the symmetry classes with common features in such a way that crystals belonging to these classes can be described by unit cells of the same type. In turn, the cells will be chosen in the most suitable way to show the symmetry actually present. Point groups 1 and i have no symmetry axes and therefore no constraint axes for the unit cell; the ratios a:b:c and the angles a , P, y can assume any value. Classes 1 and are said to belong to the triclinic system. Groups 2, m, and 2/m all present a 2 axis. If we assume that this axis coincides with the b axis of the unit cell, a and c can be chosen on the lattice plane normal to b. We will then have a = y = 90" and P unrestricted and the ratios a:b:c also unrestricted. Crystals with symmetry 2, m, and 2/m belong to the monoclinic system. Classes 222, mm2, mmm are characterized by the presence of three mutually orthqgonal twofold rotation or inversion axes. If we assume these as reference axes, we will obtain a unit cell with angles a = P = y = 90" and with unrestricted a:b:c ratios. These classes belong to the orthorhombic system. For the seven groups with only one fourfold axis [4,4,4/m, 422,4mm, 42m, 4/mmm] the c axis is chosen as the direction of the fourfold axis and the a and b axes will be symmetry equivalent, on the lattice plane normal to c. The cell angles will be a = P = y = 90" and the ratios a:b:c = 1:l:c. These crystals belong to the tetragonal system. For the crystals with only one threefold or sixfold axis [3, 3, 32, 3m, 3m, 6, 6, 6/m, 622, 6mm, 62m, 6/mm] the c axis is assumed along the three or sixfold axis, while a and b are symmetry equivalent on the plane perpendicular to c. These point groups are collected together in the trigonal and hexagonal systems, respectively, both characterized by a unit cell with angles a = /3 = 90" and y = 120°, and ratios a:b :c = 1:1:c. Crystals with four threefold axes [23, m3, 432, 43m, m3m] distributed as the diagonals of a cube can be referred to orthogonal unit axes coinciding with the cube edges. The presence of the threefold axes ensures that these directions are symmetry equivalent. The chosen unit cell will have a = P = y = 90' and ratios a :b:c = 1:1:1. This is called the cubic system.
1
17
18
1 Carmelo Giacovazzo The Bravais lattices In the previous section to each crystal system we have associated a primitive cell compatible with the point groups belonging to the system. Each of these primitive cells defines a lattice type. There are also other types of lattices, based on nonprimitive cells, which can not be related to the previous ones. In particular we will consider as different two lattice types which can not be described by the same unitcell type. In this section we shall describe the five possible plane lattices and fourteen possible space lattices based both on primitive and nonprimitive cells. These are called Bravais lattices, after Auguste Bravais who first listed them in 1850.
Plane lattices An oblique cell (see Fig. 1.14(a)) is compatible with the presence of axes 1 or 2 normal to the cell. This cell is primitive and has point group 2. If the row indicated by m in Fig. 1.14(b) is a reflection line, the cell must be rectangular. Note that the unit cell is primitive and compatible with the point groups m and 2mm. Also the lattice illustrated in Fig. 1.14(c) with a = b and y # 90" is compatible with m. This plane lattice has an oblique primitive cell. Nevertheless, each of the lattice points has a 2mm symmetry and therefore the lattice must be compatible with a rectangular system. This can be seen by choosing the rectangular centred cell defined by the unit vectors a' and b'. This orthogonal cell is more convenient because a simpler coordinate system is allowed. It is worth noting that the two lattices shown in Figs. 1.14(b) and 1.14(c) are of different type even though they are compatible with the same point groups. In Fig. 1.14(d) a plane lattice is represented compatible with the presence of a fourfold axis. The cell is primitive and compatible with the point groups 4 and 4mm. In Fig. 1.14(e) a plane lattice compatible with the presence of a three or a sixfold axis is shown. A unit cell with a rhombus shape and angles of 60" and 120" (also called hexagonal) may be chosen. A centred rectangular cell can also be selected, but such a cell is seldom chosen.
(b) m ; 2 m m
Fig. 1.14. The five plane lattices and the corresponding twodimensional point groups.
I
(d)
I
i
i
4;4mm
I
(c)
m;2mm
Symmetry in crystals
1
19
Table 1.7. The five plane lattices 

Cell
Type of cell
Point group of the net
Lattice parameters
Oblique Rectangular Square Hexagonal
P P, C P P
2 2mm 4mm 6mm
a, b, y a, b, y = 90" a = b, y = 90" a=b,y=120"
The basic features of the five lattices are listed in Table 1.7
Space lattices In Table 1.8 the most useful types of cells are described. Their fairly limited number can be explained by the following (or similar) observations: A cell with two centred faces must be of type F. In fact a cell which is at the same time A and B, must have lattice points at (0,1/2,1/2) and (1/2,0, 112). When these two lattice translations are applied one after the other they will generate a lattice point also at (1/2,1/2,0); A cell which is at the same time body and face centred can always be reduced to a conventional centred cell. For instance an I and A cell will have lattice points at positions (1/2,1/2,1/2) and (0,1/2,1/2): a lattice point at (1/2,0,0) will then also be present. The lattice can then be described by a new A cell with axes a ' = a/2, b' = b, and c' = c (Fig. 1.15). It is worth noting that the positions of the additional lattice points in Table 1.8 define the minimal translational components which will move an object into an equivalent one. For instance, in an Atype cell, an object at ( x , y, z) is repeated by translation into ( x , y + m/2, z n/2) with m and n integers: the shortest translation will be (0,1/2,1/2). Let us now examine the different types of threedimensional lattices grouped in the appropriate crystal systems.
+
J Fig. 1.15. Reduction of an I and Acentred cell to an Acentred cell.
Table 1.8. The conventional types of unit cell Symbol
Type
Positions of additional lattice points
Number of lattice points per cell
P I A B C F
primitive body centred Aface centred Bface centred Cface centred All faces centred

R
Rhombohedrally centred (de scription with 'hexagonal axes')
1 2 2 2 2 2 4 3
(112,1/2, l r 2 ) (0,1/2,1/2) (1/2,0,1/2) (1/2,1/2,0) (112,112, O), (1/2,0,1/2) ~0,112,112~ (1/3,2/3,2/3), (2/3,1/3,1/3)
20 ( Carmelo Giacovazzo
Triclinic lattices Even though nonprimitive cells can always be chosen, the absence of axes with order greater than one suggests the choice of a conventional primitive cell with unrestricted a , p, y angles and a:b:c ratios. In fact, any triclinic lattice can always be referred to such a cell.
Monoclinic lattices The conventional monoclinic cell has the twofold axis parallel to b, angles a = y = 90", unrestricted p and a :b:c ratios. A Bcentred monoclinic cell with unit vectors a, b, c is shown in Fig. 1.16(a). If we choose a' = a , b' = b, c' = ( a c ) / 2 a primitive cell is obtained. Since c' lies on the (a, c) plane, the new cell will still be monoclinic. Therefore a lattice with a Btype monoclinic cell can always be reduced to a lattice with a P monoclinic cell. An I cell with axes a, b, c is illustrated in Fig. 1.16(b). If we choose a' = a, b' = b, c' = a + c, the corresponding cell becomes an A monoclinic cell. Therefore a lattice with an I monoclinic cell may always be described by an A monoclinic cell. Furthermore, since the a and c axes can always be interchanged, an A cell can be always reduced to a C cell. An F cell with axes a, b, c is shown in Fig. 1.16(c). When choosing a' = a, b' = b, c' = ( a c ) / 2 a typeC monoclinic cell is obtained. Therefore, also, a lattice described by an F monoclinic cell can always be described by a C monoclinic cell. We will now show that there is a lattice with a C monoclinic cell which is not amenable to a lattice having a P monoclinic cell. In Fig. 1.16(d) a C cell with axes a, b, c is illustrated. A primitive cell is obtained by assuming a' = ( a + b ) / 2 , b' = (  a b ) / 2 , c' = c, but this no longer shows the features of a monoclinic cell, since y' # 90°, a' = b' # c ' , and the 2 axis lies along the diagonal of a face. It can then be concluded that there are two distinct monoclinic lattices, described by P and C cells, and not amenable one to the other.
+
+
+
Orthorhombic lattices In the conventional orthorhombic cell the three proper or inversion axes are parallel to the unit vectors a, b, c, with angles a = /3 = y = 90" and general a:b:c ratios. With arguments similar to those used for monoclinic lattices, the reader can easily verify that there are four types of orthorhombic lattices, P, C, I, and F.
Tetragonal lattices In the conventional tetragonal cell the fourfold axis is chosen along c with a = p = y = 90°, a = b, and unrestricted c value. It can be easily verified that because of the fourfold symmetry an A cell will always be at the same time a B cell and therefore an F cell. The latter is then amenable to a tetragonal I cell. A C cell is always amenable to another tetragonal P cell. Thus only two different tetragonal lattices, P and I, are found. Fig. 1.16. Monoclinic lattices: (a) reduction of a
Cubic lattices
Bcentred cell to a P cell; (b) reduction of an Icentred to an Acentred cell; (c) reduction of an Fcentred to a Ccentred cell; (d) reduction of a Ccentred to a P nonmonoclinic cell.
In the conventional cubic cell the four threefold axes are chosen to be parallel to the principal diagonals of a cube, while the unit vectors a, b, c are parallel to the cube edges. Because of symmetry a typeA (or B or C)
Symmetry in crystals
1
21
cell is also an F cell. There are three cubic lattices, P, I, and F which are not amenable one to the other.
Hexagonal lattices In the conventional hexagonal cell the sixfold axis is parallel to c, with a = b, unrestricted c, a = /3 = 90") and y = 120". P is the only type of hexagonal Bravais lattice.
Trigonal lattices As for the hexagonal cell, in the conventional trigonal cell the threefold axis is chosen parallel to c, with a = b, unrestricted c, a = /3 = 90°, and y = 120". Centred cells are easily amenable to the conventional P trigonal cell. Because of the presence of a threefold axis some lattices can exist which may be described via a P cell of rhombohedral shape, with unit vectors a R , bR, CR such that aR= bR = cR, aR= PR = YR, and the threefold axis along the UR + bR + CR direction (see Fig. 1.17). Such lattices may also be described by three triple hexagonal cells with basis vectors UH, bH, CH defined according to[61
These hexagonal cells are said to be in obverse setting. Three further triple hexagonal cells, said to be in reverse setting, can be obtained by changing a H and bH to aH and bH. The hexagonal cells in obverse setting have centring points (see again Fig. 1.17)) at (O,O, O),
I
,I
,I
,
(113,213,213)
while for reverse setting centring points are at It is worth noting that a rhombohedral description of a hexagonal P lattice is always possible. Six triple rhombohedral cells with basis vectors a;, bk,
Fig. 1.17. Rhombohedra1 lattice. The basis of the rhombohedral cell is labelled a, b,, c,, the basis of the hexagonal centred cell is labelled a, b,, c, (numerical fractions are calculated in terms of the c, axis). (a) Obverse setting; (b) the same figure as in (a) projected along c,.
22
1
Carmelo Giacovazzo
ck can be obtained from a H , bH, CH by choosing: U ~ = U H + C H , bk=b,+ cH, a k = aH
+ CH,
bk = bH
+ CH,
ck=(aH+bH)+cH ck = a H+ bH + cH
and cyclic permutations of a;, bk, ck. Each triple rhomobohedral cell will have centring points at (O,0, O), (113,1/3,1/3), (213,213,213). In conclusion, some trigonal lattices may be described by a hexagonal P cell, others by a triple hexagonal cell. In the first case the nodes lying on the different planes normal to the threefold axis will lie exactly one on top of the other, in the second case lattice planes are translated one with respect to the other in such a way that the nth plane will superpose on the (n + 3)th plane (this explains why a rhombohedral lattice is not compatible with a sixfold axis).
a Fig. 1.18. Intersections of the set of crystallographic planes ( h k l ) with the three symmetryequivalent a, b, daxes in trigonal and hexagonal systems.
When, for crystals belonging to the hexagonal or trigonal systems, a hexagonal cell is chosen, then on the plane defined by a and b there will be a third axis equivalent to them. The family of planes (hkl) (see Fig. 1.18) divides the positive side of a in h parts and the positive side of b in k parts. If the third axis (say d) on the (a, b) plane is divided in i parts we can introduce an extra index in the symbol of the family, i.e. (hkil). From the same figure it can be seen that the negative side of d is divided in h k parts, and then i = (h k). For instance (1 2 3 5), (3 5 2 I), (2 0 2 3) represent three plane families in the new notation. The fourindex symbol is useful to display the symmetry, since (hkil), (kihl), and (ihkl) are symmetry equivalent planes. Also, lattice directions can be indicated by the fourindex notation. Following pp. 78, a direction in the (a, b) plane is defined by a vector (P  0)= ma nb. If we introduce the third axis d in the plane, we can write (P  0)= ma + nb Od. Since a decrease (or increase) of the three coordinates by the same amount j does not change the point P, this may be represented by the coordinates: u = m  j, v = n  j, i = j. If we choose j = (m n)/3, then u = (2m  n)/3, v = (2n  m)/3, i = (m n)/3. In conclusion the direction [mnw] may be represented in the new notation as [uviw], with i = (u v). On the contrary, if a direction is already represented in the fourindex notation [uviw], to pass to the threeindex one, i should be added to the first three indices in order to bring to zero the third index, i.e. [u  i v  i w]. A last remark concerns the point symmetry of a lattice. There are seven threedimensional lattice point groups, they are called holohedries and are listed in Table 1.6 (note that 3m is the point symmetry of the rhombohedral lattice). In two dmensions four holohedries exist: 2, 2mm, 4mm, 6mm. The 14 Bravais lattices are illustrated in Fig. 1.19 by means of their conventional unit cells (see Appendix 1.C for a different type of cell). A detailed description of the metric properties of crystal lattices will be given in Chapter 2.
+
+
+
+
+
+
+
The space groups A crystallographic space group is the set of geometrical symmetry operations that take a threedimensional periodic object (say a crystal) into itself.
Symmetry in crystals
Triclinic
Cubic
Trigonal Hexagonal
The total number of crystallographic space groups is 230. They were first derived at the end of the last century by the mathematicians Fedorov (1890) and Schoenflies (1891) and are listed in Table 1.9. In Fedorov's mathematical treatment each space group is represented by a set of three equations: such an approach enabled Fedorov to list all the space groups (he rejected, however, five space groups as impossible: Fdd2, Fddd, 143d, P4,32, P4132). The Schoenflies approach was most practical and is described briefly in the following. On pp. 1116 we saw that 32 combinations of either simple rotation or inversion axes are compatible with the periodic nature of crystals. By combining the 32 point groups with the 14 Bravais lattices (i.e. P, I, F, . . .) one obtains only 73 (symmorphic) space groups. The others may be obtained by introducing a further variation: the proper or improper symmetry axes are replaced by screw axes of the same order and mirror planes by glide planes. Note, however, that when such combinations have more than one axis, the restriction that all symmetry elements must intersect in a point no longer applies (cf. Appendix l.B). As a consequence of the presence of symmetry elements, several symmetryequivalent objects will coexist within the unit cell. We will call the smallest part of the unit cell which will generate the whole cell when applying to it the symmetry
Fig. 1.19. The 14 threedimensional Bravais lattices.
1
23
24
1
Carmelo Giacovazzo Table 1.9. The 230 threedimensional space groups arranged by crystal systems and point groups. Space groups (and enantiomorphous pairs) that are uniquely determinable from the symmetry of the diffraction pattern and from systematic absences (see p. 159) are shown in boldtype. Point groups without inversion centres or mirror planes are emphasized by boxes Crystal system Triclinic
Point group
[i3 i
Monoclinic m 2/m Orthorhombic
12221 mm2 mmm
Tetragonal
Cubic
4
(231
m3m
Space groups p1 P1 P2, P2,, C2 Pm, PC, Cm, Cc P2/m, P2,/m, C2/m, P2/c, P2,/c, C2/c P222, P222,, P2,2,2, P2,2,2,, C222,, C222, F222, 1222, 12,2121 Pmm2, PmcP,, Pcc2, PmaP,, PcaS,, PncZ,, PmnZ,, Pba2, Pna2,, Pnn2, Cmm2, Cmc2,, Ccc2, Amm2, Abm2, Ama2, Aba2, Fmm2, Fdd2,lmm2, lba2, h a 2 Pmmm,Pnnn,Pccm,Pban,Pmma,Pnna,Pmna,Pcca, Pbam, Pccn, Pbcm, Pnnm, Pmmn, Pbcn, Pbca, Pnma, Cmcm, Cmca, Cmmm, Cccm, Cmma, Ccca, Fmmm, Fddd, Immm, Ibam, Ibca, lmma p4, p41, p4,, p4, P4. 14
14, 14,
P23, F23, 123, P2,3,_12,3 ~ m 3~ , dFm3, , F a , lm3, ~ a 3 I& , PG2, Pa&?, F$32, Y . 2 , 1432, P?,32, P4,32, l4?32 P43m, F43m, 143m, P43n, F43c, 1Gd Pm_3m, Pn3n, PrnBn, Pn3m, Fm3m, Fm&, F b m , F&c, lm3m, la3d
operations an asymmetric unit. The asymmetric unit is not usually uniquely defined and can be chosen with some degree of freedom. It is nevertheless obvious that when rotation or inversion axes are present, they must lie at the borders of the asymmetric unit.
Symmetry in crystals
According to the international (HermannMauguin) notation, the spacegroup symbol consists of a letter indicating the centring type of the conventional cell, followed by a set of characters indicating the symmetry elements. Such a set is organized according to the following rules:
1. For triclinic groups: no symmetry directions are needed. Only two space groups exist: PI and PI. 2. For monoclinic groups: only one symbol is needed, giving the nature of the unique dyad axis (proper and/or inversion). Two settings are used: yaxis unique, zaxis unique. 3. For orthorhombic groups: dyads (proper and/or of inversion) are given along x, y, and z axis in the order. Thus Pca2, means: primitive cell, glide plane of type c normal to xaxis, glide plane of type a normal to the yaxis, twofold screw axis along z . 4. For tetragonal groups: first the tetrad (proper and/or of inversion) axis along z is specified, then the dyad (proper and/or of inversion) along x is given, and after that the dyad along [I101 is specified. For example, P4,lnbc denotes a space group with primitive cell, a 4 sub 2 screw axis along z to which a diagonal glide plane is perpendicular, an axial glide plane b normal to the x axis, an axial glide plane c normal to [110]. Because of the tetragonal symmetry, there is no need to specify symmetry along the yaxis.
5. For trigonal and hexagonal groups: the triad or hexad (proper and/or of inversion) along the zaxis is first given, then the dyad (proper and/or of inversion) along x and after that the dyad (proper and/or of inversion) along [1?0] is specified. For example, P6,mc has primitive cell, a sixfold screw axis 6 sub 3 along z, a reflection plane normal to x and an axial glide plane c normal to [ ~ I o ] . 6. For cubic groups: dyads or tetrads (proper and/or of inversion) along x , followed by triads (proper and/or of inversion) along [ I l l ] and dyads (proper and/or of inversion) along [110]. We note that:
1. The combination of the Bravais lattices with symmetry elements with no translational components yields the 73 socalled symmorphic space groups. Examples are: P222, Cmm2, F23, etc. 2. The 230 space groups include 11 enantiomorphous pairs: P3, (P3,), P3,12 (P3212), P3,21 (P3,21), P41 (P43), P4J2 (P4322), P4,&2 (P4&?,2), P6i (P65), P6, (P64), P6,22 (P6522), P6222 (P6422), P4,32 (P4,32). The ( + ) isomer of an optically active molecule crystallizes in one of the two enantiomorphous space groups, the (  ) isomer will crystallize in the other. 3. Biological molecules are enantiomorphous and will then crystallize in space groups with no inversion centres or mirror planes; there are 65 groups of this type (see Table 1.9).
4. The point group to which the space group belongs is easily obtained from the spacegroup symbol by omitting the lattice symbol and by replacing
1
25
26
1
Carmelo Giacovazzo
the screw axes and the glide planes with their corresponding symmorphic symmetry elements. For instance, the space groups P4Jmmc, P4/ncc, 14,lacd, all belong to the point group 4lmmm. 5. The frequency of the different space groups is not uniform. Organic compounds tend to crystallize in the space groups that permit close packing of triaxial ellipsoids.[81According to this view, rotation axes and reflection planes can be considered as rigid scaffolding which make more difficult the comfortable accommodation of molecules, while screw axes and glide planes, when present, make it easier because they shift the molecules away from each other. Mighell and Rodgers [9] examined 21 051 organic compounds of known crystal structure; 95% of them had a symmetry not higher than orthorhombic. In particular 35% belonged to the space group P2,/c, 13.3% to PI, 12.4% to P2,2,2,, 7.6% to P2, and 6.9% to C21c. A more recent study by ~ i l s o n , [ ' ~based ] on a survey of the 54599 substances stored in the Cambridge Structural Database (in January 1987), confirmed Mighell and Rodgers' results and suggested a possible model to estimate the number Nsg of structures in each space group of a given crystal class: Nsg = Acc exp { BccE21sg  Ccclmls,) where A,, is the total number of structures in the crystal class, [2],, is the number of twofold axes, [m],, the number of reflexion planes in the cell, B,, and Cc, are parameters characteristic of the crystal class in question. The same results cannot be applied to inorganic compounds, where ionic bonds are usually present. Indeed most of the 11641 inorganic compounds considered by Mighell and Rodgers crystallize in space groups with orthorhombic or higher symmetry. In order of decreasing frequency we have: Fm3m, Fd3m, P6Jmmc, P2,/c, ~ m 3 m ~, 3 m C2/m, , C2/c, . . . . The standard compilation of the plane and of the threedimensional space groups is contained in volume A of the International Tables for Crystallography. For each space groups the Tables include (see Figs 1.20 and 1.21). 1. At the first line: the short international (HermannMauguin) and the Schoenflies symbols for the space groups, the point group symbol, the crystal system. 2. At the second line: the sequential number of the plane or space group, the full international (HermannMauguin) symbol, the Patterson symmetry (see Chapter 5, p. 327). Short and full symbols differ only for the monoclinic space groups and for space groups with point group mmm, 4/mmm, 3m, 6/mmm, m3, m3m. While in the short symbols symmetry planes are suppressed as much as possible, in the full symbols axes and planes are listed for each direction. 3. Two types of space group diagrams (as orthogonal projections along a cell axis) are given: one shows the position of a set of symmetrically equivalent points, the other illustrates the arrangement of the symmetry elements. Close to the graphical symbols of a symmetry plane or axis parallel to the projection plane the 'height' h (as a fraction of the shortest lattice translation normal to the projection plane) is printed. If h = 0 the height is omitted. Symmetry elements at h also occur at height h + 112.
Symmetry in crystals
4. Information is given about: setting (if necessary), origin, asymmetric unit, symmetry operations, symmetry generators (see Appendix l.E) selected to generate all symmetrical equivalent points described in block 'Positions'. The origin of the cell for centrosymmetric space groups is usually chosen on an inversion centre. A second description is given if points of high site symmetry not coincident with the inversion centre occur. For example, for ~ n 3 ntwo descriptions are available, the first with origin at 432, and the second with origin at 3. For noncentrosymmetric space groups the origin is chosen at a point of highest symmetry (e.g. the origin for ~ 4 2 c is chosen at 4lc) or at a point which is conveniently placed with respect to the symmetry elements. For example, on the screw axis in P2,, on the glide plane in PC, at la2, in P ~ a 2 at ~ ,a point which is surrounded symmetrically by the three 2, axis in P2,2,2,. 5. The block positions (called also Wyckoff positions) contains the general position (a set of symmetrically equivalent points, each point of which is left invariant only by application of an identity operation) and a list of special positions (a set of symmetrically equivalent points is in special position if each point is left invariant by at least two symmetry operations of the space group). The first three block columns give information about multiplicity (number of equivalent points per unit cell), Wyckoff letter (a code scheme starting with a at the bottom position and continuing upwards in alphabetical order), site symmetry (the group of symmetry operations which leaves invariant the site). The symbol adoptedr9]for describing the site symmetry displays the same sequence of symmetry directions as the space group symbol. A dot marks those directions which do not contribute any element to the site symmetry. To each Wyckoff position a reflection condition, limiting possible reflections, may be associated. The condition may be general (it is obeyed irrespective of which Wyckoff positions are occupied by atoms (see Chapter 3, p. 159) or special (it limits the contribution to the structure factor of the atoms located at that Wyckoff position).
6. Symmetry of special projections. Three orthogonal projections for each space group are listed: for each of them the projection direction, the HermannMauguin symbol of the resulting plane group, and the relation between the basis vectors of the plane group and the basis vectors of the space group, are given, together with the location of the plane group with respect to the unit cell of the space group. 7. Information about maximal subgroups and minimal supergroups (see Appendix l.E) is given. In Figs. 1.20 and 1.21 descriptions of the space groups Pbcn and P4222 are respectively given as compiled in the International Tables for Crystallography. In order to obtain space group diagrams the reader should perform the following operations:
1. Some or all the symmetry elements are traced as indicated in the spacegroup symbol. This is often a trivial task, but in certain cases special care must be taken. For example, the three twofold screw axes do not intersect each other in P2,2,2,, but two of them do in P2,2,2 (see Appendix 1.B) .
1
27
28
1
Carmelo Giacovazzo
Pbcn
Orthorhombic
P 2,lb 2 / c 2 , / n
No. 60
Origin at
i on I c 1
Asymmetric unit
OSxli; 0
Symmetry operations
Fig. 1.20. Representation of the group Pbcn (as inlnternational Tables for Crystallography).
OlzS:
Patterson symmetry P m m m
Symmetry in crystals
No. 60
CONTINUED
Generatorsselected ( I ) ;
1
29
Pbcn
( 1 0 0 ) ; ( 0 1 0 ) ; t(0.0,)); (2); (3); (5)
Positions
8
d
1
(1) x (5)x ' , j , ~
Reflection conditions
Coordinates
Mulliplicity. Wyckoff letter. Site Spmetry
(2) x + ~ , J + : , z + ~ (3) f ,p,i+i ( 6 ) x+:,y+;.5+: ( 7 ) x.J',z++
( 4 ) x+:,y+i,r ( 8 ) x'+:,y+i,z
General : Okl : k = 2 n h01: 1 = 2 n hkO: h +k = 2n hOO: h = 2n OkO: k = 2n 001: 1 = 2 n Special: as above, plus
hkl: h+k=2n hkl : h + k , 1 = 2 n hkl : h + k , l = 2 n Symmetry of special projections Along [001] c 2 m m bl=b al=a Origin at 0,O.z
Along [ 1001 p 2g m al=ib b'=c Origin at x.O.0
Along [010] p 2g m bl=a a'= Origin at O,y,O
Maximal nonisomorphic subgroups 1 [2]P2,22,(P2,2,2) 1;2;3;4 [ 2 ] P1 1 2 , / n ( P 2 , l c ) 1; 2; 5 ; 6 [2]P12/cI(P2/c) 1;3;5;7 [2]P2,/b11(P2,/c) 1;4;5;8 1 ; 2; 7 ; 8 [ 2 ] P b c 2 ,( P c a 2 , ) [ 2 ] P b 2 n( P n c 2 ) 1 ; 3; 6 ; 8 [2]P2,cn(Pna2,) 1;4;6;7 IIa none IIb none Maximal isomorphic subgroups of lowest index IIc [ 3 ] P b c n ( a 1 =3 a ) ; [ 3 ] P b c n ( b 1 =3 b ) ; [ 3 ] P b c n ( c 1 =3 c ) Minimal nonisomorphic supergroups I none I1 [2]Abma(Cmca);[2]Bbab(Ccca);[2]Cmcm;[2]1bam;[2]Pbcb(2a1= a ) ( P c c a ) ; [ 2 ] P r n c a ( 2 b 1 =b ) ( P b c m ) ;[ 2 ] P b mn(2c1= c ) ( P m n a )
30
1
Carmelo Giacovazzo
Tet rag on al
P4222
No. 93
Patterson symmetry
P 4/m m m
Origin at 2 2 2 at 422 1 Asymmetric unit
Olxli;
OIySI;
0Izl$
Symmetry operations
Fig. 1.21. Representation of the group P4,22 (as in International Tables for Crystallography).
2. Once conveniently located, the symmetry operators are applied to a point P in order to obtain the symmetry equivalent points P', P", . . . . If P', P , . . . , fall outside the unit cell, they should be moved inside by means of appropriate lattice translations. The first type of diagram is so obtained. 3. New symmetry elements are then placed in the unit cell so producing the second type of diagram. . Some space group diagrams are collected in Fig. 1.22. Two simple crystal structures are shown in Figs 1.23 and 1.24: symmetry elements are also located for convenience.
The plane and line groups There are 17 plane groups, which are listed in Table 1.10. In the symbol g stays for a glide plane. Any space group in projection will conform to one of these plane groups. There are two line groups: p l and pm. A periodic decoration of the plane according to the 17 plane groups is shown in Fig. 1.25.
Symmetry in crystals
No. 93
CONTINUED
Generators selected ( I ) ;
t (I ,O,O);
t
(0, I ,0); t (O,O, I); (2); (3); (5)
Positions Reflection conditions
Coordinates
Mulliplicily. Wyckofl kllcr. S ~ l esymmetry
General: 001: I = 2 n Special: as above, plus 4
o
..2
x,x,+
f,f,i
f,x,+
x,f,+
Okl: I = 2 n
4
n
..2
x,x,$
f.1,:
f,x,:
x.f,?
Okl: I =2n
4
1
.2.
x,O,+
f,O.f
O.x,O
O,f,O
hhl : I = 2n
4
h
2..
1 , , ,L, z
f ,:,z+:
2
f
2.22
+,+,+ it+,+
hkl : I = 2 n
2
e
2.22
O,O,+
hkl : I = 2n
+,i,T
f,$,f+f
O,O,+
hkl : 1 = 2 n
hkl : h + k + l = 2 n
2
b
222.
f,f,O
f,f,i
Symmetry of special projections Along [OOI] p 4 m m a'=a bl=b Origin at 0,O.z
hkl : I = 2 n
Along [I001 p2n1tn a'=b bl=c Origin at x,O,O
Maximal nonisomorphic subgroups I (2]P4,1 1 ( P 4 2 ) 1;2;3;4 [2]P221(P222) l;2;5;6 [ 2 ] P 2 1 2 ( C 2 2 2 ) 1;2;7;8 IIa none IIb [ 2 ] P 4 , 2 2 ( c 1 = 2 c ) ; [ 2 ] P 4 , 2 2 ( c ' 2= c ) ; ( 2 ] C 4 , 2 2 , ( a 1 = 2 a , b 1 = 2 b ) ( P 4 , 2 , 2 ) ; [ 2 ] F 4 , 2 2 ( a 1 =2a,b1= 2b,c1= 2 c ) ( 1 4 , 2 2 ) Maximal isomorphic subgroups of lowest index IIc [ 3 ] P 4 , 2 2 ( c 1 = 3 c ) ; [ 2 ] C 4 , 2 2 (a1= 2 a , b l = 2 b ) ( P 4 2 2 2 ) Minimal nonisomorphic supergroups I I21P4Jmmc; [ 2 ] P 4 J t n c m ; [ 2 1 P 4 2 / n b c ;[21P42/nnm;[31P4232 I1 ( 2 ] 1 4 2 2 ; [ 2 ] P 4 2 2 ( 2 c 1 =c)
Along [I101 p 2 m m a'= + (  a f b ) bl=c Origin at x,x,$
1
31
32
1
Carmelo Giacovazzo
00
o+
00+
4
0 010 o+
0 0+0 0 
0 0+O
0 0+0 o+
TI1 1
: ! I 1 

0"; 
O+

P 2/m
C2 00+


o+
4
+
c
I
 0 0
+
Fig. 1.22. Some space group diagrams.
On the matrix representation of symmetry operators A symmetry operation acts on the fractional coordinates x,y, z of a point P to obtain the coordinates (x', y', 2') of a symmetryequivalent point P':
The R matrix is the rotational component (proper or improper) of the symmetry operation. As we shall see in Chapter 2 its elements may be 0 , $1, 1 and its determinant is f1. T is the matrix of the translational component of the operation. A list of all the rotation matrices needed to conventionally describe the 230 space groups are given in Appendix 1.D.
Symmetry in crystals
/
33
Fig. 1.23. A P2,2,2, crystal structure (G. Chiari, D. Viterbo, A. Gaetani Manfredotti, and C. Guastini (1975). Cryst. Struct. Commun., 4,561) and its symmetry elements (hydrogen atoms are not drawn).
Fig. 1.24. A P2,/c crystal structure (M. Calleri, G. Ferraris, and D. Viterbo (1966). Acta Cryst., 20, 73) and its symmetry elements (hydrogen atoms are not drawn). Glide planes are emphasized by the shading.
34
1
Carmelo Giacovazzo Table 1.10. The 17 plane groups Oblique cell Rectangular cell Square cell Hexagonal cell
Fig. 1.25. A periodic decoration of the plane according to the 17 crystallographic plane groups (drawing by SYMPATI,a computer program by L. Loreto and M . Tonetti, pixel, 9, 920; Nov 1990).
P I , ~2 pm, pg, a n , ~ 2 m m P, ~ V ,~ 2 9 9c2mm , p4, p4nm~p4gt11 p3, p3rn1, p31n1,p6, p6mrn
When applying the symmetry operator C1= (R,, TI) to a point at the end of a vector r, we obtain X' = CIX = RIX + TI. If we then apply to r' the symmetry operator C2, we obtain
X = C2Xf= R2(RlX + TI)
+ T2= R2RlX + R2Tl + T2.
Symmetry in crystals Since the symmetry operators form a mathematical group, a third symmetry operator must be present (see also pp. 1112), C3 = C2C1= (R2R1, R2T1+ T2),
(1.12)
where R2Rl is the rotational component of C3 and (R2T, +T2) is its translational component. In particular the operator C2= CC will be present and in general also the CJ operator. Because of (1.12) C1 = [RJ, (RJ'
+ . . . + R + I)T].
(1.13)
Let us now apply this result to the space group P6,. Once we have defined the R and T matrices corresponding to an anticlockwise rototranslation of 60" around z, we obtain all the six points equivalent to a point r by applying to it the operators CJ with j going from 1 to 6. Obviously C6= I and C6+j= CJ. For this reason we will say that the 6, operator is of order six (similarly 2 and m are of order two). If r is transferred to r' by C = (R, T) there will also be an inverse operator C' = (R', TI) which will bring r ' back to r. Since we must have C'C = I, because of (1.12) we will also have R'R = I and R'T + T' = 0, and therefore C1
= (R1, R~T)
(1.14)
where Rl is the inverse matrix of R. In the P6, example, Cl = C5. When all the operators of the group can be generated from only one operator (indicated as the generator of the group) we will say that the group is cyclic. All symmetry operators of a group can be generated from at most three generators. For instance, the generators of the space group P6,22 are 6, and one twofold axis. Each of the 12 different operators of the group may be obtained as C',, j = 1, 2, . . . , 6, say the powers of 61, or as C2, the twofold axis operator, or as their product. We can then represent the symmetry operators of P6'22 as the product {C1){C2), where {C) indicates the set of distinct operators obtained as powers of C. Similarly there are two generators of the group P222 but three of the group ~ 4 3 mIn . general all the operations of a space group may be represented by the product {C1){C2){C3). If only two generators are sufficient, we will set C3 = I, and if only one is sufficient, then C2 = C3 = I. The list of the generators of all point groups is given in Appendix 1.E. So far we have deliberately excluded from our considerations the translation operations defined by the Bravais lattice type. When we take them into account, all the spacegroup operations may be written in "a very simple way. In fact the set of operations which will transfer a point r in a given cell into its equivalent points in any cell are: { c ~ {c2} } {c3} (1.15) where T = mla m2b m3c is the set of lattice translations. The theory of symmetry groups will be outlined in Appendix 1.E.
+
+
Appendices 1.A The isometric transformations It is convenient to consider a Cartesian basis (el, e2, e3). Any transformation which will keep the distances unchanged will be called an isometry or
1
35
36
1
Carmelo Giacovazzo an isometric mapping or a movement C. It will be a linear transformation, in the sense that a point P defined by the positional r x t o r r = xe, ye2 ze3 is related to a point P', with positional vector r' = x f e l y1e2 zfe3by the relation
+
+ + +
with the extra condition
RR= I
or
R = R'.
R indicates the transpose of the matrix R and I is the identity matrix. We note that X and X' are the matrices of the components of the vectors r and r' respectively, while T is the matrix of the components of the translation vector t = Tlel T,e2 T3e3. A movement, leaving the distances unchanged, will also maintain the angles fixed in absolute value. Since the determinant of the product of two matrices is equal to the product of the two determinants, from (1.A.2) we have (det R)'= 1, and then det R = f1. We will refer to direct or opposite movements and to direct or opposite congruence relating an object and its transform, depending on whether det R is +1 or 1.
+
+
Direct movements Let us separate (l.A.l) into two movements: X1=X0+T Xo = RX. (1.A.3) adds to each position vector a fixed vector and corresponds therefore to a translation movement. (1.A.4) leaves the origin point invariant. In order to find the other points left invariant we have to set Xo = X and obtain
(1.A.5a) will have solutions for X#O only if det (R  I) = 0. Since det (R  I) = det (R  RR) = det [(I  R)RJ = det (I  R) det R = det (I  R) = det (R  I), then this condition is satisfied. Therefore one of the three equations represented by (1.A.4) must be a linear combination of the other two. The two independent equations will define a line, which is the locus of the invariants points; the movement described by (1.A.4) is therefore a rotation. In conclusion, a direct movement can be considered as the combination (or, more properly, the product) of a translation with a rotation around an axis. If in eqn (1.A.1) is R = I then the movement is a pure translation, if T = 0 the movement is a pure rotation. When the translation is parallel to the rotation axis the movement will be indicated as rototranslation. An example of direct movement is the transformation undergone by the points of a rigid body when it is moved. Another example is the anticlockwise rotation around the z axis of an angle 8; this will move r(x, y, z ) into
Symmetry in crystals
r1(x', y', z') through the transformation xl=xcosOysinO y1=xsin8+ycos0 which in matrix notation becomes X' = RX, with (l.A.5b)
R' can be obtained by substituting 8 with 8 and it can be immediately seen that, in agreement with (1.A.2), R = Rl. We will now show that any direct movement can be carried out by means of a translation or a rotation or a rototranslation. Let us suppose that an isometric transformation relates the three noncollinear points A, B, C with the points A', B', C' respectively. If a is the translation bringing A on A', then, if also B and C superpose on B' and C', the movement is a translation; if not, then the complete superposition can be achieved by a rotation R around an axis 1 passing through A'. If 1 is perpendicular to a, the movement resulting from the combination of the rotation and translation operations is still a pure rotation around an axis parallel to 1 (see Appendix l.B). If a is not perpendicular to 1, then it can be decomposed into two translational components a1 and a2, one perpendicular and the other parallel to 1. The product of R times al is a pure rotation around an axis parallel to 1, which, when composed with a2, results in a rototranslation movement.
Opposite movements An opposite movement can be obtained from a direct one by changing the sign to one or three rows of the R matrix. For instance, when changing the sign of the third row, we substitute the vector ( x ' , y', 2') with (x', y', zl), i.e. the point P' with its symmetry related with respect to a plane at z = 0. This operation is called a reflection with respect to the plane at z = 0. Changing the signs of all three rows of the R matrix implies the substitution of the vector (x', y', z') with (x', y ', 2')) i.e. of the point P with its symmetry related with respect to the origin of the coordinate system. This operation is called inversion with respect to a point. We may conclude that each direct movement, followed by a reflection with respect to a plane or by an inversion with respect to a point yields an opposite movement. On the other hand an opposite movement may be obtained as the product of a direct movement by a reflection with respect to a plane or by an inversion with respect to a point.
1.B. Some combinations of movements Only those combinations of movements explicitly mentioned in this book will be considered (for further insight, the reader is referred to the splendid book by Lockwood and ~acMillan[~I). The stated laws may be interpreted
1
37
38
1
Carmelo Giacovazzo
Fig. 1.B.1. (a) Composition of two reflections; (b) composition of two rotations about parallel axes; (c) composition of two rotations, the first through cuand the second through a,about parallel axes; (d) composition of two rotations about axes passing through a point.
in terms of combinations of symmetry operations if all the space is invariant with respect to the movements. 1. Composition of two reflections. In Fig. l.B.l(a) the two reflection planes m, and m, are at a dihedral angle a and intersect along a line, the trace of which is in 0 . The image of OQ with respect to m, is OQ1 and the image of OQ, with respect to m, is OQ,. It is possible to superpose OQ to OQ, by a rotation of 2 a around the axis through 0 . We may conclude that the product of the two reflections is a rotation of 2 a around 0 ; in symbols mlm2 = R. The product is not commutative (m,m, # m,m,): in fact by first reflecting OQ with respect to m, and then reflecting the image with respect to m, we obtain a 2 a rotation in the opposite direction. 2. The Silvester theorem relative to three parallel rotation axes. The traces of the three axes on the plane of Fig. l.B.l(b) are A, B, C. The Silvester theorem states that consecutive anticlockwise rotations of 2a, 2P, 2y around A, B, C respectively produce the identity. In fact, because of point 1, the rotations are equivalent to reflection operations with respect to the three pairs of planes ACAB, BABC, CBCA respectively and all these reflections cancel each other out. Since a P y = n, two successive rotations of 2 a and 2P around A and B respectively, will be equivalent to a rotation of +(2a 2P) around C. When a = P, the third axis goes to infinity and the resulting movement is a translation.
+ +
+
Symmetry in crystals
In Fig. l.B.l(c) AC moves to AB by a rotation of a around A; by a a rotation around B BA goes to BD. The resulting movement brings AC to BD and can be achieved by a translation of DA = 2AB sin (a12) perpendicular to the direction of the rotation axes and at an angle of ( n  a)/2 with respect to AB. In symbols: R,RI_,=T. We can then deduce the following point 3. 3. A rotation and a translation perpendicular to the rotation axis combine in a resulting rotation movement around an axis parallel to the original axis. 4. The Silvester theorem relative to three rotation axes passing through a point. In Fig. l.B.l(d) ABC is a spherical triangle with angles a , P, y in A, B, C respectively. If A, B, C are in a clockwise order, rotations of 2a, 2P, 2y around A, B, C leave the figure unchanged. In fact, because of point 1, the three rotations correspond to the products of the reflections with respect to the pairs of planes AOCAOB, AOBBOC, BOCCOA respectively, and these reflections cancel each other out. Since a + p + y > n, then consecutive rotations of 2 a around A and of 2P around B are equivalent to a rotation of 2y around C, with 2y # (2a 2P). 5. Coexistence of rotation axes passing through a point: the Euler theorem. We will study this problem using the Silvester theorem treated in point 4. In Fig. l.B.l(d) let OA and OB be two symmetry rotation axes of order m and n respectively. The angles a and P are chosen in such a way that 2 a = 2n/m and 2P = 2nln. Because of the Silvester theorem, anticlockwise rotations of 2 a and 2P around OA and OB are equivalent to a 2y anticlockwise rotation around OC. C is therefore a symmetry axis of order p = 2nI2y = nly. The angles of the spherical triangle are then nlm, n l n and nlp. Since the sum of the angles must be greater than n, the inequality l l m l l n l l p > 1 follows. The possible solutions of this inequality are: 1, 2, 2 with 1 integer >1; 2, 3, 3; 4, 3, 2; 5, 3, 2. We can now consider the different solutions, keeping in mind that the surface of a sphere of radius r is 4nr2 and that of a spherical triangle is ( a P y  n)r2:
+
+
+
+ +
(a) Solution 1, 2, 2. a , p, and y are equal to n12, n12, n l l respectively and A and B may be chosen on an equatorial circle with C as a pole. The binary axes are therefore always at 90' with respect to the 1 axis. Values of 1 different from 2, 3, 4, 6 correspond to noncrystallographic groups which occur as possible symmetries of molecules or as approximate local site symmetries in crystals. (b) Solution 2, 3, 3. a , p, and y are equal to n12, n13, n13 respectively and the area of the spherical triangle is nr2/6. On the sphere there will be 24 such triangles. The 24 n / 2 angles meet four at a time at six vertices and the 48 n13 angles meet six at a time at eight vertices. This implies the presence of three twofold axes and of four threefold axes. The three twofold axes will be perpendicular one to the other and can be assumed as the axes of a reference system. The four threefold axes run from the centre to the points (1,1, I), (1,  1, I), ( 1,1, I), (1, 1,l). The group of rotations is consistent with the symmetry of a tetrahedron.
(c) Solution 4, 3, 2. a , p, and y are equal to n/2, n13, n14 respectively and the area of the spherical triangle is nr2/12. On the sphere there will
1
39
40
1
Carmelo Giacovazzo
Fig. 1.8.2. Stereographic projections of the 32 crystallographic point groups.
be 48 such triangles. The 48 n / 2 angles meet four at a time at twelve vertices, the 48 n / 3 angles meet six at a time at eight vertices and the 48 n / 4 angles meet eight at a time at six vertices. A total of six twofold axes, of four threefold axes, and of three fourfold axes will be present. The three fourfold axeswill be perpendicular one to the other and can be assumed as the axes of a reference system. The threefold axes are located along the [I, 1,1], [I,  1, 11, [I, 1, 11, [I, 1, 11 directions, while the twofold axes are on the bisecting lines of the angles between the fourfold axes. The group of rotations is consistent with the symmetry of a cube and of an octahedron (see Fig. 1.10). The mutual disposition of the symmetry elements in the 32 crystallographic point groups is illustrated in Fig. 1.B.2, where the so called 'stereographic projections' are shown. The c axis is normal to the plane, the a axis points down the page, and the b axis runs horizontally in the page from left ro right. A stereographic projection is defined as follows (see Fig. l.B.3(a)). A unit sphere is described around the crystal in C. A point P (terminal of some symmetry axis) in the $ 2 hemisphere is defined in the ( x , y ) plane as intersection P' of that plane with the line
Symmetry in crystals
1
41
connecting the point with the south pole of the unit sphere. If the point to be projected is in the 2 hemisphere then the north pole is used. In Fig. l.B.3(b) parts of the stereographic projections for m3m are magnified in order to make clearer the statements made in the text. (d) Solution 5, 3, 2. This solution, which is compatible with the symmetry of the regular icosahedron (20 faces, 12 vertices) and its dual, the regular pentagondodecahedron, (12 faces, 20 vertices), but not with the periodicity property of crystals, will not be examined. It is however of particular importance in Crystallography as symmetry of viruses molecules and in quasicrystals.
poie
6. Composition of two glide planes. In Fig. 1.B.4 let S and S' be the traces of two glide planes forming an angle a and 0 be the trace of their intersection line. The translational components OA and OB are chosen to lie on the plane of the drawing and Q is the meeting point of the axes of the OA and OB segments. X, Y, and Q' are the reflection images of Q with respect to S, S', and to the point 0, respectively. The product S'S moves Q to Q' and then back to Q. Since S'S is a direct movement it leaves Q unchanged and corresponds to a rotation around an axis normal to the plane of the figure and passing through Q. Since S'S moves first A to 0 and then to B, the rotation angle AQB = 2a. Note that the two glides are equivalent to a rotation around an axis not passing along the intersection line of S and S'. 7. Composition of two twofold axes, with and without translational component. From point 5 we know that the coexistence of two orthogonal twofold axes passing by 0 , implies a third binary axis perpendicular to them and also passing through 0 (see Fig. l.B.5(a)). The reader can easily verify the following conclusions: (a) if one of the two axes is 2, (Fig. l.BS(b)), then another 2 axis, at 114 from 0 and intersecting orthogonally the screw axis, will exist; (b) if two 21 intersect in 0 (Fig. l.B.5(c)), then another 2 axis perpendicular to them and passing at (114,114) from 0 will be present; (c) if a pair of mutually perpendicular 2 axes is separated by 114 of a period (Fig. l.BS(d)), then a 2, axis orthogonally intersecting both axes will exist; (d) if a 2 and a 2, axis are separated by 114 of a period (Fig. l.B.5(e)) there will then be a new 2, axis normal to both of them and intersecting the first 2, axis at 114 froin the 2 axis;
Fig. 1.8.3. (a) Geometry of the stereographic projection. (b) Angular values occurring in m3m stereographic projection.
(e) if two orthogonal screws are separated by 114 of a period (Fig. l.B.5(f)), then a third screw axis normal to them and passing at (114,114) from them will be present.
1.C. WignerSeitz cells The 14 Bravais lattices are compatible with cells which are different from those conventionally associated to them. A conventional cell is a parallelepiped: as such it may be considered as a particular type of polyhedron. There are several families of polyhedra with which we can fill up the space
Fig. 1.8.4. Composition of two glide planes.
42
1
Carmelo Giacovazzo
Fig. 1.8.5. Various arrangements of three orthogonal binary axes. The length of the graphical symbol for screw axes i n the plane of the page corresponds t o half repetition period.
by translation. A very important type is the one obtained through the Dirichlet construction. Each lattice point is connected with a line to its nearest neighbours. We then trace through the midpoints of the segments the planes perpendicular to them. These intersecting planes will delimit a region of the space which is called called the Dirichlet region or WignerSeitz cell. An example in two dimensions is given in Fig. l.C.l(a) and two threedimensional examples are illustrated in Fig. 1.C. l(b, c) . The WignerSeitz cell is always primitive and coincides with the Bravais cell if this is rectangular and primitive. A construction identical to the WignerSeitz cell delimits in the reciprocal space (cf. Chapters 2 and 3) a cell conventionally known as the first Brillouin zone. There will be 14 first Brillouin zones corresponding to the 14 Bravais lattices. We recall here that to a lattice I in direct space corresponds an F lattice in reciprocal space and vice versa (see Appendix 2.D); then, the first Brillouin zone of an I lattice will look like a WignerSeitz cell of an F lattice and vice versa. The Brillouin zones are very important in the study of lattice dynamics and in electronic band theory.
Fig. 1.C.1. Examples of WignerSeitz cells.
Symmetry in crystals
1.D. The spacegroup matrices All the rotation matrices R needed to conventionally describe all 230 space groups will be listed. They operate according to the relation X' = RX. The matrices are grouped following the directions along which they operate, and for the hexagonal and trigonal systems they are preceded by the letter H. They may be constructed using the following practical criterion: in the first, second, and third columns are the coordinates of the points symmetry related to points (1,0, O), (0,1, O), and (0,0,1) respectively. The determinant of a matrix will have a +1 or a 1 value depending on whether the represented operation is of rotation or of inversion type. This number, together with the trace (sum of the diagonal elements) of a matrix, are characteristic of the symmetry element: element 1234612346, trace 3 i 0 1 2 3 1 0 1 2 , determinant l l l l l i i i i i . The matrix of the fi operator may be simply obtained from that of the n operator by multiplying by the matrix corresponding to the i operator: 0 i = ( i 1o 1
:).
This corresponds to changing the sign of all the elements of the original matrix. Therefore in the following list we will not give all the 64 matrices necessary to describe the space groups, but only the 32 matrices corresponding to proper symmetry elements. Direction [0 0 01
Direction [I 0 01 2
(~ 0 0 ° 1) o o i
( 1 )
0H 2 = 0 1 0
o o i
4
0)
( l o O); ( l o ~ 0 0 14 3 = O 0 1 . o I 0' 0 1 0
Direction [0 1 01 2 =( i0 o10 O) ;
o o i
); H 2 =O 1 O1 O) ; 3 =( O 0 O1 i O
o o i
l o o
(yg;)
4 3 = 0 1 0 .
Direction [0 0 11
i o o
1 1 0
o i o
1
43
44
1
Carmelo Giacovazzo
Direction [ l 1 01
Direction [l 0 11 0 0 1
Direction [0 1 11
Direction [l
i 01
Direction [ i 0 11
Direction [0 1 I]
Direction [I 1 11 0 0 1
0
1 0
o i
0
o o i
l o o
o i o
Direction [I1 11
Direction [l
i 11
Symmetry in crystals Direction [I 1 ?I 3
( ~
0
0); 0 13
T o o
(O O T ) 2 ' 1 0 0 . 0 i 0
Direction [2 1 0]
Direction [ l 2 01.
1.E. Symmetry groups A group G is a set of elements g,, g2, . . . g,, . . . for which a combination law is defined, with the following four properties: closure, the combination of two elements of the group is an element of the group gigj =gk; associativity, the associative law (gigj)gk= gi(gjgk) is valid; identity, there is only one element e in the group such that eg = ge = g; inversion, each element g in the group has one and only one inverse element g' such that glg = ggl = e. Examples of groups are: (1) the set of all integer numbers (positive, negative, and zero), when the combination law is the sum. In this case e = 0, g' = g; (2) the rational numbers, excluding zero, when the law is the product: e = 1, g  l = l/g; (3) the set of all n x n sonsingular matrices under the product law: e is the diagonal matrix with aii = 1;
+ +
(4) the set of all lattice vectors r,,,,, = ua vb wc with u, v, w positive, negative, or null integers, when the combination law is the vector sum: gl = g. then e = g,,,,, The number of different elements of a group is called the order of the group and can be finite or infinite. If a group also possesses the commutative property gigj=gigi for any i and j, then G is said to be Abelian. With reference to the examples given above, (I), (2), (4) are infinite and Abelian groups, (3) is infinite and nonAbelian. If g is an element of G, all powers of g must be contained in G. An integer n may exist for which then gn+'= g, gn+2= g2, . . , If n is the smallest integer for which (l.E.l) is satisfied, there will only be n distinct powers of g. Since gJgnj= gnjgi = e, then gnj is the inverse of gi. The element g is then said to be of order n and
1
45
46
1
Carmelo Giacovazzo Table 1.E.1. List of generators for noncyclic point groups. There are 2 1 proper generators in all Point group
Generators
Point group
2/m 222 rnrn2 rnrnrn
4oro1, 2roio1 2 ~ 1 0 0 1210101 ~
Jrn 62rn 622 6/m
2[1001' 210011
2110011 ~ 1 0 1 0 1 ~
Generators
210011 422 4/ rn 4rn rn 42rn 4Jrnrnrn
~ [ ~ o o 3I , 1 i o ~ 4100111?[0011 ~ [ I O O I ~2 [ i i o 1 T r r o o i ~2 [ i i o 1 ?[looit 4 i i o i
210011
32 3rn
3 1 o o i 1Triooi ~ 310011~ 21ioo~
the set of all powers of g is a group of order n: G I = (g, g 2 , . . . , gnl, gn = e). A group, such as (1.E.2), in which all the elements are powers of a single generating element, is called cyclic. All cyclic groups are Abelian, but the converse is not true. An example of cyclic group of order n is the set of rotations around a given axis, which are multiple of an angle a = 2nln. Any point group can be represented as the product of powers of at most three elements, which are the generators of the group. In Table l . E . l the list of the generators of the noncyclic groups is reported. We also note that the definition of the generators is not unique. For instance in the class 222 we may chose the generators 2[,ooland 2[olo1,or 2,,,] and 2[00,1,or 210101 and ~[ooI]. When the physical properties of the group elements are not specified the group is said to be abstract. From a mathematical point of view all its properties are determined by its multiplication table. For a group of n elements this table has the form:
We note that 1. Each element appears once and only once in a given row (or column) of the table. In order to demonstrate this statement let us consider the ith row of the table and suppose that there are two different elements gj and gk, for which gigj = gigk = g,. Then g, would appear twice in the row, but by multiplying the two equations by g;' we obtain g, = g,, in contrast with the hypothesis. 2. Each row (column) is different from any other row (column); this property follows immediately from property 1. 3. For abelian groups the table is symmetric with respect to the diagonal.
Symmetry in crystals Table 1.E.2. The 18 abstract groups corresponding to the 32 crystallographic point groups Point group
Order of the group
Characteristic relations
1
i,2, m 3 4.4 2/m, mm2, 222 6, 6, 3 32.3m mmm 4/m 4mm, 422.42m g/m 3m, 62m, 6mm, 622 23 4/mmm 432.43m m3 6/mmm m3m Groups having the same multiplication table, even though their elements might have different physical meaning, are called isomorphous. They must have the same order and may be considered as generated from the same abstract group. For instance the three point groups 222, 2/m and mm2 are isomorphous. To show this let us choose g,, g,, g3, g4 in the following way. group 222: 1, 2, 2, 2; group 2/m; 1, 2, m, i; group mm2; 1, m, m, 2. The multiplication table of the abstract group is
In Table 1.E.2 the 32 crystallographic point groups are grouped into 18 abstract groups and for each of them the defining relationships are listed. We note that all cyclic groups of the same order are isomorphous.
Subgroups A set H of elements of the group G satisfying the group conditions is called a subgroup of G. The subgroup H is proper if there are symmetry operations of G not contained in H. Examples of subgroups are: (1) the set of even integers (including zero) under the sum law is a subgroup of the group of all integers; (2) the point group 32 has elements g, = 1, g2 = 310011,g3 = 3, = 3l, g4 = 2[1m1,g5 = 2[0101,g6 = 2[iio1;H = (gl, g2, g3) is a subgroup of G;
1
47
48
1
Carmelo Giacovazzo
(3) the point groups 1, 2, I, m are subgroups of the point group 2/m;
(4) 222 is a subgroup of 422; (5) the set T of all primitive lattice translations is a subgroup of the space group G. Conversely G may be considered a supergroup of H. Subgroupgroupsupergroup relationships are very important in the study of phase transitions and of orderdisorder problems.
Cosets Let H = (h,, h2, . . .) be a subgroup of G and gi an element of G not contained in H. Then the products giH = (gihl, g h ,
. . .) and Hgi = (hlgi, h2gi, . . .)
form a left and a right coset of H respectively. In general they will not be identical. Furthermore H can not have any common element with giH or Hgi. In fact, if for instance, we had gihi = hk, it would follow that gi = hkhjl, i.e. contradicting the hypothesis, gi would belong to H. It can be shown that two right (or left) cosets, either have no common element or are identical one to the other. This allows us to decompose G with respect to H in the following way:
It follows that the order of a subgroup is a divisor of the order of the group and if this is a prime number, the only subgroup of G is e and G must also be cyclic. The decomposition of the group 2/m into separate left cosets with respect to the subgroup 2 is: The number of distinct cosets obtained from the decomposition of a group with respect to a subgroup is called index of the subgroup. In the previous example, the index of the subgroup 2 of the group 2/m is two. A coset is never a group because it does not contain the element e.
Conjugate classes An element gi is said to be conjugate to an element gj of G if G contains an element gk such that gi = gklgjgk.
(1.E.5)
If g, is fixed and gk varies within G, then the set of elements gi forms a class of conjugate elements.
In agreement with relation (1.E.5) the element e forms a class on its own. Since each element of G can not belong to two different classes, it is possible to decompose G into the factorized set G = e U T, U T2 U . . . . A physical or geometrical meaning may be attributed to the classes. In
Symmetry in crystals the transformation (1.E.5), let the element g, be a coordinate transformation due to a symmetry operator and the element gj a matrix operator related to another symmetry operation. Since g, is transformed by (1.E.5) (see eqn (2.E.7)), the operators belonging to the same class are changed one onto the other by coordinate transformations represented by the elements of the group. For instance, for the point group 32 three classes may be set up: (el, (3,3'), (2[iool,~ [ o I D2~iiol.I ], As we will see later, the character is identical for the matrix representation of all the elements of the same class. The following rules may be useful to set up the pointgroup classes: the classes are formed by one element only for the point groups up to orthorhombic; this means that each symmetry operator commutes with all the others; in an Abelian group the classes are formed by only one element; the operators identity, inversion, and reflection with respect to a mirror plane perpendicular to the principal symmetry axis (the axis with the highest order), are each in a separate class.
Conjugate subgroups Let H be a subgroup of G and g an element of G not in H. Then all the elements g  l ~ g ,form a group. H and glHg are conjugate subgroups.
Normal subgroups and factor groups If the right and left cosets of the subgroup H are the same, i.e. Hg, =g,H for every i, then g;'Hg, = H. This relation is still valid when g, is in H since both g,H and g, belong to H. Conversely, if a subgroup is transformed into itself when applying all the elements of the group, the corresponding left and right cosets must be equal. Subgroups which are transformed into themselves by applying all the elements of the group, are called invariant or normal. They must contain complete classes. For instance the subgroup 2 of the point group 2/m is normal since 1(1,2) = (1,2)i, m(1, 2) = (1, 2)m. Furthermore, in the group 32, the subgroup (1,3,3') is normal, while (1,2i1,1) is not; the subgroup T of all the primitive lattice translations is an invariant subgroup of the space group G. Let H be a normal subgroup of G with index p, while n is the order of G. Because of (1.E.4) the order of H is n/p. We observe that for H and all its distinct cosets, the following multiplication law may be established: (g,H&H) = giHHgj = giHgj = g,&H Besides, it is: (g,H)'(gi~)= H'~&H = el
We can now define a new type of group of order p, called a factor group or quotient group, indicated by the symbol G/H: its elements are cosets of
1
49
50
1
Carmelo Giacovazzo
H. The following multiplication table is for the quotient group (we assume = e).
rrl
For instance, for the quotient group (2/m)/2, (1.E.6) becomes
As a further example let us consider the elements of the point group 4mm: e, 4, 43, q2 = 2, Z[lool,2[olol,Z[llol, Z[liol.Five classes may be formed: (e), (21, (4, 43), (Z[iool,Z[oio]), (Z[iio172[iiol). The subgroup H = (e, 2) is invariant and the factor group with respect to H may be written as: H, 4H, Z[100]H7Z[llop. The relat~onbetween G and G / H is a n / p + 1 correspondence, i.e. G , H. In detail glH = H , e, g2H ,f,, . . . , g,H + fp. A correspondence of this type (many + one) is called homomorphism and G / H is said to be homomorphic with G. Isomorphism is then a special case of homomorphism for which there is a one to one correspondence. A homomorphic correspondence allows us to reduce the study of the multiplication laws of the group G to that of the multiplication laws of the smaller G / H group. To display many of the abstract definitions given so far, we consider as major example, the point group G = 23: say
Readers will find the four classes:
and the ten subgroups
2[,11), and G are invariant subgroups. of which only {I), (1, 211,1, 2[olo17 2[ooll): we Calculate now the factored group of H = (1, 211,1, 210101, multiply it by an element not in H, say 3[1111,and obtain We take now an element not in H or in 3[llllH, say 3flll], and we get
Symmetry in crystals
The group is now exhausted and we may write On assuming g1 = e, then {e, 3[1111H,3fl11]H) form a group under the following multiplication table
This group is homomorphic with G itself if we associate the elements in H to e, the elements in 3[111]H with the 'element' 3[,l11H, the elements in 3elllH with the 'element' 3tl11]~.
Maximal subgroups and minimal supergroups The number of subgroups of a space group is always infinite. They may bp the sitesymmetry groups (groups without a lattice), or line groups, ribbon groups, rod groups, plane groups, or space groups. For example, the set T of all the primitive lattice translations is a subgroup (invariant) of the space group. Further subgroups may be found by considering the set of all the translations defined by a superlattice. We are here interested only in subgroups which are space groups themselves. Let us first recall the concept of proper subgroup. A subgroup H is called proper subgroup of a group G if there are symmetry operations of G not contained in H. Now we define maximal subgroups: a subgroup H of a space group G is called a maximal subgroup of G if there is no proper subgroup M of G such that H is a proper subgroup of M. For example, P112,, P1211, P2,ll are maximal subgroups of P212121, while P1 is not maximal. For every H, according to (1.E.4), a right coset decomposition of G relative to H may be made. The index of the decomposition determines the degree of 'dilution' of the symmetry in H with respect to that in G. Such a dilution may be obtained in three different ways: 1. By eliminating some symmetry operators (e.g., from G = P212121 to H = P2,ll). Subgroups of this kind, are called Translationengleiche or t subgroups. Since the point group P of G is finite, the number of subgroups, and therefore, of maximal subgroups, is finite. All the maximal subgroups of type t for any given G are listed in the Znternational ~ a b l e sas type I maximal nonisomorphous subgroups (see Figs 1.20 and 1.21). 2. By loss of translational symmetry, i.e. by thipning out the lattice. Such subgroups are called Klassengleiche or k subgroups and are classified as type 11. A subset of k subgroups are those belonging to the same space group G or to its enantiomorphic: their number is infinite and they are called maximal isomorphous subgroups. Those of lowest index are listed as IIc in the International Tables. For example, if G = (2222, maximal isomorphous subgroups of lowest index are C222 with a' = 3a or b' = 3b and C222 with c' = 2c. Maximal nonisomorphous subgroups of C222 are also P222, P2J12, P2,22, P2212, P222,, which have the same conventional cell: for practice1
1
51
52
1
Carmelo Giacovazzo
reasons they are labelled as subgroups of type IIa. Space groups with primitive cells have no entry in the block IZa. Some further subgroups of C222 are C222, (with c' = 2c), I222 (with c' = 2c) and I2,2,2, (with c' = 2c). These subgroups have conventional cells larger than that of C222 and are denoted as subgroups of type IIb. For k subgroups the point group P of G is unchanged.
3. By combination of 1 and 2. In this case both the translation group T and the point group P of G are changed. A theorem by Hermann states that a maximal subgroup of G is either a t subgroup or a k subgroup. Thus in the International Tables only I, IIa, IIb, and IIc subgroups are listed. Sometimes we are interested to the possible space groups G' of which a given space group G is a subgroup. G' is called a minimal supergroup of the group G if G is a maximal subgroup of G'. Of course we will have a minimal t, or a minimal nonisomorphous k, or a minimal isomorphous k supergroup G ' of G according to whether G is a maximal t, or a maximal nonisomorphous k, or a maximal isomorphous k subgroup of G'. The minimal nonisomorphous supergroups of C222 are: of type t: of type k:
Cmmm, Cccm, Cmma, Ccca, P422, P42,2, P4,22, P42,2, ~ 4 r n 2~, 4 ~~ 24 b, 2 ~, 4 n 2 P622, , P6,22, P6,22, F222, P222 (with a ' = a/2, b' = b/2).
Maximal subgroups and minimal supergroups for threedimensional crystallographic point groups With trivial changes the definitions of maximal subgroup and minimal supergroup given above for space groups may be applied to threedimensional crystallographic point groups. For example, it will be easily seen that Laue symmetry is always a minimal supergroup of index 2 of a noncentrosymmetric point group. A scheme showing the subgroup and supergroup relationships for point groups is illustrated in Fig. 1.E.1. Maximal invariant subgroups are indicated by full lines: if two or three maximal invariant subgroups exist with the same symbol then double or triple full lines are used. A set of maximal conjugate subgroups is referred to by a broken line. For example, from 3m three conjugate subgroups of type m can be formed. Thus a dashed line refers 3m to m. Furthermore, from 422 two invariant subgroups of type 222 with index 2 can be formed (no symmetry operation of 422 refers one subgroup to the other). Thus in Fig. l.E.l a double solid line refers 422 to 222.
Limiting groups in two and three dimensions In two dimensions there are two types of point groups:
For very large values of the order of the rotation axis the two types approach w and am respectively. From the geometrical point of view w and wm are identical, and our standard notation will be wm (the situation
Symmetry in crystals
Fig. 1.E.1. Group, subgroup, supergroup relationships for point groups (from International Tables for Crystallography).
a,# a m occurs when the rotation direction is taken into account: i.e. for a magnetic field round a disc). In three dimensions a point group can include continuous rotations about one or about all axes (this is a consequence of the Euler theorem applied to such a limiting case). In the first case two groups can be identified, wm and w 2 , according to whether there is or not a mirror perpendicular to a, axis mm (the symmetry of the two groups can be represented by a circular cone and
w m
by a circular cylinder respectively). The symbol  represents the case in mm which continuous rotation about any axis is allowed (the symmetry is represented by a sphere).
Representation of a group If a square matrix d can be associated to each g E G , in such a way that when gigj = g k also didj = d,, then the matrices form a group D isomorphous with G. These matrices form an isomorphous or exact representation of the group: the order n of the matrices is the dimension of the representation. In accordance with this point of view, in Chapter 1 we have represented the symmetry groups through square matrices of order 3. Different representations of G may be obtained through a transformation of the type When condition (1.E.7) is verified for the two representations rl(d,, d 2 , . . .) and r2(dI, d;, . . .) then the two representations are said to be equivalent, since q can be interpreted as a change of coordinate system. It is often possible to find a new coordinate system for which each matrix d
1
53
54
1
Carmelo Giacovazzo is transformed into
with dl of order m < n and d2 of order (n  m). If this can not be obtained by any transformation, then the representation is called irreducible; otherwise it is called reducible. Sometimes dl and d2 can be further reduced, and at the end of the process each matrix d j will be transformed into qld,q = diag [djl), dj2), . . . , d,(")]= d,' where dji) are themselves matrices. The matrices dl1), dp), dill, . . . all have the same dimension. Similarly dl2),di2),di2),. . . have the same dimension. From the rule of the product of blocked matrices it follows that (dl1),d$'), dS1),. . .) form a'representation of the group, as well as (dl2),ds2),dS2),. . .), etc. It can be shown that for finite groups the number of irreducible representations is equal to the number of classes. For instance an isomorphous (reducible) representation of the point group 32 is
Also the twodimensional irreducible representation
and the onedimensional nonexact (homomorphic) representations exist:
Character tables The sum of the diagonal elements of a matrix, elsewhere called trace, in group theory is called character and is indicated by ~ ( g It) is obvious that ~ ( g , )defines the dimensionality of the representation. The complete set of characters for a given representation is called the character of the
Symmetry in crystals
1
55
representation. Since the traces of two matrices related by a coordinate transformation are identical, the characters of two equivalent representations will be identical (the converse is also true). Several properties of a point group may be deduced from the characters of its irreducible representations alone. It is therefore convenient to set them up in tables called character tables. Each row of the table refers to a particular irreducible representation and each column to a given class.
1.F. Symmetry generalization Only a few intuitive elements of this subject are given, since a full treatment would exceed the limits of the present book. The reader is referred to specific texts or
The symmetry groups G: A space may or may not be periodic in all its m dimensions. The corresponding symmetry groups are indicated by GT, with m 3 n, where n is the number of dimensions of the subspace in which the group is periodic. In this space only symmetry operations transforming the space into itself will be allowed. For instance in the G: groups, describing objects periodic in one direction and finite in the other two, at least one line will remain invariant with respect to all symmetry operations.
The G1 groups 1. Gh groups. In a onedimensional space (a line), which is nonperiodic, only two symmetry operators are conceivable: 1 and ? (which is the reflection operator m). The only two (point) groups are therefore 1 and I.
2. G: groups. Besides the 1 and ? operators, they contain the translation operator. Only two groups of type G: are then possible.
The G2 groups 1. G?, groups. In a 'twodimensional space (a plane), which is nonperiodic, the only conceivable operators are those of rotation around an axis perpendicular to the plane and of reflection with respect to a line on the plane. The number of (point) groups is infinite, but there are only ten crystallographic groups (see p. 16). 2. ~f (border) groups. In a twodimensional space, periodic in one dimension, only the symmetry operators (and their combinations), which transform that direction into itself, are allowed. We may therefore consider reflection planes parallel or perpendicular to the invariant direction, glides with translational component parallel to it and twofold axes. There are seven Gf groups (the symmetries of linear decorations) which are represented in Fig. 1.F.1.
3. G$ groups. There are the 17 plane groups described on the pages 30 and 34.
t
aat:2
           t.a 1   +    I t.m ++++t:zm IIt:m Fig. 1.F.l. The seven border groups
at:2,a
56
1
Carmelo Giacovazzo
The G3 groups 1. G; groups. There describe nonperiodic spaces in three dimensions. The number of (point) groups is infinite (see Appendix l.B), but there are only 32 crystallographic point groups (see pp. 1116). 2. G: (rod) groups. Rod groups may be considered as arising from the combination of onedimensional translation groups with point groups G;. They describe threedimensional objects which are periodic in only one direction (say z). This must remain invariant with respect to all symmetry operations. The only allowed operations are therefore n and ri axes coinciding with z, 2 and 3 axes perpendicular to it, screw axes and glide planes with a translational component parallel to the invariant direction. There are 75 G: crystallographic groups. In Table l.F.l the rod group symbols are shown alongside the point groups from which they are derived. The first position in the symbol indicates the axis (n or ri) along z, the
Table 1.F.1. The 75 rod groups Point group
Rod groups
1 2 3 4 6 Im 2mm 3117 4m m 6mm m 2/m 4/m 6/m m2m 2 2 2 mmm 4 2 2 rnrnrn 6 2 2 mmm 12 222 32 422 622 1
1 2 3 4 6 Im 2mm 3m 4mm 6m m m 2/m 4/m 61m m2m 2 2 2 mmm 4 2 2 mmm 6 2 2 mmm 12 222 32 422 622 1
3
3 4
6  2 1m  2 3m 4m2 6m2
6
4
1 2
m  2 3m 4m2 6m2
21 31 41 61 Ic 2,mc 3c 4,mc 6,mc 2,/m 421m 6,/m m2c 2, 2 2 mmc 4 , 22 mmc 6, 2 2 mmc 2,22 312 4,22 6,22
2 1C
2
3C
4c2 6c2
Symmetry in crystals
second position refers to axes (n or i i ) in the plane (x, y) normal to the invariant direction, the third position for axes in the (x, y) plane bisecting the previous ones. Glides in the z direction are denoted by c. 3. G: groups. There are called layer groups and d e s ~ r i b e [ ~ , ~the ,~~,'~] symmetries of doubly periodic threedimensional objects. They are useful in describing the patterns of walls, panels, and, at an atomic level, in describing structures with layer molecular units. Let us denote by z the direction perpendicular to the layer plane. It will be the vertical axis from now on: directions in the plane will be called horizontal. Rotations can only occur about a vertical axis, and if twofold, also about a horizontal one. No more than one horizontal reflection plane can exist, otherwise translational symmetry should also occur along the z axis. The layer groups can be enumerated according to the five nets quoted in Table 1.7 for the plane lattices. In Table 1.F.2 the 80 layer groups are divided in blocks, each block divided by the subsequent by a double line: each block refers to a specific net (in sequence, parallelogram, rectangular, centred rectangular, square, hexagonal) and contains the point groups compatible with the net and the corresponding layer groups. The number of point groups which can be used is 31: the 32 threedimensional point groups minus the five incompatible groups 23, m3, 432, 43m, m3m plus four second settings (this time the z axis is distinguishable from x and y: so 2 is different from 12, or 2/m from ?2/m, . . .). The first position in the layer group symbol gives the type of cell, the second refers to the z direction. The third and fourth positions refer: (a) for rectangular nets, to x and y respectively; (b) for a square net, to x (and therefore to y) and to a diagonal direction; (c) for a hexagonal net, to x (and therefore symmetry related axes) and to diagonals directions. As subgroups of the G; groups we may consider the G: groups, which are obtained by projecting the Gq groups along the axis normal to the singular plane. 4. G: groups. These are the 230 space groups (see pp. 2230).
The 64,groups The threedimensional Euclidean space may be insufficient to describe the symmetries of some physical objects. We can therefore introduce one or more additional continuous variables (e.g. the time, the phase of a wave function, etc.), thus passing from a threedimensional space into a space with dimensions m > 3. In a fourdimensional Euclidean space the symmetry groups G: may be constructed from their threedimensional projections G:, which are all well known. Thus there are 227 point groups G: and 4895 groups Gi.
The groups of colour symmetry Groups in which three variables have a geometrical meaning while the fourth has a different physical meaning and is not continuous, are
1
57
58
1
Carmelo Giacovazzo Table 1.F.2. The layer groups Point group
Plane groups
1 2 rn 1
P1 P2 prn p2/m P1
1rn
plm
plb
2rnrn
p2rnm
p2bm
p2ba
rn2m
prn2rn pn2,m
pm2,a pn2a
pa2,m pb2rn
2 2 2 
2 2 2 Pl 222 22,2, Pmmm rnbrn 222 22,2 p2  2A2 p22  l2L brnm bm a P b b i Pbba22121 p22,2 PP,b2a2 2 nrnm nbm
Tim
mrnm
1rn 2mm m2m 2 2 2 mmm 12 222  2 1m
c l rn c,mrn cm2m 2 2 2 Cmmm c12 c222  2 clrn
4 4m rn 41rn 4 2 2 mmrn
P4 p4mm p4m/m 4 2 2 Pmmm P4 ~ 2 2 p4m2
Pb p2/b
pa2a pb2,a

4
422 4m2
p4grn p4/n 2 2 42,2 422 p 4A r n g m Pr n g m Pngm ~ 4 2 ~ 2 p4g2 p42rn
p42,rn
Symmetry in crystals
1
59
particularly important in crystallography. For instance: 1. The position and orientation of the magnetic moments of the cobalt atoms in the CoA1204structure (space group ~ d 3 m may ) be described by means of a twocolour group (see Fig. l.F.2(a)) in which each colour corresponds to a given polarity of the magnetic moment. Groups of this type are also called 'groups with antisymmetry' or 'blackwhite' symmetry. More complicated cases require more colours, and the term colour symmetry is used. Classical groups involve only neutral points. As a further example let us consider the case of NiO, a material used in the ceramic and electronic industries. At room temperature, NiO is rhombohedral with edge length a , 2.952 A and a~ =. 60'4': aR approaches 60" with increasing temperature, and, above 250°C, NiO is cubic with ac2: 4.177 A. The relation between the two cells is shown in Fig. l.F.2(b): the same set of lattice points is described by the primitive rhombohedral unit cell and by the facecentred cubic cell provided that aR= 60' exactly and a R = a/*. If the cube is compressed (or extended) along one of the four threefold axes of the cubic unit cell then symmetry reduces from cubic to rhombohedral (the only threefold axis is the compression axis). The polymorphism of NiO is due to its magnetic properties. Each Ni2+ ion has two unpaired spins (the [Ar]3d8 electronic configuration). At room temperature the spins in NiO form an ordered antiferromagnetic array: layers of Ni2+ with net spin magnetic moments all in the same direction alternate with layers of Ni2+ with magnetic moments all in the opposite direction, as in Fig. l.F.2(c). In these conditions the threefold axis is unique and the structure is rhombohedral. Above 250°C the antiferromagneti~ordering is lost: the rhombohedral + cubic transition occurs and NiO displays ordinary paramagnetism.

2. If we project a G: group, in which a 6, axis is present, on a plane perpendicular to the axis, we obtain a G; group. But, if we assign a different colour to each of the six atoms related by the 6, axis, we will obtain a colour group G;,@)with a clear meaning of the symbols. In the groups with antisymmetry there will be four types of equivalence between geometrically related objects: identity, identity after an inversion operation, antiidentity (the two objects differ only in the colour), identity after both an inversion operation and a change in colour. A general rotation matrix may be written in the form
\ O 0 0 R44/ where R4, = 1 or +1 depending on whether or not the operation changes the colour. For the threedimensional groups with antisymmetry we observe that, because of the existence of the antiidentity operation 1' (only the colour is changed), the antitranslation operation t' = t l ' will also exist. New types of Bravais lattices, such as those given in Fig. 1.F.3, will come out. As an example, in Fig. l.F.2(c) the quasicubic magnetic unit cell of NiO has an
Fig. 1.F.2. Examples of structure described by an antisymrnetry group: (a) CoAI,O, magnetic structure; (b) geometrical relation between a facecentered cubic unit cell and a primitive rhombohedral unit cell; (c) antiferromagnetic superstructure of NiO (only ~ i ' +ions are shown).
60
( Carmelo Giacovazzo edge length twice that of the chemical unit cell. It may be seen[14]that if the five Bravais lattices are centred by black and white lattice points (in equal percentage) then five new plane lattices are obtained. In three dimensions there are 36 black and white Bravais lattices, including the traditional uncoloured lattices.
?
fg I
/
b,
9
b
?' Fig. 1.F.3. Two antisymmetrical Bravais lattices.
References 1. Shubnikov, A. V. (1960). Krystallografiya, 5, 489. 2. Shubnikov, A. V. and Belov, N. V. (1964). Coloured symmetry. Pergamon, Oxford. 3. Bradley, C. J. and Cracknell, A. P. (1972). The mathematical theory of symmetry in solids. Representation theory for point groups and space groups. Clarendon Press, Oxford. 4. Lockwood, E. H. and MacMillan, R. H . (1978). Geometric symmetry. Cambridge University Press. 5. Vainshtein, B. K. (1981). Modern crystallography I: Symmetry of crystals, methods of structural crystallography. Springer, Berlin. 6. (1983). International tables for crystallography, Vol. A, Space group symmetry. Reidel, Dordrecht. 7. Dougherty, J . P. and Kurtz, S. K. (1976). Journal of Applied Crystallography, 9, 145. 8. Kitaigorodskij, A. I. (1955). Organic crystallochemistry. Moscow. 9. Mighell, A. and Rodgers, J. R. (1980). Acta Crystallographica, A36, 321. 10. Wilson, A. J. C. (1988). Acta Crystallographica, A44, 715. 11. Fischer, W., Burzlaff, H, Hellner, E., and Donnay, J. D. M. (1973). Space groups and lattice complexes, NBS Monograph 134. National Bureau of Standards, Washington, D.C. 12. Alexander, E. and Herrmann, K. (1929). Zeitschrift fur Kristallographie, 70, 328. 13. Alexander, E. (1929). Zeitschrift fur Kristallographie, 70, 367. 14. Mackay, A. L. (1957). Acta Cryst., 10, 543.
CARMELO G I A C O V A Z Z O
Introduction In this chapter elements of crystallographic computing are described. Material is treated in order to answer daytoday questions and to provide a basis for reference. Among the various topics, those which are of more frequent use have been selected: axis transformations, geometric calculations (bond angles and distances, torsion angles, principal axes of the quadratic forms, metric considerations on the lattices, structure factors, Fourier calculations,. . .). The method of least squares and its main crystallographic applications are treated in greater detail. For practical reasons some calculations useful in characterization of thermal ellipsoids are developed in Appendix 3.B . The following notation is adopted: rl. r2 denotes the scalar product between the two vectors rl and r2, rl A r2 is their cross product, r will be the modulus of r. S1S2is the (row by columns) product of two matrices S1and S2: S is the transposed matrix of S, and S is the determinant of the square matrix S. We will also distinguish between coordinate matrices and vectors. For example, with respect to a coordinate system [0, a, b, c] the vector r will be written as
where X is the coordinate matrix and A is the matrix which represents the basis vectors of the rectilinear coordinate system.
The metric matrix Let [0, a, b, c] be our coordinate system. The scalar product of r, and r2 is
.
+ zlc) . (x2a + y2b + z2c) =xlx2a2+yly2b2+ zlz2c2+ (x1y2+ x2y1)ab cos y + ( ~ 1 +~ X2 ~ Z ~ )cos L IPC+ ( Y ~+zY~ ~ z ~cos ) ~CY c
rl r2 = (xla + ylb
62
1
Carmelo Giacovazzo
or, in matrix notation,
G is the metric matrix, also called the metric tensor: its elements define both the moduli of a, b, c and the angles between them. The value of its determinant is G = a2b2c2(1 cos2 a  cos2j3  cos2 y
+ 2 cos a cos P cos y)
(2.2) which (see Table 2.1 and p. 69) is equal to V2 (square of the volume of the unit cell). If r, = r2= r then (2.1) becomes r2 = XGX = x2a2+ y2b2+ z2c2+ 2xyab cos y
+ 2xzac cos j3 + 2yzbc cos a
(2.3~)
which gives the modulus square of a vector. We c8n now calculate the following: 1. The interatomic distance d between two atoms positioned in (xl, y,, z,) and (x2y2z2)Denoting A1 = a(xl  x2), A3 = c(zl  22) A2 = b(yl  y2), gives d2 = A: A; A$ + 2A1A2COSY + 2A1A3cos P 2A2A3cos a. (2.3b)
+ +
+
2. The angle 8 between two vectors cos 0 = ~,GX,l(r,r~).
(2.4)
3. The cross product r2 A r3:
4. The scalar triple product rl r2 A r3:
is the volume of the unit cell The following formulae of vector algebra are also recalled for future convenience:
Some properties of the rotation component R of the symmetry operators
.. can now be proved: 1. If a, b, c define a primitive cell, the elements of R are integers. Indeed the relation Xr = RX transforms lattice vectors r into lattice vectors r r . Both r and r r have integer components, consequently also the elements of R must be integers. 2. A symmetry operator does not change the moduli of the vectors and the angles between vectors: i.e. r; ri = r, r2. Therefore, according to (2.1), X;GX; = XlRG~X2= XlGX2, from which
.
Only the matrices R which satisfy (2.9) can be symmetry rotation matrices in the coordinates system defined by G.
3. Multiplying the second eqn (2.9) by R gives GR= W G . If only determinants are taken into consideration then R = f1 arises. Properties 1, 2, 3 can be verified for the rotation matrices quoted in Appendix 1.D.
The reciprocal lattice Very useful in metric calculations (as well as in diffraction geometry), the reciprocal lattice was introduced by P. Ewald in 1921. Let a, b, c be the elementary translations of a space lattice (called here a direct lattice). A second lattice, reciprocal to the first one, is defined by translations a*, b*, c*, which satisfy the following two conditions:
Equation (2.10a) suggests that a* is normal to the plane (b, c), b* to the plane (a, c) and c* to the plane (a, b). The modulus and sense of a*, b*, c* are fixed by (2. lob). According to (2.10a) a* may be written as where p is a constant. The value of p is obtained if the scalar product of both the sides of (2.11) by a is taken: a*.a=l=p(b~c.a)=pV from which p = 1/V. Equation (2.11) and its analogue may then be written as
or, in terms of moduli,
Equation (2.10) also suggest that the roles of direct and reciprocal space may be interchanged: i.e. the reciprocal of the reciprocal lattice is the direct
Crystallographic computing
1
63
64
1
Carmelo Giacovazzo
lattice. Therefore 1 a=,(b*~c*),
v
1 b =  ( c* A a * ) ,
c =
1
v * (a* A b*).
v*
(2.13)
It may be easily verified that the reciprocals of triclinic, monoclinic, . . . lattices are triclinic, monoclinic, . . . themselves. However, the reciprocal of an F lattice is an I lattice and vice versa (see Appendix 2.D). In detail: 1 . In monoclinic lattices b* JJ b while a* and c* are in the plane (a, c): then
a* = l / ( a sin p), a*=y*=n/2,
c* = l l ( c sin P),
b = llb, p*=n/3.
2. In rhombic, tetragonal, and cubic lattices a* )I a, b* (1 b, c* 1) c, and 3. In trigonal and hexagonal lattices c* )I c while a* and b* are in the plane (a, b ) : For the rhombohedrical basis
a* = p* = y * ,
cos a* = COS @ / ( I
+ COS a ) .
Some relations between direct and reciprocal bases are discussed in Appendix 2.A: a summary is given in Table 2.1. Some important properties of the reciprocal lattice are: 1 . The scalar product of two vectors, the first defined with respect to the reciprocal basis and the second to the direct basis, assumes a very simple expression:
Table 2.1. Relationships among direct and reciprocal lattice parameters. Inverse relationships are obtained by interchanging t h e starred by unstarred parameters b* acsinp . V '
a*=.b c s i n a V ' sin a* = sin p* = sin y*
=
v abc sin p sin y ' abc sin a sin y '
v abc sin a sin p '
c*  a b sin y
v
*  cos /3 cos y  cos a
cos a 
sin p sin y
*~cosa~~sycosp cospsin a sin y *~cosacospcosy cosy sin a sin p
V = abc(1  cos2 a  cos2P  cos2 y + 2 cos a cos P cos y)'I2 = abc sin a sin p sin y* = abc sin a sin p* sin y = abc sin a* sin /3 sin y
v* = 1/v
Crystallographic computing
1
65
2. The vector r i = ha* + kb* + lc* is normal to the family of lattice planes (hkl). In Fig. 2.1 the plane of the family nearest to the origin is drawn. In accordance with p. 8 the vectors (A0), (B0) and (C0) are equal to alh, blk and cll respectively. Consequently (BA) = blk  alh,
(CA) = cll  a l h ,
(cB) = cll  blk.
Therefore
.
r i (BA) = (ha* + kb* + lc*) (blk  a l h ) = 0, r ; . (CA) = r ; . (CB) = 0 . Since r i is perpendicular to two lines in the (hkl) plane, it is normal to the plane. Fig. 2.1. The plane of the faniily (hkl) nearest to the origin.
3. If h, k, 1 have no common factor, then
where dH is the spacing of the planes (hkl) in the direct lattice. This may be proved by observing that dH is equal to the length of the normal ON to the plane ABC from the origin 0. Since r i has the same direction as ON,
r r;
d H = (alh) .=
1 ria
4. As well as for direct lattice, a metric matrix G* may be defined for the reciprocal lattice:
It may be easily verified that Consequently (see (2.1) and (2.3) for the direct lattice) from which
+
+
+
d H = (h2a*2 k2b*2 1 2 ~ * 22hka*b* cos y*
+ 2hla *c*cos /3* + 2klb *c*cos
(2.17b)
is easily obtained. Specific expressions of d H for the various crystal systems are given in Table 2.2.
Basis transformations In threedimensional space the coordinate system defined by the base vectors a ' , b r , c r may be defined in terms of the base vectors a, b, c by
66
1
Carmelo Giacovazzo Table 2.2. The algebraic expressions of 4, for the various crystal systems
Cubic Tetragonal Orthorhombic Hexagonal and trigonal ( P ) Trigonal (R)
( h2
a2
+ k2 + 1') sin2 a + 2(hk + hl + kl)(cos2acos a) 1 +2cos3cu3cos2~
Monoclinic
h2 I? 1' 2hlcosP 2 . 2 +7+2.2a sln fi b c sin /3 ac sin2P
Triclinic
(1  cos2 a  cos2 /3  cos2 y
+ 2 cos a cos fi cos y )  l ( $
sin2 a
21h 2hk +(cos y cos a  cos p ) + (cos a c0s.p  COS y ) ca ab
three equations (suppose the transformation leaves the origin invariant)
where mi,are any real numbers. In matrix notation (2.18) is written as
+ + + +
The reverse transformation will be A = M'A'. The vector r = xa yb zc may be written in the new coordinate system A' as r' = r = x'a' y'b' z'c'. Introducing (2.18) into the r' expression leads to
The reverse transformation is X' = (M)'X. It should be noted that (2.20) provides the transformation rule for the components of the vector r while the vector itself is unaffected (r' = r) by a change of axes. The metric matrix G' in A' may be calculated by substituting into (2.1) a ' , b', c' for a, b, c and then using (2.18). The result is The unit cell volume defined by A' is V' = a'
A
.
b' c' therefore, according
Crystallographic computing
to (2.19) and (2.5), V ' = V M . Thus, for any transformation of axes the unit cell volume is multiplied by the determinant of the transformation matrix. The set of matrices conventionally used to pass from centred cells to primitive ones and vice versa is shown in Table 2.C.1 (however, transformation matrices are not unique). Let us now apply (2.20) to derive the transformation rules of a quadratic form. Let
be a quadratic form defined in the coordinate system A. In accordance with (2.20) X Q X = X ' M Q M X 'from which
Q' = MQM
or Q = M  ~ Q ' ( M )  ~ .
(2.22)
A special linear transformation is that which relates a' = a * , b' = b*, c' = c* to a, b , c (in this case A' will be replaced by A*). Let us show that in this case M = Gl = G*. Write the vector r = xu + yb + zc as
(in terms of reciprocal axes
r' = r* = x'a* + y'b*
+ z'c* = (r' .a)a* + (r'
b)b* + (r' c)c*). (2.24)
On assuming in (2.23) r = a *, b *, c*, the following relations
. . .
. .
.
a* = (a* a*)a + (a* b * ) b + (a* c*)c b* = (b* a*)a + (b* b*)b + (b* c*)c C* = (c* a*)a + (c* b*)b + (c* c*)c are respectively obtained, which in matrix notation reduce to
A * = G * A or A = G A * .
(2.25)
It is easily seen that relations (2.25) are special cases of (2.19). Similarly:
1. Relations (2.26) are special cases of (2.20) X=G*X* or X*=GX.
(2.26)
They transform components defined in direct space into components defined in reciprocal space and vice versa. In accordance with (2.1) and (2.26) we have
.
rl r2 = XlGX2 = XIX; = Xax;.
(2.27)
In particular r2 = r*2= X X * is the square modulus of a vector.
2. Equations (2.28) are special cases of (2.22): Additional transformation rules are given in Appendix 2.E. The reader is referred to the splendid book by sandsr1]for further insight.
( 67
68
1
Carmelo Giacovazzo
Transformation from triclinic to orthonormal axes Geometrical calculations are often more easily made in an orthonormal than in a crystallographic frame. Let
(I)
A=
E=
and
(i)
be the crystallographic and the orthonormal bases respectively. Then, according to (2.18), E = MA, and inversely A = M'E. If we choose (see Fig. 2.2) el along a, e2 normal to a in the (a, b) plane, e3 normal to el and e2 (and therefore parallel to c*), then the unit vectors ala, blb, clc are referred to el, e2, e, by means of
/a
where (I,, I,, I,), (m,, m2, m,), (n,, n2, n,) are direction cosines of the unit vectors ala, blb, clc in E. Therefore ClT=Cm?=Cn:=l. i
C
Fig. 2.2. Orthonormalization of crystallographic bases.
i
i
From Fig. 2.2 it may be deduced that 1, = 1, 12= 0, 1, = 0, m2 = sin y,
m l= cos y, nl = cos p.
m3 = 0,
Since cos a = C mini = cos cos p + sin sin n2 i
we obtain
n2 = (cos a  cos p cos y)/sin y = sin
p cos a*.
Furthermore, from the relation Ci n: = 1
n, = sin p sin a*= l/(cc*) is easily obtained. Finally
(fI))=(co:y
cos p
0 0 siny sin p cos a* ll(c*c)
from which =(bc:s c cos p
0 0 b sin y 0 c sin /3 cos a* l / c *
)(,)
The matrix M to use in E = MA is therefore 1/a cos y/(a sin y) a * cos p*
0 l/(b sin y) b * c o s a * c*
= WIJL (2.30)
Crystallographic computing
A crystallographic frame may be orthonormalized in infinite ways. For example, el may be chosen along a* and e2 in the plane (a*, b*): e3 is then along c. In this case M=
("d*~;~* 0
c*cosp* b*siny*  c * s i n p * c o s a llc
and ~

l
=
l l a * cot y*/a* a cos /3 0 l/(b*siny*) b c o s a 0
C
Also, we may choose el along a* and e2 along b (then e3 is in the plane (b, c)). We obtain l l ( a sy sp*) l l ( b t a tp*)  l l ( b ty sp*) ll(c s a tp*) M=( 0 0 l/b 0 ll(b t a ) ll(c s a )
(2.31~)
and
where sy, cy, ty stand for sin y, cos y, and tan y, etc. . . . The family of all the possible transformations M which orthonormalize a given frame A according to E = MA may be obtained from the following decomposition of the metric matrix G of A:
Such a relation is obtained by requiring that in (2.21) the condition G' = I is satisfied. The volume of the unit cell defined by a, b, c may be easily obtained if M is known. Indeed, if we express a, b, c in terms of el, e2, e3 according to (2.30), and if (2.5) is then used for calculating a b A c, then the result
.
V =a b
A
c = det (M')
is obtained. Furthermore, since det (Ml Ml) = v2= G, the assumption made on p. 62 according to which G is the square of the volume of the unit cell is also proved.
Rotations in Cartesian systems In a righthanded Cartesian coordinate system [0, el, e2, e3] the anticlockwise rotation of a vector r through angle al about el or through a2 about e2 or through cu3 about e3 produces a vector r' = R,r where s = x , y , z
1
69
70
1
Carmelo Giacovazzo
and 0
cos a,
0 sin a,
sin a,
0 cos a2
(
c a s ia Rz(a3) = sin a3 cos a3
0)
Since the matrices are orthogonal, the following relations hold: R(a) = Rl(cu) = Rl(a) = R(a).
Corresponding clockwise rotations are obtained by changing a;. into a;.. Matrices corresponding to rotatoryreflection operations about el, e2, e3 are obtained by replacing in (2.32) the integer 1 by 1. Matrices corresponding to rotatoryinversion operations about el, e2, e3 are obtained by changing the signs of all the elements. The traces of the matrices that represent proper rotations, rotatoryreflection and rotatoryinversion operations are 1 2 cos a, 2 cos a  1, 2 cos a  1 respectively. It should be noted that rotating r about el, e2, e3 in anticlockwise mode is equivalent to rotating el, e2, e3 in clockwise mode. For example if the framework [0, el, e2, e3] may be superimposed to the new framework [0,e;, eh, e;] by a clockwise rotation through a, about e3, then E' = R,(a3)E. According to (2.20), X ' = R;l(a3)x = R,(a,)X, which corresponds to an anticlockwise rotation of a vector r in E.
+
See now some useful applications: 1. Rotation about the unitary vector I in a rectilinear coordinate system. Given the crystal base A = (a, b, c), an orthonormal base E = (el, ez, e3) may be chosen (E = M A ) such that el coincides with 1. In accordance with (2.32) a rotation about 1 in E is represented by R,, and, according to Table 2.E.1, the same rotation in A is represented by R = MR,(M)'. As an example we calculate in the hexagonal system the matrix corresponding to an anticlockwise rotation through x about a. According to (2.30) and (2.31) the matrices M and MI are
from which (cos  1)/2 cos x = 0 aflsinX/(2c) 1
R = MR,(M)~
c sin x / ( a f l ) 2 c sin Xl(afl) cos x
Incidentally, it may be noted that the ratio a/c is unconstrained. Thus R (which is an integer matrix) may correspond to a symmetry axis along a in
Crystallographic computing
the hexagonal system only if x =O, n (onefold or twofold proper or improper axis). The reader will easily find that the general rotation matrix about b in the monoclinic system is
.=(
cos x + cot plsin x 0 c sin %/(asin p) 0 1 0 a sin xl(c sin$) 0 cos x  cot /3 sin x
R will correspond to a symmetry operator if
= 0,
n.
2. Explicit expression for the rotationmatrix R about the unit vector I in an orthonormal system. Let I,, I,, I, be the direction cosines of 1 in the orthogonal system A. A new orthonormal system E = (el, e,, e,) is chosen so that 1 coincides with el: then, according to (2.29),
where mij are suitable parameters. The matrix corresponding to a rotation about I in A is then
where sx and cx stand for sin x and cos X.
3. Sequence of rotations about the same axis or about different axes. The overall effect of a sequence of three successive rotations R,(w), Ry(q), Rx(q) on the vector r may be so described: from which
X
= RxRyR,X = RX
where cqcw cqso c q s o + sqsqcw c q c o  sqsqsw sqcq sqsw  cqsqcw s q c o c q s q s o c q c q
+
and c q stands for cos q , s q for sin I$, etc. . . . If the three rotations are made in different order, the overall effect changes. As an example, the reader will easily verify that rotating r through 120" about e3 and then through 90" about el leaves r in r" where
1
71
72
1
Carmelo Giacovazzo
and
4. Eulerian angles. In Fig. 2.3(a) two orthonormal frameworks [ 0 , el, e2, e3] and [O, el, e;, e;] are shown. The axis OK, called the line of nodes, is the intersection of the (el, e2) and (e;, e;) planes and is perpendicular both to e3 and e;. E may be superimposed to E' by three anticlockwise rotations in the following order: (a) rotate about e3 by the angle 81 (OK and el are now identical); (b) rotate through 8, about OK which will bring e3 into coincidence with e;; (c) rotate about e; by O3 which then brings el to el and e2 to e;. Suppose now that r is a vector with coordinates X in the spacefixed system and coordinates X' in a bodyfixed system: then X and X' are connected by
Fig. 2.3. (a) Eulerian angles. (b) Spherical polar coordinates.
where cei and soi stand for cos ei and sin Oi respectively. The Eulerian angles can also be used in order to calculate, in any crystallographic system A, the rotation function corresponding to any desired rotation. The simplest procedure could be: (a) Transform coordinates in A (say XA) into coordinates in E (say XE). If E = MA, then according to (2.20), X, = (M)lXA. For example, M may be (2.31a) or (2.31b) or (2.31~). (b) Transform the Cartesian coordinates into a rotated set of axes. Then XE transforms in XI, = REuXE. (c) Return these coordinates into the system A. Then the inverse operation described in (a) has to be made. The final coordinates are Xj, = M X =~ MR,,(M)'X~ so that the desired rotation function is
the full range of rotation operations is
Crystallographic computing
Since Eulerian angles are difficult to visualize it is preferred to specify a rotation in terms of spherical polar coordinates (see Fig. 2.3(b)). The rotation about a given axis is specified by the angle x and the polar coordinates and q, define the direction of the rotation axis. According to Fig. 2.3(b) the orthonormal coordinates x , y, z are given by Since (2.32b) represents the anticlockwise rotation matrix about the unit vector 1 in an orthonormal frame we can replace the direction cosines 11, 12,l3 of the rotation axis 1 by
Il
= sin
I)
cos q,,
l2 = cos q,
l3 = sin
qj
sin q,
and so obtain the expression of the rotation matrix Rsp in terms of the rotation angle x and the spherical polar coordinates q, and q : CX+ (1  cx)s2*c2Q) s*sQ)sx+ (1 cx)c*s*cQ) cx + (1  c x ) c 2 ~ R,, = s * s q s ~ +(1  c ~ ) c v s v c q , c ysx (1  cx)s2*cQ)sq, s*cQ)sx (1  cx)c*s*sq,
(
cvsx (1 cx)s2*cQ)sQ)  (1  C X ) C I ~ S ~ S Q ) cx + (1  c~)sz*s2Q)
S~CQ)SX
Since
all rotation operations qre included in
Some simple crystallographic calculations The reader is referred to Appendix 2.B for calculations concerning crystallographic directions and planes. Here we limit ourselves to the description of some calculations which occur very frequently in crystal structure analysis.
Torsion angles For a sequence of four atoms A , B, C, D, the torsion angle o(ABCD) is defined as the angle between the normals to the planes ABC and BCD (see Fig. 2.4). By conventiod2] w is positive if the sense of rotation from BA to CD, viewed down BC, is clockwise, otherwise it is negative. Note that w(ABCD) and w(DCBA) have the same sign; furthermore, the sign of a torsion angle does not change by rotation or translation, and is reversed by reflection or inversion. According to the definition (see again Fig. 2.4) cos o =
.
b ) (b A c) ab2c sin a sin y b
(a A
(a A b) A (b A c) b sin w = ab2c sin a sin y
which, owing to (2.7) and (2.8), become cos w =
cos a cos y  sin /3 , sin a sin /3
sin o =
Vb ab2c sin a sin y
'
Fig. 2.4. Definition of the torsion angle w .
1
73
74
1
Carmelo Giacovazzo
If the vectors a * , b * , c* reciprocal to a , b , c are considered, it may easily be seen from Table 2.1 that w coincides with P*.
Best plane through a set of points Consider a set of p atoms at positions rl, r2, . . . , r, where rj = AX,.. The best plane through them is that for which the sum of the squares of the distances of the atoms from the plane, multiplied by the weights of the atomic positions, is minimum. Such a plane is characterized by the minimum of the function (see eqns (2.B.5) and ( 2 . B . 7 ) )
where d is the distance of the plane from the origin of the coordinate system, n = n , a + n2b n,c = A N = nFa* nib* ngc* = A*N* is the normal to the plane. The weights w, should be taken as being inversely proportional to the variances of the atomic positions in the direction normal to the desired plane, but they are often assumed to be unitary. If the atoms are considered as point masses of weight w j , the least squares plane coincides with the principal plane of least inertia. The minimum of Q will be searched with respect to d and n:, n z , n; under the condition that n is a unit vector. This kind of problem is best solved by the method of Lagrange multipliers. The function to minimize is thenL3]
+
=
+
+
C w j ( A * x j d ) 2  A ( N * G * N * 1).
(2.34)
i
The partial derivative of (2.34) with respect to d gives
from which
d = N * [ ( F w j x j ) ( ? w,)'1 = N*Xo.
(2.35)
Equation (2.35) states that the plane passes through the centroid ro = Owing to (2.35), eqn (2.34) becomes
ao.
where r; = r;.  ro and
Note that N * S N * is the weighted sum of the squares of the distances of the atoms from the plane. Setting to zero the derivative of (2.36) with respect to
Crystallographic computing
N* (in practice with respect to the components n:, SN*  AG*N* = 0, which may be also written as (A hl)N = O
ng, nz) gives (2.37)
where A = SG and N = G*N* (see Table 2.E. 1). Writing (2.37) as AN = AN and multiplying both sides for N* gives The eigenvalue A is therefore the weighted sum of the squares of the distances of the atoms from the plane, N is the corresponding eigenvector. There are three solutions of eqn (2.37), which in general correspond to three different A values, say A, >AP 3 A., Each eigenvalue of A gives a stationary value of Q ' : the three corresponding eigenvectors N, NP, N, define the principal axis of inertia of the system of atoms when considered as points of masses w,, . . . , w,. The best plane corresponds to the eigenvalue A, and coincides with the plane passing through ro and normal to N, (see eqn (2.B.6)), while A, and N, define the worst plane. Furthermore, N,*Xi is the distance of the ith atom from the best plane and N i x ; and N/TXI are useful to prepare a diagram of the projection of the system of atoms on to the best plane. The search of the best plane is remarkably simplified if Cartesian systems are used (then G = G* = I).
Best line through a set of points This problem is strictly connected to results described in the above subsection. It may be shown that the least squares line passes through the centroid ro of the atoms and is normal to the plane corresponding to the eigenvalue A,.
Principal axes of a quadratic form Let be the quadratic form. Finding its principal axes is equivalent to finding the directions n in which q is stationary. As in calculating the best plane through a set of points, the problem may be solved via the Lagrange multipliers by minimizing The derivative of q' with respect to N brings to from which
(A  Al)N* = O where A = QG*, and N* = GN is the general eigenvector the components of which are referred to the reciprocal axis. The eigenvalue A gives the value of q in the n direction. Indeed, if (2.38) is written as AN* = AN* and both sides
1
75
76
1
Carmelo Giacovazzo
are multiplied by N we obtain
Substituting the three eigenvalues A,, A,, A, into (2.38a) provides the three eigenvectors N:, N;, N: which represent the principal axes of q. If the quadratic form is referred to the reciprocal basis (i.e. q * = H$H = Pllh: + 2P12hk+ . . . + P3,12) the problem may be solved in the same way on condition that G* and N* replace G and N respectively. As an example let us determine the principal axes of an atomic thermal ellipsoid for which PI1= 0.00906, P12= 0.00049, P13 = 0.00102, PZ2= 0.00401, P23 = 0.00038, P3, = 0.01424. Let the orthohombic unit cell parameters be a = 8.475, b = 10.742, c = 5.8991$. The function to minimize is which, derived with respect to N*, leads to the condition Since N = G*N*, that condition may be written ($G  Al)N = 0 . The corresponding secular equation is
Expansion of the determinant produces the cubic equation
which has solutions A, = 0.483, AB = 0.448, A, = 0.677. Using the first root gives
0.1677 0.0565 0.0354 (0.0352 0.0203 0.0132) 0.0733 0.0438 0.0125
(I::)(!). =
n3,
Since the three equations are linearly dependent n,, and n2, can be found in terms of n,,: n,, = +0.2592n3,, n2, = 0.185n3,. The eigenvector N, will have unitary modulus (remember that n,,, n,,, n,, are the components of N, in A) if n3, = 0.1515. Therefore N, = [0.0393, 0.0280, 0.15151. In an analogous way N~ = [0.0139, 0.0866, 0.05871 and N, = [0.1097, 0.0210, 0.04921. Since
each eigenvalue A fixes the value of q* along the corresponding eigenvector. If this conclusion is referred to the tensor U* = j3/(2n2), (see eqn (3.B.6)
Crystallographic computing
the following relations follow: A3
( ~ 2=)~ 2n2
(2.38b)
)
~ meansquare displacement along the ith principal axis. where ( u ~ is) the The reader will easily find, for the example above, that the rootmeansquare displacements along the principal axes are 0.156& 0.151 A and 0.185 A respectively. It would be worthwhile remembering two basic properties of the eigenvectors: (1) eigenvectors corresponding to different eigenvalues are orthogonal to each other; (2) the matrix M = (GV)l, where V is the eigenvector matrix
transforms the basis A into a Cartesian coordinate system A' in which the axes are the eigenvectors of $. Indeed, according to (2.E.8), $ transforms into $' = VG$GV. Because of (2.38b)
so that
Metric considerations o n the lattices The results obtained so far can be used to characterize lattices and their properties.
Niggli reduced cell A unit cell defines the lattice: conversely any lattice may be described by means of several types of cell. However, a special cell exists, called ,the Niggli reduced cell, which uniquely describes the lattice:[41it is primitive and is built on the shortest three noncoplanar lattice translations (the ~ e l a u n a ~reduction [~] procedure is also a suitable tool for the identification of a crystal lattice: readers will find careful description of it in some recent papers["']). A unit cell characterized by the three shortest noncoplanar translations is called a Buerger cell.[92101 Several algorithms can be used to obtain it. The easiest is: lattice vectors of magnitudes r,,,,, are calculated by (2.3) where u, v, w vary over the smallest integers set (usually between 3 and 3). The
1
77
78
1
Carmelo Giacovazzo
smallest three noncoplanar translations will be the Buerger cell edges. This cell is, however, not unique: if it is, then it coincidesiwith the Niggli cell. For 7 of the 14 Bravais lattices a unique Buerger cell exists,[''] while in a face centred cubic lattice (see later) two Buerger cells can be found. In other lattice types up to five types of Buerger cell can be found (the values 4 and 5 occur only in triclinic lattices) according to whether some conditions on the parameters of the conventional cell are satisfied or not. For example, the triclinic lattice described by a Buerger cell with
may be described by means of four other Buerger cells having the same a, b, c values, but with
a = 60°00', a = 120"001,
P = 86'24', P = 93'36',
a = 117'57',
/3 = 93'36',
a = 113'58',
P = 100°48',
y = 75'31';
y = 100'48'; y = 104'28'; y = 104'28'.
It will be shown later that only the first of the five cells is the Niggli cell. If gij are the elements of the metric matrix, the Niggli cell is defined by the following conditions:[129131 1. Positive reduced cell (all the angles
($) nm where B, = A N ~ ~ from A , which variance and covariance values for the parameters may be calculated. In particular the variance of the es'timated parameters is given by C WH(AFH)~ oii= (bii) 1 nm
"
where bcl is the ith diagonal element of B;'. It is easily seen that increasing the number of observations reduces the variance of the parameters ((bii)' and n are mutually related in an inverse fashion so that the standard varies as If the quality of the data is improved then deviation WH = 1/ah will increase: since (bii)' varies inversely with w it follows that standard deviations of the parameters are proportional to a,. The standard deviations of the parameters are a useful guide during the refinement process. If they are sufficiently small, the refinement process may be considered complete if the ratios (calculated shiftslstandard deviations) are sufficiently small (e.g. less than 0.20.3). Correlation coefficients between two parameters are given by
6
m).
pI'. = b../(b..b..)112. I' 11 I1 pi, can range from 0 to f1: as a rule, pi, s 0.20.3 are frequent, pi, = f1 refers to two completely dependent parameters, one of which has to be eliminated. As already stressed, owing to the presence of systematic errors very often the working matrix Nf experimentally available is referred to Mf by an unpredictable relation much more complex than a scaling factor. In these cases the technique of multiplying the working variancecovariance matrix B;' by $I($) in order to obtain M, may be highly questionable. A report[511 of the International Union of Crystallography Subcommittee suggests that besides indices R or R, as given in eqns (5.3) and (5.85) the goodness of fit ratio $I($) (see also eqn (5.86)) should be also reported in publications as a global measure of fit.
Practical considerations on crystallographic least squares Crystallographic leastsquares refinement may not be a trivial task. Suppose that, for a structure of modest complexity (40 atoms in the asymmetric unit), n = 4000 reflections have been measured. Generally speaking, an overall scale factor, 120 positional, and 240 anisotropic thermal parameters should be refined, for a total of 361 parameters. Then a square matrix B of order 361, with m = 361 x 36012 = 64 980 distinct elements will arise, each one constituted by a summation on thousants of terms. The computing time
Crystallographic computing
1
99
(Cpu) and the storage (St) needed for a 'structure factor calculationleastsquares refinement' cycle will comply with the following table: Step
Cpu
St
Calculate structure factors Calculate derivatives Calculate normal matrix
nrn nrn nrn2
n rn rn(m
Invert matrix Calculate shifts AX
m3 rn
+ 1112
In accordance with the above table, computing time and storage rapidly increase with the complexity of the structure, so that the task soon becomes prohibitive even for large and fast computers when largescale problems (thousands of parameters) are treated. A useful suggestion arises by observing that the elements on the principal diagonal of B are sums of squares, so that they are always positive and rather large. On the contrary, the offdiagonal elements are sums of products which may be positive or negative; therefore they are generally expected to be smaller than diagonal elements. Accordingly computer storage and computing time may be reduced by setting all offdiagonal elements to zero (diagonalleastsquares approximation). That is equivalent to assuming a complete statistical independence among the parameters, but this is often unrealistic. For example:
(1) errors in the thermal parameters generate a systematic error (larger to high sin 8 / A ) on IF[,,which on its turn produces a bias into the estimate of the scale factor K; (2) in oblique coordinate systems, nonnegligible correlations between some coordinates of the same atom may be found. Indeed an error on a coordinate is compensated by errors on some other coordinates (see Fig. 2.10);
(3) a high correlation will be found among the site occupancy and temperature factors if they are contemporaneously refined. An alternative to the diagonal approximation is the blockdiagonal approximation; a first block may involve the correlation between the scale and the overall thermal parameter; the other blocks, one for each atom, are 9 x 9 matrices comprising positional and anisotropic temperature factors (a 4 x 4 matrix for an isotropic atom). The matrix B will then appear as in Fig. 2.11. Larger blocks are sometimes used; e.g. all the atoms in the same molecule could belong to the same block; or, also, a block for all positional parameters and a block for all vibrational parameters with the overall scale factor; or, . . . . The storage requirement for the block diagonal approximation is certainly smaller than for full matrix methods. Each refinement cycle is faster, but convergence is slower: so the complete refinement process requires more cycles and almost the same computing time. Thus the major advantage of the method is the lessened storage requirements for problems too large to be treated by a full matrix. A very large saving of computer time has been recently achieved by
Fig. 2.10. P(xo, yo) is the true atomic position. If an error A, is introduced, the 'best' value for x i s obtained by minimizing, along the line yo A y = const, the distance of the atom from the true position P. That produces A, = A, cos y.
+
Fig. 2.11. A scheme for blockdiagonal approximation.
100
I
Carmelo Giacovazzo
application of the fast Fourier transform (FIT) algorithm. FFT based programs allow fullmatrix refinement of protein structures at a reasonable cost (see Appendix 2.1 for some details). A critical point in least squares is the occurrence of large correlation coefficients among parameters: this can give rise to illconditioned (determinant close to zero) B matrices and therefore to serious problems for the calculation of B' and for the accuracy of AX. That occurs when the following conditions hold. 1. Two atomic sites nearly overlap because of some structure disorder (or some error).
2. The symmetry of the structural model is higher than the spacegroup symmetry in which refinement is made. As an example, let us suppose that refinement of two symmetry independent molecules has been unsatisfactorily carried out in P2/m. The question arises as to whether or not the space group is really centrosymmetric. Refinement in P2 is then carried out on four symmetry independent molecules, the second two obtained from the first two by application of the inversion centre. Then the new B matrix will be singular: indeed the imaginary parts of the structure factors are vanishing, the derivatives of IFI, with respect to pairs of positional parameters referred by the inversion centre have equal moduli and opposite signs, the derivatives with respect to corresponding pairs of thermal parameters have equal moduli and signs. Since the elements of B are sums of products of derivatives, pairs of lines will be identical or opposite, so that B is singular. To overcome this difficulty small random shifts are applied to parameters when refinement moves from the first to the second space group. However, the matrix still remains illconditioned and further unpredictable shifts can be generated. A more efficient procedure is that which modifies the normal matrix to limit the parameter shifts (not equivalent to dumping shifts after the matrix solution). As a further example, a singularity may occur when two atoms with the same x and y coordinates but differing by a 50 along the x axis are refined without using reflections with h odd. 3. Symmetry constraints are not introduced. For example if an atom lies on 4[rn11,the following constraints will hold: Pll = fizz, PZ3= P13= PI, = 0. If pll and pzzare erroneously refined as if they were independent, the matrix B will have two rows and two columns equal and will be singular.
4. In some noncentrosymmetric space groups the origin may float in some directions. The normal equations matrix will become singular if the atomic coordinates of one atom along the free directions are not fixed (e.g. z in Pca2,, or x and z in Pm). Such a practice was frequently used in the primitive least squares programs but provides incorrect estimated standard deviations unless the full variancecovariance matrix is used. The problem may be solved by constraining (or restraining, see p. 107) the sum of the free coordinates to a constant value. An efficient leastsquares program should:
1. Provide easy ways for applying symmetry constraints to parameters of atoms in special positions. These are handled by not refining some
Crystallographic computing
parameters or by equivalencing atomic parameter shifts. For example, in a hexagonal space group for an atom in special position at (x, h,z) the only independent positional variables are x and z, so that
Analogous problems occur for thermal parameters: symmetry constraints on them are described in Appendix 3.B.
2. Allow for a variety of weighting schemes (see p. 369). The weights play a critical role in any refinement process. In the initial stages of refinement artificial weights may be used to accelerate convergence (e.g. w, = 1 for all reflections is commonly used when a partial structure is under refinement). In the final stages the weights should reflect the accuracy of the individual observations (w, = 1/02(IFIO)should be deduced from an analysis of the experiment). Then observations which are believed to be unreliable get very small weights. Unfortunately it is not trivial to assess the accuracy of observations and the correctness of the assumed model. A long list of errors[521can affect the values of the deviates (IFHlo IFHlc)and therefore the results of a crystal structure analysis: experimental accidents (fluctuating power in the incident beam, crystals moving on their mounts, etc.); statistical fluctuations in quantum counts; crystal damage by the incident beam; errors in corrections for absorption, background radiation, thermal diffuse scattering, extinction, anomalous dispersion, anisotropic and/or anharmonic vibration, disorder, multiple reflections; deviations from the isolated atom approximation; incorrect symmetry assignment; correlation among observations. Different types of errors can have similar effects and may be compensated by others. For example, absorption and extinction corrections tend to reduce intensities at low sin 6/Avalues more than at high values: thus errors in correcting these effects produce, as a partial compensation, errors in the thermal tensors. In most cases the effects of each type of error cannot be estimated: then the standard deviation of individual intensity measurements is assumed as the standard deviation calculated from counting values plus an additional term which allows for errors of an undefined nature. It should be stressed that estimated variances of observations, and therefore weights, should not be based on counting statistics alone. Indeed variances estimated in this way are proportional to the intensities themselves: the consequence is that low intensities will systematically have lower variances than high intensities. That results in a bias in the estimate variances, and consequently (the GaussMarkov theorem states that only if errors are random and uncorrelated it may be expected that the leastsquares methods give the best unbiased estimate of the parameters) in a bias in the parameter estimates which may be of some relevance in highprecision structure determinations. In these cases it is highly recommended that all symmetry equivalent reflections are measured, that the averaged intensity is used in least squares, and that the variance based on counting statistics is combined with that arising from differences among symmetryequivalent data.[511 The possible presence of errors may be checked by observing that S is expected to be distributed like X2 with n  m degrees of freedom. For large n  m values x2/(n  m) is expected to be close to unity: so, if w,, = l/&
1
101
102
1
Carmelo Giacovazzo the expectation (see Appendix 2.H) for 3 is ( 3 ) = n  m. Accordingly the set of observations may be divided in large subsets (any significant criterion may be used for obtaining subsets: intensity ranges, or intervals of Bragg angles, or parity of Miller indices, etc.): then the weighted sum of discrepancies for each subset may be analysed. Each jth sum should be nearly (n  m)(p,/n), where p j is the number of terms in the jth subset. If some unexpected behaviour appears then one may guess that some source of error has not been taken into account, and weight should be suitably changed. A practical weighting criterion which takes into account all random experimental errors for which precise estimates are not available from experiment may be so described: the lFlorange is subdivided into a number of intervals each containing approximately the same number of reflections. For each ith interval the average (IFlo)i and the difference (AF),= ((IFIo IFJ,))i are calculated. Plotting (AF), versus (IF,[) (see Fig. 2.12) will show a distribution of points which can be approximated by an analytical function such as
. Fig. 2.12.
p(lFl0) = a0 + a1 IF10 + a2 IFIi + a3 IF[:. The weighting scheme will be designed in order to make differences (A&) constant; thus
More efficient empirical weights which make ( A F ) ~constant as a function of lFlo can be obtained through truncated Chebyshev polinomials.[531 But the above practices are not able to eliminate systematic errors or correlation among errors. If a careful check does not suggest any new strategy the only way for lessening the effects of systematic errors is based on a weighting scheme based on the deviates (IFo[ I&[). Wang and ~ o b e r t s o n [ modified ~~] leastsquares weights by adding to the calculated variance a term which is a fundion of the disagreement between the experimental and the expected distribution of the deviates. Robustresistant techniques[551also use weights based on the deviates. Due to some random or systematic errors, or to imperfections in modelling parameters, or to many other reasons it may occasionally occur that a small number of data, called outliers, show a very large discrepancy with respect to the corresponding calculated values. Least squares are very sensitive to the presence of large residuals which, having a high leverage, may cause nonnegligible distorsions in results. A naive approach, often used in practice, may be to discard outliers by setting to zero the corresponding weights. The robustresistant techniques decrease weights when disagreement increases, so avoiding any discontinuity in the process.
3. Allow for a proper choice of the number of reflections to be included in the refinement. In order to save computing time, or to avoid many lowquality data reducing the efficiency of the process, reflections for which IF1 < qo(lF1) are often excluded from the refinement (q depends also on the number of available data: q = 2, 3 is a frequent choice. Higher values of q could bring to a unsatisfactory ratio number of observations/number of parameters).
Crystallographic computing However, the omission of observations is equivalent to assigning zero weights to them. If a((F1) depends on IF1 such a practice preferentially discards lowintensity reflections so introducing a bias in the process. Often, that has little effect on the results,[56]but sometimes it discards important information (very unreliable results can be obtained when a structure with superstructure effects is refined without using weak reflections). The problem of identifying meaningful changes in R produced when the model is altered has been faced by ~ a m i l t o n . [ He ~~~ considered ~~] the weighted residual (5.88) instead of the conventional residual (5.85), and proposed the test (known now as Hamilton's test) based on the ratio T = Rw(1)lRw(2),where Rw(l) and Rw(2) (with Rw(l)> Rw(2)] are obtained from the two different models. In the practice T = R(l)/R(2) is often used because usually Rw(1)/Rw(2) R(l)/R(2). The test compares T with the function

If the computed T satisfies T > Rm,,m,a the hypothesis can be rejected at the 100a% significance level (a significance level of a = 0.05 is commonly used). Tables for Frn,,,,, were computed from Hamilton. For large values . of n  m (very frequent in crystallography). where
x2 is the well known chisquare function: in these cases
As an example, let us suppose that two leastsquares refinements based on the same number of parameters m and on the same number of observations n are carried out by two different investigators. The refinements resulted in two different R factors, say R(l) > R(2). The hypothesis 'the m parameters obtained by investigator 1 are consistent with the experimental data' may be rejected at the cu significance level if T > Rm,n m, a. Sometimes the two models used for refinement involve a different number of parameters. For example one refinement is carried out where b parameters are held fixed. Then Hamilton's test may be so modified: the value of T given by
T=
R (b fixed param., m  b varied param.) R (all m param. varied)
may be tested against values of
For example, a leastsquares refinement was first carried out up to the R(l) value on assuming that all the atoms have isotropic temperature factors (ml is the number of parameters). A subsequent refinement was carried out up to a residual R(2) < R(l) on assuming anisotropic atoms (m2>m1 is the number of parameters). The hypothesis 'all the atoms
1
103
104
1
Carmelo Giacovazzo
vibrate isotropically' may be rejected at the a significance level if
As a further example, let us suppose that refinement in a centrosymmetric space group (say P2/m), stops with the residual R(l), while refinement in a noncentrosymmetric space group (say P2 or Pm) results in the residual R(2) < R(1). If ml and m2 are the numbers of parameters for the two refinements, the hypothesis that the correct space group is centrosymmetric may be rejected at the a significance level if
A last remark on the crystallographic leastsquares technique concerns which function to minimize. In place of the function S defined by eqn (2.67) the function
is sometime minimized. The normal equations (2.68) still hold if w, is replaced by wk= wH/(4 IF^^!), 6 IFHlc/6~j by 2 IFH[, (6 IFH1,/G~j)and, in D, [IFH10  lFHlcl [IFHI:  IFHI:]. There is still a strong disagreement[51]over the question of whether S or S t should be used in refinement. In favour of (FIrefinement it may be observed[s8] that 6 IFI2/6xi is small if IFI2 is small: thus weak reflections have too weak a leverage in IFI2refinement. Arguments in favour of IF 12refinement are based on the observation[s93601 that I FI are obtained from intensity data via a square root. This is a nonlinear operation which may introduce a bias proportional to the variance of IFI2.Furthermore the ( 2 so widely used in practice is not appropriate formula a(lF()= a ( l ~ 1 ~ ) /IF() for zero or close to zero IF1 values, for which a(lF1) become infinite or extremely large (we must, however, mention that methods[613621 for obtaining more reliable IF1 and a((F1) from 1 ~ and 1 ~o(lFI2) values are now available).
Constraints and restraints in crystallographic least squares The accuracy of the derived parameters is generally small (e.g. it would be found that CC distances in a phenyl group were in the range 1.21.3 A, which is highly improbable) when at least one of the following conditions occurs: 1. Low ratio between the number of the observations and the number of parameters to refine. The ratio is particularly unfavourable for biological macromolecules. Indeed, owing to their intrinsic flexibility, the amplitudes of the thermal vibrations from the average positions are rather large (usually between 0.2 and 0.7 A), so limiting the diffraction data to a resolution of about 2 A. While to a resolution of 0.86 A (typical limit
Crystallographic computing
for small molecules) there are about 30 observations for each coordinate being refined, at 2.7 A the number of parameters is nearly equal to the number of the observations. 2. Atoms with very large atomic number and very light atoms coexist in the unit cell. Then modest errors on the heavyatom parameters cause strong errors on the lightatoms parameters. 3. Too high thermal motion, presence of structural disorder, etc. Only poor and scarce data are then available. If, however, some prior stereochemical information is available on parts of the structure its use in the leastsquares procedures may increase the degree of overdetermination of the system and improve the accuracy of the results. Three methods will be briefly recalled here.
Rigid body refinemenP1 If the structure contains rather rigid molecular fragments of well established geometry (e.g. benzene rings), the number of parameters to refine may be considerably reduced. The atoms concerned are initially regularized to some ideal geometry which is preserved during the refinement. For each rigid group of n atoms the number of independent positional parameters reduces from 3n to 6 ((xo, yo, zo) parameters defining the position of some reference point and w, 3 , q5 for the group orientation). Thermal parameters are usually considered to be isotropic, and, to keep the number of parameters small, a single overall thermal parameter may be assumed for the group. Leastsquares calculations could be performed according to the following scheme.[641For the jth atom of the group let Xi be the coordinates with respect to the system A defined by the conventional unit cell, Xi' the coordinates (in A) with respect to a set of orthogonal internal axes A', Xi" the coordinates with respect to an orthogonal cell of unit dimensions (say A ) oriented in some way with respect to A. Assume A" = MA where M is given by (2.31~)or a similar matrix. A rotation matrix R may be then defined which aligns A = (ey, e;, e;) on to A' (say A' = RA): according to the discussion on p. 72 the matrix R may be expressed as the product of three successive anticlockwise rotations, say by about e,, by 3 about the new e2, and by q5 about the new el. Then X," = RX; (see Table 2.E.1) and
The atomic coordinates so obtained may be used in the usual manner for calculating structure factors. The problem is now to calculate the appropriate contribution for the rigid parameters x,, yo, zo, w, v, q5 to the matrix of normal equations. Derivatives with respect to such parameters are calculated from those for the atomic parameters Xi using the chain rule: i.e.
a lFH1c
6 lFHIc axo
j=1
ax, '
1
105
106
1
Carmelo Giacovazzo
and, for a group temperature factor B,,
The size of the normal matrix is therefore reduced, convergence is accelerated but there is no remarkable saving in computing time (derivatives with respect to each atomic parameter have to be calculated for each structure factor and chain rule implemented). The success of this method relies on the accuracy of the assumed geometry: if this is wrong systematic errors on other parameters will be introduced (e.g. the symmetry of phenyl groups sometime deviates remarkably from the sixfold symmetry[651). A technique related to, but not coincident with, rigid body refinement is that used for putting hydrogen atoms into structures (Xray data). Sometimes H atoms are geometrically positioned at the end of each round of LSQ, but more frequently H parameters ride upon those of a reference atom (riding refinement). In this last case the normal matrix has to be modified in order to take into account all physical parameters (the common practice fixes the thermal parameter of H, which is set equal to that of the reference atom). At the end of calculations H and the reference atom will have the same positional estimated standard deviations, while the bond distance between them must have an estimated standard deviation equal to zero (if the full variancecovariance matrix is used in the calculation).
Constraints via Lagrangian multipliers In the absence of complete information on a fragment's geometry one may wish to fix some molecular parameters (e.g. some bond distances and angles are fixed to given values, a group of atoms is held in coplanar arrangement, etc.). In such cases Lagrangian multipliers can be used: the function to minimize is h
where the (generally nonlinear equations) represent the fixed constraints. Usually the available model X0 will not exactly satisfy (2.69). The problem will be linearized by expanding both the IFHIcsand the Gis in Taylor series:
where G: = G,(XO) and 6 ~ ~ is 1the6 derivative ~ ~ of G calculated in XO. The normal equations can be derived by settling to zero the derivatives (with respect to Ax and A) of S:
Crystallographic computing
The augmented normal equations, expressed in terms of partitioned matrices, are
where mjq = i(6G:/6xj). Even if a large variety of stereochemical constraints can be taken into account by the method, the approach is not very attractive for largesize problems: indeed the order of the normal matrix is increased.
Use of restraints Soft, flexible constraints (say restraints) may be imposed to some functions of the parameters in order to permit only realistic deviations of their values from fixed standard ones. These functions are used as supplementary observations, so that the order of the normal equation matrix is neither increased nor reduced. In this situation the function to m i n i m i ~ e [ ~ ~ is, ~ ' ]
where gq is the function describing the gth restraint, g,, is its standard (or optimal) value, w, is the weight to associate to the qth restraint. The normal equations are obtained by expanding S in Taylor series and equalling to zero its derivatives (with respect to AX):
The effect of restraints is therefore to add contributions to the elements of the normal equation matrix. Thus parameters highly correlated can be found, but this is expected since parameters are deliberately correlated by restraints. For example, a restraint may be to set an interatomic distance d (bonded or nonbonded) to a given value taken from the literature. If we recall, according to p. 62, that where
and so on. Another restraint may be: the sum of all the atomic coordinates along a polar direction can be fixed to its current value in order to keep fixed the centre of gravity of the molecule and so determine the origin. Several other types of restraints can be imposed (see Chapter 8, p. 564) and they concern van der Waals distances, planarity of groups, chirality (a restraint on the chiral volume about an asymmetric carbon atom may maintain the conformation in the correct hand), bond and torsion angles, thermal
1
107
108
1
Carmelo Giacovazzo
motion, positional and thermal parameters related by noncrystallographic symmetry, potential energy functions, etc. Also, the sum of site occupancies of two or more atoms can be restrained to some fixed value when disorder problems occur. When the number of restraints is sufficiently large the equations are overdetermined and refinement will also converge with lowresolution data. The approximate nature of the restraints well agrees with our approximate knowledge of the chemistry involved. A basic difficulty of their use is to assess an optimal weighting scheme: indeed the first component of S is in electrons squared while the second may be considered an energy quantity, where w, plays the role of an effective force constant. A convenient mechanism is to indicate the relative precisions (i.e. the expected standard deviations) of the restraints and scale them with respect to the observations. As an example, let us suppose that the bond distance dj is to be restrained to a set value. If the weights of Xray observations are (as usually) sufficiently accurate but on an arbitrary scale, the normalization factor &, = CHw ~ ( A F ~ )~m/ )( ~may be obtained. Then the restraint equation involving di with estimated standard deviation o(dj) is given the weight
Very small standard deviations make restraints equivalent to constraints. If refinement provides a bond distance differing from dj by several times a(di) it should be concluded that experimental data are in conflict with the fixed restraint. Applications of constraints and/or restraints in leastsquares processes usually lead to larger residuals than by unconstrained refinement. That does not necessarily mean that the constrained solution fits less well to the data. A sensitive criterion may be to compare estimated standard deviations obtained by constrained and unconstrained refinements. When constraints are applied both S and n  m increase but oii(see p. 98) may be larger or smaller according to circumstances. An alternative criterion may be the use of the Hamilton's test (see p. 103).
Alternatives to the method of least squares In the above sections some deficiencies of least squares have emerged, deficiencies which invite the application of alternative methods. In statistical sciences the main alternative to least squares are maximumlikelihood methods. Let us suppose that the errors e defined by (2.47) are distributed according to some probability density function P(e). The likelihood function L is then given by
Since P is everywhere greater than or equal to zero, its logarithm is a monotomically increasing function of the argument. Thus the maximum of L is attained when In L is a maximum. If the error function is Gaussian then ~ ' ~[e?/(2o?)] P(ei) = ( 2 ~ o ? )  exp
Crystallographic computing
where a is the variance of the ith observation. Then
Since the second and third terms are constant, In L has its maximum when
where wi = l/a:. We have so shown that, if the distribution of the errors is Gaussian, and observations are weighted by the reciprocal of the variance, the leastsquares and the maximumlikelihood methods provide equivalent results. Conversely, if errors are not distributed according to a Gaussian model, the method of least squares does not lead to a maximumlikelihood estimate. The above results also explain why least squares are practiclly the only ones used in crystallographic refinement: they only depend on the variance of the errors while maximumlikelihood methods require the knowledge of the distribution of the errors. When this is available maximumlikelihood methods provide better estimates of the parameters, since such methods can exploit more information. However, such a situation is very infrequent in crystallographic refinement, where only rather imperfect estimates of the variances are available. Parameters may also be estimated by maximum entropy methods, which, based on Jaynes' extension of Shannon's theory, require the maximization of the entropy. But such methods, as well as maximumlikelihood methods, are far from being competitive with least squares in most of crystallographic applications.
Rietveld refinement The basis of the technique Powder diffraction patterns (see p. 293) may be collected in a step scan mode: intensity is measured for a given interval of time, and the theta and twotheta axes are then stepped to the next position. The pattern is then indexed: i.e. appropriate Miller indices are associated with observed reflections and simultaneously accurate unitcell dimensions are calculated. Because of unavailable experimental errors in the estimates of the diffraction angles and because of the frequent overlapping of peak intensities, indexing is a rather difficult task for relatively large cell volumes and/or lowsymmetry crystals. Several approaches are today available for this aim: implemented in computer programs, they often provide more than one solution, so that proper figures of can be used to distinguish between bad and good solutions. The reader will find general remarks on the various approaches, and tests on their efficiency, in a paper by ~hirley[~'] ,and in some more recent paper^.[^"^^] This stage of analysis is followed by the examination of possible systematic absences to suggest a space group. If a (even imperfect) structural model is available then the intensity yi, observed at the ith step may be compared with the corresponding intensity
1
109
110
1
Carmelo Giacovazzo
yic calculated via the model. According to ~ i e t v e l d , the ~~~ model ] may be refined by minimizing by a leastsquares process the residual S = C Wi
I~
io
yic12
where wi, given by (wi)' = 0; = B:~ + o;~, is a suitable weight. oi, is the standard deviation associated with the peak (usually based on counting statistics) and a,, is that associated with the background intensity yib. yic is the sum of the contributions from neighbouring Bragg reflections and from the background:
where s is a scale factor, Lk is the Lorentzpolarization factor for the reflection k, Fk is the structure factor, mk is the multiplicity factor, Aerk= 28,  20k where 28, is the calculated positon of the Bragg peak corrected for the zeropoint shift of the detector, and G(Ae,k) is the reflection profile function. The parameters to adjust by refinement include unit cell, atomic positional and thermal parameters, and parameters defining the functions G and yzb* The determination of an accurate model for the profile function G(Aock) is one of the fundamental problems in both singlepeak and in Rietveld analysis. This is particularly true today when highresolution neutron and Xray spectra are available: deficiencies in the profile model are no longer lost in relatively large instrumental diffraction profiles. The shape of a diffraction peak depends on several parameters: the radiation source, the wavelength distribution in the primary beam (e.g. possibly selected by a monochromator crystal with its specific mosaic spread), the beam characteristics (as influenced by slits and collimator arrangements between the primary radiation source and monochromator, between monochromator and sample, and between sample and detector), the detector system. Accordingly, there are many choices of analytical peakshape functions. We quote: (Gaussian) ; cli2
2(1 + CIX;k)l nHk
(Lorentzian);
(1 + c2xfk)2
(modif. 1 Lorentzian);
"'(1 + c3xfk)1'5
(modif. 2 Lorentzian);
'L 2
~tHk
2Hk
with 0 s q G 1 (pseudoVoigt);
Crystallographic computing
r(B) r ( p  0.5)
52 (1 + 4c4x:,)p 7tk
(Pearson VII);
where Co = 4 In 2, C1 = 4, C, = 4 (  I), ~ C3 = 4 (2213 I), C4= 21f8 1, Xik = AOik/Hk. Hk is the fullwidth at halfmaximum (FWHM) of the kth Bragg reflection, and r is the gamma function. It is easily seen that the pseudoVoigt function presents the mixing parameter rj which gives the per cent Lorentzian character of the profile. When P = 1, 2, m, Person VII becomes a Lorentzian, modified Lorentzian, and Gaussian function respectively. Of some use also is the pure Voigt function which is the convolution of Gaussian and Lorentzian forms. The FWHM is usually considered to vary with scattering angle according to (2.71) (FWHM), = ( U tan2 8 V tan 8  w)'"
+
for the Gaussian component,[781according to (FWHM), = X tan 8 + Y/cos 8
(2.72)
for the Lorentzian component.[791 U, V, W, and/or X, Y are variable parameters in the profile refinement. Besides analytical functions nonanalytical functions arising from an analysis of resolved peaks may also be usedL8'] to describe peak shape (in the Rietveld method the peak shape is not the end but a tool of the method). There is no well established approach to the background. It is mainly due to insufficient shielding, to diffuse scattering, to incoherent scattering (rather high for neutrons), to electronic noise of the detector system. The background and its variation with angle is usually defined by refinement of the coefficients of a power series in 28:
where the b, terms are refinable parameters. All the above described parameters are introduced in the Rietveld refinement process according to (2.70). The agreement between the observations and the model is estimated by the following indicators:[s11 /C (2) The weighted profile R,, = [C wi(yi0 ~ i c ) ~ ~iy?o]l'~*
(3) The Bragg RB= C JZko  Ikcll(CZko). The values I,, are obtained by partitioning the row data in accordance with the Ik, values of the component peaks. where N and P are the (4) The expected R E = [ ( N  P)/(X number of profile points and refined parameters respectively.
(5) The goodness of fit GofF = C wi(yio Y , ~ ) ~ /( N P ) = (R,,/R,)~, which should approach the ideal value of unity. The most meaningful indices for the progress of refinement are R,, and GofF since they show in the numerator the quantity being minimized . Also RB is of considerable use since it depends on the fit of structural parameters more than on the profile parameters.
1
111
112
1
Carmelo Giacovazzo
The use of restraints in the Rietveld method has proved to be of particular usefulness for complex structures.[80,82,831
Some practical aspects of Rietveld refinement The generation of instrument profile calibration curves usually precedes Rietveld refinement. Such an analysis allows one to set up the angular dependence of the peak shape. A peak profile may be expressed as where b(28) is the background function, f(28) is a specimen related function, and w(28) *g(28) is the socalled instrument function. This may be considered as the convolution of the function g(28) representing the diffractometer's optics and a second function w(8) representing the wavelength distribution of the incident radiation. As a first step, diffraction profiles from a standard specimen (e.g. silicon, corundum, or quartz standard materials) devoid of crystallite size or strain broadening effects are collected: in this case f (28) may be represented by a delta function and (2.73) becomes If a single wavelength is used (i.e. in synchrotron or neutron experiments) a single peak may be represented by one or by a combination of the functions described in the previous subsection. If a Cu Xray source is used and a2 and a, are not eliminated by some experimental device (i.e. a germanium monochromator) a compound profile consisting of three split functions has to be chosen, one for each spectral component. The number of variable parameters in the profile function may be reduced by fixing a, and a3 intensities relative to a, intensity via a previous profilefitting experiment. Analogously, the angles for a2and a3lines may be fixed according to their wavelengths, and their FWHM can be set equal to that of al. The correct profile function is in general obtained by trialanderror methods from single well behaved profiles of the standard material. The goodness of the profile fit is measured by
where y,, and y,, are the observed and calculated values at the position 28,. For good experimental data the R value is expected to be around one per cent. The values of the profile parameters may be refined for each single peak collected from the standard: each peak is separated and analysed in a region with enough points to allow a good sampling of background on each side of the peak (a parameter for background may also be refined). In particular, the values of FWHM obtained from refinement are used for a first estimate of the U , V, W values in eqn (2.71) and/or of X , Y values in eqn (2.72). It is worthwhile mentioning that standard specimen data are also used for the determination of wavelength A (if necessary) and for the zeropoint calibration 28, of the detector scale. Analysis of the specimen profile f usually follows instrument profile
Crystallographic computing
calibration. Specimen broadening of the profiles is often present: it is traditionally assumed to be Lorentzian if profile broadening is present. The profile analysis of the full diffraction pattern is often used to peak positions and peak heights for each reflection: from them lattice parameters are calculated and refined in an iterative way. Peaks generated by overlapping of more reflections are deconvoluted and integrated intensities of individual hkl are calculated, together with their standard deviations and their correlations (see Appendix 3.A, p. 184). A specific feature of Rietveld refinement is that the number ot observations N can be chosen arbitrarily large simply by decreasing the step interval in 28. The increase of N does not remarkably affect the conventional Rietveld agreement but decreases the parameter estimated standard deviations approximately in proportion to N'". Such an improvement is often fictitious. For example, a single Bragg reflection may be measured using 10, 100, or 1000 steps. The observed intensities are not statistically independentFa7]and, for single peaks, yield structural information nearly equivalent to a single integrated intensity count (even if the precision obtained by 1000 steps count may be higher than by 10 or 100 counts). As a consequence the correlation among observations becomes higher with N = 10, 100, 1000 and leastsquares residuals A, = y,,  y , , are correlated themselves, i.e. they tend to assume the same sign. In such a situation DurbinWatson dstatisti~s['~I may be used to assess the nature of correlation. It is based on the parameter
For no serial correlation a d value close to 2 is expected. For positive serial correlations adjacent A tend to have the same sign and d will be smaller than 2, whereas for negative serial correlation (alternating signs of adjacent A) d is expected to be larger than 2 (and smaller than 4). The parameter d may be tested against the 0.1 per cent significance point via the formula[891
where P is the number of leastsquares parameters involved in the calculations. Q < d < 4  Q if consecutive terms are uncorrelated, if d < Q or d > 4  Q consecutive terms tend to have positive or negative serial correlation. dstatistics suggest that an optimum value of the step width is[901 between onefifth and onehalf of the minimum FWHM of well resolved peaks. The success of the Rietveld method is based on some fundamental requirements: 1. A starting model for atomic positional and thermal parameters should be available in advance. That can be provided by the following procedure:[911(a) deconvolution techniques and profilefitting methods are used to derive intensities Zk of individual reflections and to resolve overlapping peaks; (b) integrated intensities are calculated and structure solved by direct or Patterson methods. The same intensities are then used in a fullmatrix leastsquares refinement as for singlecrystal structure determination. Because of peak overlapping, this time error margins for each
1
113
114
1
Carmelo Giacovazzo
observation and correlation among reflections intensities could be processed to calculate a nondiagonal matrix Mf (see pp. 913). 2. The crystallites should be randomly distributed. That is not easy to achieve in practice.[92,931 Traditionally preferred orientations are minimized by loose packing of the powder: however, sufficient compression improves homogeneity and reduces surface roughness effects. If a specimen spinner is used in the experimental setup the preferred orientation can be characterized by a few parameters only, thus it may be introduced in a rather simple way in the fitting schemes and in Rietveld refinement. If the preferred orientation is not taken into account, errors in the relative intensities may occur which limit the accuracy of the refinement process. Some geometries are less sensitive to this problem (i.e. Guinier cameras). The problem is also minimized in neutron diffraction because of the large transmission specimen, but it is severe when synchrotron radiation is used because the number of crystallites correctly oriented to reflect the parallel beam is much smaller.[941 The most simple way to correct the intensities calculated from the model structure is to use an empirical correction function depending on @, the acute angle between the preferred orientation plane and the diffracting plane k:, Ik(corr) = IkPk(@).
Pkmay be ~ a u s s i a n ,951 [~~~
or of trigonometric type1961
p is a parameter to refine in the refinement process. 3. The crystallites should be of equal size. Particles much larger than 10 pm should be removed from the sample, as well as very small particles (
C pj(r  5).
(3.21)
j=1
The amplitude of the scattered wave is
I2 N
FM(r*)=
pj(r  q) exp (2nir* r) dr
S j=1
=
21
pj(Rj) exp [2nir* (q + R,)] d ~ ,
j=l
N
=
S
.
J;(r*) exp (2nir* q), j=l
where J;(r*) is the atomic scattering factor of the jth atom (thermal motion included; in the previous section indicated by fa,). The fact that in eqn (3.21) we have neglected the redistribution of the outer electrons leads to negligible errors for FM(r*), except in case of small r* and for light atoms, where the number of outer electrons represents a consistent fraction of Z. p,(r), as defined by (3.21), is the electron density of a promolecule, or, in other words, of an assembly of spherically averaged free atoms thermically agitated and superimposed on the molecular geometry. Such a model is unsatisfactory if one is interested in the deformation of the electron density consequent to bond formation. In a real molecule the electron density is generated by superposition of molecular space orbitals V iwith occupation ni:
Since pmolecule can be decomposed into atomic fragments, a finite set of appropriately chosen basis functions can be used to represent each jth atomic fragment (see Appendix 3.D). Then where Ap models the effects of bonding and of molecular environment (in particular, pseudoatoms may become aspherical and carry a net charge). By Fourier transform of Ap the deformation scattering is obtained:
The diffraction of Xrays by crystals
Since the core deformation scattering is negligible AF practically coincides with deformation scattering of the valence shells.
Diffraction b y a crystal One threedimensional infinite lattice can be represented (see Appendix 3.A, p. 174) by the lattice function
where 6 is the Dirac delta function and r,,,,, = ua + vb + wc (with u, v, w being integers) is the generic lattice vector. Let us suppose that p,(r) describes the electron density in the unit cell of an infinite threedimensional crystal. The electron density function for the whole crystal (see Appendix 3.A, p. 183) is the convolution of the L(r) function with pM(r):
As a consequence of eqns (3.A.35), (3.A.30), and (3.22) the amplitude of the wave scattered by the whole crystal is
+
where V is the volume of the unit cell and r i = ha* + kb* Ic* is the generic lattice vector of the reciprocal lattice (see pp. 635). If the scatterer object is nonperiodic (atom, molecule, etc.) the amplitude of the scattered wave FM(r*) can be nonzero for any value of r*. On the contrary, if the scatterer object is periodic (crystal) we observe a nonzero amplitude only when r* coincides with a reciprocal lattice point: The function F,(r*) can be represented by means of a pseudolattice: each of its points has the position coinciding with the corresponding point of the reciprocal lattice but has a specific 'weight' FM(H)/V. For a given node the diffraction intensity I,, will be' function of the square of its weight. Let us multiply eqn (3.25) scalarly by a , b, c and introduce the definition (3.5) of r*: we obtain The directions s which satisfy eqns (3.26) are called diffraction directions and relations (3.26) are the Laue conditions. Finiteness of the crystal may be taken into account by introducing the form function @(r): @(r) = 1 inside the crystal, @(r) = 0 outside the crystal. In this case we can write
1
151
152
1
Carmelo Giacovazzo
and, because of eqn (3.A.35), the amplitude of the diffracted wave is where O(r) exp (2nir* r) dr =
D(r*) =
exp (2nir'
.r) dr
S
and 52 is the volume of the crystal. Because of eqn (3.A.40) the relation (3.27) becomes
+ 1 , FM(H) x 53
=
D (r*  r i ) .
If we compare eqns (3.28) and (3.24) we notice that, going from an infinite crystal to a finite one, the pointlike function corresponding to each node of the reciprocal lattice is substituted by the distribution function D which is nonzero in a domain whose form and dimensions depend on the form and dimensions of the crystal. The distribution D is identical for all nodes. For example, let suppose that the crystal is a parallelepiped with faces Al, A,, A,: then D(r *  ,Ad2 ,Ad2 ,A312 exp [2ni(x * x y *y z *z)] dx dy dz.
+
A1/2
A2/2
+
A3/,
If we integrate this function over separate variables, it becomes, in accordance with Appendix 3.A, p. 174 D(r*) =
sin (nAlx*) sin (nA,y *) sin (nA3z*) nx * JCY * nz *
(3.29)
Each of the factors in eqn (3.29) is studied in Appendix 3.A and shown in Fig. 3.A.1 (p. 174). We deduce: 1. The maximum value of D(r*) is equal to A,A,A,, i.e. to the volume S2 of the crystal; 2. The width of a principal maximum in a certain direction is inversely proportional to the dimension of the crystal in that direction. Thus, because of the finiteness of the crystals each node of the reciprocal lattice is in practice a spatial domain with dimensions equal to A;'. In Fig. 3.6 some examples of finite lattices with the corresponding reciprocal lattices are shown. When we consider the diffraction by a crystal the function FM(H)bears the name of structure factor of vectorial index H (or indexes h, k, 1 if we make reference to the components of r;) and it is indicated as:
x fi N
FH=
exp (2nirG . q )
j=l
where N is the number of atoms in the unit cell. In accordance with
The diffraction of Xrays by crystals
1
153
Fig. 3.6. Direct and reciprocal lattices for: (a) a onedimensional lattice; (b) a twodimensional lattice in the form of a rectangle; (c) a twodimensional lattice in the form of a circle; (d) a cubic crystal in the form of a sphere; (e) a cubic crystal in the form of a cube; (f) a crystal in the form of a parallelepiped (from Kitaigorodskii, A. 1. (1951). The theory o f crystal structure analysis, Consultants Bureau, New York).
p. 64 we write
xf j N
FH=
+
(3.30a)
fi sin 2nHXj.
(3.30b)
exp (2niAxj) = A H iBH
j=1
where
x N
AH=
N
f j cos ~ J G H X ~ BH , = j=1
j=1
According to the notation introduced in Chapter 2, we have indicated the vector as rlT, and the transpose matrix of its components with respect to the reciprocal coordinates system as H = (hkl). In the same way I;. is the jth positional vector and the transpose matrix of its components with respect to the direct coordinates system is xi = [xi yj zj]. In a more explicit form (3.30a) may be written
Fhkl =
xf j
imag. axis
exp 2ni(hxj + kyj
I
+ lzj).
j=1
In different notation (see Fig. 3.7)
FH= IFH(exp (iq,) where qH= arctan (BH/A.HI.
(3.31)
'
qHis the phase of the structure factor FH. If we want to point out in eqn (3.30a) the effect of thermal agitation of the atoms we write, in accordance with p. 149 and Appendix 3.B real axis
N
FH=
fOj j=1
exp (2niHxj  8 n 2 4sin2 8/A2)
Fig. 3.7. F, is represented in the Gauss pla_nefor a crystal structure with N = 5. It is cui = 2zHX,.
154
1
Carmelo Giacovazzo N
&, exp (2niAXj  2n2AU?H)
FH= j=l
depending on the type of the thermal motion (isotropic or anisotropic) of the atoms. f,, is the scattering factor of the jth atom considered at rest. Let us note explicitly that the value of FH, in modulus and phase, depends on the atomic positions i.e. on the crystal structure. Details of the structure factors calculation from a known structural model are given on pp. 878 and Appendix 2.1.
Bragg's l a w A qualitatively simple method for obtaining the conditions for diffraction was described in 1912 by W. L. Bragg who considered the diffraction as the consequence of contemporaneous reflections of the Xray beam by various lattice planes belonging to the same family (physically, from the atoms lying on these planes). Let 8 be (see Fig. 3.8) the angle between the primary beam and the family of lattice planes with indices h, k, 1 (having no integer common factor larger than unity). The difference in 'path' between the waves scattered in D and B is equal to AB BC = 2d sin 6. If it is multiple of A then the two waves combine themselves with maximum positive interference:
+
Fig. 3.8. Reflection of Xrays from two lattice dis planes belonging to the family H = (h, k, I). the interplanar spacing.
2dHsin 8 = nA, Since the Xrays penetrate deeply in the crystal a large number of lattice planes will reflect the primary beam: the reflected waves will interfere destructively if eqn (3.32) is not verified. Equation (3.32) is the Bragg equation and the angle for which it is verified is the Bragg angle: for n = 1, 2, . . . we obtain reflections (or diffraction effects) of first order, second order, etc., relative to the same family of lattice planes H. The point of view can be further simplified by observing that the family of fictitious lattice planes with indices h' = nh, k' = nk, I' = nl has interplanar spacing d H = j dHIn. NOWeqn (3.32) can be written as
/
I
0
/ Fig. 3.9. Reflection and limiting spheres.
(3.33) 2(dH/n)Sin 6 = 2dH,sin 8 = where h', k', I' are no longer obliged to have only the unitary factor in common. In practice, an effect of diffraction of nth order due to a reflection from lattice planes H can be interpreted as reflection of first order from the family of fictitious lattice planes H ' = n H. It is easy to see now that eqn (3.33) is equivalent to eqn (3.25). Indeed, if we consider only the moduli of eqn (3.25) we will have, because of eqns (2.14) and (3.6), r* = 2 sin 8/A = lld,.
The reflection and t h e limiting spheres Let us outline (see Fig. 3.9) a sphere of radius l/A in such a way that the primary beam passes along the diameter 10. Put the origin of the reciprocal
.
The diffraction of Xrays by crystals lattice at 0. When the vector rtT, is on the surface of the sphere then the corresponding direct lattice planes will lie parallely to IP and will make an angle 6 with the primary beam. The relation OP=r~=l/dH=IOsin6=2sinB/A holds, which coincides with Bragg's equation. Therefore: the necessary and sufficient condition for the Bragg equation to be verified for the family of planes (hkl) is that the lattice point defined by the vector ri lies on the surface of the sphere called the reflection or Ewald sphere. AP is the direction of diffracted waves (it makes an angle of 28 with the primary beam): therefore we can suppose that the crystal is at A. For Xrays and neutrons A  (0.52) A, which is comparable with the dimensions of the unit cell (10A): the sphere then has appreciable curvature with respect to the planes of the reciprocal lattice. If the primary beam is monochromatic and the crystal casually oriented, no point of the reciprocal lattice should be in contact with the surface of the Ewald sphere except the (000) point which represents scattering in the direction of the primary beam. It will be seen in Chapter 4 that the experimental techniques aim to bring as many nodes of the reciprocal lattice as possible into contact with the surface of the reflection sphere. In electron diffraction A 0.05 A: therefore the curvature of the Ewald sphere is small with respect to the planes of the reciprocal lattice. A very high number of lattice points can simultaneously be in contact with the surface of the sphere: for instance, all the points belonging to a plane of the reciprocal lattice passing through 0. If r i > 2/A (then dH< A/2) we will not be able to observe the reflection H. This condition defines the socalled limiting sphere, with centre 0 and radius 2/A: only the lattice points inside the limiting sphere will be able to diffract. Vice versa if A > 2a,,,, where a,,, is the largest period of the unit cell, then the diameter of the Ewald sphere will be smaller than rg,, (the smallest period of the reciprocal lattice). Under these conditions no node could intercept the surface of the reflection sphere. That is the reason why we can never obtain diffraction of visible light (wavelength 5000 A) from crystals. The wavelength determines the amount of information available from an experiment. In ideal conditions the wavelength should be short enough to leave out of the limiting sphere only the lattice points with diffraction intensities close to zero due to the decrease of atomic scattering factors.

Symmetry in reciprocal space There are some relationships among structure factors relative to different indexes H which are originated either from the physics of diffraction and from the crystal symmetry. Let us give the relevant rules.
Friedel law
+
In accordance with eqn (3.30) we write FH= A H iBH.Then it will also be: F, = AH iBH and consequently Q)H
= Q)n
(3.34)
1
155
156
1
Carmelo Giacovazzo The value of V  H is opposite to the value of rpH.Since the intensities IHand I, depend on and IF^^^ respectively, we have
From that the Friedel law is deduced, according to which the diffraction intensities associated to the vectors H and H of the reciprocal space are equal. Since these intensities appear to be related by a centre of symmetry, usually, although imperfectly, it is said that the diffraction by itself introduces a centre of symmetry.
Effects of symmetry operators in the reciprocal space Let us suppose that the symmetry operator C = (R, T) exists in direct space. Then the points r;. and r,! whose coordinates are related by X,! = RXj T are symmetry equivalent. We wonder which kind of relationships brings in the reciprocal space the presence of the operator C. Since
+
xfi x fi N
F"R exp ( ~ J T ~ H=T )
.
exp ( ~ J T ~ H R Xexp ; ) (2niHT)
;=l
N
=
exp ~ J T ~ H ( R +XT); = FH
j=1
we can write F", = FHexp (  ~ J T ~ H T ) .
(3.35)
Sometimes it is convenient to split eqn (3.35) into two relations:
From (3.36) it is concluded that intensities ZH and I,qRare equal while their phases are related by eqn (3.37). The most relevant consequences of eqn (3.35) are described in the following.
Determination of the Laue class The Laue class of a crystal (see p. 17) may be determined by means of the qualitative examination of the diffraction intensities. Let Pl[(x, y, z)] be the space group (symmetry equivalent positions are shown in square brackets). The only symmetry operator is the identity, and its use in eqn (3.36) does not give us any useful result. Anyhow, because of the Friedel law = IFHI holds. If the space group is PI [(x, y, z), (2, jj, Z)] we can use R2 in eqn (3.36) and consequently obtain F, = FH. In this case the Friedel law does not add any additional observable relationship. In conclusion, the diffraction intensities from crystals with symmetry P1 and PI will both show a centre of symmetry or, in other words, they will show the symmetry of the Laue class I. As a further example let P2 [(x, y, z), (x,y, 2)] be the space group. By introducing R, in eqn (3.36) and by applying the Friedel law we obtain the following relationship (symmetry equivalent reflections):
The diffraction of Xrays by crystals
If the space group was Pm [(x, y, z), (x, y, z)], by using R2 and by applying the Friedel law we would obtain eqn (3.38) again. If the space group was P2/m eqn (3.38) would be obtained again only by using matrices R2, R3, and R, in eqn (3.36). This time the Friedel law does not add any additional relationship to those obtained from eqn (3.36). We can conclude that the symmetry of the diffraction intensities from crystals belonging to space groups P2, Pm and P2/m is that of the Laue class 2/m. The reader will easily verify that the crystals belonging to groups P222, Pmm2, and P2/m 2/m 2/m show intensity symmetry of the 2/m 2/m 2/m Laue class: IFhkrl = I F h d = = IFiid =IFl=IFhkl hkll  IFhill = IFhkil and those belonging to space groups P4, ~ 4 P4/m , show the intensity symmetry
of the Laue class 411x1.
Determination of reflections with restricted phase values Let us suppose that for a given set of reflections the relationship HR = H is satisfied. If we apply (3.37) to this set we will obtain 2qH= 2nHT + 2nn from which qH= XHT
+ nn.
(3.39)
Equation (3.39) restricts the phase qHto two values, XHT or X(HT+ 1). These reflections are called reflections with restricted phase values, or less properly, 'centrosymmetric' . If the space group is centrosymmetric the inversion operator
will exist. In this case every reflection is a restricted phase reflection and will assume the values XHT or ~ ( H +T 1). If the origin is assumed on the centre of symmetry then T = 0 and the permitted phase values are 0 and n. Then according to eqn (3.30b), FHwill be a real positive number for q, equal to 0, and a negative one for qHequal to n. For this reason we usually talk in centrosymmetric space groups about the sign of the structure factor instead of about the phase. In Fig. 3.10 FHis represented in the complex plane for a centrosymmetric structure of six atoms. Since for each atom at q another symmetry equivalent atom exists at q, the contribution of every couple to FHwill have to be real. As an example of a noncentrosymmetric space group let us examine P2A2,, [(x, y, z), (i x, J , 4 + z), ( i + x, 4  y, 2), (ii,+ y,  z)] where the reflections (hkO), (Okl), (h01) satisfy the relation HR = H for R = R2, R3, R4 respectively. By introducing T = T2 in eqn (3.39) we obtain
1
157
158
( Carmelo Giacovazzo imag. axis
Fig. 3.10. F, is represented in the Gauss plane for a centrosymmeJric crystal structure with N = 6. It is q = ZRHX,.
qhko = ( n h l 2 ) + nn. Thus qhkowill have phase 0 or n if h is even, phase fn12 if h is odd. By introducing T = T3 in eqn (3.39) we obtain qok[ = (nk12) + n n : i.e. q o k l will have phase 0 or n if k is even, fA12 if k is odd. In the same way, by introducing T = T, in eqn (3.39) we obtain qhol= (n112) + n n : i.e. q h 0 i will have phase 0 or n if 1 is even, fn12 if 1 is odd. 4 )to (3x14, 7 ~ 1 4or ) to ( n / 6 , 7 n / 6 )or Phase restrictions to ( ~ ~ 154~, ~ 1or . . . , can be found for some space groups. The allowed phase values depend Table 3.1. Restricted phase reflections for the 32 crystal classes Point group
Sets of restricted phase reflections
1 1 m 2 2/m mm2 222 mmm 4
None All (0, k, 0 ) (h,O, I ) All [ ( h ,k, 0 ) masks (h, 0, O), (0, k, 0)l Three principal zones only All (h, k,O) (h, k, 0 ) ; (0,0, I ) All (h, k,O); {h,O, I ) ; { h , h, I ) [(h, k, 01, { h , h, 011; [ { h , 0, I ) , (O,O, 111 [(h, k, 01, { h , 0,0), { h , h, O)] All None All { h, O,fi,O) { h , 0, h, I ) All ( h , k,O) (O,O, 1 ) All [ { h , h, I ) , { h , h, 0 ) , (O,O, / ) I [(h, k, 01, { h , h, 0), { h , 0, O)] (h,k,O); (h,O,I); ( h , h , I ) All { h, k, 0 ) All ( { h , k. O), { h ,h, 011 { h , k,O}; { h , h, I } All
p
4
4/ m 422 42m
p
p
p
The diffraction of Xrays by crystals
on the translational component of the symmetry element and on its location with respect to the cell origin. A different point of view may also be used: the existence of reflections with restricted phase is due to the presence of symmetry elements which at least in projection simulate the centre of inversion. For instance, the projection of a structure in P2,2,2, along the c axis is centrosymmetric: correspondingly, the reflections belonging to the zone (hkO), being insensitive to the z coordinate, have restricted phase values. The reader will easily verify that zones orthogonal to axes 2 , 4 , 4, and 6 (and, of course, to the corresponding screw axis) have symmetry restricted phases, as well as zones parallel to the axes 2 , 4, 6. In Table 3.1 the sets of restricted phase reflections are given for the 32 crystal classes.
Systematic absences Let us look for the class of reflections for which HR = H and let us apply eqn (3.35). This relation would be violated for those reflections for which AT is not an integer number unless IFHI = 0 . From this fact the rule follows: reflections for which HR = H and AT is not integer will have diffraction intensity zero or, as usually said, will be systematically absent or extinct. Let us give a few examples. In the space group P2, [ ( x , y , z ) , ( 3 , y 1, Z ) ] the reflections (OkO) satisfy the condition HR, = H. If k is odd, HT, is semiinteger. Thus, the reflections (OkO) with k # 2n are systematically absent. In the space group P4, [ ( x , y, z ) , (2, P, 1 + z ) , (JJx, , +z ) , ( y ,3, 2 z ) ] only the reflections (001) satisfy the condition HR, = H for j = 2, 3, 4 . Since HT, = 112, AT3= 114, HT4= 3114, the only condition for systematic absence is I # 4n, with n integer. In the space group PC [ ( x , y , z ) , ( x , j , z + +)I the reflections (h01) satisfy the condition HR, = H. Since HT, = 112 the reflections (h01) with 1 # 2n will be systematically absent. Note that the presence of a glide plane imposes conditions for systematic absences to bidimensional reflections. In particular, glide planes opposite to a, b, and c impose conditions on classes (Okl), (hol), and (hkO) respectively. The conditions will be h = 2n, k = 2n, 1 = 2n for glide planes of type a, b, or c respectively. The reader can easily check the data listed in Table 3.2. Let us apply now the same considerations to the symmetry operators centring the cell. If the cell is of type A, B, C, I, symmetry operators will exist whose rotational matrix is always the identity while the translational matrix is:
+
+
respectively. If we use these operators in eqn (3.35) we obtain: the relation HR = H is satisfied for any reflection; the systematic absences, of threedimensional type, are those described in Table 3.2. A cell of type F is simultaneously A, B, and Ccentred, so the respective conditions for systematic absences must be simultaneously valid. Conse
1
159
160
1
Carmelo Giacovazzo Table 3.2. Systematic absences Set of reflections
Symmetry elements
Conditions none h+k+l=2n h+ k=2n k+l=2n h+l=2n h+ k=2n k+l=2n h+l=2n h+ k+I=3n hk+I=3n
Lattice
hkl
i
Glideplane
11 ( 0 0 1 )
Glideplane
11 ( 1 0 0 )
a b n d
hku
b c n d
Okl
C
Glideplane
11 (1 1 0 )
b n d
Screwaxis
11 b
2 1 ~ 4 ~ 4 1 ~ 4 ~
hhl
Oku
quently only the reflections for which h, k, and 1 are all even or all odd will be present. The same criteria lead us to establish the conditions for systematic k 1# 3n for obverse setting and h  k 1# 3n for reverse absences (h setting) for a hexagonal cell with rhombohedra1 lattice. Rules for systematic absences may be also derived by using the explicit algebraic form of the structure factor. Suppose, for example, that the space group contains a cglide plane perpendicular to the b axis (then ( x , y, z) and (x, j , z + 4) will be symmetry equivalent points). The structure factor is then
+ +
+
Nl2
f j exp 2ni(hx,
Fhkl=
+ kyj + lz,)
j=1
+
NI2
f j exp 2ni[hxj  ky, ,=I
+ l(z, + ;)I.
The diffraction of Xrays by crystals
For 1 even
~ 1 2
+
Fhkl= 2 x fi exp [2ni(hxj lz,)] cos 2nkyj; j=1
for 1 odd Ni2
Fhkl= 2 x fi exp [2ni(hxj
+ lz,)] sin 2nky,.
j=l
It is easily seen that Fhol= 0 for 1 odd, in accordance with our previous results.
Unequivocal determination of the space group Determination of the space group is an important first step in any crystal structure analysis. From the qualitative examination of the diffraction intensities (which leads to the identification of the Laue class) and from the analysis of the systematic extinctions 58 space groups are unequivocally determinable (without making any distinction between enantiomorph couples). The symbols of these groups are printed in bold character in Table 1.9. As an example, suppose that relations (3.38) and systematic absences (OkO) for k = odd and (h01) for I = odd are observed. Then the space group P2Jc is unequivocally deduced since: (1) the cell has to be primitive (no systematic absences involving threedimensional reflections are observed); (2) the Laueclass is 2/m (from (3.38)); (3) a twofold screw axis along b and a cglide plane normal to b do exist according to systematic absences. Sometimes the identification of space group extinctions is disturbed by the presence of one or a few reflections seemingly violating one of the extinction rules (e.g. only one (hkO) reflection with h k =odd has a meaningful nonzero intensity). One way to produce such forbidden reflections is the Renninger effect, described in Appendix 3.B, p. 191, which occurs when two or more reciprocal lattice points happen to intersect the reflection sphere simultaneously. One way to avoid the Renninger effect is to rotate the crystal about the reflecting plane's normal and repeat measurements. Space groups which are not unequivocally determined could, with few exceptions, be unambiguously identified if their point group is known. The methods which can give us information about point groups have been schematically described in Chapter 1 (p. 15) (crystal habit, piezoelectricity, pyroelectricity, etc.). Let us add to them the anomalous dispersion effects (see p. 165) and the statistical methods (see Chapter 5, p. 322) based on the expectation that the distribution of the intensities is influenced by the presence of symmetry elements and, in particular, it is different for centrosymmetric and noncentrosymmetric space groups.
+
Diffraction intensities The theory so far described is called kinematic: basically it calculates interference effects between the elementary waves scattered inside the
1
161
162
1
Carmelo Giacovazzo volume of the crystal. However, it neglects two important phenomena: when the incident wave propagates inside the crystal its intensity decreases gradually because a part of its energy is transferred to the scattered beam or it is absorbed; the diffracted waves interfere with each other and with the incident beam. The theory which takes into account all these phenomena and analyses the wave field set up as a whole is called the dynamic theory of diffraction. It was initiated by ~wald:[']later on Laue showed that Ewald's theory is equivalent to analysing the propagation of any electromagnetic field through a medium having a periodically varying complex dielectric constant. The description of the dynamical theory is out of the scope of this book. The reader is referred to specialist books or review articles[2331 for exhaustive information. Only a dynamical effect of particular importance for crystal structure analysis, the Renninger effect, will be here described (in Appendix 3.B, p. 191) in any detail. Other dynamical interactions will be described on the basis of the kinematical theory properly modified by Darwin and other authors. Dynamic effects develop gradually in a crystal: it may be shown that for sufficiently small thicknesses the incident beam is not weakened considerably, the diffracted waves are not yet so strong as to give rise to remarkable interference effects with the incident beam and the effects of absorption are negligible. Under these conditions (theoretically, thicknesses o, the expression of Ed is not very different from that of a free electron. Therefore Thomson scattering is only applicable when o >> w,. We define now the scattering factor for an electron as the ratio
While the imaginary term is always positive, the real term is negative when o < wo and positive when o > 01,. From the quantumtheory point of view, the frequency wo coincides with that of a photon with just sufficient energy to eject the electron from the atom. Such an energy corresponds to the wavelength A, = 2nc/wo corresponding to the absorption edge. Thus it may be expected that a remarkable deviation from Thomson scattering will arise when the primary beam wavelength is close to an absorption edge of the atom being considered. An important question is whether Af' and f " vary with diffraction angle. Existing theoretical treatments suggest changes of some per cent with sin e/A but no rigorous experimental checks have been made so far: therefore in most of the routine applications Af' and f " are considered to be constant. For most substances at most Xray wavelengths from conventional sources dispersion corrections are rather small. Calculated values for CrK, (A = 2.291 A), CuK, (A = 1.542 A), and MoK, (A = 0.7107 A) are listed in the International tables for xray crystallography, Vol. 111. In some special cases ordinary Xray sources can also generate relevant dispersion effects. For example, holmium has the L3 absorption edge (1.5368A) very close to CuK, radiation: in this case the holmium scattering factor is not the same for K,, and K,, wavelengths. The following dispersion corrections are cal~ulated:[~~1 CuK,,(A= 1.5406 A): CuK,,(A = 1.5444 A):
Af = 15.41
fl'
3.70
Aft =  14.09
fu
3.72

Furthermore, the holmium L2 absorption edge (211.3905 A) is very close to the CuKBwavelength (A = 1.3922 A), so giving rise to Af'= 11.88,
f"~8.75.
The diffraction of Xrays by crystals
1
167
Fig. 3.13. Anomalous scattering terms A f ' and P'for: (a) gadolinium near the L3 edge; (b) samarium near the L, edge.
If synchrotron radiation is used, its intense continuous spectrum may be chosen to high precision in order to provoke exceptionally large anomalous scattering. Very large effects have been measured["] for rareearth elements in the trivalent state near L3 absorption edges (corresponding wavelengths are of crystallographic interest because edges span from 2.26A for lanthanum to 1.34 A for lutetium). In Fig. 3.13 we show the anomalous scattering terms Af' and f" for gadolinium and samarium near the L3 absorption edge: spectacular effects as large as 30 electrons/atom could be measured. Since anomalous dispersion may induce substantial variation of the diffracted intensities depending on the wavelength used, anomalous scattering is an important tool for solving crystal structures (see Chapter 8). Several recent works suggest an important role for multiplewavelength methods: the power of such methods depends on the distances between the working points representing f i n the complex plane.[l21As an example, we plot in Figs. 3.14 (a) and (b) the complex scattering factor Af' if" near the L3 edge for gadolinium and samarium respectively. Now we will give only a few elementary ideas about the effects of anomalous dispersion: we postpone the methodological aspects for crystal structure analysis until Chapter 8. Let suppose that a noncentrosymmetric crystal contains N atoms in the unit cell from which P are anomalous scatterers and the remaining Q = N  P atoms are normal scatterers. Then
+
where + and  indicate that the magnitudes are calculated for the vectors H and  H respectively. The subscripts P and Q indicate that the structure factors are calculated only with the contribution of P or Q atoms
(b) ~ ~ ; ~ ; ~ ~ L edge; (b)samarium nearthe ne edge.
~
~
~
~
168
1
Carmelo Giacovazzo
imag. axis
imag axis
1
real axis
Fig. 3.15. (a) Relation between F, and F, when anomalous dispersion is present; (b) relation between F, and F!, when anomalous dispersion is present.
respectively:
x f,! P
Fb+ =
exp 2niHXj;
j=1
The vectors F+ and F are described in Fig. 3.15(a). In Fig. 3.15(b) F + and (F)* are shown: the latter is the complex conjugate of F and they are symmetric with respect to the real axis: The difference AZ = J F + ~IF(^ ~ is known as the Bijvoet difference[13] and can be easily calculated by means of Fig. 3.15(b):
from which
AZ = 4 (F'JIF:( cos q. Furthermore In general, as we can see, IFHI= I F,1 is no longer valid, i.e. the Friedel law is not satisfied in the presence of anomalous dispersion. The value of AZ depends on the collinearity of F; and F&. If they are collinear then (F+I= IF1: but this happens by mere chance. AZ is a maximum when Fp and FQare approximately at the right angles. The Friedel law is satisfied if: the structure is centrosymmetricin this case IF+[and IFI are always equal; the reflection is centrosymmetric even if the structure is noncentrosymmetric; the crystal is constituted of only one chemical element which is the anomalous scatterer. As a last observation it should be mentioned that besides Xray, neutron and gammaray anomalous dispersion are also very useful in crystal structure analysis. Neutron anomalous dispersion techniques employ
The diffraction of Xrays by crystals
nuclear isotopes with resonances in the range of thermalneutron energies (see p. 198 for further details). Gammarays are elastically scattered by the electrons of the atoms in the crystal. An elastic resonant scattering by the nucleus (Mossbauer effect) also occursthe transition involves energies comparable with those employed in conventional Xray diffraction. Since both the processes are coherent, scattering by resonant nuclei (there are no other nuclear scattering contributions) and by electrons can occur simultaneously and interfere with each other. An ideal nucleus for gammaray resonance is j7Fe; its 14.4 keV resonance corresponds to a wavelength of 0.86 A. A widely used experimental setup includes a radioactive source which emits the 14.4 keV radiation in the decay of the parent isotope j7Co. This produces a resonance effect in 57Fe (this atom may naturally be present in the crystal or implanted by techniques such as those used for isomorphous replacement) which is superimposed on the various Bragg reflections upon the gamma radiation elastically scattered by all the atoms in the crystal, iron atoms included. Since 5 7 ~ has e a natural abundance of about 2.2 per cent, isotopic enrichment techniques must be applied in order to provide a sufficiently large resonant scattering. The frequency of the incident radiation may be modified by moving the radiation source, at low velocity (some mm sl), towards or away from the crystal (linear Doppler effect). The anomalous scattering amplitudes increase dramatically in going from Xray to neutron to gammaray. Conversely, the intensities of the radiation sources decrease dramatically. This is the most severe drawback for the use of gamma rays: relatively large signals are produced by relatively very weak radiation sources.
The Fourier synthesis and the phase problem If the structure factors are known in modulus and phase the atomic positions are unequivocally determinable. Indeed, according to eqn (3.A.16) the electron density is the inverse Fourier transform of F(r*): F(r*) exp (2nir*
p(r) = 1
=
r) dr*
Fhklexp [2ni(hx
+ ky + lz)].
(3.45)
Vh,k,l=2
x = [x, y, z] are the fractional coordinates of the point defined by the vector r. The atomic positions will correspond to the maxima of p(r). If in eqn (3.45) we sum up the contributions of H and H we will have FHexp (2niHX) + F  H exp ( 2 n i ~ x ) = (AH+ iBH)eXp (  ~ J G ~ H + X )(AH iBH)eXp ( ~ G ~ H X ) = 2[AHcos 2 n ~ + x BHsin 2nHXI
1
169
170
(
Carmelo Giacovazzo
from which
x [A,,, cos 2n(hx
+ ky + l z ) + Bhklsin 2n(hx + ky + lz)] (3.46)
is obtained. The righthand side of (3.46) is explicitly real and is a sum over a half of the available reflections. The mathematical operation represented by the synthesis (3.46) can be interpreted as the second step in the process of formation of an image in optics. The first step consists of the scattering of the incident radiation which gives rise to the diffracted rays with amplitudes FH.In the second step the diffracted beams are focused by means of lenses, and by interfering with each other they create the image of the object. There. are no physical focusing lenses for Xrays but they can be substituted by a mathematical lens (exactly, by Fourier synthesis (3.46)). Because of the decrease of the atomic scattering factors the diffraction intensities (and consequently IFH\)weaken 'on average' with the increase of sin B/A, and can be considered zero for values above a given (sin B/A),,, = 1/(2dmin).Since the reflections at high values of sin B/A, give the fine details of the structure (small variations of the atomic coordinates can produce big changes in highangle structure factors) the quantity dm, is adopted as a measure of the natural resolution of the diffraction experiment. dmin depends on different factors such as: the chemical composition of the crystal (heavy atoms are good scatterers even at high values of sin B/A), the chemical stability under the experimental conditions of temperature and pressure, the radiation used (the resolution improves when we pass from electrons to Xrays and neutrons), the temperature of the experiment. Roughly speaking, for Xrays dm,, can reach the limit of 0.5 A in inorganic crystals, 0.71.5 A in organic crystals, and 1.03 A in protein crystals. Because of the limit of natural resolution or of an artificially introduced limit (for instance in order to save time and calculations) the electron density function will be affected by errors of termination of series. The effect can be mathematically evaluated by calculating the function pr(r) available via the function @(r*) is the form function: @(r*)= 1 inside the available reflection sphere, @(r*)= 0 outside this sphere. According to eqn (3.A.35) we have
Fig. 3.16. (a) Electron density p ( r ) ; (b) electron density obtained via a Fourier synthesis with series termination errors.
If r * is the radius of the available reflection sphere, according to Appendix 3.A, p. 181, T[@(r*)] is a function with a maximum at r = 0 and the subsidiary maxima of weight decreasing with l/rL. The effect of the convolution (3.47) is qualitatively represented in Fig. 3.16. In particular, even if p(r) is positive everywhere, pl(r) can be negative in more or less extended regions: the atomic peaks can be broad and surrounded by a series of negative and positive ripples of gradually decreasing amplitude. The number of reflections used in practice in eqn (3.46) varies from several tens or hundreds, for unit cells of small dimensions, to several tens of thousands for macromolecules.
The diffraction of Xrays by crystals
In order to reveal the atomic positions, pr(r) is sampled upon a threedimensional grid whose spacings along each of the unitcell axes have to be fixed with some care. If the grid is too coarse the interpolation between grid points to find the maximum of the electron density may be uncertain, if the grid is too fine a great deal of computing may be unnecessary. In absence of symmetry, at a resolution dm,, there are
measurable (only N,/2 independent) reflections and the number of grid points is Np = v / h 3 where A is the grid spacing (say 0.20.4 A in the three directions). In practical cases N, and N, are rather large: for instance, for V = 1000 A3, dmin= 0.8 A , A = 0.25 A, we have N, 8180 and Np 64 000. If symmetry is present the amount of calculation is smaller. The number of independent reflections to be measured is roughly N,/(tm) where z is the centring order of the cell and m the multiplicity factor of the Laue class (this is not strictly exact as the multiplicity factor refers to general reflections of type (hkl) and may be different and less than m for certain zones of reflections). Furthermore, it will be sufficient to sample p upon the grid points lying inside the asymmetric unit for reconstructing the whole content of the cell. For instance, let P2/m be the space group with a = 7.8 A, b = 16.2 A and c = 8.1 A and /3 = 93'. If we divide a and c into 33 and b into 66 intervals the grid spacing will have a sufficient and almost identical resolution in all three directions. The number of grid points lying inside the asymmetric unit (114 of the unit cell) is now 33 x 33 x 17 = 18 513. Very often the volume of the unit cell is much larger than 103A3 (V > lo6hi3 is not infrequent for macromolecules). Thus even with the use of highspeed computers, the calculation of p is a fairly arduous task involving timeconsuming procedures. Different algorithms are used to make calculations faster. The most convenient are the BeeversLipson technique and the fast Fourier transform algorithm by Cooley and Tookey (see Chapter 2, pp. 8890, and Appendix 2.1). Unfortunately, it is not possible to apply eqn (3.47) only on the basis of information obtained directly from Xray diffraction. Indeed, according to eqn (3.41), only the moduli IFHIcan be obtained from diffraction intensities because the corresponding phase information is lost. This is the socalled crystallographic phase problem: how to identify the atomic positions starting only from the moduli IFH(.A general solution to the problem has not been found, but there are methods we can successfully apply (see Chapters 5 and 8).


Modulated crystal structures So far our attention has been devoted to condensedmatter systems with perfect threedimensional space group symmetry. In recent years numerous systems have been found which can be considered as perfect crystals with periodic distortion (from some basic structure) of the atomic positions (displacive modulation) and/or of the occupation probability of atoms
1
171
172
1
Carmelo Giacovazzo (density modulation). The presence of periodic distortions is revealed from the existence of the socalled satellite reflections, generally weak, which are regularly distributed around the socalled main reflections. If satellite reflections can be labelled by rational indices in terms of the reciprocal lattice L* of the basic structure, then the distortion periods are commensurate with the translation periods of the basic structure and a new lattice Lr* can be introduced which contains L*. In such a case the main and the satellite reflections are called substructure and superstructure reflections respectively (see page 80). For some crystals the positions of the satellite reflections vary continuously with respect to L*, depending on the temperature. In these cases we have to admit that satellite reflections can assume nonrational indices, or also, that the periodic distortions are incommensurable with the translation periods of the basic lattice. The result is the socalled incommensurately modulated structure (IMS). In order to prove the existence of satellite reflections we briefly examine the simple case of a onedimensionally displacively modulated structure when the displacement vector field is a harmonic function.[76] In a perfect crystal the jth atom in the unit cell defined by the lattice vector r,, = ua + vb + wc is located at r,,, = ry ru. In a harmonically modulated crystal it will be
+
r U= , ry
+ ru + g, sin [2nK . (ry + ru)  @,I,
where ry is now the average position of the jth atom, and gj and 4, are its displacement wave amplitude and phase respectively. K is the modulation vector, which may be expressed in the reciprocal space by K = k,a* k2b* k,c*. The contribution of the jth atom to the structure factor is now given by
+
+
fi(r*)C exp 2nir* {ry
+ ru + g, sin [2nK . (r? + ru)  @,I)
U
.
=fi(r*) exp (2nir* r ? ) x exp (2nir* r,,) u
x exp {2nir* .g, sin [2nK (r? + ru)  @,I)
(3.48)
where fi(r*) is the usual atomic scattering factor. To the last exponential term in (3.48) the Jacobi expansion
x +m
exp (iz sin a ) =
exp (ima)J,(z)
m=m
may be applied. Jm(see Fig. 3.17) is the Bessel function of the first kind of order m, satisfying J,(z) = (l)"Jm(z). Then (3.48) reduces to
.
.
fi(r*) exp (2nir* r y ) x exp (2nir* ru) x
u
x exp {im[@, 2nK
(r;
+ r,)]}J,(2nr* .g,)
m
=fi(r*) exp (2nir* r y ) x J_,(2nr*
.g,)
m
Fig. 3.17. The Bessel functions J,,(z),n = 0,1,2,3.
x exp {im(@, 2 n K . ry)}x exp [2niru . (r*  mK)]. u
The diffraction of Xrays by crystals
Provided the number of cells in the crystal is large enough the sum over u leads to (1/V) 6 ( H  r* + mK) where H = ha* kb* + lc*. Consequently the reflections occur for r* = H' = H + mK: for m = O we have main reflections (H' = H), for m # 0 satellites are defined. We also see that four indices are now needed for the identification of a diffraction effect. The structure factor of the reflections H' = (h, k, 1, n) may then be written as
+
N
=
.
A(H1)exp (2nir* r y ) ~ , ( 2 n ~ 'gj)(l)m j=l
X
exp (2niK
r;) exp (
[email protected]). (3.49).
According to Fig. 3.17 the average intensity of satellite reflections rapidly decreases with m. The above formalism may be extended to onedimensionally density modulated structures and also to multidimensional (harmonic or not) modulations. The above results also suggest that the reciprocal lattice of an IMS is aperiodic in the threedimensional space, and that the symmetry group of an IMS cannot be a threedimensional space group. We will show in Appendix 3.E (main references will also be given) that such a reciprocal lattice may be transformed into a periodic lattice provided a higherdimensional space is taken into consideration. Thus the symmetry in the threedimensional space can also be a poor residue of the full symmetry in the higherdimensional space.
Appendices 3.A Mathematical background
The Dirac delta function In a threedimensional space the Dirac delta function 6(r  ro) has the following properties 6 = 0 for r f ro,
6 = w for r = r o ,
6(rro) d r = 1 (3.A.1)
where S indicates the integration space. Thus the delta function corresponds to an infinitely sharp line of unit weight located at ro. It is easily seen that, if ro = xoa + yob + zoc, then 6 (r  rO)= 6 (X  x0) 6 (y  yo) 6 (2  20).
(3.A.2)
6(x xo) may be considered as the limit of different analytical functions. For example, as the limit for a + 0 of the Gaussian function
Of particular usefulness will be the relation
where x* is a real variable. It easily seen that (3.A.4) satisfies the properties
1
173
174
1
Carmelo Giacovazzo
Fig. 3.A.l. The function Y = (sin 2 n g x ) / ( n x )is plotted for g = 1,3. Clearly Y (  x ) = Y ( x ) .
(3.A.1): indeed its righthand side may be written as exp [2nix* ( x  xo)]dx * = lim
sin [2ng(x  xO)] n(xxo) '
The function sin [2ng(x  xO)]I[n(x  xO)]takes the maximum value 2g at x = x o (see Fig. 3.A.1), oscillates with period l / g , and has decreasing subsidiary maxima with increasing x : the value of its integral from w to + w is unitary for any value of g. Therefore the limit for g+ w of sin [2ng(x x O ) ] / [ n (x xO)]satisfies all the properties of a delta function. Consequently we can also write:
6 ( x  xo) = lim . g
sin [2ng(x  xo)] n(xx0) .
In a threedimensional space (3.A.4) becomes
d(r  4 ) =
I,*
exp [2nirS ( r  ro)]dr*
(3.A.6)
where S* indicates the r* space. Two important properties of the delta function are: 6 ( r  ro)= 6(ro r ) (3.A.7) f ( r )  ro) =f (r0)  ro). Indeed, for r # ro, left and righthand members of (3.A.7) are both vanishing, for r = ro both are infinite. From (3.A.7)
is derived. Consequently
The lattice function L Delta functions can be used to represent lattice functions. For example, in a onedimensional space a lattice with period a may be represented by +m
6 ( x  x,)
L(x) = ,=o(r
where x, = nu and n is an integer value. L ( x ) vanishes everywhere except at
The diffraction of Xrays by crystals
the points nu. Analogously a threedimensional lattice defined by unit vectors a, b, c may be represented by
+ +
where r,,,,, = ua ub wc and u, v, w are integer values. Accordingly, in a threedimensional space: (1) a periodic array of points along the z axis with positions z, = nc may be represented as += f'~(r>= w ) ~ ( Y I  2,); (3.A.12)
C
n=m
(2) a series of lines in the (x, z) plane, parallel to x and separated by c may be represented by
(3) a series of planes parallel to the (x, y) plane and separated by c is represented by +m
P3(r) =
C
S(z  z,).
(3.A.14)
,=m
The Fourier transform The Fourier transform of the function p(r) is given (for practical reasons we follow the convention of including 2n in the exponent) by r
p(r) exp (2nir* r) dr.
(3.A.15)
The vector r* may be considered as a vector in 'Fourier transform space', while we could conventionally say that r is a vector in 'direct space'. We show now that p(r) =
i*
F(r*) exp (2nir'
.r) dr*.
(3.A.16)
Because of (3.A.15) the righthand side of (3.A.16) becomes p(r')
(l*
.
exp [ 2 d r * (r'  r)] dr*) dr',
which, in turn, because of (3.A.6), reduces to
h
p(r') d(rf  r) dr' = p(r).
Relations (3.A.15) and (3.A.16) may be written as F(r*) = T[P(~)], p(r) = T'[F(r*)]
(3.A.17) (3.A.18)
respectively: we will also say that p is the inverse transform of F. Obviously TlT[p(r)l= p(r)
1
175
176
1
Carmelo Giacovazzo
but ?T[p(r)l = T[F(r*)I = ~ (  4 F(r*) is a complex function: by denoting A(r*) =
1 1
.
p(r) cos (2nir* r) dr
S
B(r*) =
p(r) sin (2nir* r) dr
S
then We calculate now the Fourier transform of p(r). Since
I,
P(r) exp (2nir'
r) dr =
I,
p(r) exp [2ni(r*
. r)] dr = A(r*)  iB(r*),
it may be concluded that where F(r*) is the complex conjugate of F(r*). If p(r) is symmetric with respect to the origin, say p(r) = p(r), because of (3.A. 17) and (3.A.21) it will result F(r*) = FV(r*), or, in other words, F(r*) will be a real function (B(r*) = 0). Vice versa, if F(r*) = F(r*) then p(r) is symmetric with respect to the origin. If p(r) = p(r) then F(r*) = FW(r*),so that F(r*) is pure imaginary (then A(r*) = 0).
Some examples of Fourier transform In a onedimensional space (3.A.15) becomes
Let us consider some examples for p(x). 1. Gaussian function :
Since +m
exp [$hu2
+ itu] du =
then T[p(x)] = F(x*) = exp (  2 ~ c ~ a ~ x * ~ ) .
(3.A.25)
It should be noted that the larger the 'width' of p(x), the smaller is that of F(x*) (see Fig. 3.A.2(a)) 2. Exponential function : p(x) = exp (g Ix 1). Its Fourier transform is the Cauchy function (see Fig. 3.A.2(b))
The diffraction of Xrays by crystals
Fig. 3.A.2. Examples of Fourier transform.
3. Rectangular aperture: for g < x < g,
p(x) = c
otherwise p(x) = 0.
Then ~ ( x *=) cly exp (2nix*x) dx = c
sin (2ngx *) nx *
which is plotted in Fig. 3.A.1.
4. Dirac delta function: p(x) = 6(x). Then (see Fig. 3.A.2(c)) +m
F(x*) =
6(x) exp (2nix*x) dx = 1.  CD
If p(x) = 6(x  a ) then F(x*) = exp (2niax*).
5. Onedimensional finite lattice: pp = C;E, 6(x  nu), where represents a set of N = 2p + 1 equally spaced delta functions. Then
x P
T[pp(x)] =
P
exp (2ninax*) =

cos (2nnax*) n=p
n=p l
2
2 sin (nax *) .=, 1 2 sin (nax *) =
2 cos (2nnax *) sin (nax *)
,sin [n(2n + l)ax*]  sin [n(2n  l)ax*]
pp
1
177
178
1
Carmelo Giacovazzo 
1 {sin [n(2p + l)ax*] sin [ n ( 2 p  l)ax*] 2 sin (nax *)
+ sin [n(2p  l)ax*] sin [n(2p  3)ax*] + sin [n(2p + l)ax*] sin [n(2p  l ) a x * ] ) sin [(2p + 1)nax*I  sin Nnax * sin nu*
sin m x *
'
The function sin N n y f(y)== is plotted in Fig. 3.A.3 for N = 6 , 7. When y = h ( h is an integer value) numerator and denominator of the righthand member of (3.A.27) both vanish. Then the value of f ( y ) (as determined from its limit for y +h ) is equal to N if N is odd; if N is even, then f ( y ) is equal to N if h is even, to N if h is odd. Between each pair of main maxima there are N  2 subsidiary peaks. Each main peak has width equal to 2 / N ( 1 / N is that of the subsidiary peaks), therefore it becomes sharper as N increases. Furthermore the ratio between the amplitude of a main peak with respect that of a subsidiary one increases with N. What we noted for f ( y ) may be easily applied to (3.A.26), whose principal maxima are at x* = hla. 6. Onedimensional infinite lattice :
According to 5 above the Fourier transform of p will be F ( x * ) = lim N=
sin Nnax * sin nax* '
The function F ( x * ) will present infinitely sharp lines at x* = h l a of weight l l a . Indeed sin N m x * 1 &*=lim sin nax * a
I& +&
Whichever the value of
Fig. 3.A.3. The function f ( y ) = s i n N n y l s i n n y for N = 6,7.
E',
I&
+'sin N n y sin n y dye
when N+m the value of the integral is unity.
The diffraction of Xrays by crystals
Consequently we could write
or, in words, the Fourier transform of a onedimensional lattice with period a is a onedimensional lattice with period l l a represented by delta functions with weight l/a.
7. Threedimensionalfinite lattice:
Its Fourier transform is F(r*) = =
x x x P1
P2
u=p1
u=p2
9
P3
.
exp (2nir* ru,u,w)
w=p3
. .x P2
exp (2niur' a )
.
exp (2nivr' b)
P3
2
exp (2niwr*
.e)
 sin Nina . r* sin N2nb r* sin N3nc. r* sin n a . r* sin n b r* sin JGC r* '
+
+
where Nl = (2p1 1), N2 = (2p2 I), N3 = (2p3 + 1). In accordance with point 5, each of the terms in the righthand side of (3.A.29) is maximum when r* satisfies with integer values of h, k, 1. It is easily seen that the solution of the above three equations is given by r: = h a *
+ kb* + lc*,
where
and V = a b A c. The vectors a*, b*, c* are nothing else but the basic vectors of the reciprocal lattice defined in 3 2.3. When Nl, N2, N3 are sufficiently large then F(r*) has appreciable values only in the reciprocal lattice points defined by the triple of integers H = (h, k, 1).
8. Threedimensional infinite lattice:
Its Fourier transform is the limit of (3.A.29) for Nl, N2, N3 tending to infinity: F(r*) =
lim N,,N~,N+
sinNlna . r * sinN2nb . r * sinN3ncar* sin n a . r* sin n b r* sin JGC r* '
.
According to points 6 and 7 F(r*) represents a threedimensional lattice by an array of delta functions the weight of which may be calculated by
1
179
180
1
Carmelo Giacovazzo integrating F(r*) on a domain dV* about a specific lattice point H. Since dV* = d h a * . dkb* ~ d l c = * V* d h d k d l because of the point 6 ~ ( r *d)v * = V*
I ', 'l
lim N,.N~.NP=
sin N,nh sin nh sin N2nk ,, sin nk
x dhl
E2
sin N,nl d l = V * = 1 v sin n~
dkkl_3 E3
arises. In conclusion, the Fourier transform of a lattice in direct space (represented by the function L(r)) is the function L(r*)IV:
which represents a lattice again (called the reciprocal lattice) in the Fourier transform space.
9. Fourier transform of a onedimensional periodic array of points along the z axis, as defined by (3.A.12). Then
10. Fourier transform of a lattice plane lying on the plane z = 0 and with translation constants a and b. Then p(r) = b(x  nu) 6(y  nb) S(z) and
Fourier transform of spherically symmmetric functions If p(r) is spherically symmetric we can represent r and r* in spherical polar coordinates (r, 0, cp) and (r*, %*, cp*) defined by (see Fig. 3.A.4)
,I.
x = r sin p, cos 8
. . /
'
y*
z = r cos p,
with r > 0, 0 < cp 6 n, 0 s 8 < 2n. Analogous transformations could be written for r*. Without loss of generality we can choose z along the r* direction: then r r* = rr* cos cp. Furthermore, for each point with coordinates (r, 8, cp) another point will exist, equivalent to the first, with coordinates (r, n + 8, n  cp). The contribution of both the points to the integral (3.A.15) will be exp (2nirr* cos cp) exp [2nirr* cos ( n  p,)] = 2 cos (2nrr * cos 9). Thus (3 .A.15) reduces to
+
3~
Fig. 3.A.4. Polar and Cartesian coordinates.
y = r sin g, sin 8
F
r
)
n
2n
p(r)cos(2nrr*coscp)r2sincpdrdp,d%
The diffraction of Xrays by crystals
1
181
where r2 sin rp is the Jacobian of the transformation (from Cartesian to polar coordinates) Integration over rp and 8 gives
1 m
F(r*) =
4nr2p(r)
0
sin 2nrr * dr = 2nrr *
Q U(r) sin2nrr2nrr** dr
(3.A.33)
where U(r) = 4nr2p(r) is the radial distribution function. Thus F(r*) is also spherically symmetric and its value at r* = 0 is given by F(0) =
U(r) dr. 0
As an example, let p(r) be a spherically symmetric function equal to 1 for r S R and vanishing elsewhere. Its Fourier transform F(r*) =
6 2
4s2
sin 2nrr* 2nrr *
r sin 2nrr* dr = $ n ~ ~ r p ( y )
where rp(y) = 3(sin y  y cos y)Iy3 and y = 2nr*R. The function q ( y ) is plotted in Fig. 3.A.5. The main maximum occurs at y = 0. Intensities of the subsidiary maxima decrease when y increases. The distance between consecutive maxima is inversely related to R.
Convolutions The convolution (or folding) of two functions p(r) and g(r) (it will be denoted by p(r) *g(r)) is defined by the integral
where S is the r space. Note that in (3.A.34) the integrand is a function of both u and r while the integral is only a function of u. The relation between p(r) and g(r) is symmetrical in forming their convolution. That may be proved first by replacing in (3.A.34) r by R = u  r and after R by r: then Convoluting two functions very often has the effect of 'broadening' the one by the other. As an example, the convolution of two Gaussian functions N(a,, al) and N(a,, a;?)is the Gaussian function N((a: 0;)ll2, a , a,). The convolution operation appears in many scientific areas, and is involved in the interpretation of most experimental measurements. For example, when the intensity of a spectral line is measured by scanning it with a detector having a finite slit as input aperture, or when a beam of light passes through a groundglass screen and is broadened out into a diffuse beam. Suppose in the second example that p(8) is the angular distribution of the incident beam and g(B) is the angular distribution which could be obtained if the incident beam was perfectly collimated. For any given p(8) the angular distribution of the transmitted beam is given by:
+
+
+
Fig.3.A.5. Thefunction p,y ,=B(sin y ycos y ) / y 3 is plotted as a function of y = 2nr'R.
182
( Carmelo Giacovazzo That may be explained by observing that the component of the transmitted beam emerging at angle 0 due to the light component incident at angle 8 ' (and therefore deviated through the angle 8  8') has intensity p(01)g(8 0'). If interference effects are absent the total intensity in the direction 0 is the integral of p(O1)g(8  8') over all values of 0'. A very important theorem for crystallographers is the following: T [ P ( ~*) g(r)l = T[p(r)l T[g(r)l. The lefthand side of (3.A.35) may be written
(3.A.35)
p(r)g(u  r) exp [2ni(u r*)] dr du where r and u vary in S and S" respectively. Denoting u = r T[p(r) * g(r)] =
11 I, S'
=
p(r)g(rt)exp [2ni(r
(3.A.36)
+ r' gives
+ r') . r*] dr dr'
S
.
p(r) exp [2ni(r. r*)] d r l g(rt) exp [2ni(rt r)] dr' S'
In an analogous way the reader will prove that
If g(r) = p(r) (3. A.34) will represent the autoconvolution of p(r) with itself inverted with respect to the origin: in crystallography it has a special significance, the 'Patterson function', and will be denoted by P(u). It is
the transform of which, according to (3.A.3.9, is given by
+
T[P(u)] = [A(r*) iB(r*)][A(r*) iB(r*)] = (F(r*)I2. (3.A.39) It is now easily seen that the Fourier transform of an autoconvolution is always a real function: therefore, in accordance with the conclusions of p. 176, P(u) will always be centrosymmetric even if p(r) is not.
Convolutions involving delta functions Because of (3.A.8) and (3.A.34)
If r and u are assumed to belong to the same space, choosing the same coordinate system transforms the above relation onto 6 (r  ro)* p (r) = p (r  ro).
(3.A.40)
We see that the convolution of p(r) with 6(r  r,) is equivalent to a shift of the origin by r , (see Fig. 3.A.6(a)). Suppose now that f (x) is a function defined between 0 and a. Because of (3.A.10)
The diffraction of Xrays by crystals
~(x,Y)
0
w
0
0
0
0
183
Fig. 3.A.6. Convolutions of the function fwith: (a)the Dirac 6 ( x  a ) delta function; (b) a onedimensional lattice. In (c) the convolution of the function f(x, y ) with a twodimensional lattice is shown.
0
where p(x) is a periodic function defined between a and +w, equal to f(x) for 0 s x s a and with period a. Indeed each term in the summation corresponds to a function equal to f(x) but shifted by na (see Fig. 3.A.6(b)). It may be concluded that each function p(x), periodic with period a, may be considered as the convolution of the function f (x) = p(x) defined between 0 and a, with an array of delta functions located at the lattice point positions. This result may be generalized to a threedimensional space. Indeed
where: f (r) is a function defined for 0 s ' x s a, 0 s y s b, 0 s z s c; p(r) is a function defined for x, y, z between w and + w , periodic with periods a, b, c, and equal to f ( r ) when O s x s a , O S y s b , O s z s c . In conclusion, a threedimensional periodic function p(r) may be considered as the convolution of a function defined in an elementary cell with a threedimensional lattice, this last represented by the lattice function L.
Some properties of convolutions Let p(x) and g(x) be two onedimensional distributions defined in the interval (a,+w) and C(u) their convolution. Consider the characteristic equation of C(u): += +m +m p(x)g(u  x) exp (itu) dx du. C(U)exp (itu) du =
L (L
1
)
184
1
Carmelo Giacovazzo Table 3.A.1. Properties of distributions under the convolution operation
Changing the variable u into q = u  x gives +rn
C(u) exp (iru) du =
+"
p(x) exp (itx) dxlm g(q) exp (itq) dq (3.A.42)
which implies that the characteristic function of a distribution obtained by convolution is equal to the product of the characteristic functions of the constituent distributions. From (3.A.42) several properties of great import follow. Setting t = 0 in (3.A.42) gives
where A represents the area under the distribution. Taking the derivative of (3.A.42) with respect to t and setting t = 0 yields
Thus, the mean of the convolution is equal to the sum of the means of the constituent distributions. By extending the procedure Table 3.A.1 may be obtained. The following notation has been used:
are the central moments of order p for the convolution distribution (similar expression can be derived for the constituent distributions). Accordingly po= 1, 111 = 0, p, coincides with the variance a', while yl = p3/a3 and y,= [(p4/a4) 31 are the skewness and the excess parameters for any distribution.
Deconvolution of spectra Often it occurs that an experimentally measured function C may be considered as the convolution of the functions p and g. If p is known in advance then it may be of some interest to obtain g. That frequently occurs in spectroscopy or in powder diffraction, where a spectrum is often constituted by overlapping peaks and it is wanted to deconvolute from such a spectrum a given lineshape function. Effects of such selfdeconvolution
The diffraction of Xrays by crystals
1
are:['"16] the component lines are more clearly distinguished, their location, area, etc. are more correctly defined, the signal to noise ratio is increased. Let us consider C as the convolution of the lineshape function p and of the ideal spectrum g. Then p may be decon~oluted[l~~ from C by taking the Fourier transform of
and by calculating T k l = T[C]/Tbl. (3.A.43) g is finally obtained as inverse Fourier transform of the righthand side of (3.A.43):
An example of what can be achieved is shown in Fig. 3.A.7. In (a) a diffractogram of quartz measured between 67" and 69" is shown, in (b) a possible Fourier selfdeconvoluted spectrum is drawn. The widths of deconvoluted lines are narrower, peak centroids shift as a result of changes in degree of overlap: since integrated intensities of peaks are retained (see p. 184) more careful estimates of integrated intensities of single peaks may now be accomplished. The practical use of (3.A.44) is not always straightforward.[183191 The limited instrumental resolution and the random errors 'associated with experimental data are a difficult problem. In particular, random errors are usually amplified by the process so that the righthand side of (3.A.44) could coincide with a function g' substantially different from g. Filtering operations or supplementary considerations are then introduced to reduce spurious features.
3.B Scattering and related topics
Compton scattering A photon of energy hv (v = CIA) moving along the direction so is scattered by a completely free electron located in 0 , initially at rest. Let s be the direction of the scattered photon, 28 the scattering angle, hv' = hc/(A dA) its energy and mv2/2 the recoil electron energy. Conservation of energy (neglecting any relativistic effect) requires
+
which may be approximated to hc A2
 dA = $mu2
Conservation of momentum requires
28 Fig. 3.A.7.
185
186
1
Carmelo Giacovazzo
which, on assuming A + dA = A, may be reduced to h imv =  sin 8. A
(3.B.3)
Finally, v may be eliminated from (3.B.1) and (3.B.3) so as to obtain
The anisotropic temperature factor Thermal agitation will cause the atoms to fluctuate about their equilibrium positions. Let us suppose that the force field around an atom located at the origin of the coordinate system (its equilibrium position) is anisotropic and harmonic. Then the meansquare vibrational amplitude is different for different directions and equal in the two ways of the same direction. In any rectilinear coordinate system defined by A = [a, b, c] let p ( r l ) be the probability of finding the atomic centre moved in r t = x t a + y l b + z'c = X'A. In general d e t exp [~(X'U'x')], p(xl, y', z t ) = ( 2 ~ r )  ~ / ~ (U)1'2
(3.B.5)
where U is the variancecovariance matrix (it represents a symmetrical tensor)
u=
i
1
(x'" (xtyt) (xtzt) (x'y') ( y f 2 ) (y'z') = ( x t X ' ) . (xtzt) (ytz') (zt2)
The Fourier transform of p(X1) gives
+
X*~ + . . .)I q(X*) = exp (2n2X*u*x*) = exp [  ~ ? G ~ ( U T ~2U&.x*y* = exp (X*/3X*) = exp  ( p , , ~ + *~ 2P12x*y*+ . . .)I where U* is the variancecovariance matrix expressed in reciprocal coordinates and
Usually crystallographic leastsquares calculations (see p. 94) provide estimates of the tensor fi from which U* is easily derived via eqn (3.8.6). Then the atomic scattering factor, calculated for r* = r & and corrected for thermal motion is (see p. 153)
fo exp (HPH) =fo exp [2n2(Au*H)] where fo refers to the atom at rest. In order to obtain U from U* we only need to apply eqn (2.28). We obtain U = GU*G from which In accordance with a well known property of tensors, the meansquares vibrational amplitude (u2) in the direction defined by the unit vector n = NA = N*A*, is given by (u2)(,) = NUN = N*u*N*.
(3.B.8)
The diffraction of Xrays by crystals Let us now express n as a ratio between a vector r = XA = X*A* parallel to n and its modulus: n = rlr. Then eqn (3.B.8) may be written as
or also
From (3.B.9) the following relations arise:
The following exercises may be useful to clarify some aspects of the subject: Calculate the Pijs corresponding to the isotropic temperature factor Biso defined by (3.19). If in (3.19) sin2 8/A2= r*'/4 = 1/(4dh) is replaced by (2.17b) then
$ = BisoG* /4 is obtained. If $ is the anisotropic tensor in the coordinate system A, calculate its expression in A' = MA. According to (2.A. 15) $' = (M)~$M,. If $ is the thermal tensor of a given atom, calculate the tensor $' of the atom referred to the first one by the symmetry operation C = (R, T). In accordance with (2.A. 16) $' = R$R. Calculate the principal axes of the ellipsoid describing the anisotropic temperature factor $ and their orientations with respect to the crystallographic axes. See p. 76. Calculate the isotropic temperature factor equivalent[201 to a given anisotropic temperature factor (often the anisotropic parameters are deposited and equivalent isotropic are published). The equivalent isotropic motion is defined as that one which gives rise to the same value of (u2): in our case ( u ~= () u ' ~) ~ ~~~ . ~ ~ ~ Let us suppose that eigenvalues A,, A,, and A3 of the anisotropic tensor $ have been calculated. Then, according to (2.38b) we can write (u2)aniso=
1
$(A1 + A2 + A3)
while, for an isotropic motion (see eqn (3.19))
(3.B.lOa)
1
187
188
1
Carmelo Giacovazzo
Isotropic and anisotropic motion will be then equivalent if Let us now observe that, under a transformation of axes, the matrix $G transforms, because of eqns (2.E.8) and (2.21), according to in other words, PG transforms in the same way as a rotation matrix of a symmetry operator (see eqn (2.E.1)). Therefore the trace of $G is invariant under the transformation and, according to p. 75, it is constantly equal to A, + A, A,. At the end we can replace eqn (3.B.lOb) by the most simple equation
+
1 1 (u2)equiv = 2 Tr (PO) = 6~ i,j The reader will easily derive from (3.B.lOd) specific formulae for specific crystallographic systems: e.g. for cubic, tetragonal, and orthorhombic systems (u2)equiv= (Plla2+ P22b2 + P 3 3 ~ ~ ) 1 ( 6 ~ d ~ ) , for hexagonal and trigonal systems (hexagonal setting) etc. Readers are referred to Schomaker and ~ a r s h [ ~for l ] the estimated standard deviation of (u2) In reports of crystal structure determination thermal motion is usually presented in direct space by means of a probability ellipsoid. Each ellipsoid is centred on the mean position of the atom: the surface has constant probability density obtained, in accordance with eqn (3.B.9, on assuming
jpulx'= ~2 where C is a chosen constant. The probability P that a thermal displacement falls within the ellipsoids may be calculated as P(c)=~
p(X')dXr.
ellipsoid
The most often used value is C = 1.5282: then[''] the ellipsoid encloses 50 per cent of the trivariate Gaussian probability density.
Symmetry restrictions on the anisotropic temperature factors Coefficients Pii as provided by crystallographic leastsquares procedures (see p. 94) are affected by various error sources: for example, experimental errors on diffraction intensity measurements, inadequacy of the atomic scattering model, wrong or unapplied absorption correction (see Chapter 4), existence of nonharmonic force fields around the atoms, etc. Thus the thermal parameters estimated by least squares could be physically unrealistic; for example the variancecovariance matrix U should not result positivedefinite. Necessary and sufficient conditions for positiveness are (det U) > 0; Uii > 0; and UiiUi,> 0 for i, j = 1, 2, 3.
The diffraction of Xrays by crystals
If the above conditions are violated then atomic vibrations could be described by imaginary ellipsoids or by paraboloids or by hyperboloids, with the obvious meaning that experimental data are not of sufficient accuracy to justify the use of anisotropic temperature factors. If an atom lies on a special site of a space group the components of the thermal tensor are restricted according to the site symmetry. Indeed the thermal ellipsoids must remain invariant after application of the n symmetry operations which leave invariant the site. In accordance with point 3 in the previous section the relations arise, from which the $ restrictions can be derived. Such restrictions can also be obtained in an easier way by using Wigner's theorem according to which the symmetry of the $ restrictions is displayed by the matrix
Since no atomic position is left invariant after the application of glide planes or screw axes, only point symmetries have to be taken into account. Furthermore, ellipsoids are centrosymmetric, thus no additional $ restriction arises if an inversion centre is added to the site symmetry, or if a mirror plane is replaced by a twofold axis perpendicular to the plane. Thus it is not difficult to understand that ellipsoid symmetry is one of the following three cases: (1) spherical symmetry, for atomic sites with symmetry 23 and its supergroups; (2) ellipsoid of revolution, for site symmetries 3, 4, 4, and 'noncubic' supergroups; (3) general ellipsoid. For site symmetry 222 and its orthorhombic supergroups the orientations of the ellipsoid axes is fixed by symmetry; for site symmetry 2, m, or 2/m only the orientation of one ellipsoid axis is fixed by symmetry. In Table 3.B.1 all the conventional special positions are collected in seven b l o ~ k s . [ ~Each ~ , ~block ~ ] shows the possible point groups to which each site may belong, the 'minimal' site symmetry characterizing each position and a crossreference number identifying the type of $ restrictions described in Table 3.B.2. The letter h, when present, warns that an hexagonal setting is involved and the letter w suggests that the rule holds for hexagonal and nonhexagonal settings. To make Table 3.B.1 clearer we note that all the special positions in the first block belong to one of the point groups m3m, 43m, 432, m3, 23. According to previous observations, we now neglect whether symmetry axes are proper or improper; thus the 'minimal' symmetry 311111 210011 is associated with the sites. Conversely, under the same convention, all sites with symmetry 2[,,] 211001i or 2[rn11Z[lool or 2[ooll2 k 0 ~ ~ l or ?[,ll 211001 or 2[,,] 2[loo1are all represented in block five of Table 3.B.1 by the site with 'minimal' symmetry 2[,,] 2[1001 To make Table 3.B.2 clearer we observe that case No. 23 may be rewritten as: P11, P33 = P22' P121 P13 = P121 P23.
1
189
190
1
Carmelo Giacovazzo
Table 3.B.1. Site symmetry table giving key for the 29 types of symmetry prestrictions m3m, 43m, 432, rn3,23
2/m, m, 2 l W2001]
3[1111 2 [ ~ ~ 1 1
I6 17 18 19 20 21 22 23 24 25 26 27 28
0101
6/mmm, 6m2, 6mm, 622, 6/m, 6, 6, 3m, 32, 3, 3 W h 310011 9 w
1001
0
1
21iio1 101,
4/mmrn, 42m, 4mm, 422 4ffr~4,4 4l0011
I 20111
4[~1~1 411~~1
2
2
h 3 Il h 4 tl
1001
0
2210] 1201 0101
3rn, 3m, 32, 3, 3 5 6 7 8
%iil
3[iii1 3[1i11 3[iii1 rnrnrn, rnm2, 222 2[00,1 2[1001 w 2[001, 2[1101 210101 2[1011 2~001 ~[OIII h 210011211001 h ~ [ O O ~210101 I
i, 1 1
29
10 11 12 13 14 15
Table 3.B.2. Symmetry firestrictions. Crossreference No.
Pi1
P22
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15
A A A A A A A A A A A A A A A
A A B B A
P33
A C A B A A A D A A A A A C A B C A C B A B B B C B C
Pi2
Pi3
P23
O 0 O 0 O 0 O 0 D D  D D D D D / 2 0 O 0 D 0 O E O 0 B/2 0 A/2 0
0 0 0 0 D
Crossreference No.
16 17 18 19 20 21 D D 22 D 2 3 0 24 0 25 0 26 0 27 F 28 29 0 0
Pi1
Pz,
P33
A A A A A A A A A A A A A A
B B B A A B B B B B B B B B
C C C C C A A B B C C C C C
Pi2
D O O D D D D D D B/2 A/2 B/2 A/2 D
Pi3
P2,
0 0 E 0 0 F E E E E E D E D D F D F F/2 F 0 F E 0 E E/2 E F
The diffraction of Xrays by crystals
1
The Renninger effect and experimental phase determination by means of multiple diffraction experiments Let us suppose that the two nodes HI and Hz are simultaneously at the surface of the reflection sphere: according to eqn (3.25) it will have to be By subtracting the second equation from the first we obtain (sl  s2)lA = r&  r& = r&H2.
(3.B.12)
Equation (3.B.12) sets up that the diffracted beam Hz can act as an incident beam for the reflection H1  HZ which is thus in the diffraction position (see Fig. 3.B.l(a)). Therefore, to the beam diffracted in direction sl by lattice planes H1 a twicereflected beam overlaps, first from the planes Hz and then from the planes HI  Hz (see Fig. 3.B.l(b)). In the same way the beam diffracted in direction s2 from the planes Hz will overlap with a twicereflected beam, first from the planes H1 and then from the planes Hz  HI. In general, when diffraction data are collected for crystal structure solution, the multiple diffraction (Renninger) effect can be considered as a disturbance. As already noted, it can be the reason for apparent violation of the systematic extinctions (but the shape of their diffraction peaks is different from that of the normal reflections and therefore easily recognizable). On the other hand, the threebeam diffraction effect can be treated in accordance with dynamic diffraction theory and used for the experimental solution of the phase problem. This point of view is extremely promising, and a short account is given here. First ~ i p s c o m b [investigated ~~] the possibility of using multiple diffraction intensities for phase determination, but conclusive results were not obtained. In spite of many subsequent investigations, only in more recent years[2s301has it become clear that dynamical theory applied to threebeam diffraction is a powerful tool for the experimental solution of the phase problem even for common (say imperfect) crystals. General solutions for the threebeam case are now available which provide a satisfactory interpretation of experimental results. The reader is referred to a recent book[311for a review of the various contributions and a description of the Fig. 3.8.1. Renninger effect described in: (a) reciprocal space; (b)direct space.
191
192
1
Carmelo Giacovazzo Detector
I
 scan
Fig. 3.8.2. *scan experiment described in: (a) direct space; (b) reciprocal space.
(b)
Ewald sphere
theoretical background: here a short account of the results is given in accordance with Hummer and ill^.[^^] The interference between the wave directly diffracted from H1 planes (primary reflection) and the 'Renninger Umweg wave' generated from Hz and HI  H, scatterings produces a wave whose intensity depends on the triplet invariant phase Without anomalous dispersion effects it is equal to Such an intensity can be measured by a qscan experiment (see Fig. 3.B.2): the integrated intensity IH,(3)is monitored while the crystal is rotated about the vector r:, and scanned through the threebeam position. The integrated 3scan profile may be approximately calculated (except for a range very close to the threebeam setting) according to (see Fig. 3.B.3)
where the Ds are the amplitudes of the excited wavefields in the crystal (the intensities are given by 1= 1 D 12). In eqn (3.B. 13) DL, is the twobeam amplitude of the reflection HI, D, is the amplitude of the Umweg wave defined by
Du = R W ) F H ~ F H ,  H ~ .
Ciare suitable parameters.
Fig. 3.8.3. Diagram of the interference between the unperturbed twobeam amplitude Do and the Umweg resonance term D,.
lR(+)l and A(3) are the modulus and phase of the complex resonance[331 term R ( q ) = )R(q)l exp (iA(+)] which governs the amplitude and the resonance phase shift of the Umweg wave. Typical resonance curves for IR(q)1 and A(q) are given in Fig. 3.B.4. IR(q)I is highest near the threebeam position. A(q) varies from zero to n when 3 is scanned through the threebeam position: it is less than n/2 when H, is inside the Ewald sphere; it is between n/2 and n when it is outside. Equation (3.B.13) and (3.B.14) may be used to interpret the main features of typical qscan profiles (we assume that r;, crosses the Ewald sphere from inside (. 3 . < 0) to outside ( 3 > 0)). Suppose Q, 0: for 0 and with negligible incoherent scattering. 3. The threedimensional Fourier synthesis with coefficients F,,,, gives the positions of the nuclei (they do not necessarily coincide with the atomic positions found by Xray diffraction). The peak heights are proportional to the b values of the corresponding nuclei: if b is negative, the peak is negative too. Fourier syntheses with coefficients F,, give the spin density distribution of the magnetic atoms. 4. Since b does not depend on sin 8/A nuclear scattering decreases only because of the temperature effect. Thus reflections with high values of sin 8lA can be collected giving atomic positions and thermal parameters with accuracy higher than from Xrays. In many cases X and ndiffraction experiments are both performed in such a way that accurate maps of the electron density can be obtained.
The diffraction of Xrays by crystals
5. The energy of a neutron with wavelength of 1A is of the order of 0.1 eV, which is comparable with the energy of the modes of thermal vibration of the crystal. This causes inelastic scattering but also allows for the possibility of studying energy changes with good accuracy.
6. Some additional information about neutron diffraction experiments with pulsed neutron sources should be useful. In diffraction techniques using monochromatic radiation, intensities are measured by moving a detector to different scattering angles OH chosen according to Bragg's law A. = 2dHsinOH. At spallation neutron sources, where the neutron beam is pulsed, the discrimination among neutrons with different wavelengths may be accomplished by their time of arrival at the detector (time of flight): thus diffraction effects can be measured at a fixed scattering angle $0:
AH = 2dHsin OO. From de Broglie's relation mu = h/A (m and v are mass and velocity of the neutron respectively) the following relation arises: mv = m(Llt) = hlA, where L = L, L,. Here L, is the flight path from moderator to sample and L2 is that from sample to detector. Then
+
tH= 505.555LdHsin O0 where L is measured in meters, A and dH in A, t in ys. Thus time of flight depends linearly on both the flight path and on the wavelength. In addition the equations suggest that resolution improves with increasing flight path. Area detectors (see Chapter 4) are the best choice for timeofflight techniques. Indeed, even if the source is on for brief pulses the full spectrum may be used (in monochromatic techniques coupled with a reactor the source is on all the time but a small portion of the spectrum is used).
3.C Scattering of Xray by gases, liquids, and amorphous solids
Introduction In this appendix we will describe the scattering of Xrays from gases, Iiquids, and amorphous solids. No attempt will be made to deal exhaustively with the great amount of work made in the field: only the basic principles of the phenomena will be described. For further information the reader is referred to specialist papers on the subject or to some enlightening books.[3w1] First ~ e b y e [ ~(but ' ] see also ~ h r e n f e s t ~realized ~ ~ ] ) that no arrangement of molecules of finite size could be considered completely random. The most random array which can be imagined is that of a monoatomic gas: but even in this case the finite size of the atoms prevents their approaching one another within a distance smaller than a given threshold. According to
(
201
202
1
Carmelo Giacovazzo
Debye, two types of effects could be found on the diffraction patterns: (1) the effects due to the more or less fixed spatial arrangements of the atoms in the molecules (even if molecules have random positions and orientations), called 'internal interference effects'; (2) the effects due to the mutual configuration of the molecules, which may be not arbitrary since it is conditioned by their dimensions and their packing, called 'external interference effects'. The relative importance of the two types of effects is a matter of degree. Indeed, for monoatomic gases external interference effects are dominant, while for polyatomic gases internal interference effects are not negligible. Again in liquids (or amorphous solids) the existence of average interatomic distances produces well marked external interference effects: if the liquid is composed of groups of atoms the internal interference effects are again not neglibible. In the following sections some formulae will be developed which refer to the coherent scattered radiation. However, in experiments the total, say both coherent and incoherent radiation, is usually collected; in the case of amorphous bodies the incoherent radiation may be an important fraction of the total radiation. According to the discussion on p. 147, the incoherent intensity relative to one atom is given by k
where k varies over the individual electrons of the atom. If we sum (3.C.1) over all the atoms in the assemblage the total incoherent scattering is obtained, which is a smooth function slowly increasing with sin B l A . Such a function has to be subtracted from the total scattering pattern: only after that can the coherently scattered intensity be used to deduce structural parameters.
Diffraction from a finite statistically homogeneous object Usually the motion of atoms or molecules in gases and liquids is extremely rapid compared with the duration of a diffraction experiment. In these conditions the phase value of F(r*) has no practical interest while its modulus can provide useful information on the statistical distribution of the atoms. Indeed the measured diffraction intensity is the weighted sum of contributions arising from the various configurations of the atoms. A similar conclusion holds for amorphous materials, for which trying to calculate the atomic positions has no practical meaning while it is possible to estimate interatomic distances (on which diffraction intensities depend). Suppose that the object we want to investigate is finite and statistically homogeneous, of volume a. In accordance with eqn (3.27) and the Patterson function becomes P(u) =
I R
p d r ) p d r + u)@(r)@(r+ u) dr.
(3.C.2)
The product @(r) @(r + u) is always vanishing except when both the points
1
The diffraction of Xrays by crystals
+
r and r u are inside the object: in this case @(r)@(r+ u) = 1. The space domain in which this condition is verified is a function of u and will be denoted by Qv(u), where 0 6 v(u) 6 1. It is readily seen from Fig. 3.C.1, that Rv(u) is the volume which belongs to the object and to the object shifted by u. Furthermore, v(u) is centrosymmetric (v(u) = v(u)), it decreases with increasing u and takes its maximum for u = 0 (v(0) = 1). Accordingly
'
203 I
\
\ \
\
+& ,
I I 1
I
I
where RY(U)=
I"
+
@(r)@(r u) d r = @(r)* @(r).
(3.C.4)
Fig. 3.C.1. The dashed area has volume Rv(u)
For homogeneous objects (3.C.3) may be written as where P,(u) is the Patterson function for the unit volume. According to (3.A.37) The Fourier transform of Qv(u), according to eqns (3.C.4), (3.A.37), and (3.A.21) is T[Qv(u)] =
j Qv(u) exp (2nir"
u) du = ID(r*)12
(3.C.6)
so that Since @(r) is real, 1D(r*)l2 is centrosymmetric: its maximum value is 1 D (0).1' According to (3.27) D (0) = 52 so that Furthermore, according to (3.C.6)
Q* ID(r*)l2dr*
=
L
.
Pv(u) d u b *exp (2nir* u) dr*
From (3.C.8) and (3.C.9) it is easily deduced that 1D(r*)12rapidly decreases with (r*l, and is appreciably different from zero in a domain near the origin NU of the reciprocal space (when the diffracting object is a crystal, (D(r*)I2 f repeats itself around each lattice point: the larger is 52, the smaller the A domain). Replace in (3.C.9) the decreasing function ID(r*)I2 by a constant which is equal to its maximum value 52' in a volume w defined by S2'w = 52 (see Fig. 3.C.2 for a onedimensional example). Then an approximate estimate of the domain volume is obtained, say w = 1/52, together with its approximate dimension rz ( 1 / ~ )=~l/ro, ' ~ where ro is the average dimension of the Fig,3.C.2. Thetypicalform diffracting object. function of r*.


r* of , D ( r X , as ,~a
204 ( Carmelo Giacovazzo
In terms of diffraction angles the width of the diffraction peak near the origin of the reciprocal space may be obtained from the Bragg relation (2/r,*) sin 8, (2Ir:) 8, 2roeo= A from which


For Cu K, radiation and an object with ro = 0.1 pm it is 8, = 4.4 x On assuming that diffraction around the central peak may be observed down to 8 = low3,0.1 pm constitutes the upper limit for the dimension of the object.
Diffraction from a finite statistically homogeneous object with equal atoms Suppose that the object is composed of N atoms of a single type, and Nl is the number of atoms contained in the unit volume (of course fluctuations from this value are possible due to thermal motion or to structural features of amorphous solids). Then v, = l/Nl is the average volume available for each atom. Equations (3.C.5) and (3.C.7) may be written in terms of autocorrelation functions of atomic density rather than of electron density. Let us define P(r) = Pa(r) * qa(r) where pa(r) is the electron density relative to one atom and qa(r) is the probability of finding an atom in r. Then P(u) = Pa(r) * Pa(r) and IF(r*)I"
* qa(r) * qa(r)
.
T[P(u)] = f '(r*) T[Pa(u)]
(3.C.11)
where P,(u) is just the autocorrelation function of the atomic density. Let Pal(u) be the function Pa(u) calculated for the unit volume. Then, according to (3.C.5) Pa(u) = Qv(u)Pal(u) and (3. C. 11) becomes Let us now express Pal(u) in a more convenient form. On assuming the origin on an atomic site, the probability of finding a second atom in the volume dv at the extremity of the vector u is dp(u) = dvlv, only for a completely random atomic distribution. In general we could write
where p(u) is a distribution function defining the configuration of the atoms. In general p(u) is not easily found. A very simple model for which p(u) may be rigorously calculated was proposed by Zernicke and ~ r i n s : [it~ concerns ~] the onedimensional arrangement on a segment of length L of N rigid spherical particles of diameter d. Figure 3.C.3 shows p(u) as a function of four values of the particle concentration dll, where 1 = LIN is the average length allotted to each particle. It is easily seen that always p(u) = 0 when u < d (the spheres are impenetrable). At very small concentrations (quasizero volume particles which do not exert any influence on each other) p(u)
The diffraction of Xrays by crystals
v=
(d)
is similar to the atomic distribution of the perfect gas. For higher concentrations the model represents distributions similar to those found in real gases, liquids, and amorphous solids. p(u) will oscillate about unity at short distances from the origin, while p(u) 1 at long distances. Oscillations of p(u) are larger for higher concentrations. When dl1 becomes maximum the close packing of the particles gives rise to a perfect lattice of period d: then very sharp maxima of p(u) will occur at u = nd (full shortrange and longrange order). Let us now denote by z(u) the probability of finding an atom in the element of volume dv located at the extremity of the vector u from an atom located at the origin. Then

It may be noted that l / v l is not only the asymptotic value of z(u) but also its mean value. Indeed, integrating z(u) on the unit volume gives
from (3.C. 12) the relation follows. Write now (3.C.14) by emphasizing the oscillating part of p(u):
1
205
Fig. 3.C.3. The distribution p ( u ) for onedimensional arrangements of objects of length d as a function of the compactness.
206
1
Carmelo Giacovazzo
Then the Fourier transform of z(u) is
and (3.C. 16) becomes (Nl = NlQ) N F(r*)12= f2(r*)60* v1
N ~ ( r * ) ~ ' +f2(r*)(l
1 + T[p(u)
 l]) * lD(r*)12.
Vl
The function ID(r*)I2 can be considered very broad with' respect to the Dirac delta function but very sharp with respect to T[p(u)  1] (which in disorder structures is a function slowly varying with r*). According to (3.C.9) the integral of the ID(r*)I2 peak is Q: therefore
In terms of the normalized intensity I ~ ( r * ) l 'eqn (3.C.18) becomes
[p(u)  11exp (2niu r*) du The first term in (3.C.19) corresponds to the peak at the origin of the reciprocal space. It is detectable only at very small angles and it is distinguishable from the primary beam (see the previous section) provided the diffracting object is very small (say, 118 (e.g. for highpressure gases) IE(O)(' < 0, which is not acceptable: for such cases the diffraction by gases closely resembles that by liquids or amorphous solids, for which supplementary considerations are needed (see p. 212). Since electron scattering is much more intense than Xray scattering (see p. 195) electron diffraction is preferable for gases. Very small quantities of gas can be used with shorter exposure times, and peaks can be measured at greater values of sin 81A. Gas electron diffraction a p p a r a t ~ s [ ~ usually ~ , ~ ~consists ] of an electron gun, a sample injection system, and the detector: the last is often a photographic plate. Typical electron accelerating voltages, highly stabilized, are between 30 and 80 kV, with exposure times of a few minutes. In order to compensate the fast decay of the scattered intensity with sin @/A a rotating sector is introduced into the path of the scattered electrons: it is a metallic disc designed in such a way that the intensity reaching the photographic plate is larger at larger scattering angles. In these conditions the diffraction pattern will emphasize highangle interference effects, whose intensity will now be
+
I
sin 011 Fig. 3.C.4. Schematic diagram of the scattered intensity from a monoatomic gas.
Fig. 3.C.5. Schematic diagram of the diffraction pattern for the diatomic molecule CI,.
210
1
Carmelo Giacovazzo
Fig. 3.C.6. Electron diffraction patterns from
C,H,NO, gas (working temperature about 353 K, two camera di~tances).'~''
sufficient to be measured by a microphotometer. After the background elimination, the scattering optical density distribution is converted into electron distribution. In Fig. 3.C.6 two gasphase electron diffraction patterns[481of nitrobenzene C6H,NO2 are shown (corresponding to two different positions of the plate). The experiment was made in order to determine, in combination with ab initio molecular orbital calculations and Xray singlecrystal structure analysis of several derivatives, the molecular structure of C6H5NO2 in the planar and orthogonal conformation. From data in Fig. 3.C.6 the onedimensional spectrum in Fig. 3.C.7 may be derived. In the figure the curve sM(s) is given where M(s) = (I,  Ib)lZb, s = 4n sin 8/A, I, is the total observed radiation, Zb is the background intensity. The corresponding radial distribution curve p ( u ) is shown in Fig. 3.C.8: the positions of the most important distances are marked by vertical bars whose height is proportional to the weight of the distances. The geometrical parameters of the theoretical model (the molecule as a whole was supposed to have a binary symmetry, while a local mm2 symmetry was assumed for the benzene ring and the nitro group), together with vibration amplitudes, were refined by a leastsquares process applied to molecular intensities: the good final agreement may be deduced from the small differences between the E and T curves.
The diffraction of Xrays by crystals
I
I
0
5
I
I
  
A  3 
V
v
fb
10
I
I
I
0
1
2
V
!
I
20
25
I
I
30
35
s (Am'
A n 
v
V
I
r(A)


v 
I
I
4
5
1
Fig. 3.C.7. Molecular intensity curves (E, experimental; T, theoretical) for C,H,NO, (gas electron diffraction, two camera distances). Also shown are the difference
I
I
6
7
211
Fig. 3.C.8. Radial distribution curves for CH , , NO, (E, experimental; T, theoretical). Also shown is the difference curve (ET).'~'
212
1
Carmelo Giacovazzo
Diffraction by liquids and amorphous bodies In liquids or amorphous bodies each molecule may be considered in contact with a certain number of neighbours. Thus both internal and external interference effects will dominate the diffraction pattern. Let us first consider an atomic liquid: if atoms are assumed to be hard spheres which do not exert any force on each other the distribution p(u) may be cal~ulated.[~~1 In Fig. 3.C.9(a) p(u) is plotted for two values of the concentration parameter C (ratio between the effective volume occupied by the spheres and the total volume of the liquid). The corresponding I E(r*)I2 functions may be derived by application of (3.C.21) and are shown in Fig. 3.C.9(b). Their main features are: (1) for small values of r* it is 1 E(r*)I2 < 1; (2) a large maximum occurs at about r* =0.95/d. Its intensity increases with C while its position does not vary; (3) for lage values of r* 1E(r*)I2 tends to unity as for perfect gases. In spite of the purely geometrical nature of the model the diffraction pattern of monoatomic liquids closely satisfies the model predictions. In Fig. 3.C.10 the IE(r*)I2 curve of liquid mercury is shown: its Fourier transform (eqn (3.C.22)) shows a maximum a little over 3 A. A further example concerns the diffraction pattern of water. As it is well known, the molecules are strongly polar and Vshaped with 0  H distances 1/d r* of about 1 A, and nearly tetrahedral HOH angles (109"). For our purposes, (b) they may be geometrically represented by spheres of about 2.8 A diameter. Fig. 3.12.9. (a) Distribution functions P ( u )for hard spheres of diameter dfor two values of the The water scattering curves[s01 at 1.5 "C and 83 "C are shown in Fig. I~ concentration parameter C. (b) I E ( ~ * )curves 3.C.ll(a); the corresponding radial distribution curves are given in Fig. corresponding to the two distribution shown in (a). 3.C.ll(b). The main maximum for the radial distribution occurs at a radius of about 2.8 A while a second broader maximum occurs at about 4.5 A, nearly vanishing at high temperature. Such results suggested to Bernal and ~ o w l e r [ ~that l ] the arrangement of H 2 0 molecules in water may be described as a brokendown ice structure in which each molecule tries to bind four neighbours: since bonds are continually breaking and reforming at any instant each molecule is bonded to fewer than four neighbours. As a last example, examine now Fig. 3.C.12, where the diffraction patterns by vitreous silica, a cristobalite crystal powder, and silica gel are shown. The main maxima of all the three curves nearly overlap: but cristobalite shows numerous sharp maxima while only one maximum occurs in vitreous silica. Furthermore, vitreous silica intensity decreases with sin 8/A as we have just seen for liquids, while silica gel shows increasing intensity toward small sin OlA. The radial distribution function for vitreous shows a first peak at r = 1.62 A and a second one, at 2.65 A: that indicates that the tetrahedral coordination in the crystalline state persists in the vitreous state (but here the orientations of the tetrahedral groups are randomly distributed). The vitreous state is essentially homogeneous (diffraction intensity decreases at small sin $/A as for liquids) while silica gel  is made from very small discrete particles (10100 A) with voids among 0.5 1 2 r * them (diffraction intensity increases at small scattering angles: see the next section). Fig. 3.C.10. I E ( ~ * ) /curves ' for liquid mercury.
The diffraction of Xrays by crystals
1
213
Smallangle scattering Smallangle scattering is a technique for studying structural features or inhomogeneities of colloidal dimensions.[401For wavelengths of about 1A the typical angular domain of the technique ranges up to one or two degrees. We have already seen (p. 204) that when diffraction occurs from a finite statistically homogeneous object of volume S2 a central peak in the intensity curve may be measured which becomes broader as the object size decreases, and does not depend on the internal structure of the object. Its intensity distribution varies according to (3.C.18):
Since diffraction is considered at very small angles f (r*) will coincide with the number of electrons per atom. Thus the above equation reduces to
We consider now a system constituted by N particles with electron density p randomly dispersed in a homogeneous medium of electron density po (solvent). Particles are supposed to be separated from each other widely enough, thus they will generate independent contributions to the diffracted intensity. The system may also be thought of as a medium of constant p, and macroscopic volume S2 to which N particles are summed with density Ap = p  p,. If S2 is sufficiently large the central peak due to the homogeneous medium is totally unobservable, while the observed intensity distribution may be ascribed to electron inhomogeneties only. In this case the mean scattering power for particle is
where IDP(r*)l2is the average value of )DP(r*)l2over all the possible particle orientations. Different shapes of particles will give rise to different shapes of the scattering function in reciprocal space: ideal scattering intensities can therefore be calculated for spherical, cylindrical, flat, ellipsoidal, etc., particles. The results are all rather similar, particularly in the central range, but remarkable differences occur at larger angles. It may then be expected that in the central part a universal approximation for all particle shapes must exist Let us assume the origin 0 in the centre of gravity of a particle of volume
Fig. 3.C.11. (a) 1 f ( r * ) l 2water scattering curves at 1 .5"C and 83 "C; (b) the corresponding distributions 4nu2p(u).
S i l ~ c aGel
I
Vit. SIO,
.
 #   '
.......
..
.
..... .... ..::. . .:.;:. . . . . . .. .. .... .... .......,..:..: , .
.
.: :
.
:.
.
.. Fig. 3.C.12. Diffraction patterns for silica gel, vitreous SiO,, and for cristobalite.
214
1
Carmelo Giacovazzo
up and let us estimate Dp(r*)=
l
exp (2nir* r) dv.
(3.C.32)

At very small angles we can expand the exponential function in (3.C.32) in power series: it will suffice to expand cos 2nr* . r according to cos 0 1 0'12. In Cartesian coordinates
.
+ y2P2+ z2y2)2,
cos 2nr* r = 1 
where a; p, y stand for the cosines between r* and Cartesian axes. When integration is performed the contribution of mixed products vanishes by hypothesis (the centre of gravity has been located at the origin) and we have
((u21
Dp(r*) = v,  2n2r*2
x2 dx
+ 82j y2 dy +
y21
z2 dr).
Since we are interested to calculate IDP(r*)l2, say the average of IDP(r*)l2 over all particle orientations, we have to rotate Cartesian axes about the origin. We can then replace (u2, P2, y2 by ( a 2 ) = ( p 2 ) = (y2) = 5 SO as to obtain
where r2 stands for (x2+ y2 + z2) and R = ( l v ) ( r2 du) UP
is the radius of gyration (= the mean square distance) of the particle with respect to its centre of gravity. According to (3.C.31) the scattering power per particle will be
where n, = ( p  p,)vp. By taking the logarithm to the base 10
is obtained. If lg ~ ~ , ( r * ) lis' plotted against ( 2 0 ) ~a curve will be obtained which, at small values of 0, is close to a straight line with slope (u = 5.715R;lA2, from which the gyration radius R, = 0.418~is obtained.
The diffraction of Xrays by crystals
In Fig. 3.C.13 the Guinier plot for a lowconcentration solution of haemocyanin from Astacus leptodactylus is shown.[54]The reader will easily derive from the figure (CuK, radiation used) a gyration radius of R,= 62 A. The radius of gyration is connected to the geometrical parameters of some simple homogeneous bodies in the following way:[s5] sphere of radius r:
R i = 3r2/5; hollow sphere (limiting radii r, and r2):
ellipsoid (semiaxes a, b, c):
~ 2=, (a2 + b2 + c2)/5; prism with edge lengths a, b, c:
R: = (a2 + b2 + c2)/12; elliptic cylinder (height h ; .semiaxes a, b): hollow cylinder (height h, radii r,, r2): Other important parameters can be evaluated directly from the scattering data: among others the molecular weight (from the scattering intensity at zero anglesrs6]),the total surface of the particles for unit mass (from the region where the smallangle scattering tends to zero[s73s8]), and the volume of the particle. This latter may be obtained by integrating (3.C.31) over all the reciprocal space (by extrapolation of r*2~ ~ , ( r *at) lvery ~ small r*):
According to (3.C.9) the above relation reduces to from which up may be derived. So far we have considered particles dispersed in a homogeneous solvent and widely separated from each other. If the concentration of the particles increases the mutual interference will enter into play and the scattered intensity is no longer the sum of the individual particle scatterings. As described in on p. 206 a probability function p(u) can be introduced: then 4m2p(u) du will represent the number of particles with distance u lying in the interval (u, u du) from a particle at the origin. Then the scattering power per particle will be (see eqn (3.C.21))
+
2 " ( r * ) = ( ~ ~ ( r * ) ~ )( l + u[p(u)  11sin (2nr*u) du r*v1 0 where (IFp(r*)12)is the squared modulus of the structure factor of a particle
1
215
%
,
I 1
2
3
4
10512tv2
Fig. 3.C.13. A Guinier plot.
5
6
216
1
Carmelo Giacovazzo
averaged over all orientations. From the above equation the function p ( u ) may be derived by inverse Fourier transform.
3.D About electron density mapping The accurate determination of charge density distribution is of basic importance in several scientific areas. For example, for the study of (1) electronic structure of metals and alloys;
(2) metalligand interaction; (3) variation of solid state properties (i.e. conductivity) with temperature. Spatial partitioning of charge density can also answer some specific questions, such as the location of lonepair maxima, the net charge of a particular atom, the excess charge accumulated in a covalent bond, and so on. Such results can be attained only if the selection of the compounds, the process of measuring diffraction data, and their subsequent treatment is carried out with great care. Among the various desiderata we mention the following. 1. Compounds with a small valencetocore ratio are less suitable to charge density studies. If we assume that the number of valence electrons per unit volume is approximately constant for different compounds, the valencetocore ratio is fixed by the number of core electrons per unit volume. Stevens and ~ o ~ ~ e introduced n s [ ~ ~ the ] criterion 1
core
as a possible criterion to estimate the suitability of a system for charge density studies (V is the volume of the unit cell). S varies from 35 for the firstrowatom organic crystals to 0.10.3 for metals and alloys. Crystals with S < 1 require extremely precise diffraction data and careful work. 2. Centrosymmetrical crystals are often preferred (in acentric crystals the phases of the structure factors cannot be uniquely determined).
3. Collection of diffraction data has to be carried out at low temperature. Then thermal diffuse scattering can be neglected (a posteriori corrections are seldom accurate), high resolution data become available (then accurate structural parameters can be calculated), and electron charge density can be easily deconvoluted from the atomic thermal vibrations. 4. Sophisticated measuring programmes should be used, in order to perform optimal scanning mode and profile analysis, decide differentiated measuring times (in order to obtain a set of structure factors with equal variance), prevent multiple scattering, and perform careful correction for extinction, absorption, anomalous dispersion, etc.
5. When possible, neutron data should also be collected in order to obtain nuclear positional and thermal parameters which are unbiased by asphericity in the atomic charge density.
218
1
Carmelo Giacovazzo
Yq,, = 3 sin2 6 cos 241 = 3(s:  s:) Y;,, = 6 sin2 6 sin @ cos @ = 6sxsy Yq,, = 3 sin 6 cos 6 cos 4 = 3sxs, Y;,, = 3 sin 6 cos 6 sin 4 = 3sys, Y;,, = 6 cos2 6  2 = 6s;  2 Y',,, = 15 sin3 6 cos 341 = 15(s:  3s,2)sx Y;,, = 15 sin3 6 sin 341 = (45s:  1 5 s ; ) ~ ~
1
quadrupoles.
Y;,, = 15 sin2 6 cos 6 cos 241 = 15($  s;)s, Y:, = 30 sin2 6 cos 8 sin cos @ = 30s,sys, Yg,,= 1.5 sin 6(5cos2 6  1)cos @ = 1.5(5s; l)s, $J
Y:,, = 1.5 sin 6(5 cos2 6  1) sin @ = 1.5(5s:  l)sy Y;,, = 10 cos3 6  6 cos 6 = (10s;  6)s,
I
octapoles.
In Fig. 3.D.1 some electron density plots in special sections of direct space are shown.[611 In most organic molecules the expansion (3.D.2) may be stopped at octapoles: then the deformation charge density is described by a linear combination of 16 terms, for which 16 population parameters have to be estimated. In some formulations[621the freeatom valence shell is modified by an expansioncontraction radial parametrization in order to take into account the fact that an atom will expand or contract when it becomes more negative or more positive. Such a feature may be incorporated into a perturbed valence density p:,,ence(r) given by where pvaIenceis, as in eqn (3.D.1), the freeatom ground state density, PValenc, is the valence shell population, and k3 is a normalization factor. If k > 1 the atom is contracted relative to the free one [indeed p l ( r ) is proportional to p(kr) with kr > r]. The atomic scattering amplitude has the same type of multipole expansion as the atomic charge density. By Fourier transformation of (3.D.2) one obtains
where 6*,
#* are angular components of the Bragg vector,
and ji(x) is the spherical Bessel function of order 1. From (3.D.3) the calculated structure factors Fcalcare easily obtained. Then (full or blockdiagonal) leastsquares refinement can be carried out: as well as the usual positional and thermal parameters for each atom, the population parameters of the deformation terms may also be refined. Such a formalism should improve (with respect to traditional crystallographic refinements) the agreement between observed and calculated structure factors.
220
1
Carmelo Giacovazzo Suitable Fourier syntheses can be calculated and analysed in order to reveal the effects of interatomic bonding on the charge clouds. Fourier maps of large usefulness are 1 Ap(r) = y
x
( 4 ( H )  F2(H)) exp (2niH. r)
H
where
6 = F c a ~ cmultipole, , F2 = F c a ~ cfree , atoms. AP is then the deformation map, i.e. the difference between the atomic densities represented by spherical harmonics and those represented by free atoms;
F' = Fobs,F2 = Fcalc,rnultipole Ap is then the residual density, e.g. the part of electron density not accounted for by the multipole model;
4 = Fobs, F2 = Fcalc, free atoms,under the condition that F2 is calculated with parameters from highorder (HO) refinement (highorder reflections are unaffected by chemical deformation of valence orbitals and locate atoms carefully). Ap is then denoted as a (X  XHO)deformation map;
Fl = Fobs,F2 = Fcalc,free atoms,with fi calculated as in (3) but for core electrons only. Ap is the (X  X,,) valence map;
4= Fobs, F2= Fcalc, free atoms,with
F2 calculated with parameters from neutrons or a joint highorder Xray and neutron data. Then Ap is the X  N or X  (XHO N) deformation map;
+
4 = Fobs, = Fca~c,~reeatorns, with F2 calculated as in (5) from core electrons only. Ap is then a X  (XHO N) valence map.
+
The estimation of the charge density model obtained at the end of calculations is different according to whether least squares or Fourier methods have been used[671.However, direct and reciprocal fitting are nearly equivalent: indeed, if we assume in (3.D.4) that Fl = Fobs,F2= Fcalc, AF = Fobs(H) Fcalc(H),and we calchlated the difference Patterson
I
x
1 Ap(r)Ap(r + u) dr =  I A F cos ~ ~2nH u, V H then for u = 0 we obtained
Thus leastsquares parameters which give the best fit between observed and calculated structure factors are expected to give rise to the lowest variance in Ap. Direct evaluation of atomic or molecular charges, of dipoles and higher moments, etc, can be obtained from the estimated population parameters or directly from the electron d e n ~ i t y . [ For ~ ~ ,example, ~~] the net charge on atom j is
The diffraction of Xrays by crystals
1
221
when the integration is made over the (not always easily defined) atomic volume. Also, the dipole moment of a molecule may be calculated as
where the integration is over the molecular volume.
3.E Modulated structures and quasicrystals
Embedding of modulated structures in higherdimensional space In Chapter 3, pp. 1713, it has been suggested that incommensurately modulated structures (IMS) can be better described in higherdimensional spaces. From now on S, and L, will denote ndimensional space and lattice respectively, while SX and L,* will be their reciprocals. We will show that the reciprocal lattice L: of an IMS, even if aperiodic in ST, may be transformed into a (3 d)dimensional periodic lattice (say LT+d) by embedding the IMS in a metrical (3 + d)dimensional space S3+,. Let us suppose that the reciprocal vector H of a main or of a satellite reflection may be written in S: as
+
where and kf, k:, k: are the a * , b*, c* components of Ki. One of them should be irrational for incommensurate modulation. Since (3 + d) indices hi are necessary to label a single diffraction effect, we will speak of ddimensional periodic modulation or of ddimensional modulated structure. In Fig. 3.E.1 a section of the threedimensional diffraction pattern of a onedimensional modulated structure is sketched. The main reflections are marked by the largest spots. with basis vectors A L:+d lattice may now be
bl = a * , b2 = b*, b3 = c*, b3+i= Ki
+ ei
(i = 1, . . . , d) (3.E.2)
Fig. 3.E.l. Onedimensional modulated structure: sketch of a section of the threedimensional diffraction pattern, showing main and satellite reflections.
where the eis are unit vectors perpendicular to S g Then in S:+, a reciprocal vector may be written as
a*
0W W
Q
M W W ns
v
According to hypotheses, H is the projection of H' in ST. Consequently the whole threedimensional diffraction pattern LT is the projection in ST of a (3 d)dimensional reciprocal lattice L,*+,. In Fig. 3.E.2 such a projection is shown schematically for a onedimensional modulation: Sz is represented by a horizontal line, el is a unit vector perpendicular to ST, main and satellite reflections are labelled by M and W respectively. In S3+dthe (3 d)dimensional direct lattice L3+dis defined by the set of
a
w
L,
el 0
0
+
+
Fig. 3.E.2. From SX to S:. Main and satellite reflections are denoted by M and W respectively.
222
1
Carmelo Giacovazzo
vectors ai reciprocal to bi according to the conditions ai . bj = 4,. We have
where a, b, c are reciprocal to a * , b * , c * . The reciprocity condition is easily verified: for example,
If a position is defined in S3 by it will be defined in S3+, by
where Indeed, the first three coordinates in S3 and in S3+dcoincide, owing to the fact that L3 is the projection of L3+, along ei; any point r in S3 satisfies the relations
In accordance with (3.E.3)
so that x3+,
= k{xl
+ k h 2 + k&x3
is obtained, which coincides with (3.E.4). If in S3+, the new coordinates
The diffraction of Xrays by crystals
1
223
are introduced, it may be concluded that S3 is defined by tj=O for j = l ,
. . . , d.
The electron density p ' in S3+dis periodic in (3 be calculated in the usual way: p(xl,
1
2
. . . , ~ 3 + d=) 
+ d)dimensions and may
FH,exp
hl,...,h~+,~
j=1
where V is the volume of the unit cell in S3. According to reciprocity rule (the Fourier transform of a projection corresponds to a section and vice versa) the electron density distribution p in S3 is the section of p ' with S3. Therefore in S3+dthe shape of the atoms is a hypersurface which extends in the extra dimensions. In Fig. 3.E.3, a schematic representation of p ' for a onedimensional modulation is described. A scattering formalism for a large variety of modulated structures is now a ~ a i l a b l e : [ ~ substitutional ~~~I and/or displacive modulations of each of the atoms in the crystal may be taken into account, together with the translational or rotational displacement of a molecule or one of its segments in molecular crystals.
Quasicrystals In a famous paper by Shechtman, Blech, Gratias, and cahn17'] electron diffraction patterns of a rapidly solidified A1Mn alloy were shown which suprisingly displayed fivefold symmetry. Sharpness of the spots suggested longrange translational order, but the presence of the fivefold symmetry violated the sacred rules of crystallography. In particular, by rotation of the specimen, fivefold axes (in six directions), threefold axes (in 10 directions) and twofold axes (in 15 directions) could be revealed: the subsequent ascertainment of the existence of an inversion centre fixed, for this AlMn phase, the icosahedral point group m55. Somewhat later a large number of alloys with 'forbidden' symmetries were found: such kinds of materials (providing electron diffraction patterns displaying sharp peaks and forbidden symmetry such as icosahedral, octogonal, decagonal, dodecagonal, etc.) are called quasicrystals. A huge amount of theoretical and experimental publications are now available: for a more comprehensive treatment of the subject and for relevant literature the reader is referred to three excellent review~.[~+'~] A useful premise to quasicrystals (as well as to the IMSs) is the definition of quasiperiodic functions. It is well known that a periodic function f (x) =f (x 1) may be uniformly approximated by finite sums of functions exp (2ninx). Accordingly, in a p dimensional space
+
f '(XI, . . . , x,)
= nl,
..., np
q(nl, . . . , n,) exp (2ni(nlxl + . . . + n,x,)
is a periodic function. However, its 'projection' on onedimensional space
f (x) =
C...,
nl,
q h ,
. . . , n,)
exp (2ni(nlv1 + . . .
+ npvP)x)
(3.E.6)
np
obtained by fixing in f ' xj to v,x is not periodic if some of the vjs are irrational. Functions which may be uniformly approximated by finite sums
Fig. 3.E.3. Schematic representation of the density p' i n S,. S, is the horizontal line: its bulging parts represent real atoms. (a) Perfect crystal; (b)density modulation; (c) displacive modulation.
224
1
Carmelo Giacovazzo
+
of functions exp [2ni(n,v1x + n,v2x2 . . . + n,v,x)] are quasiperiodic functions. We take three simple examples. 1. Let f '(x,, x,) = A 1 sin 2nx1 + A 2 sin 2nx2. If we assume X, = ax1 where cu is an irrational number then
+
f (x) = A, sin 2nx1 A2 sin 2ncux, is not periodic. 2, f (x) is the superposition of a periodic sequence of large open circles, schematically represented by C, 6(x nu), and a periodic sequence of small solid circles represented by C, G(x  rnaz12). Here, z = 2 cos (1615) = (1 + f i ) / 2 = 1.618034. . . is the golden mean, n and m are any integers. Since a and az/2 are incommensurate numbers the structure is not periodic (see Fig. 3.E.4, first line) but the diffraction pattern will display delta peaks owing to the fact that the order is perfectly maintained at long distances. The existence of delta peaks may be demonstrated by examining periodic approximations off (x). Since
successive approximations to
t
are
to which periodic structures of increasing periods a12, a, 3a, 5a can be associated. It is easily seen from Fig. 3.E.4 that better periodic approximations of the aperiodic sequence can be obtained by higher order approximants. 3. In Fig. 3.E.5(a), a square lattice with a unit cell with edge length (1 + z2)'I2 is drawn. An irrational direction is drawn, at an angle of arctan(l1z) with the cell edge. All the lattice points contained in a band parallel to such a direction and with width (1 z) are projected on it (stripprojection method), giving rise to a nonperiodic pattern (the numerical sequence is 0, 1, 2.618, 3.618, 5.236, 6.854, 7.854, 9.472, 10.472, etc.). All intervals in the projection will have length either 1 or z (L and S respectively), in the sequence SLSLLSLSLLSLLSLS.. . (Fibonacci sequence). The chain may also be written
+
x, = n ( 3  z)  ( z  1) frac(nz),
Fig. 3.E.4. An aperiodic longrange ordered structure and its periodic approximants.
0 I
0
*o o* 5a
0.
0 I
0
*o* o*
'63
The diffraction of Xrays by crystals
1
225
Fig. 3.E.5. (a) Projection of a band i n a twodimensional lattice t o obtain a nonperiodic ordered sequence (Fibonacci sequence). (b)The Fibonacci sequence results from a cut of the disconnected 'line atoms' of the twodimensional crystal with the real space S,.
where frac (x) is the fractional part of x. Since there is a weighted average lattice with constant a = (3  z) the sequence may be considered as a modulated structure with modulation factor g(x) = ( t  1) frac (x), which may be embedded in a twodimensional space. The above three examples suggest that aperiodic sequences in one dimension can be obtained by projection of periodic sequences in two dimensions. The procedure for embedding a onedimensional aperiodic sequence in a twodimensional space may be performed in accordance with the previous section. For the last example we can choose al .=(z, 1) and az = (1, z) (see Fig. 3.ES(b)): then the reciprocal average lattice is also square with basis vectors
In order to obtain the quasiperiodic onedimensional sequence on S1 (see
226
1
Carmelo Giacovazzo
again Fig. 3.E.5(b)) one has to attach parallel line elements in the lattice vertices. Thus the real onedimensional quasicrystal results from a cut of the disconnected 'line atoms' of the twodimensional crystal with the physical space S,. The procedure may be generalized to the ndimensional case: the dimension of the space S,, in which a lattice with translational periodicity is obtained is determined by the number of n rationally independent reciprocal basis vectors which are necessary to index the diffraction pattern. The real aperiodic crystal is again the cut (in the direct space) of the ndimensional crystal with the physical space. Well known twodimensional examples of quasiperiodic structures are Penrose ti ling^.[^^,^^] TWOexamples are shown in Fig. 3.E.6: in (a) tiling of the plane is achieved by putting together two rhombic units in accordance with some matching rules (without them the plane should be covered in a periodic way). The pattern shows a fivefold rotation point. In (b) 'kites' and 'darts' are used: no pentagonal symmetry is shown. ~ a c k a y [ first ~~] showed that their Fourier transform satisfies a fivefold symmetry. Octagonal, decagonal, and dodecagonal twodimensional quasicrystals are also known; all of them can be embedded in a periodic fivedimensional space. The threedimensional icosahedral lattice mentioned at the beginning of this section may be embedded in a sixdimensional space. The characteristics of the quasicrystals do not coincide with those of the incommensurately modulated structures. While the latter show main and satellite reflections, an average structure, and crystallographic point symmetry, the quasicrystals show one kind of reflection only, no average structure, and noncrystallographic point symmetry.
References
Fig. 3.E.6. (a) A twodimensional quasilattice showing one fivefold rotation point (plane symmetry 5mm). Basic oblate and prolate rhombi with their matching rules are shown: similarly arrowed edges must fit. (b) Penrose tiling with kites and darts (it does not show fivefold symmetry).
1. Ewald, P. P. (1917). Annalen der Physik, 54, 519. 2. Laue, M. von (1931). Ergebnisse der exakten Naturwissenschaften, 10, 133. 3. Pinsker, 2. G. (1978). Dynamical scattering of xrays in crystals. Springer, Berlin. 4. Darwin, C. G. (1914). Philosophical Magazine, 27, 315. 5. Darwin, C. G. (1922). Philosophical Magazine, 43, 800. 6. Zachariasen, W. H. (1967). Acta Crystallographica, 23, 558. 7. Becker, P. J. and Coppens, P. (1974). Acta Crystallographica, A30, 129. 8. Kato, N. (1976). Acta Crystallographica, A32, 453. 9. Becker, P. J. (1982). In Computational crystallography, pp. 4629. Clarendon, Oxford. 10. Chapuis, G., Templeton, D. H., and Templeton, L. K. (1985). Acta Crystallographica, A41, 274. 11. Templeton, L. K., Templeton, D. H., Phizackerley, R. P., and Hodgson, K. 0. (1982). Acta Crystallographica, A38, 74. 12. Phillips, J. C. and Hodgson, K. 0. (1980). Acta Crystallographica, A36, 856. 13. Bijvoet, J. M. (1949). Proceedings of the K. Nederlandse Akademie van Wetenschappen, B52, 313. 14. Phillips, D. L. (1962). Journal of the Association for Computing Machinery, 9 , 84. 15. Twomey, S. (1963). Journal of the Association for Computing Machinery, 10,97. 16. Kennett, T. J., Brewster, P. M., Prestwich, W. V., and Robertson, A. (1978). Nuclear Instruments and Methods, 153, 125.
The diffraction of Xrays by crystals 17. Kauppinen, J. K., Moffatt, D . J., Mantsch, H. H . , and Cameron, D. G. (1981). Applied Spectroscopy, 35, 3, 271. 18. Wiedemann, K. E., Unnam, J., and Clark, R. K. (1987). Powder Diffraction, 2, 3, 130. 19. Toraya, H . (1988). Journal of Applied Crystallography, 21, 192. 20. Hamilton, W. C. (1959). Acta Crystallographica, 12, 609. 21. Schomaker, V. and Marsh, R. E. (1983). Acta Crystallographica, A39, 819. 22. Johnson, C. K. and Levy, H. A. (1974). In International tables for xray crystallography, Vol. IV, pp. 31136. Kynock Press, Birmingham. 23. Peterse, W. J. A. M. and Palm, J. H. (1966). Acta Crystallographica, 20, 147. 24. Lipscomb, W. N. (1949). Acta Crystallographica, 2, 193. 25. Colella, R. (1974). Acta Crystallographica, A30, 413. 26. Post, B. (1977). Physics Review Letters, 39, 760. 27. Chapman, L. D., Yoder, D. R., and Collella, R. (1981). Physics Review Letters, 46, 1578. 28. Chang, S. L. (1982). Acta Crystallographica, A38, 516. 29. Hummer, K. and Billy, H. (1982). Acta Crystallographica, A38, 841. 30. Juretscke, H. J. (1984). Acta Crystallographica, A42, 127. 31. Chang, S. L. (1984). Multiple diffraction of xrays in crystals. Springer, Berlin. 32. Hummer, K. and Billy, H. (1986). Acta Crystallographica, A42, 127. 33. Ewald, P. P. (1917). Annalen der Physik, 54, 519. 34. Weckert, E. and Hummer, K. (1990). Acta Crystallographica, A46, 387. 35. Renninger, M. (1937). Zeitschrift fur Physik, 106, 141. 36. Hummer, K., Weckert, E., and Bondza, H. (1989). Acta Crystallographica, A45, 182. 37. Mo, F., Hauback, B. C., and Thorkildsen, G. (1988). Acta Chemica Scandinavica. Series A, 42, 130. 38. Guinier, A. (1963). Xray diffraction. Freeman, San Francisco. 39. Hosemann, R. and Bacchi S. N. (1962). Direct analysis of diffraction matter. NorthHolland, Amsterdam. 40. Glatter, 0 . and Kratky, 0. (1982). Small angle xray scattering. Academic, London. 41. Guinier, A. and Fournet, G. (1955). Smallangle scattering of xrays. Wiley, New York. 42. Debye, P. (1915). Annalen der Physik, 46, 809. 43. Ehrenfest, P. (1915). Proceedings of the Amsterdam Akademie, 17, 1132. 44. Zernicke, F. and Prins, J. A. (1927) Zeitschrift fur Physik, 41, 184. 45. Fournet, G. (1951). Transactions of the Faraday Society, 11, 121. 46. Hildebrandt, R. L. (1975). Molecular structure by diffraction methods, The Chemical Society, special periodic report, No. 3 (ed. G. A. Sim and L. E. Sutton). 47. Oberhammer, H. (1976). Molecular structure by diffraction methods, The Chemical Society, special perodic report, No. 4 (ed. G. A. Sim and L. E. Sutton). 48. Domenicano, A., Schultz, G., Hargittay, I., Colapietro, M., Portalone, G., George, P., and Bock, C. W. (1989). Structural Chemistry, 1, 107. 49. Kirkwood, J. G., Maun, E. K., and Alder, B. J. (1952). Journal of Chemical Physics, 85, 777. 50. Morgan, I. and Warren, B. E. (1938). Journal of Chemical Physics, 6, 666. 51. Bernal, I. D. and Fowler, R. H. (1933). Journal of Chemical Physics, 1, 515. 52. Warren, B. E., Krutter, H., and Morningstar, 0. (1936). Journal of the American Ceramic Society, 19, 202. 53. Guinier, A. (1939). Annales d e Physique, 12, 161. 54. Pilz, I., Goral, K., Hoyaerts, M., Lontie, R., and Witters, R. (1980). European Journal of Biochemistry, 105, 539.
(
227
228
( Carmelo Giacovazzo 55. Mittelbach, P. (1964). Acta Physica Austriaca, 19, 53. 56. Kratky, 0. and Porod, G. (1953). In Die Physik der Hochpolymere, Vol. 11. (ed. H. A . Stuart). Springer, Berlin. 57. Porod, G. (1951). KolloidZeitschrift 124, 83. 58. Luzzati, V. (1960). Acta Crystallographica, 13, 939. 59. Stevens, E. D. and Coppens, P. (1976). Acta Crystallographica, A32, 915. 60. Hirshfeld, F. L. (1971). Acta Crystallographica, B27, 769. 61. Stewart, R. F. (1976). Acta Crystallographica, A32, 565. 62. Hansen, N. K. and Coppens, P. (1978). Acta Crystallographica, A 3 4 909. 63. KurkiSuonio, K. (1977). Israel Journal of Chemistry, 16, 115. 64. Hehre, W. J., Stewart, R. F., and Pople, J. A. (1969). Journal of Chemical Physics, 51, 2657. 65. Stewart, R. F. (1973). Journal of Chemical Physics, 58, 4430. 66. Epstein, J., Ruble, J. R., and Craven, B. M. (1982). Acta Crystallographica, B38, 1409. 67. Rees, B. (1977). Israel Journal of Chemistry, 16, 180. 68. Hirshfeld, F. L. (1977). Israel Journal of Chemistry, 16, 198. 69. Coppens, P. (1975). Physical Review Letters, 35, 98. 70. de Wolff, P. M. (1974). Acta Crystallographica, A30, 777. 71. Janner, A. and Janssen, T. (1977). Physical Review, B15, 643. 72. Janner, A. and Janssen, T. (1980). Acta Crystallographica, A36, 399. 73. Janner, A. and Janssen, T. (1980). Acta Crystallographica, A36, 408. 74. de Wolff, P. M., Janssen, T., and Janner, A. (1981). Acta Crystallographica, A37, 625. 75. Yamamoto, A. (1982). Acta Crystallographica, A38, 87. 76. Petricek, V., Coppens, P., and Becker, P. (1985). Acta Crystallographica, A41, 478. 77. Petricek, V. and Coppens, P. (1988). Acta Crystallographica, A 4 4 1051. 78. Shechtman, D., Blech, I., Gratias, D., and Cahn, J. W. (1984). Physical Review Letters, 53, 1951. 79. Janot, Ch. and Dubois, J. M. (1988). Journal of Physics F : Metal Physics, 18, 2303. 80. Janssen, T. (1988). Physics Reports, 168, 55. 81. Steurer, W. (1990). Zeitschrift fur Kristallographie, 190, 179. 82. Duneau, M. and Katz, A. (1985). Physical Review Letters, 54, 2688. 83. Janssen, T. (1986). Acta Crystallographica, A42, 261. 84. Penrose, R. (1974). Bulletin of the Institute of Applied Mathematics, 10, 266. 85. Gardner, M. (1977). Scientijic American, 236, 110. 86. Mackay, A. L. (1982). Physica, A114, 609.
Experimental methods in Xray crystallography H U G O L. M O N A C O
Introduction This chapter discusses the experimental methods used to study the diffraction of Xrays by crystalline materials. Although, as seen in Appendix 3.B (pp. 195 and 198), electrons and neutrons are also diffracted by crystals, we will concentrate our attention on Xray diffraction. We begin discussing how Xrays are produced and how one can define the beam of radiation that will interact with the crystalline sample. The specimens that will receive our attention are single crystals and polycrystalline materials, that is aggregates of a very large number of very small crystals. We discuss the methods used to record the diffraction pattern and to measure the intensities of the Xrays scattered by these two types of specimen in separate sections. The ultimate goal of extracting structure factor amplitudes from diffracted intensities requires the application of a series of correction factors. This process, called data reduction, is discussed in the final section of the chapter.
Xray sources Conventional generators All the standard laboratory sources normally used for Xray diffraction experiments generate radiation using the same physical principles but can vary substantially in their construction details. The two types of conventional generators that are used in conjunction with the data recording devices discussed on pp. 245 and 287 are sealedtube and rotatinganode generators. Most of the techniques used for diffraction data collection require monochromatic radiation. Due to the way in which radiation is produced in the conventional generators, only a discrete number of possible wavelengths can be selected for experimental use. This limited choice and the difference in intensity are two of the major differences between this type of radiation and that generated by synchrotrons.
The origin of Xrays in the conventional sources Xrays are produced when a beam of electrons, accelerated by a high voltage, strikes a metal target and is therefore rapidly decelerated by collision with the metal atoms. Most of the electrons do not lose their
230
1
Hugo L. Monaco
energy in a single collision but do it gradually through multiple events. The result is the production of a continuous spectrum of Xrays called white radiation. If all of the energy carried by an electron is transformed into radiation, the energy of an Xray photon is Emax= hvma,= eV where h is Planck's constant, vmaxthe photon frequency and the subscript max indicates that this is the maximum possible energy, e is the charge of the electron, and V the accelerating potential. If we substitute the frequency in terms of the wavelength and
0
0.2
0.8
0.6
0.4
1.0
~avelength(i)
Fig. 4.1. Xray white radiation spectra as a function of the accelerating voltage.
A
0.2
0.5
1.0
1.5
Wavelength
2.0
(ii)
Fig. 4.2. Characteristic spectrum of copper superimposed on the white radiation spectrum. Notice the ratio of the relative intensities of the K, and Kg lines.
where the potential V has to be measured in volts and the minimum wavelength is obtained in angstroms. This equation shows that there is a minimum value for the wavelength of the Xrays that can be obtained by this process which is a function of the voltage accelerating the electrons. Total conversion of the electron energy into radiation is not a highly probable event and therefore the radiation of the highest intensity is obtained at a somewhat longer wavelength. Figure 4.1 shows some continuous Xray spectra as a function of the accelerating voltage. Notice that as the voltage is increased both the minimum wavelength and the position of the intensity maximum shift to the left. The intensity maximum is found at a wavelength which is approximately 1.5 times Amin. The total Xray intensity generated per second in this way, a quantity which is proportional to the areas under the curves, can be calculated using the equation where A is a proportionality constant, i the electrical current, a measure of the number of electrons which are generating Xrays, Z is the atomic number of the target, V the accelerating potential, and n a constant with a value of about 2. When the energy of the electrons striking the target is higher than a certain threshold value, a second type of spectrum, discontinuous and with very sharp lines, appears superimposed on the white radiation curves just described. This second spectrum is called the characteristic spectrum because its peaks are found at precisely defined wavelengths which depend on the material constituting the target. The characteristic spectrum of copper is shown in Fig. 4.2. The electrons with an energy above the threshold potential are capable of ionizing the target atoms by ejecting an electron from one of the inner shells. When that happens another electron from a higher atomic energy level can move in to fill the vacancy created and, since the new level has a lower energy, emit the energy difference as a characteristic Xray photon whose wavelength depends on the difference in energy between the two levels involved. The characteristic lines of this type of spectrum are called K, L, and M and correspond to transitions from higher energy orbitals to the K, L, and M orbitals, that is to the orbitals of principal quantum numbers n = 1, 2,
Experimental methods in Xray crystallography
and 3. When the two orbitals involved in the transition are adjacent the line is called a,if they are separated by another shell, the line is called P. Thus, the Cu K, line is produced by a copper target in which the atoms lost an electron in the orbital of n = 1 and the vacancy was filled by an electron of the orbital n = 2. The Xray photon energy is the difference between these two energy levels. Since for every principal quantum number n there are n energy levels corresponding to the possible values of the quantum number 1 (from 0 to n  I), the a and /3 lines are actually split into multiple lines that are very close to one another because the difference between these energy levels is small. Still, Xray radiation corresponding to all the possible energy differences is not observed because some energy transitions are forbidden by the selection rules. Thus, although Fig. 4.2 has a scale on the abscissa which cannot show it, the Cu K, line is actually split into a doublet, the Km1 and K,, lines, of very similar wavelengths and which are, for this reason, not easily separable. The frequency of the characteristic line corresponding to a given transition is related to the atomic number of the element that gave rise to it, Z, by Moseley's law Y = C(Z  a)2 (4.3) where the constant C depends on the atomic energy levels involved in the transition and the constant a takes into account the interactions with other electrons. Thus, in a plot of Y " ~as a function of 2 for a given transition the points corresponding to different target elements lie in a straight line and different lines are obtained for the K,,, K,,, KB1, etc., transitions. The characteristic frequency is higher the higher the atomic number and so the Mo K, line ( 2 = 42) has a higher frequency and therefore a higher energy than the Cu K, line ( 2 = 29). A full list of the wavelengths of the characteristic lines of the elements which are used in Xray diffraction studies can be found in the International tables for xray crystallography.['1 Here, we will just point out that the two most frequently used lines are the Cu K, line, 12 = 1.5418 A and the Mo K, line, 12 = 0.7107 A. Both are doublets of slightly different wavelengths as pointed out before. The intensity of a characteristic K line can be calculated using the equation: ZK = Bi(V  VK)'.' (4.4) where B is a constant, i the electrical current, and VK the excitation potential of the K series, a quantity which is proportional to the energy required to remove a K electron from the target atom. It can be shown[21 that the ratio zK/zwis a maximum if the accelerating potential is chosen to be V = 4VK. If this condition is fulfilled, the K, line is about 90 times more intense than the white radiation of equal wavelength (I,). The K,, line is approximately twice as intense as the K,, line and the ratio K,/KB depends on Z but it averages 5 (see ~ieck'']).The data collection methods that use monochromatic radiation discussed later all use K, radiation and therefore require the elimination of the Kg component of the spectrum which is always present. The methods used to achieve this are discussed on p. 241.
Sealedtube and rotatinganode generators A conventional generator consists of a highvoltage power supply with electronic controls, connected to either a sealed tube or to the cathode of a
1
231
232
1
Hugo L. Monaco
FIL
WATER
CATHODE
I
FOCUSING
I
CUP
\
1
WATER
1
FILAMENT
R OA TA X TI SI O N
Fig. 4.3. (a) A sealed Xray tube. (b)Sketch of a rotatinganode chamber. The path followed by the water that cools the anode is not shown in the figure. The anode is cylindrical and rotates about the axis shown.
rotatinganode generator. In the second case there must also be a way of making, keeping, and monitoring the high vacuum required for Xray generation. Just how high the voltage to be applied must be, can be estimated from the considerations of the previous paragraphs and taking an excitation voltage given by ~ i e c k . ' ' ] This value for the copper K energy level is 8.981 kV so if one wishes to apply a voltage of 4 times V, about 36 kV have to be applied. For molybdenum even higher voltages are required. The sketch of a sealed Xray tube is shown in Fig. 4.3(a). It consists of a cathode with a filament that emits the electrons that are accelerated under vacuum by the high voltage applied and hit the fixed anode made of the metal whose characteristic spectrum has a K, line of a wavelength which is adequate for the diffraction experiment to be performed. The high vacuum is necessary because the presence of gas molecules in the tube decreases the efficiency of the Xray generating process by collisions with the electrons in the beam. The process of Xray production discussed in the previous section is highly inefficient: only about 0.1 per cent of the power applied is transformed into Xrays, the rest being dissipated as heat. In order to avoid melting of the target, it therefore becomes necessary to cool it, which is done by circulating cold water as shown in the figure. It is the efficiency of the cooling system that ultimately determines the maximum power that can be applied to the tube. The problem of heat dissipation also dictates the choice of the focal area of the beam of electrons on the anode. This area is always chosen to be rectangular with the sides in a ratio of at least six to one. In this way, when one looks at the focused electron beam on the target, which determines the surface that produces Xrays, in the direction of the longest side of the rectangle one can see, by choosing the appropriate angle, a small square focus with a side equal to the smallest rectangle side. At the same time, the real area that dissipates heat is several times that of a square of that size. The Xrays generated come out of the tube through four beryllium windows: the two that are shown in the figure, that are found in the direction of the longest axis of the rectangular focus, and another two in a direction perpendicular to it. The first two windows are used for singlecrystal work, the others may be used when a linear focus is needed. In rotatinganode generators, the target area seen by the electron beam is continuously renovated because the anode is rotated. In this way, much higher powers per unit of focal area can be applied to the unit and consequently higher Xray intensities can be produced. Figure 4.3(b) is a sketch of a rotating anode chamber showing the two Xray windows used for singlecrystal work, the filament, placed with its longest axis parallel to the direction of the windows, the focusing cup, used to focus the electron beam on the target, and the anode which rotates about an axis parallel to the direction of the windows. In a rotatinganode generator, the chamber has to be kept under vacuum for the reasons stated before, water has to be circulated to cool the anode as is done in the case of a sealed tube, and of course the anode has to be rotated at a certain speed. The system is therefore mechanically much more complicated than a tube and it requires a fairly frequent and demanding maintenance work. Figure 4.4 is a photograph of a modern rotating anode Xray generator. ~ h i l l i p s ' ~gives ] a detailed discussion of the advantages of
Experimental methods in Xray crystallography
Fig. 4.4. A rotatinganode Xray generator. (Photograph courtesy of Enraf Nonius.)
rotatinganode generators together with an exhaustive description of the practical problems encountered in their operation.
Choice of the type of radiation As discussed above, the K, lines are those of highest intensity and therefore they are the ones that are normally used for standard Xray diffraction work. Thus, in practice, the choice of the wavelength of the Xrays generated by conventional equipment is limited to the values of the characteristic K, lines of the metals commonly used as targets. Two of these metals are most frequently used: copper and molybdenum; their K, transitions generate radiation with a wavelength of about 1.5 and 0.7A respectively. As will be seen later, for a given crystaltodetector distance and unit cell, the diffracted beams will be more separated on the detector if a longer wavelength is used. Thus, copper is used for macromolecular work in which one usually was large unit cell parameters and for the structure determination of organic molecules, which do not contain atoms that absorb this radiation strongly. Absorption of the radiation by the sample is therefore also a primary consideration in the selection of the wavelength to be used. Another consideration is the maximum resolution of the reflections that will be recorded. We saw on p. 155 that there is a limiting sphere of radius
1
233
234
1
Hugo L. Monaco
2 / A that limits the volume of reciprocal space accessible to diffraction experiments. This sphere obviously has a different size for the two types of radiation discussed and therefore molybdenum radiation may be required to record data to a resolution not accessible to copper radiation. Finally we mention the detection efficiency of the method that will be used to record the diffracted intensities. Film is a better detector for copper than for molybdenum radiation and some area detectors have been optimized for use with copper radiation. On the other hand, diffractometer counters have a very high counting efficiency for the Mo K, radiation which explains why this type of radiation is so widely used for smallmolecule singlecrystal Xray diffraction work.
Synchrotron radiation Xrays, as well as other types of electromagnetic radiation, can also be generated by sources known as synchrotron radiation facilities. In these installations either electrons or positrons are accelerated at relativistic velocities along orbits of very large radii, several metres or even hundreds of metres. These sources are, by necessity, very complex and those that produce suitable Xrays are limited, located mainly in the United States and Europe. However, since, as we will see, the Xrays they produce are in many ways much better than those generated by conventional sources, their use has grown steadily in the crystallographic community. As a result, more beam time has been made available to crystallographers and more synchrotron sources are planned for construction in different countries. Among those, the 6 GeV storage ring to be built in the USA[~]and the European Synchrotron Radiation ~ a c i l i t ~ designed ,[~] specifically to produce the best possible Xrays, promise to be of special importance is the development of this field. From the extensive literature that exists in this ever expanding field we recommend two very elementary description^,[^^'] an introductory textbook,['] and a more advanced treatise in several volumes.[g]In this last treatise chapters 1, 2, and 11 of volume 1 are specially relevant to our discussion; volume 3 of the series is totally devoted to Xray methods.
Generation of Xrays in a synchrotron radiation source
Fig. 4.5. Outline of a typical synchrotron radiation facility. The electrons or positrons are accelerated in the linear accelerator (linac) and then in the booster t o be finally injected into the storage ring where they are kept circulating for periods of several hours. The beam lines, not shown i n the figure, are tangential t o the particle trajectory. Notice the scale at the bottom of the picture corresponding t o 050 m .
It is well known that charged particles moving under the influence of an accelerating field emit electromagnetic radiation. The energy of this radiation is dependent on the velocity of the particle. If the velocity is like that of the electrons moving in an antenna, emission takes place in the radiofrequency range but when the charged particles, electrons, or positrons, move with a speed approaching that of light, the spectrum extends into higher energy regions covering the Xray range. An additional consequence of relativistic effects is a distortion of the angular distribution of the radiation. When the charged particles move at velocities approaching that of light, radiation is emitted in a very narrow cone parallel to the instantaneous velocity. In a synchrotron source the charged particles are made to move in closed trajectories, often circular or elliptical, and so the radiation is generated in cones tangent to the path followed by the particles (see for example chapter 1 of ~ o c h [ ~ ] ) . Figure 4.5 shows the essential elements of a synchrotron radiation source.
Experimental methods in Xray crystallography
Notice the scale at the bottom which gives an idea of the size of this type of facility. The basic element of the installation from which radiation is generated is the storage ring, a toroidal cavity in which the charged particles are kept circulating under vacuum. An extremely high vacuum is required or else the particles are lost by collision with the atoms present in the cavity. Prior to injection into the storage ring, the particles must be accelerated, for example, first by a linear accelerator and then by a booster as shown in the figure. The other two elements that are essential to the operation of the ring are the socalled lattice, that is the set of magnets which force the particles to follow a closed trajectory as well as performing other functions, and the radiofrequency cavity system which restores to the particles the energy they lose as synchrotron radiation. The beam lines, not shown in the figure, are tangential to the storage ring. It can be shown that a charged particle moving along a circular orbit emits as electromagnetic radiation the following power[8*9]
where P is the energy emitted per unit time, e is the particle charge, c the speed of light, E the energy of the particle, mo its mass at rest, and R the bending radius of the orbit. This equation explains why highenergy particles are required and also why only electrons or positrons are used. The power emitted by heavier particles such as protons is too low to be of significant importance. The quantity y, the ratio of the total energy to the rest energy of the particle, is of considerable importance since it is approximately related to the opening angle of the cone of radiation by where AI+!J is the emission angle in radians. A more exact relationship between these two parameters is given in reference [lo]. The total power emitted by the ring is the power emitted by a particle in one revolution multiplied by the number of particles and divided by the time it takes them to complete a revolution. The total power can be shown to be equal to[8391
P,,, = 2 6 . 6 ~ ~ ~ i
(4.7)
where the energy of the particles is measured in GeV, the magnetic field B in tesla, the current i in amperes and the power is obtained in kW. The power is thus seen to be directly proportional to the current in the storage ring. The radiation emitted at a modern storage ring comes from two sources: the bending magnets and the insertion devices. The first is the radiation we have discussed so far, the second is generated by special devices called wigglers and undulators which are briefly discussed below. An important property of the radiation generated by bending magnets is its wide spectral distribution which can be described quantitatively in terms of the spectral flux N which is the number of photons emitted per unit time interval into a relative band width AA/A into an angle element d e in the plane of the electron orbit and integrated in the vertical plane. It can be shown that the flux of radiation normalized to the ring current generated by
1
235
236
1
Hugo L. Monaco
bending magnets is equal toLs1 N(hv) = 1.256 x lo7 y Gl(y) photons s' mradI m ~  ' (0.1% band width)
(4.8)
where the factor Gl(y) is an energydependent function that can be found tabulated for example in the book by ~ a r ~ a r i t o n d o .The [ ~ ] variable y is defined as follows where E, is the critical energy associated with a magnetic field B which in keV is given by where E is measured in GeV and R, the radius of the bending magnet in metres. An alternative expression for E , is with B measured in tesla. A widely used parameter related to the critical photon energy is the critical wavelength A, E, = hv, = he/& = 12.4/Ac
(4.11)
where E, is measured in keV and A, in A. The spectra of total emitted flux for several synchrotron radiation sources is shown in Fig. 4.6 taken from ~aterlik.["] The critical wavelength, A,, is useful as an indicator of the suitability of a source for Xray experiments. As can be seen in the figure although it does not correspond to the maximum flux it is close enough to give a good idea of the position of this maximum. It can be shown that ideally the wavelength used at a synchrotron source should fall in the range 0.25ACto 4.0Ac. Table 4.1, taken from the literature,15] gives E,, A,, and other relevant parameters for the
WAVELENGTH (A) '
I
Fig. 4.6. Spectral distribution of several storage rings; a =ADONE (Frascati. Italy) (1.5 GeV, 105 mA); b = DCI (Orsay, France) (1.8 GeV, 250 mA); c = SRS (Daresbury, UK) (2.0 GeV, 685 mA); d = NSLS (Brookhaven, USA) (2.5 GeV, 500 mA); e = DORIS (Hamburg, Germany) (5.0 Gev, 100 mA); f = ESRF (Grenoble, France) (5.0 GeV, 565 mA). The critical wavelengths are indicated by arrows, notice their position relative t o the maxima. Recall that the photon energy of the Cu K, line corresponds to about 8 keV and that of the M o K, line t o about 17 keV. HOR = horizontal plane. (Figure taken from ~aterlik."")
I
124
12.4
124
0 12
I
I
1
I
PHOTON ENERGY ( K e V )
Experimental methods in Xray crystallography
1
Table 4.1. Relevant parameters of the Synchrotron Radiation Sources i n operation in 1987 (taken from reference 5) Name
Location
E(GeV)
R(m)
i(mA)
EAkeV)
Group I, E, s 0.06 keV N100 Surf II Tantalus I
Karkhov, USSR Washington, USA Wisconsin, USA
Group II, E, 0.062 keV Sor ring Siberia I Max COSY Teras ACO NSLS UV SOR Fian C60 Vepp2M Hesyrl Superaco SPRL Bessy Aladdin INSES Pakhara Sirius Adone
Tokyo, Japan Moscow, USSR Lund, Sweden Berlin, Germany Tsukuba, Japan Orsay, France Brookhaven, USA Okazaki, Japan Moscow, USSR Novosibirsk, USSR Hefei, China Orsay, France Stanford, USA Berlin, Germany Wisconsin, USA Tokyo, Japan Moscow, USSR Tomsk, USSR Frascati, Italy
Group Ill, E, 230 keV DCI SRS Vepp3 Photon Factory NSLS Bonn Siberia II BEPC Elsa Arus Spear Doris II Tristan ACC
Orsay, France Daresbury, UK Novosibirsk, USSR Tsukuba, Japan Brookhaven, USA Bonn, Germany Moscow, USSR Beijing, China Bonn, Germany Erevan, USSR Stanford, USA Hamburg, Germany Tsukuba, Japan
,30 keV Group IV, E, :
CESR Vepp4 Petra PEP Tristan
Ithaca, USA Novosibirsk, USSR Hamburg, Germany Stanford, USA Tsukuba, Japan
synchrotron sources in operation in 1987. If the spectral flux is transformed into power, i.e. the number of photons is multiplied by the energy of a photon hv, it can be shown that half the total power is irradiated below and half above the critical value A,. Other parameters of interest are the source size and the divergence of the irradiated beam. The charged particle beam in the storage ring has a Gaussian profile characterized by the parameter ox, in the horizontal and o, in the vertical plane. The full width at half maximum of the beam can then
1,I.J.)
Emittance ( x 10' m rad)
Insertion (devices)
237
238
1
Hugo L. Monaco
be calculated as 2.350 and the source area F is estimated as Similarly the angular distribution is characterized by the parameters ox, and a,, and the solid angle of emission is then estimated as Although a,, a,. and a,, a,, vary along the orbit their variations are correlated and it is thus useful to define another parameter, the emittance, which at special symmetry positions is found to be
The emittance is instead a constant along the charged particle path and it is thus another important parameter characteristic of an installation. The emittances of the synchrotron sources in operation in 1987 are also shown in Table 4.1. Another useful function, which is often used to compare the potential performance of two sources, is the spectral brightness, also called spectral brillian~e,'~] defined as the number of photons emitted per unit area of the source at point x, z over a 0.1 per cent relative band width per unit solid angle dS2 and unit time in the direction defined by the angles 3 (defined by the instantaneous velocity of the charged particle and the projection of the direction of observation onto the vertical plane) and 19 (defined by the projection onto the horizontal plane instead). It can be shown that [ ~ ] 2) the spectral brightness b is equal to (see ~ a r ~ a r i t o n d ochapter where N is the spectral flux. If one defines the central brightness b, which is the brightness for x = z = q = 0 it is obvious that
From this equation it can be seen that the brightness can be increased by increasing the flux or by decreasing the as. Decreasing the a s can be accomplished by reducing the emittance of the storage ring (eqn (4.12)). The emittance of a ring is thus a fundamental parameter to be taken into account in comparing the expected performance from two different sources. A radiation spectrum quite different from that produced by bending magnets can be obtained by the use of insertion devices. These are a series of periodically spaced magnets of alternating polarity which are inserted in a straight region of the ring and which do not alter the ideal closed orbit of the particles in the storage ring. Most insertion devices create a sinusoidal magnetic field which forces the charged particles to oscillate around the mean orbit. According to their characteristics they are called wigglers or undulators. The parameter that has to be examined to determine whether an insertion device is a wiggler or an undulator is the K parameter
Experimental methods in Xray crystallography
where a is the maximum deflection angle of the electron or positron trajectory, Bo is the oscillating magnetic field measured in tesla and A, is the period of the magnetic array measured in centimetres. Recalling that l l y is approximately equal to the natural opening angle AI), K becomes the ratio between the maximum deflection angle of the electron trajectory along the insertion device, a , and AI). When the parameter K >> 1 the device is called a wiggler. The effect of a wiggler on the emitted spectrum is to shift the critical energy E, to higher values and to increase the intensity of the radiation by a factor proportional to the number of periods of the magnetic array. No interference effects are observed and so the emitted spectrum is qualitatively very similar to that obtained from bending magnets. If the parameter K t. Some of  these values are reported in Table 5.1 and may be compared with the lEi corresponding experimental values to verify whether the structure is centrosymmetric or not. So far we have implicitly assumed that the observed structure factor moduli are on an absolute scale, but in general the values of IFhI:,,, obtained from the intensities Ihthrough eqn (3.41), are on a relative scale. Assuming that the thermal motion is isotropic and equal for all the atoms, we may write
(Fhl:bs= K t I O F ~ ~ ' exp (2~s')
(5.12)
where K' (reciprocal of the scale factor used in eqn (5.3)) is the scale factor, I°Fhl is the structure amplitude in absolute scale for atoms at rest, B is the overall isotropic temperature factor, and s = sin OIL.
Table 5.1. Theoretical values of some functions of \El obtained from the centric (5.10) and acentric (5.11) distributions and their comparison with the corresponding experimental values for the AZOS structure Theoretical Centrosymmetric
Noncentrosymmetric
Experimental for AZOS
Solution and refinement of crystal structures
1
323
Using the results of the statistical analysis of the intensities, ~ i l s o n [ ~ ] proposed a method to derive the values of K' and B. Let us consider a set of observed intensities falling within a restricted range of s, such that within this range the decrease of the f s with s may be neglected. The average value of both sides of (5.12) will be (JFobsJ2)s = K ' ( I o F J exp ~ ) ~(  2 ~(s2)) = K' C, exp (  2 ~(s2)) (5.13) from which
where (s2) is the mean value of sin2 O/A2 in the considered interval and
is computed using the tabulated values of the atomic scattering factors for atoms at rest for s = Dividing the reciprocal lattice into several intervals of s, (5.14) tells us that a linear relation will exist between In ( ( I F ~ ~ J ~ ) ~and / & (s2) ) and that a plot of these values obtained from the experimental data can be interpolated by the best straight line passing through them. The intercept of the line on the vertical axis will give us In K' and its slope the value of 2B. Figure 5.2 is an example of such Wilson plot for a typical small organic AZOS structure (pcarboxyphenylazoxycyanidedimethyl su~phoxide,[~~ hereinafter); the numerical values of the terms appearing in eqn (5.14), obtained from 1908 observed reflections, are given in Table 5.2. The main reason for the deviations of the experimental points from the straight line is the breakdown of the condition of equiprobability of all atomic positions, assumed in deriving (5.4) and (5.5); in fact, the presence of structural
m.
Fig. 5.2. Wilson plot of AZOS together with the formula of the compound.
324
1
Davide Viterbo Table 5.2. Numerical values of the different terms in eqn (5.14) employed to obtain the Wilson plot of AZOS shown in Fig. 5.2 Inter
~imitss'
1 2 3 4 5 6 7 8 9 10
Reflect
(s2)
(lF21),
Xs
0.0327 0.0655 0.0982 0.1309 0.1637 0.1964 0.2292 0.2619 0.2946 0.3110
3736.8 1359.5 821.2 420.2 292.8 234.4 146.2 73.0 52.0 46.3
2199.9 1322.9 1020.9 791.3 646.5 562.7 507.8 450.9 410.4 392.7
( I F I ~ ) . / ~ . In [(IFI):/~,I
[on no.
val
0.00000.0655 0.03270.0982 0.06550.1309 0.09820.1637 0.13090.1964 0.16370.2292 0.19640.2619 0.22920.2946 0.26190.3274 0.29460.3274
82 124 156 182 210 231 248 269 272 134
1.6986 1.0277 0.8044 0.5310 0.4529 0.4166 0.2879 0.1619 0.1267 0.1 179
0.5298 0.0273 0.2177 0.6329 0.7922 0.8756  1.2451 1.8209 2.0663 2.1378
regularities, such as the phenyl hexagon in AZOS, is in contrast with this assumption. The broken line in Fig. 5.2, obtained by leastsquare fitting, has a slope of 9.20 and an intercept of 0.72. From these values we can derive that B = 4.60 A2 and K' = 2.05. The normalized structure factors can then be calculated by means of the relation
\ K' exp (2Bs2)s
Of?
The last column in Table 5.1 gives the experimental values of several statistical indicators based on the IEl values of AZOS (space group P2,/a), which confirm the presence of an inversion centre.
The Patterson function and its use In Appendix 3.A (p. 182) the Patterson function was defined as the selfconvolution of the electron density p(r). According to (3.A.38) we have P(u) = p(r)
* p(r)
=
j p(r)p(r + u) d r
(5.16)
V
We have shown (see (3.A.39)) that the Fourier transform of P(u) is IF(r*)I2 ~ and vice versa (in symbols I ~ ( r * )=l T[P(u)]) P(u) = ~  ~ [ l ~ ( r *=) l ~IF( ] r * )I exp (2nir*
. U)dr*
v*
1
IF,)^ exp (2nih
=
V
' u).
h
Since IFh/= lFphl, we may write 1 P(u) = V
cos 2nh u h
and then P(u) = P(u), i.e. the Patterson function is always centrosymmetric even when p(r) is not. This is in agreement with the deductions of p.
Solution and refinement of crystal structures
176 concerning the centrosymmetric nature of all functions with real Fourier transform. Since 1 ~ ~ 1 depend ' on the interatomic vectors [cf. eqn (5.1)] we may expect that also P(u) will contain information on these quantities. This can be verified starting from the definition (5.16). Let us, for simplicity, suppose we have an idealized structure made up of n point atoms with an associated weight equal to their atomic number (Fig. 5.3). The integral in (5.16) then becomes a summation over the n points, and
In order to derive P(u), all the atoms of the original structure p(r,) are shifted by a fixed vector u to obtain the corresponding p(r, + u), then the products p(r,)p(r, u) are performed and finally all these contributions are summed; the products will be nonzero only when p(r, + u) #O, that is when a point in the translated structure (broken lines in Fig. 5.3) coincides with an atom of the original structure. This condition is verified only when the vector u coincides with an interatomic vector (in Fig. 5.3(a) u coincides with the vector 24), while for a general u (Fig. 5.3(b)) all point of the translated image fall into regions where p(r) is zero. In the first case the value of P(u) will be proportional to the product of the weights of the two superposed atoms, in the second P(u) = 0. In Fig. 5.3 a higher weight has been given to atom 1 (heavier atom) and in 5.3(c) the case of a vector u coinciding with the distance 14 is represented; it will be P ( u , , ~> ) P(uZ,~)) both being single Patterson peaks, as each corresponds to only one interatomic vector. Finally in 5.3(d) the case of a vector u coinciding with two parallel interatomic vectors of equal length is illustrated; two terms will contribute to the summation in (5.18) and P(u) becomes twice as large as P(u',~) and it is said to have a multiplicity of two. Let us, for instance, suppose that atom 1 is a sulphur and the others are carbons; we will then have: P(u2,4)= 6 x 6 = 36, P ( q 4 ) = 6 x 16 = 96 and, with reference to Fig. 5.3(d), P(u) = 2 x ( 6 6)=72. ~ From what we have seen so far it follows that the Patterson function will have maxima corresponding to all possible interatomic vectors within the unit cell; the height of each peak will be proportional to the product of the atomic numbers of the atoms connected by the vector u, multiplied by the multiplicity of the same vector. This concept can be further clarified by considering Fig. 5.4, where in 5.4(a) a set of N = 5 points is represented, while in 5.4(b) the corresponding distribution of interatomic vectors, and in 5.4(c) the same set of vectors, after they have been translated to a common origin, are shown; the last corresponds to the distribution of peaks in the Patterson function. The Patterson function will have the same periodicity as the electron density and therefore the size of the unit cell will be identical. On the other hand, the number of peaks in the Patterson function is much greater than that in p(r); given N atoms in the cell they will give rise to N' peaks in P(u), N of which will superpose on a single peak at the origin (they correspond to the N zero distances of each atom with itself), while the remaining N(N  1) are distributed over the cell. This higher density of peaks becomes a more serious problem for real structures with nonpointlike atoms. In fact the Patterson peaks are wider than the maxima in an electron density map. As illustrated in the onedimensional example of Fig.
+
1
325
326
1
Davide Viterbo
Fig. 5.3. Schemes for the construction of the Patterson function of a pointatom structure, in which each atom has a weight equal to its atomic number: (a) two images separated by a vector coinciding with the interatomic vector between atoms 2 and 4 of equal weight; (b) two images separated by a vector not coinciding with any interatomic vector; (c) two images separated by a vector coinciding with the interatomic vector between atoms 1 and 4 of different weight; (d) two images separated by a vector coinciding with the two parallel interatomic vectors of equal length between atoms 4. 8 and 6. 7.
(c) Fig. 5.4. (a) Scheme of a molecule formed by five point atoms; (b) corresponding representation of all possible interatomic vectors; (c) Patterson function obtained by translating all vectors in (b) to a common origin.
5.5, because of the nonzero width of the peaks in p ( x ) , the Patterson peaks will have a width twice as large. For these reasons the Patterson map of a structure, with even a moderate number of atoms, may appear as an almost featureless distribution of vector density. To overcome this problem it is convenient to employ a sharpening procedure, consisting in computing the Patterson function with coefficients IEhI2 or better IFhEh(.In fact the normalized structure factors correspond to a pointatom structure with no decrease of the atomic scattering factor with increasing sin 8/A.The (l$EhI coefficients are more convenient, because oversharpening is sensitive to the series truncation errors (cf. Fig. 3.16) and may produce spurious peaks or a downscaling of correct peaks in the map. It is also possible to eliminate the origin peak, which may obscure some short vectors, by subtracting from the coefficients the terms corresponding to the interaction of each atom with itself (i.e. the first term in the righthand side of (5.1)); the coefficient in the series (5.17) will be
Solution and refinement of crystal structures
1
327
where, of course, the 1 ~ ~ must 1 ~ sbe in an absolute scale. Figure 5.6 shows the comparison between a normal and a sharpened Patterson section. From the previous considerations about the height of the Patterson peaks, we can infer that the map will have prominent maxima when: 1. The structure contains a limited number of heavy atoms (i.e. with an atomic number Z, significantly higher than that of the other lighter atoms, ZI), giving rise to three types of peaks: 
Vectors
Height
heavy atomheavy atom heavy atomlight atom light atomlight atom
ZpZp very high Z ~ intermediate Z ~ ZIZIvery low
2. The molecular geometry is such that it will give rise to several interatomic vectors with almost the same length and direction (e.g. systems with condensed aromatic rings); these will correspond to multiple peaks. Before illustrating the methods for interpreting the Patterson function, let us first analyse how the symmetry of the crystal is reflected into the vector map. The following considerations apply: 1. Since all vectors are translated to a common origin, the symmetry elements in the crystal will be translated in the Patterson function so that they will all pass through the origin and at the same time they will lose their translational components. By applying these rules it can be seen that, of the 230 space groups, only 24 have a symmetry compatible with
Fig. 5.5. Illustration of the widening of a Patterson maximum with respect to the electron density maxima contributing to it.
328
1
Davide Viterbo
the Patterson function. Thus, for instance, we have: Crystal space group
Patterson group
Triclinic (PI, p i ) Primitive monoclinic (P2, P2,, . . . , P2,/c) Centred monoclinic (C2, Cc, . . . , C2/c) Primitive orthorhombic (P2,2,2,, . . . , . Pna2,, . . . , Pbca . . .)
pi P2/m C2/m Pmmm
2. The symmetry operators present in the crystal leave a trace in the Patterson function, consisting of particular clusterings of vector maxima ~ ] and sections. on specific lines or planes of the map, called ~ a r k e r [lines These are produced by vectors, with one or two constant components, between equivalent atoms related by symmetry elements other than the inversion centre. Thus, for instance, the space group P2,, with equivalent positions: x, y, 2; 2,y 4, Z, will have vectors between equivalent atoms located on a Harker section with coordinates (2x, 4,22). In fact
+
In the space group P2, the equivalent positions x, y, z and 2, y, Z give rise to maxima on the Harker section at (2x, 0, 22). In a similar way it can be seen that the space groups Pm and PC give rise to Harker lines with coordinates (O,2y, 0) and (0,2y, 4) respectively. The Harker lines and sections corresponding to some of the most common symmetry elements are listed in Table 5.3. The presence or lack of Harker lines or sections may also give valuable indications on the space group symmetry when this is not uniquely defined.
The heavy atom method The procedures for the interpretation of the Patterson function are greatly simplified when the structure contains a limited number of heavy atoms. The peaks due to the vectors between these atoms will dominate the map and it is therefore usually quite an easy task to derive the positions of the heavy atoms. Then, if the atoms have a sufficiently high atomic number, the information about their coordinates represents a good initial model; in fact, the term F i computed by relation (5.2) with the contribution of the M heavy atoms in the unit cell, generally represents the predominant contribution to the structure factor, as illustrated in Fig. 5.7. One may then assume that the phase @iof lFtl is a good approximation of the true phase of Fh and compute an electron density map using as Table 5.3. Harker lines and sections relative to the most common symmetry elements
Fig. 5.7. Argand diagram i n which t w o heavy atoms (with atomic scattering factors f, and f,) and six light atoms contribute t o the structure factor F; the resultant of the contributions of the two heavy atoms is quite close t o F.
2 axis 1) to a, b, c 2, axis 11 to a, b, c mmirrorI.toa,b,c a glide I to b, c b glide I to a, c c glide 1. to a, b
0, v, w ; u, 0, w ; u, v, 0 i,v, w ; u, 4, w ; u, v, u,O,0;O,v,O;O,O,w v, 0 ; 0, w u, 0 ; 0, $, w u, 0, $; 0, v,
4
4,
4,
4,
4
Solution and refinement of crystal structures
coefficients the observed amplitudes (to which all atoms in the structure will contribute) with the corresponding calculated phases $.;I The map will not only reveal the heavy atoms but also other atoms of the structure. In the most favourable cases the structure may be completed from the first electron density map, but in general it is necessary to operate in more than one cycle by the socalled method of Fourier synthesis recycling. Each cycle requires the calculation of the structure factors from the coordinates of the known atoms; their phases will then be used to compute a new electron density map. If the initial model is correct, each cycle will reveal new atoms until the structure is completed. From the previous considerations one may get the impression that it would be advantageous to have compounds containing atoms of high atomic number, but one has also to consider that their contribution to the diffracted amplitudes may became so dominant that the observed data will be almost unaffected by the contribution of the remaining light atoms. The definition of the final structure will then be rather inaccurate. It has been demonstrated empirically that the best ratio between heavy and light atoms is that for which
As the values of the ratio (5.20) become less than 1.0, then the interpretation of the Patterson function and the process of completing the structure become more and more difficult, but at the same time the accuracy of the refined positions of the light atoms will increase. As an example let us consider a hypothetical organic compound of formula C3,H3,04X, where X is a halogen considered as a heavy atom; then, supposing that there are two molecules in the cell, C 2: = 2708 and C 2; = 578, 2450, 5618 for X = C1, Br, I respectively and the ratios (5.20) will be 0.21, 0.90, 2.07 respectively. Supposing that the data measured for the three derivatives are equally good, the chlorine compound will be difficult to solve, but the refined structure will be quite accurate; with bromine the solution should be quite easy with still a reasonable accuracy of the final structure, while with iodine it will be very easy to solve the structure but its accuracy will be further reduced. In order to find the positions of the heavy atoms it is necessary to locate them with respect to the symmetry elements and to the conventional origin of the unit cell. Let as now consider some examples, assuming for the moment that the asymmetric unit only contains one heavy atom. 1. Space group PI. The vector between equivalent atoms related by the inversion centre, has component u = 2x, v = 2y, w = 22; once it has been localized on the map it will immediately give the heavy atom coordinates with respect to the origin chosen on the inversion centre. 2. Space group P2, (twofold screw axis parallel to b). As we have seen, the vector between equivalent heavy atoms gives rise to a peak on the Harker section at 2x, i, 22. From its position one may easily derive the x and z coordinates of the heavy atom; the y coordinate may be arbitrarily assigned in order to fix the origin along the twofold screw axis.? Let us
t This is correct in the process of finding a starting model formed by a heavy atom, but during the refinement a more robust way of fixing the origin should be used, as described in Chapter 2, p. 107.
1
329
330
1
Davide Viterbo
assume y = i; we will then have two equivalent heavy atoms at positions x, $, z and R, 2, which are related by an inversion centre (this is true for any makes it more obvious). The structure value of y, but the choice y factors computed with the contribution of the heavy atoms only will then be real quantities and the map obtained with the corresponding phases will be centrosymmetric, showing both the true structure and its mirror image (enantiomorph). It may be quite difficult to unravel one image from the other; a sufficient number of light atoms, all belonging to the same image, should be localized in order to break down the centrosymmetric nature of the subsequent Fourier syntheses. This may become easier when atomic groups of known stereochemistry or one or more atoms of intermediate atomic number (from Na to Cl) are present.
a,
=a
3. Space group P2Jc. This very common space group will be illustrated by means of the structure of the lowermelting isomer of methyl(phenylsulphonyl)furoxan, C 9 H s ~ 2 0 4 ~ [ s 1
The heavy atom is the sulphur and the value of the ratio (5.20) is 0.37. The general equivalent positions are: The twofold screw axis gives rise to a Harker section of type %, 4, 4  22 (Fig. 5.8(a)), while the glide plane generates a Harker line at 0,4  2y,i (Fig. 5.8(b)). Finally the inversion centre will produce a vector between equivalent heavy atoms of components 2x, 2y, 22. In Fig. 5.8(a) the highest peak is at u = 2x = 62.21100, w = 4  22 = 26.91100 and then: x = 0.189, 2 = 0.115. In Fig. 5.8(b) there is a large peak centred at v = 4  2y = 25.2/100 and therefore y = 0.124. The coordinates of the S atom found in this way are confirmed by the presence of a fairly large peak at position u = 2x = 0.384, v = 2y = 0.245, w = 22 = 0.230. Despite the low value of the ratio (5.20), the electron density map, computed with the signs derived from the contribution of the S atoms only, allowed the localization of all the other nonhydrogen atoms. The final coordinates of the sulphur in the refined structure are: x = 0.2880, y = 0.1249, z = 0.1143 (shifted by only 0.097 A from the original position). 4. Space group P212121. The highermelting isomer of methyl(pheny1sulphonyl)furoxan[81
crystallizes in this common noncentrosymmetric space group.
Solution and refinement of crystal structures
1
331
Fig. 5.8. Methyl(phenylsulphonyl)furoxan LMI: (a) Harker section u, $, w; (b) Harker line 0, v,
i.
332 ( Davide Viterbo
24 L
28 I
1
I
2133
$
I
1
I
I
I
I
J
'
(b) Fig. 5.9. Methyl~phenylsulphonyl)furoxanH M I : (a) Harker section v, w; (b)Harker section u, v, f ; (c) Harker section u, w.
i,
:,
The general equivalent positions are
The three mutually perpendicular twofold screw axes give rise to three Harker sections of the type 4,  2y, 22; 4  2x, 2y, 4; 2x, 4, 4  22 (Fig. 5.9(a, b, c)). In the first the highest peak is positioned at v = $  2y = 501100, w = 22 = 6.61100, giving y = 0.0 and 2 = 0.033. In the second the highest peak is at u =  2x = 38.2/100, v = 2y = 0/100 (in agreement with the first section) and then x = 0.059 and y = 0.0. In the third section the peak at u = 2x = 11.81100 and w = 4  22 = 43.2/100, confirming the coordinates derived from the first two sections, is not the highest peak but the fourth highest. The largest peak at 50 and 6.6 is in common with the first section, because of the special value of y = 0; the second and third peaks are
Solution and refinement of crystal structures

23 27 I
I
I
I
I
I
1
(d
probably due to an accidental superposition of several vectors connecting lighter atoms. Also in this case the Fourier map, computed with the phases due to the contribution of the S atoms only, revealed the whole molecule (excluding hydrogens) and the coordinates of the S in the final refined structure are x = 0.0589, y = 0.0094, z = 0.0343 (shifted by 0.0162 A from the original position). Let us now consider the case of a compound with more than one heavy atom, such as the complex F~,(co),,(Noc~H~)(Nc~H,),[~~ crystallizing in the space group p i with Z = 2. In Table 5.4 the coordinates of the highest peaks in the Patterson map are listed in decreasing order of height. The values of the function are on an arbitrary scale and can be scaled to their
Fig. 5.9. (Continued)
1
333
334
( Davide Viterbo absolute value by multiplying by the ratio C j Z?/P(O 0 0) = 82401364 = 22.6; the height of a single FeFe peak is Z;, = 676 in absolute scale and about 30 in the relative scale. The vectors between equivalent atoms linked by an inversion centre have components 2x, 2y, 22 and correspond to single peaks; we may therefore assume that maxima 10, 11, 12, and 13 are of this type. If we choose peak 10 as Fe(1)  Fe(1) the coordinates of Fe(1) are simply obtained by dividing its components by two. Once this has been done, we are not allowed to simply divide by two the components of peaks 11, 12, 13 to obtain the coordinates of the other Fe atoms. In fact in this way we wouldn't be sure that the other three Fe atoms are referred to the same origin as the first. Indeed in the space group PI there are eight different positions of the inversion centre where the origin may be chosen. In order to resolve this ambiguity the peaks corresponding to vectors between nonequivalent Fe atoms should be used, also taking into account the periodic nature of the Patterson function. For instance, for peak 11, we must consider the eight combinations: giving for Fe(2) the coordinates referred to the eight possible origins: Only one of these positions will account for the vectors Fe(1)  Fe(2) and Fe(1) Fe(2) in the Patterson. In our case it will be the last position; in fact u2 = 1.380, v 2 = 1.300, w2 = 1.645 will give x2 = 0.690, y2 = 0.650, z2 = 0.822. Peak 3 and peak 5 may then be interpreted as Fe(1)  Fe(2) and Fe(1) Fe(2) respectively, after these Fe(2) coordinates have been translated by 1.0 along the three axes to obtain the values listed in the bottom
+ +
Table 5.4.List of the highest Patterson peaks of the complex Fe,(CO)11(NOC2H,)(NC2H5) and their interpretation in terms of vectors between Fe atoms; Fe coordmates obtained from this interpretation Peak Origin 1 2 3 4 5 6 7 8 9 10 11 12 13
u
v
w
H
0 0.080 0.020 0.490 0.070 0.1 10 0.485 0.420 0.405 0.480 0.400 0.380 0.430 0.450
0 0.260 0.000 0.560 0.275 0.245 0.455 0.180 0.290 0.570 0.195 0.300 0.285 0.165
0 0.1 10 0.710 0.470 0.400 0.820 0.810 0.420 0.360 0.760 0.700 0.645 0.075 0.135
364 144 138 120 72 65 65 63 59 55 38 33 30 27
Interpretation
Solution and refinement of crystal structures part of Table 5.4. With a similar procedure we may deduce the coordinates of the remaining two Fe atoms listed in the table.
Advanced Patterson methods Procedures for the automatic determination of positions of heavy atoms from the Patterson function, have been developed both for small molecule^[^^^^] and for biological macromolecules.~1~161 The procedure implemented within the SHELXS86 computer program[lOlwill be briefly described. The list of the highest peaks in the Patterson map is analysed in terms of Harker and cross peaks. Several possible solutions are given and the selection of the 'best' solution to be further processed (by the methods described on pp. 36575) is done by means of two reliability indices (or figures of merit): an Rfactor based on E values (RE) and R(Patt) which measures the agreement between the observed and predicted (from the atomic numbers) Patterson values. We finally mention that there are other methods for interpreting the Patterson function, which may be applied also in the absence of heavy atoms. They are the so called vector and superposition methods which are described in some detail in Appendix 5.B.
Direct methods Introduction With the term direct methods are indicated those methods which try to derive the structure factor phases directly from the observed amplitudes through mathematical relationships. In general the phase and the amplitude of a wave are independent quantities and in order to understand how, in the case of Xray diffraction, it is possible to relate these two quantities, two important properties of the electron density function should be considered: (1) it is everywhere positive, i.e, p(r) 3 0 (positivity);
(2) it is composed of discrete atoms (atomicity). The relation between positivity and phase values may be simply understood by just imagining the computation of p(r) of a centrosymmetric structure as a Fourier series, first with all signs correct and then with all signs reversed: the first map will be everywhere positive or zero, while the second wiIl be negative or zero and therefore physically unacceptable. Two pictorial examples of how positivity restricts the possible values of the phases are described in the Appendix 5.C, while a more formal explanation will be given later. Historically, the first mathematical relationships capable of giving phase information were obtained, in the form of inequalities, by Harker and as per['^] in 1948 and then further developed by Karle and ~ a u p t m a n [ ' ~ l and by other authors. Because of their limited practical interest, they will not be treated here and the reader is referred to more specialized textbooks.[191In 1953 Hauptman and Karle['O1 established the basic concepts and the probabilistic foundations of direct methods; the great power of these methods in solving complex crystal structures had its highest recogni
1
335
336
( Davide Viterbo
Fig. 5.10. Comparison between p ( x ) and p 2 ( x ) for a onedimensional structure with equal and well resolved atoms.
tion in the Nobel Prize for Chemistry conferred in 1985 on the mathematician H. Hauptman and the physicist J. Karle. using the atomicity condition, was able to derive a Also in 1953 ~ayre,['~] very important relation. He considered that for a structure formed by well resolved and almost equal atoms, the two functions p ( r ) and p2(r) are quite similar and show maxima at the same positions. A onedimensional example is illustrated in Fig. 5.10. We have seen that the Fourier transform of p ( r ) is ( 1 I V ) f i and for the case of all equal atoms N
Fh =fh
.
exp ( 2 n i h q ) .
(5.21)
j=1
We can also define the structure factor corresponding to p2(r) N
Gh = gh
exp ( 2 n i h q )
(5.22)
j=1
where gh is the scattering factor of the 'squared' atom. The Fourier transform of p2(r) is ( l / V ) G h and, because of the convolution theorem, it will correspond to the convolution product ( l / V ) F h * ( l / V ) F h . Since Fh is a discrete function defined only at the nodes of the reciprocal lattice, the convolution integral (3.A.34) becomes a summation
From the ratio of (5.21) and (5.22) we also have
Fh = (fhlgh)Gh = OhGh, and (5.23) becomes
Oh Fh = y c FkFhk, k
which is Sayre's equation, valid for both centrosymmetric and noncentrosymmetric structures. Multiplying both sides of (5.24) by F,, we obtain
Solution and refinement of crystal structures
For large values of IFhJthe lefthand side will be large, real, and positive. It is therefore likely that the largest terms in the sum on the right will also be real and positive. It follows that, if IFkl and IFhkl also have large values, it will be @hk= 9)h+ 9)k+ 9)hkzO (5.26) which for centrosymmetric structures becomes where S(h) stands for the sign of reflection h and the symbol = stays for 'probably equal'. We note that (5.27) coincides with the indication obtained in Appendix 5.C. Relations (5.26) and (5.27) are expressed in a probabilistic form and indicate the necessity of applying probability methods to estimate their reliability. On the whole, the use of probability techniques to obtain relationships between phases and magnitudes, has proved to be the most important approach for the practical use of direct methods. We will therefore describe in more detail these methods and the procedures employed for their practical applications.
Structure invariants and semiinvariants As already mentioned, the goal of direct methods is that of obtaining the phases directly from the observed amplitudes. These last quantities are independent of the chosen reference system, while in general the phases depend on it. From the observed amplitudes we can only obtain informations on single phases or linear combinations of phases which are independent of the choice of origin (the other features of the reference system being already defined by the choice of the space group). Since their value depends only on the structure, they are called structure invariants (s.i.).[203221 The most general s.i. is represented by the product
when
Let us show that its value does not change when the origin is moved by a general vector ro. The structure factor of index h, referred to the new origin, will be N
x fi ',
FA =
.
exp (2nih (5  rO))
= Fh exp {2nih
rO) =1 41 exp [i(qh  2nh ro];
.
the modulus remains unchanged while the phase changes by Aq, = 2nh ro. The variation of the phase of the product (5.28), due to the same origin shift, will be
which is zero because of condition (5.29).
1
337
338
1
Davide Viterbo The simplest structure invariants are: N
1. Fooo= C Zigiving the number of electrons in the unit cell; its phase is j=1
always zero. 2. F h R h= IFhI2, which does not contain any phase information. 3. F,FkFh, with phase qh + qk+ called triplet invariant; we shall see that these invariants play a primary role in the procedures which will be described later. 4 . FhFkF,Fhkl with phase g,h + qk+ g,, + Vhkl called quartet invariant; its importance has been recognized in recent years.
5. With a simple extension it is possible to define quintet, sextet, etc., invariants. Considering that the practical use of these relations is still under discussion, we will just mention here that complex probabilistic formulae have been derived to allow the estimation of these higher invariants. Structure semiinvariants ( S . S . ) [ ~ ~are , ~ ~single ] phases or linear combinations of phases which are invariant with respect to a shift of origin, provided that the position of the origin is restricted to those points in the cell which possess the same point symmetry (the socalled 'permissible origins'). A basic property of a S.S.is its capability of being transformed into a s.i. by adding one or more pairs of symmetryequivalent phases. For instance, in a given space group possessing the symmetry operator C = (R, T), the phase qHis a S.S. if it is possible to find a reflection h such that
V = T H  Q ) ~ + Q ~ is a s.i., i.e. H  h hR = 0. Because of (3.37), relation (5.32) may be written as
(5.32)
+
q is independent of any choice of origin, while (p, and T will depend on it; however, the dependence is such that (5.33) holds and therefore the value of y H will not change if we move the origin within those points which maintain the vectors T unchanged (identical point symmetry). For instance in P?, g,,, is a S.S. since is a s.i. The origin is conveniently chosen on the inversion centres and then T = (0,0,0). The permissible origins are on the eight inversion centres present in the cell; any one of them, chosen as origin, will always give T = (O,O, 0). Alternatively, by applying (5.31) we can derive that the phase of g,, changes by Ag, = 2n2h ro when the origin is shifted of a vector ro. It is easy to see that Ag, = 0 (or 2nm) when the components of ro are 0 or 1 as happens for the eight inversion centres in (cf. Fig. 5.17). The qualitative example relative to the sign of F,,, described in Appendix 5.C, can now be related to a S.S.
.
Solution and refinement of crystal structures As another example, let us consider, in space group P2,, the phase q2h,0,21, which is a s.s., because is a s.i. for any value of k. When the origin is chosen on a twofold screw axis, then q = Q)2h,0,21  nk. The permissible origins are located on any of the fqur screw axes present in the unit cell (cf. Fig. 5.18). The two examples given above refer to single phases and are therefore onephase semiinvariants. We can generalize what we have seen so far to the case of the linear combinations of more phases. Thus, the combination C $h is a S.S. in PI if C h = 2H (i.e. if the three components of the sum vector are all even); in P2, it is a s.s. if C h = (2H, 0, 2L). A compact way to indicate these two conditions is: Ch = 0 mod(2,2,2) (meaning that each of the three components of the vector Ch gives a zero rest when divided by 2), and Ch = 0 mod (2,0,2) (with the same meaning as before for the first and third components, while the second must be zero). In general we may write C h = 0 mod o,, where o, is a vector, called semiinvariant modulus, with integer components; the vector C h is called the semjinvariant vector. In order to identify which phases or combinations of phases are s.s. one can refer to special tables (see, for example, ~ i a c o v a z z o [ ~in~ ]which ) the space groups are classified in such a way that those belonging to the same class have the same permissible origins. The same process may be carried out automatically on a computer following an algebraic approach.[23] Before considering probability methods, let us use the positivity property of the electron density function to obtain an indication on the value of triplet invariants. The development of the product FhFkFhk gives FhFkFhk =
z
fjl exp [2nih
. q,]
x
fj, exp [2nik
q,]
i2
il
x
fi, exp [2ni(h
 k)
.q,]
i3
For simplicity let us assume that reflections h, k, and h  k have similar sip B I A values and therefore the variation of the atomic scattering factors with the indices can be overlooked. In (5.36) we can separate the terms:
2)
I I
2 fifj,exp {2ni[(h  k) . (q,  ql)l>, ilh
which is proportional to (cf. (5.1)) IFh,I2 C, f;;
1
339
340
1
Davide Viterbo
which is proportional to IFk12i
f;;
which is proportional to IF,)^  2 f;; i
+ [k . (q,  q,)]} = R. If the electron density is positive, the atomic scattering factors, which are the Fourier transform of the electron density around each atom, will also be positive and the summation in (1) will then be positive. Recalling equation (5.A.9) the terms (2), (3), and (4) are proportional to lFh12 (lF12)) IFkI2 ( 1 ~ 1 ~and ))  ( 1 ~ )respectively ~ ) and for large values of IF1 they will be large and positive. The last term R is the only complex term, but being a sum of positive and negative quantities, it will on average be small; R may be considered as a 'noise' term. For large values of the structure amplitudes we can then write
+
FhFkFhk= C fj + K { J F ~+~ ' IF^^^+ IFhk12 ~ ( I F I ~ ) }R 3 0 .
(5.37)
i
In the case of a centrosymmetric structure this relation implies that, when IFh/, IFk[, and IFhkl are large, then the product of the three signs of the structure factors, S(h)Sfk)S(h  k) = + . This deduction is in agreement with (5.27), derived from Sayre's equation, and with the pictorial derivation given in Appendix 5.C.
Probability methods For the same reasons considered on pp. 3212, from now on we will use the normalized structure factors. The use of normalized amplitudes is also suggested by (5.37), which shows that the value of the triplet does not depend on the diffraction angle. Indeed we may note that at low sin 8/A, where the scattering power is higher, both the positive terms and the noise term R are larger, and that they decrease by comparable amounts as the diffraction angle increases. It is also important to point out that the use of normalized structure factors, corresponding to a pointatom structure, implicitly corresponds to a sharpening of the atomicity assumption for the electron density. In Appendix 5.D the probability formulae for triplet invariants are derived, here we will just consider the main results. For a noncentrosymmetric structure the distribution associated to (5.26), derived by ~ o c h r a n , ' is ~ ~given ] by (cf. (5.D.17)) where: (1) for equal atoms
Ghk = ( 2 / @ ) IEhEkEhkl;
Solution and refinement of crystal structures
1
341
Fig. 5.11. Trends of the probability distributions (5.38) for different values of the parameter G,,, given by (5.39).
(2) for nonequal atoms Ghk= 2 0 ~ 0 2 ~ IEhEkEhkl; '~
(5.39b)
N
with on=
C 27, 2, being the atomic number of the jth atom. In (5.38) L is j=1
a normalization term depending on Ghk only. P(Qhk) is a socalled von Mises distribution[251and Ghk is its concentration parameter; its trend is very similar to that of a Gaussian, as it is shown in Fig. 5.11 for different values of Ghk. All curves have a maximum at Qhk= 0, i.e, qh= qk+ qh, and their width around the most probable value narrows as Ghk increases. The variance of the relation will therefore decrease as Ghkincreases. are known (with associated If more than one pair of phases qkj, qhpk1 amplitudes I Ekjl and I Eh,]I ,), with j = 1, 2, . . . , r, all defining the same phase qh through triplet relations such as (5.40), then the total probability distribution for qh is given by the product of the r distributions of the form (5.38), which are assumed to be independent of one another; i.e.
where A is a normalization factor. The exponent of (5.41) may be developed as
where ah=
[(iG, cos oj j=1
TI1"
342
1
Davide Viterbo and
t
tan ph =
(iG, sin c+) '=I
(C G, cos j=1
I
1
with G, = Ghk, and mi = qk,+ qh+. Equations (5.42) to (5.44) are easily understood when the r relationships of type (5.40) are plotted on an Argand diagram as vectors of modulus Gi and phase mi; the angle between each vector and the real axis is an indication of a probable value of qh. In Fig. 5.12 the case with r = 5 is illustrated; it can be seen that r
r
H
AH = a,, sin Ph =
C G, sin m,,
OH = ahcos Ph =
2 G, cos LC)~
Fig. 5.12. Vector representation, in the complex
plane, of the combination of five triplets of type (5.40) involving the same reflection h.
and relations (5.42), (5.43), (5.44) become immediately clear. Finally eqn (5.41) becomes which still is a von Mises distribution with a maximum for qh= Ph and a variance[261depending on ah as shown in Fig. 5.13. For instance we may deduce that for ah= 2, (9,) = Ph f 50", while for a,, = 10, ( q h ) = Ph It 19". Equation (5.44) gives the most probable value of qh and is known as the tangent formula;[271as we shall see later, this formula plays an important role in the phase determination process. In the case of centrosymmetric structures the probability that the sign relationship (5.27) is true, is given byCz8](Appendix 5.D)
P' = 4 + $ tanh[(~,a;~"IEhEkEhkl)].
(5.46)
When several relations for the same S(h) exist the product of the different probabilities P(Eh) (given by (5.D.19)) should be considered. With a procedure similar to that described in Appendix 5.D, we obtain
Figure 5.14 shows the trend of (5.48); it can be seen that, when several terms, all with the same sign, contribute to the summation, then the absolute value of the tanh argument may become rather large and P f approaches the extreme values 1 or 0. In the past 1015 years probability methods have seen new important developments. Not only it has been possible to improve the estimate of triplets, but also to derive reliable estimates of other phase relationships, both s.i. and s.s. At the basis of the new approaches stands the following principle: 'It is possible to obtain a good estimate of s.i. or s.s. given "appropriate" sets of normalized structure factor moduli, which are statistically the most effective in determining the value of the given s. i, or s.s. '
t 2 0
0
4
8
12
16
Gora Fig. 5.13. Trend of the standard deviation, o,of the distribution (5.45) as a function of n,, defined by (5.43).
Solution and refinement of crystal structures
1
343
Fig. 5.14. Trend of P+ = $ + f tanh ( x ) (cf. (5.48)) as a function of x.
The first task will then be to identify these moduli, indicated as the phasing magnitudes, and rank them according to their effectiveness in estimating s.i. or s.s.. Given their set {JEl),the second task will be to derive the probability distribution P(@ I {IEI))
(5.49)
where @ is any phase relationship we want to estimate and the vertical bar after it stands for: 'given all magnitudes in {\El)'. Cochran's formula[24]for triplets, derived in Appendix 5.D, is a trivial example of such conditional distribution; in fact it may be seen as P(@hk I IEhl, IEkl, IEhkl). ~ c h e n k [ ~extended ~ , ~ ~ ] this principle to the case of fourphase s.i. (quartets):
Q = Q7h + Q7k + TI + Q7hkP
(5.50)
Their distribution, given the four associated magnitudes, derived by ~ i m e r s k a , [indicates ~~] that Q = 0, with a variance depending on = (2/N)
.
IEhEkElEh+k+lI
(5.51)
Because of the 1/N factor any reasonably sized structure will have very small B values, and for this reason quartets estimated in this way can not be used in practice. Schenk pointed out that quartet (5.50) could be considered = ql as the sum of two triplets, such as TI = ~ 7 , ~ 7 ,  qh+, and + qh+&.Then, if also I Eh+,I is large, we will have TI 0 and G = 0 and therefore Q = TI T, 0 with a strengthened reliability with respect to that indicated by (5.51). In a similar way we can see that the same quartet can be written as the sum of two other pairs of triplets, and that Q also depends on JE,+,I and IEk+,(. We can then say that the quartet not only depends on the four basis magnitudes IEhI, \E,I, (Ell, IE,+,+,I, but also on the three cross magnitudes (Eh+,I, IEh+lI, JEk+ll.If the last three moduli are also large, then the indication Q = 0 is strengthened. Empirically it was also found that, when the cross magnitudes have very small values, then Q n (since cos Q = 1, these are called negative quartets). Later ~auptrnan[~'] derived the probability distribution of Q, given the seven basis and cross magnitudes, and confirmed Schenk's empirical findings. He then formulated the neighbourhood principle,[331the concept
+


+

+
344
1
Davide Viterbo of neighbourhoods being very close to that of phasing magnitudes. ~ a t e r [ ~ ~ he also gave rules for deriving the neighbourhoods of the main s.i. and of some S.S.in the most common space groups. The representation theory proposed by Giacovazzo[35~361 is a generalization and a systematization of the previous ideas, as it gives precise general rules for identifying the phasing magnitudes, allowing, at the same time, a completely general use of the spacegroup symmetry. The first representation of a s.i. is formed by the invariant itself plus all symmetry equivalent s.i. differing from by a constant angle, which is a function only of the symmetry operators. The set of all basis and cross magnitudes which appear in the first representation forms the first shell of phasing magnitudes (first phasing shell). This definition will be clarified through some examples. The importance of taking the spacegroup symmetry into account is first illustrated by the case of a special triplet in the space group P2,2,2,: if the first reflection has kl even and I , odd and restricted phase 0, n , the second has h2 even and phase 0, n , and the third has consequently phase f n/2, then T = fn/2, in contrast with the indication T 0 given by (5.38) when the three normalized amplitudes are large. The symmetry operators in P212121 are: R, = I, T, = (0,0,0); R2 = (7, I , 1) (only the diagonal elements are indicated, all the others being zero), T, = (1,0, 1); R, = (1, i , i ) , T3 = (4, 4,O); R, = (T, 1, i ) , T, = (0, 4, 4); and a triplet equivalent to T may be written as

because 1, is odd and k, even. T and T', forming the first representation of the triplet, have the same G but opposite phase and their combination in a phase diagram (similar to that of Fig. 5.12) will give a null vector, which does not contradict the expected restricted value T = f n / 2 . The general use of the spacegroup symmetry in estimating triplets has been described by ~ i a c o v a z z o , [ ~who ' ~ also showed that for nonprimitive cells the l l f i factor in (5.39a) should be replaced by l / m P , where N, is the number of atoms in the primitive cell. Let us now consider the example of a quartet such as (5.50). As we have seen, Q in general depends on seven magnitudes, and when no special symmetry conditions exist, the first representation is formed just by Q and the seven magnitudes form the first phasing shell. On the other hand, if, besides the identity, there is an other symmetry operator C, = (R,, T,), which leaves some special reflections unchanged ( H = HR,) and if one of the cross reflection (e.g. h + k) is of this special type, then the quartet
is equivalent to Q [Q'  Q = 2n(h + k)T,], but with two new cross terms IEhR,+rland IEkRS+,I.In this case the first representation is formed by Q and Q ' and the first phasing shell contains nine magnitudes. Since the larger the number of phasing magnitudes the better the estimate of the s.i., a significant advantage is obtained by considering also Q'.
Solution and refinement of crystal structures
A numerical example will further clarify the above ideas; let us consider the quartet
Q = q 1 5 3 + 4)&1 + (PzI2 + Q)ji6
(C~OSS: 504, 365, 643)
in the space group P2,/c, for which R, = I, R, = ( I , 1, ?), R3 = (I, ?,I), R4= (1, ?, 1). The first cross reflection is such that (504)R4= (504), and an equivalent quartet may be set up with two new cross terms. As an example of second representation of a s.i. let us consider the case of a triplet T. Its second representation is defined as the set of all special quintets of type where H is any reciprocal lattice vector for which IEHI is large. Since the term added to T is null, then C = T, but the quintet will depend on four basis magnitudes JE,I, IEkl, IEh+kl, (EHl and on six cross terms IEh*Hl, IEk+nl, IEh+kfHI. If M vectors H are selected (80100 reflections with largest IEHI), then the second representation will be formed by M quintets and the second phasing shell will contain 10 x M magnitudes. Let us now consider a general nphase s.s.
In general (the few exceptions are beyond our scope) it is possible to find a phase qHand two symmetry operators Ci and Cj such that
is a structure invariant; h r indicates a reflection equivalent to h. Since q1 differs from @ by a constant term depending only on the symmetry operators, the estimate of q, gives at the same time the value of @. The collection of all s.i. q , , obtained by varying H , Ci and Cj forms the first representation of @ and the first phasing shell will contain all the associated basis and cross magnitudes. Let us now consider a few examples regarding onephase s.s., for which (5.55) reduces to (5.32). As we have seen, in P?, the S.S. q2, may be represented by the triplet (5.34), which alone will form its first representation with the corresponding phasing shell including the two magnitudes lEzhl and IEhl. The probability that EZhis positive was derived by Cochran and ~ o o l f s o nand [ ~ ~is~given by
which is greater than 4 when (EhI> 1 and approaches 1 as IEZhJand lEhl increase. Similarly in the space group P2, the first representation of the s.s. q2h,0,21 is given by the set of triplets (5.35) and the probability formula will be a function of all the magnitudes in the first phasing shell: IE2h,0,211 and {IEh,j,l()with j assuming all possible values of the index k within the set of measured reflections. In P2, onephase s.s. are special reflections with phase restricted to 0 or ;rt and the probability formula will be of the tanh type; we
1
345
346
1
Davide Viterbo
then have
: (
P+(EZh,O,U)= 1 + tanh
:030;312
IE2h,0,21\
C (l)*(IEhk,I2  I)) k
(5.57)
where the sum is over all values of k. The term (l)k=exp(nk) corresponds to the constant angle nk and is obtained by applying (3.37) to express the phase relation between qhkland qgki in (5.35). When all major terms in the sum have k even, then P+(E2h,o,21) > $ and S(2h, 0, 21) = when they have k odd, then P+(E2h,o,21) < $ and S(2h, 0,21) .= Formulae (5.56) and (5.57) and those for some other space groups were derived long before the concept of representation was introduced, and they were known as the C formulae[201. The second representation of a S.S. will also be illustrated by means of an example. In space group P212121let us consider the s.s. @ = q4O6) for which the first representation (5.55) reduces to the set of triplets
+.
+,
with variable k index. With an extension similar to that used to derive (5.53), the second representation is defined as the set of quintets with q varying over all reflections with IE,I large. The second phasing shell will include IEHI = IE4,,I, a term IEhI = IE2,,I for each triplet (5.58) and, for each quintet, lEql and the four cross terms IEH+,I, IEhRfql. Once the phasing magnitudes have been identified it becomes possible to derive the appropriate probability distribution (5.49). So far formulae have been derived for estimating: (1) onephase s.s, by the second representation;[3w11 (2) twophase S.S.by the first (3) triplets by the second representation (PI0 (4) quartets by the first r e p r e s e n t a t i ~ n . [ ~ ~ , ~ ~ I In most cases, the derived probability distributions for noncentrosymmetric structures have the form of a von Mises function as (5.38) and for centrosymmetric structures the tanh form of (5.48); the concentration parameter G or the tanh argument are now substituted by more complex functions of the considered phasing magnitudes, which will not be reported. Only their practical use will be illustrated in the following sections.
Fixing the origin and the enantiomorph In the previous sections we have seen how it is possible to derive the values of s.i. and s.s. from the observed magnitudes. In order to pass from these values to those of the individual phases it will be necessary to fix the origin, and, in noncentrosymmetric space groups, it will be necessary to choose between the two enantiomorphic forms compatible with the observed amplitudes; in fact, since all the phases change their sign in going from one form to the other, the same will apply to s.i. and S.S. For this reason all probability formulae, such as (5.38), only define the cosine (i.e.
Solution and refinement of crystal structures
the absolute value) of the s.i. and S.S.In order to obtain all phases referred to one form it will be necessary to fix the enantiomorph. The phase determination process can then be summarized as shown in the flowdiagram of Fig. 5 .l5. The choice of the space group with the corresponding set of symmetry operators already imposes some restrictions on the points where the origin may be localized. Indeed, only the sites with the same point symmetry will be suitable and represent the socalled permissible origins. We will then have to choose the origin among the permissible ones and this may be performed by fixing the value of a limited number of suitable phases. In order to show how this is possible, let us first consider a onedimensional structure (Fig. 5.16(a)) formed by three atoms of different atomic numbers ( 2 , = 3, Z 2 = 2, Z3 = 1 and C 2, = 6). The unitary structure factor for this structure, referred to an origin at Xo, will be
1
347
/
Estimate i s . and s,s!s
I
I
O r i g i n (and e n a n t i o m o r p h )
I
I
definition
I
Fig. 5.15. Flow diagram of the phase determination process by direct methods. 3
(i/6)
Z, sin 2nh(x,  Xo).
(5.60)
j=1
When the origin is shifted so that Xo varies from zero to the identity period a, the trigonometric terms in (5.60) will change and Ah, Bh, and therefore Uh, will follow these changes. The modulus JUhl does not depend on the position of the origin, and only the phase qh will depend on X,. Figure 5.16(b) illustrates this variation in the case h = 1: we can see that at Xo = 0, q1= 109", while at Xo = 0.7, ql = 0". A change of enantiomorph is achieved by inverting the direction of the x axis; again 1 Uhl will not change, while all phases will change their sign ( q + 360  q). Since there is only one value of Xo for which q1= 0°, then the origin is uniquely defined by fixing q, = 0". In Fig. 5.16(c) the variation of q2 with X, is also shown: it can be seen that q2goes to zero at two points, Xo = 0.26
170
292 2i6
374 3b8t40 I
85
299 223 3 k 5 it
177 131 (c)
I
92
,
Xo h.2
4658' I Us 0 . 4 4
Fig. 5.16. (a) Onedimensional structure made of three nonequal atoms; (b) values of the phase ra. for different origin positions; (c) corresponding values of the phase p,.
.
8
348
1
Davide Viterbo
and Xo = 0.76, at a distance a12 from each other. Fixing q, = O" does not define the origin uniquely, but only restricts its possible position to two points; in general, by fixing qh= 0°, the origin is restricted to h possible positions. It should finally be observed that at X o = 0.7 (position for which q1= 0") q2= 315", and a change of enantiomorph will give q2= 45". It can then be seen that the enantiomorph can be chosen by restricting the value of q, (or in general of another phase q h ) within the interval 0n (or, as in our case, n2n). Let us now generalize to three dimensions the procedure just described to fix the origin in one dimension. We will first consider the space group PI, in which any point of the unit cell is a permissible origin and therefore no semiinvariants which are not at the same time invariants exist. In analogy with the onedimensional case, we can uniquely fix the origin along the x axis by fixing the phase of the (100) reflection and thus restricting the possible origins to lie on planes parallel to (100). Similarly the origin may be fixed in the other two directions by fixing the phases q,,, and q,,. The three reflections (loo), (OlO), and (001) define a primitive cell in the reciprocal lattice, but in a triclinic lattice there are infinite ways in which a primitive cell may be chosen. Indeed, any three noncoplanar vectors
will define a primitive cell if
.
.
HI Hz A H3= V* = a* b* A c* = volume of the reciprocal cell. Using (5.61) and developing the mixed product we can easily obtain
?Z
The three vectors will then form a primitive cell if
A=
(1 1: :I
h2 k2 12 = f l . (5.63)
By fixing q,, = 0" we will restrict the possible origins to lie on planes parallel to the crystallographic planes of indices HI. If we also fix q,,, = 0°, the possible origins will be at the same time restricted to lie on planes parallel to the planes Hz, i.e. they will lie on the intersection lines between the two sets of planes. Finally, by fixing q,, = O" (with H, # mH, nH2, m, n positive or negative integers) the origin will be further restricted to be at the intersection points of the above lines with the planes parallel to the H, crystallographic planes. The number of such points within the unit cell is given by the value of A and only when the primitivity condition (5.63) is obeyed, the three phases will fix the origin in a unique way. In the space group PI the permissible origins lie on the eight distinct inversion centres in the unit cell (Fig. 5.17). When the origin is shifted, for
+
Fig. 5.17. Position of the eight distinct inversion centres in a P I unit cell, corresponding t o the positions of the permissible origins, numbered as i n Table 5.5.
Solution and refinement of crystal structures
1
349
Table 5.5. Sign variations for the reflections divided into parity groups, when the origin is placed at the different inversion centers in the P1 cell of Fig. 5.17 Origin
Parity
instance, from (O,O, 0) to (i,0, O), the phase cpH of the reflection H = (hkl) will change by nh; this is equivalent to saying that the sign of the reflection will change or not depending on whether h is odd (u for ungerade in German) or even (g for gerade). Any change of origin among the eight permissible ones will have an effect on the sign of a reflection H which will depend on the parity of the three components h, k, or 1 (cf. Table 5.5). Reflections of type ggg are structure semiinvariants and may not be used to distinguish among the possible origins. If we consider a reflection of different parity, e.g. ggu, by imposing that its sign must be , we restrict the possible origins to lie on four points (in Table 5.5 these are the origins 1, 3, 5, 7). In order to further reduce the ambiguity we will have to fix the sign of a reflection of different parity (not ggg), e.g. ugg; with reference to Table 5.5, by fixing the sign to be + , the possible origins are restricted to points 1 and 3. In order to fix uniquely the origin, we will have to fix the sign of a third different reflection. Its parity should not only be different from that of the two already chosen, but it must also be different from ugu (for which both origins 1 and 3 have a + sign); in fact the combination ggu ugg ugu = ggg is a s.s. We will, for instance, choose uug. The above rules given for PI are also valid for all primitive centrosymmetric space groups with symmetry not higher than orthorhombic. Similar procedures may be devised for the other space groups. If along a given direction the origin is restricted on points separated by 4, then it can be fixed by fixing the phase of a reflection with an appropriate parity. When the origin can be shifted in a continuous way along an axis, it is possible to fix it by using a reflection the phase of which only takes unique values within the corresponding unit period. Thus, in space group P2, (Fig. 5.18), with the b axis parallel to the twofold screw axis, the permissible origins are all the points on the four 21 axes at (0, y, 0), ($,y, 0), (0, y, i), (4, y, 4). The choice of the twofold screw axis corresponds to that of one of the four inversion centers on the projection along y ; the projection reflections h01 have restricted phases 0, n. The phases q,,,, are S.S. and indeed the (gOg) crystallographic planes pass through all permissible origins. O n the other hand, a phase quo,will have, for instance, a zero value if the origin is chosen at (0, y, 0) or (0, y, i), and a n value if the origin is on the other two screw axes. By fixing quo,= 0" the
+
+
+
Fig. 5.18. Projection along the y axis of a P2, cell with the twofold screw axis parallel t o b.
350
1
Davide Viterbo
origins are restricted on the first two 2, axes. A second phase of type qgoU (or q~,,,) will assume a zero value at (0, y, 0) and a n value at (0, y, i), and by fixing qgoU = 0" the origins are restricted to lie on the first screw axis. In order to fix uniquely the origin along the y axis, we will have to fix a phase of type q,,,, because the (hll) planes intersect the y axis only once within the period b. Let us finally consider the very common space group P2,2,2,, in which the permissible origins are located at the eight points midway between the three orthogonal, nonintersecting 21 axes. The origin may be fixed in a simple way by using reflections belonging to the three principal zones (Okl), (hol), and (hkO). These reflections have phases restricted to two values: 0, n or k n / 2 depending on whether the index following the zero, in a cyclic way, is even or odd (cf. Chapter 3 , pp. 1578). It is therefore possible to apply the rules derived for the space group PI: the origin may be fixed by fixing the phases of three zone reflections belonging to three linearly independent parity groups (not ggg). In the examples considered so far, we have always used three phases to fix the origin, and this is true for all primitive space groups up to the orthorhombic system. In the centred space groups some of the permissible origins are related by translational symmetry and are indistinguishable. For this reason the number of phases needed to fix the origin is reduced, as, at the same time, is reduced the number of allowed parity groups. Thus, for instance, in a Ccentred lattice all ugg, ugu, gug, and guu reflections are systematically absent and the origin is fixed by fixing the phases or the signs of two reflections belonging to the other four parity groups. Going from one enantiomorph form to the other will change the sign of all individual phases and, as a consequence, the sign of all linear combinations of phases. Therefore, the most general way of fixing the enantiomorph will be that of restricting a suitable s.i. or S.S. within the interval 0n. Let us for instance, consider the space group P21. Suppose that the two phases q,, and qZl3have been assigned zero value to fix the origin; they form a triplet invariant with qjil By restricting 0 S vji1 G n also 0 G Q, S n and, if its value is sufficiently far from the extreme values zero or n,this choice will fix the enantiomorph. Unfortunately the most probable value of Q, is zero and in this space group it may be difficult to properly fix the enantiomorph by restricting the phase of one reflection. This problem does not arise in the space group P2,2,2, as will be shown by the following example. Suppose that the origin has been fixed using reflections of type: uOg (with phase 0, n ) , guO (0, n ) and Ouu ( f n/2). Since all linear combinations of phases for which the sum of the indices is ggg, are S.S. in this space group, it is possible to set up S.S. with value restricted to f n/2; the choice of one of the two values allows an unambiguous choice of the enantiomorph. For instance Vuo,
+ Vu,o
= fn / 2
is a twophase s.s.; if quo,is fixed to be zero, then the sign of the s.s. will depend on the value chosen for q,,,. By choosing q,,, = n / 2 we fix the enantiomorph.
Solution and refinement of crystal structures
For a complete and general theoretical treatment of the procedures for fixing the origin and the enantiomorph in all space groups, the reader is addressed to more specialized textbook^.['^,^^] A very effective way of defining the enantiomorph, and at the same time the absolute configuration (see later), is represented by the experimental measurement of some triplet phases with value close to fn/2, by multiple diffraction experiments (cf. Chapter 3, p. 191). In general the availability of a certain number of experimental tripletphase values, which unfortunately are not easy to obtain, would be of great help in solving a structure by direct methods.
Phase determination procedures We will first describe some of the steps which are common to all direct methods practical procedures.
Normalization By the method described on p. 3234 and using equation (5.15), the values of the normalized structure factors are first calculated. Most computer programs will supply a list of reflections sorted in decreasing order of JEl and perform a statistical analysis of the normalized amplitudes as shown earlier. In some cases a more detailed statistical analysis is carried out in order to reveal the presence of pseudotranslational symmetry (cf. Appendix 5.E).[4s521 Some of the most recent programs allow one to introduce the available a priori information, such as the existence of pseudotranslational symmetry or the coordinates of a previously located fragment;[53,541 examples of the use of this information will be given later.
Setting up phase relationships We will focus our attention on triplets, the procedures for setting up other s.i. or S.S. being similar. Since the most important relations are those estimated with the highest reliability, we will only set up triplets relating reflections with large JEl.The minimum IEI value is chosen in such a way that the number of reflections employed is approximately equal to ten times the number of atoms in the asymmetric unit and usually lies between 1.2 and 1.6. For each reflection h all pairs of reflections k and Rk with large IEl must be found; the set of all relationships obtained in this way is often called the C P listing. The triplet search must take into account the reciprocal lattice symmetry and the relations between the phases of equivalent reflections. If all the indices are reconducted within the same independent portion of the reciprocal lattice, each reflection h will have to be combined with all vectors fkRi, obtained by varying R, over all rotation matrices of the space group not related by an inversion centre; if also the JEl value of reflection h f kR, is large then the triplet is retained. In general this third reflection will not be in the considered independent portion of reciprocal lattice, and it can be expressed as fHR,. The phase relationship will then become
1 351
352
1
Davide Viterbo Most computer programs store triplet relations in the form
where n h , nk, n, represent the sequential numbers of the corresponding reflections in the sorted list, with the sign indicated by (5.64), A 9 = 2n(kTi HT,) and G is either defined by (5.39) or it is the parameter obtained by means of the second representation. For centrosymmetric structures (5.64) reduces to
+
and in (5.65) the signs are of no use, while G represents the tanh argument in (5.46) or the corresponding value from the second representation.
Definition of an optimum starting set of phases From (5.64) or (5.66), given the two phases or signs in the righthand side we can derive an estimate of the lefthand side phase, the accuracy of which will increase with increasing G. We have seen that the origin may be fixed by assigning an arbitrary value to up to three phases. Even if these are chosen among the reflections involved in large numbers of triplets, in general they will not be sufficient to start up the phase determination process. It is necessary to start with a larger number of phases, and the problem is not overcome even when a limited number of reliably estimated onephase S.S. (usually fewer than five) is available. Two methods are used to define the values of the extra unknown phases necessary to start up the process. With the symbolic addition[ss2261 method these phases are assigned a symbolic value and all other phases are determined as combinations of these symbols; it is more suitable for centrosymmetric structures as we shall see later through an example. With the m ~ l t i s o l u t i o n [method, ~ ~ ~ ~ ~the ~ unknown starting phases are directly assigned permuted numerical values. This method is easier to automate and can more readily incorporate some of the most recent developments in direct methods; for this reason it is more widely used and will be described in more detail. Given the phases in the starting set, all other phases are determined one after the other in a chain process. The choice of the reflections in the starting set is therefore very important and the best starting set will be that allowing one to eliminate, as much as possible, the weak links in the chain, i.e. the poor determination of some phases by few lowreliability relationships. An optimal starting set of phases can be defined by means of the convergence procedure.[s71We have seen that a,, as defined by (5.43) is a measure of the reliability with which a phase cph may be determined combining several phase relations. If the vector representing ahin Fig. 5.12 is rotated by an angle Ph = ( G h ) in such a way that it falls on the real axis, Fig. 5.19 is obtained; it can be seen that
where Qz, = ( q h ) qkl q h p k l ZQhk1. Since at the beginning the phases are not known, a,,can not be computed, but it can be estimated a priori by
Solution and refinement of crystal structures
1
353
Fig. 5.19. Figure 5.12 rotated by an angle Ph = (v,) in order t o bring the vector ah on t o the real axis.
I
substituting each cos Qj in (5.67) with its expected value, defined as 1
Il(Gj) cos 6, exp (G, cos 9)d6, = Dl(Gj) (5.68) Io(G,) where Io(x) and Il(x) are modified Bessel functions of zero and first order. These functions and their ratio are readily available[581and Fig. 5.20 illustrates the trend of (5.68) as a function of G ; it may be seen that the ratio tends asymptotically to 1.0 as G increases. The estimated value (cu,) is then given by (COS6 , ) =
2"
and it can be computed for each reflection, before any phase information has been obtained, using the G values only. The convergence process is a step process in which, at each step, the reflection with minimum (a,,) is (temporarily) eliminated, provided it is not an accepted onephase S.S. or another reflection already included in the starting set. When a reflection is eliminated, at the same time, all phase relationships contributing to it are eliminated and the (a,,) values of the other reflections involved in these relations are updated. Since, at each step, the reflection which is less related to the remaining reflections is eliminated, the process must converge towards the group of reflections which are most strongly interrelated and are therefore the most effective in starting the phase determination process.
Fig. 5.20. Trend of the ratio, I , ( G ) / I , ( G ) ,of the modified Bessel functions of first and zero order, as a function of G.
354
1
Davide Viterbo
Before eliminating a reflection, the remaining ones are analysed to check if it is still possible to fix the origin; if not, the reflection is not removed but kept in the starting set as an originfixing reflection. If, in the final steps, a reflection is eliminated with an (a,,),which, at the elimination moment, is reduced to zero (or to a very low value), than this reflection is not (or is only poorly) connected with the remaining few reflections; on the other hand it is an essential link between these last reflections and those previously eliminated. By putting this reflection into the starting set, we assign a value to its phase and in this way we insert the missing link (or replace the weak link) in the chain process. The convergence process is repeated several times, each time adding a new reflection into the starting set, until the desired number of startingset reflections has been reached. The flow diagram of Fig. 5.21 illustrates the convergence procedure. The procedure may be further improved by assigning to each contributor to the summation in (5.69) a weight depending on (ct.,) and (a,,) .[591
Calculate
at t i m e of elimination
r
goes into starting set,
I
t
Solution and refinement of crystal structures
Figures of merit As we shall see, the phase determination process usually leads to more than one solution. Given several sets of phases it would be rather time consuming to compute and interpret all the corresponding electron density maps to see which yield the correct structure. It is instead easier to compute some appropriate functions, called figures of merit (fom), which allow an a priori estimate of the goodness of each phase set. Several functions have been proposed[60]and we will analyse those most commonly used. MABS (absolute fom) represents a measure of the internal consistency of
the employed triplet relationships in estimating the phases. It is defined as
for a correct structure A should be close to the theoretically estimated A, and MABS = 1.0. In practice it has been found that often for the correct set of phases A > A , and MABS values between 0.9 and 1.3 indicate a promising phase set. R, fom: this is a measure of how much triplets deviate from their expected statistical behavior and is defined as ~
c
=e
lo0(z h

(ah)~)be;
(5.71)
it should be minimum for the correct set of phases. tpo fom: this is defined as
where the outer summations are over a certain number (50150) of reflections with lowest lEll value. The tripletgenerating routine will have to set up also the relationships ( q Otriplets) linking each of these 1 reflections with pairs of reflections k and 1  k with large (El, the phases of which have been determined. The inner summation at the numerator corresponds to Sayre's equation (5.24) (written here in terms of normalized structure factors) relative to each reflection 1. Since [Ell= 0, the large terms in the summation must tend to cancel each other out and the correct set of phases value. This function differs from the will correspond to a minimum previous foms because it is not a selfconsistency figure among the determined reflections only, but it establishes the coherence of the obtained phases with some weak reflections not used for their determination.
vo
4.SSlFOM, SS2FOM, NTREST, NQUEST: these four functions have the same functional form:
1
355
356
1
Davide Viterbo with j = 1 for onephase s.s., j = 2 for twophase s.s., j = 3 for negative triplets, j = 4 for negative quartets respectively, and r running over all estimated relationships of each type; as shown in (5.68), D,(lGjrl) is the expected value of cosQjr. For instance in the case of negative quartets (5.73) becomes
where the summation is extended to all quartets estimated to be negative (G, < 0.0) by means of their first representation and Q, are the values of the individual quartets computed with the determined phases. The correct set of phases should give rise to the largest number of negative cos Q, values, thus maximizing NQUEST. Similarly for the other three functions, a good agreement between the estimated (through the Gj values) and the calculated cos Qj values, maximizes their values. The four foms based on phase relationships, are finally combined to give CPHASE =
TI + T2+ T3+ T4 Bl+BZ+B3+B4'
A better understanding of the statistical meaning of the MABS, R, and
qofoms was recently achieved by a more rigorous probabilistic approach,[60] which also allowed the derivation of some new effective functions. At the basis of this approach is the use of the probability distributions P(ah) of ah defined in (5.43) and P(a;) of a; defined in (5.72), derived by Cascarano et a1.[611On p. 322 we saw how the expectation values in Table 5.1 could be obtained from the distributions (5.10) and (5.11). By a similar method, from P(ah) and P(a;) it is possible to derive various theoretical moments, which may then be compared with the corresponding 'experimental' values computed using the different sets of phases; MABS and R, are related to moments of P(ah), while qo is related to a moment of P(a;), but the expected values of other appropriate functions of a,, and a; may also be derived and used as foms. Once the different foms have been calculated for each phase set it is useful to derive a combined figure of merit, CFOM; its capability of discriminating the correct set of phases will in general be higher than that of the individual functions. Different ways of combining the individual foms have been used; a more objective procedure is described by Cascarano et a1.[601in which each function is introduced with a properly estimated weight and the resulting combined fom is normalized to fall between 1.0 and 1.0. A correct set of phases should lead to CFOM==1.0, while CFOM
which is close to zero if the correlation is negligible and close to 1 for large correlation. Most programs compute the correlation matrix and output the offdiagonal elements which are greater than 0.5. No such correlation was found for AZOP. How low should the final R factor be in order to have good confidence in the quality of the refined model? The answer to this question is not straightforward, because it depends on the type and complexity of the structure and on the quality of the experimental data. Nevertheless, for small or medium size structures giving good quality crystals (as it is usually the case for most organic or organometallic compounds), with intensities collected at room temperature on a diffractometer, we should expect R values in the range 0.030.07. For very accurate lowtemperature measurements these values may be further reduced. The quality of the model should then also be assessed by looking at the standard deviations of the atomic parameters or at those of the derived geometrical quantities, such as bond distances, which should be less than 0.006A for nonhydrogen atoms. Usually as the complexity of the structure increases the quality af the crystals and of the diffraction data decreases, and, at convergence the R value may be in the range 0.080.15 for large molecules and up to 0.250.30 for macromolecules solved at low or medium resolution. In these cases the final model may still contain some fairly large errors, which may often be corrected by applying stereochemical or energy constraints (cf. Chapter 8, p. 568). The final R value will also depend on the selection of reflections used during the refinement. It is in fact common practice to discard the very
Solution and refinement of crystal structures
weak reflections, the intensities, I, of which are measured by diffractometer ; with I s na(Z), with large estimated standard deviations, ~ ( 1 )reflections usually with 2 G n G 3 (for AZOP n = 2 was used to select the 'observed' are omitted. Of course the higher is n the lower will be R, but too high a cutoff value will considerably reduce the number of observations and the leastsquares refinement will yield higher standard deviations (cf. Chapter 2, pp. 1024). There is no theoretical justification for discarding weak reflections, and a more rigorous procedure requires the use of all data with proper weights["] and a prior statistical treatment of weak reflections to account also for negative measurements.[80]On the other hand, in most cases, only for very accurate structural analyses would the latter procedure reveal significant changes in the final model. When the choice between a centrosymmetric and a noncentrosymmetric space group is ambiguous or when the structure shows pseudotranslational symmetry, the inclusion of weak reflections becomes essential.[811 In following the convergence of our refinement we have mainly used the R factor defined in (5.3); other agreement indices have been proposed, some of which are statistically more appropriate to assess the significance of small changes in the final refinement stages. Among them we recall the weighted residual proposed by ~ a m i l t o n [ ~ ~ ~
already considered in Chapter 2 (p. 103), where it was shown that the ratio of the residuals R;(l)lR&(2) obtained from two refinements of different models may be used for testing the significance of the difference between the two models. For instance this test may be used for determining the absolute configuration of optically active molecules from the effect of anomalous dispersion,[831although, as pointed out by ~ o g e r s , @some ~I caution is necessary. Although the R index is the most widely used criterion to assess the goodness of a structural model, its indications should be regarded with some caution. As an example of the weakness of the R index, let US consider the case of a structure containing one heavy atom, such as Pt, Ir, Os, or Cd, and a certain number of lighter atoms (C, N, 0 ) . Since the I$ value is less sensitive to the position of the light atoms, a model with the heavy atom correctly placed and the light atoms quite inaccurately localized will give a lower R value than a model with a small error in the position of the heavy atom and an almost correct position of the light atoms. Nevertheless the second model, with a smaller average position error and a uniform distribution of errors over all atoms, is certainly a better one. When the model is an incomplete representation of the molecule, R becomes a rather weak guide, as it measures the agreement between quantities which depend on largely different numbers of parameters (IF:] depends on all atomic parameters, while IFiI only depends on the limited number of parameters defining the incomplete model). The only valid check of the indication given by the R value is the convergence of the svbsequent Process of completing and refining the model. As mentioned in the introduction of this chapter, the refinement of a
1
371
372
1
Davide Viterbo
structural model will not converge if the model is affected by large errors. This is a direct consequence of the nonlinear nature of the problem, which, as observed in Chapter 2 (p. 93), implies the presence of several local minima in the function to be minimized. Two types of errors, which occur quite often, are particularly disturbing. 1. Incorrectly positioned molecule. It may happen that the structural model obtained by direct or Patterson methods is constituted by a correctly oriented molecule, but its position with respect to the symmetry elements is incorrect. In most cases the entire molecule is shifted by a vector corresponding to a large Patterson peak due to several superposing interatomic vectors. An example is given by the AZOP structure; the initial attempts at solving the structure by direct methods gave correctly oriented molecules, shifted from the correct position and their refinement would not converge to an R value lower than 0.25. The correct solution was only obtained after estimating the triplet invariants by their second representation. An alternative way, which is often successful when applied to structures belonging to the space group PI, would be to try to solve the structure in the lower symmetry group P I . The solution will give two molecules related by an inversion centre in a general position; this can be located by inspection and then, after translating one of the two molecules in such a way that it is referred to the inversion centre at the origin (i.e, the general coordinates of the inversion centre are subtracted from all atomic coordinates), the structure can be refined in PI. When these methods fail one can try to find the correct position by the Patterson method described in Appendix 5.B . 2. Wrong space group. As explained in Chapter 3 (p. 161), the determination of the space group from the diffraction data is not unique, and a wrong choice is more frequent than one might think. An interesting analysis of such errors is given by Marsh and ~ e r b s t e i n [ who ~ ~ ~noted ~ ~ ] that a relatively large number of structures has been reported with space group of unnecessarily low symmetry. Two types of structures can be considered: (i) those for which the reported space group has a lower Laue symmetry than that of the actual structure; and (ii) those for which the reported space group lacks a centre of symmetry, which is instead present. For the first type the correct space group may often be found using geometrical consideration^[^^^^^^ such as those implemented in the computer programs NEWLAT['~] or LEPAGE.[~'] For the second type, the refinement by leastsquares should in theory yield a singular matrix (cf. Chapter 2, p. 100), as half of the refined parameters have a linear relation (the overlooked inversion operation) with the other half; in practice this relation may not be exact, but in any case the solution of the normal equations will be very unstable with large errors in the atomic parameters and large values of their estimated standard deviations. The most common errors occur for the following space groups: P1 instead of PI, PC instead of P2,/c, C2 or Cm instead of C2/m, Cc instead of C2/c, Pna2, instead of Pnam, Cmc2, instead ~~). of Cmcm (several examples are given by Marsh and ~ e r b s t e i n [ ' ~ ~ 'They may be recognized because they usually lead to abnormal values of some bond distances and angles or of the thermal parameters, which are adjusted when the refinement is carried out in the correct space group.
Solution and refinement of crystal structures
A critical view (possibly a bit too pessimistic) of the accuracy of the reported structure determinations has been presented by ones[^'] and the reading of his paper is highly recommended. Two important effects may cause a lack of convergence in the refinement process: twinning and disorder. As we saw on p. 837, the diffraction intensities of a twinned crystal must be carefully analysed in order to separate the contributions from the different individuals forming the twin. This will be more difficult when all reflections from the two individuals superpose exactly (merohedral twins, cf. p. 85). Often merohedral twinning is not recognized and then in most cases the structure fails to be solved; even when a solution is found, it is impossible to refine the model to an acceptable R value because of the systematic errors on the observed amplitudes. Real crystals deviate from the ideal picture of a periodical perfect repetition of a unit cell. We saw on p. 148 that, because of the thermal motion, atoms oscillate around an equilibrium position and we may say that they are affected by a small dynamic disorder. But larger movements are sometimes possible in crystals, giving rise to a real dynamic disorder. Diffraction experiments will just show a timeaveraged situation and if the movement is continuous the electron density will be smeared out. On the other hand if the movement is stepwise between two or more energy minima, the total electron density will be divided between the positions of the minima. An example of such dynamic disorder in the cis form of the complex [ ( q 5 C 5 ~ 5 ) 2 ~ e 2 ( C 0 ) 2 ( ~ 2has  C been 0 ) 2 ] recently described;[921the two independent cyclopentadienyl rings show different thermal motions, which may be interpreted in terms of different rates of stepwise rotation around their fivefold axes. This hypothesis was confirmed by a recent solidstate NMR Another type of disorder may occur in crystals; it is referred to as static disorder and in this case the average contents of the unit cell is obtained by averaging over the space, i.e. over the different unit cells. An important example of this type of disorder, which is common in minerals and alloys, is the substitutional disorder where the same site is occupied by different types of atoms in different cells. The structure factors depend only on the time and spaceaveraged contents of the unit cell and the result of a diffraction analysis is this averaged contents. No distinction can be made between dynamic and static disorder and the case of a molecular fragment oscillating between two positions in all unit cells is indistinguishable from that in which half of the cells have the fragment in one position and half in the other. If a disordered structure is refined without taking into account the disorder, then only an average structure is obtained with abnormal thermal motion and the refinement will not converge. In the case of substitutional disorder the different atomic species are introduced with the same coordinates but with different occupation factors (cf. p. 87), depending on the fraction of each species. When the disorder is between, say, two positions in the cell, then the same atomic species are located in both possible positions with an occupation factor depending on the 'population' of each position (the term population will be associated with the fraction of time spent in the given position in the case of dynamic disorder and with the fraction of cells having atoms in that position in the case of static disorder); if this is not
1
373
374
1
Davide Viterbo
known one may initially assume an occupation factor of 0.5 and than refine the factor to convergence (the occupation factor is highly correlated to the temperature factor and some caution should be used in the leastsquares refinement). Only when disorder is treated in a proper way will the refinement converge to an acceptably low R value.
Absolute configuration In Chapter 3 (p. 168) it was shown that, when the anomalous dispersion effect is present, Friedel's law is no longer satisfied. We shall see in Chapter 7 (p. 489) that for compounds containing asymmetric carbon atoms, isomers of opposite chirality (enantiomers) are possible and that their solutions rotate the plane of polarized light in opposite directions. By simple chemical methods it is not possible to decide which of the two configurations corresponds to the isomer rotating the plane of the light to the right (( )rotamer). Fisher proposed to assume as reference that ( )glyceraldehyde corresponds to the configuration 5a shown in the table on p. 487 and to establish the configuration of all other chiral molecules in a relative way with respect to this convention; thus (+)tartaric acid corresponds to 7a. Since this is an arbitrary assumption there was only a 50 per cent chance of it being correct. Fortunately the first determination of the absolute configuration of NaRb(+)tartrate[941by the method described below (using the anomalous scattering of the Zr K, radiation by Rb), proved that the assumption was correct. Since then the anomalous dispersion method has been used to determine the absolute configuration of a large number of molecules and it will be shown in Chapter 8 (p. 545) that the method is also applied in macromolecular crystallography. The two optical isomers differ in hand and may be related either by an inversion or by a reflection operation (inverse congruence). t In a normal Xray experiment, with no anomalous dispersion, because of Friedel's law, the two enantiomers are indistinguishable, as they give rise to the same diffraction pattern. When one or more anomalous scatterers are present, then both IFhI and IF,I should be measured and compared with the ~  are rather computed values. Since the Bijvoet["] differences 1 ~ ~ 1IF,I2 small, and anomalous dispersion is only large for heavier atoms near their absorption edges, it is essential to apply a proper absorption correction to the diffraction data. In order to illustrate how the absolute configuration may be determined it is instructive to consider the procedure originally used by Bijvoet, Peerderman, and van ~ o m r n e l ,which ~~~~ gives reliable results only when the anomalous dispersion effect is sufficiently large and for this reason it is no longer used. The ratios IF", /IF?,,\ and IF;J/JF?,1 are tabulated for a limited number of reflections with large Bijvoet differences; a onebyone comparison of the two ratios indicates that the wrong configuration has been chosen if, when the first ratio is greater than 1, the second is less than 1 and
+
+
i We should note that the term 'absolute configuration' is not always correct in describing crystal structures, as it does not apply to the case of noncentrosymmetric but achiral space groups (polar groups with reflection symmetry operations, such as Pna2,) o r to that of achiral molecules (without asymmetric centres) crystallizing in noncentrosymmetric space roups, such as q u a r t z The term 'absolute structure' has been recently proposed and discussed$'~"
Solution and refinement of crystal structures
vice versa. If this is the case, then the correct enantiomer is obtained by &anging the sign of all atomic coordinates. When the anomalous dispersion effect is small all the reflections should be used and efficient methods have been proposed by and in the latter an absolutestructure or chirality parameter x is refined in a leastsquares process (cf. p. 97) in which the structure factor is written as
+
IF(h, x)I2 = (1  x) IFhI2 x IF,I2
(5.89)
where x is close to zero when the model and the crystal are in the same chirality, and approaches 1 if they are inverted one with respect to another.
Appendices 5.A Structure factor probability distributions We will use the central limit theorem stating that, given N independent random variables x, ( j = 1, N), each with mean value (xi) and variance (ui2, N
their sum X =
C xj has a mean value equal to the sum of the individual
i=l
mean values and a variance equal to the sum of the variances, provided that N is sufficiently large, i.e.
x N
(x) =
x 4. N
(xi)
and
a2=
j=1
(5.A.1)
j=1
Whatever the distributions of the variables xj are (they may be all different), the sum X will have a normal probability distribution
For a centrosymmetric structure the structure factor may be written as
where the sum is extended to the independent atoms only so that Fh can be considered as the sum of N/2 independent random variables xj = 2fi cos 2nh q with mean value (xi) = 24 (cos 2nh q ) .
(5.A.4)
Assuming a random distribution of the atomic coordinates, all q values will be equally probable and (cos 2nh q ) = 0; hence The variance of xj is defined as a; = (x;)  (xj)2.
1
375
376
( Davide Viterbo Because of (5.A.5) the second term is zero and cy7 = 4f7(cos22xh
. I;.) = 2f7
(5.A.7)
given that, for a randomly variable angle 8, (cos28) = 4. Because of the central limit theorem, the mean value of Fh will be
and its variance
Finally the distribution function of F is given by Pi(F) = L exp ( F2/2X).
VzZ
F has the same probability of being positive or negative and the probability Pi(lF() that its modulus has a given value is given by Pi(l FI) = 2Pi(F); substitution of (5.A.10) gives eqn (5.4). The approximate character of (5.4) is clearly indicated by the observation N
that the maximum value of IF1 is C f, while Pi(lFI) has a Gaussian shape and goes to zero only at k ~ . 1 = 1 For a noncentrosymmetric structure Fh = A h + iBh and, in analogy with the derivation of (5.A.8) to (5.A.10), we have ( A ) = 0,
0;
= 4X
( B ) = 0,
02, = 4X
(5.A.11)
and 1 P(A) = exp (  A ~ / x ) ,
m
1 P(B) = exp
m
( B2/Z). (5.A.12)
+
The joint probability that A lies between A and A dA and at the same time B lies between B and B + d B is given by the product of the two distributions (5.A. 12) 1 P(A, B) dA d B = P(A)P(B) dA dB = exp (  ( A ~+ B2)/z) dA dB. Jcx (5. A. 13) Equation (5.A.13) represents the probability that the structure factor F lies within a region of the complex plane of area dS = dA dB. If the structure factor is expressed in polar coordinates (i.e. in modulus and phase), then dS = IF1 dlFJdg, and
The distribution of the amplitude IF1 alone is obtained by integrating (5.A.14) over g, and thus (5.5) is immediately derived. From (5.A.11) we can see that also for noncentrosymmetric structures Z = ((FI2).In deriving the value of (1~1') we did not consider the effects due to the presence of
Solution and refinement of crystal structures
I
"
other symmetry elements besides the inversion centre. Let us, for instance, consider the effects due to the presence of a mirror plane, by considering the space group Pm (m perpendicular to the b axis). In Fig. 5.A.1 we can see that on the projection along the b axis, all atoms related by the m plane are superimposed; the projection of the electron density on the ac plane will only contain half of the peaks, each with double weight. The Fourier coefficients FhOI relative to this projection will have a distribution corresponding to a structure of N / 2 atoms with scattering power 26 and then
The mean intensity of the h01 reflections will be twice that of the general reflections hkl. In order to take into account the symmetry element effects, (5.A.9) is generalized to
where E will be equal to 1 for the general reflections and greater than 1 for certain classes of reflections which are influenced by the presence of symmetry elements; thus in Pm E = 2 for the h01 reflections. The values of E and the relative reflection classes for the different symmetry elements are tabulated in the International Tables.[991 We note that the calculation of the ratio of the average observed intensity for specific classes of reflections over that of the general reflections, can be used as an indicator of the presence of some symmetry elements. For instance we can distinguish between the space groups Pm and P2 by ~ 1will~ be) close , to 2 for Pm and computing the ratio ( IFhOl1')/(I ~ ~ ~which close to 1 for P2.
5.B. Patterson vector methods We will consider here the socalled vector methods[1001which allow a systematic use of the information contained in the Patterson function also when no heavy atoms are present. The Patterson function can be considered as formed by the superposition of N images of the crystal structure displaced one with respect to the other by the amount required to bring to the origin each atom in the unit cell.
1
377
Fig. 5.A.1. Space group Pm: in the projection on the plane rn the t w o related molecules superpose.
378
1
Davide Viterbo
Each image represents the ends of all the vectors from the atom at the origin to all the others. Figure 5.B.l(b) illustrates how the Patterson map oj Fig. 5.4(c) can be interpreted in terms of five displaced images of the fiveatom structure of Fig. 5.4(a), repeated in Fig. 5.B.l(a). It can be easilj seen that the same map can also be interpreted in terms of five displaced images of the enantiomeric structure. It is in theory rather simple[1011to extract one image of the structure from the overlapping set, but, as we shall see, the proposed methods may be difficult to apply in practice; these are the socalled superposition methods. Let us first consider the vector superposition in which one Patterson mar is superposed on an other in such a way that the origin of the seconc coincides with a given vector of the first; the two maps are thus separated b) an interatomic vector. The set of coincident peaks will reveal one or more
Fig. 5.8.1. (a) Four unit cells of the fiveatom structure of Fig. 5.4(a); (b)four cells of the Patterson map in which the peaks indicated by r e f e r to the central origin and those indicated by 0to the other origins; the peaks referred t o the central origin are interpreted as the superposition of five images and the peak numbers refer to the atoms linked by the corresponding vector.
0
@\,
Solution and refinement of crystal structures
\
0
\
images of the structure. In particular, if the superposition is on a single peak, the structure plus its inverse are obtained for a noncentrosymmetric structure (Fig. 5.B.2); for a centrosymmetric structure only one image is obtained. If the superposition is on a multiple peak the number of images obtained is multiplied by the multiplicity of the peak (Fig. 5.B.4(c)). When more than one image is revealed, iteration of the superposition process on different peaks will eventually yield a single image. This is illustrated in Fig. 5.B.2, where superposition of the double image on a new peak reveals one image only. The basic principle of the method may be understood by considering that, if the structure contains atoms 1 , 2 , 3 , . . . , N in the unit cell, the Patterson map P will be the superposition of the images I(l), I(2), I(3), . . . ,I(N) obtained by placing atoms 1 , 2 , 3 , . . . , N in turn at the origin, i.e. After translation by a vector 12 the new function will be where the different images are obtained by placing atoms 1 , 2 , 3 , . . . ,N in turn, not at the origin, but at the end of the vector 12. In general I1(n) will not coincide with any image I(1), I(2), I(3), . . . , I(N) unless n = 1 or 2. In fact, because of the choice of the translation 12, 11(1)= 1(2) and Ir(2) = I(l) (I(n) is the enantiomer of I(n)) as illustrated in Fig. 5.B.3; the two images left in Fig. 5.B.2 after the first superposition are indeed I(l) and I(2). Unfortunately, this simple method is only applicable in the ideal case of a Patterson function corresponding to a point atom structure. In practice we have a continuous Patterson function in which the peaks of finite width overlap; for reasonably sized molecules with no heavy atoms, also in a sharpened map, only the peaks with high multiplicity appear, while single peaks are not resolved from the background. Thus superposition on any recognizable peak will give multiple images and several superpositions will be necessary to reveal a single image of the structure. A further problem arising with vector superpositions is that the obtained image is not referred to the true origin of the cell as it is apparent from Fig. 5.B.2; the correct
1
379
Fig. 5.8.2. Patterson superpositions: are the Patterson peaks as in Fig. 5.8.1; O are the coinciding peaks when the origin of the identical map of Fig. 5.8.1 is superposed on peak 12 of the present map, indicated by the first arrow (two enantiomorphic images of the molecule are shown); +are the coinciding peaks after a second superposition on peak 13, indicated by the second arrow (only one image is shown). The reader is advised t o reproduce on transparent sheets three copies of Fig. 5.8.1 and then perform the above superpositions.
380
1
Davide Viterbo
Fig. 5.8.3. (a) Image l(1) and its enantiomorph 1(1) with their atom 1 at the origin; (b) image l(2) and its enantiomorph 1(2) with their atom 2 at the origin; (c) image  I ' ( l ) with its atom 1 on (i) peak 12 (Fig. 5.B.l(b)), DIUS the imaae ~ 'with its atom 1 i n peak 21 (enantiomorph); (d) image l'(2) with its atom 2 on peak 12, plus the image with its atom on peak 21 (enantiomorph), The shadowed images 1U) in (a) and 1(2) in (b) are found in the superposition on peak 12 of Fig. 5.8.2; they are identical to 11(2) in (d) and l'(1) in (c) respectively.
10~ationof the structure with respect to the symmetry elements can be obtained by the described later. Despite these problems, superposition methods can still be applied in practice, especially when some structural information is available. This can be of three types: ( 1 ) the stereochemistry of one or more rigid molecular fragments is known, but not their orientation and position; (2) the orientation is also known, but not the position;
(3) both orientation and position are known. Information of the first type is often available from known bond lengths and angles or from the Cambridge Structural ~atabase,[''~] and we shall see how it can be exploited. In order to carry out any superposition process it is necessary to evaluate the degree of coincidence between the peaks of the superposing maps. This is done by means of the socalled imageseeking functions;[100]three such functions have been proposed: 1. The product function ( r )= P ( r ) X P ( r  u )
(5.B.1)
Solution and refinement of crystal structures
which takes very high values when coincidences occur, but is subject to considerable background noise and is very sensitive to small errors in the value of the vector u used for the superposition.
2. The sum function
E (r) = P(r) + P ( r  u)
(5.B.2)
which is less sensitive to the errors on u, but can often produce spurious peaks and in general a high background noise. 3. The minimum function M(r) = min {P(r), P(r  u)}
(5.B.3)
which is also sensitive to the errors on u but has the advantage of a low background noise. Let us first consider how the superposition method can be conveniently applied when the location of one or more atoms (both independent and related by symmetry) in the cell is known. In this case Patterson maps with their origin at the sites of the known atoms are superposed. An example of this atomic superposition is shown in Fig. 5.B.4(d) in which two maps, with their origin at the position of atoms 1 and 1' (related by an inversion centre) respectively, are superposed. Images 1(1) and I(1') coincide and reveal the structure properly placed with respect to the origin. Atomic superposition can be used when the crystal contains a heavy atom, the position of which has been determined by the method described on p. 328. Atomic superposition in this case is facilitated by the fact that the coinciding images are made up of vectors between heavy and light atoms which are well resolved over the background of vectors among light atoms. If the ratio (5.20) is very low, the straightforward application of the Fourier recycling procedure may be inefficient and atomic superposition may be a convenient alternative. We can now describe one of the procedures[10~106] proposed to solve the Patterson function when the stereochemistry of part of the molecule is known. It is convenient to divide the process of locating a fragment of known stereochemistry into two steps: determination of the orientation and determination of the position with respect to the symmetry elements. 1. Determination of the orientation. Starting from the known molecular fragment (atomic model) it is possible to build up the corresponding vector map (vector model). This model map is superposed on the Patterson function with its origin coinciding with that of the Patterson function and then rotated in all possible orientations. For each orientation the match between the ends of the m vectors of the model and the Patterson peaks is evaluated by means of functions similar to those considered above. Their form is now: (a) product function
where P(uj) are the values of the Patterson function at the ends of the vectors;
1
381
382
1
Davide Viterbo
Fig. 5.8.4. (a) Centrosymmetric threeatom structure; (b) corresponding Patterson map; (c) vector superposition on the double peak 23 45 gives the t w o images in full and broken lines, while superposition o n the single peak 25 gives the fullline image only, shifted from the correct origin at the inversion centre; (d) Atomic superposition: are the known positions of the related atoms 1 and 1'; x , C 3 are single and double peaks of the Patterson function with its origin on atom 1; 0, O are single and double peaks of the Patterson function with its origin on atom 1'; are the overlapping peaks showing the structure referred t o the correct origin.
+
9
Solution and refinement of crystal structures (b) sum function
(c) minimum function M = min {P(ul), P(uJ
. . . P(u,)).
This function is the most sensitive and is usually preferred, but, when the absolute minimum is assumed, small errors in the model may produce small values of M even for a correct orientation. To overcame this problem it is preferable to use the mean of the n smallest values ( M ) , , where n is usually equal to 1020 per cent of the total number of vectors. [lo'] The orientation of the model can be varied following the same Eulerian scheme (a detailed description is given by Stout and ~ e n s e n [ ' ~ ~ used ] ) in most diffractometers to define the position of the reciprocal lattice vectors in terms of the three angles 8, q, and x (cf. pp. 72 and 2746). The number of orientations to be examined can be quite large and the symmetry of the Patterson function and that of the vector model can reduce the range of the rotational search. The correct orientation will correspond to large values of the functions (5.B.4), (5.B.5), and (5.B .6).
2. Determination of the position with respect to the symmetry elements. Once a likely orientation has been defined, the location of the fragment can be determined by systematically translating it in all possible positions within the asymmetric part of the unit cell and then by generating, for each position, all the vectors between the atoms of the fragment and those of the symmetryrelated fragments. Each vector set obtained in this way is compared with the Patterson function and the fit is evaluated by means of one of the functions used in the orientational search. Normally the search of the position of a fragment with respect to the different symmetry elements is carried out separately for each symmetry element, considering that: (a) when the symmetry element is a plane the search is performed only along the direction orthogonal to the plane; (b) when the symmetry element is an axis the search is a twodimensional one on the plane orthogonal to the axis; (c) when the symmetry element is an inversion centre the search is three dimensional. Because of the errors in the model the orientation and position are determined by the above method only in an approximate way. They can be further improved by shifting the atoms of the model in such a way that a better fit of the set of interatomic vectors on the maxima in the Patterson function is obtained. The described procedure operates in the Patterson space, but other methods, usually operating in the reciprocal space, such as the rotation function,[1091 have been proposed[1101131 and successfully applied, especially
1
383
384
1
Davide Viterbo
in protein crystallography (cf. Chapter 8, p. 553). They are at the basis of the socalled molecular replacement methods.[l14]For each orientation or position of the model fragment, instead of fitting the vector model, a fit is searched for between the structure amplitudes calculated for the model and the observed ones. A procedure combining direct and reciprocal space searches has been recently described by Rius and ~iravitlles.["~] Recently, Patterson orientation search routines have been incorporated into direct methods programs. A highly automated routine has been built into the DIRDIF system.[701Another example is the PATSEE routine[116] incorporated into the SHELXS86 system.[lolIn both these cases the correct position of the oriented fragment is found by direct methods.
5.C Two examples of deriving phase information from positivity Let us first consider a centrosymmetric onedimensional structure for which the amplitudes IFhJand IF2hlare large. Their contributions to the electron density function Fh cos 2nhx
p(x) = (lla) h
Fig. 5.C.1. Onedimensional centrosymmetric structure with IFh/ and lFZhllarge: curve 1 shows the trend of IFh[cos Pnhx, curve 2 that of IFh/ cos Pnhx, and curve 3 that of F I, cos 2 ~ 2 h x the ; hatched regions A and B are those in which a high value of the electron density is indicated.
k hk
1
1
1
I
will be large and are illustrated in Fig. 5.C.1, where curve 1 shows the term + 141 cos 2nhx (Fh positive), curve 2 the term  I FhI cos 2nhx ( F , negative), and curve 3 the term +IF,,\ cos2n2hx ( 4 , positive). Fh would then contribute to the electron density in the region indicated by the letter A, if positive, and in the region B, if negative; in both cases F,, will contribute to both regions only with a positive sign. It follows that, with p(x) everywhere positive, if 1 Fhl and IF,, I are large, whatever the sign of I Fh1, the sign of IF,, 1 is more likely positive. This argument can be generalized to three dimensions. As a second example we shall consider the projection of a centrosymmetric structure for which the amplitudes I FhI, I FkI, and IFh,[ are large. In Fig. 5.C.2 the traces of the three families of planes h, k, and h  k are shown as full lines, while the dotted lines are located half way. If we associate to the full lines the maxima of the terms IFhlcos2nh r, lFklcos 2nk r, IFh,I cos 2n(h  k) r contributing to the electron density function p(r), then the dotted lines will represent the corresponding minima. If I Fhl, IFkl, I Fhklare large, the corresponding terms must add up to give a preponderant contribution to p ( r ) . This will happen when cos 2nh r = +1, if Fh is positive, and cos 2nh . r = 1 if it is negative; the same applies to the other two terms. It follows that the possible maxima of the electron density will be restricted to the regions indicated by A, B, C, and D in Fig. 5.C.2, where the above conditions are satisfied for all three terms at the same time. For each region the signs S(h), S(k), S(h  k) of the three structure factors are Region S(h) S(k) S(h  k) A B C D In all cases the product S(h)S(k)S(h  k) is always positive.
.

.

Fig. 5.C.2. Threedimensional centrosymmetric structure with IFhl, IFk!, and IFh*/ large: the full lines represent the maxima of lFhl cos 2nh. r, IFkIcos2nk.rand IFh_klcos2n(h k).r,the broken lines the corresponding minima; the hatched regions A, B, C, D are those in which high values of the electron density are more likely.
+ +
+ +
+ +
Solution and refinement of crystal structures
5.D Probability formulae for triplet invariants For a structure with N equal atoms in a P I unit cell, the normalized structure factor of index h can be written as the sum of N independent terms
x
1 Eh = 
mi4x exp (2nik  5 ) exp [2ni(h  k) . q]
1 exp (2nih q) = 
f i , = l
Under the assumption that all points in the unit cell have equal probability of housing an atom, the atomic position vectors q will form a set of independent random variables. Thus also the terms g,, which are functions of q, will be random variables. Then, because of the central limit theorem, Eh will have a normal distribution with mean
and variance
1
4=N ,=I 2 ( ( E ) ( 4 ) ' ) .
(5.D.3)
Supposing that the two exponential terms in the middle formula in (5 .D . l ) are independent, we have (5,) = (exp (2nik q)) (exp [2ni(h  k) q]).
(5.D.4)
Under the assumption that Ek has a fixed value (i.e. both its modulus and phase are known), we can write[ll']
With the same assumption for Eh,, (5.D.4) becomes
and substituting in (5 .D .2)
For the real and imaginary components of Eh = A h
+ iBh we have
Similarly to (5.D. I), we can derive
2 cos 2n(h  k + k) .q = mi=l[C,(k)C,(h  k)  S,(k)S,(h  k)] m,=1 1
Ah = 
1
385
386
1
Davide Viterbo
where C,(k) = cos 2nk q
x fl
Bh =
1
,=I
and S,(k) = sin 2nk 5. Similarly
x Pi.
1 [S,(k)Cj(h  k) + Cj(k)Sj(h  k)] = 
fl, = I
(5.D.10)
where the terms (Ah)2/Nand ( B h ) 2 /have ~ been neglected, as they are of order 1/N2 [cf. eqns (5.D.8)] and become very small for any reasonable N. The conditional probability density function P(Ah, Bhl Ek, EhPk)can be expressed as the product of the separate distributions of Ah and Bh. The probability that Ah lies in the interval between Ah and Ah dAh and at the same time Bh lies in the interval between Bh and Bh dBh, is therefore given by
+
P(Ah, Bh I Eh, Eh,)
1
= exp
n
+
{[(Ah  (Ah))2+ (Bh  (Bh))2]) (5.D.13)
which gives the probability that Eh lies within an area of surface dS = dAh dBh in the complex plane. When expressing Eh in polar coordinates (modulus and phase), then dS = IEhI dlEhl d q h and
As lEhl is known, we are interested in the conditional probability P ( q h I IEhI, Ek, Eh,), simply indicated as P(qh), which can be obtained by dividing (5.D.14) by its integral with respect to qh[118]
where
and Qhk
= Q)h  q
k
 Thk.
Since qk and qh, are known dQhk= d q h and the distribution of qh is
Solution and refinement of crystal structures
equivalent to that of Qhk. The value of the integral at the denominator of (5.D.15) isr5'] L = 2n&(Ghk),where &(x) is the modified Bessel function of zero order. We can finally writeLz4]
which is equal to the Cochran distribution (5.38). In a similar way it is possible to derive the probability formulae for centrosymmetric structures.[281By applying the centrallimit theorem to
we obtain
)'Im .
[
1 exp  21 (E,  ~
k ~ h  k
(5.D.19)
Indicating by P+ or P respectively, the probability that E, has a positive or negative sign, we have
and 1 exp x = tanh x 1+ exp (2x)  exp x + exp (x) = tanh (x) 1 P +
p+=
+
(x) + exp xexp+ exp (x)
and finally
P+ = 4 + f tanh
1 (* EhI EkEh,) .
(5. D.22)
The function (5.D.22) is illustrated in Fig. 5.14; P+> 4 if S(k)S(h  k) =
+ and P+< i (and P > 1) if S(k)S(h  k) =  . If in (5.D.19) we consider the two cases S(h) = S(k)S(h  k) (with probability P + ) and S(h) = S(k)S(h  k) (with probability P) we obtain eqn (5.46), where P + is always greater than i .
5.E Pseudotranslational symmetry We will say that a structure possesses pseudosymmetry when a nonnegligible part of the atoms approximately satisfy a higher symmetry than that of the whole structure. It can be noted that, in the special case in which these atoms exactly satisfy a higher symmetry, they will identify a supergroup (see Appendix l.E) of the space group to which the whole structure belongs. An important type of pseudosymmetry is the pseudotranslational symmetry occurring when a nonnegligible amount of the electron density, say p,(r) is repeated by a pseudotranslation (in the sense that it does not necessarily correspond to a crystallographic translation) u, i.e. p,(r) = p,(r u). ~ u e r g e r [ ' ~suggested ~ , ~ ' ~ ~that such structures should be treated as
+
1
387
388 ( Davide Viterbo
the sum of a substructure, p,(r) and the complement structure, p,(r) = P(F)  P P W . A twodimensional example of pseudotranslational symmetry is shown in Fig. 5.E.l(a), where the two heavy atoms 1 and 1' are related by a centring translation, u = a12 b/2, while the light atoms occupy general unrelated positions: the heavy atoms form the substructure and the light atoms the complement structure. If the structure only contained the heavy atoms, the unit cell would be centred and, according to p. 160, the reflections with h k = 2n + 1 would be systematically absent. For the structure of Fig. 5.E.l(a), only the light atoms will contribute to these reflections (superstructure reflections), which will therefore be systematically weaker than the reflections with h k = 2n (substructure reflections) to which both heavy and light atoms contribute. Because of the presence of pseudotranslational symmetry, imposing certain relations between subsets of atomic positions, the assumption that the atomic coordinates are independent random variables is violated. In the reciprocal space this is revealed by a nonuniform value of the averaged normalized intensity, (I E, 12), when the reflections are grouped in different ways. As we have seen, the reflections have to be divided into the set of substructure reflections with high mean intensity and the set of superstructure reflections with low mean intensity. In Fig. 5.E.l(b) the case in which the pseudotranslation is only approximately obeyed, is shown. Finally, in Fig. 5.E.l(c) another example of pseudotranslational symmetry is shown, in which two similar but not equal atoms are related by a vector u = a / 3 ; the substructure reflections will have h = 3n. Statistical methods for ideiltifying the type of pseudotranslational symmetry and the related sub and superstructure reflections have been recently proposed. [49,51,1201
+
+
+
5.F Magic integers I
(c)
Fig. 5.E.1. (a) Heavy atoms exactly related by a pseudotranslation vector u = a/2 + b/2; (b) heavy atoms approximately related by a ~seudotranslationvector u = a12 b12: ,  , .Id ~. slightly different heavy atoms related by a pseudotranslation vector u = e/3.
. +
Magic integers were first introduced by White and W o o l f s ~ n and [ ~ ~allow ~~ one to represent several phases in terms of only one variable, through of the type cpi = mix (5.F.1) where the mi are the magic integers. Let us consider the example given by ~ o o l f s o n . [Three l ~ ~ ~phases, expressed for convenience in cycles (0 6 cp < 1) instead of degrees, are considered; by using the three integers 3, 4, 5 in (5.F.1), we will have 91= 3x mod (11,
cp2
= 4x mod (I),
cp, = 5x mod (1), (5.F.2)
where mod(1) indicates that the phases are always taken within the interval 01 cycles (i.e. 0360"). We will now see that, whatever the value of the three phases, it is always possible to find a value of x (0 < x < 1) for which the three equations (5.F.2) are approximately satisfied. For instance, if cpl = 0.3, 147, = 0.2, cp, = 0.7, the value x = 0.766 (Fig. 5.F.1) will give: cp, = 2.298 mod (1) = 0.298 with an error of 0.002 cycles (lo), cp2 = 3.064 mod (1) = 0.064 with an error of 0.136 cycles (49"), cp, = 3.830mod (1) = 0.830 with an error of 0.130 cycles (47").
Solution and refinement of crystal structures
1
389
The reader may assign any three values to the phases and find by trial and o 766 error, with the help of Fig. 5.F.1, the value of x which best satisfies (5.F.2). p, So far we have used the sequence of three magic integers 3, 4, 5, but other longer or shorter sequences of different integers may be used. The accuracy with which phases can be represented by magic integers depends on the values of the integers and on the length of the sequence. ~ a i n [ ~ ~ ~ , ~ ~ ~ ~ described the theory of magic integers and gave some rules for selecting those sequences which minimize the mean square deviations (Aq2) of the represented phases. It turns out that the optimal sequences m,, m2, . . . , m, are those for which 2m1 = m, + 1 and the differences m,  m,l, mnPl2 mn2, . . . , m3  m2, m2  m1 form a geometric progression of integer numbers with common ratio r 3 1. For r = 2 the progression 1, 2, 4, 8, 16, . . . will give rise to the magic integers listed in the top part of Table 5.F.1. An integer progression with common ratio less than 2 is the socalled Fibonacci series 1, 1, 2, 3, 5, 8, 13, . . . , where each term is defined as the Fig. 5.F.1. Representaton o f t h e three phases In sum of the two preceding ones (F, = Fnl Fn2) and r tends to the golden eqns (5.F.2) as a function x. number 1.618. The corresponding magicinteger sequences are listed in the bottom part of Table 5.F.1, where the column headed (Aq), , , gives the root mean square error of the phases represented with the different magicinteger sequences. The optimal sequences also have the advantage that the errors are equally distributed among the represented phases. From , increases as n increases and, for a Table 5.F.1 it may be seen that (Aq), , given n it is lower when the integers are larger (r = 2). In several multisolution programs the general phases in the starting set are expressed in the form (5.F.1) and x is explored at regular intervals in the range 01 (if the enantiomorph has to be fixed, only the interval 00.5 should be explored). The value of the interval Ax is chosen in such a way that the mean variation of the phases from one value of x to the other is of the same order of magnitude of the corresponding (Aq),,, . Ax is therefore a function of n and of the m, values and it is smaller the larger are the integers. In order to keep the number of explored x values (each value corresponding to a trial starting set of phases) within reasonable limits, it is preferable to use magic integers based on Fibonacci series, at the cost of ,. A comparison between the use of quadrant slightly higher (Aq), , permutations and that of magicinteger permutations is shown in Table 5.F.2. This comparison may be better illustrated by considering the case n = 2, for which it is possible to draw in the plane ( q l , q2), the lines q , = 2x mod (1) and q2= 3x mod (1) (Fig. 5.F.2(a)). The choice of regular
+
Table 5.F.1. Magic integer sequences based on the geometric progression with common ratio r = 2 (top) and on the Fibonacci series (bottom); (Aq),,,,,, is the root mean square error of the phases represented by each sequence
n
Sequence
(AQJ)~.~.~.
390
1
Davide Viterbo Table 5.F.2. Comparison between quadrant permutations (fn/4, f 3n/4) and the permutations obtained with magic integers based on the Fibonacci series. Quadrant
Magic integers No. permutations
No. permutations
(AV)~."I.S.
intervals along x, i.e. along these lines, gives rise to a closepacked hexagonal disposition of points in the phase space. This corresponds to a more efficient way of sampling the phase space than that shown in Fig. 5.F.2(b), obtained by quadrant permutation. This is also true for n > 2 and it may be concluded that the use of magic integers allows a considerable reduction in the number of trial permutations, while the accuracy of phase representation is kept within acceptable limits.
5.G New multisolution techniques
Fig. 5.F.2. Illustration of two phases in the plane (q,, q2): (a) Lines q, = 2xand rp, = 3x: the triangles indicate the 12 regularly spaced points, with intervals of the order of (Aq),,,,,,, giving rise to the same number of phase permutations; (b)The triangles indicate the 16 points corresponding to quadrant permutation.
In the multisolution process described on p. 360 there are two main limitations: the restricted number of startingset phases and the 'chain' character of the phase expansion process by means of the tangent formula. The first factor will make the initial steps of phase expansion very critical, as the first phases will be determined by few relationships, while the second factor will amplify the first effect in the following steps. As we have seen, the use of magic integers allows an increase in the starting set of phases without a great decrease in accuracy. At the basis of all recent developments of the multisolution techniques lies the empirical observation that it is possible to solve structures, starting with a fairly large set of phases (more than 4050 phases), even though these might be very inaccurate. The different methods proposed differ in the way in which the large initial set of phases is set up. Those using magic integers are at the basis of the computer programs MAGIC['^^] and MAG EX.["^] A limited number of phases (normally 1015), called primary phases, are expressed as qpi= mix. If two of these phases enter in a triplet with sufficiently large G, it will be possible to express also the phase of the third reflection as a combination of magic integers. For instance, if
+
+
then q s =(ml m,)x n.The new phases obtained in this way are called secondary phases. The starting set of phases will therefore include the originfixing phases, the primary and secondary phases, and their number can be up to 6070. The selection of the x values to be tried is done by means of the qmap. This is set up using all triplets relating the phases in the starting set. With a
Solution and refinement of crystal structures
procedure similar to that used in deriving relation (5.64), a triplet may be written in terms of independent reflections as where b is a constant angle depending only on the symmetry operators of the space group. If in (5.G.2) we substitute the primary and secondary phases expressed in terms of magic integers, we will obtain where M is a combination of integers and B = b +other constant terms appearing in the definition of secondary phases. The condition that all NR relationships of type (5.G.3) among the startingset phases should be as close to zero as possible (or cos CD = +1) may be expressed as NR
G, cos (M,x
@(x)=
+ B,) = max.
(5.G.4)
r=l
@ ( x ) is a onedimensional Fourier series and can be easily calculated at regular intervals of x of the order of 1/(4Mm,,). The @mapis thus obtained and its maxima indicate the best values of x. Some 100 x values, corresponding to the highest values of @@), are selected to obtain the same number of sets of numerical values of the phases, which are then further refined and expanded. An extreme radicalization of the basic idea of enlarging the starting set by allowing larger phase errors, is the random approach to the phase problem.[1271 The starting phases are now assigned random values between 0 and 360" and then refined with different techniques. The first proposed random procedure is at the basis of the program. Some 100 best interrelated phases (selected by means of the convergence procedure) form the starting set and are assigned several sets of random values. Each set is then refined by a leastsquares procedure assuming as observational equations all triplet relations of type (5.G.2). The use of a leastsquares procedure in the case of cyclic variables defined modulo 2n, needs an important warning. To obtain the correct phase values it is necessary to know the values of the righthand terms of relations such as (5.G.2) not reduced modulo 2n; or, in another way, we must know n in the equation CD = 2nn (n positive, zero, or negative integer). It may be interesting to note that this is another way in which the 'phase problem' shows up: it is generally possible to solve an overdetermined system of some thousands linear equations in terms of some hundreds of unknowns, but in our case, the cyclic nature of the variables introduces the new unknowns n, the number of which is equal to the number of observational equations. We must have some prior estimate of the n values, and this may be obtained from the starting random values of the phases; the values obtained in this way will in general not be integer and will be approximated to the nearest integer. The leastsquares procedure may now be carried out and new values of the phases obtained; these in turn will yield new estimates of the ns and the process is repeated until convergence. The advantage of this refinement procedure, with respect to the tangent formula, is that all phases are refined at the same time; the cost is a longer computing time. Each phase set, after this refinement, is expanded by the tangent formula and
1
391
392
1
Davide Viterbo
tested by some figures of merit. Applications of this method have shown that it is possible to hit the correct solution starting with a limited number (around 100) of random phase sets; the probability of getting the correct solution decreases as the structural complexity increases. The success of this and other random methods implies that, if N (=loo) is the number of starting phases, then the Ndimensional space, in which the refinement is carried out, only shows a limited number of minima; it will be sufficient'to start from a limited number of random points in this space to converge to the minimum corresponding to the correct solution. A more straightforward procedure is applied in the RANT AN['^^] program in which the random starting sets of phases, including all reflections with large (El values, are directly refined by a carefully weighted tangent formula. The initial random phases are assigned a weight w = 0.25 and at each cycle only the phases determined with a sufficiently high ah value, so that wh =: min (0. 2ah, 1) > 0.25, are accepted. Also in this case a limited number of trials (50200, depending on the structural complexity) is capable of yielding the correct structure. A similar random start procedure, but with a different strategy, has been implemented within the SHELXS86['01 program. More recently two new random procedures have been incorporated into the computer programs X M Y [ ~and ~ ~SAY , ~TAN.['^'] ~ ~ ~ In the first the initial random phases are refined by parameter shift.[1331 By this method all parameters are supposed independent so that each of them can be varied systematically from uy  nAuj to u9 nAu, in 2n steps of Aui; the value which maximizes (or minimizes) a selected function of the parameters is taken as a better value for this parameter and is used in the subsequent calculations with the next parameters. The process is continued until selfconsistency. The advantage of the parametershift method is its ability to jump away from a local extremum. In the XMY procedure the function which is maximized is
+
where Xh
=
C k
and
IEhEkEhkl
COS
(9)h
+ 9)k + qhk) (5.G.6)
A large value of F is in agreement with the most probable value of the triplets. In SAYTAN random phases are refined by means of a modified tangent formula derived from Sayre's equation (5.24) expressed in terms of normalized structure factors. Its derivation is too long to be reported here and we will just mention that it also includes quartet invariants. All the described random procedures have proved very successful in solving rather complex crystal structures. Finally we mention an alternative random procedure[1341which has
Solution and refinement of crystal structures
1
393
recently been incorporated in the SIR program[671and is indicated with the name MESS. When phases are generated at random they are in general inconsistent with positivity and atomicity of the electron density, and only the refinement process will make them comply with these conditions; on the other hand, we have seen that these two conditions are at the basis of the probability formulae for triplets or other i.s. or s.s.. In the MESS approach, the starting phases are derived from triplets perturbed by random shifts
[email protected] obeying a von Mises distribution; these phases will then comply with positivity and atomicity. Also in this case the number of trials necessary to get the solution is comparatively small and the procedure proved successful in solving several complex structures.
5.H Procedures for completing a partial model
Weights for Fourier syntheses Given the positions of some atoms, what weights should be given to the coefficients in order to obtain the 'best' Fourier map revealing the remainder of the structure? This problem was first tackled by ~ i m [ ~ ' , ' ~ ] . With reference to Fig. 5.H.1, let where FN is the structure factor of the complete structure, Fp is the contribution of the P known atoms, and FQ is the contribution of the Q unknown atoms. Ideally we should compute a Fourier synthesis with FQas coefficients, i.e.
where a = qN 9,; but in the righthand side of (5.H.2) a is unknown and the best estimate of FQ is obtained by replacing exp (ia) by its expected value (exp (ia)) = (cos a )
+ i(sin a ) = (COSa ) ;
,
since a can equally have positive and negative values, then (sin a ) = 0 and (5.H. 2) becomes
indicating that the 'best' Fourier synthesis is obtained by weighting the IFNI factors by w = (cos a ) . In order to derive (cos a ) we must first know the probability distribution of c?.. For FQ= AQ iBQ the probability distribution (5.A.13) becomes
+
1 P(AQ, BQ) = exp
JGCQ
[  (A;
+ B2Q)lCQ]
(5.H.4)
where CQ = C, f: is a summation over the unknown atoms. From the triangle in Fig. 5 . ~1 .we have
A$
+ B ~ Q = IFQI2= IFNI2+
 2 lFNlIFPIcos a
(5. H.5)
Fig. 5.H.1. Vector representation i n the complex plane of the structure factor as a sum of t w o components.
394
1
Davide Viterbo
The only unknown term is a and (5.H.6) is essentially a probability distribution of a , i.e.
P ( a ) = (1/K) exp (X cos a ) ,
(5.H.7)
where X = 2 lFN( IFpIICQand K is a normalizing constant given by (see eqns (5.D.15) and (5.D.17)) K=
$
exp (X cos a ) da = 2nIo(X).
(5.H.8)
Finally
P(a) =
exp (X cos a)
2"Io(X)
.
Recalling eqn (5.68), we may now derive
w = (cos a ) =
dm= "(X)
Io(X) '
(5.H. 10)
and (5 .H.3) becomes
When this weight is used in Fourier recycling, then IFN(= (Fobs(and the employed coefficients are
Similarly ~ o o l f s o n [derived ' ~ ~ ~ that for centrosymmetric structures
FP+ (FQ)= IFobsl tanh (X12)Sp
(5.H.13)
where Sp is the sign of Fp.
Syntheses for completing a partial model We have seen that often only part of the structure (e.g. positions of heavy atoms) can be initially determined; this information can then be combined with the Patterson function to define the rest of the structure. For this purpose Ramachandran and Raman[136]proposed several types of Fourier syntheses[13721381 with different coefficients. Among them we will recall the a and the /3 syntheses, with coefficients a synthesis
IF~(~F~
/3 synthesis
1 ~ ~ 1 ~(F;1 ~complex ; conjugate of Fp)
where the terms have the same meaning as in (5.H.1)
Solution and refinement of crystal structures
Considering (5.H.1), the Patterson coefficients IFNI2become and those of the a synthesis
where 4 and F, contribute to the background and the P peaks, F, contributes to the background and the desired Q peaks, and 4 contributes mainly to the background. A similar development for the coefficients of the /3 synthesis yields to I F ~ ( ~=/ Fp F ~I FQ+ F$ exp 2iqp
+IFQ~~/F~
(5.H.16)
where the first two terms contribute, with equal weight, to reveal the known P atoms and the unknown Q atoms respectively, while the last two terms contribute mainly to the background. An advantage of the /3 over the a synthesis is that it gives the electron density map when Fp = FN. ~ a i n [ l compared ~~] the P synthesis with the synthesis computed with coefficients (5.H.12) (also called weighted y' synthesis). From (5.H.5) the expected value may be derived and, considering that
IF~12
= ((FP
+ F~)(F; + F;)
(5.H.18)
the coefficients (5.H.12) are obtained as
where the last two terms mainly contribute to the background, the first term contributes to the known part of the structure, and the second to the desired unknown part, but only with half weight. In order to give the P and the Q peaks the same weight, as in the case of the /3 synthesis, the coefficients of the y' synthesis should be altered to
+
(2 IFNl(cos a)  IFPI) exp (iq,) = Fp + FQ FT,exp (2iqp)
+ {JFQ12 (lFQ12))lFg. (5.H.20) The new synthesis is referred to as the 2F,  F, synthesis; it has been shown that, for noncentrosymmetric structures, it contains fewer background peaks than the /3 synthesis and is more effective in suppressing the peaks corresponding to wrong atoms in the initial model. Let us conclude this paragraph with a comparison, proposed by Tollin et between the a synthesis and the optical image synthesis by holography (see any optics textbook such as ~ e y e r  ~ r e n d t [ ' ~ lThe ]). principle of holography is illustrated in Fig. 5.H.2. The waves scattered by the object Q interfere with those from a coherent point source P and the fringe pattern is recorded on a photographic plate to form a hologram (H). The intensity pattern on the hologram will depend on the phase relationships between the interfering waves from P and Q. By illuminating the
( 395
396
(
Davide Viterbo laser
n
(a) RECORDING
'reference beam
mirror
image
/  
5 '
laser Fig. 5.H.2. Scheme of the formation of a hologram.
(b) IMAGE RECONSTRUCT ION
hologram with light identical to that from P, the image of the object Q may be reconstructed. If t,(x) and t Q ( x )are the functions describing the source P and the object Q, the corresponding scattered amplitudes will be their Fourier transforms TP(s) and TQ(s). The amplitude at a point s on the hologram will be
A ( s ) = Tp(s)+ TQ(s)exp (2nias)
(5.H.21)
where a is the separation between t,(x) and tQ(x). The intensity at s on H will then be
where the s dependence has been omitted. When the hologram is illuminated by a light from the source P, the resulting modulated function will be
+
IT, = T, 1 T , [ ~ T, IT,(^
+ T $ T ; exp (2xias) + 1 T,~~TQ exp ( h i a s ) . (5.H.23)
Its Fourier transform will be the combination of the transforms of the four different terms and will show the image of the object Q. Comparison with (5.H.15) shows that the four terms of the a synthesis coefficients are formally similar to those in (5.H.23). In the case of a partially known
Solution and refinement of crystal structures
structure we observe the interference effects between the known (source) and the unknown (object) parts of the structure. In 1950 ~ r a had~ already qualitatively indicated the analogy between the heavyatom technique and holography.
References 1. Patterson, A. L. (1944). Physics Review, 65, 195. 2. Wilson, A. J. C. (1950). Acta Crystallographica, 3, 397. 3. Lipson, H. and Cochran, W. (1953). The crystalline state. vol. III: The determination of crystal structures. G. Bell, London. 4. Wilson, A. J. C. (1949). Acta Crystallographica, 2, 318. 5. Wilson, A. J. C. (1942). Nature, 150, 151. 6. Viterbo, D., Gasco, A., Serafino, A. and Mortarini, V. (1975). Acta Crystallographica, B31, 2151. 7. Harker, D. (1936). Journal of Chemical Physics, 4, 381. 8. Calleri, M., Chiari, G . , Chiesi Villa, A., Gaetani Manfredotti, A., Guastini, C. and Viterbo, D. (1976). Acta Crystallographica, B32, 1032. 9. Gervasio, G., Rossetti, R. and Stanghellini, P. L. (1979). Journal of Chemical Research (S) 334, (M)3943. 10. Sheldrick, G. M. (1985). In Crystallographic computing 3 (ed. G. M. Sheldrick, C. Kriiger and R. Goddard), pp. 1849. Oxford University Press; Robinson, W. and Sheldrick, G. M. (1988). In Crystallographic Computing 4 (ed. N. W. Isaacs and R. M. Taylor), pp. 36677. Oxford University Press. 11. Luger, P. and Fuchs, J. (1986). Acta Crystallographica, A42, 380. 12. Lenstra, A. T. H . and Schoone, J. C. (1973). Acta Crystallographica, 429, 419. 13. PavelEik, F. (1989). Journal o f Applied Crystallography, 22, 181. 14. Argos, P. and Rossmann, M. G. (1976). Acta Crystallographica, B32, 2975. 15. Rossmann, M. G., Arnold, E. and Vriend, G. (1986). Acta Crystallographica, A42, 325. 16. Terwilliger, T. C., SungHou Kim and Eisenberg, D. (1987). Acta Crystallographica, A43, 1. 17. Harker, D. and Kasper, J. S. (1948). Acta Crystallographica, 1, 70. 18. Karle, J. and Hauptman, H . (1950). Acta Crystallographica, 3, 181. 19. Giacovazzo, C. (1980). Direct methods in crystallography. Academic, London. 20. Hauptman, H . and Karle, J. (1953). The solution of the phase problem. I. The centrosymmetric crystal, ACA Monograph, No. 3. Polycrystal Book Service, New York. 21. Sayre, D. (1952). Acta Crystallographica, 5, 60. 22. Hauptman, H . and Karle, J. (1956). Acta Crystallographica, 9, 45. 23. Cascarano, G. and Giacovazzo, C. (1983). Zeitschrift fur Kristallographie, 165, 169. 24. Cochran, W. (19%). Acta Crystallographica, 8, 473. 25. von Mises, R. (1918). Physikalisches Zeitschrift, 19, 490. 26. Karle, J. and Karle, I. L. (1966). Acta Crystallographica, 21, 849. 27. Karle, J. and Hauptman, H . (1956). Acta Crystallographica, 9, 635. 28. Cochran, W. and Woolfson, M. M. (1955). Acta Crystallographica, 8, 1. 29. Schenk, H. (1973). Acta Crystallographica, A29, 77. 30. Schenk, H . (1973). Acta Crystallographica, A29, 480. 31. Simerska, M. (1965). Czechoslovakian Journal of Physics, 6, 1. 32. Hauptman, H. (1975). Acta Crystallographica, A31, 671. 33. Hauptman, H. (1975). Acta Crystallographica, A31, 680. 34. Hauptman, H. (1976). Acta Crystallographica, A32, 934.
~
[
~
~
~
~
1
397
398
1
Davide Viterbo Giacovazzo, C. (1977). Acta Crystallographica, A33, 933. Giacovazzo, C. (1980). Acta Crystallographica, A36, 362. Giacovazzo, C. (1974). Acta Crystallographica, A30, 626, 631. Giacovazzo, C. (1978). Acta Crystallographica, A34, 562. Burla, M. C., Nunzi, A., Polidori, G., Busetta, B. and Giacovazzo, C. (1980). Acta Crystallographica, A36, 573. 40. Burla, M. C., Nunzi, A., Giacovazzo, C. and Polidori, G. (1981). Acta Crystallographica, A37, 677. 41. Cascarano, G., Giacovazzo, C., Calabrese, G . , Burla, M. C., Nunzi, A , , Polidori, G. and Viterbo, D. (1984). Zeitschrift fur Kristallographie, 167, 34. 42. Giacovazzo, C., Spagna, R., VickoviC, I. and Viterbo, D. (1979). Acta Crystallographica, A35, 401. 43. Cascarano, G., Giacovazzo, C., Polidori, G . , Spagna, R., and Viterbo, D. (1982). Acta Crystallographica, A38, 663. 44. Burla, M. C., Giacovazzo, C., and Polidori, G. (1989). Acta Crystallographica, A45, 99. 45. Cascarano, G., Giacovazzo, C., Camalli, M., Spagna, R., Burla, M. C., Nunzi, A., and Polidori, G. (1984). Acta Crystallographica, A40, 278. 46. Giacovazzo, C. (1976). Acta Crystallographica, A32, 958. 47. Busetta, B., Giacovazzo, C., Burla, M. C., Nunzi, A., Polidori, G., and Viterbo, D. (1980). Acta Crystallographica, A36, 68. 48. Ladd, M. F. C. and Palmer, R. A. (ed.) (1980). Theory and practice of direct methods in crystallography. Plenum, New York. 49. Cascarano, G., Giacovazzo, C., and LuiC, M. (1985). Acta Crystallographica, A41, 544. 50. Cascarano, G., Giacovazzo, C., and LuiC, M. (1987). Acta Crystallographica, A43, 14. 51. Cascarano, G., Giacovazzo, C., and LuiC, M. (1988). Acta Crystallographica, A 4 4 176. 52. Cascarano, G., Giacovazzo, C., and LuiC, M. (1988). Acta Crystallographica, A44, 183. 53. Camalli, M., Giacovazzo, C., and Spagna, R. (1985). Acta Crystallographica, A41, 605. 54. Burla, M. C., Cascarano, G., Fares, E., Giacovazzo, C., Polidori, G., and Spagna, R. (1989). Acta Crystallographica, A45, 781. 55. Zachariasen, W. H. (1952). Acta Crystallographica, 5, 68. 56. Germain, G. and Woolfson, M. M. (1968). Acta Crystallographica, B24, 91. 57. Germain, G., Main, P., and Woolfson, M. M. (1970). Acta Crystallographica, B26, 274. 58. Abramowitz, M. and Stegun, I. A. (1964). Handbook of mathematical functions. National Bureau of Standards, Washington, D.C. 59. Burla, M. C., Cascarano, G., Giacovazzo, C., Nunzi, A , , and Polidori, G. (1987). Acta Crystallographica, A43, 370. 60. Cascarano, G., Giacovazzo, C., and Viterbo, D. (1987). Acta Crystallographica, A43, 22. 61. Cascarano, G., Giacovazzo, C., Burla, M. C., Nunzi, A., and Polidori, G. (1984). Acta Crystallographica, A40, 389. 62. Cascarano, G. (1990). Doctorate thesis. University of Bari; Cascarano, G., Giacovazzo, C., Camalli, M., Spagna, R., and Watkin J . D. (1991). Acta Crystallographica, A47, 373. (And references therein.) Altomare, A., Cascarano, G., Giacovazzo, C., Guagliardi, A., Burla, M. C., Polidori, G., and Camalli, M. (1994). Journal of Applied Crystallography, 27, (in press). 63. Schenk, H. and Kiers, C. T. (1985). In Crystallographic computing 3 (ed. G. M. Sheldrick, C. Kriiger, and R. Goddard), pp. 2005. Oxford University Press.
35. 36. 37. 38. 39.
Solution and refinement of crystal structures
64. Peschar, R. and Schenk, H. (1987). Acta Crystallographica, A43, 751. 65. Karle, I. L., Karle, J., Mastropaolo, D., Camerman, A., and Camerman, N. (1983). Acta Crystallographica, B39, 625. 66. Main, P., Fiske, S. J., Hull, S. E., Lessinger, L., Germain, G., Declercq, J. P., and Woolfson, M. M. (1980). MULTAN80: A system of computer programs for the automatic solution of crystal structures from xray diffraction data. Universities of York and Louvain. 67. Burla, M. C., Camalli, M., Cascarano, G . , Giacovazzo, C., Polidori, G., Spagna, R., and Viterbo, D. (1989). Journal of Applied Crystallography, 22, 389. 68. Cerrini, S., Lamba, D., Burla, M. C., Polidori, G., and Nunzi, A. (1988). Acta Crystallographica, C44, 489. 69. Karle, J. (1968). Acta Crystallographica, B24, 182. 70. Beurskens, P. T., Bosman, W. P., Doesburg, H. M., Gould, R. O., Van den Hark, Th. E. M., Prick, P. A. J., Noordik, J. H., Beurskens, G., Parthasarathi, V., Bruins Slott, H. J., and Haltiwanger, R. C. (1985). Program system DZRDZF, Technical Report, Crystallography Laboratory, University of Nijmegen. 71. Sim, G. A. (1959). Acta Crystallographica, 12, 813. 72. Sim, G. A. (1960). Acta Crystallographica, 13, 511. 73. Stewart, J. M. and Hall, S. R. X T A L user's manual, Technical Report TR1364.2. Computer Science Center, University of Maryland; Skelton, B., Hall, S. R., and Stewart, J. M. (1988). In Crystallographic computing 4, (ed. N . W. Isaacs and M. R. Taylor), pp. 32553. Oxford University Press. 74. Gabe, E. J., Le Page, Y., Charland, J. P., Lee, F. L., and White, P. S. (1989). Journal of Applied Crystallography, 22, 384. 75. Betteridge, P. V., Prout, C. K., and Watkin, D. J. (1984). CRYSTALS. University of Oxford; Watkin, D. J. (1988). In Crystallographic computing 4, (ed. N . W. Isaacs and M. R. Taylor), pp. 35465. Oxford University Press. 76. Viterbo, D., Calleri, M., Calvino, R., and Fruttero, R. (1984). Acta Crystallographica, C40, 1728. 77. Hughes, E. W. (1941). Journal of the American Chemical Society, 63, 1737. 78. Cruickshank, D. W. J. (1970). In Crystallographic computing (ed. F. R. Ahmed), pp. 18797. Munksgaard, Copenhagen. 79. Hirshfeld, F. L. and Rabinovich, D. (1973). Acta Crystallographica, A29, 510. 80. French, S. and Wilson, K. (1978). Acta Crystallographica, A34, 517. 81. Schwarzenbach, D. (1989). Acta Crystallographica, A45, 63. 82. Hamilton, W. C. (1964). Statistics in physical science, pp. 157162. Ronald, New York; (1965). Acta Crystallographica, 18, 502. 83. Bijvoet, J. M. (1949). Proceedings of the Koninklijke Nederlandse Akademie van Wetenschap, B52, 313. 84. Rogers, D. (1981). Acta Crystallographica, A37, 734. 85. Marsh, R. E. and Herbstein, F. H. (1983). Acta Crystallographica, B39, 280. 86. Marsh, R. E. and Herbstein, F. H. (1988). Acta Crystallographica, B44, 77. 87. Santoro, A., Mighell, A. D., and Rodgers, J. R. (1980). Acta Crystallographica, A36, 796. 88. Le Page, Y. (1982). Journal of Applied Crystallography, 15, 255. 89. Mugnoli, A. (1985). Journal of Applied Crystallography, 18, 183. 90. Spek, A. L. (1988). Journal of Applied Crystallography, 21, 578. 91. Jones, P. G. (1984). Chemical Society Reviews, 13, 157. 92. Braga, D., Gradella, C. and Grepioni, F. (1989). Journal of the Chemical Society, Dalton Transactions, 1721. 93. Aime, S., Botta, M., Gobetto, R., and Orlandi, A. (1990). Magnetic Resonance in Chemistry, 28, 552. 94. Bijvoet, J. M., Peerdeman, A. F., and van Bommel, A. J. (1951). Nature, 168, 271.
1
399
400
( Davide Viterbo Jones, P. G. (1984). Acta Crystallographica, A40, 660. Glazer, A. M. and Stadnicka, K. (1989). Acta Crystallographica, A45, 234. Flack, H. D. (1983). Acta Crystallographica, A39, 876. Bernardinelli, G. and Flack, H . D. (1985). Acta Crystallographica, A41, 500; (1987). Acta Crystallographica, A43, 75. 99. (1959). International tables for xray crystallography, Vol. 11, pp. 3557. Kynoch, Birmingham. 100. Buerger, M. J. (1959). Vector space and its application in crystal structure investigation. Wiley, New York. 101. Wrinch, D . M. (1939). Philosophical Magazine, 27, 98. 102. Allen, F. H., Bellard, S. A., Brice, M. D., Cartwright, B. A , , Doubleday, A . , Higgs, H . , Hummelink, T . , HummelinkPeters, B. G., Kennard, O., Motherwell, W. D. s . , Rodgers, J. R . , and Watson, D. G . (1979). Acta Crystallographica, B35, 2331. 103. Nordman, C. E. and Nakatsu, K. (1963). Journal of the American Chemical Society, 85, 353. 104. Nordman, C. E. and Kumra, S. K. (1965). Journal of the American Chemical Society, 87, 2059. 105. Nordman, C. E. (1985). In Crystallographic computing 3 (ed. G. M. Sheldrick, C. Kriiger, and R. Goddard), pp. 2329. Oxford University Press. 106. Nordman, C. E. and Hsu, L. Y. R. (1982). In Computational crystallography (ed. D. Sayre), pp. 1419. Oxford University Press. 107. High, D. H . and Krout, J. (1966). Acta Crystallographica, 21, 88. 108. Stout, G. H. and Jensen, L. H . (1989). Xray structure determination, pp. 3125. Wiley, New York. 109. Rossmann, M. G. and Blow, D. M. (1962). Acta Crystallographica, 15, 24. 110. Tollin, P. (1966). Acta Crystallographica, 21, 613. 111. Tollin, P. (1976). In Crystallographic computing techniques (ed. F. R. Ahmed), pp. 21221. Munksgaard, Copenhagen. 112. Wilson, C. C. and Tollin, P. (1986). Journal of Applied Crystallography, 19, 411. 113. Wilson, C. C. (1989). Acta Crystallographica, A45, 833. 114. Rossmann, M. G. (ed.) (1972). The molecular replacement method. Gordon and Breach, New York. 115. Rius, J. and Miravitlles, C . (1987). Journal of Applied Crystallography, 20, 261. 116. Egert, E. and Sheldrick, G. M. (1985). Acta Crystallographica, A41, 262. 117. Woolfson, M. M. (1954). Acta Crystallographica, 7, 61. 118. Hamilton, W. C. (1964). Statistics in physical science, pp. 1718. Ronald, New York. 119. Buerger, M. J. (1956), Proceedings of the National Academy of Sciences of the U S A , 42, 776. 120. Fan HaiFu, Yao JiaXing, and Qian JinZi, (1988). Acta Crystallographica, A44, 688. 121. White, P. S. and Woolfson, M. M. (1975). Acta Crystallographica, A31, 53. 122. Woolfson, M. M. (1976). In Crystallographic computing techniques (ed. F . R. Ahmed), pp. 10614. Munksgaard, Copenhagen. 123. Main, P. (1977). Acta Crystallographica, A33, 750. 124. Main, P. (1978). Acta Crystallographica, A34, 31. 125. Declercq, J. P., Germain, G . , and Woolfson, M. M. (1975). Acta Crystallographica, A31, 367. 126. Hull, S. E., Viterbo, D . , Woolfson, M. M., and Zhang ShaoHui, (1981). Acta Crystallographica, A37, 566. 127. Baggio, R., Woolfson, M. M., Declercq, J. P., and Germain, G. (1978). Acta Crystallographica, A34, 883. 95. 96. 97. 98.
Solution and refinement of crystal structures
128. Declercq, J. P., Germain, G . , and Woolfson, M. M. (1979). Acta Crystallographic~,A35, 622. 129. Yao JiaXing, (1981). Acta Crystallographica, A37, 642. 130. Debaerdemaeker, T. and Woolfson, M. M. (1983). Acta Crystallographica, A39, 193. 131. Debaerdemaeker, T. and Woolfson, M. M. (1989). Acta Crystallographica, A45, 349. 132. Debaerdemaeker, T., Tate, C., and Woolfson, M. M. (1985). Acta Crystallographica, A41, 286. 133. Bhuiya, A. K. and Stanley, E. (1963). Acta Crystallographica, 16, 981. 134. Burla, M. C., Giacovazzo, C., and Polidori, G. (1987). Acta Crystallographica, A43, 797. 135. Woolfson, M. M. (1956). Acta Crystallographica, 9, 804. 136. Ramachandran, G. N. and Raman, S. (1959). Acta Crystallographica, 12, 957. 137. Srinivasan, R. (1961). Acta Crystallographica, 14, 607. 138. Ramachandran, G. N. and Srinivasan, R. (1970). Fourier methods in crystallography. WileyInterscience, London. 139. Main, P. (1979). Acta Crystallographica, A35, 779. 140. Tollin, P., Main, P., Rossmann, M. G., Stroke, G. W. and Restrick, R. C. (1966). Nature, 209, 603. 141. MeyerArendt, J. R. (1972). Introduction to classical and modern optics, pp. 41327, PrenticeHall, Englewood Cliffs, N.J. 142. Bragg, W. L. (1950). Nature, 166, 399.
1
401
Ionic crystals FERNANDO SCORDARI
Introduction This chapter deals with a class of natural and synthetic compounds that, at least to a first approximation, can be treated as being composed of oppositely charged spheres. We start by illustrating some important chemical and physical concepts that are later on applied to the organization of ionic crystals. For instance, we shall see how it is possible to rationalize some atomic structures in terms of the energetics of crystal formation. To this end, the ionic model, attractive for its simplicity, will be used even if departure from the predictions are common particularly when bonds have quite prevalent covalent character. The closepacking model of spheres is examined closely and used as a helpful tool to describe many structures. Finally we see how the concepts and principles illustrated previously are very useful for the systemization of several ionic structures with different degrees of complexity.
The structure of the atom Atoms with a single electron We know from quantum that the motion of the electro~(e) in a hydrogen atom can be described by means of the wave function Y(x, y, z), or orbital, and that IY(x, y, z)I2 dv expresses the probabjlity of finding the electron in a given element of volume, dv. The electron can assume different states of energy, each distinguished by four quantum numbers n, 1, m, s: (1) n, the principal quantum number, is related to the energy of thg electron, and can have any positive integral value from 1 to w; (2) 1, the azimuthal quantum number, expresses the angular momentum h/2n) (where h is Plank's constant) of the path ~f module (= the electron and determines the form of its orbital: orbitals are indicated by the letters s, p, d, f, g . . . . and correspond respectively to 1 = 0 , 1, 2, 3, 4 . . . n  1 ;
v m
(3) m, the magnetic quantum number, (1 s m S +1) represents the angular momentum component in the direction of the magnetic field and characterizes the orientation of the orbital;
(4) s, (s = fi), the spin quantum number, determines the way in which the electron spins.
404 ( Fernando Scordari
Using the spherical coordinates r, 6 , q (see Fig. 6.1) Y(x, y, z ) can be resolved into the products of three functions with separate variables: Y(r, 6, q ) = R n , l ( r ) e 1 , ~ ( 6 ) @ r n ( ~ ) .
\
X Fig. 6.1. Relationship between the orthogonal coordinates x y, zand the spherical coordinates r, 8,
v.
(6.1)
While R;,,(r) gives the probability of finding the electron at a certain distance from the nucleus, the form and the orientation of its orbital are determined by 8 and @. The functions R, 8 and @ take different algebraic forms according to the quantum numbers with which they are associated. The probability of finding the electron in a spherical shell of volume 4nr2 dr, at a distance of r from the nucleus, is 4nr2R;,,(r) dr. The function Dnal(r)= 4 ? ~ r ~ R ; , ~ is ( r )known as the radial probability function. It is represented in Fig. 6.2 for orbitals Is, 2s, 2p, 3s, 3p, and 3d. The presence of secondary maxima, occurring before the main maximum, produces some important effects. For example when the electron is located in the 3s orbital it is more penetrating than that when it is in the 3p, (as shown in Fig. 6.2) whereby we can deduce that the ionization energy required by the 3s electron is greater than that required by the 3p electron. Let us examine now the angular part of Y(r, 6 , q ) . The spatial shapes of the angular probability functions are illustrated in Fig. 6.3. These configurations allow us to estimate the magnitude of the v vector that is proportional to the probability (summed over all distances) that the electron will be found in that direction.
Atoms with more than one electron The basic configuration of the electrons of an atom can easily be deduced by means of the aufbau principle, or gradual building up of atoms. This exploits the Pauli principle and a scale of the relative energy of the orbitals. The Pauli principle can be synthesized as follows: in an atom no two electrons exist which have all four quantum numbers, n, 1, m, and s, the same. Therefore two electrons belonging to the same orbital, as defined by the first three quantum numbers, must spin in opposite ways.
Fig. 6.2. Radial probability functions for orbitals 1s: 2% 2p. 3% 3p, and 3d for the hydrogen atom.
&&% r
(4)
Ionic crystals
dXby2
I
d ~2
d
x
~
~
X
Z
dyz
(d
1
405
Fig. 6.3. Angular probability functions for: (a) s; (b) P, P,, P,; and (c) dx2,,2, dr2, dVr dxrl dyz orbitals.
The energy of the orbitals for various neutral atoms increases in the following order:
This experimental scale, though not always reliable (see Fig. 6.4),
Fig. 6.4. Relative energy of various orbitals versus the atomic number Z.
406
1
Fernando Scordari
nevertheless constitutes a good guide for the building up of atomic structures and especially for the location of valence electrons. For example the outermost electrons of Rb and Sr occupy the 5s orbital rather than the 4d, exactly as predicted by the energy scale. The relative energy of the orbitals versus Z is shown in Fig. 6.4. Following the aufbau principle the orbitals are filled gradually as shown below: Chemical element
Orbital
n
I
m s
Electrons
On the same principle, the entire periodic table can be obtained in the same way, as illustrated in Table 6.1. Elements whose valence electrons are in the s orbitals belong to groups IA or IIA: alkaline metals have only one valence electron in their s orbital, while alkalineearth metals have two. The elements in groups from IB to VIIIB, known as transition metals, have their external electrons in orbitals (n  l)d which immediately precede the last orbital ns. Those elements whose valence electrons are in the p orbitals belong to groups I11 to VIIIA. Such elements are known as posttransition metals and nonmetals, and are separated roughly in the Table 6.1 by a broken line. Helium (in the hatched square) can be placed either in group IIA, taking into account its electron configuration, or in group VIIIA, taking into account its chemical behaviour similar to that of the other noble gases. Finally there are the lanthanides and actinides which are characterized by a gradual filling of the f orbitals preceding by two places (n  2) the last orbital s(n).
Interactions between ions Notes on chemical bonds A knowledge of the structure of an atom allows reasonable predictions to be made about interactions between adjacent atoms. At this point it will be useful to recall certain general concepts of chemistry. The influence which the nuclear charge has on the external electrons varies according to which orbitals they occupy and to what degree they are shielded by the electrons closer to the nucleus (see p. 419). Such variations in electrons attraction can be evaluated by means of: ionization energy (IE); electronic affinity (EA); electronegativity (EN). I E is the energy needed to remove an electron from the orbital of an atom to an infinite distance. The closer the electron is to the nucleus the greater the energy required. First, second energy of ionization, and so on, indicate the increasing quantities of energy necessary to free electrons 1, 2, etc. In accordance with recent thermodynamic conventions endothermic
Table 1. T h e p e r i o d i c t a b l e of e l e m e n t s a n d c o n f i g u r a t i o n s of i n t e r n a l e l e c t r o n s ( f i r s t c o l u m n ) a n d v a l e n c e e l e c t r o n s ( f i r s t r o w ) . T h e o x i d a t i o n s t a t e s in c o m p o u n d s a r e g i v e n in t h e u p p e r p a r t of t h e cases, with t h e m o s t i m p o r t a n t u n d e r l i n e d nner !lectronc
0
2 10
18 16 i4
16
t
"Light metals. bTran~itionmetals. "The stair step running from boron to astatine, divides nonmetals from posttransition metals. Nobel gases.
408
1
Fernando Scordari Table 6.2. Partial series of the electronegativity of elements i n accordance with Sander~on[~' Element EN
Element EN
Element
EN
Element
EN
H He Li Be B C N
V2 Cr2+ Mn2+ Fe Co2+ Ni2+ Cu Zn2+ Ga3+ Ge4+ As3+ Se Br Kr Rb Sr Y zr2+ Nb Mo Tc Ru
Rh Pb Ag Cd In Sn2+ Sn4+ Sb Te I Xe Cs Ba La Ce Pr Nd Prn Sm Eu Gd Tb
1.47 1.57 1.72 1.73 1.88 1.58 2.02 2.19 2.34 2.50 2.63 0.69 0.93 0.92 0.92 0.92 0.93 0.94 0.94 0.94 0.94 0.94
DY Ho Er Trn Yb Lu Hf Ta W Re 0s Ir Pt Au Hg TI+
0.94 0.96 0.96 0.96 0.96 0.96 0.98 1.04 1.13 1.19 1.26 1.33 1.36 1.72 1.92 1.36 1.96 1.61 2.01
0 F Ne Na Mg Al Si P S CI Ar K Ca Sc ~i'+
2.31

0.86 1.61 1.88 2.47 2.93 3.46 3.92 4.38 0.85 1.42 1.54 1.74 2.16 2.66 3.28 3.92 0.74 1.06 1.09 1.13
+
1.24 1.35 1.44 1.47 1.70 1.75 1.14 1.86 2.10 2.31 2.53 2.76 2.96 3.17 0.70 0.96 0.98 1.OO 1.12 1.24 1.33 1.40
TI^+ Pb2+ Pb4+
energy (absorbed by the atom) is marked positive, while exothermic energy (given off by the atom) is marked negative. E A is the energy given off when an electron is added to the valence shell of an atom. The acquisition of a first electron by nonmetallic atoms involves the giving off of energy. However, the acquisition of a further electron is an endothermic process, as the addition of the first electron has brought the atom to a sort of 'saturation' level. EN expresses the property of an atom to attract electrons to itself when it combines. It is difficult to evaluate this property, since, unlike IE and EA, it depends also on the nature and number of the atoms with which it bonds. Since the vast majority of elements can form large numbers of combinations, the E N cannot be an invariable value for each element. The various methods u ~ e d [ ~to, ~define ] E N have led to various electronegativity series. The semiempirical series adopted here is that of ~ a n d e r s o n , [illustrated ~] in Table 6.2. Two atoms or ions are influenced by two forces: attraction (Fa) and repulsion (F,). The algebraic sum of their relative energies, E, and E,, is indicated by E. The minimum of this function, E,, in correspondence to R = R e , represents the energy gain of a couple of ions in 'contact', as opposed to the energy they would possess at an infinite distance. R, is the bond length in correspondence with which the forces of attraction and repulsion are balanced. The bonds can be divided orientationally into two categories: (1) strong bonds with energy E, > 90 kcal moll; (2) weak bonds with energy E, < 35 kcal mol'. Type (1) bonds are due to direct interaction between the outermost
lonic crystals
orbital electrons. If the bond electrons tend to be concentrated in the region between the atoms, then the bond is termed covalent (e.g. an H, molecule). If, instead, the outermost electrons tend to be transferred from one atom to the other, giving origin to high concentrations and impoverishments in comparison with the original electronic densities, then the bond is referred to as an ionic bond (e.g. an NaCl crystal). Finally, if the bond electrons belong to the whole crystal, then the bond is known as metallic (e.g. crystalline Na). Most compounds are characterized by bonds of an intermediate nature which are referred to as heteropolar covalent bonds. The degree of ionicity of a bond (ID) can be evaluated if the difference in electronegativity between two atoms involves (X and Y) is known, (AENxy = ENx  ENy). If the bond between them is simple, then, in accordance with ~ a u l i n ~ ID , [ ~can ] be estimated by means of the following equation: ID = 1  exp [O.~~(AEN,,)~].
(6.2) Using Table 6.2 for NaC1, KC1, and LiF the following values for ID can be obtained: 0.77, 0.80, 0.90. Type (2) bonds are due to weaker, essentially electrostatic, forces like van der Waals forces or hydrogen bond.['] Van der Waals forces are present in all compounds: together with hydrogen bonds they play a primary role in molecular crystal structure (see Chapter 7). Hydrogen bonds are fundamental for the cohesion of many compounds like proteins, molecular crystals, hydrated salts, etc.
lonic crystals The periodic table (Table 6.1) and Table 6.2 show that the E N of elements varies with a certain regularity. In fact it increases much more from left to right (along the periods) than from bottom to top (along the groups). The further apart two elements are in a given period, the greater is the difference in electronegativity between them, and the more markedly ionic are the bonds of the compounds they form together. The various types of bonds which form between the atoms play an important role in determining geometrically the structural pattern and the physicochemical properties which characterize a crystalline substance. In molecular crystals, more or less complex, finite, atomic aggregates can be found, i.e. molecules, within which considerably stronger covalent bonds are formed than the van der Waals bonds which are formed between the molecules (see Chapter 7). In nonmolecular crystals the protagonists are atoms or ions (simple or complex) which are held together by more or less localized bonds, and in limited cases of maximum polarization, by Coulomb interactions. This chapter will deal with nonmolecular crystals, in particular ionic crystals. The following questions will be considered: 1. What conditions must be satisfied in order that a combination of ions may be considered stable? 2. What are the configurations that such combinations give rise to? The energy associated with a given ions' disposition will be analysed
1
409
410
1
Fernando Scordari briefly in order to answer the first question, while the atomic building of some typical structures will be analysed in order to answer the second. Gibb's free energy, G = E  TS + PV, indicates the stability of a crystalline structure. The term P V (pressure x volume) can be omitted if the pressure is not high, thus free energy takes the form: where F is Helmholtz's free energy, E is the internal energy of the crystal, T is the absolute temperature, and S is the entropy. E, known also as cohesion energy, is the sum of two terms: E = UL + Ev.
(6.4)
UL is the static term, also known as lattice energy, (see p. 411), and expresses the potential energy of the immobile ions in the equilibrium positions. Ev is the dynamic term which expresses the vibration energy of the mobile ions oscillating around the equilibrium positions. If the temperature is not very high and the structure is well ordered, i.e. if for Ev and TS P, then the fourth electron will go to fill a t2, orbital, forming a lowspin complex (two electrons which spin in opposite direction plus two electrons which spin in the same way give a compound which is not very paramagnetic). If the A, < P, then the fourth electron will go to fill an e, orbital, forming a highspin complex (four electrons which spin in the same way give a very paramagnetic compound). Table 6.4 shows the CFSE relative to high and lowspin configurations, for octahedral sites. We will now examine the case of a transition metal in a tetrahedral configuration. Figure 6.8(b) shows four ligands at the vertices of a tetrahedron. The three d orbitals, which we shall call tZ, are nearer to the ligand than are the other two e orbitals. This implies that, unlike an octahedral coordination, in a tetrahedral coordination the three t2 orbitals have more energy than the two e orbitals (Fig. 6.7(a)). The crystal field separation value is indicated by A, and is inferior to the Ao(A,lA, = 419) for two reasons: (1) because there is no direct interaction between the ligands and the d
Table 6.4. CFSE for transition metals of the first series i n octahedral configurations Number of d electrons
Ion
Highspin configuration t,,
0 1 2 3 4
5 6 7 8 9 10
0 1 ,i2+v3+ 2 3 v2+cr3+Mn4+ 3 cr2+~n3+ 3 ~n'+Fe~' ~ e ' + ~ o ~ + N i ~ 4+ 5 co2+Ni3+ 6 Ni2+ 6 cu2+ 2n2+~a3+Ge4+ 6
Lowspin configuration
e,
CFSE (A,)
t,,
1 2 2 2 2 3 4
0.0 0.4 0.8 1.2 0.6 0.0 0.4+P 0.8+2P 1.2+3P 0.6+4P 0.0+ 5P
0 1 2 3 4 5 6 6 6 6 6
ca2+sc3+Ti4+
e,
CFSE(A,)
1 2 3 4
0.0 0.4 0.8 1.2 1.6+ P 2.0 2P 3P 2.4 1.8+3P 1.2+3P 0.6+4P O.O+5P
+ +
Ionic crystals
orbitals of the metal ion; This explains why, as experience has demonstrated, tetrahedral complexes have only highspin configurations. Table 4.5 shows the CFSE relative to highspin configurations for tetrahedral sites. At this point it will be useful to list the factors, which are at times mutually opposed, which govern cation coordination: voluminous ligands favour tetrahedral coordination (see p. 425); the position of the ligand in the spectrochemical series (see p. 415) favours tetrahedral coordination if on the left, octahedral if on the right: a high ligand charge favours octahedral coordination, because it increases Ao, which in turn favours the formation of lowspin complexes, increasing the number of electrons in tZgorbitals; the CFSE favours octahedral complexes, both because A. = (9/4)A,, and because the CFSE of tetrahedral complexes is generally less than those of octahedral complexes (cf. Tables 6.4 and 6.5). If the CFSEs of Table 6.5 are multiplied by the scale factor 419, they can be compared with the CFSE of Table 6.4, and the octahedral site stabilization energy, OSSE (i.e. the difference between the CFSEs concerning octahedral and tetrahedral sites), can be calculated in A. units (see Table 6.6).
Applications of lattice energy calculations Lattice energy calculations make it possible not only to rationalize a series of observations arising from structural analyses, but also to resolve certain problems without recourse to Xray techniques. Amongst the numerous applications of lattice energy calculations, easily computed with the aid of
Table 6.6. OSSE for transition metals of the first series. For the ions involved see Table 6.4
CFSE, A, unit
CFSE, high spin
OSSE high spin
CFSE, low spin
417
Table 6.5. CFSE for transition metals of the first series in tetrahedral configurations. For the ions involved see Table 6.4
(2) because there are four ligands instead of six.
Number of d electrons
1
OSSE low spin
Number of d electrons
Highspin configuration e
t,
CFSE(A,)
418
1
Fernando Scordari various automatic programmes,[72132141 are the following: (1) the distribution of cations in different sites; (2) the effect of the distribution of certain cations in certain sites on the position of others;
(3) structural predictions; (4) solutions to structural problems; (5) the determination of charge distribution in complex ions; (6) the estimation of the elastic constants of stable minerals subjected to very high pressures; (7) the effects of temperature and pressure on structures Let us examine some examples in more detail. U, was calculated for 16 isostructural compounds with olivine, including certain berylites, borates, phosphates, and silicates.[1s1 The structure of olivine, space group (s.g.) Pbnm, can be described as a distorted hexagonal closestpacked system of oxygen atoms (see p. 444). The six coordinated cations occupy two sites which are not crystallographically equivalent, M(1) and M(2) respectively, at the centre (0.0,0.0,0.0) and on the mirror plane. In silicates with an olivinetype structure these cations may be monovalent, bivalent, or trivalent (Li+, Na+, M ~ ' + ,Fez+, c a 2 + , Fe3+, etc.). Potential energy calculations indicate that if the ionic radii of the cations are comparable, then the cations with smaller charges will prefer the M(l) site. If, instead, the ionic radii are of quite different sizes, then the cation with the greater volume will prefer the M(2) site. In accordance with the calculation, where re(Li+) = 0.76 = re(Sc3+)= 0,745 A, the compound Li+Sc3+[Si04]is found to have Li+ in M(l) and Sc3+ in M(2). Moreover, where r e ( ~ g 2 +=) 0.72 # re(Ca2+)= 1.00 A, the compound MgCa[Si04], monticellite, has Mg2+ in M(l) and Ca2+ in M(2). Another example is the influence of the Al/Si distribution on the sites occupied by Na+ in albite (AlSi,O,) at high temperatures.[161Here too the calculations agree with the experimental data, that is to say, the concentration of A13+ in a particular tetrahedral site determines the site which the Na+ will occupy. The determination of the structure of an inorganic crystal by means only of calculations of potential energy has serious practical drawbacks if suitable crystallochemical information is lacking initially. It would be necessary to do an enormous number of trials, moving the atoms in all possible directions, if their precise positions are not known initially. ~ e c e n t l ~ , [ ' ~ ] starting from the ideal structure of olivine, it has been noticed that the compact regular layers of oxygen atoms used as input in the calculations are deformed in the process of potential energy minimization, just as the actual structure shows them to be.
Ionic radius An important factor which influences the geometry of the structure of ionic compounds is the socalled ionic radius. It expresses the 'dimensions' of an
Ionic crystals
ion considered as a rigid sphere. Since a finite value of r, when D,,[(r) = 0 (Fig. 6.2), does not exist, 'atomic radius', and thus also 'ionic radius', are merely conventional terms. Nevertheless, data derived from structural determination by means of Xray techniques suggest that d M x (the interionic distance between a cation M and an anion X) is the sum of the two 'radii' characteristic of the two adjacent ions. The problem which needs solving is how to divide d M x between the anion and the cation. With this aim, ~ a u l i n g [considered ~] certain alkaline halides, characterized by pairs of isoelectronic ions such as NaF, KC1, RbBr, CsI, and calculated their effective charge Z,, = Z  S. Z expresses the formal charge, while S indicates a screening effect which depends on the distance of the electrons from the nucleus and on which orbital they occupy. This effect can be explained on the basis of the radial distribution curves (Fig. 6.2), which show how s orbital electrons provide better shielding for electrons of other orbitals than they, in turn, receive from them. For example, 2p orbital electrons are better shielded than the 2s orbital electrons, because the latter are nearer to the nucleus. In order to evaluate S, certain principles suggested by Slater are followed: 1. Group the electrons as follows: 2. Use the multiplication coefficients 0.35 and 0.85 for electrons belonging to the groups (ns, np) and ((n  l)s, (n  1)p) respectively and 1 for those belonging to the group ((n  2)s, (n  2)p) or to any preceding group. It is preferable to use 0.30 to 0.35 in the case of groups (Is). 3. If the electrons belong to groups (nd) or (nf), use the coefficients 0.35 and 1, respectively, for electrons which belong to the same group, or for those which belong to the next group to the left. For example, for the compound NaF:
and, in accordance with ~ a u l i n ~ ,since [ ~ ] the ionic radius is inversely proportional to Z,,, and it is known that d M x = 2.32 A, we can obtain:
By resolving the system (6.21), re(Na+) = 0.95 and re(F) = 1.36 A can be obtained, which agree perfectly with the ionic radii quoted by ~auling.[~I This procedure can be extended to analogous isoelectronic compounds. Various ionic radius systems have been proposed, amongst the most accurate, thanks to the large number of structures examined, are those which have appeared Effective ionic radii extracted from Shannon's original work[lglare given in Table 6.7. These systems show that: 1, Cations are generally smaller than anions. The average radius of the outermost occupied orbital varies considerably from the least electronegative atom to the cation, but very little from the most electronegative atom to the anion, e.g. ro(Li) = 1.586, ro(Li+)= 0.186 A and r,(K) = 2.162, ro(K+)=
1
419
420
1
Fernando Scordari
Table 6.7. Effective ionic radii ( r e ) versus coordination number (CN) according to Shannon[lgl Ion
CN
Spin
re
Ion
CN
Spin
re
Ion
CN
Spin
re
1
Ionic crystals Table 6.7. (Continued) Ion
CN
Na'
Na' Nb3+ Nb4+
Nb5+
~
d
Nd3+
Ni2+
Ni3+ Ni4+ yo2+ Np2+ NP3+ NP4+ Np5+ NP6+ Np7'
o2
OH
os4+ os5+ os6+ os6+
os7+ os8+ p3+ p5+
pa3+ pa4+ pa5+
pb2+
~
+
Spin
re
Ion
CN
Spin
re
Ion
CN
Spin
re
Ion
CN
Spin
re
421
422
1
Fernando Scordari
0.592 A. In the anions the added electron increases the radius by a few per cent, e.g. ro(C1) = 0.725 A, ro(C1) = 0.742 A and ro(Br) = 0.851, r,(Br) = 0.869 A. 2. The dimensions of the atoms decrease along the period (with n a constant), the alkaline metals having the largest dimensions, and increases sharply along the group from top to bottom (with n a variable). This occurs because the dimensions of an atom depend both on n and on Zeff,which act on the atomic radius producing contrasting effects. Thus an increase in n tends to increase the atomic volume (the most probable radius increases with n, see Fig. 6.2), while an increase in Z,, tends to contract orbitals. For example, the Z,, calculated with Slater's principles for Na and C1 are respectively 2.20 and 6.10, while for Li and Cs they are 1.3 and 2.2. In the first case the sharp increase in Z,,, which is not countered by n (which is constant), induces a decrease in the dimensions from Na to C1. In the second case the regular increase in n, hardly countered at all by the effects of Z,,, induces a notable increase in the atomic volumes from Li to Cs. Obviously this also follows for the ionic radius. 3. The ionic radius varies with the coordination number (CN). Note that the repulsion forces increases with the CN, which in turn increases the effective ionic radius re of the ion of the opposite charge (the cation). The lattice energy allows this trend to be quantified approximately. (6.15) can be rewritten as:
E =  AMzlz2e2+CNB R R" where AM is Madelung's constant (which has taken the place of 1.39) and CN, which is defined below, is the coordination number (which has taken the place of the number 2, that is the two anions coordinated by the cation, see Fig. 6.5 and eqn (6.13)). For R = Re, dEldR = 0, from which we can work out:
Let us suppose that ions of opposite charges can crystallize just as well into a CsCl type structure as an NaCl (halite) or ZnS (wurtzite) one. Assuming that the intermediate value n = 9, we obtain:
The result of (6.24) indicates that the interionic distances of a CsCl type lattice (R,) are 2.3 per cent greater than those of an NaCl type lattice (R2), while (6.25) shows that those of a ZnS type lattice (R3) are smaller than it by =4 per cent. Since the anion radii remain more or less the same, the variations occur almost entirely in the cation radius. 4. The ionic radius depends on the electronic spin state. There is a close relationship between ionic radius and spin state in transition metals. In fact,
Ionic crystals
1
423
as explained on p. 415, A. and A, depend on the type of ligands, and the coordination polyhedra which the ligands form around the transition metal. If, for example, A. is high, then the first six electrons tend to occupy the lower energy level orbitals, while if A. is low they occupy both energy levels (Fig. 6.7). These differences in turn affect the ionic radii of the transition metals which have from four to seven electrons in their d orbitals. To be more precise, electrons with high spin have a larger radius than those with low spin (Fig. 6.9).
5. The ionic radius is influenced by polarization. Two ions of opposite charges, if they are far enough apart, have coinciding barycentres of their positive and negative charges. When the ions are brought together a distortion of the electronic charge known as polarization, takes place, which is greater in the anion. Combination requires a sort of participation on the part of the electronic charge, and therefore a certain degree of polarization, or covalent bonding. In accordance with ~ajan,['O]the polarization depends on: (a) the dimensions of the cation and its charge; (b) the dimensions of the anion and its charge; (c) the deviation of the electronic configuration from that of a noble gas.
Fig. 6.9. Dependence of the effective ionic radii on the spin state in transition metals of the 1st series: (a) = bivalent; (b) =trivalent. The full circles refer t o lowspin configuration, the open circles refer t o highspin configuration.
424
1
Fernando Scordari
This means, for example, that for alkaline metals the polarization power increases according to the following scale: Li+ > Nai > K+ > Rbf > Cs+ (ionic potential, 0 = Z / r , increases from right to left). Regarding the anions, the greater the dimensions of their outermost electrons, the weaker are their bonds, due both to the greater distance from the nucleus and to the increasing shield effect. It follows that the polarizability of halogens varies according to the scale: I > Br > C1 > F, analogously with that of haicogens. Anions with a high negative charge, such as As3 and p3, are particularly easily polarized. Moreover, it has been shown above how the different peripheral electrons are shielded by the s, p, and d type electrons. Therefore, although ~ i ' +has approximately the same ionic radius as Mg,'+ it polarizes more than Mg2+ one extra contiguous anion: this effect is even more noticeable between Cu+ and Naf.
Maximum filling principle The lattice energy of No pairs of ions can be expressed as the sum of the potential energy contributions (uij) relative to all the possible pairs whose components are distant rij: 1 'No UL=uij(ri,) (with i # j). 2 i.j=1
2
(6.26)
The lattice energy is minimal if the total potential energy is minimal, this occurs when: (1) the interatomic distances are as close as possible to the equilibrium distances (R,); (2) the number of ions at, or very nearly at, the equilibrium distance is as high as possible. These conditions are general and apply to crystals having simple structural units, or complex units connected to similar units by central or near central forces of attraction. The maximum filling principle can be expressed as follows: 'Simple (atoms or ions) or complex (groups of atoms or ions) structural units on which central or near central attractive forces act tend to increase contact with each other to the maximum, whilst reducing their distances to a minimum'.
By supposing that the ions behave as if they were rigid spheres on which central, or almost central, forces are acting, we can hope to: (1) predict the most probable arrangement of the anions which surround the cation (coordination polyhedra), by means of a simple geometric rule (radius ratio rule); (2) describe certain atomic building by means of dense mechanical models based on rigid spheres of equal radius (closest packings).
Ionic crystals
1
425
Coordination polyhedra It is sometimes convenient to illustrate crystal structures by means of coordination polyhedra, in order to underline the geometrical relationships which characterize structural frameworks. Often such polyhedra continue to exist beyond the crystal state as definite physicochemical realities, e.g. [siO4I4 tetrahedra in silicate melts, or Fe(H20),.,(SO4), octahedra where 1< n < 1.3, in aqueous solution of iron s ~ l ~ h a t e . [ ~ ~ ] The term coordination is used to refer to the atoms or ions which surround a central atom or ion. If it is not otherwise specified below, it may be assumed that the central ion is the cation (M) surrounded by the anions (XI. The Xs at a tangent to M are known as the first nearest neighbours of M and constitute the first coordination shell. The coordination number (CN) is equal to the number of the first nearest neighbours, i.e. to the number of bonds formed by an atom. The next Xs, at a tangent to the first nearest neighbours, are known as the second nearest neighbours of M, and form the second coordination shell, and so on. Sometimes the first coordination shell is not easily distinguished from the second. In such cases the uncertainty is expressed by attributing two numbers to the CN, e.g. 6 2. The distances dMx are all equal when M occupies certain symmetrical positions, e.g. M in 3, with CN = 6; otherwise the dMx vary, if only a little, from their average. The coordination polyhedron of M can be obtained by 'joining the dots', i.e. all the centres of X. Some of the possible coordination polyhedra are shown in Figs. 6.10 and 6.11. They can be found in structures as isolated polyhedra, and/or connected to polyhedra of the same or another type.
+
Radius ratio rule If the ions are considered as behaving like rigid spheres, an attempt can be made to predict by geometrical means which coordinations will be preferred. The parameter used for this purpose is p, = (r,/r,). Figure 6.11 shows some of the most common regular geometrical dispositions and their relative p, ratios. The p, values for a given anion increases as rM, and thus the number of contacts also increase. From Fig. 6.11 it can be deduced, for example, that within the range 0.155 S p, < 0.225 a triangular coordination is stable, since for p, < 0.225 cations and anions are no longer adjacent in tetrahedral coordination; thus it is no longer possible. However, the results obtained by geometrical methods must be integrated with further energetic considerations. Figure 6.12 shows the trend of U, versus p, for CsCl, NaC1, and ZnS type structures having the following ratios:
This formalism not only indicates the coordination number around each ion, but also allows their stoichiometry to be deduced, which for the three
Fig. 6.10. Some coordination polyhedra. (1) tetragonal pyramid, (2) trigonal bipyramid, (3) trigonal prism, (4) onecap trigonal prism, (5) sevenvertex polyhedron, (6) pentagonal bipyramid, (7) trigonal dodecahedron, (8) twocap trigonal prism, (9) threecap trigonal prism, (10) icosahedron, (11) truncated tetrahedron, (12) rhombododecahedron, (13) pentagonododecahedron, (14) truncated octahedron. The coordination number of each polyhedron is indicated below it.
426
1
Fernando Scordari
Polyhedron
Anions
Relationships between rM and rx
Dumbbell
B
A H
Triangle
C
Tetrahedron B
Square
. D
/ C
~
A
B
Octahedron
Square antiprism or Thomson's cube
Cube
Hexagonal cuboc.
Cuboctahedron
Fig. 6.11. Other very common coordination polyhedra. At the side of each polyhedron there is its coordination number, name, and the procedure followed to calculate and p,.
A B = 2 r x , A O = r M + r X , m 1= (AD  F G ) / 2 AH' = r X g ,AH = r x m , 00' = = / 2 , O'C = r X G (00')' = ( A O ) 2 , (rM/rX)' 2rM/rx ( G + 2 ) / 2 = 0
+ (m)'
+
Ionic crystals
1
427
compounds in question is M:X = 1:1. From Fig: 6.12 it results that: (1) the UL trends are characterized by three discontinuity points in correspondence to the values p, = 0.732, 0.414, 0.225; (2) the UL trends favour a CsCl type structure when p, > 0.71, and an NaCl type when 0.71 > p, > 0.32; (3) the UL(NaCl) curve is closer to that of the UL(CsC1) than to that of the UL(ZnS).
Fig. 6.12. U, pattern versus p,. From the point of view of the energy, the minimum p, values for CsCI, NaCI, and ZnS type structures are lower than those predicted by geometrical means. The difference is most accentuated i n the range between an NaCl and a ZnS type structure (0.32 instead of 0.41).
The reasons why these discontinuities exist become clearer on observing Fig. 6.13. In (b) an octahedron of M(X), composition is shown, while in (a) and in (c) the same polyhedron for a larger cation (M' > M) and for a smaller one ( M < M) are illustrated respectively. In accordance with (6.17), the value of UL(NaC1) decreases gradually from configuration (a) to configuration (b), since Re < R:. However, UL does not vary in the range 0.32 < p, < 0.414, that is to say, between configurations (b) and (c), since the anions already adjacent in (b) cannot come any closer together. Thus Re has the same value in both configurations (b) and (c). Configuration (d) is preferred to (c) if, in accordance with the UL(NaC1) trend of Fig. 6.12, there is another cation M"' < M so that p, < 0.32. In the same way, an NaCl type structure is likely to be preferred to a CsCl type when p, < 0.71, i.e., for p, values a little below the discontinuity point (p, = 0.732).
PO @ L3 .,
(4
(b)
Applications of the concept of ionic radius To assume that an atom is rigid, and also spherical, is obviously a gross simplification of the physical reality. Accurate studies[221to determine p(r) have shown, for example, that in MgO the electronic cloud of the oxygen only partially wraps the cation: therefore the terms sphere and ionic radius lose any meaning. Despite this, however, the concept of ionic radius often produces satisfactory results. Alkaline halides and, to a lesser extent, alkalineearth metal oxides are the compounds to which a mechanical atomic model is most easily applied. Such compounds with an MX stoichiometry should have structures with a CN = 8, if the ionic radii r,(M)
Fig. 6.13. (a), (b), and (c) illustrate the changing relationships between equal anions (white circles) in an octahedron, as the cations vary i n size (broken circles). Configuration (c) becomes unstable and could evolve into configuration (d) if pe < 0.32.
428
1
Fernando Scordari LI
+
Na"
K+ RbiCs'
Fig. 6.14. Three fields are shown (T, 0, C), delimited by t w o unbroken lines (p, = 0.73,0.41). In accordance with geometrical criteria, they represent stability areas for the alkaline halides. The broken line (p, = 0.32) shows the reduced T field according t o the energy indications of Fig. 6.12. The diamonds and squares show the type of coordination polyhedron on which the real halide structures are based: octahedra and cubes respectively.
Fig. 6.15. Taking into account ionic radii r,(A) and r,(B) the stability fields for A2B04 structures are shown. These fields conform t o the following structure types: (a) 0K2S04, (b) Na2S04(thenardite), (c) (Mg, Fe), SiO, (olivine), (d) Be2Si04 (phenakite), (e) A12Mg0, (spinel), (f) Sr2Pb04, (g) K2NiF4, (h) FeJaO,, (i) A12Ba04.
and r,(X) are more or less the same. Otherwise, such compounds are governed by the cation coordination number (since the cation is generally smaller than the anion) and the stoichiometry. The dimensions of the cation depend on the CN (see p. 422). Therefore ambiguity remains as to the ionic radius dimensions when the structure (and thus the CN) is not known. Let us compare the theoretical data with the experimental data for the halides. 'Average' ionic radii for a CN = 6 are used, for example, CsBr (r, = 1.67, rx = 1.96 A) forms a compound Cs': Br = 8:8, in accordance with both the radii ratio: (p, = 0.85) and the stoichiometry (M:X = 1:l). Also for NaCl both the p, = 0.53 and the stoichiometry indicate a compound Na+:Cl = 6:6, in accordance with the results of structural analysis. The rule of the radius ratio predicts M:X = 4:4 structures in the higher field T (p, < 0.41), M:X = 6:6 in the intermediate field 0 (0.41 G p, < 0.73), and M:X = 8:8 in the lower field C (p, > 0.73). Experimental data, on the other hand, shows that almost all the structures are of M:X = 6:6 type, two are of M:X = 8:8 type (CsI, CsBr), and one, CsC1, can crystallize in either type of coordination. In Fig. 6.14 a broken line is shown for p, = 0.32, which corresponds to the point of intersection of the NaCl and ZnS curves in Fig. 6.12. The first anomaly involves the T field. The incongruence between the observed structure M:X = 6:6 and the predicted structure M:X = 4:4 by the radius ratio rule is only apparent. Considering Fig. 6.12, NaCl type configurations are stable for 0.32 < p, < 0.41, i.e. the values observed. The other anomaly involving the lower field, C, is constituted by M:X = 6:6 structures and can be explained by considering not only the interactions between ions of opposite charge, but also those between ions of similar charge in the CN function, and the geometric relationships between the coordination polyhedra (see p. 435). However, if re(IVLi+)were used for LiI, p, = 0.27 would be found to be the right value. The configuration Li+:I = 4:4 would gain potential energy and would therefore seem likely to be preferred, which is contrary to the experimental data. Another example can be illustrated by means of Fig. 6.15, as deduced by ~ h i l l i p s . [ ~The ~ I 'fields of stability' for the most important structures of A2B04 composition are shown. The diagram was obtained empirically on the basis of about 130 structures using the effective radii of the cations in octahedra1 (r,) and tetrahedral (r,) coordinations. Such a diagram makes it possible to work out the field in which a certain A,BO, structure prevails, even if some borderline cases may be contrary to the general trend. Improvements in structural predictions can be obtained by considering not only geometrical factors but also chemical factors, such as polarization. Graphs for compositions of M,X, type have been obtained by plotting the average quantum number n (which indicates roughly the dimensions of the ions) on the y axis and the electronegativity difference, AEN (which indicates the degree of polarization of the bond),[241on the x axis. The prediction is improved if p,AEN is used instead of AEN. Finally using effective mean ionic radii, several have found quantitative relations between crystallographic and compositional parameters in garnets. So according to as so,[^^] it is possible to calculate the oxygen fractional coordinates, the metaloxygen distances, and the cell
Ionic crystals
edge of oxide garnets and hydrogarnets as follows:
where r(X), r(Y), and r(Z) are the mean ionic radii respectively of cations 8, 6, and 4 coordinated, and (OH) are the number of OH groups present in the formula unit (f.u.) of garnets:
Closest packings Most metals, some compounds of the type MX, MX, etc., and others with a more complex stoichiometry, take on structures which can be described by means of closest packings of rigid spheres of equal radius. Let us denote by packing coefficient (ci) the ratio: ci =
C (VaIVc)
(6.27)
where C Va is the volume of the atoms or anions contained in the elementary cell of volume Vc. For discussion of the concept of ci see Appendix 6.A. According to the maximum filling principle, ci + max. Hexagonal closest packing (HCP) and cubic closest packing (CCP) satisfy this requirement. When analysing their characteristics, it should be borne in mind that in the common structures, ions, atoms, or groups of either, replace rigid spheres forming the socalled closestpacking structures. The basis of the HCP and CCP dispositions is a layer of spheres (layer A) packed as closely as possible similar to that illustrated in Fig. 6.16. This layer has the following characteristics: every sphere is in contact with another six spheres; between every three spheres there is a space, known as a hole, every sphere is surrounded by six holes, one third of each of which belongs to it, so a total of two holes can be associated with each sphere. Such holes, which are all alike from a physical point of view, are indicated by b (white) and c (black). Spheres belonging to the next layer may correspond to the b or the c holes of layer A, and are thus said to belong to
1
429
430
1
Fernando Scordari
Fig. 6.16. A compact layer of spheres characterized by triangular cavities indicated by white spaces (b) and black spaces (c). At the top of the sketch on the left is shown the symmetry of the layer A (6m), while on the right is shown the symmetry of a pair of layers AB (3m).
layer B or layer C. With reference to a hexagonal mesh of sides a, and a2, in general a sphere may correspond to any of three possible holes: a (for layer A) belonging to site (Oa, + Oa2+ nh) b to site ((2/3)a, + (1/3)a2+ nh), and c to site ((1/3)al + (2/3)a2 + nh), where n is a whole positive number including zero and h is a vector perpendicular to the compact layer of a module h (which is equal to the distance between two successive compact layers). HCP is characterized by an ABAB . . . type sequence, while CCP is characterized by an ABCABC . . . type sequence. The two characteristic sequences which represent HCP and CCP and their orientation with respect to the compact layers, are illustrated in Fig. 6.17. The HCP cell is projected in the direction [OOl] 11 h, while the CCP cell is projected in the direction [ I l l ] 11 h. An HCP cell contans two spheres (that of a simple hexagonal cell contains one); a CCP cell contains four, as does a facecentred cubic (FCC) lattice (for this reason it is possible to use FCC or CCP with the same meaning). It is possible to identify four types of polyhedra in both packings: cuboctahedra, octahedra, tetrahedra, and triangles. The first, illustrated in Fig. 6.11, can be traced by joining the centres of the 12 spheres around a central sphere of equal radius. The other three can be traced by joining the centres of the spheres which correspond to the three possible holes of the closest packings: octahedral, tetrahedral, and triangular.
Fig. 6.17. An ABAB.. . sequence of layers determines a compact hexagonal cell (top), while an ABCABC . . . sequence determines a compact cubic cell (bottom).
Ionic crystals
1
431
Many cations have a radius of just the right size, compared with that of the oxygen atoms, that they can occupy tetrahedral or octahedral holes. Let us examine, therefore, these two types of holes more closely in order to find out what is their quantitative ratio to the spheres. In Fig. 6.18 a layer A (black spheres) and a layer B (white spheres) are shown. Supposing that the sequence is an ABAB . . . type, a sphere marked S (belonging to layer A and not visible in the figure) is surrounded by a total of 12 spheres (six of A and six of two B layers, above and below A). It contributes to the formation of: (1) six octahedral holes ( 0 ) three of which are shown in the figure; the other three can be obtained by a symmetry plane m which passes through A; (2) eight tetrahedral holes, three of which, shown in the figure, are in correspondence with the three spheres marked with a thick T and one of which is in correspondence with the sphere marked S and three of the spheres marked with the same T; the other four can be obtained by a symmetry plane m which passes through A.
.. Fig. 6.18. Octahedral, 0, (top right) and tetrahedral. T. (bottom right) holes with relative coordination polyhedra &a& out from t w o fo~~o~in~compact~a~e~~.
Since six spheres are needed to form an octahedral hole and every sphere helps to form six holes, obviously there is a ratio of one hole to each sphere. Four spheres are needed to form each tetrahedral hole, while each sphere helps to form eight tetrahedral holes, so there is a ratio of two tetrahedral holes to each sphere. A layer of octahedral holes (OL) is enclosed by two layers of spheres, as are two layers of tetrahedral holes (TL), through they are orientated in different directions (see Fig. 6.32). This situation is common both to HCP and CCP, consequently a double layer of spheres has the following characteristics in both HCP and CCP: 1. Octahedra which share edges. 2. Tetrahedra which, differently orientated (TL, and TL,), share edges. 3. Octahedra and tetrahedra which share faces. The differences between HCP and CCP are in the geometric elements shared by the polyhedra in the direction perpendicular to the layers; these are the differences which concern us most here. HCP has all the octahedra and half of the tetrahedra sharing faces with polyhedra of the same type, the other half of the tetrahedra sharing vertices, and finally the octahedra and tetrahedra sharing vertices and edges. Instead, CCP has (Fig. 6.19) all the octahedra sharing faces with half of the tetrahedra, the other half of the tetrahedra sharing vertices, and finally the octahedra which share edges, as do half of the tetrahedra. It follows that, for example, while in HCP the octahedra share faces in the direction perpendicular to the OL and edges parallel to the OL, in CCP the octahedra share edges only. Such differences are very important for certain ~toichiometries[~~] as we shall see below, since they affect the stability of the structure and thus which type of packing is preferred. There are two coefficients which characterize closest packings. The first is q (6.27), which has a value of 0.74 both for HCP and CCP. It is easily found, remembering that an elementary HCP cell contains two spheres
Fig. 6.19. An FCC cell. The tetrahedral (black triangles) and octahedral (white diamonds) holes of a CCP are shown. Note that the number
~~~~~[~~j:~:","~",:~~~~~$~~ of that of the tetrahedral holes.
432
1
Fernando Scordari
Fig. 6.20. The centres of the three spheres marked A and the centre of the sphere marked B together form a trigonalpyamid. It canbe = D V 3 / 2 , HH'= deduced from this t h a ~ BH' : l / 3 ( B H 1 )= DV3/6, h = ~ 9 6 1 3h, / D = q 6 / 3 = 0.8165.
while a CCP one contains four (Fig. 6.17). For example, the side of an , D is the diameter of a sphere. elementary CCP cell will be a,, = ~ j 6 where The volume of a sphere is V, = 4.189(D/2)3 from which c, = 4v,/a3 = 0.74. The other parameter is the ratio hlD. Since h = [ ( ~ V ' 3 / 2 ) ~ ( ~ f i / 6 ) ~ ](see " ~ Fig. 6.20) it follows that h l D = 0.8165. For example, in HCP, co = 2h, therefore colD = 1.63. Combinations of HCP and CCP can create an indefinite number of closestpacking structures. The repetition period, nh, will be in the range , p , is the maximum dimension of the crystal perpen2h S nh ~ p , where dicular to the closestpacked layers which the sequence can reach when the structure is completely disordered. As n increases, the number of possible sequence combinations grows very rapidly. For example, there is only one possible packing for n =4: ABACA; for n = 6 there are two: ABCACBA and ABABACA; but for n = 20 the number of possible packing rises to 4625. One of the following ways can be chosen to derive the possible packings: the first is to count all the possible sequences once having generated them;[301the second is to obtain them by means of combinatorial analysis.[311Figure 6.16 shows the symmetry of a closestpacked layer (6mm) and of a pair of such layers (3m). The minimum symmetry content common to all closest packings is P3ml. Other symmetries are represented by all those space groups which can have as a subgroup P3ml (see also Fig. 1.E.1), i.e. ~ 3 m 1 ,~ 6 m 2 ,Pb3mc, P6,/mmc, R3m, ~ g m ~, m 3 m .For HCP and CCP the space groups are respectively: P63/mmc and ~ m 3 m . When real structures are considered the symmetry may be reduced, due not only to the arrangement of the cations which occupy the various holes, but also to the distortions which the cations produce in the lattice. Therefore, some structures belonging to systems different from those just examined can be described as closest packings, distorted to a greater or lesser degree. There are other close packings characterized by spheres with fewer next neighbours. These are the PTP (primitive tetragonal packed), the BCT (bodycentred tetragonal), and the BCC (bodycentred cubic). The first has c, = 0.72 and CN = 11, the second (not found in the known structures) has c, = 0.70 and CN = 10, the third (taken on by several structures) has c, = 0.68 and 8 6 spheres of the same type coordinated around a central sphere, eight at a distance of D and six at a distance of 1.150 (Fig. 6.21). HCP and CCP, on the other hand, have 12 spheres all at the same distance from the central sphere.
+
Fig. 6.21. A BCC cell. The central sphere is surrounded by eight spheres at a distance of D and six more distant spheres at 1.150 ( 2 0 = 1V3, where / i s the side of the cell).
Ionic crystals
Pauling's rules Ionic bonds play an important role in the building up of structures for the vast majority of minerals. In fact, even the groups (Si04)4, (SO4)', (C0,)', which have prevalently covalent bonds internally, can be seen as large negative ions bonded to the cations by essentially ionic interactions. The general principle of the minimization of potential energy can be applied to such compounds. The Pauling rules are derived from this principle.
Pauling's first rule This rule synthesises the geometric relationships which tend to be established between cations and anions in a stable structure, introducing the concept of the ionic radius. A coordination polyhedron is formed around each cation. The distance between the cation and the anion is determined by the sum of the radii, while the coordination number of the cation is determined by the radius ratio.
The maximum number of anions, compatible with the equilibrium conditions imposed by the minimum potential energy, surround the cation. Too many anions would increase the cationanion distance, thus making the structure less stable than if the distances are very close to Re. The optimum distance is the sum of the ionic radii: rM r,. However, the cationanion distances do not depend only on the ionic radii of the cation and anion involved, but also on the average radius of each of the other cations.[321In structures of a certain complexity, it can happen that not all the cations have optimum CN and dMx distances. In such cases some cations, above all the largest ones with the lowest valence (formal charge), are the first to take on higherenergy coordinations, followed by smaller highervalence cations which tend to form more rigid coordinations. It follows that the lowest coordination expected for Na+ (which taking into account the oxygen has p,=0.71) is 6, but in sodalite, Na8C12[Si6A16024], it has CN = 4 (302 + ICl), while Si4+,half of which is substituted by AP+, has its usual CN, i.e. 4.
+
Pauling's second rule Known as the valence sum rule, this rule analyses the electrostatic balance: The valence of an anion in a stable ionic structure tends to compensate the strengths of the electrostatic bonds which reach it from the cations situated at the centres of the polyhedra of which the anion is a vertice, and vice versa.
In practice, this rule means that the electrostatic balance is satisfied by the cations belonging to the primary coordination. If V is the valence of an anion, vi and (CN,), are respectively the valence and the coordination number of the ith cation, then we can define the electrostatic bond strength as si = V~/(CN,)~. The rule can be summarized as: v=& (6.28) i
where i is extended to all the cations coordinated by the anion in question.
1
433
434
1
Fernando Scordari For highsymmetry, simple ionic structures it is possible to give a single value to the bond strengths and to find the valence of a given ion by multiplying the bond strength i times. For example, for NaCl (space group ~ m 3 m ) the , bond strength which reaches a given C1 from a given Na+ is 116. Since there are 6 Na+ surrounding each C1, all equidistant from it follows:
The same procedure can be applied as a rough guide to rutile, Ti02 (space group P42mnm) whose structure is based on slightly distorted Ti06 octahedra. Each ~ i cation ~ + coordinates six 02and around each oxygen there are three Ti4+, This means that each oxygen receives 416 of the + , valence of titanium. Since very 0' is surrounded by three ~ i ~then:
which is exactly the opposite of the oxygen valence. In structures with irregular polyhedra, like brookite (a polymorph of the compound TiO,) which is characterized by strongly distorted Ti06 octahedra, this simple model needs to be modified slightly. In order to calculate the strength of each electrostatic bond, or more correctly the bond valence (s), Brown and ~ h a n n o n [proposed ~~] the following equation:
where so, Ro, and N are empirical constants. For so = 1, Ro = R,, the parameter R1 represents the expected bond length when the valence is assumed to be one. In such as a case (6.29) becomes:
By inserting the correct values for R, and N for each cation[341and the bond distance R, which can be deduced from the structure, s can be determined. For example Na+, Mg2+, A13+, Si4+,P5+, and s6+have values of R1 = 1.622 A and N = 4.290. The experimental bond valence can be obtained by applying (6.30). The agreement between the experimental and the theoretical valence is very good, generally the difference does not exceed 5 per cent. If the agreement is not satisfactory for an ionic structure it can be ascribed to the following: (1) the structure has not been correctly determined; (2) the structure has not been interpreted properly, or certain bonds have been overlooked, or the wrong atoms have been ascribed to certain sites (e.g. Si4+ in place of A13+ or vice versa). (3) The cations have stereochemically active lonepair electrons (e.g. sb3+). Amongst the various applications of this method[351it is often used by crystallographers to distinguish 0' from (OH) and H 2 0 in some complex mineral structures.[361Calculated bond valences can be used through (6.28) to calculate experimental atomic valence and so the oxidation state of an
Ionic crystals
1
435
Pauling's third rule This summarizes, from a qualitative point of view, the influence that the fact that the coordination polyhedra share geometric elements has on the potential energy and thus on the stability of the structure: The sharing of sides and, in particular, of faces between coordination polyhedra reduces the stability of a structure. This effect is accentuated where there are cations with high valence and low coordination number.
In order for the potential energy to be minimal it is necessary that:
(1) the distances between the cations should be as great as possible, compatible with the existence of the structure itself, (2) the cations should be shielded as much as possible from each other. Figure 6.22 illustrates the distances between cations for certain regular polyhedra. As can be seen, the fulfilment of conditions (1) and (2) are less likely, for any given pair of polyhedra, when they share an edge than when they share only a vertice, and least likely when a face is shared. The least probable of all the configurations are two tetrahedra which share an edge, and above all two tetrahedra which share a face. This explains why in silicates the tetrahedra [SiO4I4 are found either isolated or sharing vertices; they hardly ever share edges and never share faces. For tetrahedra containing cations with a higher charge, like [PO4I3, even the likelihood
Fig. 6.22. Geometrical relationships between some regular polyhedra. Considering the oxygens as touching rigid spheres with a radius of re = 1.40 A, the following intercation distances can be calculated: = 3.43, 4, =
1.98, 0(,=1.14, do,=3.96, %,=2.80, d,,=2.29, 4,=4.85, dc, =3.96, d,, = 2.80A. The sketch at the bottom shows the different shielding effects produced by three or four anions together on the underlying cation.
436
1
Fernando Scordari
that they will share vertices is reduced, so much so that in the case of group having yet higher cation charges, like [S0,I2, that it is almost nil. Figure 6.22 shows that do, = dCf.However, in octahedral coordinations the shielding of the two cations is more accentuated. This explains why numerous halites tend to keep the NaCl structure rather than that of the CsCl, favoured by p,. Structures like CsCl are only possible if the anions are large enough to keep the cations far enough apart, as can be observed in the case of CsC1, CsBr, CsI (in the NaCl structure type, the distance between two cations for CsF is 4.24 A and 4.92 A for CsCl). It should be remembered here that, in accordance with the indications of Fig. 6.22, ionic compounds with an MX stoichiometry (see p. 437) crystallize not with an HCP lattice, but with a CCP lattice (e.g. NaC1, MgO, CaO, etc.). This is because the energy levels involved in the formation of the two packings seen along h is different: in the case of CCP the octahedra MX6 share edges, while in the case of HCP they share faces. On the basis of what has been said, the question of how to realize the ~ [ ~ can ~ ~be understood. This relative stability of certain ~ i 0 polymorphs compound has three polymorphic modifications: rutile, brookite, and anatase. The structural differences concern mainly the way in which the TiO, octahedra are linked to one another. In rutile, brookite, and anatase, each octahedron shares respectively two, three, and four edges with a similar number of other octahedra. The structural stability of brookite is less than that of rutile, while anatase is the least stable, as predicted by the third Pauling rule.
Pauling's fourth rule The fourth rule is an obvious corollary of the third, and so no further comment is necessary: In a crystal containing various cations, those with high valence and a low coordination number tend not to allow the coordination polyhedra which they form to share any features.
Pauling's fifth rule The fifth rule, known also as the parsimony principle, states that: The number of essentially different constituents in a crystal tends to be small.
This rule summarizes the common observation that most of the nonfluid substances that surround us are crystalline and not amorphous. This means that the number of structural units, having considerable differences for instance with regard to volume and chemical properties, tends to be low for any given substances. Source applications of these rules together with symmetry and other crystallochemica1parameters are given in Appendix 6.B.
Ideal a n d defect structures The preceding paragraphs have dealt mainly with the principles which underlie the structural building of ionic compounds.
Ionic crystals Some simple, or at least not very complex, atomic configurations, characterized at most by few dozen atoms per elementary cell, will now be examined. Particular attention will be given to ideal structures, i.e. those structures in which it is possible to single out an elementary cell 100 per cent representative of all the cells that make up the crystal. In such cases all the crystallographic sites which are symmetrically equivalent (including the translation) must be occupied by the same chemical species and the resulting compound is defined as an ideal chemical formula. In defect structures the relative positions of the atoms are not regular throughout the crystal. Thus the representative cell is a statistical cell which expresses the probability that a certain site will be occupied by a given atom. In such cases the compound is better defined by a crystallochemical formula, which, apart from taking into account the stoichiometry, considers also the percentage of presences (occupancy) of a certain chemical element in a given crystallographic site. For example, the compound MgA1204 (spinel) parent of the spinels, is a normal spinel (see p. 442) and adopts the following ideal structure: Mg2+ occupies only the tetrahedral sites, while A13+ occupies the octahedral ones. The compound Fe304 (magnetite) is instead an inverse spinel (see p. 442) in which Fe2+ occupies only octahedral sites, while Fe3+ occupies half tetrahedral sites and half octahedral ones. Therefore the structure of magnetite can be represented by a particular cell of statistical significance having its tetrahedral sites occupied by Fe3+ and its octahedral sites occupied by 0.5 Fe2+ and 0.5 Fe3+. This structural peculiarity is evident from the crystallochemical formula Fe3+ (Fe::, Fe;:),O4 which substitutes the less explanatory stoichiometric formula Fe304. Moreover, the composition of a nonstoichiometric magnetite Fe,,O,, can be rationalized from its crystallochemical formula in the following way: ~ e ~ + ( ~ eFe:& , , 00.0,)204.In fact the reason why it is not stoichiometric becomes clear immediately: it is due to the substitution of Fe2+ by Fe3+,with the necessary abandoning of 5 per cent of the octahedral sites and the formation of gaps (represented by the square). From the point of view of symmetry, the space group ~ d 3 madopted both by the spinel and by the magnetite, represents in the first case true symmetry and in the second statistical symmetry. IG the next section some classes of simple structures, defined on the basis of their stoichiometry, will be analysed briefly. The silicates, included amongst the ionic compounds by tradition, will be considered briefly from the point of view of their classification.
MX structures As predicted by the third Pauling rule, the packing definitely preferred by MX compounds is CCP, while BCC is rare, and HCP is never adopted. It can be seen from the stoichiometry of these compounds that all the octahedra are occupied and that therefore an HCPbased structure is decidedly less probable than a CCPbased structure. In the first case, in fact, the octahedra share edges and faces, while in the second the octahedra only share edges. The nonexistence of hexaognal packing in the structures of MX compounds can be best explained with help of Fig. 6.23.
1
437
438
1
Fernando Scordari
Fig. 6.23. In (a) an unstable layer of cations (white spheres) and anions (black spheres) of equal radius R / 2 , is illustrated. By moving alternate rows in the direction of the arrows a distance of R / 2 , the stable layer illustrated in (b) is obtained. In (c) the structure of NaCI, or halite is shown.
A compact layer like that shown in Fig. 6.23(a) is not stable due to the strength with which like charges repel each other. Such effects are considerably attenuated if alternate rows are translated a distance of R/2 in the direction of the arrows (Fig. 6.23(a)) to give a regular one positiveone negative ion pattern (Fig. 6.23(b)). In order that a succession of layers of the same type (along the perpendicular to the layer examined) should be stable it is necessary that a second layer be translated by R. The successive translation (equal to R) of a third layer brings us back to the initial configuration. Such a succession of layers gives rise to a cubic structure like that of NaCl, space group Fm3m, or in other words, a CCP of C1 ions with all the octahedral sites filled by Na+. This tendency is strengthened if the cations are bivalent, which is why MX compounds almost always adopt CCP type packings. Apart from the halides previously mentioned (see p. 427), other examples are: periclase (MgO), wustite (FeO), bunsenite (NiO), manganosite (MnO), and lime (CaO). Some alkaline halides also crystallize naturally: villiaumite (NaF), halite (NaCl), sylvine (KCl), and carobbite (KF).
MX2 and M,X structures
Ca2+ OFFig. 6.24. A representation of the structure of fluorite, CaF,. In the figure the cubic coordination polyhedra of the ca2+ (black circles) are outlined, together with the geometrical relationships between them. The elementary cell (dotted lines) consists of four such polyhedra occupied by calcium and four similar empty polyhedra.
Such compounds present a wide range of structures, of which only a few are illustated here. Fluorite (CaF,), cubic, space group Fm3m, is shown in Fig. 6.24. Each cation Ca2+ is surrounded by eight F positioned at the vertices of a cube, while each anion F is surrounded by four Ca2+ positioned at the vertices of a tdtrahedron (Ca2+:F = 8:4). The structure adopts a quasiclosest packing of F similar to BCC, with half of the sites at the centre of the cube empty and half occupied by Ca2+ alternately, in substitution of F (p, > 0.73) at 112, 112, 112. Due to the alternate filling of these sites the cubes share edges instead of faces, and consequently the cations are further apart and better shielded (see Fig. 6.22). Various compounds such as SrCl,, BaCl,, and others with more complex formulae in which some cations are substituted by other cations e.g. 2Ca2+ t K+ + ~ a ~ 3Ca2+ + , + 2K+ + U4+ (for + read 'are substituted by'), etc. have a CaF, type structure. The ratio M:X = 6:3 is favoured when p, < 0.73 allowing the formation of structures similar to that of rutile (TiO,). The tetragonal structure of rutile, space group P4,/mnm, can be described as HCP. Figure 6.25 illustrates a layer of octahedra (OL) seen (a) perpendicular to and (b) parallel to its extension, while Fig. 6.26(a) shows a packing of OL layers of the type shown in Fig. 6.25(b). The black octahedral are occupied, the white are
Ionic crystals
empty. Figure 6.26(b) shows a structure of rutile obtained by the distortion of the ideal HCP as seen in Fig. 6.26(a). This is in agreemwnt with p, and with the stoichiometry of rutile which predicts that half of the octahedral holes will be occupied. The occupation of the holes occurs in such a way that the octahedra share edges and vertices, never faces, as is illustrated in Fig. 6.26(c). This feature means that HCP is preferred to CCP, in which the octahedra share edges only. Minerals with a structure like that of rutile include: sellaite (MgF,), pyrolusite (MnO,), cassiterite (SnO,), stishovite (SiO,) a highpressure compound, with Si4+hexacoordinated. A TiO, type structure is certainly one of the most common among strongly ionic binary compounds such as fluorides and oxides. It is also common amongst more complex compounds in which the Ti4+ is substituted by cations with a then + tapiolite (FeTa206) is similar radius: e.g. if 3 ~ i ~,+~ e , + 2 ~ a ~ + bystromite (MgSb206) is formed, or if instead 3Ti4++ ~ g , +2Sb5+ formed. Another structure typical of compounds with a ratio of M:X = 6:3 is that . has a layered of brucite (Mg(OH),): trigonal with space group ~ 3 m l It structure which can be described by means of HCP. There are two possible ways for half of the octahedral HCP holes to be occupied without the octahedra sharing faces: the first has already been illustrated for rutile; the second involves all the octahedra of alternate octahedral layers being occupied (e.g. OLA occupied entirely and OLB left completely free in Fig. 6.26(a)). Brucite is an example of the second type. It is more advantageous from the point of view of energy to fill every other octahedron of each row, as happens in rutile, rather than to occupy all the octahedra of OLA and none of OLB. This is because in the first case the octahedra are linked by (six) vertices and (two) edges, but in the second by (six) edges only. The layered structure of rutile is due to the permanent OH dipoles which link together the fully occupied octahedral layer;@]they are known as 'brucitic layers'. Minerals with a brucite type structure include: portlandite (Ca(OH),), pyrochroite (Mn(OH),), nibrucite (Mg4NiO(OH),). Another group of minerals with brucitic layers, space group ~ 3 mwhich , conform to CCP is: chlormagnesite (MgCl,), lawrencite (FeCl,), scacchite (MnCI,). If the cationanion positions of fluorite are inverted, an antifluorite
+
A OLB OLA OLB
OLA
B A B A
1
439
Fig. 6.25. An octahedral layer (OL) obtained by combining t w o compact layers of spheres of equal radius. In (a) it is seen perpendicular t o its extension, in (b) parallel t o its extension.
Fig. 6.26. In (a) (on the right) a sequence of ideal compact layers ABAB.. with the corresponding sequence of octahedral layers OLAOLBOLAOLB.. (on the left), seen parallel t o their extension. The rows of black octahedra (perpendicular to the sheet) are occupied, while the white ones are empty. In (b) the distorted closest packing is shown, while in (c) the rows of occupied octahedra are outlined, and their extension along the axis c, i n the structure of rutile TiO,.
.
.
440
1
Fernando Scordari
structure is formed with a ratio of M:X = 4:8, as seen in the compounds Li20, Na20, K 2 0 , Rb20. Such a structure can be described as a CCP having all its tetrahedral holes occupied by monovalent cations. Note that in this case an HCP would be impossible, since the tretahedra would have to share faces, thus bringing the alkaline cations into close contact.
MX3 and M2X3 structures Bayerite and gibbsite, two polymorphic modifications of the compound Al(OH),, have MX, stoichiometry: they are both monoclinic with space groups C2/m and P2,ln respectively. Their structure (M:X = 6:2) is based on a layer similar to that of brucite. As can be seen from their stoichiometry, only one third of their octahedral holes are occupied, while the presence of OH groups indicates that their structure is layered like that of brucite. It is useful to double the stoichiometric formula: A12(OH),, and then to divide it into (OH); and Al2(OH);+. This expedient makes it easy to illustrate that there is a layer of unoccupied octahedra, which overlies another layer of octahedra twothirds occupied (Fig. 6.27(a)). An HCP type packing, with partially occupied, similarly orientated octahedral layers, alternating with empty octahedral layers results[391(bayerite, Fig. 6.27(b)). Leaving the relative positions of the cations out of consideration, in gibbsite, two occupied octahedral layers, like that shown in Fig. 6.27(a), are related by a plane of symmetry m which passes through the empty layer, so the same orientation of the layers recurs every other full layer (Fig. 6.27(c)). In actual fact the arrangement of A13+ cations does not allow for the plane m. Moreover, the substitution of 3 ~ g 4 ~ 2A13+ + 0,reduces the symmetry from trigonal (brucite) to monoclinic (bayerite and gibbsite). Both corundum (aA1203) and haematite (aFe203)have an M:X = 6:4 ratio, are rhombohedra1 with space group R ~ C Their . structures are characterized by a bayeritetype layer (Fig. 6.27(a)). It can be deduced from their stoichiometry that the octahedral holes are two thirds occupied. The structure of corundum can be obtained translating the bayerite layers by 113 (01 + a,). Perpendicularly to the bayeritetype layers the octahedral holes are ordered so that one empty octahedron is followed by two occupied octahedra which share a face. This explains not only the type of lattice, R, but also why the structure is stable. In fact the translation has the same effect as a rotation of the bayerite type layer through 120" would have with the consequent turning of the empty octahedral holes around a threefold
+
Fig. 6.27. (a) The layer characteristic of bayerite, AI(OH),; 1 indicates the mesh of bayerite, 2 that of corundum, aAl,O, whose structure is based on the same type of layer; (b) shows the structure of bayerite seen in the direction (010) as a sequence of alternately empty and occupied OL; (c) shows the sequence of OL typical of gibbsite, ANOH),.
OLB
1

C
OLA
OLB
I
I
I
Ionic crystals
1
441
screw axis. As far as stability is concerned, it is indeed the presence of the two empty octahedra, above and below the two occupied octahedra, that allows the two cations which populate them to move as far apart as possible. This improves the shielding, since the three oxygens shared are brought closer together, and thus reduces the electrostatic repulsion. The octahedra occupied by ~ l and ~ Fe3+ + are, in fact, rather distorted, having three longer distances and three shorter ones (Al0 = 1.86(x3) and 1.97 A(x3); Fe0 = 1.95(x3) and 2.21 A(x3)).
A,B,X,
structures
A very large number of compounds of great geological, crystallochemical, and applicative interest belong to this class. Some structures are illustrated below in which A and B represent monovalent to pentavalent metals and X is generally oxygen. llmenite (FeTiO,) and perovskite (CaTiO,) have ABX, stoichiometry. Ilmenite is isostructural with corundum, in which the cations are substituted according to the following scheme: 2A13+ (Fez+,~ g ' + ) ~ i ~ Such + . cations are ordered so that the octahedra of one layer are occupied by Fez+ and those of the next layer are occupied by Ti4+. It follows that two contiguous octahedra belonging to two adjacent layers are occupied by ~ e ' + and by ~ i ~so+that , the average valence (+3) of the two cations remains the same as that of the two corresponding cations in corundum. The specialization of the octahedral sites, half occupied only by Fez+ and half only by Ti4+,determines the disappearance of the glide c. Thus the space group R ~ C (corundum) becomes R3. A number of structures with various valences (shown in brackets) have a similar structure to ilmenite, including LiNbO,(+ 1, +5); MgTiO,, FeTi03(+2, $4); Mn(Fe, Sb)03, aAlZO3, aFez03 (the last two can be considered as particular cases of the structure of ilmenite) and Ti203, V203(+3, +3). In these compounds A and B have similar ionic radii ( ( r e ) = 0.65 A), therefore they occupy two octahedral holes of a CCP type packing. If, however, the cation is too large to fit into the octahedral holes, another type of structure with the same stoichiometry is formed (perovskite type). Thus, as Na+, K+, Ca2+,Sr2+,Ba2+,pb2+,etc., cations have an ionic radius equal to that of the anions when have CN = 12, they can substitute an X (0', F) anion. If one quarter of the X anions are substituted by such cations, then a particular type of CCP is obtained, a representative cell of which is illustrated in Fig. 6.28.
+
Fig. 6.28. Contents of an elementary cell of perovskite, CaTiO,. Note the coordination 12 of the ca2+ (hatched circles). The octahedral holes not occupied by caZ+ are marked X.
442
( Fernando Scordari
Fig. 8.29. (a) A projection, parallel to a,, of the elementary cell of spinel (MgAI,O,). The number next to the circles indicate the heights ( ~ 1 1 8 ) respectively of M ~ (odd) ~ + AI,+ (even, above the circles) and 0' (even pairs, below the circles). In (b) the contents of two subcells T and 0, which alternate regularly along, a,, a,, and a, giving rise to the spinel cell (illustrated in (c)), are outlined.
Ti4+ occupies one quarter of the octahedral holes available, i.e. only of those which have no direct contact with the larger cations. Compounds with a similar structure to that of perovskite include: NaNb03(+l, + S ) ; BaZr03(+2, +4); LaA103, LaFe03(+3, +3). The term spinels is used to indicate a considerable group of compounds with a similar structure, having the general formula AB2X4.This term is the extension to the group of the name of spinel (MgA120,), a mineral characterized by a slightly distorted CCP type structure. In normal spinels the cations marked A occupy tetrahedral holes (t), while those marked B occupy octahedral holes (0). The range of their radii depends not only on the tolerance of the structure, but also on the type of anion: X = 0', s*, se2, Te2, F, CN. According to the stoichiometry of spinels one eighth of the tetrahedral and half of the octahedral holes of an FCC cell should be occupied. In actual fact, such an arrangement would result in an unstable structure because of the need for occupied tetrahedral and octahedral holes to share faces. However, the structure becomes stable if two FCC subcells share, so to speak, their work: essentially one gives space to cations in coordination of 4(T), while the other only gives space to those in coordinations of 6(0) (see Fig. 6.29). In this case, in fact, the occupied tetrahedra and octahedra share vertices. This leads to the succession of cells TOT . . . along a l , a2, and a3, which in turn leads to a cell consisting of eight subcells with a total atomic content of A,B1,X3,. In this section only spinels with AB204will be considered. Type B cations can have a charge of +1, +2, or +3, while type A cations can have a corresponding charge of +6, +4, or $2 V.U.(valence unit). Thus from the point of view of valence, there are three possible types of spinel: (+6, +I), (+4, +2), (+2, +3). In inverse or antispinels, the type A cations occupy octahedral sites, whereas the type B cations are equally divided between octahedral and
Ionic crystals ( 443 tetrahedral sites. Consequently, the formula that describes normal spinels is (A),(B2),04 while that of inverse spinels is (B),(AB),O,. The two formulae represent extreme cases, since spinels of various degrees of inversion commonly exist. The following general formula for spinels can be given (A,,B,),(A,B2,),04, where i (inversion parameter) represents the fraction of A cations which are hexacoordinated. The choice of configuration, inverse or normal, and the degree of inversion depend on a delicate network of factors[61which can be summarized as follows: (1) temperature; (2) Madelung's constant and u parameter; (3) orderdisorder phenomena; (4) ionic radius; (5) charge; (6) CFSE; (7) polarization. If we establish the origin of the cell of spinels (space group ~ d 3 m at ) 43m, the equivalent 32 positions of the anions in an ideal packing, can be generated, starting with the atomic coordinates u, u, u (u = 318). Therefore the distortion of the actual packing can be measured by means of the u parameter. In order to illustrate better the structure of spinels, Fig. 6.29 was obtained by translating the origin of the cell by 118, 118, 118. Only (+2, +3) spinels will be analysed here. Factor (1). Recently, by means of neutron and Xray diffraction, the range (750850 "C according to some authors,[401600700 "C according to others[411)within which transition of the orderdisorder type occurs in the spinel MgA1204 has been specified. Figure 6.30(a) shows the effect of temperatureL411on the u parameter. u falls rapidly in the area within the broken lines, which corresponds to the transition normal + inverse spinel. However, it would seem that this transition is not complete, since it stops at 1200 "C, when i = 0.30. Factors (2) and (3) can be examined together. It has already been shown the Madelung's constant, AM, depends on the lattice geometry. The distortion of the lattice, which can be measured by means of u, influences the value of AM;moreover, since AM and U, are in direct proportion (see eqn (6.17)), the configuration with the highest AM value is favoured. The trend of AMplotted against u is illustrated in Fig. 6.30(b) for normal spinels (ns) , ordered inverse spinels (ois) , and disordered inverse spinels (dis) . From the figure it can be seen that for u > 0.379, AM(ns)> A,(dis) and that for u >0.381, AM(ns)>AM(ois). This is the main reason why almost all ($2, $3) spinels with u > 0.381 are normal. Factors (4) and (5) counteract one another. Factor (4) indicates that the smallest cations ought to occupy the tetrahedral sites, while the largest + cations are very often ought to occupy the octahedral sites. Since B ~ type smaller than type cations, this means that (+2, +3) spinels should be prevalently inverse. Experience, however, shows that exactly the opposite is true. Factor (5) takes into account the Pauling7s second rule, according to which the charge of the cation is more or less neutralized by the anions of the first coordination shell. Consequently, the cations with the highest charges (B3+) would tend to occupy the sites with the highest coordination number (in this case octahedral sites), thus favouring normal (+2, +3) spinels. Factor (6) considers the effects of the crystal field on transition metals. The latter, due to the weak crystal field of the oxygens, almost all adopt highspin configurations in spinels. It should be remembered that cations with a do or d5 electronic configuration (spherosymmetrical) include: Mn2+,
.375
380
.385
U
(b) Fig. 6.30. Shows the trend of the distortion parameter, u,versus the ternDerature ("C) for MgAI,O,. Note the rapid fall bf u (at 650 "C) which indicates the rapid inversion of the spinel. (b) Illustrates the trend of the Madelung constant A, versus u. The abbreviations ns, ois, and dis indicate normal spinel, ordered inverse spinel, and disordered inverse spinel.

444
1
Fernando Scordari
~ e ~Zn2+, + , Ga3+. It is possible to predict accurately which type of spinel will occur, if the AM and the OSSE indications agree. If, on the other hand, they do not agree, one or other type of spinel may prevail, depending on the balance of all the factors involved. For example, (+2, +3) type spinels such as MgV204, MgCr204, MgMn204, are normal, since they have u = 0.385 (and thus AM favours ns); moreover, Mg2+ is spherosymmetrical and the OSSE definitely suggests that octahedral sites will be preferred by v 3 + , Cr3+, ~ n ~ + . Now let us consider the spinels NiMn204, NiFe204. They have respectively u = 0.383, 0.381, therefore there is a slight AM bias towards ns. On the other hand, the OSSE favours Ni2+ rather than Mn3+ while for Fe3+ it is nil. Hence spinels with highest degree of inversion are the result. Finally the minerals magnesioferrite (MgFe204), magnetite (FeFe204), and trevorite (NiFe204) have respectively i = 0.90, 1.0, 1.0. In the first compound the OSSE of Fe3+ is zero and AM= 0.382, so there is no clear indication. However, Fe3+ tends to prefer tetrahedral sites, owing not only to the polarization (factor (7)), but also to its relatively small ionic radius (re(Fe3+)= 0.645, rc(Mg2+)= 0.72 A). In the other two compounds AMdoes not give clear indications, while the OSSE of Fe2+ and Ni2+ decidedly favour these two cations for octahedral sites, therefore the degree of inversion is maximum. t Factor (7) can play a decisive role when the other factors counteract each other. Therefore, if AM does not clearly favour either of the two configurations, polarization can play an important part either strengthening, or even overturning the A, indications. The effects of polarization are particularly noticeable where ~ e ~Ga3+, + , and 1n3+ are concerned. For example, in jakobsite (MnFe204) the AM favours a normal configuration (u = 0.385)) the OSSE = 0 both for and ~ e ~The + .effect of polarization is to partially invert the AMindications, giving rise to a spinel with i = 0.20. For other interesting aspects concerning the question of spinels see, for example, Greenwood,[6]~ u r n s , [ ' ~ ]v a n s , [ ~ ~ ] and ~ t t o n e l l o . [ ~ ~ ] Olivines are minerals with a general formula M2[Si04] where M represents various cations, which are essentially bivalent and hexacoordinated. Belonging to the olivine group are: forsterite Mg2[Si04],fayalite Fe2[Si04], tephroite Mn2[Si04], monticellite CaMg[SiO,], kirschsteinite CaFe[SiO,], glaucochroite CaMn[SiO,], knebelite MnFe[Si04]. In particular, olivine is a solid solution of forsterite and fayalite (Mg,, Fe,,) [SiO,], while in the Caolivines pairs of cations such as Ca2+ and Mg2+, Ca2+ and Fe2+, Ca2+ and Mn2+ occupy quite distinct sites. Referring to the two minerals forsterite and fayalite, the composition given above can also be given as Fo,Fal,, or simply Fox. Olivine is found in large quantities in the earth's lower crust, and it is generally supposed to be particularly abundant in the earth's upper mantle. The ideal structure of aolivine can be described as HCP with (according
t Incidentally, the inversion and the complete disorder between Fez' and Fe3+ in octahedral sites make magnetite an excellent conductor of electricity. This is due to the ease with which ~ e ' +and ~e~~ exchange electrons. Below 153 "C the Fez+ cations become ordered, reducing noticeably the capacity of magnetite to conduct electricity.
Ionic crystals
to its stoichiometry) half of its octahedral holes occupied by Fe2+ or Mg2+ and one eighth of its tetrahedral sites occupied by Si4+.The closest packed layers are parallel to (100) and the octahedral holes are occupied in such a way that chains of occupied and empty octahedra form zigzags along the c axis (Fig. 6.31). Two layers similar to that shown in Fig. 6.31, at a distance of a12 are translated by b/2, so that occupied octahedra overlie empty octahedra. In this way, in fact, as the Pauling's third rule predicts, it is not possible for the occupied octahedra to share faces. As pressure increases forsterite["I becomes unstable and transforms itself giving rise first to a spinel type structure (/3 and y), then to an ilmenite type structure and finally, when P > 200 kbar, to two structures: a perovskite type structure, and periclase as follows: 2Mg2Si04, 2MgSi03 + 2Mg0.
O n the classification of silicates First of all, can the structures of silicates be described by means of closest packings? The answer to this is not always affirmative: let us examine why this is so. If AEN(Si0) = 1.72, then eqn (6.2) predicts that between the silicon and the oxygen interactions will be established, with a percentage of covalent bonds more or less equal to that of the ionic bonds. As far as the coordination of the Si4+ is concerned, the covalent bond necessitates the formation of four hybrid sp3 orbitals, or in other words, the angular probability of finding an electron is greatest in the direction which connects the centre of a regular tetrahedron to its vertices (these directions form angles of 109'28' between each other). On the other hand, the rule of radius ratio predicts a CN = 4 for the ionic bond. Experimentally Si4+ is nearly always found to be tetracoordinated, but occasionally hexacoordinated Si4+ has also been observed. The cations which most frequently occur in the structures of silicates are: A13+, Fe3+, ~ e ~Mg2+, + , Mn2+, Ca2+, Nai, K+. Some of these, positioned around the theoretical limit of two possible coordinations, can form various ~ =' 0.38, therefore CN = 4, 6. polyhedra with the anions: e.g. for ~ 1 p, Other cations are of a size to prefer coordinations of 4, 6, 8, or even 12. It has already been mentioned that the structure of olivine can be described as HCP, even if a rather distorted one (c, = 0.60). The distortion is due to the fact that octahedra and tetrahedra share edges. In fact the distortion depends both on the difference in length between the 00 distances of the tetrahedron [SiO4I4 (2.6A) compared to that of the octahedron(z2.8 A), and on the electrostatic repulsion. Other structures with characteristics less similar to those of closest packings are also possible in silicates. Figure 6.32 illustrates an octahedral layer (OL) and two diversely orientated tetrahedral layers (TL, and TL,), which are fitted one into another to form a double layer of spheres (anions), typical of closest packing. This complex layer will be referred to as OTL. There are several ways of filling the holes of a closepacked structure. Let us consider two borderline events. Firstly, both the tetrahedral and octahedral holes of the layer OTL shown in Fig. 6.32 could be filled, and of each successive layer. Secondly, the octahedra of one layer (OTL,) and the
1
445
,,,
s,,l, a ,aver of distoned octahedra tyflcal of the structure of olivine, (Mg, Fe),[SiO I. The f
d by ~ g "Or Fez+
446
1
Fernando Scordari
Fig. 6.32. A layer of octahedra (OL) and two diversely orientated layers of tetrahedra (TL, and TL,), whose polyhedra form the holes characteristic of a double compact layer of equal spheres.
tetrahedra of the overlying layer (OTL,) could be filled alternately, in accordance with the stoichiometric constraints. The configurations relative to the first hypothesis imply structures of higher potential energy generally, due either to the more frequent sharing of geometric elements, or to other factors. For example, if there is not sufficient oxygen to form isolated [si0,I4 groups the tetrahedra would tend to condense. The ideal closest packing would require an ~ i  0  ~angle i of 109"28', but, owing to the considerable percentage of ionic bond between silicon and oxygen, the two Si4+ atoms tend to move away from each other (thus improving the shielding) forming angles which on average are of 140". If, however, one of the two Si4+ is substituted by A13+, then ~ 1  0  s i angles well below 140" (118") can be formed. Intermediate figures (e.g. fully filled octahedral and partly filled tetrahedral holes) lead to structures with potential energy half way between those of the two configurations hypothesized above. Bearing in mind what has been said, the structure of phlogopite, KMg,[AlSi3O,,](OH), will now be analysed. Supposing that it conformed to closest packing (c, = 0.56) its stoichiometry would indicate that one quarter of the octahedral holes are occupied by Mg2+ and one sixth of the tetrahedral holes are occupied by A13+ or Si4+.In actual fact, of four successive OTL, one is completely filled by Mg2+ (octahedral holes), two immediately above and below each have one third of the tetrahedral holes filled, while the last layer contains K+ cations (CN = 12) equal in number to the A13+ which substitute Si4+. To summarize, in phlogopite a layer of tetrahedra TL, is followed by a layer of octahedra OL, which is followed by another tetrahedral layer TL,, and finally there is a layer of K+ ions which connects two tetrahedral layers TL1 and TL,. Figure 6.33(a) represents one of the two tetrahedral layers (TL,). Every
Fig. 6.33. A layer of tetrahedra is represented in (a) (TL,). The black tetrahedra are occupied by si4+,while the white ones are empty. This determines, as can be seen in (b), the reorganization of the layer in rings with an OHgroup at the centre, and also, as shown in (c), the relationship between the ring of tetrahedra and a group of octahedra of an OL typical of phlogopite, KM,,[AISi,O,,I(OH),.
Ionic crystals
tetrahedron shares three vertices with similar tetrahedra, as shown in the figure, so that every vertex is shared by three tetrahedra. If three of the contiguous tetrahedra (e.g. 5, 6, 7 of Fig. 6.33(a)) were occupied by cations with average valence >3, the Pauling's second rule would be infringed. In fact, supposing that they are occupied by either 3Si4+, or 2si4+ AP+, or even Si4+ 2A13+,the shared oxygen still received respectively 3, 2.75, 2.50 v.u., far higher than the necessary value of 2. Therefore, with respect to closest packing, there are two important differences. The first is that the group of seven tetrahedra, shown in Fig. 6.33(a), gives rise to a ring of six tetrahedra (Fig. 6.33(b)), leaving an OHgroup in the centre instead of the oxygen which acted as the vertex of the empty tetrahedron (7 of Fig. 6.33(a)). This pseudohexagonal ring fits well into the overlying octahedral layer (Fig. 6.33(c)), and allows a ~ i  0  ~ angle i of about 140". The layer of oxygens which constitutes the base of the ringforming tetrahedra has c, =0.76, while the layer of oxygens to which the vertices of the tetrahedra and the OH group contribute has c, = 0.88. The latter of these two values is nearer to the theoretical value, c, = 0.91. The other difference is represented by the anions around K f . This cation, unlike the Ca2+ of perovskite, is not surrounded by six anions in the plane (OOl), which is characterized by K+ cations; instead the twelve coordination is achieved by six oxygens belonging to the ring of tetrahedra of the overlying layer (TL,) and six belonging to that of the underlying layer (TL). The examples examined above refer to silicates with hexacoordinated cations which are relatively small, such as A13+, M ~ ' + ,Fez+, Fe3+. For such cations the edge of the octahedron (2.8 A) is similar in length to that of the tetrahedron (2.6 A), as the structure of olivine demonstrates, in which they are shared. If larger cations are present, such as Na+ and Ca2+, they adopt coordinations with CN 3 6. If CN > 6, then the holes made available by closest packing do not fit the requirements of the cation. If CN = 6, octahedra with edges >3.8 A are formed, edges considerably longer than the edges of the tetrahedra. In this case a pair of tetrahedra inscribing a trigonal prism of side 4.1 A is often necessary. Such a prism is incongruous with the polyhedra of a closest packed OTL. As a result, in order to describe in rational terms the structures of silicates, it is necessary to abandon the mechanical model used so far. It is helpful to make use of particular coordination polyhedra, the type of links which are established between them, and other parameters.
+
+
Liebau's crystallochemical classification The simplicity of a classification system depends basically on the number of parameters on which it is based. For the silicates this number was originally low (Bragg 1930) and has gradually increased as our knowledge of atomic structures has grown ( ~ o l t a i , [~~i ~e b] a u [ * , ~ ~ ~ ) . The crystallochemical classification proposed by takes into account the close relationships which exist between structure, chemical composition, thermodynamic stability, and reactivity in silicates. Given the strong prevalence of structures with Si4+ in tetrahedral coordinations over
1
447
448 ( Fernando Scordari
Si4+ in octahedral coordinations, attention will be given here only to the former, while Liebau considers both. Since the silicon can be substituted by other cations such as A13+ and to a lesser extent by p5+,Ge4+,Fe3+, Be2+, the tetrahedron [ ~ i 0 ~will ]  be ~ represented more generally as [TO4]below. The first problem to be solved is that of establishing which tetrahedra can reasonably be considered as part of the silicate anion. Liebau proposes the following criterion: 'If, under certain thermodynamic conditions, an element replaces some of the silicon atoms in a given silicate crystal structure so that the crystallographic positions are statistically occupied by silicon and the other cation, then this cation is recognized as part of the silicate ion7. For example, two phases of potassium feldspar, KAlSi308, known as sanidine hT (high temperature) and microcline 1T (low temperature) are similar since they have A13+ and Si4+ in tetrahedral coordination, but differ in that the two cations show different degrees of disorder. This disorder is maximum in the first phase, K[(A1Si,)08] while it is minimum in the second, KAl[Si308], since here the tetrahedral sites tend to be completely occupied by either A13+ or si4+. These two phases are the end members of a series characterized by different degrees of ~ l ~ + / disorder ~ i ~ +and they are an example of the phenomenon known in thermodynamics as secondorder phase transition. As the temperature rises the feldspar passes from one phase to the other as the degree of Al/Si disorder varies, without the first phase being destroyed (in this case it would be a firstorder phase transition). For this reason, in accordance with Liebau, the formula for fully ordered microcline 1T is not KAl[Si308], but is similar to that of sanidine hT, i.e. K[A1Si,08]. It follows that, assuming [A1Si308]is the building unit, both phases belong to socalled framework silicates. Noting that Si0 bonds are generally stronger than M0 bonds (where M is a cation other than silicon) the crystallochemical classification of silicates takes into account the various possible modes of condensation of the tetrahedra [TO,]. First of all, the number of polyhedra which are linked to a given polyhedron by vertices, edges, or faces is defined as s (connectedness). When these polyhedra are tetrahedra [TO,] vertices are shared, and since each tetrahedron has four vertices, s = 0, 1, 2, 3, 4. If the tetrahedron is isolated it is called singular (QO),if it shares one vertice it is called primary (Q1), two secondary (Q2), three tertiary (Q3), and four quaternary (Q4); concisely QS = QO,Q1, Q2, Q3, Q4. The parameters on which the crystallochemical classification of silicates is based are:
1. Nan= number of anion types in a silicate. Nan= 1, uniformanion silicates; Nan> 1, mixedanion silicates. 2. CN = coordination number. In naturally occurring compounds only tetrahedra [TO,] and exceptionally octahedra [TO6], are present. 3. L = linkedness, type of link. L = 0, 1, 2, 3: for L = 0 the tetrahedron is isolated, for L = 1, 2, 3 the tetrahedron shares respectively one vertex, one edge, one face with a similar tetrahedron. In Fig. 6.22 (first row) the relationships between two tetrahedra for L = 1, 2, 3 are shown. 4. B = branchedness, type of ramification. The tetrahedra [TO,] can be condensed linearly (see Fig. 6.34), giving rise to limited groups, single
Ionic crystals ( 449
.b (4
(b)
(c)
(d)
Fig. 6.34. Some unbranched fundamental anions (u6f.a.); (a) a pair of tetrahedra, (b) an unbranched group of three tetrahedra, (c) a single unbranched chain, (d) a single unbranched ring.
chains and rings. They are characterized by tetrahedra with s G 2 and constitute the socalled unbranched fundamental anions (uBf.a.1. Complex anions of the same type (uBc.a.) can result from the condensation of uBf.a. Branched fundamental anions (brf.a.) can also
be obtained by condensing tetrahedra. They include tetrahedra with l S s 6 4 (Fig. 6.35). By condensing brf.a., brc.a. can be obtained. Branched anions can be divided into openbranched (oB) or loopbranched (1B) ones. In the first case, one or more tetrahedra constitute a sort of 'branch' which is joined to the nonbranched anions by means of a single geometric element (vertex, edge, or face). In the second case, more than one element is shared, e.g. two vertices (see Fig. 6.35). The condensation of more than one fundamental anion generates the following types of anions (see Fig. 6.36): uB f.a. + o B f.a. = hB c.a. (h =hybrid branched c.a.) oB f.a. + IB f.a. = olB c.a. (mixedbranched c.a. combination of open loopbranched anions)
+
In conclusion the branchedness (B) of silicates can be uB or br (unbranched or branched); while branching can be of various type: oB, IB, olB, hB. 5. M = multiplicity, i.e. the finite number of tetrahedra that are linearly linked in a 'short chain' of tetrahedra, or the number of rings, single
Fig. 6.35. Some branched fundamental anions (6rf.a.). The branches can consist of one or more tetrahedra (dotted). The figure illustrates: (a) oB triple tetahedron; (b) and (c) oBsingle rings; (d) oBsingle chain; (e) IBsingle chain; (f) olBsingle chain.
450
1
Fernando Scordari
Fig. 6.36. Fundamental anions (f.a.)and complex anions (c.a.1: ( a ) uBf.a., (b) 0Bf.a.. ( c ) 1Bf.a.. ( d ) uBc.a., ( e ) 0Bc.a.. (f) IBc.a., (g) hB c.a., (h) 0Bc.a.. ( i ) IBc.a., (j) hBc.a., (k) 01Bc.a.. (I) h6c.a.
(i) chains, or single layers linked to a complex ring, chain, or layer respectively; rarely is M 5. The condensation of groups of connected tetrahedra (i.e. multiple tetrehedra), rings, single chains, or single layers does not alter the dimensions of the fundamental silicate anions which are involved in the condensation.
6. D =dimensionality. The silicate anions can have the following extensions: finite (D = 0), infinite in one (D = I), two (D = 2), or three (D = 3) directions. When D = 0, the symbols t and r are used respectively to indicate groups of tetrahedra (terminated anions), and cyclic anions (rings). 7. P or Pr = periodicity of the chain (P) or ring (P'). Silicate anions with D = 1, 2, 3 are based on fundamental chains of tetrahedra. The parameter P expresses the number of tetrahedra which determines the repetition period of an unbranched chain (if a branched chain is considered the tetrahedra which constitute the branches should be left out). Figure 6.37 illustrates some fundamental chains of different periodicity. If the anions are cyclic the symbol Pr, which expresses the periodicity of a ring (i.e. the number of tetrahedra within a single ring) is used, excluding, therefore any branches. In order to avoid confusion, when choosing which fundamental chain is characteristic to a silicate with D = 1, 2, 3, it is necessary to take into account certain rules: (a) Fundamental chains with lowest periodicity running parallel to the
Ionic crystals
1
451
Fig. 6.37. (a), (c), and (el illustrate unbranched chains, while (b), (d),(f), (g), and (h) illustrate branched chains. The following pairs have the same periodicity: for (a) and (b) P = 2, for (c) and (d) P = 3, for (e) and (f) P = 4, for (g) and (h) P=5.
direction of the shortest identity period within the silicate anion are chosen. If rule (a) is satisfied by more than one chain, the fundamental chains are chosen such that their number is lowest. Once rules (a) and (b) have been satisfied, the third rule indicates the following order of preference (for fundamental chains): unbranched > loopbranched > openbranched > mixedbranched > hybrid (for > read 'is preferred to'). order in which the various parameters have been presented represents the classification hierarchy: superclass (N,,), classes (CN), subclasses ( L ) , branches ( B ) , orders ( M ) , groups (D), subgroups (r or t), families (P, Pr). If there are a number of silicates with the same type of silicate anion, i.e. silicates belonging to the same family further subdivisions can be made. The following criteria are particularly important: (1) the Si:O atomic ratio of the silicate anions;
(2) the degree of stretching of a chain. As far as criterion (1) is concerned, it should be noted that two or more rings, or two or more single chains having P > 1, can join together via all or
452
1
Fernando Scordari only part of their tetrahedra. As a result, complex anions with various Si:O ratios are generated, depending on the portion of the tetrahedra involved. As far as criterion (2) is concerned, Liebau proposes that the degree of stretching should be measured by means of the stretching factor (A), which can be obtained as follows:
where I, is the identity period of the chain, 1, is the length of the edge of the tetrahedron, both in A, and P is the periodicity of the chain (the number of tetrahedra needed to identify the period). Since amongst all the silicates so far discovered shattuckite, C U ~ [ S ~ , ~ ~ ] (has ~ Hthe ) , ,most stretched chain, it is taken here as a point of reference. From it the value 1, = 2.7 A can be obtained (equal to half of the repetition period of the chain, which is two tetrahedra [Si04]4). Thus for shattuckite f, = 5.40 A12 X 2.70 A = 1.00 while for enstatite, Mg2[Si206], (I, = 5.21 A, P = 2) f, = 0.956 and for alamosite, Pb,,[Si,20,6], (I, = 19.63 A, P = 12) f, = 0.606. The crystallochemical classification presents the same periodicity characteristics as the periodic system of the elements, so that, for example, by gradual condensation of [TO4] tetrahedra in a linear way, uB anions can be generated that are linked only by means of vertices in the following way: (1) for D = 0 the number of tetrahedra that can be condensed linearly increases as M increases, so that for M , w, D i. 1; in which case a single uB chain will result; (2) for D = 1 the number of chains increases with M, and for M D + 2, thus forming a single uB layer;
w,
(3) when single layers are condensed and for M , w, D + 3, a threedimensional building of tetrahedra, i.e. uB framework is obtained. By varying M and D the whole of Table 6.8 can be obtained, which lists Table 6.8. Chemical and mineralogical (in round brackets) nomenclature of silicates
D= 0
D= 0
M=l
M=2
M=3
Oligosilicates
Monosilicates
Disilicates
Trisilicates
(1
(Nesosilicates)
Cyclosilicates
Monocyclosilicates
(Sorosilicates) Dicyclosilicates
( D=1
Polysilicates
(
I
(1
I
Phyllosilicates
Monopolysilicates
(
Dipolysilicates
Tectosilicates
(
Tripolysilicates
I
...
(Inosilicates) Monophyllosilicates
Diphyllosilicates (Phyllosilicates)
D=3
...
Tricyclosilicates
(Cyclosilicates)
(1
D =2
... . ..
Tectosilicates (Tectosilicates)
I
Triphyllosilicates
...
'
1 I
Ionic crystals
the chemical and mineralogical (in round brackets) nomenclature of silicates.
Structural formulae A structural formula should contain the largest possible amount of information and therefore should include the parameters used in crystallochemical classification. Some of the parameters CN and P are best used only when there is some perplexity: the first is written in square brackets as a righthanded superscript to the cation, while the second is written without brackets as lefthanded supercrript to the cation. Other parameters, Nanand L, can be deduced directly from the structural formula. Therefore a structural formula containing the essential parameters is as follows:
M, indicates cations which do not belong to the silicate anion; the meaning of the other symbols has already been given. For D = 0 the interpretation of the symbol is not unequivocal and can therefore be substituted by r or t, depending on whether the silicate anion is cyclic or not. For D = 1, 2, 3 the symbols L, 2, 2 indicate clearly that the silicate anions are respectively chains, layers, and threedimensional framework of tetrahedra. Sometimes it is useful to complement the formula by the following suffixes: (IT), (mT), (hT), (lP), (mP), (hP). They indicate that the phase described by the formula is of low (l), medium (m), or high (h) temperature (T) and/or pressure (P). Some examples: A @ A ~ [{OB, ~ ] 3t) [Si50,,](OH, F),,04Cl
zunyite
The bracketed righthand superscripts to A13+, indicate the two coordinations of the A13+ in the structure of zunyite. Since there are no indications for Si4+, it is implicit that CN = 4. The symbols in curly brackets indicate that the silicate anion consists of a group of openbranched tetrahedra {oB), three of which determine the multiplicity M = 3 (see Fig. 6.3.5(a)). The content of the square brackets indicates that the group consists of five tetrahedra and that therefore the 'branches' of the silicate anion are the remaining two tetrahedra [SiO4I4. Ca2A12Sn{oB,l r ) [ 4 S i 6 0 1 , ] ( O ~ ) 2 . 2 ~ 2eakerite 0 The structural formula informs us that the silicate anion is openbranched {oB) and that it is a single ring {lr). The content of the square brackets indicates that the unbranched part consists of four tetrahedra [SiO4I4 and that the 'branches' consist of two tetrahedra [SiO4I4 (see Fig. 6.35(b)). For other structural formulae and for illustrations of the silicate anions described therein, see Figs. 6.386.42.
Relationship between classification parameters and properties of the cations The properties of nontetrahedral cations, in particular, electronegativity and valence, have a strong influence on the structure of silicate anions.[451 Here, the direct influence of the nontetrahedral cations on the parameters which govern crystallochemical classification will be examined.
1
453
454
1
Fernando Scordari
Fig. 6.38. Ideal configurations of certain silicate anions and structural formulae: (a) olivine (Mg, Fe), {US, lt}[SiO,]; (b) ilvaite CaFe,(Fe, Mn){uB, 2t}[Si,O,IO(OH); (c) benitoite BaTi{uB, lr)lSi3091; (d) taramellite Ba,(Fe3+, Ti),B,{uB, 1r}[Si4O,,I,O,CIX; (e) tourmaline XY Z B {US, 1r} [Si,0,9~0,(~,+0H, F), , , Fe , where x = ~ a ;af2+; Y = ~ i +Mg ~ n ' + ,~ e ~ A13+; ', Z = A13+, M ~ ' + ;(f) steacyite K,,(Na. Ca),,Th,,{uB,2r}[ S,O i ,I the fundamental anion is dotted.
Fig. 6.39. Single chains with different periodicity (P), structural formulae and stretching factors (f,) for the following minerals: (a) a hypothetical mineral, M(uB,I L}[s~o,I, f, = 1; (b)enstatite, Mg,{uB, 1 ,}[S1,0,1, f, = 0.965; (c) wollastonite, ca,{u~, 1 L)[s.,I 0 I,f, = 0.904; (d) krauskopfiie, H,Ba,{uB, ,}[Si4O,,I~4H,O, fs=0.783; (e) rhodonite, (Mn, Ca),{uB, 1 ~}[s,~,o,,], f, = 0.906; (f) stokesite, Ca,Sn,{uB, 1 ,)[S1,0,,1~4H,0. f, = 0.718; (g) pyroxmangite, (Fe,Ca, Mn),{uB, 1 ~}[S~,O,,I, f,= 0.923; (h) f, = 0.606. The alarnosite, Pb,,{uB, 1 ~}[s~,,o,,], periodicity (P) is as the silicon stoichiometric coefficient.
1. CN: the coordination number of silicon depends in particular on the EN of the anions (X) of the first coordination shell. If the anions are strongly electronegative, as is fluorine (see Table 6.2), the tendency CN > 4 is increased (SiF,), if weakly electronegative tetrahedral groups are formed. In the case of oxygen, the EN is lower than that of fluorine, but is still high. Therefore the silicon of both natural and artificial compounds is found both in tetrahedral or octahedral (a few cases) coordinations. The Si0 type of bond is influenced by the cations (M) belonging to the second coordination shell of the silicon: the highly electronegative M cations give a more ionic character to the Si0 bond. This, obviously, affects the CN (CN > 4 is slightly favoured), the effective charge of the silicon (positive), and, when CN = 4 the overall charge of the tetrahedra (negative). The effects of repulsion between the silicate anions can be evaluated by means of the distortions which can be seen above all in the S i  o  ~ i bond angles, but also to a lesser extent in other parameters.
2. L: the stability of a silicate anion decreases as L increases, an inverse tendency would violate Pauling's third rule. This explains why no silicate
Ionic crystals
1
455
Fig. 6.40. Double chains in which the fundamental anion is hatched, and the structural formulae of: (a) sillimanite, Alie'{u~,2 ~}['(AIs~o,)I(~T);(b) tremolite, ~ ~xonotlite, )2; Mg,Ca,{uB, 2 ~ } 1 2 ~ i 4 ~ l , 1 2 ( (c) Ca,{uB, 2 l}13si 0 (d) narsarsukite, 2 ~ } ? ~ / ~ h , ~ ] 0(d) , ; can also be Na,Ti,{uB, obtained by condensating the unbranched rings {US, lr}[Si,O,,l (dotted in figure) and the latter formula has tobe changed into Na,Ti,{uB, mr) I~S~,O,~IO,.
anions with CN = 4 are found with L > 1 (at present only one case has been found with L = 2). Highly electsonegative cations favour a higher degree of linkedness because the [SiOJ effective charge tends to be reduced. 3. B: branched silicate anions, in particular branched ring anions, are less stable than unbranched varieties, due Do the shwter average SiSi distances. If, however, cations with high EN are present, then the stability of such silicate anions is increased, since they attenuate the effective negative charge thus reducing the repulsion between the tetrahedra. The stabilizing effect of such cations decreases as D increases, because in such cases the effective charge of the tetrahedra [TO,] ako decreases. 4. M: the number of structures with increasing M falls drastically both in the oligosilicates and in the cyclosilicates, and in polysilicates and phyllosilicates. This is due to the decided increase in the potential energy of structures as M increases. To examine this phenomenon the differences in energy between linear groups of tetrahedra will be analysed. It should be borne in mind that the greater their distance from the tetrahedron which terminates the group, the less tmo contiguous tetrahedra will vary from the point of view of energy. For example two Q1 tetrahedra are similar from the point of view of energy because they each start and terminate a group. Two Q1 tetrahedra and one Q2, belonging to a group of three tetrahedra are very different from the point of view of energy, because the distance that separates Q2 from the external tetrahedron Q1 is only that of one tetrahedron. Finally, in a single unbranched chain every tetrahedron has practically the same energy as that next to it, since both are more or less at the same distance from the end tetrahedron. In contrast a linear group of tetrahedra could, from an energetic point of view, be regarded as being constituted by different structural units. To this the principle of parsimony is applied (see p. 436, Pauling's fifth rule), according to which the smaller the number of structural units a
Fig. 6.41. Single and double layers (the fundamental chain is hatched) and the structural formulae of: (a) muscovite, l ( ~ talc, ~), KAI,{uB, 1 ~ ) [ 2 ( ~ ~ ~ i , ) ~ l , and MgAuB, 1 _.l2si 0 NOH),; (b) apophyllite, KCa,{uB, 1 , } ~ ~ i , 0 , , l & ~ ~ 0 ~ ) ~ 8(c) ~~0; hexacelsian, Ba{uB, 2 ,}I (AISi)O,],(hT).
,
456
1
Fernando Scordari
structure is composed of, the more stable it is. This explains the uniform number reduction of the groups as M increases. What has been said above regarding linear groups can be extended to chains or layers, by considering the whole chain or the whole layer as a structural unit, instead of a tetrahedron.
5 . D: the general rule is that where there is a fixed Si0 ratio, the silicate anions tend to join together, in accordance with D+max. Though there are exceptions to this rule, it can be justified by the fact that condensation of the [siO4I4 tetrahedron results in a better local electrostatic valence balance, in accordance with Pauling7ssecond rule. 6: t, r: multiple tetrahedron silicate anions are more stable than cyclic ones. In fact, since the average Si4+Si4+ distances are greater for the former, the force of repulsion between Si4+ and Si4+is less.
(c) Fig. 6.41. (Continued)
7: P: the periodicity of a chain can be evaluated, in general, by means of the stretching factor f,. The higher this factor, the more the chain is stretched, and the lower is P. There are, however, important exceptions where P increases with f, (pyroxenoids and pyroxenes).
8. f,: this factor depends, in particular, on EN and on the average valence
( v ) of the cations. Strongly electropositive cations tend to increase the negative charge of the [TO4] groups; therefore the repulsive forces which act between these groups are greater and as a result f, + 1. Vice versa, strongly electronegative cations, by reducing the charge of the [TO4] groups, reduce f, and so P tends to increase. An increase in the ( v ) of the cations has a similar effect. In fact, when ( v ) is high, a greater number of oxygens of the chain must be involved in cationoxygen bonds. As a consequence f, is reduced and P increases. The ionic radius of the cation has more effect on the distortion of the polyhedra than on the periodicity P. The greater the difference between the silicon radius and that of the other cations, the greater this effect will be. 9. Nan: bearing in mind still the principle of parsimony, it can be stated that the number of the structural units, distinguished either chemically or geometrically, must be as small as possible. This explains why the vast majority of silicates have Nan= 1; only a few structures have Nan= 2 (e.g. okenite, Ca,,{uB, 2 ~)[3Si6016]{~B, 1 ~)[3Si6015]2.18H20) and there are no known crystal structures at present with Nan> 2; however in glasses, melts, etc. Nan> 2 is common. Silicates with mixed anions are favoured by cations with high EN. Fig. 6.42. Threedimensional buildings of [TO,] tetrahedra, and the structural formulae of: (a) (b) cristobalite, {uB, trid mite, {US, ~}[2~i,041; J' :}[ Si,04] (note the thickened fundamental chain and how in cristobalite the layers perpendicular to [ l l l ] are all orientated the same way, while in tridymite the same layers perpendicular to [00011are turned through 180" compared to one another); (c) orthoclase, K{IB ~ } [ 3 ( ~ ~ ~ i 3 ) ~The , l ( structure m ~ ) . of orthoclase is represented schematically. The letters U and D indicate the position of the [TO,] tetrahedra with one vertex pointing either up (U) or down (D); (d) the fundamental chain IS, on which the structure of orthoclase is based (the 'branch' consists of the dotted tetrahedra).
10. s: for a given Si:O ratio of the silicate anion, high EN cations favour a high s value.
Appendices 6.A Application of the concept of the packing coefficient (ci) In general, calculated packing coefficients almost never match the expected value (0.74). It is sometimes found that structures with lower c: ( ~ 0 . 6 0 )
Ionic crystals
conform to closest packing models whereas others with ci ( ~ 0 . 7 0 )depart from them. The main reason is that in fact ions are not hard spheres but charged, elastic, and polarizable entities. In addition the atoms are sometimes too bulky to be included in the octahedral holes of a closest packing scheme; in such cases the structure would not have the greatest economy of space, i.e. it would not be the closestpacked structure. Thus the ideal conditions demanded by the mechanical atomic model are in practice never achieved. In spite of this, the packing coefficient provides useful information, mostly for structures with a high degree of ionic bonding. Assuming, for oxygen, re = 1.40 A, packing coefficients are calculated for some compounds belonging to several classes of minerals with different ionic bondcharacter. The abbreviation c.p. shows those compounds which adopt a closepacked arrangement of anions, while 6 represents density.
Oxides Periclase [MgO] Rutile [TiOz] PTridymite [SiO,] Coesite [Si02] Stishovite [SiO,] Brucite [Mg(OH)2] Gibbsite [A1(OH)3] Ilmenite [FeTi03] Spinel [MgA120,]
Carbonates Aragonite [CaCO,] Calcite [CaC03] Alstonite [BaCa(CO,),] Ewaldite [Ba3Ca2(C03)5] Shortite [Na2Caz(C03)3] Tychite [NazMgz(C03)4(S04)] Gaylussite [Na2Ca(H20)5(C03)z]
ci= 0.61 (6 = 2.93) ci= 0.56, c.p. (6 = 2.71) ci= 0.51 ci= 0.55 ci= 0.53 ci= 0.55 ci= 0.51
(a Fig. 6.42. (Continued)
Borates Kotoite [Mg3(B03),] Tincalconite [NazB405(OH)4.3H20] Kernite [NazB406(OH)2~3H20] Borax [Na2B405(OH)4.8Hz0] Sinhalite [MgAl(BO,)] Aksaite [Mg(B304(0H)2)2.3H20] Gowerite [Ca(B304(OH)z)z~3H20]
ci= 0.67, C.P. ci= 0.55 ci= 0.53 ci= 0.53 ci= 0.76, c.p. ci= 0.44 ci= 0.42
Sulphates Baryte [BaSO,] ci= 0.53 ci= 0.50 Chlorothionite [K2Cu(S04)C12] Fibroferrite [Fe(OH)S04.5H20] ci= 0.53 Parabutlerite [Fe(OH)S042H20] ci= 0.60 Hohmannite [Fe(Hz0)4[(S04)20]~4HzO] ci= 0.58 Coquimbite [Fez(S04)]9H20 ci= 0.55
1
457
458
(
Fernando Scordari
Phosphates Triphylite [ ~ i ( ~ e ' Mn2+)P04] +, Heterosite [(Mn, Fe)P04] Hydroxylapatite [Ca,(OH)(PO,),] Brushite [CaHP04.2H20] Moraesite [Be2(OH)P04.4H20] Struvite [NH4MgP04.6H20]
Silicates Forsterite [Mg2Si04] Larsenite [PbZnSiO,] Monticellite [CaMgSiO,] Humite [Mg7(0H,F)&304),] Zircon [ZrSiO,] Grossular [Ca3Al2Si3OI2] Enstatite [Mg2Si206] Anthophyllite [Mg7Six022(OH)2] Pyrophyllite [A12Si40,,(OH)2] Orthoclase [KAISi,Ox] Some remarks concerning the relationships between the anion arrangement and the packing coefficient are helpful. The compound CaCO, crystallizes in two structures (polymorphs): calcite (c, = 0.56) and aragonite (c, = 0.61). Calcite can be described by means of a closepacked oxygen arrangement with & triangular and 4 octahedral sites filled respectively by C4+ and Ca2+. This packing is not the closest possible for CaC0, because Ca2+is surrounded by six oxygens, i.e. in this structure, calcium shows the lowest CN among those adopted (see Table 6.7). If pressure increases, a more compact structure (aragonite in which Ca2+ has CN = 9) originates; this structure no longer conforms td the closest packing model. The compound SiO, gives rise to several phases. Some of them are considered here, they are: (1) Ptridymite, stable between 870 and 1470 "C; (2) coesite, roughly stable from 30 to 100 kbar; and (3) stishovite, a very highpressure phase, stable above 100 kbar. Ptridymite structure (c, = 0.50, 6 = 2.22) is an infinite threedimensional framework of [SiO4I4 tetrahedra. It can be sliced into sheets of tetrahedra like muscovite (Fig. 6.41(a)) but arranged in such way that the tetrahedra vertices alternate up and down. The structure of coesite (c, = 0.67, 6 = 2.91) is quite dense and somewhat more complex compared with that of Ptridymite. The main difference between them concerns the second and following Si4+coordinations that, of course, are greater for coesite. This explains the different packing coefficients, though none of them (see p. 429 and following) conforms to the closest packing. Stishovite has an exceptionally high packing coefficient (c, = 0.99) and a density (6 = 4.29) much greater than that of /3tridymite or coesite. The structure is rutile type, TiO,, (Fig. 6.26, (c)), so it conforms to the closest packing model. The very high pressure under which stishovite crystallizes forces Si4+ to renounce its habitual four for an unusual six coordination. According to the mechanical closest packing model it is impossible to have c, = 1, unless we suppose that the available space of the structure is
Ionic crystals
almost completely filled by oxygens having an approximate volume of a ball with re = 1.40 A but geometrical form by no means spherical. The compound grossular, Ca3Al2Si3OI2,belongs to an important group of minerals known as garnets. In spite of the high packing coefficient (ci = 0.66), grossular does not have a close packed structure (see Appendix 6.B). Here we note that Ca2+ cannot replace 0' as occurs in perovskite. Let us consider the structure of perovskite (Fig. 6.28) and its chemical formula in the form Ca4Ti4 hIz4Ol2 (El represents the empty tetrahedral site). Figures 6.19 and 6.28 show that if grossular were to adopt a perovskitetype structure in half of the cells shown in Fig. 6.28, si4+ in tetrahedral holes would be in contact with Ca2+. After all, according to the examples quoted, the packing coefficient is trustworthy only in a few cases, i.e. for those structures having suitable cations and a high degree of ionic bonding (as happens in several oxides). Its value can give little information on the real atomic packing, which can sometimes be enhanced only by further crystallochemical parameters (see Appendix 6.B).
6.B Structural inferences from crystallochemical parameters The effective ionic radius re, the packing coefficient (ci) and the valence electrostatic rule (V = 2,) can sometimes be profitably used to foresee some important structural features particularly when simple crystal structures are considered. First of all one should extract all the possible information from the chemical formula. On p. 437 we have seen that for the compounds of MX type, the coordination numbers of M and X can vary provided that the ratio 1:l is preserved; for instance in NaC1, M:X= 6:6 and in CsBr M:X = 8:8. Again, in the MX2 compounds the coordination number of M and X can change, the ratio M:X = 2:l being equal. So, salts like S O 2 , Ti02 and CaF2 have the ratio M:X = 2:l and respectively the following coordination numbers: 4:2, 6:3 and 8:4. From these remarks the following rule can be derived: in a given structure, if no bond between identical atoms forms, M and X coordination numbers of compounds M,Xp, are in the ratio p:m. This rule can also be applied to more complex structures like A,B,Xp. First let us define the average cation coordination number ( m , ) : where CNA and CNB are respectively the coordination numbers of cations A and B. The relationship between and the average anion coordination number ( m , ) is expressed by
m,

CN,/CN, = p l(m
+ n).
64.2)
Replacing A . l in A.2, the latter can be written as Some examples are given, in order of increasing structural complication, to understand the relationships between chemical formula, crystallochemical
(
459
460
1
Fernando Scordari parameters, and symmetry, showing how they can sometimes have predictive value. At first, we will assume tentatively that the ionic structures having ci> 0.60 can be described in terms of a closepacked anion arrangement with cations filling the holes, even if in some cases this hypothesis does not hold (as some of the following examples will prove). 1. Periclase, MgO, Fm3m, and Z = 4, has a packing coefficient ci= 0.62. According to the accredited Mg2+ CN, 4, 5, 6, 8 (see Table 6.7) this cation can fill the tetrahedral (half) or the octahedral site of a structure based on a closepacking model. Moreover the space group Fm3m and the number of formula units Z = 4 informs us that Mg2+ and 02lie at 4,i, 4 and 0 , 0 , 0 or vice versa, from which = CN, follows. Using (A.3) in the more simple form mCN, =pCN, we reach an obvious conclusion, i.e. Mg2+ and 02have the same CN, (4 or 6) and of course for both coordinations the electrostaticvalence principle is satisfied. To solve the CN dilemma, we observe that periclase is isotype with lime, CaO, and that accredited CN, for Ca2+ are 6, 7, 8, 9, 10, 12 (Table 6.7). Only 6 and 8 belong both to Mg2+ and Ca2+ CN, sets, consequently only the octahedral sites of a closedpacked anion arrangement can be filled.
m,
2. Rutile, Ti02, P4,/mnm, and Z = 2, has a packing coefficient c, = 0.74. The accredited CN, of Ti4+ are 4, 5, 6, 8 (Table 6.7). Therefore, according to the close packing and valence requirements, Ti4+ can fill tetrahedral or octahedral sites. The octahedral site stabilization energy (OSSE = 0) cannot remove the uncertainty regarding the site, even if the high electrical charge informs us that Ti4+ prefers the octahedral site. El. can be observed that, according to the space group, Ti4+can be placed at 0, 0, 4 or 0, 0, 0 and that 02can lie on 2/m or 4 or mm (from 4e to 4g according to International = CN,. No Tables of Xray Crystallography Vol. A) in this case profitable information can be drawn from isotype structures, but we know that Nb4+ and ~ a can ~ replace + Ti4+ in very high percentage ( ~ 0 . 4 0 )The . common CN for these two cations, i.e. 6, indicates that very probably, Ti4+ prefers the octahedral site. From (A.3) the calculated oxygen coordination number is = 3, i.e. three Ti4+ surround one 02whereas, as shown above, Ti4+ seems linked to six oxygens.
m,
m,
3. Ilmenite, FeTiO,, ~ 3 and , Z = 2, has a packing coefficient c, = 0.66. According to the space group, two ~ e and ~ two + Ti4+ can lie on a threefold axis or one of them on a threefold axis and the other on the two independent 3 (la, lb). As for the oxygen atoms, they can be situated on the two independent i (3e, 3d) or in the general position 1 (6f); in both cases (i or 1) CN, must be an integer. The accredited CN, for Fe2+ and ~ i ~ + are respectively 4, 6, 8 and 4, 5, 6, 8 (Table 6.7), so either Fe2+ or ~ i may ~ + fill tetrahedral and/or octahedral sites. From (A.3) three different can be calculated for ilmenite:
m,
 
1.4 + 14= 3CNx;  CN,  = 813  CN, = 1013 1.4 + 16= 3CNx; 1.6 + 1.6 = 3CNx;CN, 4.

Only the third result agrees with the statement that
m, must be an
Ionic crystals integer and precisely it tells us that four cations are linked to each oxygen without specifying their nature. Applying the electrostaticvalence rule to +, + the three possible combinations 1Fe2+ 3Ti4+, 2Fe2+ 2 ~ i ~ 3Fe2+ lTi4+,we found respectively 2.33, 2, 1.67 V.U.(valence units). So 2Fe2+ and 2Ti4+ are the cations coordinated by one oxygen atom, in agreement with the stoichiometry.
+
+
4. Perovskite, CaTiO,, ~ m j m ,and Z = 1, has a packing coefficient c, = 0.62. The space group and Z inform us that Ca2+ and Ti4+ are in m3m (la, lb) and that oxygen lies on 4/mmm (3c or 3d), i.e. the number of cations arotlnd it is an integer and, what is more, even. The accredited CN, for Ca2+ are 6, 7, 8, 9, 10, 12 and for ~ i they ~ ' are 4, 5, 6, 8. So according to c, and CN, Ca2+ and Ti4+ should fill, like ilmenite, octahedral sites. This eventuality would require that 5 of the octahedral si;es be filled by Cd2+and Ti4+ and that consequently several edges (three are in the sheet) be shared between Ca2+ and Ti4+ octahedra. Now we observe that for CN = 6, different from ilmenite (re = 0.61 (Fe2' low spin) and re = 0.605 A (Ti4+), the Ca2+ and Ti4+ effective ionic radii are quite different: re = 1.00 (Ca2+) and re = 0.605 A (Ti4+).This strong difference is reflected on the octahedral edges that, if shared, would involve a strong strain in the structure and consequently the increase of its potential energy. Moreover for CN = 12, the Ca2+ effective ionic radius (re = 1.34 A) matches well with the 02one, so we have a special close packing form in which of oxygens are replaced by Ca2+. For Ti4+ in tetrahedral or octahedral sites and Ca2' 12coordinated, (A.3) gives respectively = or = 6, supporting the hypothesis that Ti4+ is sixcoordinated like the oxygen. As far as the nature of the cations around the oxygen is concerned, the valence sum principle indicates that around the oxygen atom there are two Ti4+ and four Ca2+. 5. Zircon, ZrSi04, I4,/amd, and Z = 4, has a packing coefficient c, = 0.70. In accordance with the space group and the number of formula unit Z, zirconium and silicium are located at 42m (4a and 4b). In theory, oxygen can be placed at 2/m (8c and 8d) or at 2mm (8e x 2), but it can easily be shown that starting from the unit cell parameters, a = 6.60 and c = 5.98 A, the calculated interatomic distances zr4+0; and Si4+02 do not match well with those obtained from the effective ionic radii (Table 6.7). For instance, supposing the cation (M4+), i.e. zr4+ or Si4+, at 0, 0, 0 (4,) and 02at 0, $, (8c), then the M4+02 calculated distance is 1.81 A # 1.66 (Si4+0') and 2.12 (zr4+02). On the other hand the situation does not improve if 02is located at 0, 0, z because the calculated Zr4+0 and Si4+0 distance sums are: 2.99 A (5.9812 A) # 3.78 A (1.66 + 2.12 A). These kinds of argument support the hypothesis that 0' is situated on 2 or = CN,. m (16f or 16g or 16h), so The packing coefficient would suggest that zircon adopts a closepacking structure. However, if Si4+ cations are located at the habitual tetrahedral holes, assumes integer values (A.3) when zr4' fill tetrahedral sites or when it is 8 or 12coordinated. Let us now consider, besides ZrSiO,, the zircon isotype structures: coffinite, USi04; thorite, ThSi04; Hafnon, HfSiO,. The accredited CN, (Table 6.7) of the bigger cations are: 4, 5, 6, 7, 8, 9 (zr4+);6, 7, 8, 9, 12 (u4+);6, 8, 9, 10, 11, 12 (Th4+);4, 6, 7, 8 (HP+). They show that some CN, (6 and 8) are present in all the four cations. This peculiarity together with the results of (A.3) suggest that a packing,
a
m,
m,
m,
m,
1
461
462
1
Fernando Scordari different from the close packing, in which Zr4+ is 8coordinated, characterizes the crystal structure of zircon. In addition we note that the electrostatic valence balance is not compatible with a structure having Zr4+ in octahedral sites. In fact, since the oxygen atom is shared by Si4+ and Zr4+, the bond strengths coming from Si4+ (+1 v.u.) and from zr4+ (+4/6 or +8/6v.u.) do not balance 02valence. By means of (A.3), we can conclude that around 02there are three cations, the nature of which can be specified by means of the electrostaticvalence rule: two zr4+ and one Si4+. 6. Spinel, MgA1,04, ~ d g m Z , = 8 has a packing coefficient ci= 0.70. In the unit cell there are 8Mg2+, 16A13+,and 320'. Magnesium lie on 43m (8a or 8b), aluminium on 3m (16c or 16d), and consequently oxygen is on = CN, is an integer. If the civalue and the accredited CN, 3m (32e), so for Mg2+ (4, 5, 6, 8) and for A13+ (4, 5, 6) are taken into account, then the spinel structure would seem to conform to a closepacking one with tetrahedral and/or octahedral sites partiallyfilled. On the other hand, (A.3) leads to three possible configurations for CN, integer: (1) Mg2+ and ~ l in ~ tetrahedral; (2) Mg2+ in tetrahedral and A13+ in octahedral sites; and (3) half ~ l in~tetrahedral + and half in octahedral together with Mg2+. The calculated of oxygen is three for the first and four for the other two configurations. As concerns other factors influencing crystal structures, the effective ionic radius seems to favour A13+ in tetrahedral and Mg2+ in octahedral sites, whereas the formal charge indicates that cations follow the opposite behaviour pattern. The quoted ambiguity allows us to understand why direct and inverse spinel structure exists, as is better explained in a more general way at p. 443. Finally, for cations located in tetrahedral sites, both the chemical formula and the valence balance require two ~1~~ and one Mg2+ around 0'whereas when Mg2+ and ~ l are~ respectively + in tetrahedral and octahedral holes the chemical formula indicates that oxygen is surrounded by one Mg2+ and three ~ f + .
m,
m,
7. Pyrope, Mg3Al2Si3O1,, 1a3d, Z = 8, has packing coefficient 0.73. The number of formula units Z and the space group suggest that A13+ lies on 32 or 3 (16b or 16a) and that Mg2+ and Si4+are on 222 and 4 or vice versa. As regards the oxygen atoms these can be located on 3 (32e), 2 (48f and 48g), or 1 (96h) axes. The shortest interionic distances between cations, lying on 222 (24c) and 4 (24d), and oxygen lying on 3 (32e) or on 2 axes (48f and 48g) have the following values: 3.09 and 2.865 A, far from those inferred from Table 6.7, i.e. Mg2+0 = 2.29 A or Si4+0 = 1.66 A. Besides symmetry, valence balance and chemical formula requirements would seem to exclude the location of an oxygen atom on the quoted special positions, so the most reliable point symmetry for oxygen atom seems 1. The CN, used for Mg2+in the latter analysis were limited to 6 and 8 because pyrope is an isotype with grossular, Ca3A12Si3012 and the common CN, between Mg2+ and Ca2+ are 6 and 8. The modified form of equation (A.3) applicable to pyrope is It can be easy verified that only when Ca2+ has CN = 8, whole number, i.e. = 4.
m,
m, become a
+
Ionic crystals Finally by means of the chemical formula and the application of the electrostaticvalence rule it is possible to characterize the oxygen coordination, i.e. two Mg2+, one A13+, and one Si4+. Generally speaking it is difficult to imagine making a correct inference on the atomic organization of a complex structure without having some preliminary information or without any assumption concerning it. For instance, coquimbite has (Fe3+,A1),(S0,),.9H20, ~ 3 1 c , 2 = 4, V = 1760.5 A3 and ci= 0.55. If the usual CN, 6 and 4 for this kind of structures are respectively assumed for Fe3+ and S6+ and if it is supposed that Hf forms no bifurcated hydrogen bonds in coquimbite, then the CN, of oxygen can b e inferred. In fact using (A.4) we have 2.6 34 2.18 = 21CN,, from which = 2.86 can b e estimated. The structure informs us that: O(1) and O(2) are shared by one ~ e (or ~ A13+) + and one S6+; O(3) and O(4) are shared by one S6+ and two H + ; 0,(1) and 0,(2) are shared by one ~ e (or~ A13+) and two H + ; 0,(3) is shared by four HC. This configuration leads to the quoted = 2.86.
+ +
m,
m,
References 1. Cartemel, E. and Fowles, G. W. A. (1966). Valency and molecular structure. Butterworth, London. 2. Huheey, J. E. (1983). Inorganic chemistry. Principles of structure and reactivity, (3rd edn). Harper, New York. 3. Vainshtein, B. K., Fridkin, V. M., and Indenbom, V. L. (1982). Modern crystallography II. Springer. Berlin. 4. Pauling, L. (1959). The nature of the chemical bond. Cornell University Press, Ithaca. 5. Hamilton, W. C. and Ibers, J. A. (1968). Hydrogen bonding in solids. Benjamin, New York. 6. Greenwood, N. N. (1970). Ioniccrystals, lattice defects and nonstoichioimetry. Butterworths, London. 7. Catti, M. (1978). Acta Crystallographica, A34 974. 8. Cotton, F. A. and Wilkinson, G. (1980). Advanced inorganic chemistry, (4th edn). Wiley, New York. 9. Orgel, L. E. (1960). A n introduction to transitionmetal chemistry ligand field theory. John Wiley, New York. 10. Basolo, F. and Johnson, R. (1964). Coordination chemistry. Benjamin, New York. 11. Ballhausen, C. J. (1962). Introduction to ligand field theory. McGrawHill, New York. 12. Burns, R. G. (1970). Mineralogical applications of crystal field theory. Cambridge University Press. 13. Busing, W. R. (1981). W M I N , computer program to model molecules and crystals in terms of potential energy functions, U.S. National Technical Information Service, ORNL5747. 14. Catlow, C. R. A. and Cormack, A. N. (1984). Acta Crystallographica, B40, 195. 15. Alberti, A. and Vezzalini, G. (1978). Zeitschrift fur Kristallographie, 147, 167. 16. Brown, G. E. and Fenn, P. M. (1979). Physics and Chemistry of Minerals, 4, 83. 17. Parker, S. C., Catlow, C. R., and Cormack, A. N. (1984). Acta Crystallographica, B40, 200. 18. Shannon, R. D. and Prewitt, C. T. (1969). Acta Crystallographica, B25, 925. 19. Shannon, R. D. (1976). Acta Crystallographica, A32, 751. 20. Fajans, K. (1923). Naturwissenschaften, 11, 165.
+
1
463
464
1
Fernando Scordari 21. Magini, M. (1979). Journal of Chemical Physics, 70, 317. 22. Redinger, J. and Schwartz, K. (1981). Zeitschrift fur Physik, B40, 269. 23. Phillips, J. C. (ed.) (1974). Treatise o n solid state chemistry, Vol. 1. Plenum, New York. 24. Pearson, W. B. (ed.) (1972). Crystal chemistry and physics of metals and alloys. Wiley, New York. 25. Basso, R. (1985). Neues Jahrbuch fur Mineralogie. 3, 108. 26. Hawthorne, F. C. (1981). Journal of Solid State Chemistry, 37, 157. 27. Lamgley, R. H. and Sturgeon, G. D. (1979). Journal of Solid State Chemistry, 34, 79. 28. Novak, G. A. and Gibbs, G. V. (1971). American Mineralogist, 56, 791. 29. Moore, P. B. and Smith, J. V. (1970). Physics of the Earth and Planetary Interiors, 3, 166. 30. International tables for xray crystallography, Vol. 11, (1959). Birmingham: Kynock Press. 31. Iglesias, J. E. (1981). Zeitschrift fur Kristallographie, 155, 121. 32. Basso, R. (1985). Neues Jahrbuch fur Mineralogie, 3, 108. 33. Brown, I. D. and Shannon, R. D. (1973). Acta Crystallographica, A29, 266. 34. Brown, I. D. and Wu, K. K. (1976). Acta Crystallographica, B32, 1957. 35. Brown, I. D. (1978). Chemical Society Reviews, Vol. 7, No. 3. The Chemical Society, London. 36. Scordari, F. and Stasi, F. (1990). Neues Jahrbuch fur Mineralogie, 161, 241. 37. Siisse, P. and Tilmann, B. (1987). Zeitschrift fur Kristallographie, 179, 323. 38. Evans, R. C. (1976). A n introduction to crystal chemistry (2nd edn). Cambridge University Press. 39. Ottonello, G. (1986). Physics and Chemistry of Minerals, W, 79. 40. Baumgartner, O . , Preisinger, A , , Heger, G., and Guth, H. (1981). Acta Crystallographica, A37, C187. 41. Yamanaka, T. and Takeuchi, Y. (1983). Zeitschrift fur Kristallographie, 165, 65. 42. Liu, L. G. (1976). Physics of the Earth and Planetary Interiors, 11, 289. 43. Zoltai, T. (1960). American Mineralogist, 45, 960. 44. Ribbe, P. H. (1982). Orthosilicates, (2nd edn), Reviews in Mineralogy No. 5. Mineralogical Society of America, Washington. 45. Liebau, F. (1985). Structural chemistry of silicates. Springer, Berlin.
Molecules and molecular crystals GASTONE GILL1
Chemistry and Xray crystallography Crystal and molecular structure Xray diffraction from crystals was discovered at the beginning of this century and it soon became evident that it was suited to the investigation of the structure of matter at atomic resolution level. Diffraction applications of Xrays and, later on, of other radiations of comparable wave length, such as electrons or thermal neutrons, developed rapidly allowing the scientific world to obtain, for the first time, a detailed knowledge of the intimate atomic distribution in elements, organic and inorganic substances, natural and synthetic fibres, and even liquids. It became clear, however, over the years, that the level of image resolution achievable was strongly dependent on the aggregation state of matter. Currently we know that a resolution of a few thousandths of an angstrom is actually obtainable only by diffraction experiments carried out on relatively perfect single crystals, both organic and inorganic, while macromolecular crystals of proteins (haemoglobin, myoglobin, and enzymes) cannot give an accuracy better than, say, 0.5 A and fibres or liquids produce poorly resolved images, which can be considered barely giving much more than a hint of the true molecular structure. The experimental resolution achievable is to be compared with the natural resolution needed by classical chemistry. For example, carboncarbon distances are typically 1.54 for single bond, 1.39 for aromatic compounds, and 1.33 and 1.20 A for double and triple bonds, respectively; thus a total range of 0.034 A covers the fantastic change of properties and reactivities between alkynes and alkanes and the much smaller range of 0.006 A separates aromatic from alkene chemistry. Taking into account that two bond distances cannot be reasonably compared at less than four e.s.d. (estimated standard deviations), we must conclude that no valuable chemical information is contained in CC distances known with an e.s.d. greater than 0.01 A and, therefore, in crystal structures where the e.s.d.s on atomic positional coordinates are greater than about 0.007 A. This value sets a clear limit on diffraction experiments. Only elements, minerals, and small molecules easily develop into longrange ordered threedimensional arrays of perfect or ideally imperfect crystals, and only diffraction experiments on such crystals can provide independent experimental evidence of direct relevance to chemistry. Conversely, synthetic or natural macro
466
1
Gastone Gilli
Table 7.1. Atomic van der Waals radii (A). H in aromatic rings 1.00 A; C perpendicularly to the benzene ring 1.77 A. Data according to ~ o n d i [ ~ l C1.70 Si 2.10
N1.55 P 1.80 As 1.85
01.52 S 1.80 Se 1.go
H 1.20 F1.47 CI 1.75 Br 1.85 1 1.98
molecules, which crystallize as highly defective hydrated monocrystals in the most favourable case of globular proteins, but often as fibrous materials having simple onedimensional order, cannot give much more than the overall shape of the diffracting molecule and their study is to be considered more a branch of highresolution microscopy than a part of the structural chemistry in a strict sense. The expression structural crystallography is often used for identifying the branch of sciences producing direct knowledge of the structure of matter by diffraction methods. Within structural crystallography there are divisions which have become traditional: crystal chemistry of metals and alloys, minerals, molecular and macromolecular crystals are usually taught in different courses, and their scientific achievements published in different journals. This is a kind of functional partitioning, different parts of crystallography being dealt with according to their usefulness to other disciplines. There are, however, more scientifically founded reasons for a subdivision, which originate from the differences that the knowledge of the crystal structure may have for different classes of chemical substances. This knowledge is of primary value when the atomic binding forces within the crystal can be classified as true chemical bonds, as is the case for covalent, metallic, or ionic crystals, where the nature of the bond can be understood only on the basis of the knowledge of the crystal itself. For instance Na,, G, and Si, molecules are well known in the gas phase but their properties cannot explain why metallic sodium, diamond or graphite, and silicon may be electronic conductors or insulators or semiconductors. In the same way the reason for the stability of ionic substances is found in the ordered arrangement of alternating anions and cations within crystals where any simple relationship between chemical formula and crystal structure is completely lost. A good example, taken from wells,[ll may be that of the series of AX iodides: HI, AuI, CuI, NaI, and CsI; only the first term gives biatomic molecules at room temperature, while the others are solids where A is surrounded, in order, by 2, 4, 6, and 8 atoms of X. The other extreme is represented by the class of molecular crystals where chemical substances, typically organic and organometallic compounds, exist as discrete molecular entities packed together by weak dispersion or dipolar forces. Interatomic distances within the crystal can be generally grouped in two clearly distinct distributions, a first of bond distances within the molecule and a second one of the much longer contact or van der Waals distances among atoms of different molecules. Nonbonded atoms on different molecules tend to behave much like noninteracting hard spheres that cannot approach at a distance shorter than the sum of their encumbrance radii, called van der Waals radii, rvdW,and reported in Table 7.1. If the crystal is fused or vapourized by heating or dissolved by a solvent the crystalline order is destroyed, but the geometry and pattern of interatomic connections within the molecules, apart from possible partial rotations around single bonds, remain unchanged. In this case the crystal structure (intended as crystal packing) is less important, the chemical information being mainly concentrated in the molecular structure which, in principle, could be determined in any other state of aggregation of matter. In fact, methods for accurate determination of structure in liquids or in solutions are not actually available and gas phase
Molecules and molecular crystals
1
467
methods (microwave spectroscopy and gas electron diffraction) allow us to study only small and preferably symmetrical molecules, so that crystal structure determination often remains the only practicable way in which to obtain detailed information on the molecular structure of chemical compounds. Taking into account the importance of the knowledge of the molecular structure of both synthetic and natural substances, it is not surprising that Xray structure determination of molecular crystals has so far been used as a simple tool for determining molecular configurations and conformations and that crystal packing has mostly been seen either as an irrelevant factor or as an unwanted cause of perturbation of the freemolecule geometry. Only recently has the idea that crystal packing could be important in itself in the study of molecular interactions been widely, if not generally, accepted.
The growth of structural information Xray crystallography of molecular crystals has been so successful in chemistry that the last three decades have registered an almost exponential growth of the number of structures published per year. Structural data had to be collected in computerized databases, and the Cambridge Structural Database (csD),[~]as at April 1990, contained bibliographic, chemical, and numerical results for some 84 464 organic and organometallic compounds. Figure 7.1 show a histogram of the new entries in the CSD in the period 196586.13] The number of complete structural analyses published up to 1960 was only 579 (45 from 193545, 212 from 194555, and 322 from 195560) and this number is now exceeded tenfold by the structures determined per year. The factors which have determined such a rapid evolution in the field are scientific (development of direct methods theory), technological (improvement in automatic singlecrystal diffractometers), and organizational (distribution of complete systems of crystallographic computer programs). All these factors must also be considered with the parallel evolution of fast electronic computers, without which Xray crystallography would have remained that slow and patient skilled work well known to the scientific world until the end of the 1950s. The effects produced in chemistry by this extraordinary wealth of structural information are enormous, and for a vivid analysis of this
1965
1970
1975 Year
1980
1985
Fig. 7.1. Number of new crystal structures registered each ear in the Cambridge Structural Database (CSD)81 from 1965 t o 1986. Structures containing d or fblock metals are indicated by shading. (Reproduced by permission from Orpen eta/.[ ''I)
468
1
Gastone Gilli phenomenon the reader is referred to the second part of the Dunitz's book Xray analysis and the structure of organic molecules.[41The attempts aimed to interpret, rationalize, and understand this continuously growing mass of data give rise to problems far beyond the limits of a single chapter, being dealt with by the scientific discipline of structural chemistry, initiated more than 50 years ago by Linus ~ a u l i n g ' in ~ ] his famous book The nature of the chemical bond and the structure of molecules and crystals. A n introduction to modern structural chemistry. The present chapter is intended to summarize the structural chemistry of molecular crystals. As regards its content, it has been necessary to be severely selective of topics. The discussion is strictly confined to the nature of molecular crystals and to the stereochemical aspects of molecules which are directly derived from the results of structural investigation. Final applications, such as structureproperty studies in chemistry and molecular biology or pharmacology have been completely excluded. The topics have been divided in two parts, according to whether they refer to single molecules or molecular crystals as a whole and can be so summarized: (1) molecular crystals: molecular interactions, their nature and effect on the crystal packing; elements of crystal thermodynamics and polymorphism; (2) single molecules: classical stereochemistry; molecular geometry and chemical bond; molecular mechanics; interpretation of molecular structures and the structure correlation method.
The nature o f molecular crystals Generalities Molecular crystals are ordered packings of discrete physical entities, i.e. molecules. Most of them consist of neutral molecules, and it is those which are mainly discussed here, though some may sometimes contain ions (e.g. organic carboxylates, alkylammonium halides) as well. The energy of formation of the crystal from the isolated (gas phase) molecules is called lattice energy, U; typical values of U for molecular crystals are 0.54 kcal mol' for noble gases, 1020 kcal mol' for most neutral organic compounds and up to 4050 kcal mol' for neutral molecules of relevant complexity. By comparison with some typical  U values for ionic (e.g. 188 in NaC1, 629 in CaF,, 3804 in A1203 and 3137 kcal mol' in Si0,) or covalent crystals (some 171 and 283 kcal mol' for diamond and Sic, respectively) it can be seen that the forces determining the packing in molecular crystals are much weaker than those of ionic or covalent chemical bonds. suchweaker intermolecular forces can be approximately classified as follows.
Repulsion or exchange forces Most stable molecules have closed electron shells, that is all their molecular orbitals are doubly occupied and cannot accept other electrons without violating the Pauli principle. Accordingly, they repel other molecules trying to come too close. Repulsive forces exert their effects at very short range, decrease with the ninth to twelfth power of the interatomic distance and grow quite rapidly only when two nonbonded atoms try to get closer than
Molecules and molecular crystals
1
469
CH
_C,.
. \.'
1
3
4
r (A)
k
their proper contact distance, given by the sum of their van der Waals radii (Table 7.1).
Dispersion or London f o r c e ~ [ ~ l l ] These are weak shortrange attractive forces which decrease with the sixth power of the intermolecular distance and are caused by the mutual attraction of the small transient dipoles that molecules can induce in each other. They give the greatest contribution to the lattice energy in crystals of neutral molecules even if the energy of any single interaction is very small. Dispersion energy between two molecules is usually expressed as the sum of the crossed interactions between all pairs of atoms on the two molecules and the sum of repulsion and dispersion energies is named nonbonded energy, En,. When plotted versus the interatomic distance, r, the nonbonded energy displays a typical minimum at a distance nearly equal to the sum of van der Waals radii of the two atoms (Fig. 7.2). Such a minimum is quite shallow, being of the order of a few tenths of a kcal moll.
Dipolar forces Molecules having permanent dipole moments experience electrostatic attraction when properly oriented (orientation forces). According to ~ i t a i ~ o r o d s k i ,such [ ~ I attraction forces must cancel out in crystals having only translational symmetry operations (space group PI); for other space groups it has been estimated that the dipoledipole interactions may contribute one tenth of the lattice energy for molecules having dipole moment of 34 D, while their contribution becomes negligible when the dipole moment is less than 1D.
Monopolar forces Monopoles are associated with ions, a situation which is not very common in molecular crystals and is not discussed here in detail. Two main points, however, deserve particular attention: ionic interactions are known to cause a quite relevant increase in lattice energies as can be shown, for example, by the comparison of these energies for acetic acid and sodium acetate, respectively 17.4 and 182 kcal moll; monopolemonopole interactions are longrange forces whose energy decrease only with the first power of the
Fig. 7.2. Curves of nonbonded energy as a function of internuclear distance, E,,(r) versus r, for the CC, CH, and HH interactions calculated by using the atomatom potentials given by ~ i g l i o [ '(full ~ ] curves) and ~ l l i n ~ e r [ ' ~ ' (broken curves).
470
1
Gastone Gilli
interionic distance (Coulomb law) and in this respect differ from all other short or veryshortrange intermolecular forces.
Hydrogen bonding[l"lsl With the exception of monopolar forces, Hbonds are the highestenergy interactions in molecular crystals. They greatly affect the way in which molecules are packed, in the sense that the observed packing is almost inevitably that allowing the maximum number of such bonds to be made. Moreover, Hbonding is, by itself, the most relevant nonbonded interaction in nature, being the main factor determining the structure of water, the folding of proteins, and the pairing of bases in DNA. For this reason most crystal packing studies are essentially attempts to understand the laws governing the intermolecular Hbonding in an easily reproducible experimental environment, that given by the molecular crystal. Hbonding occurs when a hydrogen atom is bonded to two (or sometimes more) other atoms. This situation may be depicted schematically as DHA, where D is the Hbonding donor and A the acceptor. In principle all atoms more electronegative then hydrogen (C, N, 0 , F, S, C1, Se, Br, I) can play the role of A and D , though stronger hydrogen bonds are necessarily associated with the most electronegative ones (N, 0 , F, Cl). Several theoretical studies have been devoted to clarifying the nature of the bond in Hbonding complexes and in particular the relative contributions of different terms to its total energy. Probably the most popular and quoted partitioning scheme is that developed by Umeyama and ~ o r o k u m a [ for l ~ ~the treatment of (H20), and (HF), dimers. It makes use of the energy decomposition analysis developed within the ab initio SCFMO theory[203211 where the total Hbonding energy is partitioned in four terms: the repulsion or exchange energy and the electrostatic, polarization, and charge transfer attraction energies. The authors were able to conclude that the main attractive term is electrostatic and that the contribution of charge transfer is small, so that Hbonding can be qualitatively defined as an electrostatic more than charge transfer or simply electrostatic interaction. Hbonds can be classified (Fig. 7.3) according to their topology as intramolecular, intermolecular, or bifurcated and, according to their energy, as going from weak to very strong. 1. Weak Hbonding can be observed for any couple of donor and acceptor atoms whenever the two groups cannot achieve the correct approach for some sterical reason. The main factor is usually the DHA angle which, for maximizing the electrostatic interaction between the DH dipole and the negatively charged acceptor, must be in the range of some 160180". A good example comes from the intramolecular Hbonds closing five, six, or sevenmembered rings; the Hbond closing a fivemembered ring is always weak (and so weak that the hydrogen of its DH group forms, whenever possible, a second bifurcated hydrogen bond with another acceptor (Fig. 7.3(g1)). A second reason why a Hbond is to be classified as weak comes from the small intrinsic electronegativities of the Hbonded partners, the most classical case being that of the CHA interactions.[221 2. Medium Hbonding is typical of water, alcohols, amines, amides, and carboxylic acids. Its geometry is rather well defined: the 0H0 group
Molecules and molecular crystals
$ \
1
471
//OH0
'CR
RC \OAH
  04
Fig. 7.3. Different types of Hbonds. Intermolecular Hbonds forming threedimensional nets in water (a), dimers in carboxylic acids (b), chains in hydrofluoric acid (c), and bicyclic dimers between guanine and cytosine in DNA Id), Intramolecular Hbonds closing sixmembered rings (e) are stronger than those closing fivemembered rings (f).Two examples of intermolecular bifurcated Hbonds (g, g'). Charge assisted Hbonds (CAHB) (h) and resonance assisted Hbonds (RAHB) (i) are stronger than the usual Hbonds between neutral groups. An example of a very strong Hbond, the difluoride ion (j).
tends to be linear; the DH distance is not significantly lengthened with respect to that observed in the absence of Hbond; the DA contact distance is practically identical to the sum of the van der Waals radii of A and D, that is the van der Waals radius of the interleaving H atom is almost zero. A wealth of thermodynamical data['*] shows that its formation enthalpy is in the range 28 kcalmol'. In more detail, it is some 4.8 kcal moly' for the water dimer and 4.7, 5.4, 5.8, 8.6 kcal molI, respectively, for the Hbonds formed by carbonyl, amide, ether, and amine acceptors with the phenol as donor.[151 3. Mediumstrong Hbonding can be thought to derive from medium Hbonding strengthened by the presence of positive and/or negative charges. A possible range of energies is 620 kcal mol'. It seems reasonable to distinguish two different cases: (a) charge assisted and (b) resonance assisted Hbonding.
(a) Charge assisted Hbonding (CAHB) arises from net ionic charges on the donor and/or the acceptor groups. The effect of charge in strengthening the Hbond is documented by the data collected[231 on the Hbonds formed between the intrachain or terminal groups of oligopeptides and aminoacids: the average N0 contact distance is 2.840, 2.908, 2.912, and 2.929 A, respectively, for the Hbonds ) C=OH,N+, COOHN ( and COOeH3N+, ) C=OHN (.
472
1
Gastone Gilli
(b) Resonance assisted Hbonding (RAHB) is similar to CAHB but with the difference that the strengthening charges arise from polar resonance form^;[^^,^'] the only system extensively studied is that of Pdiketone enols where the resonance O=CC=COH()0C=CC==OH+ strengthens the intramolecular 0H0 bond in such a way that the 00 distance can become 2.417 A and the calculated Hbond energy 12.719.7 kcal mol' (values to be compared with those for the water dimer: d,, = 2.74 A , AH = 4.8 kcal mol'). In these compounds an appreciable lengthening of the 0  H bond with consequent shift of the proton towards the central interoxygen position is also observed. 4. Very strong Hbonding appears to be inevitably associated with ions. It is characterized by relevant lengthening of the DH distance, nearly central position of the proton, DA distances definitely shorter than the sum of van der Waals radii, and bond energies intermediate between true Hbonding and covalent bonding. Complexes like [FHF]or [H,OHH,O]+ have Hbond enthalpies of 150250 and 130150 kcal molI and must be considered true chemical species where the charge transfer (covalent bonding) is relevant and we may speak of Hbonding only in a formal sense.
Charge transfer[2G291 Intermolecular charge transfer or donoracceptor interactions occur between electron donors (Lewis' bases) and acceptors (Lewis' acids). They establish an at least partially covalent bond between highly polarizable groups, which is often described as the formation of a molecular orbital by electron donation from the highest occupied molecular orbital (HOMO) of the donor to the lowest unoccupied molecular orbital (LUMO) of the acceptor. Classical examples are the molecular complexes NH, BF3 = H3NBF,, I, I = [III], or the molecular crystal of iodine, where the I, molecule is both an acceptor along the interatomic axis and a donor perpendicular to it. Such a type of interaction occurs in crystals only in the presence of large and easily polarizable (soft) atoms. Another type of donoracceptor interaction which has been actively studied in the recent past is that present in metallic or semiconducting organic crystals, a class of mixed crystals which contain planar donor and acceptor molecules packed in separated (segregated) infinite stacks and have given rise to great interest for their potential applications in electronics. For a recent review on their structural aspects see references.[301
+
+
Intermolecular forces and crystal packing We may wonder whether a generic knowledge of intermolecular forces can give us some general insight into the way in which molecular crystals are packed. It is not difficult to show that the relative molecular positions are mainly determined by shortrange forces. Calling r the interatomic distance, the repulsion energy drops nearly with r12, the attractive dispersion energy tends to zero with r6, and the attractive electrostatic energy decreases with r'. These facts have important implications, because the electrostatic energy changes so slowly within the lattice that it is practically unable to
Molecules and molecular crystals displace the molecules from their sharp minima, already determined by the shortrange balance of repulsion and van der Waals interactions of the outer atoms of the molecule, so that these latter remain the true controlling factor of the packing arrangement. The only exception to this rule is represented by the hydrogen bond, which is electrostatic in nature but requires a quite specific geometry in the donoracceptor DHA interaction and, moreover, involves energies much greater than dispersion interactions do. The relevant role played by shortrange van der Waals forces in the crystal packing helps us to understand the apparently paradoxical fact that the large majority of molecular crystals belong to a few space groups having secondorder symmetry elements. Since van der Waals forces are both adirectional and additive, the energy of any single atom is lower the higher the number of atoms of other molecules surrounding it at contact distances is or, in other words, the most stable crystal is that in which molecules pack themselves with the highest coordination number. A simple geometrical analysis of the problem has been carried out by ~ i t a i ~ o r o d s kwho ~ [ ~has ' shown that rows of molecules staggered by a glide lattice operation can produce a very efficient close packing (coordination of twelve) by repeating a molecule of arbitrary form in the space groups PI, P2,, P2,/c, Pca2,) Pna2, and P2,2,2, or a centrosymmetric ~iloleculein the space groups PI, P2,/c, C2/c or Pbca. These space groups are actually those most frequently observed for molecular crystals.
A more detailed analysis of intermolecular forces
Dispersion energy The first theoretical treatment of dipersion forces is due to ond don[^] (so that they are often called London forces), who used the perturbation theory to obtain the following simplified equation for the dispersion energy E(r) of two molecules whose centres are separated by the distance r E(r) = (3/2)a;a;1,1,r~/(1,
+ I,)
(7. la)
where a; and a; are the molecular polarizability volumes and I, and I2their first ionization potentials. For identical molecules it becomes E(r) = (3/4)a'21r6
(7. lb)
showing that the attraction energy increases for molecules having high polarizability and ionization potential values and is of the general form  ~ r  ~where , c is a constant mainly determined by the value of a'.E(r) is the only attractive energy among neutral molecules without permanent dipole moment and determines all phase transition temperatures of the substance. Polarizabilities are known to increase with the molecular volume and with the number of n bonds (particularly extended systems of conjugated bonds) and are essentially a measure of how much electron clouds can be displaced from their equilibrium positions around the nuclei; higher polarizabilities imply stronger intermolecular attractions and this is the reason why, at room temperature, larger molecules give crystals, smaller ones give liquids, and only very small ones are gaseous. It may be said that dispersion forces (or more basically polarizabilities) are the true reason why molecular crystals can exist.
1
473
474
1
Gastone Gilli
Units for dipole moments and polarizabilities Magnitudes of dipole moments are generally quoted in debyes (D), where 1D = 3.336 x I O  ~ O C ~A. dipole consists of two charges +q and q separated by a distance R is calculated as p = qR and is directed from the negative to the positive charge. Taking as unit of charge the electron (le = 1.602 x 1019C) and of length the angstrom (1 A = 10'Om) or the bohr (1 bohr = 0.529177 A = a" = radius of the first hydrogen orbit) the following equivalences hold: l e A = 4.800 D and l e Bohr = 2.542 D. A moderate electric field E induces in a molecule a dipole moment p according to p = a E , where a is called molecular polarizability; p and E being vectors, a is a second rank tensor but usually only its scalar value a = (Ciai)1'2/3 is given as polarizability volume a' = a/4ne0, whose units are simply A3 = lopz4cm3. Typical values of a' are 0.82, 2.63, 1.48, and 10.5 .A3 for Hz, C12, H 2 0 , and CCl,, respectively.
Repulsion (or exchange) energy and total nonbonded energy The repulsion forces two molecules experience when their outer atoms come into contact are of quantum nature and derive from the Pauli principle; they register the impossibility for closedshell molecules to accept other electrons in their doubly occupied molecular orbitals. Unfortunately no theoretical treatment for the calculations of repulsion energies is known, so that they must be evaluated empirically and this is done according to two different approximations. In the first, the repulsion energy is expressed as a exp (br), where a and b are constants to be determined; the total nonbonded energy assumes the socalled 6:exp or Buckingham's form["] Enb(r)= a exp (br)  ~ r  ~ .
(7.2) In the second approximation the repulsion energy is of the type ar" where a is a constant to be determined and n an integer in the range 815 (usually 12); in such a case the nonbonded energy is in the socalled 6:n or LennardJones' form[lol
Atomatom potentials When the interacting bodies are atoms (e.g. noble gases) the distance r can be taken as the internuclear distance. In the case of molecules some complications arise and the atomatom approximation is most commonly used: the total interaction energy between two molecules is expressed as the sum of those among the constituent atoms. The twoatom potentials in the generalized form Enb(r)= A exp (Br)rD  Cr6
(7.4) are often named atomatom potentials. Values for the A, B, C, and D parameters are not derived from theory but determined by experiment, such as gas deviations from ideality, compressibility of liquids and solids, and neutron scattering by liquids. Otherwise, the parameters minimizing the difference between observed and calculated values of some physical quantity (typically lattice energies and cell parameters for crystals; bond distances, bond angles, and torsion angles for molecules) are used. Equation (7.4) requires four constants for any pair of atoms, which can be
Molecules and molecular crystals
1
475
a problem when the number of different atoms increases. For this reason other forms of (7.4) are used, such as which corresponds to (7.4) with B = 0, D = 12, A = &*r*12,and C = 2 ~ * r * ~ or , (k,r/r*)  k , ( ~ * l r ) ~ ] E,,(r) = ~ * [ kexp
(7.5b)
which is identical to (7.4) by putting D = 0, A = kle*, B = k,lr*, and C = ~ * k , r *and ~ where k,, k,, and k, are simple rescaling constants. For any atom i only two values are tabulated: its van der Waals radius rl and an Enb energy parameter E,, which are used to calculate the parameters of any ij interaction as r* = rl + r, and E" = (E,E,)'/~.The quantities r* and E* assume the meaning of position and depth of the potential well of the curve En, versus r (Fig. 7.4). This formula greatly simplifies data tabulation because it E* requires only two values per atom instead of three or four for each pair of atoms. Several tabulations of atomatom potentials are available and an exhaus Fig. 7.4. Meaning of the parameters eI and rl tive literature is reported in the recent book by Pertsin and ~itai~orodski.['] eqns (7.5a, b). Generally speaking, potentials are not transferable from one application to another, being more suited to fit phenomena they are derived from. Tables 7.2 and 7.3 report typical potentials used for crystal packing studies[12]and for molecular mechanics and conformational analysis calculations.[131As an example, Fig. 7.2 compares the curves calculated for the CC, CH, and HH interactions by means of the two different potentials; although the general shape and the position of the minima are similar, the agreement is rather poor. This is typical of semiempirical quantities since they do not derive from a unique theoretical fundamental but are just a set of parameters which only need to be internally consistent in such a way as to reproduce a given physical quantity; what really matters is that they work, which they usually do if used within their own range of applicability.
Electrostatic energies The study of interactions among permanent molecular multipoles is simplified by the fact that the energy involved rapidly decreases with the order of the multipole itself and it is generally admitted that the role played by quadrupoles is negligible. Even considering only the first two terms of multipolar expansion the number of terms remains relevant, that is monopole with monopole, dipole, and induced dipole together with dipole with dipole and induced dipole. However, a great simplification can be reached in some cases because interactions with induced dipoles can be usually neglected in lattice energy calculations and crystals of neutral molecules (practically the only case so far studied) do not need monopoles to be taken into account. A point of general interest concerns the value of the electric permittivity E (normally expressed as the product of the dielectric constant E, and of the vacuum permittivity E,, so that E = E,EJ which is included in all of the following equations. In interactions decreasing rapidly (e.g, with rP6 in the dispersive or dipoledipole interactions) E, is assumed to be unitary as in a vacuum because the space around the atom considered can be taken as empty within the short distance (usually 15 A) to which the calculations are
in
476
1
Gastone Gilli Table 7.2. Atomatom potential parameters according to ~ i ~ l i o to [ ' ~be' used in crystal packing calculations. Units of kcal mol'. Q represents CI or S and Me the methyl group. Potentials are of the form given in eqn (7.4) Pair
A
B x ~ o C~
D
Table 7.3. Atomatom potential parameters according to ~ l l i n g e r [ ' ~for ' molecular mechanics calculations in kcal mol'. Potentials are of the form given in eqn (7.5b) with k, = 8.28 x lo5, k2= 13.59, and k3 = 2.25 Atom
r*
E*
Molecules and molecular crystals
extended. When monopoles are involved the energy decreases only with the first or second power of distance; calculations must be extended to a wide range and the value of E, to be used becomes a complex and barely known function of the distance in consequence of the shielding effects produced around the ion by the interleaving atoms. 1. Monopolemonopole interactions occur in crystals containing ions. The interaction energy of ions i and j having formal charges qi and qj located at a distance rij is
where E = E,EO is the electric permittivity. The constant (1/4neO)depends on the units used and is 332.145 kcal mol' A e2 or 1389.70 kJ mol' A e'; it has a value of one when atomic units are used, that is energies are in hartrees (1 hartree = 627.7 kcal molI) and distances in bohr (1 bohr = 0.529177 A). 2. Monopoledipole interaction energy is calculated according to where r is the distance between the charge q and the central point of the dipole p, and @ the angle between r and the direction of the dipole. 3. The case of dipoledipole interactions is of great interest as most neutral molecules have small dipole moments associated with chemical bonds between atoms of different electronegativities, whose vector sum produces, unless it does not vanish because of symmetry, the overall molecular dipole moment. The interaction energy is calculated according to two main models. In the dipolar model the bond dipole moments are tabulated for all bonds of interest or directly calculated from the known values of atom electronegativities. The interaction energy between two dipoles pi and pj whose centres are separated by the vector q is
and the total dipoledipole energy, ED,, in the crystal is one half of the A slightly different way could be sum of all the intermolecular terms that of summing up all the small bond dipoles into the overall molecular dipole moment and of computing the total energy over all molecules. In the monopolar model the total energy is calculated as the sum of all atomic partial charges qi according to
where atoms i and j are on different molecules. Partial charges can be obtained from standard semiempirical or ab initio quantum mechanical calculations, approximate semiempirical m ~ d e l s [ ~ or, ~ ~ more ~ ' ] recently, as deformation densities[331experimentally determined by Xray diffraction. 4. Hydrogen bonding has already been treated and only potential fields for the calculation of its energy remain to be discussed. Since the Hbond is essentially ionic in nature, the total interaction energy of the fragment
1
477
478
1
Gastone Gilli
DHA (D = donor, A = acceptor) can be divided in two terms: the usual nonbonded energy, Enb, and an electrostatic (or dipolar) term that takes into account the partial charges on the donor and acceptor groups. Starting from the empirical observation that the D . . . A contact distance is practically equal to the sum of the van der Waals radii of D and A as though the H atom does not exist, it seems clear that any potential assuming a van der Waals radius of zero for the hydrogen (see eqn (7.5)) and localizing suitable partial charges (or dipoles) on DH and A will describe reasonably well the Hbonding energy, the preference for a linear DHA arrangement included, as this optimizes both the van der Waals repulsion and electrostatic attraction between A and D. This is essentially the strategy used by the potential energy fields more recently proposed for describing the bond,[^*^^] though other approaches are also
Thermodynamics of molecular crystals It is of relevant interest to obtain even an approximate evaluation of the different terms contributing to the total free energy of a molecular crystal. The discussion essentially follows the lines of the treatment given by ~ i t a i ~ o r o d s k iand [ ~ ] is restricted to the simple case of a crystal constituted by rigid molecules at atmospheric pressure. These conditions allow some simplifications. As regards the effect of pressure, the Gibbs free energy function G = H  TS differs from the Helmholtz function F = U  TS for the term pV = G  F = H  U, which is the work done by the system against the external pressure. As the coefficient of thermal expansion is very small in crystals, the expansion work is irrelevant at atmospheric pressure and we can put G = F. Moreover, if the molecule is conformationally rigid, intermolecular forces are unable to modify the internal molecular geometry and the following partitioning of the free energy is acceptable where F,, and Fmo, are the inter and intramolecular contributions to the total crystal free energy. In this approximation Fmo, could be separately calculated at any temperature from the frequencies of the internal vibrational modes of the rigid molecule by the usual methods of statistical thermodynamics; the same methods allow us to calculate another molecular quantity which will be shown to be necessary, the contribution of internal vibrational modes to the molar heat capacity, Cmo,. Within our approximations the molar free energy of the crystal can be written as U is the lattice energy or total potential energy of the intermolecular interactions. Even if the interatomic forces are temperature independent, U is temperature dependent as a consequence of the slight increase of the cell parameters with temperature, so that it must be written U(T) = Uo+ AU(T), where Uo is the lattice energy at absolute zero (a term large and negative) and AU a small positive term increasing with the temperature and equal to zero for T = 0, representing the expansion work against the internal cohesion forces. It causes a difference between the molar heat
Molecules and molecular crystals
capacities at constant pressure and volume and from this difference can be actually calculated as A U(T) = J": (C,  C,) dT. KOis the zeropoint energy, that is the crystal vibrational energy at zero kelvin; it is known that it may have some relevance only for molecules of extremely small moment of inertia (N2, 0 2 , CO) and strongly directional bonds (H20). In common crystals it is very small (=c=c\\\
Hbi4Oil
I
HWC4OH
I
a l a
\bj
1
0,
\b
b

E 0 0 ~ 7 a , b , c
/a
brc=c=c
8 a.b
1
487
488
1
Gastone Gilli
opposite directions, a property by which they can be identified and which explains their older name of optical isomers. Molecules having an internal symmetry plane cannot have enantiomers because they are their own enantiomer. In such molecules the possible diastereoisomers are often and traditionally called geometrical isomers. Common cases are planar molecules (ethylene derivatives, planar rings, and squareplanar complexes). However, geometrical isomerism is not another type of isomerism but just a particular name given to diastereoisomerism in a specific situation. The condition for a molecule to show enantiomerism (i.e. to exist as a couple of enantiomers) is that it cannot be superimposed on to its mirror image in any of its possible conformations. Such a molecule is said to be dissymmetrical or chiral. Since rotations are allowed operations in trying to superimpose the molecule with its mirror image, the most general condition for chirality is the lack of molecular rotaryreflection axes, a condition which excludes the presence of both internal symmetry centres (S2 = 1) and planes (Sl = m) . The most frequent cause of chirality is the presence of an asymmetric carbon atom, that is a tetrahedral carbon bonded to four different atoms or atomic groups as, for instance, in glyceraldehyde (5a, 5b). The number of possible isomers increases with the number of asymmetric atoms. The cr,Pdibromocinnamic acid, having two asymmetric carbons, produces four different stereoisomers (6a6d); the pairs (6a, 6b) and (6c, 6d) are enantiomers while all other pairs are diastereoisomers. Tartaric acid (7a7c) illustrates the case where one of the two enantiomeric pairs vanishes because the parent diastereoisomer has an internal symmetry plane (7c: a meso form). This last example elucidates another interesting aspect of enantiomerism. The meso form depicted in (7c) cannot exist in practice because it is a highenergy eclipsed conformation. However, any pair of right and lefthanded torsions of the same entity will generate a pair of enantiomers which are isoenergetic, independently of the shape of the potential energy curve; being isoenergetic, they will be present in the pure liquid or in solution with exactly the same populations causing the compound to be optically inactive. Chirality can be associated with a variety of other bond situations which can produce tetrahedral arrangements, as in allenes (Sa, Sb), spirocompounds, quaternary ammonium salts, or bis(benzoy1acetonato)beryllium (9a: one enantiomer shown). It can be also associated with nonaromatic cyclic systems: for example, all rings with an odd number of terms and two different nongeminal substituents have two asymmetric carbons producing two diastereoisomeric pairs of enantiomers, as shown by the cyclopropane derivative (10a10d). An example of chirality in coordination chemistry is given by the chelate octahedral complexes of the type [ C ~ ( e n ) ~ ](~l l+a , l l b ) or [cisCoC12(en),]+, where en stands for ethylenediamine. Of particular interest are pyramidal atoms, i.e. those having tetrahedral hybridization but a hybrid orbital occupied by a nonbonding pair. It was suggested many years ago that molecules similar to the amines NHR,R2 and NR,R,R, should exist in two enantiomeric forms which, however, have never been observed. The reason is that the two enantiomers (12a) and (12b) exchange rapidly in solution by pyramidal inversion through a planar
Molecules and molecular crystals
transition state having an energy higher only by a few kcal moll. Further investigations have shown than other potentially chiral compounds of trivalent phosphorus and arsenic have higher interconversion barriers and that their enantiomers may be actually resolvable, at least at low temperature. The absolute configuration of an enantiomer (i.e. its actual atomic disposition in space) is a problem which cannot be tackled by chemical methods. All attempts to obtain it from the sign of optical activity in solution, the property which is more strictly related to enantiomerism, have failed. The first absolute configuration of an enantiomer was only accom~ ~(+)tartrate ] of sodium and plished in 1951 by Bijvoet and c o  ~ o r k e r s [on rubidium by anomalous scattering methods, as discussed in Chapter 5. Since then absolute configuration determination has become routine. The nomenclature for identifying enantiomers has changed over the years and reflects the discovery of new techniques for their study. The oldest one simply reports the sign of the optical activity (+ or ); later on Fisher, in his fundamental studies on carbohydrates, discovered the stereochemical series and enantiomers were named after the series they belonged to (D or L). More recently Cahn, Ingold, and i re lo^[^^] introduced the RS nomenclature which describes exactly the spatial arrangement of groups or atoms as obtainable from Xray diffraction studies. In this context it is worthwhile to remark that chemical nomenclature has been developed for solutions and not for the crystal state, so that some misunderstandings can sometimes occur. As far as enantiomers are concerned, it is known that the usual chemical synthesis can only produce a 1:l mixture of the two enantiomers which is called racemic mixture; it can be separated (resolved) by reacting it with other chiral molecules by which the two enantiomers are transformed into diastereoisomers; only the more recent asymmetric synthesis can produce single R or S enantiomers. When a pure enantiomer crystallizes, it can only adopt a polar space group (i.e. without S, rotaryreflection axes), otherwise the symmetry element would generate the other enantiomer; this is the case, for instance, for all natural aminoacids or proteins. The crystallization of the racemic mixture may be a more complex problem. Usually the mixture is thermodynamically more stable and crystallizes as a homogeneous solid containing equimolecular amounts of both enantiomeric molecules which is termed racemate. The crystal obtained is usually centrosymmetric with the two enantiomers related by a symmetry centre, though sometimes it happens to be polar with a double (or of higher even multiplicity) asymmetric unit allocated to both enantiomers. In the rare case that the racemate is less stable than its components, the racemic mixture crystallizes in a polar space group with spontaneous resolution of the enantiomers, that is it produces two types of enantiomeric crystals, each one containing just one enantiomer (which is, incidentally, the way Louis Pasteur discovered enantiomers for the first time). This fact is the origin of a not uncommon error in structural determination, that of determining the absolute molecular configuration without taking into account the fact that the bottle from which the crystal was taken contains one half of crystals of the opposite configuration. The subject of chiral crystals can become quite difficult to understand in its generality because there are also space groups which are chiral by themselves and not because they have to allocate chiral objects (e.g. P31
1
489
490
1
Gastone Gilli and P3J. Moreover, what has been said for configurational enantiomerism has to be extended to conformational enantiomerism because conformations become fixed within the crystals. For more details the reader is referred to a more specialized treatment.[571 Going back to the other isomers, it has already been remarked that geometrical isomerism is the traditional way of indicating diastereoisomerism in molecules having an internal S,. Classical examples are cistrans isomers in ethylene derivatives (13a, 13b), synanti isomers in oximes (14a, 14b) or azocompounds (15a, 15b), cistrans isomers in square planar (16a, 16b) or octahedral (17a, 17b) complexes, and merfac (meridionalfacial) octahedral complexes (18a, 18b). Geometrical isomerism is also observed in saturated cyclic compounds where the substituents can be over or under the ring plane. For instance, fourmembered rings substituted as in (19) can only show geometrical isomerism in consequence of their internal mirror plane; accordingly (19a) and (19b) are cistrans isomers. Complete nomenclature rules for geometrical isomers are a ~ a i l a b l e . [ ~ ~ > ~ ~ ]
Conformational isomerism Conformational isomers (rotational isomers, rotamers, conformers) are the molecular states corresponding to minima of the potential energy curve expressed as a function of the torsion angle around a single bond. With reference to Fig. 7.8, states b, d, and f are conformers while a, c, and e are transition states; all are possible conformations. As is the case for all stereoisomers, conformers can have mutual relationships of enantiomerism or diastereoisomerism; so conformers b and f are enantiomers while b and c (or c and f) are diastereoisomers. The energy barrier protecting conformers is usually rather small (515 kcal moll) and much smaller than that protecting configurational isomers. For reference, the thermal activation barrier for cistrans isomerization around a double CC bond (13a, 13b) is some 40 kcal moll. However, it is not the height of the barrier that can distinguish between conformational and configurational isomers but the fact that conformers differ in a rotation around what is a single bond (even if with partial doublebond character) in the ground state of the molecule. This rule allows us to classify as conformers the enantiomers produced by hindered rotation in o, ordisubstituted diphenyls (20a, 20b), although the interconversion barrier is so high that they can be resolved at room temperature. Such resolvable conformers are sometimes reported as atropoisomers.
Ring conformations It seems reasonable to assume that a ring containing single bonds, e.g. cyclohexane, could have different conformations describable by a potential energy curve of the type shown in Fig. 7.8, having minima and maxima corresponding to ring conformers and transition states. The difficulties arise when trying to define the independent variables that the potential energy is a function of, and this for the evident reason that the torsion angles fixing the conformation are not mutually independent but related by the condition of ring closure. The problem is not easy to solve and only some basic concepts will be discussed here; the mathematical complications will be discussed in the next section.
Molecules and molecular crystals
Let us focus our attention on the origins of the energy barrier which separates the different conformers. As it will be discussed in more detail later (p. 507), the deformation of a molecule can be conceived of in terms of displacements of its bond distances, bond angles, and torsion angles from their optimal equilibrium values. The deformation energy needed rapidly decreases in the order bond stretching or compression, bond angle bending, and torsion around single bonds, while the torsion around double bonds requires energies in between stretching and bending. Since energies of single bond torsions are very small, transitions between conformations which can occur without angle bending will have an almost null activation barrier. In this case the ring is flexible because many different combinations of the two isoenergetic (degenerate) conformations become possible. The pathway interconverting isoenergetic conformations is called, for reasons to be discussed later, a pseudorotation path. Classical examples of degenerate conformations are the envelope (E) and twisted (T) conformations of cyclopenthane (Fig. 7.9) and the boat (B) and twistboat or twisted (T) conformations of cyclohexane (Fig. 7.10). The opposite occurs when it is impossible for the molecule to change conformation without bond angle deformation (or, in general, bond stretching or rotation around double bonds). In this case the molecule is rigid and its actual conformation is protected by a barrier which can be of the order of magnitude of 10 kcal mol' for saturated rings and somewhat greater if there are double bonds stiffening the ring. Figure 7.10 shows the somewhat idealized shape of the potential energy curve of cyclohexane as a function of a generalized coordinate of conformational interconversion as could be obtained by the molecular mechanics methods. The rigid conformation of cyclohexane is the chair (C), which is the most stable and is transformed into the T form through a transition state called halfchair (H) which is some 11kcal mol' higher in energy. T and B are almost isoenergetic and can be interconverted practically without any activation barrier (pseudorotation). C, B, and T are the three lowenergy conformations of cyclohexane and therefore its three conformers according to the definitions given in the previous section. The number of possible independent conformers of a ring can be determined by the use of simple considerations. A planar ring of N atoms has 2N degrees of freedom, out of which two are of translation, one of rotation, and 2N  3 of inplane vibration. Allowing the atoms to vibrate out of plane, that is the ring to become puckered, the number of vibrational
CONFORMATIONAL COORDINATE
1
491
Fig. 7.9. The two degenerate conformers of cyclopenthane (E =envelope, T = twisted) and their symmetries. The ring conformation is flexible because the t w o conformers can interconvert with zero activation energy along a pseudorotation path. Any observed conformation can be described as a linear combination of E and T.
Fig. 7.10. Idealized potential energy profile of cyclohexane as a function of a generalized coordinate of conformational interconversion as could be obtained by the methods of molecular mechanics. C = chair, B = boat, T = twistboat or twisted, H = halfchair. B and T a r e degenerate and ~ r o d u c flexible e ring conformations; C is the rigid lowenergy conformer.
492
1
Gastone Gilli
degrees of freedom becomes 3N  6 with an increment of (3N  6)  (2N  3) = N  3, which is just the number of outofplane independent vibrations or independent puckering conformers. So three four five six and sevenmembered rings should have, respectively, zero, one, two, three, and four puckering conformers. This kind of reasoning allows us to know the total number of possible conformers but not their nature, a much more difficult task to be discussed in the next section. Another qualitative consideration can be derived from the examples already given. For cyclopentane there are 5  3 = 2 conformers (E and T), which are isoenergetic or degenerate and flexible because they can interconvert along a pseudorotation path. For cyclohexane the conformers are 6  3 = 3, out of which two (B and T) are degenerate and flexible while the other one (C) is single and gives the lowestenergy rigid conformation. By generalization: a Nmembered ring has N  3 possible conformers which are arranged two by two in flexible mutually interconverting degenerate pairs; if N  3 is odd, the last single conformer is rigid and has the lowest possible energy. Accordingly, cycloheptane will have four possible conformers arranged in two flexible pairs while cyclooctane will have one more rigid lowenergy conformation, which is the ground state of the ring.
Ring conformation and group theory The problem of determining the N  3 independent lowenergy conformations (conformers) of a Nmembered ring is reducible to that of finding the normal outofplane vibrational modes of the ring, which can be easily solved by applying group theory[581 to equilateral polygons. The method will be illustrated for five and sixmembered rings and its understanding requires some previous knowledge of group theory. From a formal point of view the problem is the same as that of finding the molecular orbitals of planar rings within the Hiickel theory. Let us consider the regular hexagon of Fig. 7.11, where the outofplane displacements are represented by the small vertical arrows. The hexagon belongs to the point group D,,, whose character table is reported in Table 7.5. The reducible representation for outofplane vibrations is obtained by
Fig. 7.11. A system of coordinates for describing the outofplane vibrations of a sixmembered ring.
Molecules and molecular crystals Table 7.5. Character table for the point group D, Dgh A A ,,
E l
B,, B ,, E,l E ,, A,, A, El, B," El, E",
2C6
, l 1 1 1 1 1 1 2 1 2 1 1 1 1 1 1  1 1 1 2 1 2 1
2C3
Cz
l 1 1 1 1 1
l
1 1 1 1 1 1
l 1 1 1 2 2 1 1 1 1 2 2
i
3C;
3C;
l 1 1 1
l 1 1 1
1 1 1 1
0 0
0 0
2
1 1 1 1
1 1 1 1
0 0
0 0
2 1 1 1 1 2 2
2S3
2S6
ah
3ad
3av
1 1 1 1 1 1 1 1 1 1 1 1
1 1 1 1 1 1 1 1 1 1 1 1
1 1 1  1 1 1 1 1 0 2
1 1 1 1
2
0
1 1 1 1 1  1 1 1
2 2
0 0
xZ
+ y2, z2
R,
0 (R,, R,,) 0
(x:, yz), (X
Yr x ~ )
1 1 z 1 1 0 (x,y)
0
applying all the group symmetry operations to the six small vertical vectors of Fig. 7.11; the character for any class of symmetry operations (or column of the character table) is given by the number of small vectors not moved by the symmetry operation. It is easily seen that the characters of such representation, r 6 , are
which can be resolved by standard methods"rn a combination of the four irreducible representations (i.r.)
according to the equation r6= A,, + El, + B,, + EZu. The normal modes of outofplane vibration (or modes of puckering) are now to be found and, for the sake of clarity, let us make reference to the final results shown graphically in Fig. 7.12. The modes transforming as AZu and El, are immediately found from Table 7.5 to correspond to rigid body motions (respectively translation along z and rotation around x and y). A base for B,, (i.e. a representation transforming under the group operations as B,,) is easily found because it has to be symmetrical with respect to C, and antisymmetrical with respect to C6 and therefore corresponds to alternate positive and negative outofplane displacements (conformation C in Fig. 7.10); calling zi one of such displacements, the vibration is described by the function where 6'I2 is a simple normalization factor granting that
C iz: = 1. A base
t The number of times nithat the i.r. Ti appears in the reducible representation T' is given by
where h is the order of the group (in the present case 24) and x,(R) and x ' ( R ) are the characters of the symmetry operations Tiand T', respectively.
1
493
494
1
Gastone Gilli
Fig. 7.12. Normal modes of outofplane vibration (ring puckering) of a sixmembered ring and their symmetries. Any mode belongs to an irreducible representation of the point group D ,, and is therefore orthogonal to the others.
for E2, is not intuitive and must be found by ordinary group theory methods. A first base can be obtained by associating the outofplane displacement to atom 1 of the ring and operating on it by all symmetry operations multiplied by their characters. The required base is the sum of all the terms obtained, that is
which is a base for (or is transformed as) the boat conformation B and can be written in normalized form as As E2, is twodimensional, the degenerate partner of 4, remains to be found; it can be done by the same technique operating on z2 instead of zl and obtaining the normalized function which, however, is not orthogonal to @, because S = $ @,$J dv = 112. To make the two functions orthogonal the Schmidt orthogonalization procedure is used,? obtaining the orthogonal function required in normalized form
GT = 4112(~2+ 23  z5+ z6)
(7.19)
which is the base for describing the puckering of the twisted conformation T. GB and GT belong to the same i.r. and are degenerate, at least for infinitesimal zi displacements, and all their linear combinations are allowed
t If the two already normalized functions 4, and 4, are not orthogonal, i.e. [ 4,4, du = S # 0, the new function 4' = 4,  SG, is orthogonal to +,, as can be shown by simple substitution.
Molecules and molecular crystals solutions; this means that any linear combination of T and B conformers is an allowed conformation of the ring or, in other words, that the two conformers T and B can interconvert with zero activation energy along a pseudorotation path. It is now useful to find an analytical expression for describing the displacements z, of a ring whose puckering amplitude is (C, zf)'I2 = q. It is convenient to define the z, values with reference to the mean ring plane, which is fixed by the condition of nontranslation (C, z, = 0) and by those of nonrotation around the x and y axes; these last conditions can be obtained by equating to zero the sum of the vertical displacements weighted by the functions representing the two components of the rotational i.r. El, of Fig. 7.12, that is
2 zisin [2x(i  1)/6] = 0 i
where i can assume the integer values from one to six. Moreover, it can be verified by simple computation that the following functions give the same displacements as 4, in (7.17) and 4, and 4, in (7.18) and (7.19), and therefore are transformed by the operations of the point group D6,, as the i.r. BZgand E2, of Fig. 7.12
E;,: @,(i) = zi= 3'I2q2 cos [4n(i  1)/6]
El,: @,(i) = zi= 3112q2sin [4n(i  1)/6]
(7.23)
where 6'I2 and 3'12 are normalization factors and q3 and q2 the mean puckering amplitudes of the two vibration modes. The function describes the outofplane displacements of the C k2GTdescribes those of the conformer while any linear combination k,& degenerate B and T conformers. For the properties of trigonometric functions, such combinations can be written as
+
where 42 is a phase angle having values of 0, 60, 120, 180, 240, or 300" for the pure B conformations and 30, 90, 150, 210, 270, or 330" for the pure T conformations. Equations (7.21) and (7.24) describe analytically the conformations of a sixmembered ring in terms of the three parameters q3, 9,) and G2 and the N  3 possible conformations remain characterized as the three C, B, and T conformers. The characterizing parameters (9,) q2, G2) are more generally identified as the N  3 generalized puckering coordinates, that is the N  3 variables necessary and sufficient to define any outofplane deformation of the ring. q3 and q2 are called puckering amplitudes and G2 the phase angle and any possible conformation of the sixmembered ring corresponds to a point in the threedimensional space spanned by the orthogonal base ( q 2 , $ 2 ) q3).
1
495
496
1
Gastone Gilli For example 'C4t corresponds to 9, = q, q2 = 0, and @, undefined, while , 3 , 6 ~B4,', , 2,5B, 4C1 differs only for having 9, = 9. Moreover, 1 , 4 ~B2,s, and B3,6 have all 9, = 0, q2 = q, and @, = 0, 60, . . . , 300°, respectively, while 4T2, 6 ~ 23, ~ 1 'T4, , ' T ~ , and 'T, still have 9, = 0 and 9, = q but $J2 = 30, 90, . . . , 330") respectively. The actual value of q = (C, z?)li2 is determined by the equilibrium value of the bond angle, a , defined by the ring atoms. It is selfevident that q will be zero for an equilateral hexagonal ring having a = 120" and it can be shown that 9, is equal to 6 6 ' " ~ for an equilateral C ring of side R and tetrahedral internal ring angles (e.g. cyclohexane) . It has already been remarked that any possible ring conformation is defined by the triplet of values (q,, $J2,9,) in a Cartesian system of axes; otherwise these coordinates can be expressed as polar coordinates (Q, 0, $1, where Q is the total puckering amplitude defined as
and
= @2,while 0 is an angle in the range 0  ?G such that
q2 = Q sin 0 and 9, = Q cos 0.
300 
5 

2 ) l ' (
(")
Fig. 7.13. The three activated states of puckering of a sixmembered ring and their symmetries (E = envelope, H = halfchair, S = screwboat).
(7.26)
In this way any conformation is represented by a point on a sphere of radius Q, 'C4 being at the north pole ( 0 = 0", $J undefined) and its enantiomer 4C1 at the south pole, while B and T interconvert along a pseudorotation path which is on the equator (6 = 90") in correspondence to all possible values of @. The previous discussion was mainly concerned with the lowenergy conformers C, B, and T. The ring, however, also has highenergy transition states and there is general agreementUs9]that these are the envelope (E), halfchair (H), and screwboat (S) conformations of C,, C2, and C2 symmetry, respectively, as shown in Fig. 7.13. Cremer and ~ o p l e [have ~~] shown that the E and H forms are located at tan 0 = fv(3/2) and fv 2 , respectively, and ~ o e y e n s [ ~that ' ] the S form occurs for tan 8 = f(1 v2). This last author has reported a complete map of the six conformations, usually called canonical, in polar coordinates, which is reported in Fig. 7.14 with some modifications. The figure has the further meaning that all maximum circles indicated are possible interconversion among conformations. The TB pseudorotation circle is the equator, while along the meridians the C conformation is converted to B through E or to T through H and S. The problem of the conformations of a fivemembered ring can be solved by the same methods. The ring has only two puckering coordinates because N  3 = 2; it belongs to the point group D,,, whose character table can be obtained from any group theory text. The reducible representation for the outofplane vibrations is
+
t According to the nomenclature usually employed, the conformations chair, boat, and twisted (or twistboat) are called C, B, and T and the atoms which are over or under the mean plane of the ring are indicated by upper left or lower right indices. So, 2 3 5 is~ a boat ring having the atoms number two and five directed upwards and B,,, its enantiomer while *T, is a twisted ring with the second atom pointing up and the fifth one pointing down.
Molecules and molecular crystals
1
497
Fig. 7.14. Polar projection of the northern part of the sphere reporting, for an arbitrary value of Q , the positions Band $C of the canonical conformations of a sixmembered ring. The southern hemisphere contains the enantiomeric conformations in centrosymmetric positions.
+ +
which can be decomposed as T, = A'! E'; Ei, where A; and E;' correspond to translation and rigid body rotations, respectively. The puckering modes belong to the twodimensional i.r. E; and a base for them, found by the usual methods, is shown in Fig. 7.15. The two conformers found, envelope (E) and twisted (T),are degenerate and all their linear combinations are possible conformations on a pseudorotation pathway. By analogy with (7.207.24) the nontranslation and nonrotation conditions are
Fig. 7.15. Normal modes of outofplane vibration (ring puckering) of a fivemembered ring and their symmetries. E =envelope, T = twisted.
zicos [2n(i 1)/5]= 0, i
zisin [2n(i 1)/5]= 0, i
and the functions describing the puckering displacements are
@=(i)= zi= (2/5)lIzq2sin [4n(i  1 ) / 5 ] ,
(7.29)
where i can assume all integer values from one to five and (2/5)'12 is a normalization factor providing that C iz? = q:, q2 being the puckering amplitude. Since E' is twodimensional, any linear combination k1GE+ k2GT belongs to Ei and can be written as
(
498
Gastone Gilli
4,C;3E
where 4, is a phase angle having values of 0, 36, 72, 108, 144, 180, 216, 252, 288, and 324" for the ten E conformations and 18, 54,90, 126, 162, 198, 234, 270, 306, and 342" for the other ten T conformations, intermediate values of @, corresponding to mixtures of the two along the pseudorotation path. The complete pathway is shown in Fig. 7.16.
'T,
1~
30
4
~
"v
$2
E
A
*,
YJT4 Computation of puckering coordinates
FE 3
d
:
EI
4
T~
Fig. 7.16. Pseudorotation wheel describing the conformations which can be assumed by a fivemembered ring during the changes of the phase angle $,.
The theory given in the previous section concerns equilateral and isogonal rings. However, the equations obtained can also be used for irregular rings without loss of generality, at least as regards the Cremer and Pople treatment,[601which makes use of the displacements zifrom the ring mean plane. Other methods using the values of the endocyclic torsion angles (e.g. that proposed by Altona et al.[621for fivemembered rings) may not have the Same degree of generality. Several Computer programs[63264] are available for the computation of the puckering parameters according to Cremer and ~ople.[~'] The procedure usually includes: transformation from crystal to orthogonal coordinates; passage to the system of coordinates defined by (7.20) or (7.27), having their origin at the centre of gravity of the ring, the z axis perpendicular to the mean ring plane and the y axis passing through the first ring atom; determination of the parameters q and $J (or Q, 8, and $) satisfying eqns (7.21) and (7.24) or (7.30). An example of application to the fructose and glucose rings of the molecule of sucrose is reported in Table 7.6. The fivemembered fructose ring has q2 = 0.353 A and G, = 265.1". By comparing the calculated value of Gz with those of Fig. 7.16, it is found that the ring conformation is very near 4 ~ with 3 a small component of E3. The sixmembered ring has a Q value of 0.556& i.e. it is more puckered than the fivemembered ring. The calculated values of 8 = 5.2" and $ = 183.7" indicate, when compared with Table 7.6. Atomic coordinates and puckering parameters for fructose and glucose rings of the molecule of sucrose (coordinates from Brown and Levy, Acta Crystallographica, 839, 790 (1973)) Atom
N
Orthogonal coordinates
Puckering coordinates
Puckering parameters: q, = 0.353 A,
Puckering parameters: q, = 0.050 A, q, = 0.554 A 0 = 0.556 A,
4,
+, = 265.1"
= 183.7"
8 = 5.2", @I = 183.7"
Molecules and molecular crystals those of Fig. 7.14, that the ring conformation is an almost perfect 'C, with a and E,. very small distortion towards 5H4
Molecular geometry and the chemical bond An overview of bond theories One of the central topics of structural chemistry concerns the interpretation of the observed molecular geometries in terms of the existing theories of chemical bonding. Theories derived from the fundamentals of quantum chemistry include ab initio[65,661and ~ e m i e m p i r i c a l [ ~ ~methods. ~~] In principle both classes of methods (in particular the first ones) are able to reproduce all the details of the experimental geometries with the great additional advantage of giving them a theoretical justification in terms of molecular orbital energies, shape, and symmetry. The main difficulties arise from the great complexity of the calculations involved even for molecules of relatively small dimensions. The situation is not so different from that discussed in connection with the problem of molecular structure determination by microwave spectroscopy or gas electron diffraction. Great accuracy can be achieved at a reasonable cost of both human effort and computer time only for molecules of very small dimensions in comparison with those Xray crystallography is used to deal with. Another important aspect concerns the objective difficulties many crystallographers may have in understanding the fundamentals of quantum chemistry needed for a not completely acritical use even of the most known and generally available compter programs (e.g. GAUSSIAN[~~] for the ab initio programs or MIND013, MNDO[~"and AM^[^'] for the semiempirical ones). It is then not surprising that, in spite of the fact that quantummechanical calculation programs have been implemented in most molecular graphics systems commercially available, the most popular bond theories used in interpreting molecular geometries remain the qualitative or semiquantitative theories, that is those always based on quantum chemistry but with the different aim to produce concepts of easier application for practical scientists. It is these theories which will be briefly reviewed here.
1. Valence bond (VB) In VB theory the molecular geometry is interpreted in terms of the concepts of hybridization and separability of localized a bonds and localized or delocalized n bonds. The x bond delocalization is treated by means of the concept of resonance between canonical forms, through, more recently, the Huckel molecular orbital method limited to the n electrons (Pi H M O ) [ ~has ~ ] been frequently employed. The idea of localized bonds is the logical foundation of molecular mechanics (see p. 506ll), which gives an interpretation of the molecular geometry in terms of balls (atoms) connected by springs (the chemical bonds), and, as previously discussed (see p. 486), is the basis of all definitions of classical stereochemistry. 2. Valence shell electron pair repulsion (VSEPR) theory.[763771 This is probably the most used qualitative tool for the interpretation of the shapes of molecules containing maingroup elements, while its applicability to compounds of transition elements is rather limited. The VSEPR model has
1
499
506)
1
Gastone Gilli
been considered destitute of theoretical background for a long time and only recently has it been interpreted in terms of basic quantum chemistry.[781 3. Transition metalligand bond theories. The VB and crystal field (CFT)[~~~'] theories were the first ones to try an interpretation of structure and bonding in coordination compounds. The introduction of molecular orbital methods in coordination and organometallic chemistry has given origin to the ligand field theory ( L F T ) , [ ~ ~which , ~ ~ ] is of great value for the understanding of the energetics and geometry of these compounds. A specific semiquantitative tool developed in the frame of LFT for calculations concerning electronic spectra, magnetic properties, and equilibrium geometries has been the so called angular overlap model ( A O M ) , [ ~ ~ ~ ~ ] whose application has been successively extended to the study of the molecular geometry of compounds of maingroup 4. Qualitative molecular orbital theories (QMOT). The first attempts to interpret geometries of simple compounds of the AB2 type in terms of molecular orbitals were made by ~ a l s h . [ His ~ ~ ]method was successively extended to a series of small molecular systems, such as AB3, AB4, A2B4, A2B6, functional groups, e t ~ . [ ~ ~h ~ e, ~development ~ , ~ ~ ~ of~ QMOTs ~ ] in interpreting molecular shapes has been paralleled by the great impact these theories have had in the field of organic chemical kinetics (frontier orbitals Moreover, QMOTs are having increasing applications in the interpretation of the geometry of organometalic compounds by the methods developed by ~ o f f m a n n , [ ~which ~  ~ ~are ] based on the partitioning of the molecule into fragments and which are of semiquantitative nature as molecular orbitals are evaluated by E H T (extended Huckel theory),[951an extension of the classical Hiickel method taking into account also o electrons.
5 . Perturbative methods. These are based on the firstorder (FOJTE) and secondorder (SOJTE) JahnTeller effects. F O J T E [ ~ ~ is] of great importance in understanding the geometrical distortions which lower the molecular energy by removing the orbital degeneration[971and has found its most typical applications in the study of the coordination polyhedra of d9 c ~ m ~ l e x e s .The [ ~ ~SOJTE , ~ ~ ~ has similar applications but in closedshell molecules. It has been mainly developed by earso on['^^] extending a first paper by arte ell;['^'^ it has been extensively used for predicting geometries of compounds of maingroup elements.[862871
6. Other qualitative theories. A rather simple model which has provided remarkable agreement between experimental and predicted structures is the hard sphere model proposed by ~ a r t e l l [ l ~and ' ] developed by ~ l i d e w e l l . [ ' ~ ~ ] It makes the hypothesis that molecular geometry is mainly determined by the repulsions among first nonbonded neighbours, each having an individual nonbonded radius. Other theories having a more limited range of application have been proposed, such as the three centrestwo electrons bond in boron chemistry, the trans influence in square planar complexes or the theories based on the acidbase concept, which have proved to be of great utility in interpreting charge transfer effects in molecular crystals and have been reviewed by several In view of the concise character of the present exposition, it has been decided to limit the discussion to the VSEPR and VB theories, which are
Molecules and molecular crystals
1
501
certainly the most popular models used in structural crystallography. Moreover, only compounds of maingroup elements will be taken into account.
The VSEPR The VSEPR theory assumes that the relative ligand arrangement around a central atom is determined by the mutual repulsions of bonding or nonbonding (lone) pairs of electrons. Bonding and nonbonding pairs are identified from the Lewistype electronic structure of the molecule. The method can be summed up in the following few rules: Rule 1. Electron pairs repel each other and adopt the geometrical disposition which minimizes mutual repulsions; Rule 2. Lone pairs take more room than bonding pairs; Rule 3: The space occupied by a bonding pair decreases with the increasing electronegativity of the substituent; Rule 4. The two bonding pairs of a double bond (and, more so, the three bonding pairs of a triple bond) occupy more space than a single bond does. Calling A the central atom, X the bonding pair (or the generic ligand connected by it) and E the nonbonding pair, Rule 1 can be used to predict the geometry of a large number of compounds (Fig. 7.17). BeCl,, BF,, and CF, are AX,, AX,, and AX, molecules and will have linear, trigonal, and tetrahedral geometries, respectively. Molecules of type AX3E (NH,, pH3, NF,, PF,, or AsC1,) are pyramidal and those of type AX,E, (H20, H2S, H,Se, or OF,) are bent (angular). Molecules of the type AX, may be either trigonal bipyramidal, or square pyramidal. According to VSEPR calculations, the first geometry is slightly more stable and, in fact, AX, molecules (PF,, AsF,, and PCl,) are usually trigonal bipyramidal. Finally, molecules belonging to the types AX, (e.g. SF6) and AX,E (e.g. IF5) display the expected octahedral and square pyramidal geometries. For AX4E (TeCI,, SF,), AX3E2 (ClF,, BrF,), and AX2E3 (XeF,, IC1;) it is necessary to establish whether the nonbonding pairs are in the axial or equatorial positions of the trigonal bipyramid. According to rule 2 the nonbonding pair takes more room and should prefer the equatorial position where it makes angles of 120, 120, and 90" with the vicinal electron pairs (the three angles would be 90" for the axial position). Similar considerations predict that AX,E, molecules (e.g. [ICl;]) are square planar with the nonbonding pairs in trans positions. An interesting feature of VSEPR is its ability to interpret fine structural details. For example, Rule 2 predicts that increasing substitution of X by E will cause a narrowing of the remaining XAX angles because of the greater space taken by the lone pairs. The effect is generally observed, as exemplified by the series CH, (AX,), NH3 (AX,E), and H 2 0 (AX2E2) where the XAX angle decreases in the order 109.5, 107.3, and 104.5". Rule 2 can be considered a particular case of Rule 3 since the nonexistent substituent E can be thought of as the least electronegative of all the possible X ligands. This last rule is thus the most suited for understanding the angular changes caused by substitution and predicts that the XAX angle decreases while the electronegativity of X increases. Although a few exceptions are known, the effect is correctly observed in a variety of cases. For example, the XAX angle is 103.8 in OF, and 104.9 in H,O, 102.1 in NF, and 106.6" in NH,. In the halides of the maingroup
AX,
AX3E
AX2E2
AX,
AX,E
AX3E, AX2E31
AX,
AX,E
AX,E2
L Fig. 7.17. Prediction of the shape of simple ~ ~ ~ ~ ~ e R :Ectron ~ ~ ~ pairs (lone pairs), TP =total number of electron pairs(bondingandnonbonding); HYB=typeof VB hybridization.
502
1
Gastone Gilli
elements of the type AX2E2or AX3E the bond angles are known to increase in the order F < Cl < Br = I. Another well documented[1061series of electronegativitydependent angular variations concerns the monosubstituted benzenes. The endocyclic CCC angles in ipso (that is that carrying the substituent) changes with the substituent itself, being 117.2 for N(Me),, 118.1 for CH,, 120.00 for H (unsubstituted benzene), 121.4 for C1, 121.8 for CN, and 123.4" for F. It is evident that the angle is wider the greater is the electronegativity of the substituent group. Rule 4 explains why the bond angles trans to a multiple bond are smaller than usual, as can be illustrated by some examples in the X2A=Y system. The XAX angle should be 120" in the absence of perturbing effects but becomes respectively 108 and 111" in F2C=0 and C12C=0, where both the doublebond repulsion and the high electronegativity of the substituents contribute to the squeezing of the angle. The effect of the double bond is better seen when the X substituent is less electronegative, for example in H2C=0 and (NHJ2C=O, where the XCX angle is 108" in both compounds.
Valence bond (VB) theory[5,73,741 The VB theory is too well known to require a detailed exposition and only some aspects concerning the interpretation of molecular geometries will be discussed here. The mutual orientation of the bonds departing from a central atom is interpreted in terms of hybrid orbitals (HO), which are linear combinations of the atomic orbitals (AO) of such an atom; typical sp, sp2, sp3, sp3d, and sp3d2 HOS assume relative orientations which are respectively linear, trigonal, tetrahedral, trigonal, bipyramidal, and octahedral (Fig. 7.17) and the overlapping of the HOs with the correct AOs of the bonded atoms generates the frame of the a bonds within the molecule. After the formation of all the a bonds between the central atom and its surrounding ligands, the generic set s'pmdn of hybrid orbitals can allocate only (1 m + n ) bonding or nonbonding (lone) pairs, which require twice as many valence electrons. The hybridization state of the central atom remains determined by the total number of valance pairs available, while its connectivity is also affected by the number of nonbonding pairs which occupy an H O without adding any bonded atom. Moreover, electron pairs implied in n bonding are irrelevant for determining the hybridization state. So, CH,, NH,, and H 2 0 have all eight valence electrons (sp3 hybridization) but only CH, is tetrahedral while NH3 is pyramidal (one nonbonding pair) and H 2 0 is bent (two nonbonding pairs). Application of these rules to the examples of the previous section shows that VB gives exactly the same results obtainable by the use of VSEPR theory (see Fig. 7.17). In VB theory the double bonds do not affect the shape of the molecule, which is strictly determined by the net of its a bonds. Double and triple bonds are conceived of as a bonds to which one or two further n bonds are added and the only effect of such an addition is to shorten the bond distances. The idea of single or multiple localized bonds between two given atoms is clearly an oversimplification of thexomplex manybody interactions between nuclei and electrons within the molecule. However, it has proved to be accurate enough to allow tabulations of characteristic bond
+
Molecules and molecular crystals Table 7.7. A selection o f characteristic b o n d distances i n organic molecules ( i n A); R = alkyl, A r = aryl, ar = aromatic CC CC rC
C N rN r=N C0
C0
r0 CS rS CSi
sp3sp3 sp3sp2 sp3sp aromatic )*c( )C=C=C( )C==C=C=C( sp3sp3 R0R RCOOR RCOOH RCOOR C(ar)OR RCOO)c=O =C=O C(sp3)SC(sp2)Sc(sp3)~i
1.54 1.51 1.46 1.39 1.33 1.31 1.28 1.20 1.47 1.27 1.16 1.43 1.34 1.31 1.44 1.36 1.25 1.20 1.16 1.82 1.76 1 .7l 1.87
CP CH C F CCI CBr C l NH 0 H SS 00 NN N=N N0 N=O
c(sp3)P C(sp3)H C(ar)H c(sp3)F C(sp2)F C(sp3)CI c(spZ)CI C(sp)CI c(sp3)~r C(sp2)Br C(sp)Br C(sp3)l C(sp2)l RSSR ROOR ) NN ( N=N) NO)N+O NO2 N=O
distance^[^^'^^^] which are reasonbly reproducible from molecule to molecule. Table 7.7 reports a selection of characteristic bond distances observed in organic molecules.
Bonds of intermediate multiplicity are interpreted within the VB theory in terms of resonance, as shown for the simple cases of benzene (7.1) and carbonate ion (7.11). The structure of the molecule is represented as a resonance hybrid between different limit forms, called canonical. The hybrid justifies the fractional bond order, for instance 1.5 in benzene (7.1) and 1.33 in the C0 bond of the carbonate ion (7.11). Such a fractional number has been called bond number, n, by pauling,['I who has proposed different formulae for its evaluation. The most used is Ad = d(n)  d(1) =  c log,, n
(7.31)
where d(1) and d(n) are the distances of a single and nple bond, respectively, and c is a constant to be determined. Some applications of this equation will be discussed in the last part of this chapter. VB is particularly suited for rationalizing small changes of bond distances and angles in terms of substituent electronegativities. The discussion follows the treatment given by ~ e n t [ " land ~ starts from the elementary consideration that sp, sp2, and sp3 hybrids have decreasing s character (50, 33, and 25 per cent, respectively). This leads to important consequences: 1. Since the s A 0 is at a lower energy than the p orbital, the
1
503
504
1
Gastone Gilli
electronegativity of an atomic valence increases with the s character of the valence itself, that is an atom binding by one of its sp HO is more electronegative than when it binds by an sp2 HO or by an sp3 HO. If the HO in question allocates a nonbonding pair (NB), the basicity of the atom will be affected according to the rule that the greater is the s character of the HO donating the lone pair, the worse will be the atom as a donor. Accordingly ketones, where the lone pair is on an sp2 HO, are weaker bases than ethers, where it is on an sp3 HO. Likewise nitriles RC=N are weaker bases than pyridine C,H,N, that, in turn, is weaker than ammonia NH3, in agreement with the fact that nitrogen hybridization changes from sp to sp2 to sp3. 2. The best superposition of two ns AOs occurs at a smaller internuclear distance than that between np AOs and then bond distances become shorter with the increasing s character of the HOs involved. In fact the CH bond is 1.09 in methane, 1.O7 in ethylene, and 1.O6 A in acetylene, the single bonds C(sp3)C(sp3), C(sp3)C(sp2), and C(sp3)C(sp) have decreasing bond lengths of 1.54, 1.51, and 1.46 A and, finally, doublebond distances decrease along the series ) C=C( , ) C=C==C( , and ) C=C=C==C( in the order 1.33, 1.31, and 1.28 A. It may be remarked that this contraction is not a constant for all the elements but seems to increase with the electronegativity of the atom, as shown by the series carbonhalogen in Table 7.7. 3. The bond angles steadily increase with the increasing s character of the HOs, the angle between sp3, sp2, and sp HOs being respectively 109.47, 120, and 180". Smaller changes caused by electronegativity differences are rationalized by the socalled Bent's rule:11111The p character of an atom tends to concentrate in its HOs pointing towards more electronegative substituents, the effect being stronger the less electronegative the atom itself is. All the substituents can be arranged, starting from the lone pair, in order of increasing group electronegativity and the narrowest bond angles will be those implying the most electronegative ligands. The effect is well documented. The X0X angle is 111, 109, 104.9, and 103.8" in (CH3)20, CH30H, H 2 0 , and F 2 0 , but only 100 and 92" in CH3SH and H2S in view of the smaller electronegativity of sulphur. In the AX3 series the XAX angle is 109, 106.6, and 102.1" in N(CH3)3, NH3, and NF,, 100 and 93.3" in P(CH3)3 and pH3, 96 and 91.5" in As(CH,)~and ASH,. Bent's rule is the VB equivalent of Rules 2 and 3 in the VSEPR theory and it can be shown to include even Rule 4. In the Y=AX2 fragment the n bond contributes to shorten the X=Y bond length, causing a parallel increase of s character in the a bond and, in turn, an increase of the p character of the HOs pointing to the X substituents so that the XAX bond angle is narrowed.
Hybridization. The machinery A generic HO is a linear combination of AOs,
4,
and the problem consists of finding the set of aij values matching the required molecular fragment geometry. A few rules allow us to set up a
Molecules and molecular crystals
system of linear equations: 1. The coefficients must be such that any HO is transformed into one of its equivalent orbitals by all the symmetry operations of the fragment. 2. The HOi must be orthonormal, that is
3. Since the atomic orbitals @ j are orthonormal the sum over all HOs of the squares of the coofficients of any @ must be unitary, that is
Ci a; = 1
for any j.
As an example, let us build up the three trigonal HOs in the plane (xy). The axes are chosen in such a way that HO, points along x and H 0 2 and HO, are in the (x, y) and (x, y) quadrants, respectively. Let us write the HOs as
The s orbital has spherical symmetry and must be equally shared by the three HOs; since C ia: = 1 for condition (3), it must be that a, = a, = a, = 11Y3. c, is zero because p, is orthogonal to HO, in view of the axes chosen and therefore a: b:= 1 for (2), so that b1 = 21v6. Since H 0 2 and H 0 3 are symmetrical with respect to the a, containing x and c: c: = 1, it results that c2 = c3 = 1/v2. Likewise b2 = b, = 1Iv6 because of condition (2). The final HOs are
+
+
HO, = 1/Y3 s + 21v6 p,, H 0 2 = 11Y3 s  1 l v 6 p, + 1 / v 2 p,, H 0 3 = 1 / v 3 s  l / v 6  1/Y2 p,.
(7.36)
It is easy to check that condition (1) is fulfilled for all the symmetry operations of the point group D,, that the trigonal AX, fragment belongs to. The hybridization index n of each HO is defined as the ratio between the sum of the squares of the p A 0 coefficients and the square of the s coefficient. In this case n1 = n2 = n, = 2 and the hybridization is termed sp2. Alternatively, the s and p characters (S and P, respectively) of the HO can be used, as defined by the conditions n = PIS = P l ( 1  P ) = (1  S)/S and S P = 1 and by the inverse relationships S = ll(n + I), P = nl(n 1). In the present case S = 0.33, and P = 0.666. By the same methods it can be calculated that the two spHOs (n, = n2 = 1) oriented along x have equations HO1 = (s + p,)/v2 and H 0 2 = (s  p,)/v2 and that four equivalent sp3 HOs (n, = n2 = n, = n4 = 3), oriented in such a way that each HO makes the same angles with the
+
+
1
505
506
1
Gastone Gilli
Cartesian axes, have equations
T /*p;, , 0
/
,
a
 Y
Fig.
4
,.,*.
1 I I
 , /
I
,
Ir
X
HO,
I
HO,
a
   
I'
"02
Y
1'
Definition of the coordinate system and labelling of the relevant angles between hybrid orbitals in the AX2Y2 (left) and AX2Y (right) systems discussed in the text.
Both HO coefficients ail and hybridization indices n have been worked out starting from symmetry considerations. If the HO geometry is not exactly linear, trigonal, or tetrahedral the n values are no longer integer but become fractional numbers and not necessarily equal. Equations for the calculus of the ail and n values have been reported[11231131 for some particular geometries, that is the quasitetrahedral systems AX2Y2 of symmetry C2, and AX2YZ of symmetry C, and the planar quasitrigonal AX2Y system of symmetry C,,. For the AX2Y2system of C2, symmetry (left side of Fig. 7.18) it has been shown that n, = n2 = sec a , n3 = n, = sec /3 and that the angles a and /3 are related by the equation cot2 (a/2) cot2 (/3/2) = 1. By putting a = 109.47" we obtain nl = n2 = n3 = n4 = 3, /3 = 109.47", S = 0.25, and P = 0.75 for any HO, in agreement with the theory. In the water molecule ( a = 104.9") the two HOs pointing to the hydrogens have n =3.89, S = 0.20, and P = 0.80 and the angle between the lone pairs is calculated to be /3 = 114.8", in agreement with Bent's rule because the p character is found to concentrate on the HOs pointing to the more electronegative substituents, that is the hydrogens. The opposite case occurs in (CH3)20, where the methyl is an electron donating group; the observed angle a is 111°, allowing us to calculate that n = 2.79, S = 0.26, and P = 0.74 for the HOs directed towards the CH, groups and /3 = 108". In the planar system AX2Y (Fig. 7.18, right side) the important relationships become nl = n2 = sec cu and n, = tan2 (ct.12)  1. Only if cu = 120" it will be that nl = n2 = n, = 2, while n1 = n2 > n3 for a < 120" and nl = n2 < n, for a > 120". Since a is smaller or greater than 120" when H 0 3 is directed towards substituents less or more electronegative, Bent's rule is obeyed. These few examples can help to illustrate some interesting and not always well understood aspects of VB theory that can be summarized as follows:
+
(1) The hybridization indices are, in general, fractional numbers which become integers only for a few very special geometries;
(2) the hybridization indices and the p and s characters of the HOs are straightforwardly calculable from the bond angles and vice versa; (3) Bent's rule is not a simple qualitative rule but can be quantified, at least in a number of simple cases.
Molecular mechanics Molecular mechanics is a method for calculating the equilibrium geometries and other properties of ground state molecules on the basis of a purely classical mechanical model. The molecule is considered to be a set of atoms connected by elastic springs, and to any internal molecular coordinate (bond
Molecules and molecular crystals
distances and angles, torsion angles, distances between nonbonded atoms, etc.) is assigned a natural equilibrium value. To any displacement Ax from the natural value is associated a restoring force proportional to the displacement itself, F = k AX, and an energy proportional to its square, E = k(Ax)'/2. Molecular mechanics is essentially an attempt to assign parametric values to all natural equilibrium values and force constants k, whose complete set is called a force field and whose knowledge will allow us to calculate the potential energy hypersurface for the movement of the atoms within the molecule. The energy calculated assumes the meaning of the deformation or steric energy of a particular geometry of the molecule with respect to its equilibrium geometry. The values of the parameters defining the force field are obtained empirically by comparison of observed and calculated molecular geometries. Other properties can be optimized as well, most frequently the formation enthalpies and the vibrational frequencies. In particular a force field able to calculate both geometries and frequencies is called a consistent field. The central point remains that of being able to calculate the properties of the maximum number of different molecules using the minimum number of constants transferable from one molecule to another. The present discussion is necessarily concise and more details can be obtained from r e ~ i e w s [ ~ ~and ~ ' ' ~books['23,1241 ] available on the subject. Several molecular mechanics computer programs are distributed by QCPE (Quantum Chemistry Program ~ x c h a n ~ e ) . [ ~ ' ~ ] The total energy, E, is considered to be the sum of different contributions
which are, in the order, the stretching, bending, stretchingbending, outofplane bending, torsion, nonbonded, and electrostatic energies and have the following meaning: 1. Bond stretching. The total energy of stretching or compression of all chemical bonds of the molecule is of the form N
Es = (112)
C ks,i(Al,)'
(7.38)
i=l
where the sum is extended to all the N bonds within the molecule, ks,i are the differences between the their stretching force constants and Ali = li actual and equilibrium bond lengths. This model tends to overestimate the energy needed to produce very large lengthenings because, in such a case, the bond becomes increasingly yielding in consequence of the decreased overlapping of orbitals. It is common practice to add a small cubic term of the type k , , , ; ( ~ l ~ )where ~, kScjiis a small negative constant taking into account this last effect. 2. Bond angle bending. Its total energy is expressed as
where the sum is extended to all the M bond angles, AOi = Oi  Oo,; are the differences between the actual and equilibrium bond angles, and kb,i the bending force constants. Bending energies are smaller than stretching energies by an order of magnitude because angles are much more yielding
1
507
508
1
Gastone Gilli
than distances. Also in this case a cubic term can be added, which is of the type kb,,i(h8i)3and where kbc,iis a small negative constant. 3. Stretchingbending terms. An improved force field is obtained if proper allowance is made for the fact that the narrowing of a bond angle is paralleled by the legthening of the two encompassing bonds and vice versa. If 8i,ABcis the angle delimited by the bonds li,ABand li,BCconnecting the three atoms A, B, and C, the stretchingbending energy is defined as
A
C
B
H
/
O

where ksb,iare the corresponding force constants and Ali and AOi have the usual meaning. The term Esbis small in comparison with the previous terms and is neglected in some force fields. A field containing it is called a valence force field; this differs from the UreyBradley force field which presents a different treatment of the A . . . C geminal interactions and is not discussed here. A~   c P> B
Fig. 7.19. inplane and outofplane deformations of a trigonal sp2 atom.
o
4. Outofplane bending. In the deformations concerning trigonal sp2 atoms it is useful to distinguish between inplane and outofplane deformations (Fig. 7.19). The inplane deformations concern the angles APB, AP0, and BP0 and are dealt with by eqn (7.39), while the outofplane deformations are the displacements from zero (A8) of the angles CAP, CBP, and C0P. The associated energy is
for any single sp2 atom of the molecule. 5 . Torsions. All force fields include energy terms accounting for the rotations around bonds. The corresponding force constant is relatively large for rotations around double bonds but very small for rotations around single bonds. A common expression for the torsional energy is
E , = C [Vl(l + cos @)I2+ V2(1 cos
[email protected])/2+ V3(1+ cos
[email protected])/2] (7.42) where @ is the torsion angle (180" s @ s 180°), V,, V2, and V3 are the force constants, and the sum is extended to all sequences 1234 of bonded atoms in the molecule. The second term has the value zero for @ = 0 and f180" and maxima for @ = f90; it is used to describe the rotation around double bonds and in this case V1 = V3 = 0. The third term is equal to zero for @ = f60°, f180" and has maxima for @ = 0, f120"; it describes the rotation around single bonds connecting sp3 atoms. The first term is zero for @ = 180°, has a maximum for @ = 0°, is used as a small corrective term in special cases, and is often neglected. 6. Nonbonded interactions. The corresponding energy, Enb, can be expressed by the atomatom potentials discussed on p. 474. The interactions among all the atoms of the molecule are taken into account, with the exclusion of those between first neighbours (12 or bonded atoms) and second neighbours (13 or vicinal atoms). Thirdneighbour (or 14) interactions are considered in both the Enband E , terms. Special treatment
Molecules and molecular crystals has sometimes been reserved for the lone pairs on etheric oxygens or aminic nitrogens by considering them as pseudoatoms localized at about 1A from the atom and having their own atomatom potentials. 7. Electrostatic interactions. It has already been shown on p. 477 that electrostatic interactions can be evaluated as interactions among partial charges localized on the atoms or among small dipoles associated with each chemical bond. Both methods are used in molecular mechanics. A relevant number of different force fields proposed by different a ~ t h o r s ' ' ~are ~ ]currently available and Table 7.8 reports, as an example, the
Table 7.8. Force field parameters for alkanes and nonconjugated alkenes according to M M ~ / M M P ~ . [ ' ~Force , ' ~ ~constants * ' ~ ~ ~ i n kcal mol' A2 or i n kcal mol' deg'; bond moments (b.m.) in D. In the symbol (e,),, n indicates the number of additional hydrogen atoms bonded to the central atom. I= C(sp3), 2 = C(sp2), 3 =H. Final energies i n kcal mol' 'Stretching' Atoms
111 113 313 112 212 213 121 122 222 123 223 323
(k,, = k,) k,/2 lo
0.0083 0.0053 0.0042 0.0083 0.0083 0.0053 0.0083 0.0083 0.0131 0.0053 0.0053 0.0042
109.47 108.50 112.80 109.47 109.47 108.50 116.60 121.70 120.00 119.50 120.00 122.40
b.m.
110.51 108.51 111.10 110.51 110.51 108.51 120.50 118.80
'Stretchingbending' k,, Atoms
'Torsions' Atoms
4
110.20 107.90 109.47 110.20 110.20 107.90
'Outofplane bending' Atoms ko0&
&
5
'Nonbonded interactions' Atom ri Ei
1
509
510
1
Gastone Gilli parameters used by the program M M ~ / M M P ~for [ ~ ~hydrocarbons. ] The parameters of any force field are optimized to reproduce the experimental geometries of some reference molecules and used for predicting those of other chemically similar molecules. A force field developed for the alkanes will reproduce their observed geometries with a precision comparable with the experimental e.s.d. For other classes of molecules, such as alkenes, alcohols, ethers, thioles, esters, carboxylic acids, etc., the agreement between observed and calculated quantities is definitely worse in view of complications arising from the treatment of ndelocalized systems, partial double bonds, lone pairs, intramolecular hydrogen bonding, or highly polar groups. The discrepancies increase again when attempting to develop a force field able to deal with several functional groups at the same time and its seems unlikely that a universal field of sufficient accuracy will ever be obtained. Let us now consider a few practical aspects of molecular mechanics calculations. Conformations undergo by far the greatest changes in a molecule, bond distances and angles being inevitably constrained to the proximity of their equilibrium values. It is therefore useful to conceive of the total potential energy as a hypersurface in a space where it is the ordinate, while the torsion angles are the abscissae. On this hypersurface there are as many minima as there are possible conformers (i.e. conformations of relative minimum energy; see pp. 484 and 4902) of the molecule. Such minima are separated by regions of higher energy, where it will be possible to identify passages of relative minimum mapping the pathways of interconversion from one conformer to another. A typical molecular mechanics calculation starts from a given geometry, either obtained from the crystal structure or built up from standard values of distances and angles, and optimizes all the parameters in such a way as to reach, in a minimum number of program cycles, the molecular geometry corresponding to the nearest energy minimum. This is not necessarily the absolute minimum; that can be identified with certainty only by repeating the calculations starting from as many initial geometries as are necessary to systematically map the energy hypersurface. When the main minima have been found, the surrounding region can be scanned to evaluate the shape and the height of the energy barriers which separate one minimum from another. The energy profiles for 1,2dichloroethane of Fig. 7.8 and for cyclohexane of Fig. 7.10 are typical results of molecular mechanics calculations. A great number of organic molecules have been studied by the methods of molecular mechanics, whose success and popularity are due to the fact that it is a theoretical method which is very fast and extremely easy to understand. It does not require experimentation because the initial model can be obtained from tabulations of characteristic distances and angles. The computing time is very short with respect to the time needed by quantummechanical calculations. A benchmark carried out on propane[651has shown that the full geometry optimization requires times in the ratios 1:12:l3:662:5665 when accomplished, in order, by MM2, MIND0/3, MNDO, and GAUSSIAN82 with 321G and 6.31G* basis sets. Since molecular mechanics is so fast that it can optimize the geometry of molecules having the complexity of cholesterol in a few minutes of computer time, it has the additional advantage that large parts of a potential
Molecules and molecular crystals hypersurface can be calculated at a reasonable cost, giving information not only on the geometry of the different conformers but also a general view of the molecular motions and interconversion pathways. This is not to say that molecular mechanics can give the best solution to all problems of conformational analysis. It presents several pitfalls, some of which have already been discussed, and all of which are essentially related to the lack of transferability of the force field parameters among different chemical classes. However, it cannot be denied that its use gives to the crystallographer the possibility of understanding aspects of the molecular geometry (particularly its dynamics) which are not accessible through crystal structure determination.
Molecular hermeneutics: the interpretation of molecular structures Correlative methods in structural analysis The mass of structural data obtained by Xray crystallography of molecular crystals has been the object of many attempts at systematization and rationalization. Altogether they define a wide borderline area of interest which does not really belong to any traditional chemical discipline and is developing by itself along often not well defined tracks and with purposes which can appear somewhat confused, though all are essentially aimed at understanding the relationships between the experimentally determined molecular structure and the properties the molecule will display in gases, liquids, solutions, and in chemical and biochemical reaction environments. Though we may suppose it is a branch of structural chemistry, such an area, for the moment, does not even have a precise name, so that we are left free to use the name of our choice. Structureproperty relationships has often been used though interpretation of molecular structures is certainly much more correct. To pay homage to the scholarly tradition of translating scientific sentences into ancient Greek, I would suggest the name molecular hermeneutics which has the meaning of the science, or the art, of molecular interpretation. Irrespective of the name we choose, all attempts at systematic interpretation of molecular structures have one point in common: they make use of correlative methods, being based on the comparison of extended sets of structural parameters (distances, angles, geometries of specific molecular fragments, inter or intramolecular contact distances, etc.) which are correlated among themselves or with other physical properties. The simplest of these attempts are intended to produce tables of standard bond distances and angles, but most of them are devoted to clarify the systematic aspects of a variety of chemical situations such as the characteristics of the inter and intramolecular hydrogen bonding in crystals and molecules, the typical geometries of organic functional groups, the trans influence in coordination compounds, the role of n backbonding in organometallic compounds, the structural requirements which organic metals or semiconductors must fulfill, or, as extensively discussed in connection with the VSEPR and VB theories, the effects that electronegativity and hybridization changes produce on the geometries of simple molecules.
1
511
512
1
Gastone Gilli As it is impossible to give even a summary of these systematic studies, it has been chosen to discuss in some detail a single method of systematic investigation of molecular geometries, the socalled structure correlation m e t h ~ d [ ~ , " " ~which ~ ~ ] , can be considered to be an attempt to obtain information on the dynamic behaviour of molecules from the inevitably rather static crystal data. The basic idea of the method is as follows. Usually, internuclear distances found in molecular crystals fall into the two distinct fields of bonding and nonbonding distances, which are separated by a forbidden gap going from the longest bond to the shortest contact distance. For instance, this gap is extended from 1.48 (singlebond distance) to 3.25 A (sum of van der Waals radii) in the case of the CN distances. In real crystals, however, several interatomic CN distances have been found to fall in this interval, a fact that seems interesting because any situation intermediate between bonding and nonbonding is typical of chemical reactions. As early as 1931 Eyring and ~ o l a n y i [ l suggested ~~] that any chemical reaction could be described as a lowenergy path on a potential energy hypersurface (or surface) of the reaction itself, which is the function giving (within the BornOppenheimer approximation) the total potential energy of the system as a function of the relative positions of all the atomic nuclei. The reaction pathway is that trajectory (reaction coordinate) which connects the points of relative minimum on the surface and leads from the reagents to the products through the higher energy transition or activated state. For the scope of this account it is sufficient to make reference to the classical examples reported in all books on physical chemistry, such as the reactions H Hz Hz H or Hz D H HD, or to the elementary accounts on the subject which are a ~ a i l a b l e . [ ~ ~ ~  ~ ~ ~ ] If it were possible to take snapshots of the molecules taking part in the reaction at different points of the reaction pathway, the relative positions of the atomic nuclei along the course of the reaction would become known. The basic idea of the structure correlation method consists in assuming that the instantaneous displacements of the nuclei during a reaction can be represented by the images of the reaction centre obtainable from a great number of crystal structures where the centre itself happens to be deformed by local inter and intramolecular perturbations; in this hypothesis, the different images need only to be ordered in a rational sequence to give the progressive deformations of the reaction centre along the reaction coordinate. This picture of a chemical reaction is directly and even more naturally applicable to a particular class of chemical transformations, the conformational interconversions, for which it has already been shown that the relative conformers' populations are determined by the depth of the minima on the potential energy hypersurface (the enthalpic term) and by their shape (the entropic term), while activation barriers for interconversion of conformers are straightforwardly interpretable as heights of the saddle points on the lowestenergy routes (conformational interconversion pathways) connecting different conformers on the hypersurface itself.
+
+
+
+
Some threecentrefourelectron linear systemsr126~128~1341 It is well known that the solubility of iodine in water is increased by the presence of iodide ions, a fact explained by the formation of polyiodide I;
Molecules and molecular crystals
1
513
Fig. 7.20. Correlation diagrams of the interatomic distances (in A) for three linear threecentrefourelectron systems: (a) triiodide anions, (b)thiathiophthenes, and (c) linear 0H ... 0 hydrogen bonds. (Reproduced by permission from ~ u r ~ i . ' ' ~ ~ ' )
ions by a charge transfer reaction where the Lewis base I donates to the empty n* orbital of I,. Several crystal structures containing the I; ion are I, angle of 175180". The known: the anion is nearly linear with an I,I, bond distance in the I, molecule is 2.67 A and the sum of the van der Waals radii is 4.30 A. Actual structures show many interleaving distances, the shortening of the I, . I, distance being always associated with a lengthening of the I,I, one, and vice versa. In general the anion is strongly asymmetric in presence of small cations and tends to become symmetrical I, distances is shown in with larger cations. A plot of the I,I, versus I, Fig. 7.20(a). The experimental points are clearly arranged on an equilateral hyperboloid whose analytic form can be derived from Pauling's formula (7.31)

Ad = d(n)  d(1) = c log,, n where n is the bond number, d(n) and d(1) the bond distances for the bond numbers n and 1, respectively, and c a constant easily determined as c = Ad'llog 2, being Ad' the bond length increment for the symmetrical anion having n = 112 (currently c = 0.85 for a Ad' of 0.26 A). Assuming that the single bond is shared among the three atoms, it can be written and the resulting function for c = 0.85 is drawn as a continuous curve in Fig. 7.20(a); only one branch of the hyperboloid is shown since the second one, obtainable by interchanging I, with 13, is identical because of ion symmetry. The points on the curve may be supposed to represent the geometrical changes occurring along the reaction coordinate of the process The shape of the upper part of the curve indicates that the approach of the I; ion to the iodine molecule is much more rapid than the lengthening of
514
1
Gastone Gilli
the I,I, distance up to the point of formation of the activated complex, whose dissociation will quickly occur along the lower branch of the curve. From a slightly different point of view, all the curve can be considered to map the deformations along the antisymmetric stretching vibration of the activated complex up to its complete dissociation. Similar correlations have been reported for the groups SS . . . S (Fig. 0 (Fig. 7.20(c)), respectively found in thiathio7.20(b)) and 0  H phthenes (7.111) and in different structures containing nearly linear hydrogen bonds. The rule of bond number conservation expressed by (7.43) is found to hold also in these two cases with parameters d(1) =2.02, A d 1 = 0.31, and c = 1.03 A for (7.111) and 0.96, 0.26, and 0.85 A for the hydrogen bond. The curves calculated in this assumption are indicated by the continuous lines and are seen to approximate well the experimental data.

Nucleophilic addition to organometallic compounds
Fig. 7.21. Coordinate system used for cadmium complexes. Ax and Ay are the differences between the actual CdX and CdY distances and the corresponding single bond standard values. Azis the vertical displacement of the Cd atom from the S,S,S, plane.
Fig. 7.22. Correlation diagram for the bond length increments Axand Ay in cadmium complexes. (Reproduced by permission from B"rgi,[1351
)
Cadmium complexes have been studied by Biirgi in 1973 in the earliest application of the structure correlation method.[1351These compounds are normally tetrahedral but can assume quasitrigonal bipyramidal five coordination by adding a further ligand at a distance greater than that of the other four ligands (Fig. 7.21). Eleven crystal structures were found having three sulphur atoms as equatorial ligands and a fifth ligand Y at different approaching distances on the normal to the triangular face of the tetrahedron and lying on the same line containing the Cd atom and the trans ligand X. X and Y happen to be iodine, sulphur, or oxygen atoms. The system of coordinates used is described in the caption of Fig. 7.21. By plotting the experimental values of Ax versus Ay (Fig. 7.22) it is found that the points are arranged on a curve which can be interpreted in terms of bond number conservation (eqn (7.43)) with Ad' = 0.32 and c = 1.05 A. Another correlation is obtained by plotting Az as a function of Ay (upper part of Fig. 7.23) and Ax (lower part). Each structure is represented by two points having coordinates (Ax, Az) and (Ay, Az); Ax = 0 corresponds to the fragment CdS3X of tetrahedral geometry, which is represented at the same time by the point in the left lower corner and by another point at Ay = a outside the upper right corner. The leaving of X caused by the approaching of Y moves the two representative points towards the centre, where they collide at the point Ax = Ay = 0.32 and Az = 0 corresponding to the trigonal bipyramidal structure. Figures 7.22 and 7.23 may be interpreted as the geometrical changes occurring along the reaction of nucleophilic substitution S,2
Y+CdS3XS[Y...CdS3..*X]SYCdS3+X . The reaction starts with CdS3X tetrahedral and Y at infinite distance. The approach of Y causes an increasing lengthening of the trans CdX bond and
Molecules and molecular crystals
1
515
a flattening of the CdS3 pyramid until trigonal bipyramidal transition state formation. Afterwards X starts leaving and finally the new tetrahedral species YCdS3 is formed. The continuous curve of Fig. 7.23 is calculated by the equations Ax = c log [(0.84 + Az)/1.68], Ay = c log [(O.84  Az)/1.68], making use of the already known value of c = 1.05 A. The two equations are derived from the usual bond number conservation rule n, n, = 1, where n, is the bond number of CdX and n, that of CdY, but expressed as a function of the angle 8, the average XCdS angle. The two relations n, = (1  3 cos 8)/2 and n, = (1 + 3 cos 8)/2 satisfy the rule because for 8 = 90" (trigonal bipyramidal geometry) nx = n, = 0.5 and for 8 = 109.47" (tetrahedral geometry) nx = 1 and n y = 0. Pauling's formula (7.31) becomes
+
Ax = clogn,= clog [(I 3cos 8)/2], Ay = c log n y = c log [(I 3 cos 8)/2],
+
(7.45)
and, since the equatorial CdS bond has a nearly constant value of 2.52 A, we can put Az = 2.52 cos 8, which gives eqns (7.44) when substituted in (7.45). Another case studied is that of the organometallic compounds of s ~ ( I v ) . [ ' ~Similar ~] methods give a convincing mapping of what could be the reaction pathway for the S,2 nucleophilic reaction with configuration inversion
Fig. 7.23. Correlation diagram for the bond length increments A x a n d A y against the vertical displacement Az. (Reproduced by permission from ~ i i r g i . " ~ ~ ' )
It is interesting to remark, however, that the same paper reports the mapping of the reaction pathway of the S,3 process SnR2X2+ 2Y
* [SnR2X2Y2]G SnR2Y2+ 2X,
a trimolecular reaction which cannot realistically occur according to the principles of chemical kinetics. This seems to suggest that structure correlations do not simply map possible reaction pathways but, more generally, the lower regions of the potential energy hypersurface for the relative movements of the nuclei irrespective of the fact that they correspond or not to real chemical reactions or conformational rearrangements.
Nucleophilic addition to the carbonyl group Nucleophilic addition of aminic nitrogen to carbonyl is one of the first and more studied examples of structure correlation^,['^^^'^^] though the analogous addition of oxygen has been also reported.['39] Molecules where the nitrogen is forced near the carbonyl carbon at a distance shorter than the sum of the van der Waals radii are mainly rings of the type (7.IV) and (7.V) or 1,8disubstituted naphthalenes (7.VI). In the original paper 14 structures having the required characteristic were reported and the coordinate system for their analysis is shown in Fig. 7.24. Final results are summarized in Fig. 7.25, which describes the course of the geometrical deformations of the carbonyl group caused by the approaching of the nucleophile. As this
Fig. 7.24. Coordinate system used for describing the approaching of the aminic nitrogen t o the carbonyl. dl and 4 are the N . . C and C==O distances, respectively: the distance of the carbon atom from the (RR'O) plane is a measure of carbonyl pyrarnidalization and is termed A.
.
516 ( Gastone Gilli
Fig. 7.25. The coordinate system is that of Fig. 7.24 projected on the (NCO) plane. The open circles indicate the positions of the nitrogen atoms (top), of the bisector of RCR' (bottom left) and of the carbonyl oxygen (bottom right) i n the 14 (AL) structures considered. (Adapted from Bijrgi and ~ u n i t z . ' ' ~ ~ ' )
approaches the carbon (i.e. d l decreases), the plane containing the carbon and the two R and R' substituents bends away causing an increasing pyramidalization of the carbon which rehybridizes from sp2 to sp3, while the C=O distance is slightly increased. It seems of interest that the nucleophile does not approach the carbonyl plane perpendicularly but makes an almost constant N . C==O angle of 110°, which has been interpreted in terms of elementary banana bond considerations but also shown to match the results of ab initio quantummechanical calculations.[41The constraint arising from the fixed 110" angle is more clearly seen in (7.VI). The two NR2 and COR groups would both be expected to be splayed outwards in order to reduce their van der Waals repulsions but the CN bond is actually found to be splayed inwards by the need to maintain the correct approach angle to the carbonyl C=O bond. When looking at the dependence (Fig. 7.24) between A (carbonyl group pyramidaiity) and d l (N . C distance) it is found that they are correlated according to the regression line a function which gives the maximum pyramidal character of the carbon atom, A,, = 0.437 A, for d l = 1.479 A (taken as standard distance for the CN single bond). By assuming that the CN bond number can be expressed as n = (A/A,,,)~ the above equation changes into
d l = 0.85 log n
+ 1.479
(7.47)
which is nothing more than the usual Pauling equation (7.31).
A case of conformational rearrangementr140,1411 The fragment c ( s p 2 )  ~ ( s p ~(7.VII) ) is contained in a variety of organic molecules, such as anilines (7.VIIIA) and naphthylamines (7.VIIIB), amides (7.VIII 0 ) and thioamides (7.VIII S) (X = 0 , S), amidines (7.VIII N) (X = NR), and enamines (7.VIII D) (X = CR,). It displays a definite tendency to be planar, which can be accounted for by the
Jx)
Molecules and molecular crystals
contribution of the polar form (7.VIIa) to its ground state. The cistrans isomerization barrier has been measured by a number of dynamic NMR experiments to be in the range 522 kcalmol' (on average, 20.7, 18.1, 12.8, 9.0, and 5.1 kcal mol' for thioamides, amides, amidines, enamines, and anilines respectively, in agreement with the fact that the contribution of the polar form decreases with the decrease of electronegativity of X). In spite of the general tendency to planarity, there are many crystal structures where the group is deformed by rotation around the CN bond or by nitrogen pyramidalization, or by both, mainly in consequence of intramolecular steric hindrance. The structure correlation method was used with the aim of mapping the coordinate of cistrans isomerization of the group. A coordinate system for the outofplane deformation can be obtained by the usual methods of group theory; the resulting orthogonal coordinates are the angle of twisting around the CN bond, t ( t = 0 and 180" for the planar cis and trans geometries, t = f90" when the two halves of the group are perpendicular) and the two outofplane bendings of nitrogen, x,, and carbon, x,, ranging from zero (sp2 atom) to 60' (sp3 atom). Calling $,, 4,) $31 and $, (Fig. 7.26) the four torsion angles 1234, 5236, 5234, and 1236, it is found that[142,143]
1
517
c
+
+ Z
XN
Xc 

Fig. 7.26. lnternalcoordinatesystem describing the outofplane deformation of the c ( s p 2 )  ~ ( s p ~ ) fragment. (Reproduced by permission from Gilli et al.[14")
A total of 90 fragments belonging to 68 crystal structures were found from CSD.[~]The xc values are always very small (on average 1.7"), indicating that the carbon sp2 has greater resistance to outofplane bending and that this motion can be neglected. Conversely X, shows a wide variation assuming values up to f55". Figure 7.27 shows the correlation diagrams of
Fig. 7.27. Correlation diagram of X , versus r for anilines (A), naphthylamines (B), enamines (D), and amidines (N). Data for amides and thioamides (not shown in the figure) would cluster in the lower left corner with r s 15" and ,yN S 27'. (Reproduced by permission from Gilli et
518
1
Gastone Gilli
xN against
z for all the chemical classes except amides and thioamides. These latter cluster in the lower left corner with t c 1.Y and X, S 27", showing the greater resistance to outofplane deformation of these compounds in agreement with the larger electronegativities of the oxygen and sulphur atoms. Compounds of the other classes undergo more severe distortions which appear to be of two different types. The first, producing simple nitrogen pyramidalization, occurs for t nearly equal to zero and for increasing values of xN and can be called a butterfly deformation. The second, which could be called combined, associates nitrogen pyramidalization (increasing xN) with a rotation around the CN bond (increasing z). The diagonal straight line of Fig. 7.27 ideally separates mostly butterfly (on the left) from mostly combined (on the right) distortions. The combined motion admits a simple interpretation. In the planar fragment the nitrogen is sp2 hybridized and its p, A 0 is implies in a n bond with the p, A 0 on the carbon. The rotation around the CN bond causes a decoupling of the n system while the nitrogen rehybridizes engaging its p, A 0 into an sp3 HO carrying the lone pair. The opposite mechanism ia also possible: the planar nitrogen undergoes an outofplane vibration (butterfly motion) which causes the rehybridization of the atom from sp2 to sp3. The sp3 HO on nitrogen is essentially decoupled from the p, A 0 on carbon, the double bond fades, and the rotation around CN becomes possible. This second mechanism seems to be preferred because Fig. 7.28 shows that XN (a measure of the nitrogen rehybridization) is strongly correlated with a lengthening of the CN distance which almost encompasses the full variation range of dCN (from 1.27 to 1.44 A going from double to single C(sp2)N(sp3) bond), while no similar correlation can be established with z, the rotation angle around the CN bond.[1411 From the point of view of the structure correlation method the butterfly motion corresponds to a simple outofplane vibration and does not produce
Fig. 7.28. Correlation diagram between the &, bond distances and the x, values for all fragments studied (A = anilines, B = naphthylarnines, D = enarnines, N = arnidines, 0 = amides, and S = thioamides). (Reproduced by permission from Gilli et
Molecules and molecular crystals ( 519
Fig. 7.29. The relative movements of the fragment atoms along the reaction pathway identified by the broken curve of Fig. 7.27, showing the steps leading from the planar .ground state Toto the two enantiomeric transit~onstates T, and TZ. Further rotation around the CN bond would transform the cis isomer on the lee into the trans isomer on the right (not shown). (Reproduced by permission from Gilli et at.[14")
any chemical change. Conversely, the combined motion can be considered to be representative of the geometrical changes experienced by the fragment along the pathway of a cistrans isomerization reaction. The broken curve of Fig. 7.27 maps the most probable pathway leading from the planar ground state To, having t = X, = 0°, to the transiton state located at ( t , x,) = (90, 4 0 " ) ; since the rotation can occur in two opposite directions, two enantiomeric TI and T2 transition states will be equally possible and Fig. 7.29 shows the geometrical changes the fragment is undergoing along the two enantiomeric pathways indicated by the broken curve. It is seen that the atom movements start with an outofplane deformation of the nitrogen and are followed by the rotation around the CN bond. It seems of great interest to show whether the proposed reaction pathway does actually map a relative minimum path on the potential energy hypersurface. What is needed is an energy model for the outofplane motion of the c(sp2)N(SP~)fragment. A rather simple molecular mechanical model has been proposed11411by modification of a first model given by Winkler and ~ u n i t z , [ lthat ~ ~ ]is V ( T ' ,xN)= (CTIB 4
+ IB)(l
cos t r ) / 2
QP(1I COS tr)&/2 d IB(1
COS
Z')(COS3xN 1)/4, (7.49)
where the total potential energy expressed as a function of t ' = 22 and X, is assumed to depend on three predetermined parameters, CTIB = cistrans isomerization barrier, ZB =inversion barrier of the pyramidal sp3 nitrogen, and QP = force constant for the outofplane bending of the sp2 nitrogen. The energy is zero at the origin in correspondence to the planar geometry and increases with X& for t' = 0" along the outofplane vibration of the planar nitrogen; for x,=O and 2' = 180" the function has the value CTIB IB, differing from CTIB for the energy needed to make planar the sp3 nitrogen, while it assumes the exact value of CTIB only for the hypothetical transition state geometry ( t ' = 180" and X, = 60"). The two expressions (1 cos t ' ) and (1  cos t ' ) are introduced in order to progressivelv cancel the second term of (7.49) re~lacineit bv the third term, while
+
+
520
1
Gastone Gilli z' changes from zero to 180' and, accordingly, the nitrogen hybridization from sp2 to sp3. The values of the constants have been chosen as average values from those of the different classes of compounds. The CTIB value is in the range 522 kcal mol', QP is evaluated from vibrational spectroscopy and molecular mechanics to be some 510 kcal mol' radP2, and IB can be assimilated to the inversion barrier of ammonia, usually reported as =6 kcal moll. Values chosen were CTIB = 14, IB = 8 kcal mol', and QP = 8 kcal molI rad2. Equation (7.49), however, evaluates the position of the = 60", which does not correspond to that transition state at t ' = 180' and found from Fig. 7.27 as far as is concerned. The reason is that some allowance must also be made for the 14 nonbonded interactions, that is
xN xN
where En,,can be obtained by the methods of molecular mechanics. Here it has been calculated assuming R, = R, = R, = methyl and X equal to a nonexistent atom intermediate between oxygen and methyl group. The final V' function calculated in such a way is shown in Fig. 7.30 and represents the potential energy hypersurface for an imaginary molecule which is the average of all different compounds of all chemical classes investigated. In spite of the approximations made, it has the correct shape and the agreement with experiment becomes more convincing when the experimental points are plotted on it. They appear to be nicely located along the energy valley leading from the planar ground state to the transition state, which is now more correctly located at t' = 180" and X, = 50".
Fig. 7.30. Total potential energy (kcal mol') surface as calculated from eqn (7.50) as a function o f t = t1/2and x,. Experimental points include all compounds except amides and thioamides. (Reproduced by permission from Gilli et
Molecules and molecular crystals
Resonance assisted hydrogen bonding (RAHB) 6diketones are known to undergo easy enolization and in two recent structure correlation methods have been applied to the Pdiketone fragment in its en01 form (7.IXa,b) in order to understand what happens to the fragment geometry when perturbed by intramolecular, (7.X), or intermolecular, (7.XI), hydrogen bonding. The reason why this
particular system was studied originates from the empirical observation that the nconjugated system present in the 6diketone en01 HOCR=CRCR=O fragment undergoes greater delocalization when it forms either intramolecular or infinite chain intermolecular hydrogen bonding. The nature and the entity of this effect is shown in Table 7.9. Here the standard distances are those tabulated['091 for pure single and double bonds, the unperturbed ones are an average of nine fragments that cannot make Hbonds (having OR instead of OH). The unperturbed geometry is a 87:13 mixture of the resonance forms (7.IXa) and (7.IXb) according to Pauling's formula (7.31). However, when the fragments form Hbonds all distances undergo changes consistent with an increased contribution of the polar form (7.IXb), which becomes respectively 29 per cent for the intermolecular and 48 per cent for the intramolecular cases reported in the table; at the same time the contract 00 distance, which is typically 2.74 A in the 0  H . 0 bond in ice, becomes much shorter, being respectively 2.575 and 2.485 A in Table 7.9. Selected bond distances (A) for the Pdiketone enol fragment. %(7.IXb) = per cent contribution of the polar form (7.IXb) according to Pauling's formula (7.31); the standard 00 contact distance in parentheses is that observed in ice
Perturbed by: Intermolecular Hbond (7.XIIa
1.316
1.372
1.431
1.238
2.575
29
Intramolecular Hbond (7.X)b
1.281
1.398
1.410
1.279
2.485
48
Neutron data from Jones, R. D . G. (1976). Acta Crystallographica, 8,32,2133. bSernrningsen, D . (1977). Acta Chem. Scand. Sect. 8, 31, 114.
a
1
521
522 ( Gastone Gilli
the two cases, while the 0  H bond distance (0.95 A in the absence of Hbonding and according to Table 7.7) is lengthened up to 1.24 A in the last compound of Table 7.9. 25 Xray or neutron structures of pdiketones and In a first Pketoesters were studied, 22 of type (7.X) and 3 of type (7.XI), and the discussion reported here concerns this first analysis. Later on[2591491 the investigation was extended to a much larger set of fragments (81 and 37 for (7X) and (7.XI), respectively) but without obtaining significant differences in the final results. In summary, all the following phenomena are observed to occur together: (1) increased delocalization of the nconjugated system; (2) strengthening of the 0  H  . 0 bond as indicated by the shortening of do, and the lengthening of d,, distances; (3) shift of the proton position towards the middle point of the 0 . . . 0 contact. The three effects may occur with different intensities but maintain the same intercorrelation for both intramolecularly (7.X) or intermolecularly (7.XI) bonded fragments (the intramolecular Hbond is usually stronger and causes greater n delocalization) and even for different classes of compounds (e.g. Pdiketone enols form stronger Hbonds and are more delocalized than the enols of Pketoesters or /3ketoamides). While the Hbond strengthening is easily measured by both d o   , and dSH changes, a specific geometric parameter is needed in order to describe the n system delocalization. The simplest way consists in using symmetry coordinates for the inplane antisymmetric vibration of the group (7.X) or (7.XI), that is q , = d4  d l and q , = d ,  d,. Clearly q , = q , = 0 for the totally delocalized structure, while the greatest values will occur for the standard bond distances of Table 7.9. Figure 7.31 reports the scatter plot of
4'I N
'y
0
a
N
.05
.
k
.,A'
It
U
Fig. 7.31. Scatter plot of q, versus q, (in A) for the 25 fragments studied. The plot is centrosymmetric as any point can be plotted twice in view of the equivalence of the enolketonic (EK) and ketoenolic (KE) isomers. The full squares and stars refer t o the standard and unperturbed geometries of Table 7.9, respective1 (Reproduced by permission from Gilli et al!2'1)
.
?4
s
/
' a&/ .lo/
/
0" ,
'
INTRA HE
* o
INTER HB
AVERAGE UNPERTURBn STANDARD
Molecules and molecular crystals
1
523
q2 versus ql for the 25 compounds studied. The plot is centrosymmetric as any point can be plotted twice in view of the equivalence of the enolketonic (EK) and ketoenolic (KE) isomers, and its centre identifies the fully delocalized structure. The full squares and stars refer to the standard and unperturbed geometries of Table 7.9, respectively. The broken line connecting EK and KE is calculated from the condition of bond number conservation (p. 513). Since q1 and q2 are linearly dependent, a single coordinate Q = q1+ q2 can be used, which has values of 0.0, 0.320, and +0.320 A for the fully ndelocalized and the fully nlocalized EK and KE structures, respectively. Alternatively the fragment geometry can be described by a coupling parameter, A, according to which the state of any fragment is a mixture A(EK) + (1 A)(KE); it assumes the values of 1.0 for EK, 0.0 for KE, and 0.5 for the fully delocalized form. The scatterplot of doo against Q = ql + q2 for the 25 fragments considered is reported in Fig. 7.32. The plot displays m symmetry with respect to the delocalized structure having Q = 0 or A = 0.5 owing to the equivalence of the EK and KE structures. Very short 0 . .  0 distances are seen to be associated with small values of lQl, that is with relevant delocalization of the nconjugated system. The plot of the variations of the dSH and of the contact do,, distances against dso is shown in Fig. 7.33. Although data are necessarily more disperse owing to the known difficulties in locating protons by Xray diffraction (only three were neutron structures), the plot clearly indicates that the shortening of the 0 . . . 0 distance below 2.5 A causes the two bond (0H) and contact (OH . . . 0 ) distances to become progressively equal, though a perfectly centred positioning of the proton is never achieved. The observed correlations are in agreement with the model which, in its qualitative aspects, is illustrated in Fig. 7.34. Let us assume firstly that the double C=C is substituted by a single CC bond; the 0  H . . 0 bond established will be the balance between two different factors: the energy of
2.4t
.32
.20
.lo
I
0
.lo
I
.20
b 32
Fig. 7.32. Scatter plot of do, versus Q. The plot has rn symmetry because of the equivalence of EK and KE structures. Full and open circles indicate intra and intermolecular Hbonds, respectively. (Reproduced by permission from Gilli et
524
( Gastone Gilli
Fig. 7.33. Scatter plot of &, and do,, distances against the contact do, distance.
the Hbond itself (EHB)and the van der Waals energy originated from the attractive and repulsive terms of the 14 interactions (Evdw). Reestablishing now the double C=C bond, the resonance (7.IXa) tt (7.IXb) will cause a neat shift of electrons from left to right (Fig. 7.34), which will stop when the minimum of ERES E B P is attained, where the first term is the resonance energy gain and the second the energy needed to dissociate the opposite partial charges on the terminal oxygens. The charges have the correct sign for strengthening the Hbond with consequent shortening of d o   , and lengthening of d., The movement of the proton to the right is equivalent to a negative charge going to the left and the global effect is the annihilation of the partial charges initially set up by resonance, so allowing an increased contribution of the polar forrn (7.IXb) and a further strengthening of the Hbond, an imaginary process going on until the minimum of the function
+
Fig. 7.34. A graphical representation of the resonance assisted hydrogen bonding (RAHB) model. (Reproduced by permission from Gilli e t
(7.51) E = E H B+ E v m+ ERES+ EBP is attained. The Hbond formed has quite specific features and, in view of the strict interplay of n delocalization and Hbond strengthening which causes it, has been called[241resonance assisted h y d r ~ g e n bonding (RAHB). It is essentially a charge assisted Hbond where, however, the charges do not arise from the presence of ions but from the resonance in a heteroconjugated system. The RAHB model is supported by a wealth of spectroscopic data and theoretical calculations for which the reader is addressed to the original paper. What is more important here is to discuss whether the correlation among geometrical parameters can be interpreted in terms of the potential energy hypersurface of the fragment. The approximate energy partitioning used in (7.51) can be evaluated quantitatively since semiempirical equations are available for all the four terms. E H Bis the total energy, including both attraction and repulsion terms, of the 0  H . . . 0 bond as a function of = r and d o _  , = R. It can be written as E d r ., R ) and has been dH , calculated by the equation proposed by Lippincott and ~ c h r o e d e r [ ~ for ~,~*] \
Molecules and molecular crystals
1
525
all the desired values of r at the R value for which the energy was a relative minimum. In such a way R turns out to be a function of r and is known for any value of r. ERE, can be calculated by the method proposed by Krigowski et a1.[1441which is known to give the resonance energy of a nconjugated system from its bond distances with fairly good accuracy. EBp is the energy required to create the opposite fractional charges fq on the two terminal oxygens and can be easily evaluated by means of the coefficients of the atomic ionization energy versus electron affinity curves tabulated by Hinze and ~ a f f 2 for [ ~the~ main ~ ~ elements. ~ ~ ~ ~Finally, EVdw can be calculated by the methods and equations already discussed in the section on molecular mechanics. The final potential energy map calculated according to (7.51) for acetylacetone (R, = R, = CH,, R, = H) is shown in Fig. 7.35 as a function of two coordinates: the bond number of the 0  H bond, n(0H) (which is 1.0 assumes the value of 0.97 hl, and in the absence of Hbonding when d,, 0.5 when the hydrogen is equally shared by the two oxygens and ,d , = do,, = 1.25 hl), and the coupling parameter A (which assumes the values of A = 0, 0.5, and 1 for nlocalized EK, fully ndelocalized, and nlocalized KE fragment structures, respectively) or its related quantity Q. Figure 7.36 illustrates the physical meaning that can be given to the four corners and the central point of the plot of Fig. 7.35 while Fig. 7.37 shows a threedimensional representation of the potential energy map in the same coordinate system. The potential energy map is centrosymmetric in consequence of the fragment symmetry and displays a diagonal valley of lower energy which can
PROTON TRANSFER
Fig. 7.35. Total potential energy map (kJ mol') calculated according t o eqn (7.51) for acetylacetone ( R , = R, = CH,, R, = H) as a function of the coupling parameter A and the n(0H) bond number. The physical meaning of the four corners and of the cental point of the plot are illustrated i n Fig. 7.36. The star indicates the gas electron diffraction structure of acety~acetone['~"and the full points the Xray or neutron structures analysed. (Heproduced by permission from Gilli et
526
1
Gastone Gilll *PROTON
TRANSFER
I
0 FORMAL
J
0.5 CHARGE
1
Fig. 7.36. Geometries assumed by the fragment in the five positions of the energy map of Fig. 7.35corresponding to the four corners and to the central point. The diagonal line is a zerocharge line for the fragment because it is the locusof points for which the partial charges generated by resonance are exactly compensated by the shift of the proton.
Fig. 7.37. Threedimensional representation of the potential energy map of Fig. 7.35 in the same coordinate system. The path for the reaction of proton transfer transforming the EK into the KE isomer is clearly shown as an energy valley whose saddle point corresponds to the fully ndelocalized form having the proton in the middle of the two oxygens.
be considered as the path of the reaction of proton transfer transforming the EK form into its KE isomer. Figure 7.38 shows the geometrical changes which the fragment undergoes along the reaction pathway and Fig. 7.39 reports the energy profiles along the same path. The curve A' has been calculated without taking into account the two terms related to resonance (ERE,and EBp);it is essentially representative of Hbonding in water and, in fact, it reproduces quite well the water distance values (r = 1.01 A, R = 2.74 A) and of the proton transfer barrier (some 40 kJ moll). The curve A is calculated for acetylacetone by the use of all terms of (7.51) (Figs. 7.35 and 7.37); the introduction of the resonance term lowers the total energy by 42.5 kJmoll, increasing the Hbond energy (already 20 kJ mol' in water) to the relevant value of 62.5 k3 moll; at the same time the proton transfer barrier is reduced to 34.8 kJ mol' and the 0  H distance is lengthened until r = 1.08 A (associated R = 2.50 A). The structure of acetylacetone has been recently determined by gas electron diffra~tion"~''and the corresponding geometry, marked by a star in Fig. 7.35, is seen to be very close to the calculated energy minimum. In the same figure are reported as full points the geometries of all the 25 fragments investigated. It seems interesting that all of them are correctly located inside the diagonal energy valley though, of course, not in the minimum, which has been specifically calculated for acetylacetone. As far as their exact position is concerned two main factors can be discerned. The first is electronic, and we have already remarked that Pdiketone enols form much stronger Hbonds than the enols of Pketoesters or Pketoamides. The second is steric in nature, the strongest Hbonds being associated with bulky R, and R, substituents. For example, strictly similar calculations carried out On hexamethylacetylacetone by the use of (7.51) show that the energy minimum is shifted to r = 1.11 and R = 2.48 A, while the Hbond energy increases to 82.5 kJ mold' and the proton transfer barrier decreases to 27.5 kJ m0lI.
Molecules and molecular crystals
Resonance assisted hydrogen bonding (RAHB) is therefore a mechanism of synergistic interplay of resonance and Hbond formation. It can be generalized by calling it a mechanism of interplay between Hbond and resonance in heterodienes or, more generally, heteroconjugated systems:
1
527
H
Fig. 7.38. Geometrical deformations experienced by the fragment along the pathway of the proton transfer transforming the EK into the KE isomer.
7. Xll
7.Xlll
From this point of view, the Pdiketone enols so far discussed correspond to the heterodienic scheme (7.52) (X = Y = O), but the RAHB mechanism is supposed to operate independently of the number of interleaving carbon atoms provided the conjugation between the lone pair on X and the C=Y double bond is maintained. In the X = Y = 0 series the scheme (7.55) represents carboxylic acids which, in fact, are well known to give strongly Hbonded dimers (Fig. 7.3, scheme b), though a more convincing proof of RAHB could come from the observation of strongly delocalized and Hbonded heterotrienes (7.53) and heterotetraenes (7.54). Structures corresponding to these fragments have been recently analysed[251and found to display the expected behaviour. Compounds (7.XII) behave as totally
Fig. 7.39. Energy profile along the reaction coordinate of proton transfer transforming EK into KE as mapped along the mainly diagonal pathway of lowest relative energy of the map of Fig. 7.35 (curve A). Curve A' is the same curve but calculated omitting the ERE,and E,, terms i n eqn (7.51); it can be considered t o represent the proton transfer in water. The horizontal lines mark the zeropoint energies which are slightly different i n water and acetylacetone.
528
1
Gastone Gilli
7. X I V
7. x v
7.XVI
7.XVll
/
8"k NH0
/
7. X I X
I
1
1
7.XXlll
ndelocalized heterotetraenes with bond 5 not participating to the conjugation; the opposite bonds n and n ' (n = l, 2, 3, and 4) are nearly equal and the 0  H . . 0 is extremely short (on average, do, = 2.47 and do, = 1.18 A). In a strictly similar way compounds (7.XIII) show total delocalization of the heterotrienic system and display one of the shortest d o   , distances ever observed, i.e. 2.425 A. Up to now we have proved that RAHB is active in the enolone fragment (7.XIV) (or in other diketone enols with longer conjugated systems) forming intramolecular or, sometimes, intermolecular Hbonds. All these compounds have the oxygen as the only heteroatom. However, other heteroconjugated systems having different heteroatoms are putatively implied in this phenomenon via intramolecular or intermolecular (including dimerization) Hbond formation, such as enaminones (7.XV), enaminoimines (7 .XVI) , enolimines (7 .XVII) , amideamidine complexes (7 .XVIII) and amide dimers (7.XIX). Preliminary data confirming the strong n delocalization of Hbonded enaminones (7.XV) and enolimines (7.XVII) have already been reported,[1481and the formation of amide dimers (7.XIX) has been discussed by several a ~ t h o r s . [ ~ ~ , ~ ~ ]
Molecules and molecular crystals
Possible biochemical and biological implications originate from the fact that the amideamidine complex (7.XVIII) is present in both thymineadenine (7.XX) and cytosineguanine (7.XXI) PIbonded couples determining the doublehelix structure of DNA; in addition, cytosineguanine coupling (7.XXI) implies another much wider cycle of Hbonds and mconjugated double bonds. Strictly similar considerations can be made in connection with the Hbonds determining the secondary structure of proteins: both ahelices (7.XXII) and 0pleated sheets (7.XXIII) contain long chains of nheteroconjugated systems connected by Hbonds and differ only because each ahelix contains three of such chains which are nearly parallel and isoriented, while in 0pleated sheets the arrangement of the chains is antiparallel.
References 1. Wells, A. F. (1975). Structural inorganic chemistry (4th edn). Clarendon, Oxford. 2. Bondi, A. (1964). Journal of Physical Chemistry, 68, 441. 3. Allen, F. H . , Bellard, S., Brice, M. D . , Cartwright, B. A., Doubleday, A., Higgs, H., Hummelink, T., HummelinkPeters, B. G., Kennard, O., Motherwell, W. D. s . , Rodgers, J. R., and Watson, D. G. (1979). Acta Crystallographica, B35, 2331. 4. Dunitz, J. D. (1979). Xray analysis and the structure of organic molecules. Cornell University Press, Ithaca, N.Y. 5. Pauling, L. (1960). The nature of the chemical bond and the structure of molecules and crystals. A n introduction to modern structural chemistry (3rd edn). Cornell University Press, Ithaca, N.Y. 6. Kitaigorodski, A. I. (1973). Molecular crystals and molecules. Academic, New York. 7. Kaplan, 1. G. (1986). Theory of molecular interactions. Elsevier, Amsterdam. 8. Pertsin, A. J., and Kitaigorodski, A. I. (1987). The atomatom potential method. Springer, Berlin. 9. London, F. (1930). Zeitschrift fur Physikalische Chemie, B11, 222, 236; (1930). Zeitschrift fur Physik, 63, 245. 10. LennardJones, J. E. (1931). Proceedings of the Physical Society, 43, 461. 11. Buckingham, R. A. (1938). Proceedings of the Royal Society of London, A168, 264. 12. Giglio, E. (1969). Nature, 222, 339. 13. Allinger, N. L. (1975). MMlIMMP1, QCPE No. 318. Indiana University. 14. Hamilton, W. C., and Ibers, J. A. (1968). Hydrogen bonding in solids. Benjamin, New York. 15. Pimentel, G . C., and McClellan, A. L. (1960). The hydrogen bond. Freeman, San Francisco; Pimentel, G. C., and McClellan, A. L. (1971). Annual Reviews of Physical Chemistry, 22, 347. 16. Kollman, P. A , , and Allen, L. C. (1972). Chemical Reviews, 72,283; Kollman, P. A. and Joesten, M. D. (1982). Journal of Chemical Education, 59, 362. 17. Schuster, P., Zundel, G., and Sandorfy, C. (ed.) (1976). The hydrogen bond, Vols. I, 11, and 111. NorthHolland, Amsterdam. 18. Emsley, J. (1980). Chemical Society Review, 9, 91. 19. Umeyama, H., and Morokuma, K. (1977). Journal of the American Chemical Society, 99, 1316. 20. Morokuma, K. (1971). Journal of Chemical Physics, 55, 1236.
1
529
530
1
Gastone Gilli
21. Kitaura, K., and Morokuma, K. (1976). International Journal of Quantum Chemistry, 10, 325. 22. Taylor, R., and Kennard, 0. (1982). Journal of the American Chemical Society, 104, 5063. 23. Gorbitz, C. H . (1989). Acta Crystallographica, B45, 390. 24. Gilli, G., Bellucci, F., Ferretti, V., and Bertolasi, V. (1989). Journal of the American Chemical Society, 111, 203. 25. Gilli, G., and Bertolasi, V. (1990). In The chemistry of enols (ed. Z . Rappoport). Wiley, New York. p. 713. 26. Bent, H. A. (1968). Chemical Reviews, 68, 587. 27. Gutmann, V. (1978). The donoracceptor approach to molecular interactions. Plenum, New York. 28. Kitaigorodski, A. I. (1984). Mixed crystals. Springer, Berlin. 29. Huheey, J. E. (1983). Inorganic chemistry (3rd edn). Harper and Row, New York. 30. Ibers, J. A., Pace, L. J., Martinsen, J., and Hoffman, B. M. (1982). Structure and Bonding, 50, 1. 31. Del Re, G. (1958). Journal of the Chemical Society, 4031. 32. Gasteiger, J., and Marsili, M. (1980). Tetrahedron, 36, 3219. 33. BerkovitchYellin, Z., and Leiserowitz, L. (1982). Journal of the American Chemical Society, 104, 4052. 34. Lifson, S., Hagler, A. T., and Dauber, P. (1979). Journal of the American Chemical Society, 101, 5111. 35. Dauber, P., and Hagler, A. T. (1980). Accounts of Chemical Research, 13, 105. 36. Spackman, M. A. (1986). Journal of Chemical Physics, 85, 6579, 6587. 37. Lippincott, E. R., and Schroeder, R. (1955). Journal of Chemical Physics, 23, 1099. 38. Schroeder, R., and Lippincott, E . R. (1957). Journal of Physical Chemistry, 61, 921. 39. Born, M., and von Karman, T. (1912). Physikalische Zeitschrift, 13, 297. 40. Born, M., and Huang, K. (1954). Dynamical theory of crystal lattices. Clarendon, Oxford. 41. Willis, B. T. M., and Pryor, A. W. (1975). Thermal vibrations in crystallography. Cambridge University Press. 42. Califano, S., Schettino, V., and Neto, N. (1981). Lattice dynamics of molecular crystals, Lecture Notes in Chemistry, Vol. 26. Springer, Berlin. 43. Pawley, G. S. (1970). In Crystallographic computing (ed. F. R. Ahmed). Munksgaard, Copenhagen. p. 243. 44. Kitaigorodski, A . I. (1970). In Advances in structure research by diffraction methods, Vol. 3, (ed. R. Brill and R. Mason). Pergamon, Oxford. p. 173. 45. Cahn, R. S., and Ingold, C. K., (1951). Journal of the Chemical Society, 612. 46. Cahn, R. S., Ingold, C. K., and Prelog, V. (1956). Experientia, 12, 81. 47. Klyne, W., and Prelog, V. (1960). Experientia, 16, 521. 48. Mislow, K. (1965). Introduction to stereochemistry. Benjamin, New York. 49. Hallas, G. (1965). Organic stereochemistry. McGrawHill, New York. 50. Cahn, R. S., Ingold, C. K., and Prelog, V. (1966). Angewandte Chemie International Edition in English, 5, 385. 51. Eliel, E. L., Allinger, N. L., Angyal, S. J., and Morrison, G. A. (1966). Conformational analysis. Wiley, New York. 52. Natta, G., and Farina, M. (1968). Stereochimica. Mondadori, Milan. 53. IUPAC 1968 Tentative rules, section E , fundamental stereochemistry, Information Bulletin No. 35; (1970). Journal of Organic Chemistry, 35, 2849. 54. Stoddard, J. F. (1971). Stereochemistry of carbohydrates. Wiley, New York. 55. Balaban, A. T. (ed.) (1976). Chemical applications of graph theory. Academic, New York.
Molecules and rnolecular crystals Bijvoet, J. M., Peerdeman, A. F., and van Bommel, A. J. (1951). Nature, 168, 271. Rogers, D. (1975). In Anomalous scattering (ed. S. Ramaseshan and S. C. Abrahams). Munksgaard, Copenhagen. p. 231. Cotton, F. A. (1971). Chemical applications of group theory (2nd edn). Wiley, New York. Cano, F. H., FocesFoces, C., and GarclaBlanco, S. (1977). Tetrahedron, 33, 797. Cremer, D. and Pople, J. A. (1975). Journal of the American Chemical Society, 97, 1354. Boeyens, J. C. A. (1978). Journal of Crystal and Molecular Structure, 8, 317. Altona, C., Geise, H. J., and Romers, C. (1968). Tetrahedron, 24, 13. Parkanyi, L. (1980). RING. Hungarian Academy of Sciences, Budapest. Nardelli, M. (1982). PARST. University of Parma, Italy. Clark, T. (1985). A handbook of computational chemistry. Wiley, New York. Hehre, W. J., Radom, L., Schleyer, P. v. R., and Pople, J. A., (1985). Ab initio molecular orbital theory. Wiley, New York. Pople, J. A., and Beveridge, D. L. (1970). Approximate molecular orbital theory. McGrawHill, New York. Dewar, M. J. S. (1969). The molecular orbital theory of organic chemistry. McGrawHill, New York. Murrell, J. N., and Harget, A. J. (1972). Semiempirical selfconsistentjield molecular orbital theory of molecules. Wiley, London. Frisch, M. J., HeadGordon, M., Schlegel, H. B., Raghavachari, K., Binkley, J. S., Gonzalez, C., et al. (1988). GAUSSIAN 88. Gaussian Inc., ~ittsburgh, PA. Bingham, R. C., Dewar, M. J. S., and Lo, D. H. (1975). Journal of the American Chemical Society, 97, 1285, 1294, 1302, 1307, 1311; Dewar, M. J. S . , and Thiel, W. (1977). Journal of the American Chemical Society, 99, 4899, 4907. Dewar, M. J. S., Zoebisch, E. G . , Healy, E. F., and Stewart, J. J. P. (1985). Journal of the American Chemical Society, 107, 3902. Coulson, C. A., (1961). Valence. Oxford University Press, London. McWeeny, R. (1979). Coulson's valence. Oxford University Press, London. 75. Streitwieser, A. Jr. (1961). Molecular orbital theory for organic chemists. Wiley, New York. 76. Gillespie, R. J. (1972). Molecular geometry. Van NostrandReinhold, London. 77. Gillespie, R. J. (1963). Journal of Chemical Education, 40,295; (1970). 47,18. 78. Bader, R. F. W., Gillespie, R. J., and MacDougall, P. J. (1988). Journal of the American Chemical Society, 110, 7329. 79. Orgel, L. E., (1966). An introduction to transitionmetal chemistry (2nd edn). Wiley, New York. 80. Bethe, H. (1929). Annalen der Physik, 3, 135. 81. Van Vleck, J. H. (1932). Physical Review, 41,208; (1935). Journal of Chemical Physics, 3, 803, 807. 82. Ballhausen, C. J., (1962). Introduction to ligand field theory. McGrawHill, New York. 83. Dunn, T. M., McClure, D. S., and Pearson, R. G. (1965). Some aspects of crystalfield theory. Harper and Row, New York. 84. Schaffer, C. E., and
[email protected],C. K. (1965). Molecular Physics, 9, 401. 85. Schaffer, C. E. (1973). Structure and Bonding, 14, 69. 86. Burdett, J. K. (1978). Chemical Society Review, 7, 507. 87. Burdett, J. K., (1980). Molecular shapes. Theoretical models of inorganic stereochemistry, p. 23. Wiley, New York. 88. Walsh, A. D. (1953). Journal of the Chemical Society, 2260, 2266, 2288, 2296, 2301, 2306.
1
531
532
1
Gastone Gilli 89. Gimark, B. M. (1979). Molecular structure and bonding. Academic, New York. 90. Lowe, J. P. (1978). Quantum chemistry. Academic, New York. 91. Woodward, R. B., and Hoffmann, R. (1970). The conservation of orbital symmetry. Academic, New York. 92. Fujimoto, H., and Fukui, K. (1974). In Chemical reactivity and reaction paths (ed. G. K. Klopman). Wiley, New York. 93. Elian, M., and Hoffmann, R. (1975). Inorganic Chemistry, 14, 1058. 94. Hoffmann, R. (1981). Science, 211, 995. 95. Hoffmann, R. (1963). Journal of Chemical Physics, 39, 1397. 96. Jahn, H. A., and Teller, E . (1937). Proceedings of the Royal Society of London, A161, 220. 97. Jotham, R. W., and Kettle, S. F. A. (1971). Inorganic Chimica Acta, 5, 183. 98. Gaio, J., Bersuker, I. B., Garay, J., Kabesova, M., Kohout, J., Langfelderova, H . , Melnik, M., Serator, M., and Valach, F. (1976). Coordination Chemistry Reviews, 19, 253. 99. Hathaway, B., Duggan, M., Murphy, A., Mullane, J., Power, C., Walsh, A., and Walsh, B. (1981). Coordination Chemistry Reviews, 36, 267. 100. Pearson, R. G. (1969). Journal of the American Chemical Society, 91, 1252, 4947; (1970) Journal of Chemical Physics, 52, 2167; 53, 2986. 101. Bartell, L. S. (1960). Journal of Chemical Physics, 32, 827; (1968). Journal of Chemical Education, 45, 754. 102. Glidewell, C. (1975). Inorganic Chimica Acta, 12, 219; (1976). Inorganic Chimica Acta, 20, 113. 103. Cotton, F. A., and Wilkinson, G. (1980). Advanced inorganic chemistry (4th edn). Wiley, New York. 104. Pimentel, G. C., and Spratley, R. D. (1969). Chemical bonding clarified through quantum mechanics, HoldenDay, San Francisco. 105. Purcell, K. F., and Kotz, J. C. (1977). Inorganic chemistry. Saunders, Philadelphia. 106. Domenicano, A., Mazzeo, P., and Vaciago, A. (1976). Tetrahedron Letters, 13, 1029. 107. Sutton, L. E . (1958). Tables of interatomic distances and configuration in molecules and ions, Special Publication, No. 11. The Chemical Society, London. 108. Sutton, L. E. (1965). Tables of interatomic distances and configuration in molecules and ions, Special Publication, No. 18. The Chemical Society, London. 109. Allen, F. H . , Kennard, O . , Watson, D. G., Brammer, L., Orpen, A. G . , and Taylor, R. (1987). Journal of the Chemical Society Perkin Transactions 11, S1. 110. Orpen, A. G., Brammer, L., Allen, F. H . , Kennard, O . , Watson, D. G., and Taylor, R. (1989). Journal of the Chemical Society Dalton Transaction, S1. 111. Bent, H . A. (1960). Journal of Chemical Education, 37, 616; (1961). Chemical Review, 61, 275. 112. Dewar, J. S., Kollmar, H . , and Li, W. K. (1975). Journal of Chemical Education, 52, 305. 113. Gilli, G. and Bertolasi, V. (1983). Journal of Chemical Education, 60, 638. 114. Allinger, N. L. (1976). Advances in Physical Organic Chemistry, 13, 1. 115. Altona, C., and Faber, D. H . (1974). Topics in Current Chemistry, 45, 1. 116. Engler, E. M., Andose, J. D . , and Schleyer, P. v. R. (1973). Journal of the American Chemical Society, 95, 8005. 117. Ermer, 0. (1976). Structure and Bonding, 27, 161. 118. Hursthouse, M. B., Moss, G. P., and Sales, K. D. (1978). Annual Reports of The Chemical Society. Section B: Organic Chemistry, 75, 23.
Molecules and molecular crystals 119. Kitaigorodski, A. I., (1978). Chemical Society Review, 7, 133. 120. White, D. N. J. (1978). In Molecular structure by diffraction methods, Vol. 6, (ed. L. E. Sutton and M. R. Truter). The Chemical Society, London. p. 38. 121. Osawa, E., and Musso, H . (1982). Topics in Stereochemistry, 13, 117. 122. Boyd, D. B., and Lipkowitz, K. B. (1982). Journal of Chemical Education, 59, 269. 123. Ermer, 0 . (1981). Aspekte won Kraftfeldrechnungen Volfgang Bauer, Munich. 124. Burkert, U. and Allinger, N. L. (1982). Molecular mechanics. American Chemical Society, Washington, D.C. 125. Allinger, N. L., et al., M M l I M M P l , QCPE 318; Allinger, N. L., and Yu, Y. H. MM2, QCPE 325; Warshel, A. and Levitt, M. QCFFIPI, QCPE 247; Huler, E., Sharon, R., and Warshel, A. MCA, QCPE 325; Andose, J. D., Engler, E. M., Collins, H. B., Hummel, J. P., Mislow, K., and Schleyer, P. v. R. BIGSTRN, QCPE 348; Iverson, J. D., and Mislow, K. BIGSTRN2, QCPE 410; Browman, M. J., Carruthers, L. M., Kashuba, K. L., Momany, F. A., Pottle, M. S., Posen, S. P., et al. UNICEPP, QCPE 361. 126. Biirgi, H. B. (1975). Angewandte Chemie, International Edition in English, 14, 460. 127. MurrayRust, P. (1978). In Molecular structure by diffraction methods, Vol. 6, (ed. L. E. Sutton and M. R. Truter). The Chemical Society, London. p. 154. 128. Biirgi, H. B., and Dunitz, J. D. (1983). Accounts of Chemical Research, 16, 153. 129. Biirgi, H. B., (1985). In Static and dynamic implications of precise structural information, Reports of the 11th International School of Crystallography, Erice, Italy. p. 245. 130. Eyring, H., and Polanyi, M. (1931). Zeitschrift fur Physikalische Chemie, B12, 279. 131. Atkins, P. W. (1986). Physical chemistry (3rd edn). Oxford University Press. 132. Sathyamurthy, N. and Joseph, T. (1984). Journal of Chemical Education, 11, 968. 133. Miiller, K. (1980). Angewandte Chemie, International Edition in English, 19, 1. 134. Biirgi, H. B. (1975). Angewandte Chemie, International Edition in English, 87, 461. 135. Biirgi, H. B. (1973). Inorganic Chemistry, 12, 2321. 136. Britton, D . , and Dunitz, J. D. (1981). Journal of the American Chemical Society, 103, 2971. 137. Biirgi, H. B., Dunitz, J. D., and Schefter, E . (1973). Journal of the American Chemical Society, 95, 5065. 138. Biirgi, H. B., Dunitz, J. D . , Lehn, J. M., and Wipff, G. (1974). Tetrahedron, 30, 1563. 139. Biirgi, H. B., Dunitz, J. D., and Shefter, E . (1974). Acta Crystallographica, B30, 1517. 140. Gilli, G . , and Bertolasi, V. (1979). Journal of the American Chemical Soceity, 101,7704. 141. Gilli, G . , Bertolasi, V., Bellucci, F., and Ferretti, V. (1986). Journal of the American Chemical Society, 108,2420. 142. Winkler, F. K., and Dunitz, J. D. (1971). Journal of Molecular Biology, 59, 169. 143. Biirgi, H. B., and Shefter, E., (1975). Tetrahedron, 31, 2976. 144. Krygowski, T. M., Anulewicz, R . , and Kruszewski, J. (1983). Acta Crystallographica, B39, 732. 145. Hinze, J. and Jaffk, H . H. (1962). Journal of the American Chemical Society, 84, 540; (1963). Journal of Physical Chemistry, 67, 1501.
1
533
534
1
Gastone Gilli 146. Hinze, J., Whitehead, M. A., and Jaffk, H. H., (1963). Journal of the American Chemical Soceity, 85, 148. 147. Iijima, K., Ohnogi, A., and Shibata, S. (1987). Journal of Molecular Structure, 156, 111. 148. Ferretti, V., Bellucci, F., Bertolasi, V., and Gilli, G. (1985). Proceedings of the IX European Crystallographic Meeting, Torino, p. 337. 149. Bertolasi, V., Gilli, P., Ferretti, V., and Gilli, G. (1991) Journal of the American Chemical Society, 113, 4917.
Protein crystallography
Introduction Protein crystallography, the subject of this chapter, is a specialized branch of crystallography that investigates, by using diffraction techniques on single crystals, the threedimensional structure of biological macromolecules.[lsl For a long time, good quality single crystals were obtainable only for globular proteins. Nowadays, other biological macromolecules, like tRNA, polysaccharides, and polynucleotides, give crystals suitable for Xray analysis. Therefore, the techniques for structure solution and refinement described in this chapter apply to all cases where crystals with a high portion of unordered solvent can be grown. Despite the fact that crystals of proteins have been known since the beginning of the century, only around 1960 were the first structures, myoglobin and haemoglobin, e l ~ c i d a t e d . ~Their ~ ] resolution was made possible mainly by the development of the isomorphous replacement technique. Since then, a lot of theoretical and technical advances have been made: among them, the use of anomalous dispersion, molecular replacement, and the development of oscillation techniques in data collection of crystals with large cell dimensions. At the end of the 1970s the growth of computing power made possible the refinement in reciprocal space. In the meantime, the introduction of powerful and affordable graphic stations brought the development of interactive graphic software, allowing faster interpretation of electron density maps and model building. Only in very recent years has the availability of synchrotron radiation and twodimensional detectors made data collection a routine procedure. An idea of the 'state of the art' of protein crystallography is given by the Brookhaven Protein Data Bank (thereafter called PDB),[~]which collects coordinates of the macromolecular structures solved, mainly by Xrays. Looking at the January 1989 release, one finds, perhaps with some surprise, that only 413 sets of coordinates are available (plus 86 bibliographic entries, that is structures solved but not yet deposited).? They include 10 polysaccharides, 26 DNA fragments, 6 tRNA, and 18 model structures. The remaining 353 are protein structures, including 14 virus coat proteins: taking into account the fact that most of them are related proteins or variants of the same molecule (there are for example 34 lysozyme variants or mutants, 12 haemoglobins, and 8 myoglobins), this number must be considered quite small and demonstrates that solving the structure of a new macromolecule ? I t must be remembered that the Protein Data Bank cannot be considered fully representative of the macromolecular structures so far solved, since not all of them are quickly deposited.
536
1
Giuseppe Zanotti
still remains a long and demanding job. But possibly the reason for the relatively low number of new structures published every year is the crystallization process, a field in which technical (and theoretical) advances have proceeded very slowly and which remains the more uncertain step in protein structure determination.
Protein crystals It is the solvent content that makes the difference between a classical molecular crystal and a protein crystal: in the former, all the atoms can be described in terms of a regular lattice, whilst in the latter a crystalline array coexists with a high portion of material in the liquid state. The mother liquid, whose content can range approximately from 30 to 75 per cent or more, has a strong influence on the behaviour of this kind of crystal, making them very peculiar and creating some advantages along with some obvious disadvantages. Among the latter, the major one is that protein crystals are much less ordered than classical crystals, not only for the large amount of unordered material present in the crystal itself, but also because surface groups of the macromolecule in contact with the solvent can show a great mobility. As a consequence, diffraction data cannot be measured to the resolution normally attainable with 'small' molecules. On the other hand, among the advantages, the environment of the macromolecule in the crystal is not too different from that of the solution from which the crystal was obtained (the influence of the solvent on the conformation of the protein cannot be underestimated) and we can profit from the solvent in the preparation of heavyatom derivatives, as will be described in the next paragraph. A last important point must be remembered about protein crystals: since inversion symmetry elements are not allowed, the number of possible space groups is reduced from the original number of 230 to 65 (see Chapter 1, p. 24).
Principles of protein crystallization The process of crystallization of a macromolecule is very complex and poorly understood. A theoretical treatment of it, despite recent progress,[s1 is at present impossible. Nevertheless, a lot of experience has been accumulated on the crystallization of watersoluble p r ~ t e i n s , [ ~ , and ~ , ~ a~ J ~ ] crystallographer starting with enough pure material has a reasonable chance of succeeding in obtaining Xray quality crystals. The same does not yet apply to membrane proteins, the crystals of which have been very seldom obtained.[12,13] Growth of a protein crystal starts from a supersaturated solution of the macromolecule, and evolves towards a thermodynamically stable state in which the protein is partitioned between a solid phase and the solution. The time necessary before the equilibrium is reached has a great influence on the final result, that can go from an amorphous or microcrystalline precipitate to large single crystals. The supersaturation conditions can be obtained by the addition of precipitating agents and/or by modifying some of the internal parameters of the solution, like p H and temperature. Since a
Protein crystallography Table 8.1. Precipitating agents commonly used for growing protein crystals suitable for Xray analysis. The list is not intended to be exhaustive Class
Examples
Inorganic salts
(NH4),S04, Na,SO,, NaCI, KCI, NH4CI, MgSO,, CaCI,, NH,NO,, LiCl
Organic salts
Citrate, acetate, formate cetyltrimethyl ammonium salts
Organic solvents
Ethanol, isopropanol, acetone, dioxane, 2methyl2,4pentanediol(MPD)
protein is a labile molecule, all the extreme conditions of precipitation, pH, and temperature should be avoided. And indeed, the understanding of the biological and physiological properties of the macromolecule via the determination of the threedimensional structure is much easier if crystals are grown in conditions not too far from the physiological environment in which the molecule operates. The precipitants frequently used can be divided into three categories: salts, organic solvents, and polyethylene glycols (PEG). A list of the more common among them is reported in Table 8.1. 1. pH. The pH value has a strong influence on the solubility, which has a minimum at a pH close to the isoelectric point of the macromolecule. 2. Salt concentration. Ionic strength can have opposite effects on protein solubility, i.e. solubility decreases exponentially with increasing ionic strength, a phenomenon known as saltingout, but it also has a minimum at very low ionic strength, the saltingin effect. In practice, precipitation can be achieved by increasing the salt concentration or by dialysing the solution of protein against water. 3. Organic solvents. Precipitation properties of organic solvents can be ascribed to the double effect of subtracting water molecules from the solution and to decreasing the dielectric constant of the medium. They can sometimes have effects on the protein conformation too, and for this reason they should be used with caution.
4. PEG. PEG is a precipitating agent with peculiar properties: it is a polymer, available in molecular weights ranging from about 200 to 20 000 Da;t its effect on solubility, along with some properties in common with salts and organic solvents, is due to volume exclusion property: the solvent is restructured and phase separation is consequently promoted. PEG is of wide applicability, and has been demonstrated to work with proteins that were crystallized with other precipitating agents.[lO] Several others parameters and factors can influence the crystallization process: among them, the protein concentration, the temperature, the presence of cations that sometimes stabilize the conformation of the protein, and the purity of the sample. The presence of contaminants can be extremely important in preventing the formation of crystals suitable for Xray analysis.
t The molecular weight is expressed in Dalton, I Da = 1.6604 X
g.
1
537
538
1
Giuseppe Zanotti
The solvent content of protein crystals The amount of the solvent contained in a protein crystal has been discussed by ~ a t t h e w s , [ ' ~who ] analysed data from 116 distinct crystal forms. He defined the quantity VM, given by the ratio of the volume of the unit cell divided by the total molecular weight of the protein in the cell. Therefore, ,V represents the crystal volume per unit of protein molecular mass: it is practically independent from the volume of the asymmetric unit and mostly V has a value depends on the solvent content. In the crystals examined, , ranging from 1.6A3 ~ a  'to about 3.5A3 Dal, but more extreme values have been found. A special trend can be observed if the molecular weight of V and the proteins is taken into account: small proteins tend to have small , big proteins a large one, which is understandable, since a low ,V means a low solvent content. Calling V,,,, the crystal volume occupied by the protein, V; its fraction with respect to the total crystal volume V and M,,,, the mass of protein in the cell: since the first term in parentheses represents the specific volume of the protein and the second the reciprocal of VM, and remembering that molecular weight is expressed in Da: If we assume a value of about 1.35g cmP3 for the protein density, as a first approximation:
V; v:,,"

1.23/VM
(8.3)
v;.
(8.4)
=1
The most important information contained in VM is not the solvent content, but the molecular mass of macromolecule in the crystal cell. Very often the number of molecules per asymmetric unit can be determined unambiguously, when the molecular weight of the protein is known, at least approximately. For monomeric proteins, or for those without the possibility of internal symmetry, the number of molecules in the cell is relevant only for the subsequent steps in structure determination. For multimeric proteins, composed of identical subunits, this number may be of relevant biological consequence: in fact, if some of the internal symmetry elements are coincident with the crystallographic ones, the relative arrangement of such subunits in the molecule is immediately available.[151 The experimental determination of the density of the protein crystal, along with that of the dried content of the crystal itself, can allow a quite accurate determination of the molecular mass of the protein contained in the asymmetric unit, and consequently the molecular weight of the protein. These techniques have been reviewed by ~ a t t h e w s , [ ' ~but ] the reader must be warned that the experimental measurement of the density of such kinds of crystals is difficult and the results very often uncertain.
Preparation of isomorphous heavyatom derivatives Isomorphous heavyatom derivatives are of paramount importance for the solution of the phase problem in protein Their prepara
Protein crystallography Table 8.2. Representatives of heavyatom compounds used i n protein crystallography for preparation of derivative^[^,^' (Ac = acetate) Classes
Examples
Platinum compounds
K,PtCI, K,Pt(CN),, K,Pt(NO,),, Pt(NH,),CI, or Br,, PtCI,, PtCI,, Pt(ethylenediamine)CI,
Mercury compounds
HgCI,, HgAc,, mersalyl acid, pchloromercuribenzoic acid, methylmercury acetate, ethylmercury chloride
Uranyl salts
UO,(NO3),
Rare earths
SmAc,,
Others
KAuCI,, KAu(CN),, PbAc,, PbCI,, (CH,),PbAc ASNO, K,lrCI,
EuCI,
tion is made possible by their quite high solvent content: the presence of channels of disordered or only partially ordered liquid allows the diffusion of relatively small compounds into the crystal. Reactions among the diffused compounds and eventual accessible reactive sites of the protein can take place. In some special cases, protein molecules are derivatized in solution and subsequently crystallized, but the former procedure is simpler and it is advisable to try it first. In practice, the crystal is soaked in a solution of its mother liquid in which the heavyatom compound has been dissolved. A list of the more commonly used heavyatom derivatives is given in Table 8.2. Concentration of heavy atoms and time of soaking are the most relevant variables: they can range from 0.001 M to 0.1 M and from a few hours to several days (these numbers must be considered only a rough indication, since extreme cases have been reported). These conditions strongly depend on the protein under study, on the precipitating agents, on the pH used, and on the temperature. 1. pH. At high pH (greater than 9) the acidic groups of the protein are mostly negatively charged, and potentially they can react with cations. At the same time, many heavy atoms form insoluble hydroxides. At low pH, on the other hand, potentially reactive groups will be protonated and prevented from reacting.
2. Precipitating agents. High salt concentration is not the ideal medium for heavyatom reaction with proteins, not only because the solubilization of the compound can be prevented by a very high salt concentration, but also because ions in the solution will compete with the protein. Polyethylene glycol solutions on the contrary provide favourable conditions for heavyatom reactions, since PEG does not react with most of the compounds commonly used.
3. Temperature. There is an obvious kinetic effect of temperature on heavyatom reactions, which are slower at 4 "C than at room temperature. Very often preparation of heavyatom derivatives is a trial and error technique, unless some special features of the macromolecule are known a
1
539
540
1
Giuseppe Zanotti
priori. When the threedimensional structure has been solved, a rationale for the behaviour of the specific system can be inferred: unfortunately, at that time it becomes useless.
How isomorphous are isomorphous derivatives? The term 'isomorphous derivative' ideally indicates a crystal where some solvent molecules have been replaced by some group of atoms with more electrons, without any alteration of the structure of the protein or of the crystal lattice itself. In practice, this never happens: the introduction of a bulky compound which interacts with some of the atoms on the surface of the protein will give rise to local movements and displacements of atomic groups, at least in the close vicinity of the binding site. To check if some reaction has taken place after the soaking of a crystal in the heavyatom solution, diffraction data have to be collected. To avoid wasting time, a visual inspection of a single precession photograph, compared with the same zone of the native protein, is often enough to judge about the quality of the derivative. A more quantitative test is given by the comparison of structure factor data: an agreement index, R (see pp. 309 and 312), between native and derivative data can be calculated and the entity of the substitution can be roughly evaluated from it; experience indicates that a value from 0.15 to 0.25 can be considered a reasonable agreement factor. A smaller value is an index of little substitution, too high a one must be regarded suspiciously, as a clue to nonisomorphism. Lack of isomorphism can be confirmed by other parameters: a change in cell length of less than about 1.5 per cent can be tolerated to a resolution of about 3 A , but it could be deleterious at 2 A . Furthermore, the mean difference among structure factors amplitudes must be practically constant over the entire range of 8 used: quite large differences at low resolution and very low at high resolution indicate disordered heavyatom binding, whilst an increase of the differences with d spacing is an index of nonisomorphism.['l
The solution of the phase problem The following section is entirely concerned with primary phasing, that is the determination of approximate phase angles of protein structure factors. First the two main methods used to solve the phase problem in protein crystallography, isomorphous replacement and anomalous scattering, are described, without taking into account the experimental errors. Their treatment is introduced later, along with the techniques of phase refinement. Methods to improve the electron density maps and rotation and translation functions, that in some cases can help to solve the phase problem, have been left for the end of the chapter. A brief mention of the application of direct methods to macromolecular crystallography is given in the last subsection.
The isomorphous replacement method The method of isomorphous replacement is a cornerstone in protein crystallography: not only has it been used to solve the phase problem for the
Protein crystallography first protein structures, but it remains, with few exceptions, the only procedure available to solve the structure of completely new proteins.[''] Let Fpbe the structure factor of the native protein, Fp its magnitude and rpP its phase. FpH, FpH, and rppH are the corresponding quantities of the heavyatom derivative. If we assume a perfect, 'ideal' isomorphism, the relationships between Fp and FpHis illustrated in Fig. 8.1 and can be written: where FH is a vector representing the contribution of the heavy atom 'alone'. Our final goal is to derive the value of pp, but the only quantities in the figure that can be measured are Fp and FpH.On the contrary, FHcannot be measured, but since it represents the contribution of few atoms, it can be calculated if their atomic coordinates and thermal parameters are known. Let us first describe a way to determine the positions of heavy atoms and, from them, to calculate FHand derive an estimate for rpp.
The determination of heavyatom positions For a small molecule, the heavyatom positions can be determined via a Patterson map calculated using measured amplitudes (see p. 328). The same map is not useful for a macromolecular crystal: even for a small protein, the ratio among the number of electrons of the heavy atoms and those of the macromolecule is so low, that a Patterson map calculated with the coefficients of the protein derivative will look absolutely meaningless. But if the structure factor amplitudes of two isomorphous crystals are known, various kinds of differencePatterson syntheses can be calculated. The 'true' difference~atterson[l']synthesis would be that calculated using as coefficients IF;,  F;\. This map represents the difference between the Patterson of the derivative minus the Patterson of the native protein. In fact, remembering (8.5):
The righthand side of eqn (8.6) shows that the Patterson map calculated with these coefficients will contain peaks corresponding to heavyatom heavyatom vectors, FL, and to heavyatom proteinatom vectors, the mixed terms. A more common choice among protein crystallographers is to calculate a Patterson synthesis using coefficients (FpH F,)'. This was originally called modulus difference squared synthesis, but is commonly known as The resultant map has several interisomorphous difference~atterson.['~] esting features, but the main reason for its success is that it is more representative of the heavyatom situation. In particular, in the centrosymmetric case (that is for centric? projections in a noncentrosymmetric space group), since FpHand Fp are collinear, these coefficients represent a true estimate of the value of FH. In fact:
t The word centric is used here in a general sense, indicating that phases are restricted to two values, not necessarily 0 or x.
1
541
.%
2 d,
2
I
Real axis
Fig. 8.1. Representation in the Argand plane of ~
~
i
~
'
~
~
atom derivative (F,,), assuming a perfect i~omorphismofthetwocrystals.
~
~
~
~
542
1
Giuseppe Zanotti
Since FH is usually small if compared with the modulus of the structure factors of protein and derivative, in general the relationship FH= IFPH FPI
(8.8)
will be satisfied. In few cases, when FpHand Fp are both very small, it may happen that FH=FPH FP This is called a crossover, and it can be removed from the calculation. For a centric projection a Patterson synthesis calculated with coefficients (8.8) will correspond to the Patterson map of the heavy atoms alone, that is it will contain peaks corresponding only to the vectors relating heavyatom positions. Methods to derive the atomic coordinates from a Patterson map are described on pp. 328 to 335. In favourable cases, i.e. when more than one centric projection is available, the three coordinates of the heavy atoms can be obtained. For general reflections, IFpH FPI will not be a correct estimate for FH. From Fig. 8.1:
+
F&= Fc + FEH  2FPHFPCOS ( q p  qPH).
(8.9)
If the phase angles of protein and derivative structure factors are very similar, that is if the two vectors FpHand Fp are nearly collinear, the cosine term is close to 1 and:[17] F&= F:
+ F : ~ 2FPHFP= (FPH F P ) ~ .
(8.10)
The probability distribution of the values of q,  qpHhas been analysed by ~ i m [ ~(see ~ , also ~ ~ 1p. 393): the larger the value of the product FpHFp,the more likely the difference Iqp qPHIis to be small, an vice versa. Equation (8.10) does not represent a good approximation for small structure factors, but the latter will give a small contribution to the Fourier transform. In practice, a Patterson map calculated with coefficients (8.8) will tend to the Pattersondifference of the heavy atoms alone in the noncentrosymmetric case too (for a general discussion of the features of differencePatterson maps, see Ramachandran and ~rinivasan['~]).
The single isomorphous replacement (SIR) method Once the position of heavy atoms is more or less accurately known, the calculated value of I;;I can be used to estimate the phase angle of the structure factor of the native protein. From Fig. 8.1, using simple trigonometric considerations,? we can write:
Fc, = F$ + F ~ H + 2FpFHCOS 6, cos 6 = (F;,
 Fc  F & ) / ~ F ~ F ~ ;
(8.11) (8.12)
8 corresponds to qp q H , and since qHis known, q,, the phase angle of Fp, can be derived: Fig. 8.2. Graphic construction of S.I.R. method, showing the two possible values for the phase angle of the native structure factor F,. The structure factor of the protein is a vector lying on a circle of radius Fp and centre 0. If a circle of radius F,,, the modulus of the structure factor of the heavyatom derivative, is drawn with centre in the end of the vector F,, the intersection of the two circles represents the two possible solutions of (8.13).
Equation (8.13) contains a cosine term, consequently two solutions exist for qp. This ambiguity is illustrated in Fig. 8.2, where two circles of radius Fp and FpHare drawn with centre respectively in 0 and at the end of vector FH: the intersections of the two circles represent the two possible solutions
t An alternative way of
deriving eqn (8.11) is given in Appendix 8.A
Protein crystallography
for cpp. It is important to notice that this problem is immediately solved for restricted phase reflections, for which eqn (8.12) becomes:
Since the value of FHis known from calculation and the values of FpHand Fp from observation, the relative sign of Fp with respect to FH can be determined unambiguously from the comparison of the magnitude of the three vectors (Fig. 8.3). For general reflections this is unfortunately not true, and the ambiguity between the two possible values for the phase angle must be solved with other techniques. In principle, a threedimensional electron density map could be calculated, using the two possible phase values: this kind of synthesis is called an SIR map and it will contain information about the true structure plus noise.['lI In fact, if we call cp, the correct phase value of cpp and cppw the wrong one, looking at Fig. 8.4 we can write: WSIR= FPexp (i~,)
+ FPexp (~vPw).
(8.16)
Since cp, = 1/2(cppT+ cppw), then: (8.17)
F,
1
543

FP
A
*

 FPH
FP
(c) Fig. 8.3. The sign of reflections of centric zones can be fully determined using only one heav atom derivative (after Blundell and Johnson ). When F, is small compared with F, and F,,, case (a) and (b)apply: if F,< F,,, the sign of F, is equal t o that of F,; if F,> F,, the sign of F, is reversed. The socalled 'cross over', represented in (c), may occur when F , is larae and F. is small: despite the condiiibn F,; F,,, thk sign of F, is reversed with respect t o F,.
16
From (8.17) it is evident that FsIRwill approach the correct value of Fp if cpH .= cp,,. But since we have no reason to believe the numerical values of cpH and vPTare correlated, the first term of (8.17) will give the correct electron density, while the second one will only contribute to noise. In practice the level of noise in this kind of map is so high that its interpretation is extremely difficult. A
The classical solution of the problem of phase ambiguity: the MIR technique The multiple isomorphous replacement technique, MIR, has been the first method used to solve this phase ambiguity, and it remains the more common and is widely adopted. It is based on the preparation of a second heavyatom derivative having heavy atoms bound to the protein in position(s) different from those of the first one. Let us assume we have measured coefficients from two derivatives, called FpHland FPH2,and in some way we have calculated FHland FH2(that means we know the positions of the heavy atoms of the two derivatives, relative to the same origin). The complete solution of the phase problem can be illustrated using a diagram due to ~ a r k e r , [illustrated ~~] in Fig. 8.5: a circle of radius Fp centred on the origin 0 of an Argand plane is drawn, and from 0 the two vectors FHl and FH2; they are in turn the centres of two circles of radii FpHland FPHZ respectively. Since the two derivatives are assumed perfectly isomorphous, the three circles must intersect in one point (B in Fig. 8.5): the vector OB will coincide with the structure factor of the protein. The graphical construction just described is equivalent to solving a pair of
\Real.
Fig. 8.4. The same diagram shown i n Fig. 8.2, except that now the 'true' and the 'wrong' value for the native structure factors are explicitly indicated as F,, and Fpw respectively. It can be seen that the further the t w o vectors are from each other, the more the S.I.R. phase (corresponding t o rp,) is different from rp,.
544
1
Giuseppe Zanotti
simultaneous equations like (8.13):
Real axis
In principle, two different heavyatom derivatives supply a unique, unambiguous value for the phase angle of the native protein. In practice, errors from various sources prevent system (8.18) from having an exact solution.
Anomalous scattering: a complementary (or alternative) approach to the solution of the phase problem Fig. 8.5. Harker construction illustrating the M.I.R. method. A second circle of radius F,,, and centred at the end of vector F,, has been added to the construction of Fig. 8.2. The three circles have only one common intersection, representing the solution of the two equations (8.18).
I
According to Chapter 3 (p. 167), the structure factor may be rewritten as the sum of two parts:
where the real part of anomalous scattering (the socalled anomalous dispersion) is included in F1(hkl). If F"(hk1) is not zero, the practical result is the breakdown of Friedel's law: F(hk1) is no longer equal to ~ ( i i i and ) the Friedel pairs are more correctly called Bijvoet pairs. Anomalous scattering is negligible for light atoms like carbon, nitrogen, or oxygen (that is, nearly all the atoms of a protein) and can be of practical use for a native protein molecule only in special cases, when heavy ions are bound to it. Even if for a very small protein the sulphur's anomalous scattering has been used to solve a structure ab i n i t i ~ , [in ~ ~general ] the anomalous scattering phenomenon becomes relevant for heavyatom derivatives. Equation (8.5) must be in fact modified, as shown in Fig. 3.15 and Fig. 8.6:
Real axis
Fig. 8.6. Vector diagram showing F& and F& (superscripts and  indicate_t_he two terms of the Bijvoet pairs, i.e, hkland hkl; the components are drawn reflected across the real axis). The two vectors have different magnitudes, due to the anomalous contribution of the heavy atoms. F,!, is the real and FA the imaginary component of F,.
+
I
Real axis
Fig. 8.7. For restrictedphase reflections, if only one type of anomalous scatterer is present, F:, and F& have the same magnitude, independent of the size of the imaginary component.
where superscripts + and  stands for (hkl) and (iRi), respectively. If the heavyatom derivative contains only one kind of anomalous scatterer, vectors F h and Ffl, are mutually perpendicular, and if we call QI, the phase angle of vector F h , QI, f n / 2 will be that of Ffl,. This fact can be considered practically always true for protein derivatives, and has the important consequence that anomalous effect cannot be observed if the vectors Fpand FHare collinear, for example for all the centric reflections (see Fig. 8.7). An accurate measurement of the Bijvoet pairs allows the calculation of an anomalousdifference Patterson synthesis, with coefficients:
Notice that we do not need native coefficients for the calculation, so (8.21) is also useful when an anomalous scatterer is present in the native protein crystal. A map calculated with coefficients (8.21), supposing the anomalous contribution Ffl, is small compared with Fp, which is very often true in our case, will contain maxima corresponding to vectors relating the positions of anomalous scatterers. This synthesis was for example used by ~ o s m a n n [ ~ ~ ] to determine the Hg position in two derivatives of horse haemoglobin. Other kind of anomalous Patterson maps with coefficients different from
Protein crystallography
(8.21) can be produced, like the aanomalous or the Panomalous synthesis.[Is1 The most important application of anomalous scattering in protein crystallography remains the possibility of solving the phase ambiguity discussed in the previous ~ a r a g r a p h . [ ~Let ~  ~us~ assume ] we have only one heavyatom derivative, and we have measured F;,, FFH, and FP.T Moreover, the position of the heavy atom(s) are known. Looking at Fig. 8.6, an expression for the phase angle of the derivative, whose complete derivation is given in Appendix 8.A, can be written:
F;,
 FFH= 2FA sin (qpH qH)
qPH= qHf sin' [(F:,
 F&)/2FA].
1
545
Real axis
(8.22) (8.23)
Equation (8.23) gives again two possible solutions for qp,, but since it contains a sine term, its information is complementary to that of (8.13): the phase angle can now be fully determined. Information from both sources, isomorphous replacement and anomalous scattering, is used in Fig. 8.8, where the role of the second derivative of Fig. 8.5 is played by anomalous scattering.
The use of anomalous scattering in the determination of the absolute configuration of the macromolecule Two isomorphous derivatives are, in principle, enough to determine the correct value of the phase angle qp of the structure factor, but the M.I.R. method alone does not allow us to select the correct enantiomorph for the protein. Once a righthanded system has been chosen in indexing the reciprocal lattice, the initial arrangement of the heavy atoms for the first derivative is arbitrary. In other words, the phase of FHcan be q,, as in Fig. 8.2, or qH. Once a hand has been arbitrarily selected for a heavyatom derivative, all the others must simply be consistent with it, but they can all be relative to the wrong enantiomorph. If this is the case, the electron density map will represent the mirror image of the correct structure, that is all the amino acids will have D configuration. When a medium (or high) resolution electron density map can be produced, some overall features may indicate that the wrong enantiomorph has been chosen (for example, ahelices will appear lefthanded instead of righthandedthe amino acid configuration and ahelices are described on p. 574). Then the problem can be immediately corrected by recalculating the phases with the heavy atoms arranged in the other way. However, anomalous scattering differences can be used to identify from the beginning the correct enantiomorph, using an extension of the method proposed for small molecules by B i j v ~ e t . [We ~ ~ ]have seen in the previous subsection that, at least in principle, structure factors for one single heavyatom derivative along with its anomalous differences can solve the phase ambiguity of the protein. This is no longer valid if two possibilities are taken into account for the value of q,, since now there are two possible
t Readers must be warned that measurement of Bijvoet pairs requires very accurate data collection, since anomalous differences are very often of the same order of magnitude as the experimental errors on intensities. Synchrotron radiation is extremely helpful in this respect: thd appropriate wavelengths that optimize the anomalous effect can be selected (see p. 239).
Fig. 8.8. A graphical representation of the solution of the phase problem using one heavyatom derivative and its anomalous absorption component. Two circles of radius F+,, and F, P are drawn at the end of vectors F, and F, respectively. OA is the native protein structure factor, whose phase angle is uniquely determined by the intersection of the three circles.
546
1
Giuseppe Zanotti
Real axis
Fig. 8.9. Graphical illustration of the ambiguity in the choice of enantiomorph. This figure is equivalent to Fig. 8.2, except that now two possible arrangements of the heavy atoms for the same derivative are shown. Vectors OA and OB are the two possible structure factor values for the native protein if v, is selected as the phase of the heavyatom derivative; vectors OA' and OB' those corresponding to q,, that is to the enantiomorph.
value of q, associated with every qH. Let us assume the solution for the phase angle of the derivative structure factor, from (8.A.7) and (8.A.15), is qpH= qH+ 6. We are left with another ambiguity, since the original choice of q H was arbitrary: the two possibilities are in fact qpH= qHt 6 or qpH=  qH 6, and they determine the selection of the enantiomorph (Fig. 8.9). At least two heavyatom derivatives and anomalous differences for one of them are necessary to select the correct hand of the molecule: using phases from one derivative along with anomalous contribution and the heavy atoms in the two possible arrangements, two differenceFourier of a second one are calculated. Peaks in the difference map calculated with atoms in the correct hand will be reinforced, those with the wrong one lowered.[']
The treatment of errors In the previous paragraphs, we assumed that all the measurements were errorfree and that a perfect isomorphism existed among crystals of the native protein and derivatives. This is obviously not realistic, since Fp and FPHare experimentally measured quantities and FH is calculated from approximate heavyatom positions. Experimental errors can be considered to arise from three different sources: (1) errors in intensities, mainly attributable to inaccuracy in measurements, scaling etc. ; (2) errors in position, occupancy, and temperature factor of heavyatoms; (3) lack of isomorphism, due to displacement of protein atoms and of solvent molecules close to the heavyatom binding site, etc. As a consequence, the circles of Fig. 8.5 are not expected to intersect at the same point and the system of equations (8.18) will not have an exact solution (Fig. 8.10). Following Terwilliger and ~ i s e n b e r g , [let ~ ~us ] denote the different contributions to the total error deriving from points (I), (2), and (3) as a, q, and p, respectively. It must be noticed that, whereas a, and apH,the standard deviations for Fp and FpH,are routinely evaluated (see pp. 271 and 280) an a priori estimate of q and p is impossible. The systematic treatment of errors in the isomorphous replacement was pioneered by Blow and Crick.[301They made two basic assumptions: all the errors reside in the calculated structure factor of the derivative, FpH(c,Ic); errors follow a Gaussian distribution. Consequently, a phase probability distribution for derivative j is given by:
Real axis
Fig. 8.10. Harker construction analogous to Fig. 8.5. where, due to lack of isomorphism and errors in the data, the three circles of radius F,, F,,,, and F,,, do not intersect at the same point.
 FPH(calc) in (8.24) is called lack of closure and is The difference FPH(obs) usually denoted by E,; its physical meaning is illustrated in Fig. 8.11, which is a realistic picture of what was idealized in Fig. 8.1: now the triangle formed by the three vectors F,, FPH, and FHdoes not close. The lack of closure depends from the phase of the protein, since:
ni in (8.24) is a normalizing factor and Ei is a measure of the total error. The choice of .E, is crucial and not obvious. In practice, the value commonly
Protein crystallography
.V)
i3
9
E I
(a)
Real axis
Fig. 8.11. (a) Representation of the lack of closure E, following the Blow and Crick assumption that all the errors reside i n the F,, amplitude. As a consequence of it, F,,(,,,,, is equal t o Fp~ ,,, E . (b) components of the error described in (a) are now explicitly shown: ,u is the lack of isomorphism and q the difference ., between the true and the estimated value of F The third source of error, the inaccuracy i n the measurement of Fp and F,, prevents the closure of the polygon.
+

(b)
Real axis
used is:[311 The righthand side of (8.26) represents the mean square value of the lack of closure residual. Since it depends from the resolution, it is evaluated in ranges of sin 8/A. An a priori derivation of (8.24) along with that of E; for centric and acentric reflections has been obtained by Terwilliger and ~ i s e n b e r ~asl ~a~ ] function of all the different sources of errors:
Equations (8.27a) and (8.27b) are not of direct use, since we lack a value for q and p, but from them a theoretical justification of (8.26) can be obtained.[291 If more than one derivative is present, (8.24) can be modified to give the total probability distribution of the phase of a reflection:
The sum is extended to all the j derivatives used in calculating the phases. A diagram showing P,(q,) for the hypothetical derivatives of Fig. 8.10 is reported in Figs. 8.12(a) and (b), and the total probability in Fig. 8.12(c). The lack of closure for anomalous scattering measurements assumes a different form:[25,26,291
but the probability for the phase of the structure factor due to the anomalous scattering is analogous to (8.24):
E,,, is usually smaller than Eiso and can be estimated for example from the agreement among centric reflections.[251If isomorphous and anomalous information are available for the derivative j, they can be combined to give a total probability: P,(?'P ')
= (q(iso,(q~>)(P,(an01(9~)).
(8.31)
On the basis of a different formulation of the error model. Hendrickson and
1 547
548
1
Giuseppe Zanotti ~atmann[~'] proposed a different representation of the phase probability distribution: ~ ( v P=) exp (K + A cos qp+ B sin qp+ C cos 2 q p + D sin 2qp). (8.32) Equation (8.32) has the advantage of being completely general and that new information can easily be included. Moreover, the old probability can be expressed using coefficients A, B, C, and D through a leastsquares fitting.[331Since the overall probability distribution is given by the product of individual probabilities:
if every one is cast in the form (8.32), Ptot(qp)can be obtained by the sum of the individual coefficients:
+ C. Ci cos 2 q p + C D~sin 2 q p i
i
From (8.33) or (8.34) we can calculate the probability distribution of the phase angle for every structure factor and use the most probable phase in the calculation of an electron density map. This is called the most probable Fourier, and in principle it would be a good approximation. Unfortunately, P(qp) tends to be bimodal, and the use of the most probable phase can introduce large errors (see Fig. 8.12(c)). According to Blow and Crick,[301 the Fourier which is expected to have the minimum mean square difference from the 'true' Fourier is that obtained using the centroid of the probability distribution of Fp, that is: 2n
F ~ ,= NFP ~ ~ ~~ )( 9exp ~ (MP) ) dqP
(8.35)
where N is a normalization factor: Fig. 8.12. (a) Lack of closure, cj, for the t w o derivatives shown in Fig. 8.10. c, assumes the value 0 at the intersections of the circles of radius Fp and FpHj. Since the three circles do not intersect at the same point, this happens for values of @,different for each derivative. (b) q(qp), calculated on an arbitrary scale using (8.24), for the t w o derivatives: q(p,) has a maximum every time cj = 0.(c) Combined probability for the t w o derivatives. p, represents the most probable phase, p, the Best phase, that is the centroid of the probability (see text for more details).
Equation (8.35) is equivalent to: where m is a weighting function called the figure of merit: (8.38) qP(best) can be calculated easily by developing (8.38) and observing that P(qp) can be sampled and the integral substituted by a sum:
Protein crystallography
The sum is estimated for the i values of qp at which the probability is evaluated, usually at intervals of 10 or 20 degrees. The figure of merit is a value ranging from 0 to 1 and is a measure of the reliability of the phase qp: in principle, m = 1 means an error of O" in the phase angle, m = 0.5 means an error of 60".
The refinement of heavyatom parameters Once an approximate position of one or more heavy atoms has been found, the problem immediately arising is the refinement of their coordinates, thermal parameters, and occupancy. Refinement is made difficult by the we can only have estimates of it. lack of a correct value of FH(obs): Historically, the first method of refinement of heavyatom parameters was proposed by ~ossmann,["] who suggested minimization, using classical leastsquares methods:
FH(calc) can be calculated in the usual way from the known heavyatom is available only for centric parameters, but a correct estimate of FH(,bs) reflections (see p. 541), so (8.41) should in principle be employed to refine that class of reflections and the refined parameters used to calculate all the phases. Nevertheless, since (8.8) can be considered an approximate estimate of FH(obs),expression (8.41) has sometimes been used to refine acentric data.$ Possibly the most used and most popular refinement scheme among protein crystallographers is the socalled phase refinement, introduced for the first time in the refinement of myoglobin.[341 The quantity minimized is:
which represents the leastsquares minimization of the lack of closure, where: (8.43) F ~ ~ ( c a l c= ) IFp(obs) exp ( ~ v P+ ) FH(calc)l. In general w is chosen as the reciprocal of the total error E, calculated from (8.26) for the derivative being refined.§
t In the rest of the chapter, unless otherwise specified, the sums are extended to the appropriate set of reflections. $If anomalous scattering data are available, a more accurate approximation of FH (see Blundell and ~ohnson['])is represented by
+
and upper (F,,) estimates, respectively. It has The  and values are called lower (F,,) been shown that the lower estimate would represent the correct value of FH for the large majority of the reflections. It must be considered, in any case, that when anomalous differences are low or the measurements are affected by large errors, coefficients (8.8) can be more safely used. 5 A modification of the phase refinement scheme, called MVFC (minimum variance Fourier coefficients) has been proposed by ~ ~ ~ u s c The h . [ expression ~~] minimized is again (8.42), but the sine and cosine of the phase are considered as variables. The values of the trigonometric functions estimated in the refinement are used directly for the electron density calculation, without the need to postulate a probability distribution for the phase error.
1
549
550
1
Giuseppe Zanotti
Whatever refinement scheme is selected, different procedures can be followed: refining only centric reflections is quite safe, if reflections with restricted phase represent a good portion of the total. The number of variables is also important in this respect: in general, three positional parameters, the occupancy, and an isotropic temperature factor are varied for every atom, but since the last two parameters are highly correlated, they must be refined separately. If general reflections are used, in order to avoid bias it is advisable to refine the parameters of one derivative omitting it from the phase calculation, that is refine one derivative and calculate the phases with all the others.[361This can obviously be done if several different derivatives are available. One of the difficulties in heavyatom refinement is the check of the correctness of the parameters used: this is particularly true at the beginning of the refinement, where it is sometimes difficult even to decide if the solution found is correct or not. Many quantities can be used to monitor the progress of refinement: none of them taken alone gives an absolute indication, but together they can be considered a reliable check. Different kinds of R factors have been defined:
The Cullis R factor, Rc (8.442, is calculated only for centric reflections. A value between 0.40 and 0.60 is generally considered reasonable, the only drawback being the low number of reflections used in the calculation. For general reflections, the Kraut R factor (8.45) is used instead. Since its numerator is the quantity being minimized in phase refinement, RK can be considered a good parameter to monitor the course of refinement. Unfortunately, a high degree of substitution of the derivative implies a statistically large RK, and a very low substitution a small one, so the Kraut R factor cannot be considered an indication of the correctness of the variables being refined. i An idea of the relative importance of a single derivative in the phase calculation is given by the R(modulus), defined by (8.46), which is the lack of closure divided by the modulus of the heavyatom structure factor. If its value is greater than one, the circles of Fig. 8.8 will never intersect and (8.18) will not have any solution at all. R(modulus), if calculated in shells of resolution, gives an index of the utility of that derivative at different resolutions. Often the reciprocal of R(modulus), which is called the phasing power, is quoted. Its value must be bigger than one. The last important quantity used in refinement is the figure of merit, defined in (8.38). The figure of merit gives a direct estimate of the errors in
t In the first refinement scheme, R, can also be used: R,,, = C (IF,, F,(,,,,,I)/C F, the disadvantage of it being that it is possible to obtain a completely ranging from 0.40 to 0.60. incorrect structure with a value of R,,,
Protein crystallography
1
551
phases, but it is strongly dependent on the value of the total error E : an overestimate of E will give an overoptimistic figure of merit.
Picking up minor heavyatom sites: the differenceFourier synthesis When the positions of heavyatoms have been identified and some refinement has been carried out, the next step is to check the correctness of the heavy atoms identified and the localization of other minor sites that may be present. This can be accomplished in principle by using differenceFourier techniques (see p. 366): the map that better represents the differences between observed and calculated positions of heavy atoms should be that with coefficient^:[^']
dF= F ~ ( o b s )  FH(calc).
(8.47)
Since FH(obs) is not directly measurable, (8.47) can be approximated only if anomalous differences are available. Often a map with coefficients: AF = m(FpH Fp) exp (iq,)
(8.48)
is calculated. Unfortunately, FpHFp does not correspond to FH, and moreover qp is not the phase of FH.Furthermore, since Fourier maps are strongly dominated by phases, a differenceFourier map calculated with coefficients (8.48) will tend to reproduce the peaks of the heavy atoms used in calculating the phases. A differenceFourier map of a derivative calculated with phases obtained from that derivative is normally useless, and the technique of crossdifference Fourier, that is the Fourier difference of a derivative calculated using phases for the protein obtained from all the others, is highly recommended. Unfortunately this is not always possible, since it requires at least three different derivatives. A synthesis, proven useful in picking up minor sites, is the derivative differencemap, calculated using coefficients:
dF = rn(F~~(obs)  F~H(calc))exp ( i ~ P ~ ( ~ ~ l ~ ) ) . (8.49) If the position of all the major heavy atom peaks has been determined correctly, coefficients (8.49) allow the localization of lowoccupancy sites. Figure 8.13 shows the coefficients used in (8.48) and (8.49) compared with the 'true' ones.[381
A third approach to the solution of the phase ambiguity: realspace filtering We have already seen in Chapter 4 that the positivity of the electron density can be used to obtain phase information. The same principle may be used to improve electron density maps of protein^.[^^^^] This method is called realspace filtering and can produce correct phases when good SIR data are available. Phase information can be extracted by an electron density map by a simple backFourier transform: if a suitable modification has been introduced in the map, the phases obtained by the backtransformation will be more correct than those used in calculating the
I
Real axis
Fig. 8.13. Argand diagram of the quantities used in a Fourierdifference calculation. AFis the magnitude of the coefficient used instead of F, if coefficients (8.48) are used. GFis used i n the  Fp synthesis. (Adapted from Fp Henderson and offa an.'^'')
,
,,,
552
1
Giuseppe Zanotti
map and so the new phases can be used to modify the original ones. The procedure described here, suggested by ~ a n g , [is~based ] on the same basic principle. We have seen on p. 543 that an electron density map calculated using SIR phases will contain the correct density of the molecule, covered by an enormous amount of noise. Information about the correct phases can be obtained via the following automated procedure. 1. After calculating an electron density SIR (or single anomalous scattering, SAS) map, errors are removed in direct space by evaluating for every point an average value p, from the formula: where S is a constant estimated from previously solved protein structures. 2. The value of p, estimated from (8.50) is added to any point in the map. Any negative density remaining is considered an error and set to zero. The density in solvent region is substituted with the value p, (p,,,,).
+
3. Structure factors are calculated by Fourier inversion. Now new phases are available, and they can be combined with the old ones, using one of the well known phase combination procedures.[19~20] 4. Combined phases will produce new maps, that will undergo the procedure again, until convergence is reached. An important feature of the Wang procedure is that an automatic method has been devised to decide what is solvent and what is protein, based on the practical assumption that solvent regions, like protein regions, are contiguous to some extent. The value of electron density at point j is substituted by a new value which depends from the points surrounding it, within a sphere of radius R,? according to the criteria:
where
w i= 1  rijlR
if pi > 0 and R > rij
(8.52)
Since the resulting map has large homogeneous connected regions, the molecular boundary can be revealed by a threshold density level appropriately selected. Realspace filtering methods can also be used to extend the resolution of the electron density map.
Rotation and translation functions and the molecular replacement method Sometimes it may happen that we know the threedimensional structure of a molecule and we are interested in solving the same structure in a different
t The optimum value of radius R depends mainly on the resolution: a value between 8 and 10 8, is often used to average a 3 8, resolution isomorphous replacement map.
Protein crystallography
1
553
Fig. 8.14. A simplified twodimensional illustration of (8.53).In (a) and (b)the same
\ \
\.'
(c)
space group. At other times we have reasons to believe that the conformation of a protein is quite similar to that of another that has been previously solved, which is often the case for the same protein from different species. In all the cases mentioned above, six variables, three rotational and three translational, will approximately describe the transformation from one set of coordinates to the other. In fact, if we call X the set of vectorst representing the atoms of the original molecule and X' the transformed ones, the transformation is simply described by: where [C] is a matrix that rotates the coordinates X into the new orientation and t is a translation vector. Equation (8.53) is illustrated for a twodimensional situation in Fig. 8.14, where a 'molecule' formed by three point atoms can be superimposed to an identical molecule in a different orientation by the translation of a vector t, after the rotation of an angle cu. As mentioned in Appendix 5.B (p. 383), the technique of positioning a molecule or a fragment of known structure in a crystal cell is called molecular replacement. In principle it is possible to simultaneously search for the six variables which minimize the difference between Fobs and F,,,,, but in practice this is a very hard task, even for the fastest computer.$ The solution of the problem was pioneered by Rossmann and v low,[^^] who explored the possibility of finding the orientation of similar subunits in a crystal cell without any knowledge about the translation t, making use of the Patterson function. After the correct orientation has been found, a search for the translation vector can be carried out (a collection of papers on molecular replacement is found in the book by ~ o s s m a n n ) . [ Let ~ I us first describe the methodology and the problems connected with the rotation function.
The first step in molecular replacement: the rotation function The idea of the rotation function can be easily understood by a simple twodimensional example. In Fig. 8.15(a) a 'molecule' of three idealized
t In the following discussion all the rotations will be performed in a Cartesian reference system. It is assumed that, if required, an appropriate orthogonalization is applied before a rotation is performed. $This statement is becoming untrue, due to growing availability of computing power. Subbiah and ~ a r r i s o n have [ ~ ~ shown, ~ in the test case of the human histocompatibility antigen, that an exhaustive threedimensional search at low resolution can be performed. The correct solution can also be obtained, starting from a random position, using the simulated annealing approach (see p. 569).
'molecule' is represented in different positions with res~ectto the same reference svstem. Bv a rotation'of an angle @anda translation of t, the object in (a) can be superimposed to that in (b).
554
1
Giuseppe Zanotti
Fig. 8.15. An isolated, simplified 'molecule' of three atoms. Its selfconvolution is shown in (b): since atoms are considered as points, i t is everywhere 0,except when t w o points superimpose exactly.
point atoms is represented isolated, in a orthogonal reference system. Let us imagine a twodimensional lattice of similar 'molecules' in a different orientation. In the lattice of Fig. 8.16(a) the unit cell is made by two oLsuch molecules, related by a twofold axis, denoted by 1 and 2. Maxima of its idealized Patterson function, shown in Fig. 8.16(b), can be divided in two categories: those arising from intramolecular vectors, or selfvectors, and those from intermolecular or crossvectors. Maxima belonging to the first class are indicated in the figure by circled points and are confined to a short distance from the origin. It is easy to see that by a simple rotation of 112" anticlockwise the isolated molecule can be superimposed to molecule 1 of Fig. 8.16(a), after an appropriate translation, or, by a rotation of 292", to molecule 2. The selfconvolution function of the isolated molecule (Fig. 8.15(b)) can also be superimposed to the Patterson of the crystal if we perform the same rotation. Let us define a function R(C):
where C is a matrix that rotates the coordinates of the model molecule with respect to the reference system of the crystal, P,,,,,(u) is the Patterson
Fig. 8.16. (a) A portion of a twodimensional lattice of a molecule identical t o that of Fig. 8.15 (the unit cell is dashed). (b) Its corresponding Patterson map. Circled points indicate selfvectors. Squared points are crossvectors close to the origin: some of the points of Fig. 8.15(b) accidentally superimpose t o them during rotation, giving rise t o false maxima in the rotation function.
w
l
.IIIIJ (4
Protein crystallography
function of the crystal and Pmol(Cu)is the selfconvolution function of the isolated molecule, rotated by C. The function R(C) will have a maximum when the peaks of the two functions superimpose, at least partially. The calculation of function R(C) for all the possible values of the rotational variables will allow us to determine the orientation of the known molecule in the reference system of our crystal. The righthand side of (8.54) can be Fourier t r a n ~ f o r m e d [ ~and ~'~~] reduced, neglecting a constant, to:
F(h) are the Fourier coefficients of the crystal and Fmol(p)the coefficients of the Fourier transform of the isolated molecule, rotated by C (h, h' are used here to indicate different terms of (hkl) values, p represents a point in reciprocal space of a continuous transform). Gh,h,is an interference function whose magnitude depends on h, h', and the volume used in the integration of (8.54). The function R(C) can be evaluated in real space using (8.54) or in reciprocal space, using (8.55). In both cases the computing time is strongly dependent on the sampling chosen, which in turn is related to resolution. In real space PC,,,, and Pmo,must be sampled finely enough for the resolution selected (generally this means a value around 112 or 113 the d spacing). The volume of integration is a sphere whose radius depends on the size of the isolated molecule, and this value determines the steps of the angular variables used in evaluating R(C). In reciprocal space problems are quite similar, since Fmol(p) is a continuous function, defined over all the reciprocal space. The isolated molecule can be put in an artificial cell, generally a cube whose edges can be about two to thiee times the size of the molecule, and the continuous function evaluated with a sampling appropriate to the resolution used. In practice, since (8.55) is dominated by large Fourier coefficients, it is possible to limit the numbers of F ( p ) used. A faster but more complex approach in evaluating the rotation function, the socalled fastrotation function, has been devised by ~ r o w t h e r . If~ ~we~ ] express the Patterson function in terms of spherical polar coordinates, (r, 0, q ) , for a rotation C, corresponding to the three angles cq,a 2 , ag, the rotation function can be written:
1
R(C) = PwSt(r,8, q)RPmol(r,8, q ) r 2sin 0 dr d o d q
(8.56)
where RPmolis Pmolafter a rotation C. Equation (8.56) can be expanded using Bessel functions, more appropriate to a rotation group than a Fourier series, well suited for translation operations. The use of Bessel functions requires a lot of difficult mathematics, outside the scope of this book, but the final result is that R(C) can be evaluated as a summation of two terms, one of them independent of the rotation itself. The computation time is consequently greatly reduced with respect to the use of (8.54) or (8.55).
The rotation matrix C and the choice of variables Rotation is usually performed with respect to an orthogonal system, making use of different rotational variables. Quite common are the Eulerian
1
555
556
1
Giuseppe Zanotti
rotation angles el, 02, and 83, illustrated in Fig. 2.3(a): O 1 is the rotation angle about the z axis and is positive when the rotation is clockwise looking from the origin; O2 is a rotation about the new x axis and 83 a rotation about the new z axis. The matrix C describing such a rotation is given in (2.32b).t An appropriate rotation for the three angles will cover all the space (see p. 72), but if the Patterson map presents some rotational symmetry, the rotation function will also have symmetry and a partial rotation will be sufficient. The symmetry of the rotation function is a combination of the symmetries of the two Patterson functions, PC,,,,and P,,,.[~~] The Eulerian angles make easy to describe the symmetry of the rotation function.[491Any triplets of angles 0 , ) 82, and 8, can be considered as a point of a threedimensional system, whose unit cell has dimensions 2n in all directions: a rotation a is in fact equivalent to a 2n. The resulting rotation space groups are some of those described in the International tables for xray crystallography. $ A disadvantage in using 8 angles is that when O2 is small, 8, and O3 represent a rotation about nearly the same axis, and maxima will resemble strips rather than maxima. The distortion effect can be avoided if a combination of Eulerian angles is used instead:['']
+
x
A different possibility is the use of spherical polar angles, (p, I/J, and (Fig. 2.3(b)). Angles (p and I/J define a spin axis, and a rotation of around this axis is performed. Polar angles are very useful when a particular direction has to be exploited or when a defined rotation has to take place, as is sometimes the case for selfrotation (see p. 558).
x
Translation functions Once the orientation of a known molecule in an unknown cell has been found, the next step is the determination of its absolute position. Only when one molecule is present in space group PI is this problem nonexistent, since in this case the origin of the crystal cell can be chosen arbitrarily with respect to all three axes. In all the other cases, when the reference molecule, exactly oriented, is translated in the unknown cell, symmetryrelated molecules move accordingly and all the intermolecular vectors change: only when all the molecules in the crystal cell are in the correct position, the calculated Patterson crossvectors superimpose to those of the observed Patterson (intramolecular vectors are insensitive to translation). Figure 8.17 illustrates the method. Molecule 1 is positioned in the crystal cell of the unknown structure in the correct orientation: s1 is the vector defining its position with respect to the origin. Since we do not know yet the correct position of the molecule in the cell, s1 is arbitrarily chosen. Molecule 2 is generated by the twofold axis, and its position is defined by vector s2. The correct solution is shown in Fig. 8.17(a), where the correct origin of molecule 1 is indicated by sy. As vector sl varies, all the intermolecular vectors among symmetryrelated atoms will change: they will coincide with
t In Chapter 2 the rotation matrix C is called RE, for Eulerian angles and R,, for spherical polar angles. $The reader must be warned that the Eulerian rotation matrix is not Hermitian, that is reversing the order of the Patterson functions does not produce the same rotationequivalent positions.
Protein crystallography
1
557
Fig. 8.17. (a) 'Molecules' 1 and 2 correctly oriented and positioned with respect t o a : is the vector from the symmetry element. s origin to an arbitrary point of molecule 1, and sz the corresponding one for molecule 2, which is generated from 1 by twofold rotation, to = sz sy is the translation vector from molecule 1 t o 2. (b) Molecule 1 has been translated (but not rotated, so that orientation is unchanged). Molecule 2 has moved accordingly, and now all vectors defining the molecular positions in the cell are changed. Only when t = to the t w o models, and consequently crossvectors of Patterson maps, superimpose. Determination of sy from to is straightforward.
those of Fig. 8.17(a) only when s, = s:, that is when the local origin is correctly defined with respect to the symmetry element. The determination of the translation vector is performed by comparing two Patterson maps, just as before in the rotation case, except that now we are interested in maximizing the superposition of a different class of peaks. The problem described above is in practice quite difficult, since the function representing the superposition is generally very noisy and with many small maxima. Several translation functions have been proposed, and some of them are briefly summarized in Appendix 8.B. To illustrate the principles of translational search, only the T function of Crowther and low['^] will be described here, following the treatment of atm man.['^] In the case illustrated in Fig. 8.17, the set of crossvectors of the calculated Patterson from molecule 1 to molecule 2 can be written as:
where p , and p, represent the electron density of the two molecules. If molecule 1 is now translated, a new vector s, will define its origin. At the same time molecule 2 will move into the cell, and a new function P12 can be calculated for every value of s,. Since we are looking at intermolecular vectors, it is more useful to define the translation as a function of vector t = s2  s l , which defines a local origin with respect to a symmetry element. If Pohs(u)is the value of the observed Patterson at point u, the T translation function is defined as:
Function Twill have a maximum when the two Pattersons superimpose. In reciprocal space, (8.59) can be written:[511 lohs(h)Fl(h)F~(hA) exp (2niht)
T(t) =
(8.60)
h
where F,(h) .\ is the Fourier transform of the model molecule 1 and Fl(hA) the calculated structure factor of molecule 1 after application of symmetry /
558
1
Giuseppe Zanotti
operation A. Looking at Fig. 8.17, since t = s,  s,: I,,,(h)F,(h)FT(hA) exp [2nih(s2  sl)].
T(t) =
(8.61)
h 0 The T function will have a peak at position s2 s1 = t o e s02 s1 (or s l  s2= to). The determination of sy from function T is equivalent to solving a Patterson map with only two atoms in the crystal cell. In general the T function does not need to be evaluated for the entire cell: if for example two molecules are related by a screw axis along 2, the maximum to will have coordinates (2x, 2y, 1/2), that is it will be confined only to section 2 = 112. Other types of translation functions have been developed, and some of the more commonly used in protein crystallography are summarized in Appendix 8.B. A general review on translation functions is reported by Beurskens et al. [531
Selfrotation and selftranslation functions: improving the electron density maps Sometimes more than one molecule is present in the crystallographic asymmetric unit. If we assume that they are identical, or at least very similar, we can take advantage of the independent information present in the structure factors. In fact, if we are able to identify the noncrystallographic symmetry elements relating the independent molecules, the electron density map can be averaged and substantially improved. The presence of three molecules in the asymmetric unit has allowed the solution of the structure of the haemaglutinin of the influenza virus using only SIR phases The selfrotation function is very similar to the general rotation function defined in (8.54):
where P,(Cu) is the Pl(u) Patterson function rotated by matrix C, and U(u) is a function which is 1 inside a sphere and 0 elsewhere. The function U is necessary since both Patterson maps extend to all space, but we are interested only in the superposition of selfvectors, confined to a region around the origin of the cell. The sphere defined by U generally has a diameter slightly larger than the maximum supposed molecular dimension. The choice of polar rotation angles is quite common for selfrotation and deserves a brief comment. Quite often the noncrystallographic symmetry is represented by a rotation axis, in a direction different from the crystallographic ones. In that event, the use of polar angles reduces the search for the position of the axis from a threedimensional problem to a twodimensional one: a twofold axis, for example, will correspond to a rotation of 180" around the polar axis X, and a twodimensional map (calculated for q from 0" to 360°, Il,from 0" to 360", and x = 180") will show the presence of the axis. A clear example of that is presented by Evans et a1.[551 The definition of the translational component of the noncrystallographic symmetry represents the last and possibly the more difficult step. Let us for example assume that the direction of a twofold noncrystallographic axis is
Protein crystallography
1
559
known. It has been shown[561that only the component of the translation vector t in the direction of the axis can be determined precisely. The other component of vector t, that is that perpendicular to the axis, is intrinsically an imprecise parameter, unless the molecular structure is perfectly known, which is not the case. In general, the selftranslation function (analogous to the T function previously described) is used to detect the existence of a translational component of a rotational symmetry. The steps and the possible different pathways described in the previous paragraphs for the solution of a crystal structure of a macromolecule are summarized in the scheme reported in Fig. 8.18.
I I
Crystallization
I
Space group determination
Isomorpous derivative preparation and data collection
DifferencePatterson map
1 1
Phase refinement
I
replacement
*
1  1
DifferenceFourier maps
Yd, srdetc.
derivative
measurements
Real space
I
Electron density map calculation and model building
I
Fig. 8.18. Simplified scheme summarizing some of the possible steps in the determination of the structure of a macromolecule. Some of them can be used alternatively or combined, : depending on the specific problem, that is size Refinement of the protein, previous knowledge of the structure, number of molecules in the (see Fig. 8.23) asymmetric unit, and so on.
560 ( Giuseppe Zanotti
Direct methods and the maximumentropy principle in macromolecular crystallography Direct methods, extensively described in Chapter 5 , are not yet applicable in the present form to the ab initio structural determination of a macromolecule. The main reason for that resides in the very large number of atoms to locate: additional information is needed in order to increase the reliability of the phase indication. Isomorphous replacement and anomalousdispersion data can be classified in this category, and indeed they have been often used to locate the positions of heavy atoms. For example coefficients (8.8) can be used with conventional direct methods programs and they can be very helpful in the case of a very large number of sites.LS7] Furthermore, classical direct methods have allowed, using coefficients ( F L  F,), the localization of the positions of anomalous scatterers in m e t a l l ~ ~ r o t e i n s . [ ~ ~ ~ Quite promising, but not yet fully exploited, is the use of direct methods for the determination of the phase of the protein structure factor taking advantage of isomorphous replacement and anomalousdispersion data (for a review see ~ i a c o v a z z o ) [ ~Let ~ ] . us call @,(h) and @,(k) the phases of reflections h and k, respectively, for the native data set. @pH(h)and @pH(k) are the phases of the corresponding reflections of the derivative. In addition to the classical triplet invariants introduced on p. 338:
we can make use of triplets containing mixed terms, that is relationships between phases of the two crystals:
The eight different combinations of the six phases give rise to eight conditional probability distribution for Qj, whose formulation is not discussed here. An important point, however, must be stressed: the probability distributions do not depend only on the total number of atoms present in the crystal cell (see Appendix 5.C), but also on the difference between native and derivative data. The reliability factor for a triplet phase, G, defined in (5.37) and (5.C.16), in the presence of isomorphous data must be rewritten:[60] where Np and NH are the number of protein atoms and heavy atoms in the unit cell, respectively, and Ah represents the normalized difference for
Protein crystallography
reflection h. The second term of (8.63) may substantially increase the value of the reliability factor G. A relevant application of (8.62) is that one single derivative allows in principle the determination of the phase of the protein structure factor. A similar approach can also be used in presence of anomalous dispersion data, where in addition to the classical triplet invariants:
six other equations containing mixed terms, analogous to (8.62b), can be introduced. The only limitation in the previous treatment is represented by the very high degree of accuracy necessary in the measurement of the intensities, particularly in the case of anomalous scattering data. Nevertheless, anomalous dispersion techniques are becoming more relevant, due to the possibility of performing multiwavelength experiments with synchrotron radiation. An apparently different approach to the solution of the phase problem is based on the maximumentropy principle, the application of which to crystallography was proposed by Collins[61]and that has been shown to be virtually equivalent to direct methods by ~ r i c o ~ n e .If' ~p(r) ~ ] is a density distribution, its entropy is defined as:
H
=
\ p (r) ln p (r) dr.
J
(8.65)
V
The concept of entropy is borrowed from information theory, where H measures the expected value of the total information. The 'better' distribution is that which maximizes H and which is at the same time consistent with other observations: in our case, obvious conditions are that the electron density over the entire cell is equal to F(000) and the Fourier transform of p(r) is in agreement with the diffraction data. Equation (8.65) can consequently be modified to include constraints. If some sort of previous density distribution is available, the relative entropy can be defined:[631
where q(r) is a distribution inferred by a priori information: in the absence of other information, that is if q is constant, (8.66) reduces to (8.65). The maximumentropy method has been used to expand a set of initial phases, in conjunction with other t e ~ h n i ~ u e s . Besides, [ ~ ~ , ~ ~the I structure of 15 base pair of DNA (a structure of about 600 atoms) has been recently solved ab initi0:[~~1 starting phases were determined by conventional direct methods and expanded using the maximumentropy algorithm. Although this approach has been demonstrated to fail in other simpler test cases, promising applications of direct methods to macromolecular crystallography are expected in the near future.
1
561
562
1
Giuseppe Zanotti
The interpretation of electron density maps and the refinement of the model The interpretation of electron density maps Once a phase angle estimate for the protein structure factors is available, the calculation of an electron density map is straightforward, using (see p. 170):
Fp(h)exp (iq,)
p(r) =
exp [2ni(h
r)]
(8.67)
h
where the Fourier coefficients are usually weighted by their figure of merit. The initial interpretation of the map is in general not easy, unless very good phases at high resolution are available, which is seldom the case. Therefore, the strategy generally adopted is to calculate first an electron density map at low resolution, say 56 A: these maps allow us to identify the contours of the molecules in the crystal cell, and to distinguish between solvent regions and protein. Eventually, some elements of secondary structure can be identified: ahelices will appear as cylindrical rods of diameter of about 46A. 0sheets are more difficult to distinguish, and in any case single 0strands are not visible. When the position of the molecule has been located in the unit cell, a map at medium resolution, say 3.52.5 A resolution, is calculated and an attempt to trace the polypeptide chain is made. Chain trace at this resolution is made easier, and sometimes possible, if the amino acid sequence is known. Mistakes are quite common in the interpretation at medium resolution: the connections among secondary structure elements are often difficult to recognize and amino acids can be positioned along the chain shifted from their correct position by one or more residues. Higherresolution phases, say 2 A or more, allow us to correct for this kind of mistake and to locate more accurately the amino acid side chains. Unfortunately, MIR phases very seldom extend to that resolution, and highresolution maps can be obtained using calculated or combined phases, as will be discussed later.
Interactive computer graphics and model building Lowresolution maps are traditionally drawn on a small scale on transparent sheets and are known among protein crystallographers as 'minimaps': they are very useful in giving a global view of the electron density of the unit cell. Such maps can also be used at medium resolution, since they allow a preliminary, approximate tracing of the polypeptide chain. The complete building of the molecular model in the old days was performed using an apparatus, generally homemade, called an optical comparator or 'Richard's box', from the name of its inventor.[661Nowadays, the interpretation of the electron density can be entirely performed on a graphic display: the map is shown on a video and the operator is allowed to fit a piece of chain into the density. For this purpose, the modelling software most popular among protein crystallographers is FRO DO.[^^,^^] The principle of the program is that objects displayed on the screen are divided in
Protein crystallography
1
563
Fig. 8.19. 'Chicken wire' representation of the electron density of a side chain of a histidine residue. Maps are calculated at a resolution of 2.5 A, with coefficients 2F0,,  F,,,, and calculated phases. Drawing produced by an Evans and Sutherland PS330 graphic station, using program FRO DO.'^"
two categories: those that can be manipulated, called 'foreground objects', and those that cannot be modified interactively, defined 'background objects'. Background and foreground models can be seen superimposed on each other. Program FRODO contains a dictionary of stereochemical information on natural amino acids and groups often occurring in protein molecules or nucleic acids. From this dictionary, building of a part of a polypeptide chain or a portion of a macromolecule in the preferred conformation is straightforward. The electron density, which does not need to be modified, is displayed as a background in a 'chicken wire' representation or similar, and the atomic model, or a part of it, as a foreground object. Figure 8.19 illustrates a simple model as it appears on a calligraphic screen. Atoms can be easily manipulated, by a simple rotation of a dial or movement of a light pen: they can be moved, alone or in groups, rotation around dihedral angles performed, or bonds stretched. The fitting of the built model into the electron density can be fast, if the starting phases are good enough; otherwise, a lot of time can be spent in trials. A convenient method to build the initial model of a protein has been devised by Jones and ~ h i r u ~ based , [ ~ ~on ] the idea that short elements of secondary structure can be taken from a data base consisting of coordinates of a restricted set of well refined protein structures: once some acarbons (say 1015) are roughly positioned into the density, the piece of model from the data base that better fits these atoms is searched for and used. The only disadvantage in the use of a graphic system during electron density map interpretation is that a global view of the molecular model is practically impossible, since a drawing of all the atoms of a protein gives results which are quite confusing. Nevertheless, people who built protpjy models using a 'Richard's box' are strongly in favour of interactive graphic systems.
The refinement of the structure The refinement of protein structures, with very few exceptions,[701cannot be carried out using the classical leastsquares methods. This is not due to the size of the problem, since nowadays computers are powerful enough to handle systems of equations containing thousands of variables, but to the limited number of Xray data. It has been shown in fact on p. 98 and 104 that, for an accurate definition of the parameters, the system must be largely overdetermined, that is the ratio of observations to variables (atomic
564
1
Giuseppe Zanotti Table 8.3. Number of theoretical independent reflections at different resolutions for a protein crystal with one molecule of 182 amino acids in the asymmetric unit. The solvent content is 40 per cent. The number of parameters is 4408 (1469 atoms times 3) if an overall B factor is considered, or 5876 if an individual isotropic B thermal parameter is assigned to each atom Resolution range (A)
Independent reflections
Ratio obs./var. (x, y, z )
Ratio obs./var. (x, Y, 2, 6)
coordinates, thermal factors, and sometimes occupancy) must be of the order of 10 or so, and this is indeed the case for small molecules, where diffraction data can be collected to a spacing of 0.7 8, or even more. Protein crystals are intrinsically less ordered: diffraction data are often measured to a resolution of 3.02.5 8,, sometimes 2.0 8,. A resolution of 1.5 8, can be considered quite good, and only in exceptional cases have 1.0 A data been collected.[231A typical situation is illustrated in Table 8.3, where the number of independent reflections for a mediumsize protein (182 amino acids) with a solvent content of 40 per cent are calculated at different ranges of resolution. For a ratio of observations to parameters of 10 it would be necessary to collect all possible diffraction data to a spacing of 1.28,, a resolution never attainable for such a type of crystal. For the abovementioned reasons, the first attempts to refine a protein structure were performed in real space.[711The method seeks to minimize the difference between the observed electron density, p,,,, computed by (8.67), and a calculated model density, peal,, obtained by assuming a Gaussian distribution of the electron densities centred at the atomic positions of the current model: This technique suffers from all the drawbacks of a realspace refinement procedure, the most relevant being that if poor phases are available, p,,, will be quite incorrect and the convergence of the method very slow, or it will not converge at all. There are many reasons to favour the reciprocal space refinement methods and different solutions have been proposed to overcome the problem of the underdetermination of the system: in fact, improvement of the ratio of observations to parameters can be achieved by decreasing the number of variables or by artificially increasing the number of observations. The former is called constrained least squares and the latter restrained least squares.
Constrained versus restrained least squares Constrained or rigidbody refinement? is a wellknown and widely used technique in crystallography (see p. 105): when the geometry of a group of
t Despite the distinction between them described on p. 105, rigidbody and constrained refinement are taken as synonyms i n this chapter.
Protein crystallography
1
565
atoms is accurately known and there are reasons to believe that it will not be significantly modified by the environment, the entire group can be treated as a rigid entity. In the classical case of a phenyl ring, the eighteen positional variables can be reduced to only three translational and three rotational. Bond length and valence angles in amino acids are very well known from the structures of hundreds of small peptides. In a protein, they can be held fixed to their theoretical values and only torsion angles around single bonds allowed to vary. This approach was used by ~ i a m o n d [ ~in ' ] realspace refinement, but it can be used in reciprocal space as well. Taking into account the fact that the peptide bond can be considered planar, only two torsion angles, called g, and I) (see Appendix 8.D), need to be varied for the backbone chain of every amino acid: for a protein of n residues, the parameters are reduced to about 2n for backbone plus the torsion angles of side chains. An illustration of a possible choice of constrained parameters is reported in Fig. 8.20 for a simple dipeptide. This solves the problem of underdetermination, but the model becomes in some way too rigid and the radius of convergence, that is the maximum displacement allowed for an atom in a wrong position to be corrected, becomes quite small. Constrained least squares can be applied to very different extent: the definition of rigid body can be applied to only some group of atoms or to the entire molecule. If, for example, an approximate solution of the structure has been found using the molecular replacement technique, a first refinement can be performed by considering the entire protein (or a subunit) as a rigid group and the best position in the new crystal cell can be searched for using only three translational and three rotational variables. In that event, there is the supplementary advantage that, since the number of variables is very limited, only lowresolution data need to be included in refinement, greatly increasing the radius of convergence of the method. Increasing the number of observations is another possible solution of the underdetermination problem in macromolecular refinement (see p. 107). Information from other sources can, in fact, be introduced and treated in a way similar to that used for observations coming from Xray diffraction. The use of geometrical restraints has been proposed by Konnert and end ricks on,[^^'^^] following a procedure devised by ~ a s e r [ for ~ ~ small ]
Fig. 8.20. Schematic drawing of the dipeptide phenylalaninealanine, used to illustrate the constrained leastsquares technique. Arrows indicate free rotation about the bond. All the bond lengths and valence angles are held fixed, and the peptide group and the phenyl ring planar. The total number of variables amount t o eleven: three rotation and three translations (not indicated in figure) plus five internal torsion angles. (Some of the hydrogen atoms are indicated in figure only for clarity, but they are usually not taken into account i n the refinement.)
566
1
Giuseppe Zanotti
molecules. In addition to the classical quantity minimized in crystallographic least squares:
where the summation is extended to all the i reflections, other observational functions can be added. Since distances and valence angles of amino acids are well kitown and they are not expected to deviate significantly from the ideal value, instead of considering them as fixed, we can also minimize:
d,(ideal, is the ideal value for the specific distance we are considering, d,(,,,,) is that calculated from our present model and wi is usually chosen as the reciprocal of the standard deviation of the distribution expected for the distances of type j. Notice that since di(calc)is a function of the atomic coordinates, (8.70) does not increases the number of variables. The total number of equations like (8.70) is equal to the distances that are restrained: bond lengths, the distances between one atom and the nextnearestneighbour (which is equivalent to restraining valence angles), and the firsttofourth atom distances, where the dihedral angle described by the four atoms is in some way fixed (this is for example the case of the planar peptide bonds). An example of the number of distances that can be restrained for a simple dipeptide is illustrated in Fig. 8.21. Other possible restraints in the Hendrickson and Konnert formulation are:
S3 represents the sum of the deviations of the atoms i from the plane k, which is defined by its unit normal m k and by the origin to plane distance
Fig. 8.21. The same dipeptide as in Fig. 8.20 illustrates the restrained leastsquares technique. The coordinates of any atom are allowed t o vary, but the stereochemistry is preserved by applying restraints on bond distances (full lines), bond angles (broken lines), torsion angles (dotted lines), and planarity. Nonbonded contacts are not shown i n the figure. (Adapted from Sussman, ref. [3],Vol. 115, p. 274).
Protein crystallography
1
567
d k ; ri is the vector that defines a point i whose distance from plane k has to be minimized.[751S, restrains the volume of chiral atoms, defined for an acarbon by the product of the interatomic vectors of the three atoms bound to it:
Since the sign of Vc, depends upon the handedness, S4 restrains chiral centres to their correct configuration (Fig. 8.22). S, is applied to all nonbonded atoms (except those taken into account in S2) and avoids too close contacts. Other kinds of restraints can be considered, i.e. on isotropic thermal parameters, occupancy, and noncrystallographic symmetry. It may sometimes happen, particularly during the first stages of refinement, that some part of the structure is poorly determined and the model 'blows up'. In that event, a restrain on the excessive shifts can be applied:
where rk and ro are the atomic vectors of the target and the initial model respectively. Using eqns (8.70)(8.74), the number of observational functions is now greatly increased from the original number, represented by eqn (8.69). Equation (8.75) has effect only on the diagonal terms of the normal matrix. The number of restrained parameters for the example described in Table 8.3 is shown in Table 8.4. It must be remembered that in protein crystallography 'experimental' phases are very often available. They can be included in leastsquares as an additional information that imposes another '97
=
Ci wp(qi(obs)
2 Q)i(calc))
(8.76)
.
qobsis the estimate of phase angle from isomorphous and anomalous data and qolCis the phase calculated from the model. Weights for (8.76) must take into account the cyclic nature of phase angles. Phase information is also used by Lunin and ~ r z h u m t s e v . [They ~ ~ ] suggest that only differences among crystallographic quantities be minimized, that is structure factor amplitudes and phases. Since phase probability distribution may be represented by (8.34), they assume an analogous probabilistic distribution for the module of the structure factor F for reflection i of the form: P(F;) = exp [  ( F :
F ~ ( , , , , ) ~ / ~ u ~ ] ,
(8.77)
and if structure factors moduli and phases are assumed to be mutually independent, the joint probability distribution will be given by the product of (8.34) and (8.77). The most probable model will consequently be that which minimizes:
S=
+
{ ( 1 / 2 a 2 ) [~ F:(ob,,]2 f  [ A cos qi B sin q i i
+ C cos 2 q i + D sin 2 q i ] ) .
(8.78)
Using (8.78) the multimodality of the phase distribution is taken into account.
Fig. 8.22. The chiral volume for an cucarbon atom. The central atom is chosen as the origin of the coordinate system, and vectors (r,  ,),r (rc8  ),r and (r, ),,r (8.74) are denoted s, sc8, and s, respectively. The cross product s, X sC8 is a vector perpendicular to the plane CC,C8. If it is on the same side of vectors,, as in the figure, that is if angle 0 is less than 90". the dot product between the t w o vectors is positive. If s, and sq are reversed, that is if the wrong configuration IS chosen for the cucarbon, the vectors, x sc8 points i n the opposite direction and the value of V, becomes negative.
Table 8.4. Number of restraints, following Hendrickson and ~ o n n e r t , ~ ' for ~ ' a protein molecule of 1469 atoms (excludina H) in the asymmetric unit. The example is Ye~ativeto the case of Table 8.3 Number of distances: bond distances angle distances planar 14 distances Planes Chiral centres Torsion angles Possible contacts: contacts due t o single torsion contacts due to multiple torsion possible Hbonds
568
1
Giuseppe Zanotti
A different approach to using restraints has been proposed by Jack and ~ e v i t t : ' instead ~ ~ ] of restraining stereochemistry, they minimize: where D represents the difference among observed and calculated structure factor amplitudes given by (8.69) and E is a potentialenergy function:[801
+ C k,{l + cos (me, + 6)) + C (Ar'' + BrP6).
(8.80)
The four terms on the righthand side describe bond, valence angle, dihedral torsion angle, and nonbonded interactions, respectively. Kb is the bond stretching constant and K, the bond angle bending force constant; k, is the torsional barrier and m and 6 the periodicity and the phase of the barrier. A and B the repulsive and the longrange nonbonded parameters. The summation extends to the j bonds, the I valence angles, the 8 torsion angles, and the n nonbonded interactions between all pairs of atoms separated by at least three bonds. Despite the apparently very different approach, the energy minimization and the geometrically restrained leastsquares are not too different in practice, since the final effect of (8.80) is to impose restraints on the model. Whatever method is used, special care is needed about the weights applied to the different functions. We are in fact dealing with non, homogeneous quantities, like structure factor amplitudes and interatomic distances, so the weights of the relative observational functions must be chosen in such a way that everything is put on the same scale: an overestimate of geometric restraints will in fact produce a stereochemically perfect model associated with a very high crystallographic R factor; on the contrary, an underestimate of the same weight will result in a good R factor with unreasonable bond lengths and angles.
Restrained and constrained least squares The two methods described above, restrained and constrained least squares, can be combined:[s11the molecule(s) is(are) considered as made up of rigid groups, and restraints are applied to distances among such groups. The quantity minimized, S, is the sum of three terms: where DF is (8.69), DD restrains the stereochemistry, analogously to eqns (8.70)(8.73), and DT restrains the structure from moving away from the starting set of coordinates, (8.75). All of the terms of (8.81) are functions of the atomic coordinates, generally referred to an orthogonal reference system. If a subset of these atoms is considered as a rigid group, S can be expressed, for that particular group of atoms, as a function of six rigidbody parameters, three rotational and three translational, and an arbitrary number of torsion angles, that is: where ti and R, are the translation vector and the rotation matrix of the
Protein crystallography
entire group i, Yi,, . . . , Vim are the m torsion angles and B,,, . . . , Bin the n temperature factors of group i. Since the definition of rigid group is left to the user, the entire molecule or a portion of it can be constrained, or eventually some subunits. The restrainedconstrained approach was originally devised for nucleicacid refinement, but it has been successfully used in refinement of protein A computationally quite efficient method of combining structures too.[822831 sterical restraints and rigidbody refinement has also been recently proposed. [s41
Crystallographic refinement by molecular dynamics The development of vectorial and parallel computers offers nowadays the possibility of performing molecular dynamics calculations on complex systems, including proteins in the crystal state. The application of molecular dynamics calculations to macromolecules is a quite widespread technique (for a review, see Karplus and ~ c ~ a r n m o n [ ~ but ~ ]its ) , introduction in the crystallographic refinement of protein structures had been proposed only re~ently.[~~,~~] Molecular dynamics of free atoms consists in solving the classical Newton equation of motion: To take into account the effect of the medium and the approximations used to calculate the total energy, dynamical effects can be better represented by a set of Langevin equations: where bi is a frictional coefficient, used to prevent atoms from moving away too much from their original positions, kB is Boltzmann's constant, To the temperature, and i ( t ) a random force with Gaussian distribution and properties:
The simulation starts from an initial set of coordinates. To each atom is assigned a velocity, usually at random from a Maxwellian distribution corresponding to the temperature selected, and eqn (8.83) or (8.84) is integrated at a given temperature for a given time.? New velocities are then assigned, eventually at a new temperature, and the calculation continued. The simulation is normally performed for a short period of time, usually of the order of few picoseconds. In the crystallographic refinement of macromolecules by molecular dynamics, the Xray information is used to restrain the energy of the system. The total potential energy is, in fact, considered as the sum of two
E,,, represents an empirical potential energy, analogous to that defined by (8.80), E,, is a sort of 'experimental' potential energy, and is considered as
t Numerical integration
can be performed using for example the Verlet algorithm.
1
569
570
1
Giuseppe Zanotti the sum of three terms:
Exrayin (8.87) describes the difference between observed and calculated structure factor amplitudes:
w, is a factor which puts Exrayon the same scale as the empirical potential energy term and NA is given by C w,(F,,,)~, to ensure that wA is independent of the resolution range used. The terms E p and ENBcan be included to take into account experimental information about MIR phases and crystal packing respectively. Molecular dynamics simulations can be performed at ambient temperature,[871or at higher temperature, as in the version called simulated annealing.[s69881 The latter consists in starting the simulation at room temperature, say 300 K, and heating up the system (for example at 20004000 K) and subsequently cooling down at the initial value. The advantage of going to high temperatures, unreasonable from the biological point of view, is that model can come out of local minima, and the ratio of convergence of the method is increased with respect to classical least squares. t The result of molecular dynamics calculations is a family of conformations, but the constraints imposed by Xray data restrict these conformations to all those with the lower crystallographic R factor.
The strategy of the refinement of protein structures The initial model of a protein structure is, very often, not good enough to allow for a fully automated refinement. Indeed, if some serious errors are present in the model, for example the polypeptide chain is positioned more or less correctly but the amino acids are shifted one residue or more along the chain, an automatic procedure will hardly recover from that error. Besides, the radius of convergence of constrained or restrained leastsquares methods can be evaluated to be around a half the resolution of the data used, that is not more than 11.5 A. At the beginning of the refinement, to speed up convergence, mediumresolution data (3.02.5A) can be employed. Since the number of observations at that resolution is quite low, an overall temperature factor for all the atoms is used. Afterwards, the resolution is gradually extended, solvent molecules included, and isotropic individual B factors applied. The same seems not to be true using the simulated annealing technique, which allows a more rapid and automatic convergence: the heating makes it easier to get out of the false minima without manual intervention. Some more experience nevertheless must be accumulated. A fully automated refinement was possible in the test case of the enzyme aspartate aminotransferase, refined with data at 2.8 A resolution starting from MIR t T h e term temperature must be regarded cautiously here: it does not indicate a physical temperature, but rather a parameter controlling the refinement. The simulated annealing is in fact virtually equivalent to the Metropolis algorithm (Metropolis, N., Rosenbluth, M., Rosenbluth, A , , Teller, A. and Teller, E. (1953). Journal of Chemical Physics, 21, 108792).
Protein crystallography
coordinates.[89] A careful comparison between the model of myohaemerytrin refined, starting from the same model, in one case with several cycles of restrained leastsquares and manual rebuilding and in the other case with the 'simulated annealing' technique without manual intervention has been reported.[901The two structures compare quite well, but molecular dynamics procedure could not bring the refinement to completion in a fully automated way: manual intervention is still necessary to correct for gross errors (say more than 35 A in the main chain) and to include solvent molecules. Nevertheless, simulated annealing can save a lot of human effort, at the expense of quite a long computational time. For the above mentioned reasons, some cycles of automatic minimization are usually followed by recalculation of the electron density maps and manual adjustment or rebuilding of the model. In recalculating electron density maps, a major problem is the choice of the phases and the coefficients to be used. MIR phases suffer from all the errors described on p. 546, and the isomorphism of heavyatom derivatives does not extend generally beyond 3.A or so: highresolution electron density maps are seldom achieved with MIR phases. On the other hand, calculated phases tend to reproduce the model used in calculating them, and an electron density map obtained wih calculated phases may be strongly biased. For these reasons, phases coming from independent sources, e.g. the phases from isomorphous derivatives data and those calculated from the model, can be combined to produce an improved electron density The probability distribution of calculated phases, Pcalc(q),can be evaluated by using a procedure due to ~ i m (see [ ~Appendix ~ ~ 5.H, p. 393) and can be used, along with the 'experimental' probability Ptot(q), to obtain a combined probability distribution: Pcomb(c~> = Ptot(~)Pca~c(q).
(8.89)
The new figure of merit, mcomb,obtained by (8.38) can be used to calculate a best combined electron density map. If only calculated phases are available, the Sim formula can be used to weight the Fourier coefficients. A scheme of the possible refinement procedure is illustrated in Fig. 8.23. The coefficients and phases more commonly used for Fourier syntheses are listed below, but other combinations of them are possible: mF0bs exP ( i q ~ ~ ~ ) W
W
C
O
Fobs ~ ~
S IFobs ~
exP ( i q c ~ ~ b )
 &a~cI exp (iqca~c),
(8.90) (8.91) (8.92)
 & a d exP (i~comb), ~cornb(~~obs
(8.93)
~ ~ l r n ( ~~& o ba ds exp (i~calc).
(8.94)
Equation (8.90) gives the coefficients of a classical observed Fourier synthesis. In principle, they could be used during all the stages of the refinement, but MIR phases can be improved by phase combination. Furthermore, very often they do not extend to high resolution, and calculated phases must be used instead, when a reasonable atomic model is available. To reduce bias, a Fourier map with combined phases can be calculated. Coefficients (8.92) correspond to Fourierdifference maps with calculated phases. If they are calculated from a partial model, they are
1
571
572
1
Giuseppe Zanotti Starting model (see Fig. 8.18)
Fig. 8.23. Block diagram summarizing the phases of structural refinement. The starting model is obtained by one of the procedures schematized in Fig. 8.18. The numbers of iterating cycles necessary t o reach convergence can be quite variable, depending o n the quality of the initial model. If M.I.R. phases are not available (i.e. the structure has been solved b y molecular replacement techniques), only maps with calculated phases can be used. Some of the coefficients used in electron density map calculation are described on p. 571.
Calculation of new electron density maps with new phases
Some cycles of leastsquares refinement
.
I
Structure factor calculation
I End of refinement I known as omit maps and can be useful in positioning portions of the molecule that did not appear clearly in the M.I.R. maps. Coefficients (8.93) and (8.94) correspond to a combination of a Fourier electron density map and a differenceFourier: if Fobsand F,,,, are very similar, the magnitude of the coefficients approaches to (8.91); otherwise, terms with Fobsgreater than F,,,, will have a higher weight. The practical result is an enhancement of the regions of density where severe errors are present in the model. The weight used for map calculation can be a modification of the Sim scheme or the weight obtained by the combination procedure. It must be finally remembered that the crystallographic R factor of a refined protein structure is not comparable with that of a smallmolecule crystal. Besides, owing to the low ratio between observations and variables, the R factor alone does not represent an index of the reliability of the model: molecular stereochemistry must be correct also. For example, deviations from the ideality of bond lengths, valence angles, and restricted torsion angles of about 0.01 A, 2", and l o , respectively, are considered reasonable. The crystallographic R factor of a crystal structure refined with these restraints at 2 A resolution can be reduced to a value between 0.15 and 0.20.
Protein structure The threedimensional structure of a globular protein is the resultant of a very large number of interactions. This makes it at the same time stable and flexible: a modification in a specific site can, in fact, be assimilated by small local adjustments, without altering the overall conformation. In other cases, modifications taking place in a region of the macromolecule can be transmitted and influence the conformation in zones far apart from where the movement originated, a phenomenon called cooperative or allosteric
Protein crystallography
effect.? It must also be remembered that the medium may have a relevant influence on the conformation of the macromolecule, that in vivo operates in a nonhomogeneous environment, like for example the cell cytoplasm or the cellular membrane. Flexibility can consequently be useful, or even necessary, to the protein to fulfil its biological functions. On the contrary, the picture of a molecular model resulting from the Xray structure determination is, at least apparently, a static one, the only 'dynamic' information residing in the atomic temperature factors. Nevertheless, this must not be considered in contrast with reality, since the Xray structure represents an average, over time and space, of single structures around a conformational minimum, which is representative of the conformation of the protein molecule in a solution of the same medium. On the other hand, a description of a dynamic situation is quite difficult, particularly for a complex molecule: the sort of static image that will turn out from the following discusion must be considered a necessary simplification as well as the starting point for the comprehension, at the molecular level, of the behaviour of biological systems.
General aspects Proteins are polymers of the 20 natural aminoacids (some symbols and conventions relative to amino acids are reported in Appendix 8.D). They may contain other groups, often relevant for the conformation of the molecule, like haems, prosthetic groups, carbohydrates, and so on, or they can coordinate cations (see p. 582). Nevertheless, the building blocks of proteins are the amino acids, and the protein fold* is the first and perhaps more general aspect of its structure. A polypetide chain of a given sequence, in the appropriate conditions, can refold spontaneously into its final threedimensional structure:[931all the necessary structural information must be contained in the amino acid sequences. It should therefore be possible, at least in principle, to predict from it the structure of a protein. Unfortunately, despite several efforts, this remains a hope for the future. Moreover, some simple, schematic rules relative to the forces that contribute to stabilize a structure can be summarized: they are, however, only indications and exceptions are quite comm~n.[~'~~] 1. Groups potentially able to form hydrogen bonds will be positioned accordingly: or at the surface of the molecule, where they can be hydrogen bonded with the solvent, or, when in the interior, a hydrogenbond donor will be close to an acceptor. Not necessarily all the possible interactions of this kind will be realized, but most of them usually are.
2. Polar residues in a watersoluble protein will preferably be located on the surface of the macromolecule and the hydrophobic ones in the interior (the contrary apply for lipidinteracting proteins). 3. Charged groups will be close to the surface, where they can be
t Cooperativity and allostery are not exactly synonymous, but in this context no distinction is made about them. I The term 'fold' is not used here to indicate a process, but simply the way in which the main chain is wrapped on itself.
1
573
574
(
Giuseppe Zanotti
neutralized by solvent ions. When forced to be inside, they will be stabilized by a proper counterion. As a corollary of the previous rules, particularly rule (2), the threedimensional structure of the proteins will be as compact as possible. For example, the packing density of ribonuclease S, calculated approximating the atoms to spheres of van der Waals radius, is about 0.75,[951approximately the same value found for closepacked spheres.
Levels of organization of proteins: secondary structure The concepts illustrated before, despite generalities, refer to single interactions and in practice they are not well suited to describe overall features or general aspects of the structure. A different, and perhaps more useful, approach to understanding the structure of a protein is the identification, under the apparent complexity, of regular schemes and motifs. Looking at the structure under this aspect, a hierarchical organization becomes apparent and several levels of organization, of different complexity, can be distinguished. The first local order is imposed by the hydrogen bonds formed between the NH and the carbonyl oxygen of the polypeptide chain: the regular structure generated by these quite strong interactions is called secondary structure? and results in a limited number of possible conformations, briefly described below. 1. Helices. The more common among the repetitive motifs found in polypeptide chains is the ahelix. The theoretical ahelix, predicted by Pauling et al. in 1951, is characterized by 3.6 residues per turn and a pitch of 5.4 A. A hydrogen bond is formed between the carbonyl oxygen of residue n and the NH of residue n 4. The number of atoms covalently bound in the ring closed by the hydrogen bond is 13 (Fig. 8.24). Along with the number of residues per turn, this number is sufficient to characterize the secondary structure: the ahelix is consequently called a 3.613helix.Other less common helical structures are the 310helix and the n or 416helix, characterized by an exact repetition after three and four residues respectively and a hydrogen bond between residues n and n 3 or n 5. A special case is represented by the a,,helix, which is a sort of mixture between the a and the 3,0helix. Every type of helix can also be defined by its g, and q torsion angles: their indicative values for the most common repetitive structures are reported in Table 8.5. Of course, real helices present backbone torsion angles that deviate from the ideal ones and, in addition, bending and local irregularities are observed.[961Nevertheless, they are the most regular structures found in proteins. Since natural amino acids, except glycine, are chirals, righthanded and lefthanded helices are energetically not equivalent: helices found in proteins are in practice always right handed. Amino acids assuming the torsion angles characteristics of a lefthanded helix, when found, are confined to very short pieces of chain (one or two residues), often at the end of a righthanded helix connecting a Pstrand.
+
+
t For historical
+
reasons, the amino acid sequence is called primary structure.
0C 0N 00 O
Table 8.5. Approximate torsion angles for some common regular structures (from IUPACIUB commission on biochemical nomenclature, Journal o f Molecular Biology, 52, 117 (1970)). (References about the sources of the reported values can be found in the reference; w is assumed to be 180")
Righthanded ahelix Lefthanded ahelix 3,,helix Parallelchain plated sheet Antiparallelchain pleated sheet Polyglycine Polyproline II
H
Fig. 8.24. (a) Stereo view of t w o ahelices of m y ~ ~ l o b i n(data [ ~ ~from ] PDB), connected by a short piece of chain (to simplify the representation, for every side chain only the @carbonis drawn). Helix 7 goes from residue 100 to 118 and h e l i x 8 f r o m 125 t o 148. Residues from 116 t o 119 participate also i n a type I @turn.From I 1 9 t o 124 the structure is less regular. The t w o helices are not exactly aligned, but their axes are slightly bent, a classical situation of the packing of helices, (b) Scheme of the hydrogen bond pattern for the most common types of helices: in the ahelix, 13 atoms are included in the ideal ring from the carbonil oxygen t o the NH. Only 10 atoms in the 3,,helix.
576
1
Giuseppe Zanotti
One of the reasons that helices are quite common is the possibility to accommodate in a very short length a large number of residues: all side chains in fact point away from the helical axis, giving rise to quite an efficient packing of bulky groups, one on the top of the other.C9'] The only residue that cannot be accommodated in a whelix is proline, due to the steric hindrance of its side chain and to the fact that its nitrogen is lacking the hydrogen necessary to form the hydrogen bond. Proline can be fitted properly only in the first turn of a helix, but will interrupt it, or introduce a bend, if present in any other place. A special kind of secondary structure, called polyproline helix, has sometimes been observed. Another important peculiarity of helical structures is represented by their electrostatic properties: since all the dipoles of the peptides are pointing in the same direction, the result is a net total dipole for the helix[981that may contribute, for example, in stabilizing the binding of charged species. 2. ,&structures. A 0strand is a portion of polypeptide chain in a nearly extended, pleated conformation. It is less regular than helices and its torsion angle values reported in Table 8.5 must be considered only indicative, since large variations are observed in practice. A Pstrand is normally not stable in itself, but it is stabilized by the contact with another Pstrand, with which it forms hydrogen bonds. According to the relative direction of the two chains? 0strands can be parallel or antiparallel (Fig. 8.25): they differ in the way the hydrogen bonds are formed, making the latter slightly more stable[1011and more commonly observed in proteins. Since Pchains are quite flexible, this kind of structure can present irregularities and defects: a jump of one residue in a strand is for example called a Pbulge. Several parallel or antiparallel Pstrands form a so called Psheet. Since in a 0strand amino acid side chains point alternatively in opposite directions, a Psheet has the possibility of having a polar surface and an apolar one. Finally, strands in a sheet are not exactly aligned, but are twisted with respect to each other.[lo2]
Fig. 8.25. (a) Schematic drawing of the hydrogen bond pattern for different types of 6sheets. The first t w o Ostrands run antioarallel. ihe third is parallel t o the second one (diiections of strands are indicated by arrows). Hydrogen bonds are differently oriented i n the t w o cases, the antiparallel being more favoured and more commonly found in proteins. A plus sign on the cucarbon indicates the side chain coming up from the sheet, and a minus a side chain going away from the reader. (b) Stereo view of three Pstrands of r i b o n ~ c l e a s e [ ' (data ~ ~ ' from PDB, only Cg is drawn for every side chain). The three strands 7175.1051 10, and 120124 run antiparallel each other. Notice that residues 121 and 122 have the side chains pointing i n the same direction, an irregularity called a Pbulge.
t The chain is considered to run from the N to the C terminus.
Protein crystallography
1
577
Fig. 8.25. (Continued).
3. Others. Short tight loops connecting two strands are called pturns, or hairpins, or reverse turns. Different kinds of classifications have been attempted: one of them, based on the hydrogen bond patterns, is that of MilnerWhite and ~ o e t . [ ' The ~ ~ ] more classical pturns are called type I, 11, and I11 (and type I t , 11', and 111' those with g, and q~ torsion angles reversed). A schematic pattern of two turns is illustrated in Fig. 8.26. In real structures, short pieces of polypetide chains not falling in one of the previous categories are normally found. In general their g, and 1C, torsion angles correspond to those of one of the structures discussed above, but nevertheless that portion of the molecule cannot be classified as one of the previous categories. A last important feature strongly influencing the polypeptide chain conformation is the presence of a disulphide bridge: the sulphur atoms of two cysteines form a covalent bond, connecting two pieces of polypeptide chain or even two different chains. This results in a strong stabilization of the threedimensional structure, at the expense of some local irregularities.
Polypeptide chain description In describing a polypeptide chain, the only relevant variables are in practice the two dihedral torsion angles around the NC, and C,C bonds, called cp and v : the torsion angle w is very close to 180°, owing to its partial doublebond character. Therefore, only 2n  1 numbers are enough to describe the fold of a protein composed by n amino acids. One convenient way of representing the main chain dihedral angles is the socalled Ramachandran plot,[1041where every amino acid is represented by a point of coordinates g, and q . In such a plot, regions forbidden for sterical reasons can be individuated and they represent a large portion of the total area: the backbone torsion angles of all the amino acids, with the exception
Fig. 8.26. Schematic representation of the hydrogen bonds pattern for a yturn (upper) and a fiturn (lower). Symbols for atoms are as in Fig. 8.25. (Adapted from MilnerWhite and ~oet."~~')
578
1
Giuseppe Zanotti
Fig. 8.27. Ramachandran plot for the model of bovine Ptrypsin, orthorhombic form, refined to a crystallographic Rfactor of 0.18 up to a (data from PDB). Small resolution of 1.8 A['051 squares represent glycine residues, crosses all the others. The origin of the diagram is in the centre. Contour lines correspond roughly to fully allowed and outer limit regions.
of glycine which has much more conformational freedom owing to the absence of substituents at the acarbon, should not fall into those areas. Ramachandran plots can be used during the refinement to check for the quality of the structure: amino acids falling into forbidden regions must be corrected, and values at the border or in unfavourable zones considered suspiciously. An example of such a plot is given in Fig. 8.27. Since every type of secondary structure described in the previous subsection is characterized by its own pair of theoretical g, and q values, it corresponds to a point on the plot. From the diagram it is consequently possible to individuate immediately the amount of ahelix, Psheet, and so on, present in the structure. Any information about the connectivity among residues is, on the contrary, lost. A possibly more informative, but less used, method of mapping the folding of the main chain is the diagonal plot.[106]It is a matrix with the amino acid numbers along both axes: if the distance between two residues is less than a predefined amount, the corresponding matrix element is darkened. In this kind of graphic, the major structural elements are easily visualized: an ahelix will produce a thickening along the diagonal and two antiparallel Pstrands a narrow line perpendicular to it; domains can be recognized too, and structural homologies among proteins individuated. Furthermore, the information of a diagonal plot is in a form that can easily be stored in a computer. An example of a diagonal plot is reported in Fig. 8.28.
Higher levels of organization: tertiary and quaternary structure, domains, and subunits We have previously seen that, despite the apparently very large degree of freedom of a polypeptide chain, proteins can be considered as made up by a very limited number of secondary structure elements, that is ahelices,
Protein crystallography
1
579
/3strands and turns, plus some pieces of chain in conformations more difficult to classify. The threedimensional relationships among secondary structure elements is called tertiary structure or, preferably, supersecondary structure. A careful examination of the structures solved to the present has allowed us to identify some macroscopic concepts that simplify the description of the way in which the secondary elements are held together. Of course these rules are not necessarily general, since they are based on quite a limited set of structures.
Fig. 8.28. (a) The bovine pancreatic trypsin Inhibitor, a small protein (58 amino acids) refined t o an Rfactor of 0.16 at 1.5 8, resolution['07' (data from PDB). The backbone ,, C, N, and 0 of the only, that is the atoms C main chain, are shown. (b) @carbonchain trace of the same structure. It is composed by one turn of helix, t w o long bent Pstrands and a final ahelix from residues 47 t o 56. All these elements are disposed in a quite complex way, difficult t o describe. (c) Diagonal plot for the same protein. The plot was produced using the program DGPLOT (Swanson and Bernstein, distributed with PDB). Amino acid numbers are reported on both axes, and numbers inside the diagram correspond to the distance i n A, rounded to the next integer, between the t w o cucarbons. Distances above 9 A are represented by letters. In the diagram the ahelix close t o the C terminus of the molecule is represented by the thickening along the diagonal (A in figure) and the strands from 29 t o 43 and from 6 t o 25, close to each other, by a line perpendicular t o the diagonal (B in figure). Other spatial relationships are immediately evident from the diagram: region 4348 is close i n space t o 2033 (marked C in figure).
580
( Giuseppe Zanotti
ARG PRO ASP PHE CYS LEU GLU PRO PRO TYR THR GLY PRO CY S LY S ALA ARG ILE ILE ARG TYR PHE TYR ASN ALA LY S ALA GLY LEU CY S GLN THR PHE VAL TYR GLY GLY CYS ARG ALA LY S ARG ASN ASN PHE LYS SER ALA GLU ASP CY S MET ARG THR CY S GLY GLY ALA TER Fig. 8.28. (Continued).
Protein crystallography
1
581
One example is given by packing of ahelices: it has been shown that helices tend to pack not parallel to each other, but with the axes forming specific angles: according to the way they are disposed, they can be grouped in only three classes, each of them characterized by a specific angle.[loS1 Connections between strands in a sheet too follow quite strict rules, thoroughly described by ~ i c h a r d s o n . [ ' ~ The ~ ] topology of the sheet can be illustrated by simplified diagrams, like those reported in Fig. 8.29. The physical meaning of such a diagram is discussed on p. 585. Every polypeptide chain does not necessarily fold into one single unit: a portion of it can be structurally independent and is called a domain. Although the concept is not unequivocal, its existence is widely recognized. The most simple definition of domain is that given by ~ i c h a r d s o n : [ a~ ~ ~ ] domain is a contiguous portion of polypeptide chain folded into a compact, local, independent unit. Domains are sometimes easy to recognize, as in the case of immunoglobulins, or obvious, as for calmodulin (Fig. 8.30). Sometimes they are not simple to individuate, or are even questionable. Whether a domain must be thought of as a potentially independent, stable unit or only as a compact globular region contiguous in space, is matter of discussion. The domain concept is in any case justified by the classification (i) given on p. 585. Proteins may eventually be made up by more than one polypeptide chain: often several of them, equivalent or different, interact to form a protein molecule. The assembly of such subunits is called quaternary structure and Fig. 8.29. Topology of the proteins classified as is in general essential for function: dissociation of a multimeric enzyme may 'Greek key p  b a r r e l ~ " ' ~(see ~ ' p. 585 for more result for example in a change or loss of activity. Nevertheless, subunits can details about the classification). Barrels are be considered as independent structural eldments: they can often be separated and crystallized and their overall conformation is in general not among them. Dashes indicate that the first too different from that of the subunit in the macromolecular complex from ~ ~ ~ ~ ~ ~ ~ ~ ~ which they originate. A relative reorientation of subunits has been pyruvate kinase domain 2; (c) trypsin associated with allosteric properties. A classical example of it is mammalian and 2; (d) immunoglobulin C; ( 4 Cu, Zn dimutase; (f) prealbumin; (g) haemoglobin, a tetramer formed by two distinct chains, denoted a and P. superoxide plastocyanin; (h) plasma retinolbinding protein; Two a$ dimers are related by an exact twofold axis, which in some crystal (i) immunoglobulin V; (I) fattyacidbinding form corresponds to a crystallographic one: from the oxygenated to ~ ~ ~ ~ ~ deoxygenated state the molecule undergoes a substantial change in the B  I ~ C ~ O ~ I Oand ~ Ubi~inbindins I~~ protein. quaternary (and also tertiary) structure, paired with a variation of affinity for oxygen.['l11
q

a
It
~~~~~~n~;9~s~~~d
Fig. 8.30. C, tracing of calmodulin, a small protein that binds calcium in four different binding sites["0' (coordinates from PDB). Two 'globular' domains, composed of about 6070 amino acids each, are completely separated in space, connected only by a long ahelix.
f
~
~
582
1
Giuseppe Zanotti
When a macromolecule is made up by equivalent subunits, a relevant aspect is represented by its internal symmetry. The simplest case is represented by a rotation axis: very often, in a dimeric protein the two subunits are related by a twofold axis. Multimeric proteins may present threefold and also five or sixfold axes. A combination of rotation axes can give rise to higher point symmetries, like 222 or 32. Possibly the most complex internal symmetry is represented by the coat of spherical viruses, composed by hundreds of copies of the same protein arranged in a icosahedral symmetry.[1121It must be remembered that some or all of the internal symmetry elements may or may not correspond to those of the crystal (see p. 538).
Groups other than amino acids The product of biosynthesis is a molecule containing only the 20 natural amino acids. To fulfil their function, proteins may need the presence of other groups: therefore, they can undergo posttranslational modifications or interact with other molecules. These modifications may have a strong influence on their structure. A posttranslational modification is a chemical reaction generally involving the side chain of some amino acid.? The functional groups bound are called prosthetic groups and may have the function to assist enzymes in chemical reactions, or to add to natural amino acids properties they lack, for example photochemical ones. A quite common modification is phosphorylation, largely used in nature to control enzymatic activity.[1131 Glycoproteins are the result of binding of polysaccharides. They may be bound through the oxygen of hydroxylated residues, like serine or threonine, or through the nitrogen of asparagine. Carbohydrates are quite hydrophilic and their content can reach a high percentage of the total mass of the protein molecule: glycoproteins consequently present peculiar properties and their function is matter of discussion.["41 Very few of them have been crystallized, and in general the polysaccharide moiety has been found disordered in the crystal. Cations bound to a protein can be divided in two categories: those which simply neutralize charged groups at the surface of the molecule and depend on the ionization conditions of these groups (and ultimately on pH), and those strongly coordinated, required for the stability of the conformation. The latter can influence protein activity by stabilizing one particular conformational state. The more common bound cation is ca2+, which is very abundant in cytoplasm. Among proteins that bind it, the most peculiar is calmodulin (Fig. 8.30), which has four calcium binding sites: the level of calcium bound to the protein modulates its function. Other bivalent cations commonly interacting are Zn2+, Cu2+, and ~ e ~ but + ,many other metals present in nature can be found, in different oxidation states. As an example, the ironsulphur binding site in ferredoxin is shown in Fig. 8.31. A last important case is represented by the small, generally organic, compounds noncovalently bound to proteins. The macromolecule in this case may have the function of carrier or of storage site.
t Other possibilities are: a modification of the N or the C terminal part of the molecule, or a proteolytic cleavage of a peptide bond.
Protein crystallography
1
583
Fig. 8.31. The t w o sulphuriron clusters in Peptococcus aerogenes ferredoxin are shown, along with the polypeptide chain trace of the (coordinates from PDB). Fe and S atoms are disposed alternated at the vertices of a distorted cube: each Fe atom is surrounded by four S atoms, the fourth being that of a cysteine residue.
Thermal parameters and disordered structures Special care must be used in evaluating temperature factors obtained from the refinement of a protein crystal structure. Experimental B factors include, besides thermal vibrations, the static disorder, which in such kind of crystal is particularly relevant. Owing to the high content of solvent, superficial groups of the macromolecule have the effect of partially ordering the solvent, but at the same time, as a consequence of this contact, they become very mobile. It has been shown[115]that it is possible, for very well refined structures, to distinguish the contribution to B factors of real thermal vibration from the static disorder. Moreover, during the refinement procedure thermal parameters are usually restrained, that is their variation is in some way smoothed down. In any case, the comparison of temperature factors for the same structure, ribonuclease A, independently refined by two different groups using different data[l16]shows a quantitative agreement in the trends, that is regions with an high B factor roughly correspond in both structures. As a general rule, in well refined structures main chain atoms present lower thermal motion than side chains, or in any case less disorder. In looking at crystallographic results, it must be kept in mind that a very high B factor for some residues could be either due to an intrinsic disorder of that part of the molecule, or an indication of a misinterpretation of the electron density. In some cases, small parts of the structure, often at the beginning or at the end of the polypeptide chain, or some loops protruding towards the solvent regions, are very mobile and cannot be seen at all in the map. In exceptional situations, two conformations could be differentiated for some residues.[231 The disorder can also have some functional role, as is sometimes the case for allosteric proteins, where two conformational states are present, one of them characterized by a portion of a disordered chain that becomes ordered in the other state.[117,1181In any case, as has been pointed out by ~ i c h a r d s o n , [ ' this ~ ~ ] is a case in which the crystallization process introduces a bias in the results, since less ordered or disordered proteins are likely to be more difficult or even impossible to crystallize.
Solvent structure A high portion of the solvent contained into a crystal cell can be considered not to be relevant for the macromolecule; it is simply there to fill the
584
1
Giuseppe Zanotti
channels produced by molecular contacts in the crystal. And indeed, this unordered solvent cannot be seen in an Xray diffraction experiment. Water molecules closely bound to the protein, on the contrary, can be considered as part of the structure of the macromolecule itself: a protein cannot be completely dehydrated without a complete crash of the architecture of its threedimensional structure. Tightly bound solvent molecules in the crystal are identified during the process of refinement, and can be distinguished in three groups: 1. Water molecules making hydrogen bonds with hydrophilic side chains on the surface of the protein, where often they take part in a tetrahedral or trigonal network of hydrogen bonds. Ordered waters are substantially on the first shell of coordination around the protein, or eventually in the second shell, bound to the water molecules of the first one.
2. Water molecules that serve as a bridge among parts of the main chain or other structural elements that are too far apart to form hydrogen bonds: for example, if two strands of a Psheet diverge slightly, a water molecule can make an Hbond in the middle, filli